COMPUTATIONAL PLASTICITY
Computational Methods in Applied Sciences Volume 7
Series Editor E. Oñate International Cen...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

COMPUTATIONAL PLASTICITY

Computational Methods in Applied Sciences Volume 7

Series Editor E. Oñate International Center for Numerical Methods in Engineering (CIMNE) Technical University of Catalunya (UPC) Edificio C-1, Campus Norte UPC Gran Capitán, s/n 08034 Barcelona, Spain [email protected] www.cimne.com

Computational Plasticity Edited by

Eugenio Oñate Universitat Politècnica de Catalunya, Barcelona, Spain and

Roger Owen University of Wales, Swansea, United Kingdom

A C.I.P. Catalogue record for this book is available from the Library of Congress.

ISBN 978-1-4020-6576-7 (HB) ISBN 978-1-4020-6577-4 (e-book) Published by Springer, P.O. Box 17, 3300 AA Dordrecht, The Netherlands. www.springer.com

Printed on acid-free paper

All Rights Reserved © 2007 Springer No part of this work may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, microfilming, recording or otherwise, without written permission from the Publisher, with the exception of any material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work.

Table of Contents

Preface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . vii A Multi-Scale Continuum Theory for Heterogeneous Materials F. Vernerey, C. McVeigh, W.K. Liu and B. Moran . . . . . . . . . . . . . . . . . . . . .1 Towards a Model for Large Strain Anisotropic Elasto-Plasticity F.J. Mont´ ans and K.J. Bathe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Localized and Diﬀuse Bifurcations in Porous Rocks Undergoing Shear Localization and Cataclastic Flow R.I. Borja . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37 Dispersion and Localisation in a Strain-Softening Two-Phase Medium R. de Borst and M.-A. Abellan . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 55 New Developments in Surface-to-Surface Discretization Strategies for Analysis of Interface Mechanics T.A. Laursen and B. Yang . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 Particle Finite Element Methods in Solid Mechanics Problems J. Oliver, J.C. Cante, R. Weyler, C. Gonz´ alez and J. Hern´ andez . . . . . . 87 Micro-Meso-Macro Modelling of Composite Materials P. Wriggers and M. Hain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105 Numerical Modeling of Transient Impact Processes with Large Deformations and Nonlinear Material Behavior E. Ramm, T. Erhart and W.A. Wall . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 A Computational Model For Viscoplasticity Coupled with Damage Including Unilateral Eﬀects D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto . . . . . . . . . 145

v

vi

Table of Contents

On Multiscale Analysis of Heterogeneous Composite Materials: Implementation of Micro-to-Macro Transitions in the Finite Element Setting D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .165 Assessment of Protection Systems for Gravel-Buried Pipelines Impact and Recurrent Shear Loading Caused by Considering Thermal Deformations of the Pipe B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 187 Enriched Free Mesh Method: An Accuracy Improvement for Node-based FEM G. Yagawa and H. Matsubara . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .207 Modelling of Metal Forming Processes and Multi-Physic Coupling J.-L. Chenot and F. Bay . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 221 Enhanced Rotation-Free Basic Shell Triangle. Applications to Sheet Metal Forming E. O˜ nate, F.G. Flores and L. Neamtu . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 239

Preface

This book contains state of the art contributions in the ﬁeld of computational plasticity. This topic encompasses a wide spectrum of areas in non-linear computational solid mechanics and modelling of materials and their industrial applications. Despite the apparent activity in the ﬁeld, the ever increasing rate of development of new engineering materials required to meet advanced technological needs poses fresh challenges in the ﬁeld of constitutive modelling. The complex behaviour of such materials demands a closer interaction between numerical analysts and material scientists in order to produce thermodynamically consistent models which provide a response in keeping with fundamental micromechanical principles and experimental observations. This necessity for collaboration is further highlighted by the continuing remarkable developments in computer hardware which makes the numerical simulation of complex deformation responses increasingly possible. The book contains 14 invited contributions written by distinguished authors who participated in the VIII International Conference on Computational Plasticity held at CIMNE/UPC (www.cimne.com), Barcelona, Spain, from 5th to 8th September 2005. The meeting was one of the Thematic Conferences of the European Community on Computational Methods in Applied Sciences (ECCOMAS, www.eccomas.org). The diﬀerent chapters of this book present recent progress and future research directions in the ﬁeld of computational plasticity. A common line of many contributions is that a stronger interaction between the phenomenological and micromechanical modelling of plasticity behaviour is apparent and the use of inverse identiﬁcation techniques is also more prominent. The development of adaptive strategies for plasticity problems continues to be a challenging goal, while it is interesting to note the permanence of element modelling as a research issue. Industrial forming processes, geomechanics, steel and concrete structures form the core of the applications of the diﬀerent numerical methods presented in the book. The book includes contributions sent directly by the authors and the editors cannot accept responsibility for any inaccuracies and opinions contained in the text. vii

viii

Preface

The editors would like to take this opportunity for thanking all authors for submitting their contributions. We also express our gratitude to Maria Jes´ us Samper from CIMNE for her excellent work in the edition of this volume. Many thanks ﬁnally to ECCOMAS and Springer for accepting the publication of this book. Eugenio O˜ nate Universitat Polit`ecnica de Catalunya Barcelona, Spain

Roger Owen University of Wales Swansea, United Kingdom

A Multi-Scale Continuum Theory for Heterogeneous Materials Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran Department of mechanical engineering, Northwestern University, 2145 Sheridan Road, Evanston, IL 60208-3111, USA [email protected]

Summary. For the design of materials, it is important to faithfully model the physics due to interactions at the microstructural scales [18, 17, 19]. While bruteforce modeling of all the details of the microstructure is too costly, current homogenized continuum models suﬀer from their inability to suﬃciently capture the correct physics - especially where localization and failure are concerned. To overcome this limitation, a multi-scale continuum theory is proposed so that kinematic variables representing the deformation at various scales are incorporated. The method of virtual power is then used to derive a system of coupled governing equations, each equation representing a particular scale and its interactions with the macro-scale. A constitutive relation is then introduced to preserve the underlying physics associated with each scale. The inelastic behavior is represented by multiple yield functions, each representing a particular scale of microstructure, but collectively coupled through the same set of internal variables. The proposed theory is applied to model porous metals and high strength steel. For the high strength steel the microstructure of interest consists of two populations of inclusions at distinct scales, in an alloy matrix.

1 Multi-Physics Multi-Scale Material Model 1.1 Kinematics and Virtual Power In the spririt of the work performed by Cosserat [2], Mindlin [11] and Germain [10], the building blocks of the multi-scale continuum theory are a set of kinematic variables which represent the motion within the material’s microstructure. These variables can capture the heterogeneous deformation due to the micro-mechanisms occuring at each scale. For an N-scale material, in addition to the macro-velocity ﬁeld v we introduce N-1 independent micro velocity gradients LI 1≤I≤N −1 . In the context of a ﬁrst gradient theory, the internal virtual power density is written as a linear combination of the various

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 1–11. © 2007 Springer. Printed in the Netherlands.

2

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

kinetic variables and their gradients. Integrating over the body Ω, the virtual internal power is written as:

N −1 I. I − I I← . σ : δD + β : δL − δL + β . δL ∇ δPint = dΩ. (1) Ω

I=1 I

I

where σ is the Cauchy stress, β is the Ith micro-stress and β is the Ith microstress couple. The Ith micro-stresses are interpreted as a stress redistribution arising from the presence of heterogeneities within the Ith microstructure. The kinetic virtual power, external virtual power, governing equations and boundary conditions can be found here [4]. 1.2 Constitutive Relation For convenience, we introduce the generalized stress Σ and strain D measures in a vector form containing the components of the macroscopic quantities as well as the various microscopic quantities deﬁned in the previous section. Hence, we write: 1 N −1 . Σ = σ β 1 β · · · β N −1 β

1 1←

N −1 − ← − D = D L − L L ∇ ··· L − L LN −1 ∇ . The generalized rate of deformation D is decomposed into an elastic part De and a plastic part Dp : (2) D = De + Dp . In the elastic regime, it is possible to introduce a generalized elastic matrix C such that the generalized stress increment Σ is related to the elastic part of the rate of deformation De as follows: Σ = C · De

(3)

where Σ is an objective stress rate. The plastic response is written in a multi-physics plastic potential framework. We introduce a yield function φI with the Ith micro-scale of interest. The plastic ﬂow at each scale is determined from the corresponding yield function in the context of associative plasticity.

2 Application to Porous metals Substantial eﬀort has been dedicated to the study and development of micromechanical models applicable to the plastic deformation and failure of porous metals. Two distinct mechanisms contribute to failure. The ﬁrst stage involves the independent growth of voids subject to a remote hydrostatic stress. The

A Multi-Scale Continuum Theory for Heterogeneous Materials

3

Fig. 1. Multi-scale decomposition for a two-scale porous material

second occurs when the voids a large enough to trigger a necking instability of the inter-void ligament. The second stage of failure is therefore characterized by an acceleration in the loss of load carrying capacity of the material as void coalescence occurs. The use of traditional continuum methods to treat failure of porous metals is limited due to their inability to handle localization problems. To overcome this problem, the outlined multi-scale continuum theory is used to describe the response of porous metals after the onset of localization. The additional degrees of freedom introduced through the microﬁelds can represent the inhomogeneous strains arising due to void interactions and coalescence. 2.1 Multi-Scale Model The multiscale description of porous metal is based on the deﬁnition of two domains, representing the micro- and macro-scales, respectively (Fig. 1) The kinematics are expressed in terms of the velocity v associated with the macro-scale and the rate of micro-deformation D1 . The generalized stress and rate of deformation for the two-scale porous metal can therefore be written as: 1 1 1 ← − D= D D −D D1 ∇ , (4) Σ= σ β β , where D is the symmetric part of the macro-velocity gradient, σ is the macro1

1

stress, and β and β are the micro-stress and micro-stress couple, respectively. From (1), the internal power is written as: 1. 1 ← − σ : δD + β : δD1 − δD + β .. δD1 ∇ dΩ. (5) δPint = Ω

4

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

A physical interpretation is provided as follows: the macro-stress σ represents the macroscopic response that undergoes a loss of load carrying capacity due 1 to void growth and coalescence. The presence of the micro-stress β represents the stress redistributions around voids as they grow. It provides a resistance of the matrix material to highly localized deformations. 2.2 Constitutive Relation 1

1

A two-potential plasticity model with yield functions Φ(σ) and Φ1 (β , β ) is employed to represent the material plastic behavior at the macro and microscale, respectively. Homogenization is performed over two averaging domains (macro and meso) as described. The macro-stress σ is determined by an av¯ (macro domain). The macroscopic plastic eraging operation over the RVE Ω deformation is based on an extension of the von-Mises plasticity model that incorporates the eﬀects of the porosity f . A standard yield function accounting for softening mechanisms due to void growth is given as follows: Φ = Φ (σ, f, ε) = 0,

(6)

where the material constants which appear in the function Φ are determined through cell modeling computer simulations. Microscopic plastic deformation is deﬁned as the plastic deformation of the matrix material after the onset of void coalescence. The plastic model is taken in the form of J2 ﬂow plasticity modiﬁed to account for the eﬀects of higher order stress. The microscopic yield function Φ1 is given by: 1

1

Φ1 = Φ1 (β , β , E 1 )

(7)

where E 1 is the microscopic eﬀective plastic strain. 2.3 Numerical Results We multi-scale model is now implemented and compared to a direct numerical sumilation (DNS) of a porous metal bar loaded in tension. In the DNS, the explicit microstructure is represented by a periodic distribution of circular voids of diameter 1µm and volume fraction 3%. An imperfection is introduced by making the void in the center of the specimen slightly larger than others. As localization is expected to occur around the imperfection, voids are only modeled in the central region. For the two-scale continuum simulation, the ﬁnite element discretisation is ﬁne enough to capture size eﬀects at the scale of the voids. An imperfection, in the form of a higher initial average porosity, is introduced in the center of the specimen to initiate localization. The comparison of the macroscopic plastic strain distribution for the DNS and the two-scale continuum is depicted in Fig. 2. The results are displayed at four diﬀerent times t1 , t2 , t3 and t4 . At time t = t1 , the material response reaches

A Multi-Scale Continuum Theory for Heterogeneous Materials

5

Fig. 2. Snapshots of the distribution of equivalent plastic strain in a specimen in tension for (a) the explicit microstructure (b) the equivalent two-scale continuum

Fig. 3. Comparison of the distribution of plastic strain for (a) the explicit microstructure (b) the two-scale material (c) conventional continuum model (one-scale porous model)

the macroscopic instability point (softening of the macroscopic constitutive relation due to void growth), and deformation localizes in a shear band at 45 1

1

degrees to the tensile direction. The micro-stresses β and β act to stabilize the void growth at time t = t2 . The onset of void coalescence occurs at time t = t3 in a plane perpendicular to the loading direction. This mechanism is modeled by a yielding of the micro-stresses and therefore a decrease in resistance to micro-deformation. Consequently, a plane of highly localized plastic

6

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

strain arises in the horizontal direction as shown at time t4 . The behavior of the two-scale continuum compares well with the behavior of the explicit microstructure. The main attraction of the two-scale continuum resides in the gain of computational time. For instance, the typical element size for the twoscale model is ten times as large as that used for the DNS (1 µm and 0.1 µm respectively).

3 Three-scale Model of High-Strength Steels In the previous example, two scales of analysis where considered. Physically speaking, these were the average macroscale behavior of a population of voids and the microscale behavior deﬁned by the coalescence between neighboring voids. We now consider a material in which three distinct scales can be considered. In high strength steels, previously examined within the hierarchical methodology [14, 12, 13, 15, 16, 3], the embedded particles are divided into two groups: the primary particles with the diameter around microns and the secondary particles in the range of 10 to 100 nanometers. By adding alloys during metallurgical processes, the desirable dispersed secondary particles, such as M2C carbides, are formed through precipitation or dissolved from primary particles, which blocks the dislocation path; thus, the strength of steel rise. Whereas the primary particles, such as nitrides, usually have lower toughness as compared with the iron matrix. The formation of primary particles is inevitable during manufacture process. A key-issue in steel design is to establish the relationships between the micro/nano-structures of steel and its macro-scale mechanical properties. To this end, we use the proposed multiscale continuum theory. Three mechanisms are considered here: (i)the failure at the level of primary particles, (ii) the failure at the level of secondary particles and (iii) the failure by necking of the ligaments between micro-voids [1]. 3.1 Multi-Scale Model The three levels of microstructure are shown in Fig. 4. The macro-scale contains primary particles (large square particles) and secondary particles (small circular particles). The micro-scale contains only secondary particles and the sub-micro scale represents the matrix material. Following the framework described before, we introduce the macro-velocity v, the micro-velocity gradient D1 and the sub-micro velocity gradient D2 . The internal power for a three scale material is written as: 1. 1 ← − δPint = σ : δD + β : δD1 − δD + β .. δD1 ∇ Ω 2. 2 ← − (8) + β : δD2 − δD + β .. δD2 ∇ dΩ.

A Multi-Scale Continuum Theory for Heterogeneous Materials

7

Fig. 4. Proposed multi-scale framework for the modelling of high strength steel

A physical interpretation of the various terms can be given as follows. The quantity D1 − D is the inhomogeneous deformation resulting from the localization that occurs from the nucleation of large voids (from primary particles) and the inhomogeneous deformation D2 − D is the result of the localization that occurs from nucleation of micro-voids (from secondary particles). The micro-stress at a scale is interpreted as the stress exerted by the microstructure to redistribute plastic deformation around the voids at that scale. 3.2 Constitutive Relation The failure of High Strength Steels involves mechanisms which involve the microstructure at each scale. Three yield functions are introduced: the macro1

1

potential Φ(σ) and the ﬁrst and second micro-potential Φ1 (β , β ) and 2

2

Φ2 (β , β ), respectively. Each of the above functions is associated with a failure mechanism summarized as follows: (i) void nucleation and growth at primary particles followed by strain localization of width approximately equal to the diameter of a ’primary’ void. (ii) void nucleation and growth at primary particles followed by strain localization of width approximately equal to the diameter of a ’secondary’ void. (iii) secondary-void coalescence by necking of the inter-void ligament and localization of the deformation in the neck. The macroscopic yield function Φ describes the evolution of the macro-stress and plastic strains. It represents the plastic deformation and response of the RVE and can be derived within the hierarchical methodology. The form of the constitutive relation at the macro-scale is such that: Φ = Φ (σ, f, ε)

(9)

where f and ε are the porosity and eﬀective plastic strain, respectively. This function accounts for the loss of load carrying capacity of the material due to

8

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

the cumulative eﬀects of void nucleation, growth and coalescence from both the primary and secondary particles. 1

1

The micro-stresses (β , β ) are the local stress and moment generated in the matrix by larger voids as they grow. When the matrix material fails, the microcouple and micro-stress can no longer be sustained to the same extent i.e. they yield. The yielding point of the micro-stress is controlled by the degradation and strain localization in the material between the primary particles, which is driven by the formation of a void sheet mechanism originating at the scale of the secondary particles. The microscopic plastic deformation is therefore a function of the nucleation and growth of secondary particle nucleated voids (void sheet). As such, volumetric deformation must be accounted for. A simple model can be developed in the form of a Drucker-Prager plasticity model, modiﬁed to account for the eﬀects of higher order stress. It is written in the form: 1 1 (10) Φ1 = Φ1 (β , β , E 1 ) where E 1 is the microscopic eﬀective plastic strain. The submicro-stresses provide a measure of the local stress distribution around the secondary particle nucleated voids during void growth. This mechanism is similar to that described in the previous section for porous materials. The yielding point of the submicro-stresses corresponds to the inability of the matrix material to transmit stress moments after ligament instability. Submicroscopic plastic deformation is subsequently deﬁned as the plastic deformation of the matrix material after the onset of void coalescence (necking of the ligament). The yield function is written in the form of a plasticity model modiﬁed to account for the eﬀects of higher order stress: 2

2

Φ2 = Φ2 (β , β , E 2 )

(11)

where E 2 is the sub-microscopic eﬀective plastic strain. 3.3 Numerical Results A two-dimensional plane strain analysis of a shear test was employed to evaluate the performance of the three-scale material model in shear. The behavior of high strength steel in pure shear has been investigated experimentally by Cowie et al. [5]. Two computations are performed here: (a) direct numerical simulation (DNS) of the shear test with explicit modeling of particles and (b) a computation of the same model using the three-scale steel model. A comparison is then drawn between the two simulations. The stages of shear failure are explained as follows. (a) Debonding of primary particles, and strain localization between the primary particle nucleated voids. In the multi-scale model this corresponds to the yielding of the macro-stress and the formation of a shear band of

A Multi-Scale Continuum Theory for Heterogeneous Materials

9

Fig. 5. Contours of eﬀective plastic strain at diﬀerent stages of deformation

width related to the primary particle size. During this stage the microstress remains in the elastic regime and is responsible for sustaining the observed size eﬀect. (b) Shear driven nucleation and growth at the scale of the secondary particles leads to a terminal shear instability. In the multi-scale simulation this mechanism is modeled through the yielding of the micro-stress. The size eﬀect resulting from the micro-stress can no longer be sustained. The formation of a shear band of width related to the secondary particle size is then observed. This size eﬀect arises from the existence of a sub-microstress that remains in the elastic regime. (c) As deformation increases, coalsecence of secondary particle nucleated voids will occur, leading to a rapid decrease in the load carrying capacity of the material. In the multiscale model this is captured through a yielding of the sub-microstress. No size eﬀect is then captured. This is consistent with the ﬁnal failure of a material.

4 Conclusion The outlined multiscale model oﬀers several advantages over traditional continuum theory. It can be used to model a material which contains an arbitrary number of scales of microstructure. The internal interactions in the microstructure and the resulting size eﬀects can be accounted for at each scale within the mathematical framework. The mechanisms resulting in heterogeneous deformation at each scale are modeled individually through the

10

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

introduction of mutliple plastic potentials, while being coupled through the internal state variables. This theory has been successfully applied to describe the behavior of a porous metal and a high strength steel. This multi-scale framework has been successfully used in [4] to capture the fracture toughness of a high strength steel in terms of the underlying microstructure. Improvements in eﬃcency may be possible by employing the Bridging Scale Method [7, 8, 9, 6].

Acknowledgements The authors gratefully acknowledge the support of the ONR D3D Digital Structure Consortium (award N00014-05-C-0241) and the National Science Foundation.

References 1. McVeigh C, Vernerey F, Liu WK, Moran B and Olson GB (2006) An interactive microvoid shear localization mechanism in high strength steels. Submitted to Journal of Mechanics and Physics of Solids 2. Cosserat E and Cosserat F (1909) Theorie des corps deformables. Paris: A Hermann et Fils 3. Horstemeyer MF, Lathrop J, Gokhale AM and Dighe M (2000) Modeling stress state dependent damage evolution in a cast al-si-mg aluminium ally. Theoretical and applied fracture mechanics 33:31–47 4. Vernerey FJ (2006) Multi-Scale Continuum theory for material with microstructure. PhD thesis, Northwestern University 5. Cowie JG, Azrin M and Olson GB (1989) Microvoid formation during shear deformation of ultrahigh strength steels. Metallurgical transactions 20A:143– 153 6. Wagner G, Karpov EG and Liu Wing Kam (2004) Molecular dynamics boundary conditions for regular crystal lattices. Computer Method in Applied Mechanics and Engineering 193:1579–1601 7. Kadowaki H and Liu WK (2004) Bridging multi-scale method for localization problems. Computer Methods in Applied Mechanics and Engineering 193:3267– 3302 8. Kadowaki H and Liu WK (2005) A multiscale approach for the micropolar continuum model. Computer modeling in Engineering and Science 7:269–282 9. Wagner GJ and Liu WK (2003) Coupling of atomistic and continuum simulations using a bridging scale decomposition. Journal of Computational Physics 190:249–274 10. Germain P (1973) The method of virtual power in continuum mechanics. part 2 microstructure. SIAM Journal of Applied Mathematics 25:556–575 11. Mindlin RD (1964) Micro-structure in linear elasticity. Arch. Ration. Mech. Anal 16:15–78

A Multi-Scale Continuum Theory for Heterogeneous Materials

11

12. Hao S, Moran B, Liu WK and Olson GB (2003) A hierarchical multi-physics constitutive model for steels design. Journal of Computer-Aided Materials Design 10:99–142 13. Hao S, Liu WK and Chang CT (2000) Computer implementation of damage models by ﬁnite element and meshfree methods. Computer methods in Applied Mechanics and Engineering 187:401–440 14. Hao S, Liu WK, Moran B, Vernerey F and Olson GB (2004) Multiple-scale constitutive model and computational framework for the design of ultra-high strength, high toughness steels. Comput. Methods Appl. Mech. Engrg 193(1720):1865–1908 15. Tvergaard V (1982) Ductile fracture by cavity nucleation between larger voids. J. Mech. Pys. Solids 30:265–286 16. Tvergaard V (1988) 3d-analysis of localization failure in a ductile material containing two size-scales of spherical particles. Engineering Fracture Mechanics 31:421–436 17. Liu WK, Karpov EG and Park HS (2005) Nano Mechanics and Materials: Theory, Multiscale Methods and Applications, Wiley 18. Liu WK, Karpov EG, Zhang S and Park HS (2004) An introduction to computational nanomechanics and materials. Computer Methods in Applied Mechanics and Engineering 193:1529–1578 19. Liu WK, Hao S, Vernerey FJ, Kadowaki H, Park H and Qian D (2003) Multiscale analysis and design in heterogeneous system. VII International Conference on Computational Plasticity (COMPLAS VII) 7

Towards a Model for Large Strain Anisotropic Elasto-Plasticity F.J. Mont´ ans1 and K.J. Bathe2 1

2

Universidad de Castilla-La Mancha. E.T.S. de Ingenieros Industriales C/ Camilo Jos´e Cela s/n. 13071-Ciudad Real. Spain. [email protected] Massachusetts Institute of Technology. Dept. of Mechanical Engineering 77 Massachusetts Avenue. Cambridge, U.S.A. [email protected]

Summary. The modeling of large strain anisotropic elasto-plasticity requires that the elastic response can be anisotropic, the yielding is governed by anisotropic yield functions, the hardening is anisotropic and the principal anisotropic elastic and yield directions can align themselves to more favorable stress directions during the response. For general ﬁnite element analysis, the model also needs to be macroscopically-based and computationally eﬀective. We have worked towards such a model based on using the decomposition of the deformation gradient into elastic and plastic parts, logarithmic strains, exponential mapping and the plastic spin as an internal variable. The objective of this presentation is to give basic theoretical considerations and a computational framework for this anisotropic elasto-plasticity model. We also present some numerical results.

1 Introduction Computational large strain plasticity is now well established for the case of isotropic elasto-plasticity, see for example References [1–4]. In these formulations, the use of hyperelasticity [5] was important both conceptually —to not dissipate energy during elastic cycles, see Reference [6]— and algorithmically —to avoid the integration of objective stress rates. Also, the use of the Lee multiplicative decomposition of the deformation gradient into an elastic and a plastic part [7, 8] —previously used by Bilby et al. [9]— and the formulation of the incremental equations in terms of logarithmic strains and Kirchhoﬀ stresses resulted into a remarkable simplicity for the computational return mapping algorithm [10, 11]. Indeed, the backward integration of the rate equation, via the exponential product formula, rendered the incremental algorithm in the logarithmic strain space identical to the small strain return mapping algorithm. This simplicity allowed for an extension of both the theory and the algorithm to anisotropic mixed hardening [11]. Both “unrotated” [10, 11] and spatial formulations and algorithms followed, sometimes formulated in the principal stress/strain space [12, 13]. Of course, all these formulations are Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 13–36. © 2007 Springer. Printed in the Netherlands.

14

F.J. Mont´ ans and K.J. Bathe

completely equivalent, see Reference [14]. However, if kinematic hardening is considered, special care must be used because some plastic spin eﬀects may be inadvertently introduced, resulting in completely diﬀerent response predictions, see Reference [15]. Alternatively, a special but not standard type of kinematic hardening may be considered [16]. Computational plasticity formulations based on logarithmic strains and work-conjugate stresses have now been used extensively and have also been extended successfully to applications in soil mechanics, see Reference [17]. Common to the diﬀerent formulations are the following ingredients: isotropic hyperelasticity, exponential mapping and the additive return in the logarithmic strain space. In this framework, the algorithm of Eterovi´c and Bathe [11] seems to be the ﬁrst implicit algorithm to allow for some anisotropy. This anisotropy is given by the kinematic hardening rule. The algorithm is consistently linearized in Reference [15], where it is noted that anisotropic yield functions may be directly employed in the formulation. However, all the large strain computational plasticity algorithms based on logarithmic strains are using one hypothesis: the elastic strains and the work-conjugate stress measures commute. This property only holds in isotropic elasticity and hence the previous formulations are not applicable in anisotropic elasticity. While some publications appeared recently on computational anisotropic plasticity, see for example [18–21], the published algorithms are not developed following the successful framework of using the deformation gradient decomposition into an elastic and a plastic part, logarithmic strains and exponential mapping. In many cases the eﬀect of the elastic anisotropy is considerably smaller than the eﬀect of the plastic anisotropy and, hence, elastic isotropy is assumed with an anisotropic yield function, see for example Reference [22]. The algorithm presented in [15] is then directly applicable. An important observation discussed in this reference is that, then, the plastic spin does not enter in the dissipation equation and as a consequence, any plastic rotation is possible. Hence, a constitutive hypothesis may be chosen. However, for general anisotropic elasto-plasticity the plastic spin requires special attention. In order to understand the nature and practical eﬀects of the plastic spin, researchers have proposed several ad-hoc constitutive equations, see for example [23–31]. A possible eﬀect of the plastic spin is to cause rotations of the elastic and plastic anisotropy directions during loading. These rotations take place at diﬀerent strain levels depending on the type of material considered [22], as observed and measured experimentally, see References [32–36]. Some materials preserve an almost isotropic elastic behaviour as aluminum [37, 38], and also only show a small rotation of the preferred plasticity orthotropy directions [22, 34, 35]. In these References, approximately 5o of rotation is measured for 20% of strains. Other metals such as steel contain both a substantial elastic and plastic anisotropy and show a signiﬁcant rotation of the orthotropy directions, see References [32, 33, 36]. In these works a realignment of the anisotropy

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

15

directions in steel sheets to new directions during the loading is experimentally observed for strain levels of about 10%. Considering a thermodynamical framework of continua, it seems natural to relate the development of these rotations to the plastic ﬂow and to a decrease of the stored energy. In the following sections we present a model and an algorithm to describe the plastic behaviour of metals with both elastic and plastic anisotropies, and consider the rotation of the elastic and plastic anisotropy directions. This theory is an extension of the formulation presented in References [11] and [15]. The theory employs the multiplicative decomposition of the deformation gradient, logarithmic strain measures, the exponential mapping formula and the plastic spin to govern the rotations of the elastic and plastic anisotropy directions.

2 Kinematics and Incremental Integrations In the derivation of the continuum formulation and the algorithm for the stress calculation we follow the notation used in References [1], [2] and [39]. We include in this section both the continuum and algorithmic formulations since they are closely related. 2.1 Kinematics of Deformation: Multiplicative Decomposition and Strain Rate Tensors The Lee decomposition yields the following multiplicative decomposition for the deformation gradient t 0X

=

p(t) t 0 X p(t) X

:=

e t p t 0X 0X

(1)

where, conceptually, p (t) is a conﬁguration with the elastic strains relaxed p(t) t X ≡ t0 X e and 0 X ≡ t0 X p . Of course (stress-free conﬁguration). Hence, p(t) the decomposition of Equation (1) is unique if t0 X p is known, for example, via the integration of the plastic path. The spatial velocity gradient t l = ∂ t v/∂ t x, where t v ( t x) is the time derivative of the displacements, is t

l=

−1 t ˙ t 0X 0X

(2)

and its symmetric part, the spatial deformation rate tensor, is t T t d = 12 t0 X˙ 0 X −1 + t0 X −T t0 X˙

(3)

In view of Eq.(1), Eq.(2) can be decomposed as p e −1 −1 −1 l = le + lp = X˙ (X e ) + X e X˙ (X p ) (X e )

(4)

16

F.J. Mont´ ans and K.J. Bathe

In the equations to follow we frequently omit the time left-indices when a confusion is hardly possible. The tensor p

−1

Lp := X˙ (X p )

(5)

is the modiﬁed plastic velocity gradient. The tensor Lp operates in the intermediate stress-free conﬁguration. The symmetric part of Lp is the modiﬁed plastic deformation rate tensor p pT −1 −T (6) D p := 12 X˙ (X p ) + (X p ) X˙ while its skew part is the modiﬁed plastic spin. p pT −1 −T W p := 12 X˙ (X p ) − (X p ) X˙

(7)

On the other hand, if we deﬁne L, the modiﬁed velocity gradient as the pull-back of l to the intermediate conﬁguration, we arrive at L = Le + C e Lp

(8)

where C e ≡ X e T X e is the right Cauchy-Green deformation tensor in the stress-free conﬁguration. Note that some of our deﬁnitions diﬀer from those sometimes found in the literature. For example D p is sometimes deﬁned as D p = sym (C e Lp ), see for example [40–42]. 2.2 Integration of the Plastic Deformation Gradient This section follows the same procedure presented in Reference [15]. From Equation (5), the evolution of the plastic deformation gradient tensor is given by the diﬀerential equation t ˙p 0X

= t Lp t0 X p

(9)

whose backward-Euler exponential solution is given by t p p t+∆t t+∆t p L (10) 0X 0 X = exp ∆t where the exponentialfunction of a matrix exp ∆t t+∆t Lp for small steps such that ∆t t+∆t Lp 1 can be approximated by (11) exp ∆t t+∆t Lp I + ∆t t+∆t Lp Using ∆t

t+∆t

Lp = ∆t

t+∆t

D p + ∆t

t+∆t

Wp

we have that for small steps the following property holds exp ∆t t+∆t Lp exp ∆t t+∆t D p exp ∆t t+∆t W p

(12)

(13)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

yielding the following update formulas: p −1 t+∆t = t0 X p −1 exp −∆t t+∆t W p exp −∆t t+∆t D p 0X e e t+∆t t+∆t W p exp −∆t t+∆t D p 0 X = X ∗ exp −∆t

17

(14) (15)

where the tensor X e∗ := t+∆tt X t0 X e is the trial elastic deformation gradient (i.e. with the plastic state frozen). The polar decomposition theorem applied to the trial elastic deformation gradient yields e X e∗ = Re∗ ← U −∗

(16)

e e where ← U −∗ is the trial (elastic) right stretch tensor and R∗ is the trial rotation tensor. We now deﬁne the following incremental (“plastic”) rotation t+∆t w t+∆t (17) Wp t R = exp ∆t e e Using (15) and deﬁning ← C −∗ := X ∗ deformation tensor) we obtain

e C ← −∗ =

t+∆t wT tR

exp ∆t

t+∆t

Dp

T

X e∗ (the trial right Cauchy-Green

t+∆t e 0C

exp ∆t

t+∆t

Dp

t+∆t w tR

(18)

We now deﬁne the logarithmic strains by t+∆t e 0E

:=

1 2

log

t+∆t e 0C

e E ← −∗ :=

and

1 2

e log ← C −∗

(19)

The following tensors are the measures updated to the stress-free conﬁguration C e∗ :=

t+∆t w tR

E e∗ :=

t+∆t w tR

e C ← −∗

t+∆t wT tR

(20)

e t+∆t wT E (21) tR ← −∗ For future expressions we note that (·) are the quantities (·) rotated to the ← − rotationally-frozen conﬁguration (deﬁned below), i.e.

(·) = ← −

t+∆t wT tR

(·)

t+∆t w tR

(22)

Using Equations (11) and (19), Equation (18) may be written as E e∗

t+∆t e 0E

+ ∆t

t+∆t

Dp

(23)

with the additional restriction that E e∗ 1, i.e. the elastic strains and incremental steps are only moderately large. This restriction is typically fulﬁlled in metal plasticity. Alternatively, expression (23) may be written as t+∆t e E 0← −

e E ← −∗ − ∆t

known

t+∆t

p D ← −

(24)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

19

conﬁguration is given by t+∆t0 ReT , only known after integration. Fortunately, Equations (24) and (25) show that the additive algorithm also holds in the conﬁguration in which the plastic rotation t+∆tt Rw has not been applied yet. From a continuum perspective, using the following deﬁnitions e p e ˙ e eT ˙ w wT and wp = Re W p ReT we∗ = R˙ ∗ ReT ∗ , w =R R , W =R R (30) performing the time derivative of Equation (27) and multiplying by ReT ∗ = RwT ReT to transfer the Equation to the spatial conﬁguration, we obtain

i.e.

e ˙ e eT + Re R˙ w RwT ReT R˙ ∗ ReT ∗ = R R

(31)

we∗ = we + wp

(32)

3 Free Energy Function and Dissipation Inequality The global free energy ψ is assumed to admit the additive decomposition into a stored energy function W and a hardening potential H ψ X e , X i , X i -history = W X e , X i -history + H X i , X i -history (33) where X i are internal variables which can be deﬁned by a gradient of some local internal displacements. Obviously, by objectivity, the stored energy function should depend only on the stretch part of X e , since it must remain unaﬀected by rigid body motions. We assume that the solid deforms in such a way that the total potential energy is minimum and that the dissipation energy is maximum including the eﬀect of plastic spin. We assume that the rotation of the anisotropy directions is also related to a change of the potential energy. Hence, special considerations arise for the stored energy function and the hardening potential. We incorporate these considerations in the energy function and hardening potential proposed below. 3.1 Stored Energy Function: Orthotropic Hyperelasticity Based on Logarithmic Strain Measures In the case of isotropic elasticity, the right Cauchy deformation tensor C e and the second Piola-Kirchhoﬀ stress tensor S commute. Then, the Mandel stress tensor Ξ := C e S and the symmetric part of the Mandel stress tensor, Ξ s , results in (34) Ξ s = Ξ = 12 (C e S + SC e ) = U e SU e which in terms of the spatial Kirchhoﬀ stress tensor τ may be written as Ξ s = U e X e−1 τ X e−T U e = ReT τ Re = τ¯

(35)

20

F.J. Mont´ ans and K.J. Bathe

where τ¯ is the rotated Kirchhoﬀ stress tensor [2]. Assuming isotropic elasticity, the governing strain energy function can be expressed as W = U (J) + µ E ed : E ed = U (J) + µ E e : P : E e

(36)

where E e := ln U e are the logarithmic strains, E ed := P : E e are the deviatoric logarithmic strains, P := I − 13 I ⊗ I is the deviatoric projector tensor and I and I are, respectively, the fourth and second order identity tensors. The two terms in Equation (36) represent the volumetric and deviatoric strain energies respectively. The rotated Kirchhoﬀ stress tensor is obtained as (see for example Reference [15]) Ξ ≡ Ξ s ≡ τ¯ =

∂W = JU (J) + 2µ P : E e ∂E e

(37)

whereas the skew-symmetric part of the Mandel stress tensor, Ξ w , vanishes. As also mentioned in the introduction, in anisotropic plasticity, the elastic properties are frequently considered as isotropic given that experimentally much smaller deviations from isotropy are observed for elastic properties than for plastic properties. In this work we wish to relax the assumption of isotropy for the elastic properties and allow moderate anisotropic elasticity, and hence we use the following function: t W = U t J + µ t E e : t Ad : t E e (38) where t Ad is the orthotropy structural tensor which has the same characteristic space as P (commutes with P) and is, in general, close to P. Note that in this case the volumetric component is assumed as isotropic reducing the number of independent constants to seven. Of course, a general anisotropic tensor t A (with nine constants) may also be employed with the logarithmic strain. In this case the stored energy function is of the type t

W=

1 t e 2 E

: tA : tEe

(39)

where t A−1 in the principal material orthotropy axes { t P i , i = 1, 2, 3}, may be written as —see for example Reference [1]— ⎤ ⎡ 0 0 1/Ea −νba /Eb −νca /Ec 0 ⎢ −νab /Ea 1/Eb −νcb /Ec 0 0 0 ⎥ ⎥ ⎢ ⎢ /E −ν /E 1/E 0 0 0 ⎥ −ν ac a bc b c t −1 ⎥ ⎢ A =⎢ (40) 0 ⎥ 0 0 0 1/Gab 0 ⎥ ⎢ ⎣ 0 0 0 0 1/Gbc 0 ⎦ 0 0 0 0 0 1/Gca { t P } i

where Ea , Eb , Ec are the Young’s moduli in the principal directions, νba , νca , νcb , νab , νac , νbc are the Poisson ratios and Gab , Gbc , Gca are the shear moduli. These constants need to satisfy certain conditions, see e.g. [1].

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

21

In Equations (38) and (39), the strain tensor, and thus also the elastic anisotropy tensor, are deﬁned in the unrotated conﬁguration (i.e. with the elastic rotations given by Re removed). Between time t and time t + ∆t, this conﬁguration and all objects deﬁned in this conﬁguration rotate by the amount t+∆tt Rw due to the plastic spin—see Equation (28). And during the plastic ﬂow, also the lattice rotation takes place, resulting in an additional rotation t+∆tt RA for the anisotropy directions. For example, the resulting energy of Equation (39) at t + ∆t is t+∆t

W= = =

t

t t+∆t e 1 t+∆t e E E 2 ← − : A: ← − t+∆t t+∆t e 1 t+∆t e E : A : E 2 ← − ← − ← − t+∆t t+∆t e 1 t+∆t e E : A : E 2

(41)

t+∆t A A tR ← − we imply that the tensor has rotated by t+∆t A t with respect to A. The rotation tensor t R represents the rotation of the elastic anisotropy tensors. Therefore, the energy expression in the stress-free conﬁguration is obtained by the rotation t+∆tt Rw and the rotation t+∆tt RA . The derivative of the stored energy function in absence of plastic rotations is e ˙ ˙e W = ← E A E (42) − :← −: ← − apr

where by

A =:

t+∆t

e L = Ee : A : ← −E

(43)

e e The tensor ← T = ∂W / ∂ E A E − ← − apr = ← − : ← − is deﬁned as the symmetric logarithmic stress tensor (or generalized Kirchhoﬀ stress tensor) in the rotation-free conﬁguration. If the lattice structure is not ﬁxed, the variation of the strain energy function in the rotation-free conﬁguration is ˙ = T : E˙ e + 1 E e : A˙ : E e W 2← ← − ← − − ← − ← −

(44)

The second term in Equation (44) is the work variation due to a rotation of the lattice, which after plastic ﬂow will be in a more favorable orientation. Hence A ˙ A A T as the structural this term must be negative. Deﬁning ← W − := R R t+∆t t+∆t e T A E anisotropy spin tensor and using t+∆t ← − = ← − : ← − , the second term of Equation (44) can be written in symbolic notation as 1 2

e A A e W − W E E T − ← − ← − :← ← − ← −+ e A A e = ← T : E W − W E − ← − ← − ← − ← −

e e ˙ E A E ← − :← −: ← − =

1 2

A =← T −w : W ← −

1 2

e A A e T : E W − W E ← − ← − ← − ← − ← −

(45)

22

F.J. Mont´ ans and K.J. Bathe

where ← T −w is a skew tensor deﬁned as e e T E T T E (46) ← −w := ← − ← −−← −← − Of course we can deﬁne equivalent measures in the unrotated conﬁguration: t+∆t wT T = A : E e and T w := E e T − T E e tR ← − or in the spatial conﬁguration

T :=

t+∆t

t :=

t+∆t w tR

t+∆t e t+∆t T t+∆t0 ReT 0R

(47)

eT e e = Re∗ ← T − R∗ and tw := e t − te (48)

where ee := ln V e and V e is the stretch tensor obtained from the left polar decomposition theorem. Finally we obtain ˙ = T : E˙ e + T w : W A W ← − ← − ← − ← −

(49)

˙ = T : L Ee + T w : W A W ← −

(50)

Here T w is determined once T and E e are known, i.e., it is not an independent or internal variable. The second term in the variation of the stored energy function is the variation due to the rotation of the anisotropy axes, and depends on the non-coaxiality of stresses and elastic strains. Figure 1 refers to the diﬀerent rotations and conﬁgurations used. The spatial conﬁguration for strains is known from the material conﬁguration by t+∆t 0 X. From this spatial conﬁguration we can directly obtain the trial unrotated conﬁguration (rotationally frozen) by the rotation ReT ∗ , obtained from the polar decomposition Eq.(16) of the trial elastic gradient (292 ). Then, as shown below, we obtain the plastic correction t+∆tt Rw for the trial unrotated conﬁguration, which has the ﬁnal value given by Equation (28). Due to the rotation t+∆tt Rw the preferred elastic and plastic anisotropy directions rotate by the additional amount t+∆tt RA in the form given below. Since we are assuming moderate incremental steps, both t+∆tt Rw and t+∆tt RA may be considered to commute. 3.2 Hardening Potential Consider a hardening potential of a similar form to that of the stored energy function H = Hkin +Hiso +Hw = 12 h¯ (1 − M ) 32 E i : H : E i + M ζ 2 + 12 Kw ξ 2 =

1¯ 2h

(1 − M )

3 2

i

i

E H E ← − : ← −:← − +M ζ

2

(51)

+

2 1 2 Kw ξ

(52)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity a principal orthotropy direction in the trial unrotated configuration

23

a principal strain direction in the trial unrotated configuration a principal strain direction or principal orthotropy direction in the final unrotated configuration

a principal strain direction or principal orthotropy direction in the final spatial configuration

Fig. 1. Conﬁgurations involved in the stress-integration algorithm

¯ (1 − M ) is the eﬀecwhere M is the mixed hardening parameter, 23 H := h ¯ tive kinematic hardening modulus and K := hM is the isotropic hardening ¯ plays the role of eﬀective hardening modulus. The modulus. The parameter h parameter Kw is a hardening for couple-stresses. Eq.(51) corresponds to a ¯ it SPM description of hardening, see Reference [43]. However, for constant h coincides with the SPS method. In (51) we have included the possibility of anisotropic kinematic hardening through the use of an anisotropy tensor H, H similar to Ad . The tensor ← −, rotates at the speed given by the internal spin tensor W H for similar reasons as those given for the stored energy function. We deﬁne the internal overstresses as κ :=

∂ψ and ∂ζ

κw :=

∂ψ ∂ξ

(53)

Hence, κ=

∂ψ ∂H = = Kζ ∂ζ ∂ζ

and

∂H ∂ψ = = Kw ξ ∂ξ ∂ξ

(54)

∂2ψ ˙ ∂2H ˙ ξ= ξ = Kw ξ˙ ∂ξ 2 ∂ξ 2

(55)

κw =

or κ˙ =

∂2ψ ˙ ∂2H ˙ ζ= ζ = K ζ˙ ∂ζ 2 ∂ζ 2

and

κ˙ w =

We define the internal backstress as ∂ψ ∂H i = = H← H E B i −:← − ← −s = ∂ E i ∂ E ← − apr ← − apr

(56)

Then, the derivative of the hardening potential is ˙ E i + κζ˙ + κw ξ˙ ˙ i 1 Ei : H E H˙ = ← B − + 2H ← − ← −:← − −s : ←

(57)

24

F.J. Mont´ ans and K.J. Bathe

and following the same steps as for the stored energy function 1 2H

i i H ˙ E H E B ← − :← −: ← − =← −w : W ← −

(58)

where ← B −w is a skew tensor deﬁned as i i B E B B E ← −w := ← − ← −s − ← −s ← −

(59)

Finally we have ˙ i B w : W H + κζ˙ + κw ξ˙ E H˙ = ← B − +← − ← − −s : ← i H ˙ ˙ = Bs : ← L −E + B w : W + κζ + κw ξ

(60)

However, we note that equations (51), (54) and (56) may not be formally adequate because they are deﬁned in terms of total internal strains and, as the plastic strains, they are path dependent. Hence directly assuming (60), (55) and the rate form of (56) is more appropriate, and (51) should be taken just for motivation purposes. Furthermore, Equation (33) should formally be assumed in rate form, and in the derivations to follow only the rate form will be used.

4 Mapping Tensors from Quadratic to Logarithmic Strain Space In large strain plasticity, logarithmic strain measures frequently yield simple and natural descriptions. Of course, these strains may be used in any conﬁguration simply using the proper stretch tensor to obtain them. The following relationship holds: E e = Re T ee Re

with

E e = ln U e , ee = ln V e

(61)

Hence, it is noted that for logarithmic strain tensors, the push-forward and pull-back operations are performed with the rotation part of the deformation gradient alone. One may say that the stress-free conﬁguration and the “unrotated” conﬁguration are coincident in the logarithmic strain space. Obviously, since the logarithmic strain tensors and the Almansi and Green strains are all unique for a given deformation gradient, there exist a one-to-one mapping between them. For example e E e = ME A:A

(62)

where if the spectral forms of the strain tensors are Ee =

3 i=1

ln λei N i ⊗ N i ,

Ae =

3 e 1 2 λi i=1

2

− 1 Ni ⊗ Ni

(63)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

25

ME A can be written as ME A=

3 2 ln λei Ni ⊗ Ni ⊗ Ni ⊗ Ni λe 2 − 1 i=1 i

(64)

as it is straightforward to verify. Conversely MA E=

3 λe i=1

2

−1 Ni ⊗ Ni ⊗ Ni ⊗ Ni 2 ln λei i

(65)

e is such that Ae = MA E : E . In a similar way, there is a one-to-one mapping between the deformation rate tensor and the time-derivative of the logarithmic strains. These mapping tensors may be found to be (see Reference [51]) 3 3 ln λej − ln λei s 1 ∂E e ˙ = M ⊗ M + 2 M i M j (66) ME = i i e e 2 e 2 e 2 D ∂A λ λj − λi i=1 i i=1 j=i

and 3 3 λej 2 − λei 2 s ∂Ae e 2 D 1 λi M i ⊗ M i + M˙ = e = e − ln λe M i M j 2 E ∂E ln λ j i i=1 i=1

(67)

j=i

where M i := N i ⊗ N i s

M i M j :=

1 4

(68) s

(N i ⊗ N j + N j ⊗ N i ) ⊗ (N i ⊗ N j + N j ⊗ N i ) ≡ M j M i (69)

These tensors have major and minor symmetries and represent the one-to-one mappings relating deformation rates as e ˙ e E˙ = ME D:D

e and D e = MD : E˙ E˙

(70)

respectively. Furthermore, in the rotation-frozen conﬁguration ˙ e ME˙ : D e and D e = MD : E˙ e E −D ← ← − ← −E˙ ← ← − =← − −

(71)

Also, in the stress-free conﬁguration e E˙ L Ae and L Ae = MD : L E e L ← − − − ← −E = MD : ← E˙ ←

For future use, we deﬁne two fourth order mapping tensors 1 M e3 E˙ − C e 4· ME˙ := · M W C −D ← −D ← − − ← − ← 2 ←

(72)

(73)

26

F.J. Mont´ ans and K.J. Bathe

and

1 S M := ← − 2

e3 e4 E˙ E˙ M M C C −D + ← −D ← − ·← − ·←

(74)

n where by · we imply the contraction of the n − index of the fourth order tensor with the second index of the second order tensor. Then, it can be shown that if we deﬁne D E˙ K S M S M (75) ← − := ← −:← −E˙ so that ← − =: K ← −:← −D we obtain

and

e e E˙ = K : S M + WM S = C K : M Ξ := C − ← − ← ← − − ← −D ← − ← − ← − ← − ← M e e E E K ← −:W ← − =← − K ← −−K ← −← − ≡ Ξw ← −w := K Ξ SM ← −s = K ← −:← −

(76)

(77) (78)

The tensor K is actually the generalized K irchhoff stress tensor T , see also below, and hence the conversion to the symmetric part of the Mandel stress tensor Ξ s is given by Equation (78).

5 Dissipation Inequality The stress power in the reference volume may be expressed in the intermediate conﬁguration as P ≡ S : L = S : (Le + C e Lp ) = S : (D e + W e ) + S : C e (D p + W p )

(79) (80)

where S is the pull-back of the Kirchhoﬀ stress τ to the stress-free conﬁguration. Since S is symmetric the product S : W e = 0, i.e. the modiﬁed elastic spin (which also contains the rigid-body spin) produces no work. Thus, in a rotationally-frozen conﬁguration we are left with ˙ e + S : C e Dp + W p (81) P≡← S : L = K : E ← − ← − ← ← − − − ← − ← − ← − where we used (71) and (75). Alternatively, in the stress-free conﬁguration e e p p S:L = K:← L −E + S : C (D + W ) e e p p = K:← L −E + C S : (D + W )

(82) (83)

Using Ξ = C e S, the stress power can be written as e p p S:L =K:← L −E + (Ξ s + Ξ w ) : (D + W ) e p p =K:← L −E + Ξ s : D + Ξ w : W

(84)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

27

Thus, the symmetric Mandel stress tensor produces power on the modiﬁed plastic strain rate, whereas the skew-symmetric Mandel tensor produces power on the modiﬁed plastic spin. This last work is due to the kinematic coupling produced by the Lee decomposition and the possible rotation of elastic anisotropy axes. In the case of isotropy or deformation through the orthotropy axes, the term vanishes. Neglecting the eﬀect of temperature, the dissipation inequality from the second law of the thermodynamics is D˙ = P − ψ˙ ≥ 0

(85)

˙ + H. ˙ Thus where ψ˙ is the free energy function rate, assumed to be ψ˙ = W using (49) and (60) e A i H ˙ ˙ L ψ˙ = T : ← L −E + B w : W + κζ + κw ξ −E + T w : W + B s : ←

and

(86)

e p p D˙ = (K − T ) : ← L −E + Ξ s : D + Ξ w : W

i H ˙ ˙ −T w : W A − B s : ← L −E − B w : W − κζ − κw ξ ≥ 0

(87)

Since the equality must hold for pure elastic deformations, T =K

(88)

T w = Kw ≡ Ξw

(89)

and, in consequence, The reduced (plastic) dissipation inequality is now i H ˙ ˙ D˙ p = Ξ s : D p + Ξ w : W d − B s : ← L −E − B w : W − κζ − κw ξ ≥ 0 (90)

where we deﬁned the dissipative spin tensor in the unrotated conﬁguration as W d := W p − W A

(91)

We note that if W p = W A then the skew part of the Mandel stress tensor does not contribute to the dissipation function. On the other hand, since W A is assumed to be a function of W p , if W p = 0 then W A = 0 and no dissipation takes place either due to the skew part of the Mandel stress tensor. We will assume that the following relationship holds W A = ρW p

(92)

where ρ is a material scalar parameter. Then W d = (1 − ρ) W p

(93)

We assume now –without loss of generality– that the elastic region is enclosed by two yield functions fs (Ξ s , B s , κ) and fw (Ξ w , B w , κw ), the La˙ s − γf ˙ w , where t˙ and γ˙ grangian for the constrained problem is L = D˙ p − tf

28

F.J. Mont´ ans and K.J. Bathe

i i are the consistency parameter increments. Note also that ← L −E ≡ D . If we claim that the principle of maximum dissipation holds, the stress and other internal variables are such that ∇L = 0, i.e. for the yield function expressions given ⎧ ∂L ∂fs ∂L ∂fw ⎪ = 0 ⇒ D p = t˙ and = 0 ⇒ W d = γ˙ ⎪ ⎪ ∂Ξ s ∂Ξ s ∂Ξ w ∂Ξ w ⎪ ⎪ ⎪ ⎪ ⎨ ∂L ∂fs ∂L ∂fw = 0 ⇒ L E i = −t˙ and = 0 ⇒ W H = −γ˙ ∇L = 0 ⇒ ← − ∂B ∂B ∂B ∂B ⎪ s s w w ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ∂fw ⎩ ∂L ˙ ˙ ˙ ∂fs

∂κ

= 0 ⇒ ζ = −t

∂κ

and

ξ = −γ˙

∂κw

(94) These expressions are the associated ﬂow and hardening rules for general elastoplasticity at ﬁnite strains. It is noted that if, as usual, the enclosure of the elastic region for the symmetric part is expressed in the form of fs (Ξ s − B s ...) then for associative plasticity the following relationship is automatically enforced i i p (95) L ← −E ≡ D = D Furthermore, W i does not aﬀect the dissipation function and can be freely prescribed. In view of Equation (95), and assuming that internal variables rotate as the plastic variables, we will set

and, as a consequence

Wi = Wp

(96)

Xi = Xp

(97)

The loading/unloading (complementary) Kuhn-Tucker conditions are, as usual ˙ s≡0 t˙ ≥ 0, fs ≤ 0 and tf (98) γ˙ ≥ 0,

fw ≤ 0

and γf ˙ w≡0

(99)

and the consistency conditions are t˙f˙s ≡ 0

and γ˙ f˙w ≡ 0

(100)

The formulations presented herein and in Reference [44] show some similarities with some other works, see for example References [18, 20, 45–48], but there are also some signiﬁcant diﬀerences; in particular we are using logarithmic strains in an incremental form.

6 Yield Functions There is still much experimental work needed to establish the elastic domain and yield functions for the symmetric and skew parts of the Mandel stress tensor. From the current experimental evidence it is diﬃcult to infer sound

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

29

data about a macroscopic (continuum) elastic domain for the skew part of the Mandel stress tensor, and for the plastic spin evolution. Hence, at this point a “reasonable” proposition is necessary. An ad hoc extension of the small strains theory without plastic spin follows. 6.1 Yield Function for the Symmetric Part For the symmetric part of the Mandel stress tensor the well-known Hill’s quadratic yield criterion is assumed to hold, i.e. the yield function for Ξ s is given by the expression (see for example Reference [1]) fs :=

3 (Ξ s − B s ) : Aps : (Ξ s − B s ) − 1 = 0 2κ2

(101)

where Aps is the plastic anisotropy tensor which in this work we assume to have the same preferred anisotropy directions as the elastic anisotropy tensor. Given this function, the speciﬁc values of the internal variable increments are obtained from Equations (94) and (95) as ∂fs 3 = 2 Aps : (Ξ s − B s ) t˙ D i = D p = t˙ ∂Ξ s κ

(102)

The internal isotropic variable rate is obtained as 2 ∂fs = (fs + 1) t˙ ζ˙ = −t˙ ∂κ κ

(103)

which, at the yield condition (fs = 0) takes the value ζ˙ = 2t˙ /κ. The physical meaning of ζ˙ is the eﬀective plastic strain rate, see Reference [1]. 6.2 Yield Function for the Skew Part For the skew part, in this work we consider the simplest possible yield function, of the Mises type √ (104) fw = Ξ w − 2κw where κw is the allowed yield value, which may take the value of zero. From Equation (94), the speciﬁc ﬂow variables take the form W d = γ˙

∂fw ˆw = γ˙ Ξ ∂Ξ w

(105)

√ ∂fw ξ˙ = −γ˙ = 2γ˙ (106) ∂κw ˆ w := Ξ w / Ξ w . The physical meaning of where we deﬁned the “direction” Ξ ξ˙ is the eﬀective dissipative rotation rate. Using Equations (92) and (93) we obtain 1 ρ ˆ w and W A = ˆw γ˙ Ξ γ˙ Ξ (107) Wp = (1 − ρ) (1 − ρ)

30

F.J. Mont´ ans and K.J. Bathe

One important consequence of the function fw deﬁned in Equation (104) and the expression (1072 ) is that if 1 > ρ > 0 then W A and Ξ w ≡ T w have the same direction. But as noted just after Equation (44), the term T w : W A should be negative. Hence possible values are ρ > 1 and ρ < 0. If ρ > 1 then the term T w : W A is negative and W p and W A have the same direction. If ρ < 0 then the term T w : W A is also negative and W p and W A have opposite direction. The actual rotation direction is not only determined by ρ, but also by the elastic anisotropy tensor because its shape may change the direction of Ξ w . 6.3 Coupling of Symmetric and Skew Parts The yield function Equation (104)√would mean an instantaneous rotation once Ξ w is over the allowed value 2κw . However this is not consistent with experiments, in which progressive rotations are observed. Aside, in mechanics of single crystals this rotation is not independent of the ordinary (symmetric) plastic ﬂow (Schmid’s law). Hence, in this work we propose a viscoplasticitylike ﬂow for the skew part in which the eﬀective plastic strain plays the role of the time variable. This proposed expression is m ˙ξ = < fw > ζ˙ (108) η where < · > is the Macauley bracket function, η is the “viscosity” material parameter with units of (couple-)stress and m is another material parameter. Hence, fw may have values greater than zero which relax with plastic ﬂow. In terms of consistency parameters, Equation (108) may be written as √ m 2 < fw > t˙ (109) γ˙ = κ η Hence, γ˙ is zero if either fw ≤ 0 or t˙ = 0.

7 Numerical Example In order to test the capabilities of the present theory in modelling the rotation of the anisotropy directions, we have carried out some numerical experiments. In these numerical tests, we aim for predictions of the experimental results reported in Reference [32]. In these experiments, a rotation of the material symmetry was observed when a steel sheet is strained in a direction that forms an angle θ with the rolling or prestrain direction. Details of the experiments are given in Reference [32]. Only small changes in the shape of the yield function were observed and hence the shape of the yield function can be assumed to remain constant, see also Reference [33].

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

31

However, unfortunately, in Reference [32] only the measured plastic anisotropy and its evolution are reported. Since our theory includes and indeed uses elastic anisotropy, we need to assume elastic anisotropy parameters. In a uniaxial test, a relevant degradation of Young’s modulus and a variation of Poisson’s ratio in the test direction has been reported [49]. Elastic anisotropy has also been measured in rolled steel, brass and aluminum, see for example [50]. We therefore assume the following elastic (only slightly anisotropic) material parameters: Ea = 2.04×1011 Pa, Eb = 2.03×1011 Pa, Ec = 2.10×1011 Pa, νab = 0.3, νac = 0.3, νbc = 0.3, and Gab = 0.82 × 1011 Pa. The yield stress κ0 and Hill’s yield function parameters have been reported in Reference [32], i.e. f = 0.3613, h = 0.4957, g = 0.3535 and we used N = 1.175 and κ0 = 23 × 107 Pa. The hardening has been considered as isotropic according ¯ for which the constants to the formula κ = κ∞ − (κ∞ − κ0 ) exp (−δζ) + hζ, ¯ have been deduced from the experimental data, h = 3.5 × 108 Pa, κ∞ = 1.2κ0 , δ = 30. We also used the parameters κw = 0, m = 2, ρ = −2 and η = 600 Pa. All these parameters should really be chosen based on experimental results. However, we used the mentioned values and only adjusted η to match the experimental data. Details of the numerical implementation of the theory may be found in Reference [51]. The Young’s modulus and the yield stress in the diﬀerent directions, as well as their evolution are shown in Figure 2. In this ﬁgure we also compare the predicted yield stresses with the experimental data for the case of the applied load at θ = 30o to the rolling direction. Figure 3 compares experimental data and computed results for θ = 30o , 45o and 60o . Of course, diﬀerent elastic anisotropy constants (obtained experimentally) would change the predictions, but then also the material parameters η, ρ and m should be based on experimental results. An important feature of our formulation is that diﬀerent rotation rates are obtained for diﬀerent angles, and the predictions may not be symmetric for 30 and 60 degrees —in accordance with experimental results— even though the yield function is almost symmetric about the direction 44.7 degrees with the rolling direction. This is due to the selected shape for the anisotropy tensors.

8 Conclusions We presented our research towards a model for anisotropic elasto-plasticity. The model shall represent possible anisotropic elasticity, anisotropic yield surfaces, hardening and the rotation of the elastic and plastic orthotropy directions during plastic ﬂow. Both the continuum and time integration incremental formulations are simultaneously derived since incremental formulations give some insight into the continuum formulation. The model and the integration algorithm are derived using the multiplicative Lee decomposition of the total deformation gradient into an elastic and a plastic part. However, no total plas-

32

F.J. Mont´ ans and K.J. Bathe (a)

0 2.1

11

20

40

60

80

a

100

120

140

160

180

x 10 Young's modulus E [Pa]

2.09 2.08 2.07 2.06

Prediction:

2.05 2.04 2.03 2.02

120

e = 0% x e = 2% x e = 5% x ex = 10% 140

Y

(b)

Kim & Yin exp.:

Pred. & exp.

a

ex = 0% ex = 2% ex = 5% ex = 10%

x

b (c)

q

3.6 8

(RD)

x 10

Yield stress k [Pa]

3.4 3.2 3 2.8 2.6 2.4 2.2 0

20

40

60

80

a

100

120

140

160

180

Fig. 2. (a) Prediction of the evolution of the Young’s modulus proﬁle at diﬀerent spatial strains ex for a uniaxial load at an angle of θ = 30o with respect to the rolling direction (RD). (b) Angles involved in the example. Angle of the uniaxial load with the rolling direction (θ), angle of the principal direction a with the uniaxial load (β) —initially β = θ—, angle of the Young’s modulus and yield stress shown in the curves with the uniaxial load (α). (c) Comparison of the experimental data of [32] with the prediction of the evolution of the yield stress proﬁle at diﬀerent spatial strains ex for a plane stress load at an angle of θ = 30o with respect to the rolling direction

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

33

(a) 100

80 Kim & Yin experiments, q = 30º, q = 45º, q = 60º Prediction for q = 30º Prediction for q = 45º Prediction for q = 60º

b

60

40

20

0 0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

0.09

0.1

0.06

0.07

0.08

0.09

0.1 10

ex 0

0.01

0.02

0.03

0.04

0.05

3.2 8

3

3

x 10

x 10

8

tx [Pa ]

2.8

6

2.6

4 2.4

|| tw || [Pa ]

(b)

2

2.2 2

0.1

0.09

0.08

0.07

0.06

0.05

0.04

0.03

0.02

0.01

0

ex

Fig. 3. (a) Prediction for the evolution of the principal orthotropy directions and comparison with the experimental values of Reference [32]. (b) Uniaxial stress and couple-stress evolutions

tic deformation measure is used. Plastic deformations and plastic rotations are considered only incrementally. The stresses are directly obtained from the logarithmic elastic strains, with the model assuming linear elastic anisotropy and moderate elastic strains, but accounting for possible large plastic strains. The model presented oﬀers, in particular, possibilities to simulate the rotation of the material axes observed in experiments on anisotropic elasto-plastic materials, and as an example good correlation to the experimental data of Kim and Yin has been obtained. However, clearly, the model must be studied much more. The sensitivity of the model predictions with respect to the model parameters needs to be identiﬁed, and comparisons of computed solutions with test data for many more and varied material tests need to be obtained. These studies will also identify the limitations of the model and whether the model could be simpliﬁed without signiﬁcant loss of predictive capability.

34

F.J. Mont´ ans and K.J. Bathe

References 1. Koji´c M, Bathe KJ (2005) Inelastic analysis of solids and structures. SpringerVerlag, New York 2. Bathe KJ (1996) Finite element procedures. Prentice-Hall, New Jersey 3. Sim´ o JC (1988) A framework for ﬁnite strain elastoplasticity based on maximum plastic dissipation and the multiplicative decomposition. Part I: Continuum formulation. Comp Meth Appl Mech Engrng 66: 199-219. Part II: Computational aspects. Comp Meth Appl Mech Engrng 68: 1-31 4. Sim´ o JC, Hughes TJR (1998) Computational inelasticity. Springer-Verlag, New York 5. Bathe KJ, Ramm E, Wilson EL (1975) Finite element formulations for large deformation dynamic analysis. Int J Num Meth Engrg 9: 353-386 6. Koji´c M, Bathe KJ (1987) Studies of ﬁnite element procedures—Stress solution of a closed elastic strain path with stretching and shearing using the updated Lagrangian Jaumann formulation. Comp Struct 26: 175-179 7. Lee EH (1969) Elastic-plastic deformations at ﬁnite strains. J Appl Mech ASME 36: 1-6 8. Lee EH, Liu DT (1967) Finite-strain elastic-plastic theory with application to plane wave analysis. J Appl Phys 38: 19-27 9. Bilby BA, Bullough R, Smith E (1955) Continuous distributions of dislocations: A new application of the methods of Non-Riemannian Geometry. Proc Roy Soc London Ser A 231: 263-273 10. Weber G, Anand L (1990) Finite deformation constitutive equations and a time integration procedure for isotropic hyperelastic-viscoplastic solids. Comp Meth Appl Mech Engrg 79: 173-202 11. Eterovi´c AL, Bathe KJ (1990) A hyperelastic-based large strain elasto-plastic constitutive formulation with combined isotropic-kinematic hardening using the logarithmic stress and strain measures. Int J Num Meth Engrg 30: 1099-1114 12. Sim´ o JC (1992) Algorithms for multiplicative plasticity that preserve the form of the return mappings of the inﬁnitesimal theory. Comp Meth Appl Mech Engrg 99: 61-112 13. Peri´c D, de Souza EA (1999) A new model for Tresca plasticity at ﬁnite strains with an optimal parametrization in the principal space. Comp Meth Appl Mech Engrg 171: 463-489 14. Mont´ ans FJ, Bathe KJ (2003) On the stress integration in large strain elastoplasticity. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2003. Elsevier, Oxford 15. Mont´ ans FJ, Bathe KJ (2005) Computational issues in large strain elastoplasticity: An algorithm for mixed hardening and plastic spin. Int J Num Meth Engrg 63: 159-196 16. Cuiti˜ no A, Ortiz M (1992) A material-independent method for extending stress update algorithms from small strain plasticity to ﬁnite plasticity with multiplicative kinematics. Engrg Comp 9: 437-451 17. Borja RI, Tamagnini C (1998) Cam–Clay plasticity, Part III: Extension of the inﬁnitesimal model to include ﬁnite strains. Comp Meth Appl Mech Engrg 155, 77-95 18. Papadopoulus P, Lu J (1998) A general framework for the numerical solution of problems in ﬁnite elasto-plasticity. Comp Meth Appl Mech Engrg 159: 1-18

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

35

19. Car E, Oller S, O˜ nate E (2001) A large strain plasticity model for anisotropic materials—composite material application. Int J Plasticity 17: 1537-1463 20. Miehe C, Apel N, Lambrecht M (2002) Anisotropic additive plasticity in the logarithmic strain space: modular kinematic formulation and implementation based on incremental minimization principles for standard materials. Comp Meth Appl Mech Engrg 191: 5383-5426 21. Eidel B, Gruttmann F (2003) On the theory and numerics of orthotropic elastoplasticity at ﬁnite plastic strains. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2003. Elsevier, Oxford 22. Han CS, Lee MG, Chung K, Wagoner RH (2003) Integration algorithms for planar anisotropic shells with isotropic and kinematic hardening at ﬁnite strains. Comm Num Meth Engrg 19: 473-490 23. Loret B (1983) On the eﬀects of plastic rotation in the ﬁnite deformation of anisotropic elastoplastic materials. Mech Mater 2: 287-304 24. Dafalias YF (1985) The plastic spin. J Appl Mech ASME 52: 865-871 25. Dafalias YF (1990) On the microscopic origin of the plastic spin. Acta Mech 82: 31-48 26. Anand L (1983) Elasto-viscoplasticity: Constitutive modelling and deformation processing. In Teodosiu C, Raphanel JL, Sidoroﬀ F (eds) Large plastic deformations. AA Balkema, Rotterdam 27. Dafalias YF (1998) The plastic spin: necessity or redundancy? Int J Plasticity 14: 909-931 28. Kuroda M, Tvergaard V (2001) Plastic spin associated with a non-normality theory of plasticity. Eur J Mech A/Solids 20: 893-905 29. Khan AS, Huang S (1995) Continuum theory of plasticity. John Wiley & Sons, New York 30. Levitas V (1998) A new look at the problem of plastic spin based on stability analysis. J Mech Phys Solids 46: 557-590 31. Tong W, Tao H, Jiang X (2004) Modeling the rotation of orthotropic axes of sheet metals subjected to oﬀ-axis uniaxial tension. J Appl Mech ASME 71: 521-531 32. Kim KH, Yin JJ (1997) Evolution of anisotropy under plane stress. J Mech Phys Solids 45: 841-851 33. Kowalewski ZL, Sliwowski M (1997) Eﬀect of cyclic loading on the yield surface evolution of 18G2A low-alloy steel. Int J Mech Sci 39: 51-68 34. Bunge HJ, Nielsen I (1997) Experimental determination of plastic spin in polycrystalline materials. Int J Plasticity 13: 435-446 35. Truong Qui HK, Lippmann H. (2001) Plastic spin and evolution of an anisotropic yield condition. Int J Mech Sci 43: 1969-1983 36. Boheler JP, Koss S (1991) Evolution of anisotropy in sheet steels subjected fo oﬀ-axes large deformation. In Brueler O, Mannl V, Najar J (eds) Advances in continuum mechanics. Springer, Berlin 37. R.H. Randal, C. Zener (1940) Internal friction of aluminum. Phys Rev 58: 472-473 38. Tam AC, Leung WP (1984) Measurement of small elastic anisotropy in solids using laser-induced ultrasonic pulses. Appl Phys L 45: 1040-1042 39. Dvorkin EN, Goldschmit MB (2006) Nonlinear continua. Springer-Verlag, New York

36

F.J. Mont´ ans and K.J. Bathe

40. Mor´ an B, Ortiz M, Shih CF (1990) Formulation of implicit ﬁnite element methods for multiplicative ﬁnite deformation plasticity. Int J Num Meth Engrg 29: 483-514 41. Anand L (1985) Constitutive equations for hot-working of metals. Int J Plasticity 1: 213-231 42. Sim´ o JC (1986) On the computational signiﬁcance of the intermediate conﬁguration and hyperelastic relations in ﬁnite deformation elastoplasticity. Mech Mat 4: 439-451 43. Bathe KJ, Mont´ ans FJ (2004) On modelling mixed hardening in computational plasticity. Comp Struct 82: 535-539 44. Mont´ ans FJ, Bathe KJ (2005) Large strain anisotropic plasticity including effects of plastic spin. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2005. Elsevier, Oxford 45. Tsakmakis Ch (2004) Description of plastic anisotropy eﬀects at large deformations—part I: restrictions imposed by the second law and the postulate of Il’iushin. Int J Plasticity 20: 167-198 46. Eidel B, Gruttmann F (2005) Anisotropic pile-up pattern at spherical indentation into a fcc single crystal—ﬁnite element analysis versus experiment. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2005. Elsevier, Oxford 47. Han C-S, Choi Y, Lee J-K, Wagoner RH (2002) A FE formulation for elastoplastic materials with planar anisotropic yield functions and plastic spin. Int J Solids Struct 39: 5123-5141 48. Han C-S, Chung K, Wagoner RH, S-I Oh (2003) A multiplicative ﬁnite elastoplastic formulation with anisotropic yield functions. Int J Plasticity 19: 197-211 49. Luo L, Ghosh AK (2003) Elastic and inelastic recovery after plastic deformation of DQSK steel sheet. J Engrg Mater Tech ASME 125: 237-246 50. Lauwagie T, Sol H, Roebben G, Heylen W, Shi Y (2002) Validation of the Resonalyser method: an inverse method for material identiﬁcation. Proc Int Conf Noise Vibration Engrg, ISMA2002, Leuven, Belgium 51. Mont´ ans FJ, Bathe KJ (in preparation) A framework for computational large strain plasticity—anisotropic elasticity, anisotropic yield functions and mixed hardening

Localized and Diﬀuse Bifurcations in Porous Rocks Undergoing Shear Localization and Cataclastic Flow Ronaldo I. Borja Department of Civil and Environmental Engineering, Stanford University, Stanford, CA 94305, USA [email protected] Summary. Under normal temperature porous rocks can fail either by shear strain localization or cataclastic ﬂow. Shear localization results from the coalescence of microcracks leading to a tabular deformation band, whereas cataclastic ﬂow is characterized by grain crushing and pore collapse resulting in a severely damaged but macroscopically homogeneous compacted continuum. In this paper we view the two types of instability as arising from two distinct bifurcation modes. The ﬁrst mode, predicted from the singularity of the acoustic tensor, produces a strain rate jump tensor of rank one and deﬁnes a deformation band. The second mode, predicted from the singularity of the tangent constitutive operator, is diﬀuse and produces a full-rank strain rate jump tensor. After identifying the relevant bifurcation mode, we present a framework for capturing post-failure responses through constitutive branching. The post-collapse constitutive response features a cohesion softeningfriction hardening applied either to an emerging fault for shear localization or to the bulk constitutive theory for diﬀuse pore collapse instability.

1 Introduction Under normal laboratory testing conditions porous rocks tested under triaxial compression can fail either by shear strain localization or by cataclastic ﬂow [1–4]. The relevant mode of failure depends on the conﬁning pressure and temperature under which the rock sample is tested. Trends are depicted pictorially in Figs. 1 and 2 for the case of triaxial compression testing of Adamswiller sandstone (the details of the testing are given in [4]). At lower conﬁning pressures (5 and 20 MPa) the rock sample ﬁrst compacts and then dilates until it forms a well-deﬁned shear band. This is characteristic of brittle failure. The specimen tested at 40 MPa exhibits multiple bands representing transition from localized to cataclastic failure. Multiple compaction bands are not atypical at this transition pressure, with the axial strain increasing in Fig. 1 due to porosity reduction as the thickness of the compaction bands increases (Wong, personal communication). Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 37–53. © 2007 Springer. Printed in the Netherlands.

Ronaldo I. Borja

POROSITY CHANGE (%)

STRESS DIFFERENCE, MPA

38

240

150 MPa 100 MPa

180 60 MPa

120

40 MPa 20 MPa

60

5 MPa

0 0

5 MPa 20 MPa

2

40 MPa 60 MPa

4 6

100 MPa 150 MPa

8 10

0

3

6

9

12

15

AXIAL STRAIN (%)

Fig. 1. Mechanical data for Adamswiller sandstone from six triaxial compression tests under diﬀerent eﬀective pressures as indicated. Samples tested at 5 and 20 MPa failed by shear localization; sample tested at 40 MPa exhibited multiple bands; samples tested at higher conﬁning pressures failed by cataclastic ﬂow. Figure reproduced from [4]

At higher conﬁning pressures (60, 100, and 150 MPa) the sample compacts throughout as the mean normal stress increases up to a knee in the stress-strain curve (Fig. 2b), after which an accelerated volume compaction occurs with some hardening in the principal stress diﬀerence (Fig. 1) and mild increase in the mean normal stress (Fig. 2). The micromechanical processes may be considered brittle in all specimens due to the pervasive grain-scale microcracking. However, on a macroscopic scale the modes of failure may be described very diﬀerently in that shear localization manifests a brittle mode whereas cataclastic ﬂow appears much more ductile. Though not reported for this particular sandstone, Hirth and Tullis [1] observed that cataclastic ﬂow in a porous quartzite is only a transient behavior in that when the pores have collapsed any subsequent deformation could become more localized into a shear band. This typically occurs at much higher strains, of the order 25%, and subsequent volume deformation could eventually become dilative. In this paper we employ classical bifurcation analysis to predict shear localization and cataclastic ﬂow failure modes in rocks at macroscale. Shear localization is predicted from the singularity of the acoustic tensor as described by Rudnicki and Rice [5]. The upshot of the prediction is a planar band across

Localized and Diﬀuse Bifurcations

39

EFFECTIVE MEAN STRESS (MPA)

125

(a) 100

ISOTROPIC 40 MPa

75 20 MPa

50 5 MPa

25

0 −1

0

1

3

2

4

5

EFFECTIVE MEAN STRESS (MPA)

POROSITY CHANGE (%)

(b)

500 400

ISOTROPIC

300 150 MPa

200

100 MPa 60 MPa

100

0

0

2

4

6

8

10

12

14

POROSITY CHANGE (%)

Fig. 2. Shear-induced dilation and compaction in Adamswiller sandstone: (a) samples tested at 5 and 20 MPa conﬁning pressures localized in shear across a single band, sample tested at 40 MPa exhibited multiple bands; (b) samples tested at higher conﬁning pressures failed by cataclastic ﬂow. Figure reproduced from [4]

which the velocity gradient exhibits a uniform jump while the nominal traction rate vector remains continuous. In this case the jump in the velocity gradient is a rank-one tensor. Cataclastic ﬂow does not involve a deformation band, so we predict the occurrence of this mode from the singularity of the tangent constitutive operator as described by Borja [6]. In this case the jump in the velocity gradient is a full-rank tensor obtained from the condition that the nominal stress rate remain continuous. We term a full-rank velocity gradient jump tensor as diﬀuse bifurcation, in contrast to ‘global bifurcation’ as used, for example, in [7]. A comparison of rank-one and full-rank velocity gradient tensors is shown in Fig. 3.

40

Ronaldo I. Borja

ISOTROPIC IMPLOSION

STRICT IMPLOSION

IMPLOSION

ISOCHORIC MODE

PURE COMPACTION BAND

COMPACTIVE SHEAR BAND

SIMPLE SHEAR BAND

(b)

(a)

Fig. 3. Eigenmodes for bifurcations leading to pore collapse for: (a) singular tangent constitutive operator; (b) singular tangent acoustic tensor, see Reference [6]

Grain crushing and pore collapse in rocks lead to a drastically diﬀerent material. For rocks experiencing shear localization, these processes are limited to a narrow zone called deformation band [8, 9]. In cataclastic ﬂow, on the other hand, grain crushing and pore collapse are pervasive throughout the entire volume. Deformation at post-collapse is dominated by continued grain fracturing, as well as by rigid body rotation and relative translation of the fractured grains and fragments. Eﬀectively, the ‘new’ material now behaves as a dense particulate medium possessing much diﬀerent constitutive properties than those of the intact rock. In this paper we also present a framework for constitutive branching to allow the constitutive model to capture the new material properties in both shear localization and cataclastic ﬂow failure regimes. Notations and symbols used in this paper are as follows: bold-faced letters denote tensors and vectors; the symbol ‘·’ denotes an inner product of two vectors (e.g. a · b = ai bi ), or a single contraction of adjacent indices of two tensors (e.g. c · d = cij djk ); the symbol ‘:’ denotes an inner product of two second-order tensors (e.g. c : d = cij dij ), or a double contraction of adjacent indices of tensors of rank two and higher (e.g. C : e = Cijkl ekl ); the symbol ‘⊗’ denotes a juxtaposition, e.g., (a ⊗ b)ij = ai bj . Finally, for any symmetric second order tensors α and β, (α ⊗ β)ijkl = αij βkl , (α ⊕ β)ijkl = αjl βik , and (α β)ijkl = αil βjk .

2 Shear Localization 2.1 E-mode for Shear Localization The condition for shear localization is given by Aep · m = 0 ,

ep Aep ij = NA AiAjB NB ,

(1)

where Aep is the elastoplastic acoustic tensor, Aep = ∂P /∂F is the ﬁrst tangential elastoplastic moduli tensor, P is the ﬁrst Piola-Kirchhoﬀ stress

Localized and Diﬀuse Bifurcations

41

tensor, F is the deformation gradient, m is the unit vector in the direction of velocity jump across the band, and N (with component NA ) is the unit normal vector to the band in the undeformed conﬁguration, see [10]. Determining the eigenmode (e-mode) provides an insight into the volume change response at bifurcation. Let J = det(F ) > 0 denote the Jacobian of the motion, with material time derivative J˙ = Jdiv v. The jump in J˙ induced by a non-unique velocity ﬁeld is given by ˙ = J˙ − J˙∗ = J div [[v]] = J tr [[l]] = J tr([[F˙ ]] · F −1 ) . [[J]]

(2)

Accordingly, we characterize the appropriate volume change mode from the following criteria: ˙ = (−) =⇒ contraction/implosion; sgn [[J]] (3) (+) =⇒ dilation/explosion. ˙ = 0 denotes an isochoric mode. The transition condition [[J]] For condition (1) to provide a non-trivial solution we must have inf{D(N ) ∈ |D(N ) = det(Aep )} = 0 ,

(4)

where we view the ﬁeld of determinants of Aep as a set function of N and we want the inﬁmum of this set to vanish at a critical orientation deﬁned by the band normal N . At this critical orientation the tensor Aep is singular and the vector m deﬁnes its e-mode. We determine the correct algebraic sign of this e-mode from the conditions described in [9, 10]. For shear localization the form of the jump tensor [[F˙ ]] is given by [[F˙ ]] = ϕm ⊗ N ,

(5)

where ϕ denotes the magnitude of the jump. Noting from Nanson’s formula that (6) n = (h/h0 )N · F −1 , where h and h0 are the band thicknesses in the deformed and undeformed conﬁgurations, respectively, then we get ˙ =J [[J]]

h h tr(m ⊗ n) = J (m · n) . h0 h0

(7)

The shear band mode is then classiﬁed as either compactive or dilative depending on the sign of the vector dot product m · n. Following [9], we classify a deformation band according to the following criteria: ⎧ ⎪ m·n=1: pure dilation band; ⎪ ⎪ ⎪ ⎪ ⎪0 < m · n < 1 : dilatant shear band; ⎨ (8) m·n=0: simple shear band; ⎪ ⎪ ⎪ −1 < m · n < 0 : compactive shear band; ⎪ ⎪ ⎪ ⎩m · n = −1 : pure compaction band.

42

Ronaldo I. Borja

Note that the above deﬁnitions only pertain to the speciﬁc mode at bifurcation. 2.2 Constitutive Branching for Shear Localization Slip weakening, a process describing the mechanical response of rocks from the onset of shear localization to the beginning of the residual state, provides a critical link between pre-localization and residual state behaviors. Developing a constitutive framework for this initial stage of slip instability requires knowledge of the residual state to which the slip weakening model will branch. For a shear band that is deforming by tangential frictional sliding we consider the classical Mohr-Coulomb friction law formulated in the Lagrangian description. Following [11], we take the nominal traction vector at material point X on the band as t = P · N , where N deﬁnes the unit band normal in the reference conﬁguration (determined from the bifurcation analysis). We can resolve this traction into normal and tangential components at the current conﬁguration as (9) t(X, t) = tN (X, t)n + tT (X, t)ξ , where n = N · F −1 /N · F −1 , and tN and tT are normal and tangential components obtained from tN = n · P · N ,

tT = tT ,

ξ = tT /tT ,

tT = t − t N n ,

(10)

assuming planar sliding (some metric transformation may be required for sliding along curvilinear surfaces). Note that tN (negative for compression) and tT are resolved nominal stresses representing forces in the current conﬁguration per unit undeformed area. Next we write the Mohr-Coulomb friction law at residual state using the format of classical plasticity. Let µ denote the coeﬃcient of friction; then we have ˙ , [[v]] = ζξ ζ˙ ≥ 0 , Φζ˙ = 0 . (11) Φ = tT + µtN ≤ 0 , In the above expressions Φ takes the role of the yield function at residual state, [[v]] is the velocity jump across the band (evaluated from a non-associative ﬂow rule), ζ˙ is the nonnegative slip rate, and the fourth expression is the ˙ = J tr[[l]] = 0, since Kuhn-Tucker condition. The band kinematics yields [[J]] [[v]] · n = 0 for a band that moves by tangential sliding. Furthermore, the ﬂow rule suggests that the velocity jump [[v]] across the band is fully plastic, consistent with results obtained for strong discontinuity kinematics [12, 13]. We can also accommodate a variable coeﬃcient of friction with this framework. For small slips and slow slip velocities the variation of the coeﬃcient of friction µ may be described by the Dieterich-Ruina law [14–16] ˙ ∗ ) + B ln(θ/θ∗ ) µ = µ∗ + A ln(ζ/V ˙ c, θ˙ = 1 − θζ/D

(12) (13)

Localized and Diﬀuse Bifurcations

43

where ζ˙ is the magnitude of [[v]], θ is a state variable, and A, B, µ∗ , V ∗ , θ∗ , and Dc are material parameters. The state variable θ has been linked to the changing set of frictional contacts and wear on the materials [16], and Dc is a characteristic slip required to replace a contact population representative of a previous sliding condition with a contact population created under a new sliding condition. For zero and near-zero slip velocities, such as what occurs near the tip of a nucleating fault, the expression for µ as given by the above logarithmic function becomes singular. To circumvent this problem we view frictional sliding as a rate process and add backward jumps in the spirit of the Arrhenius law to obtain the regularized form [17] µ = A sinh−1

ζ˙ µ∗ + B ln(θ/θ∗ ) . exp ∗ 2V A

(14)

This equation then predicts a zero coeﬃcient of friction at zero slip velocity. The above variable friction model has been implemented in the context of strong discontinuity ﬁnite elements [18, 19]. Note that for large slips and high slip velocities, such as those encountered in earthquake fault nucleation

(a)

(b)

(c) Fig. 4. Model for fault nucleation and propagation in rock: (a) fault nucleates (dashed line) over a characteristic distance; (b) slip weakening takes place over characteristic slip ζ ∗ ; (c) initially dilatant shear band becomes isochoric over a characteristic slip ζ

44

Ronaldo I. Borja (a)

(b)

Fig. 5. Slip weakening models for rocks during fault nucleation: (a) linear slip weakening resulting from a combined cohesion softening-friction hardening on an emerging fault; (b) nonlinear slip weakening. Shaded area GII represents shear fracture energy that has been correlated with the magnitude of an earthquake for regionalscale faulting, see [20]

processes, a much lower coeﬃcient of friction may be activated by additional weakening mechanisms such as ﬂash heating [17]. The concept of slip weakening leading to the above rate- and statedependent residual friction model was motivated by the cohesive zone models for tensile fracture and extended to the shear fracture problem by Ida [20] and Palmer and Rice [21]. To better understand this process we consider a rock through which a shear band (or fault) is nucleating and propagating, as shown in Fig. 4. At the bifurcation point we assume that slip begins to accumulate, as deﬁned by the integral

(15) ζ = ζ˙ dt , t

where the integration is taken over the slip path, see Fig. 4a. Figure 4b shows the resolved nominal shear stress tT decaying to a residual state value away from the tip of a propagating band, where the cumulative slip ζ has exceeded a value ζ ∗ ≈ 0.5 mm for most rocks (Rice, personal communication, see also [22]). Figure 5 further depicts this narrow region of slip weakening [20], in which tT decreases either linearly or nonlinearly with ζ (Figs. 5a and 5b, respectively). The shaded area GII represents the shear fracture energy that has been correlated by many authors with the magnitude of an earthquake. Figure 6 portrays the notion of constitutive branching during slip weakening in the context of classical elastoplasticity. Prior to bifurcation, plastic deformation of an intact rock is described by the yield function F = 0, which is assumed isotropic on the π-plane and dependent on all three principal Kirchhoﬀ stresses. A deformation band-type bifurcation is detected at point A, and consequently the constitutive theory branches to the slip weakening law Φ = tT − c + µtN = 0 .

(16)

Localized and Diﬀuse Bifurcations

45

A

B

Fig. 6. Slip weakening on the π-plane in principal Kirchhoﬀ stress space. Yield surface for intact rock F = 0 branches at the bifurcation stress point A to the Mohr-Coulomb failure criterion Φ = 0 for a planar fault; at residual state B the cohesion decays to zero and the failure criterion passes through the origin

This equation plots as a straight line on the π-plane. However, the slip velocity is zero at the bifurcation point, so µ = 0 initially, and the shear resistance is then purely cohesive. As slip accumulates the coeﬃcient of friction µ quickly increases while the cohesion c decays to zero. During this time tN may also vary, and the slip weakening law then plots as a fan of straight lines on the π-plane. At the conclusion of slip weakening the cohesion is zero and the shear resistance is purely frictional; hence, the straight line passes through the origin of the π-plane. This interplay between the cohesive and frictional resistances is also shown in Fig. 5a. Assuming the shear resistance on the band is purely frictional and the slipweakening constitutive law is linear, we can write an ‘eﬀective yield function’ of the form ζ ζ ∈ [ 0, ζ ∗ ] , (17) Φ = tT − t◦T − (t◦T + µt∗N ) ∗ ≤ 0 , ζ where Φ = 0 now describes a linear slip weakening. However, the condition Φ = 0 is not a trivial linear constraint to impose since t∗N is unknown during the slip weakening process. A ﬁrst-order approximation may be obtained by assuming t∗N ≈ tN [18], in which case (17) reduces to the form ζ Φ = tT − t◦T − (t◦T + µtN ) ∗ ≤ 0 , ζ

ζ ∈ [ 0, ζ ∗ ] .

(18)

This equation predicts a nonlinear slip weakening similar to Fig. 5b for the case of a variable tN , and recovers a linear slip weakening for the case of a constant tN , see [18, 19] for further details.

46

Ronaldo I. Borja

3 Cataclastic Flow 3.1 E-mode for Cataclastic Flow The condition for stationary stress rate is given by [[P˙ ]] = Aep : [[F˙ ]] = 0 .

(19)

For a non-trivial solution [[F˙ ]] = 0 to exist, we must have det(Aep ) = 0 .

(20)

The e-mode in this case is the jump tensor [[F˙ ]]. Borja [6] provides details on how the correct sign of this e-mode may be determined. To further characterize the e-mode associated with condition (19), we write τ = P · Ft ,

(21)

where τ is the symmetric Kirchhoﬀ stress tensor. Taking the jumps in the rates gives (22) [[τ˙ ]] = P · [[F˙ ]]t + [[P˙ ]] · F t . Noting that [[P˙ ]] = 0 and [[F˙ ]] = [[l]] · F at bifurcation, we get [[τ˙ ]] = (τ 1) : [[l]] ,

(23)

where (τ 1)ijkl = τil δjk and δjk is the Kronecker delta. Now, consider a rate constitutive equation of the form [10] τ˙ = αep : l ,

(24)

where αep is a rank-four spatial elastoplastic tangential moduli tensor with minor symmetry on its ﬁrst two indices. This yields an eigenvalue problem aep : [[l]] = 0 ,

aep = αep − τ 1 .

(25)

Thus, Aep is singular whenever aep is singular. The singularity of aep is of three types [23], and here we shall consider only the one relevant to pore collapse instability. We recall the polar decomposition of the deformation gradient F and spectral decomposition of the left stretch tensor V , 3 λA m(A) , (26) F = V ·R, V = A=1 (A)

(A)

(A)

where m = n ⊗ n , R is a proper orthogonal rotation tensor, λA are the principal stretches, and n(A) are the principal directions of V . Taking the time derivative gives ˙ , F˙ = V˙ · R + V · R (27)

Localized and Diﬀuse Bifurcations

where V˙ =

3

λ˙ A m(A) +

A=1

3

ωAB (λB − λA )m(AB) ,

47

(28)

A=1 B=A

m(AB) = n(A) ⊗ n(B) , and ωAB is the spin of the (Eulerian) principal axes of V. The velocity gradient can be expressed in the form l = F˙ · F −1 = V˙ · V −1 + V · Ω · V −1 ,

˙ · Rt . Ω=R

(29)

Using the spectral forms and taking the jumps gives [[l]] =

3

[[ε˙A ]]m(A)

(30)

A=1

+

3 λA (AB) λA , + [[wAB ]] m [[ωAB ]] 1 − λB λB

(31)

A=1 B=A

where wAB = Ω : m(AB) and εA = ln λA is the principal logarithmic stretch. Note that wAB arises from the ﬁnite rotation of the stretch tensor V whereas ωAB describes the spin of the principal axes of V ; the former vanishes in the inﬁnitesimal theory whereas the latter generally does not. The particular e-mode of interest is characterized by [[ωAB ]] = [[wAB ]] = 0, where the volume simply implodes at ﬁxed principal directions. In this case the jump in the velocity gradient [[l]] is equal to the jump in the rate of deformation [[d]] (since the spins are ‘frozen’), and the relevant jump tensor becomes 3 [[ε˙A ]]m(A) . (32) [[l]] = [[d]] = A=1

By a simple tensor manipulation the jumps in the principal logarithmic stretch rates, characterizing the e-mode at bifurcation, may be obtained from the eigenvalue problem 3 aep (33) AB [[ε˙B ]] = 0 , A=1

where

(A) aep : aep : m(B) AB = m

(34)

is a 3 × 3 matrix of elastoplastic moduli, which also includes the initial stress terms arising from ﬁnite deformation eﬀects. Pore collapse is characterized by the condition 3 [[ε˙A ]] < 0 . (35) A=1

Note that the e-mode predicted above is diﬀuse in the sense that it does not entail the formation of a deformation band.

48

Ronaldo I. Borja

3.2 Constitutive Branching for Cataclastic Flow As in classical continuum plasticity we consider yield and plastic potential functions, Φ and Ψ , respectively, representing yield behavior of the compacted material at the conclusion of cataclastic ﬂow. We assume that these functions depend on the Kirchhoﬀ stress tensor τ and some plastic internal variable κ. By multiplicative plasticity we write the velocity gradient as the sum of elastic and plastic parts, (36) l = le + lp , where and

le = F˙ e · F e−1 p Lp = F˙ · F p−1 .

lp = F e · Lp · F e−1 , p

(37)

p

(38)

p

Ignoring plastic spin, we have l = sym(l ) := d , and the ﬂow rule thus gives ˙ , dp = λq

q=

∂Ψ . ∂τ

(39)

Φ(τ , κ)λ˙ = 0 ,

(40)

Subject to the usual Kuhn-Tucker conditions Φ(τ , κ) ≤ 0 ,

λ˙ ≥ 0 ,

along with an appropriate hardening law, we have thus formulated a constitutive model appropriate for the ‘new’ material at post-cataclasis. It has been reported [1] that cataclastic ﬂow is only a transient behavior. When the pores have collapsed and the compacted material is loaded further, any subsequent deformation could result in a net dilatancy leading to strain localization. For porous quartzite this occurs at nominal axial strains greater than about 25%. This suggests that constitutive models for a porous but intact rock, initially exhibiting compactive tendencies, should branch to a model exhibiting dilative tendencies at the conclusion of cataclastic ﬂow. During this time the eﬀective cohesion exhibited by the intact rock decays to a near-zero value while the eﬀective frictional strength increases with increased compaction. Interestingly, these features are analogs of those encountered in the development of the slip weakening model of the previous section, with the exception that they now apply to the bulk response of the material. For a more concrete illustration, we assume the following form of the yield function to which the constitutive response branches at the onset of cataclastic ﬂow: f1 = I 13 /I 3 , (41) Φ = (f1 − 27)(I 1 /pa )m − κ ≤ 0 , where I1 = τ 1 + τ 2 + τ 3 ,

I 3 = τ 1τ 2τ 3

(42)

Localized and Diﬀuse Bifurcations

49

q

p A

B Fig. 7. Yield surface for intact rock F = 0 branches at the bifurcation stress point A into yield surface Φ(τ , κ) = 0 signifying onset of cataclastic ﬂow. Post-bifurcation yield surface undergoes cohesion softening-friction hardening. Transient cataclastic ﬂow concludes at stress point B where the compacted continuum can now potentially undergo shear localization with plastic dilatancy

are, respectively, the ﬁrst and third invariants of the translated principal Kirchhoﬀ stresses τ 1 = τ1 − a ,

τ 2 = τ2 − a ,

τ 3 = τ3 − a ,

(43)

a > 0 is a stress shift on the hydrostatic axis to account for cohesion, and pa is the atmospheric pressure (a normalizing constant). The exponent m is a given parameter describing the curvature of the surface on a meridian plane (straight line for m = 0), and κ is the slope that varies with the frictional yield strength. Lade [24] utilizes this function to characterize yielding of dense sands. The yield function described above has the shape of an asymmetric bullet with the pointed apex initially on the tensile side of the hydrostatic axis (Fig. 7) and initially coinciding with the apex of the yield surface for the intact rock, which is represented in the same ﬁgure by the boundary of the region with a compression cap. Cataclastic ﬂow-type bifurcation occurs at point A, and by requiring that Φ = 0 for this given stress state we obtain the initial value κ0 of the frictional parameter κ. Cohesion softening during cataclastic ﬂow is simulated by a degrading value of a, while friction hardening is captured by an increasing value of κ.

4 Transient Plastic Flow During slip weakening and cataclastic ﬂow, the directions of plastic ﬂow evolve from those predicted at bifurcation to those attained at residual state. To capture the evolution during these ‘transient’ conditions we can interpolate these

50

Ronaldo I. Borja

plastic ﬂow directions to satisfy the initial (bifurcation) and ﬁnal (residual) states. 4.1 Slip Weakening The region of interest is 0 ≤ ζ ≤ ζ , as shown in Fig. 4c. Inside this region the velocity jump [[v]] evolves from being parallel to m at bifurcation to being parallel to ξ when the fault begins to deform by pure tangential sliding. Interpolating linearly with ζ (as a ﬁrst-order approximation), we get ˙ ⊗N, [[F˙ ]] = ζb

(44)

where

ζ ζ β , β = 1 − m + ξ. β ζ ζ The corresponding jump in velocity gradient is b=

h0 [[l]] = [[F˙ ]] · F −1 = ζ˙ b ⊗ n . h It follows that the jump in the Jacobian rate is ˙ = Jtr[[l]] = ζ˙ J h0 1 − ζ m · n . [[J]] β h ζ

(45)

(46)

(47)

˙ = 0 when ζ = ζ , so at this level of deformation any initial This yields [[J]] dilation or compaction of the band will cease and subsequent motion will be characterized by pure tangential sliding. 4.2 Cataclastic Flow The region of interest is J1 ≤ J ≤ J0 , where J0 is the value of the Jacobian at the bifurcation point and J1 is the value at the conclusion of cataclastic ﬂow. It is ﬁtting that in this case we select J as our parameter since we are concerned with pore collapse instability and J is a measure of volume change. At the bifurcation stress we take the e-mode as the instantaneous plastic ﬂow direction, 3 p ˙ [[ε˙A ]]m(A) , J = J0 . (48) d0 = λ A=1

At the conclusion of cataclastic ﬂow the plastic ﬂow direction is given by the ﬂow rule ∂Ψ , J = J1 . (49) dp1 = λ˙ ∂τ A linear interpolation gives dp =

J − J1 p J0 − J p d + d , J0 − J1 0 J0 − J1 1

J1 ≤ J ≤ J0 .

(50)

Localized and Diﬀuse Bifurcations

51

Of course, other forms of interpolation are possible provided they satisfy the two end conditions. We emphasize that both slip weakening and cataclastic ﬂow are micromechanical processes. The plastic ﬂow theory presented in this section should thus be interpreted simply as a rough approximation of the micromechanical phenomena and not as a faithful description of the grain-scale ﬂow processes taking place during these transient periods of instability.

5 Closure We have presented a framework for mathematical modeling of shear localization and cataclastic ﬂow in porous rocks. Classical bifurcation theory provides conditions for the occurrence of these two instability modes, in which shear localization is equated to a singular acoustic tensor whereas cataclastic ﬂow is equated to a singular tangent constitutive operator. For general 3D kinematics, the corresponding e-modes are given by velocity gradient jump tensors of ranks one and three, respectively. We have also proposed a framework for constitutive branching to allow the model to capture post-bifurcation responses. Slip weakening provides a critical link to modeling post-shear localization in rocks. The process is captured by a cohesion softening-friction hardening law applied to the nucleating fault plane. A similar cohesion softening-friction hardening law has been proposed for bifurcation leading to cataclastic ﬂow, except that the law is applied to the bulk constitutive response.

Acknowledgements The author is grateful to Professor James R. Rice of Harvard University and Professor Teng-fong Wong of State University of New York at Stony Brook for discussions on the basic issues of slip weakening and cataclastic ﬂow addressed in this paper, as well as for providing numerous references relevant to this work. Discussions with Professors David Pollard and Atilla Aydin of Stanford University also helped elucidate the processes and mechanisms of rock deformation addressed in this work. Graduate student Joshua White assisted in the preparation of the manuscript. This work has been supported in part by the U.S. National Science Foundation, Grant No. CMG-0417521 (Collaborations in Mathematical Geosciences) and the U.S. Department of Energy Grant No. DE-FG02-03ER15454.

References [1] Hirth G, Tullis J (1989) The eﬀects of pressure and porosity on the micromechanics of the brittle-ductile transition in quartzite. Journal of Geophysical Research 94:17825–17838

52

Ronaldo I. Borja

[2] Men´endez B, Zhu W, Wong TF (1996) Micromechanics of brittle faulting and cataclastic ﬂow in Berea sandstone. Journal of Structural Geology 18:1–16 [3] Tullis J, Yund R (1992) The brittle-ductile transition in feldspar aggregates: An experimental study. In B. Evans and T.F. Wong, editors, Fault mechanics and transport properties of rocks. Cambridge University Press, United Kingdom, [4] Wong TF, David C, Zhu W (1997). The transition from brittle faulting to cataclastic ﬂow in porous sandstones: Mechanical deformation. Journal of Geophysical Research 102:3009–3025 [5] Rudnicki JW, Rice JR (1975) Conditions for localization of deformation in pressure-sensitive dilatant materials. Journal of the Mechanics and Physics of Solids 23:371394 [6] Borja RI (2006) Conditions for instabilities in collapsible solids including volume implosion and compaction banding. Acta Geotechnica, in press [7] Chau K, Rudnicki JW (1990) Bifurcations of compressible pressuresensitive materials in plane strain tension and compression. Journal of the Mechanics and Physics of Solids 38:875–898 [8] Aydin A, Borja RI, Eichnubl P (2006) Geological and mathematical framework for failure modes in granular rock. Journal of Structural Geology 28:83–98 [9] Borja RI, Aydin A (2004) Computational modeling of deformation bands in granular media. I. Geological and mathematical framework. Computer Methods in Applied Mechanics and Engineering 193:26672698 [10] Borja RI (2002) Bifurcation of elastoplastic solids to shear band mode at ﬁnite strains. Computer Methods in Applied Mechanics and Engineering 191:52875314 [11] Laursen TA, Simo JC (1993) A continuum-based ﬁnite element formulation for the implicit solution of multibody, large deformation frictional contact problems. International Journal for Numerical Methods in Engineering 36:3451-3485 [12] Borja RI (2000) A ﬁnite element model for strain localization analysis of strongly discontinuous ﬁelds based on standard Galerkin approximations. Computer Methods in Applied Mechanics and Engineering 190:1529–1549 [13] Borja RI (2002) Finite element simulation of strain localization with large deformation: Capturing strong discontinuity using a Petrov-Galerkin multiscale formulation. Computer Methods in Applied Mechanics and Engineering 191:2949–2978 [14] Dieterich JH (1979) Modeling of rock friction 1. Experimental results and constitutive equations. Journal of Geophysical Research 84:2161–2168 [15] Ruina AL (1983) Slip instability and state variable friction laws. Journal of Geophysical Research 88:10359–10370

Localized and Diﬀuse Bifurcations

53

[16] Dieterich JH, Kilgore BD (1996) Imaging surface contacts: Power law contact distributions and contact stresses in quartz, calcite, glass and acrylic plastic. Tectonophysics 256:219–239 [17] Lapusta N, Rice JR, Ben-Zion Y, Zheng G (2000) Elastodynamic analysis for slow tectonic loading with spontaneous rupture episodes on faults with rate- and state-dependent friction. Journal of Geophysical Research 105:23765–23789 [18] Borja RI, Foster CD (2006) Continuum mathematical modeling of slip weakening in geological systems. Journal of Geophysical Research, in review. [19] Foster CD, Borja RI, Regueiro RA (2006) Embedded strong discontinuity ﬁnite elements for fractured geomaterials with variable friction. International Journal for Numerical Methods in Engineering, in review. [20] Ida Y (1972) Cohesive force across the tip of a longitudinal shear crack and Griﬃth’s speciﬁc surface energy. Journal of Geophysical Research 77:3796–3805 [21] Palmer AC, Rice JR (1973) The growth of slip surfaces in the progressive failure of overconsolidated clay. In Proceedings of the Royal Society of London Ser. A332, pp. 527–548 [22] Wong TF (1982) Shear fracture energy of Westerly granite from postfailure behavior. Journal of Geophysical Research 87:990–1000 [23] Ogden RW (1984) Nonlinear Elastic Deformations. Chichester, Ellis Horwood [24] Lade PV (1977) Elasto-plastic stress-strain theory for cohesionless soil with curved yield surfaces. International Journal of Solids and Structures 13:1019–1035

Dispersion and Localisation in a Strain–Softening Two–Phase Medium Ren´e de Borst1,2 and Marie-Ang`ele Abellan3 1

2 3

Delft University of Technology, Faculty of Aerospace Engineering, Kluyverweg 1, Delft, The Netherlands [email protected] LaMCoS, UMR CNRS 5514, INSA de Lyon, 69621 Villeurbanne, France LTDS-ENISE, UMR CNRS 5513, ENISE, 42023 Saint-Etienne, France

Summary. In fluid–saturated media wave propagation is dispersive, but the associated internal length scale vanishes in the short wave–length limit. Accordingly, upon the introduction of softening, localisation in a zero width will occur and no regularisation is present. This observation is corroborated by numerical analyses of wave propagation in a finite one–dimensional bar.

1 Introduction Strain softening and the ensuing phenomenon of localisation have been the subject of profound investigations in the past two decades. While, initially, the incorporation of strain softening in constitutive equations was considered to be a straightforward exercise, it soon appeared that the use of strain-softening models led to an excessive dependency of the solution on the discretisation in numerical analyses. At ﬁrst, deﬁciencies in the numerical methods were believed to cause this severe mesh dependency. However, it was demonstrated that the underlying cause was the local change of character of the partial diﬀerential equations that govern the initial/boundary value problem: from elliptic to hyperbolic for quasi–static problems and from hyperbolic to elliptic in dynamic problems. This local change of character renders the initial/boundary value ill–posed, unless special interface conditions are imposed between both regimes. For ill–posed problems, numerical methods, including ﬁnite element methods, still try to capture ‘the best possible’ solution, but this solution changes for every other discretisation. To repair this ill–posedness, several proposals have been put forward. Invariably, the aim is to enrich the continuum description to include more of the underlying physical properties of the material, such as grain rotations in granular materials — the Cosserat continuum approach, e.g. [1, 2] —, the incorporation of viscosity or rate–dependency, e.g. [3, 4], or nonlocal approaches which reﬂect medium and long–range forces which emerge in materials where Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 55–66. © 2007 Springer. Printed in the Netherlands.

56

Ren´e de Borst and Marie-Ang`ele Abellan

the heterogeneity is in the same order of magnitude as the fracture process zone [5, 6, 7, 8]. While these ideas have been suggested and elaborated for single–phase media, they are also eﬀective for multi–phase media, such as ﬂuid–saturated porous solids, e.g. [9]. The question has arisen whether the diﬀusive character of the movement of the ﬂuid in such a medium already provides a physically based regularisation mechanics. Indeed, it has already been shown by Biot [10], see also Loret and co-workers [11, 12] that wave propagation in such a medium is dispersive, and, accordingly, that an internal length scale must exist. This issue has been debated intensely in recent years [13, 14, 15, 16, 17]. In a previous contribution [17], we have demonstrated that stability in a ‘standard’ two–phase medium is assured until the tangent modulus ceases to be positive, at least in a one–dimensional medium and for a normal range of material parameters. Thus, the stability condition coincides with that of a single–phase medium. Moreover, it was shown by an analysis of dispersive waves that the length scale associated with wave dispersion vanishes in the short wave–length limit. In this contribution, we supplement the previous analysis by a more comprehensive study in which the momentum balance in the ﬂuid is kept explicitly in the analysis, which enables the identiﬁcation of the second wave speed in the mixture. The main conclusion of the previous study, namely that the length scale associated with wave dispersion vanishes in the short wave–length limit, so that no regularisation exists, is corroborated by the present analysis, and therefore put on a solid basis.

2 Governing Equations We consider a two–phase medium subject to the restriction of small displacement gradients and small variations in the concentrations [18]. Furthermore, the assumptions are made that there is no mass transfer between the constituents and that the processes which we consider, occur isothermally. With these assumptions, the balances of linear momentum for the solid and the ﬂuid phases read: ˆ π + ρπ g = ∇ · σπ + p

∂(ρπ vπ ) + ∇(ρπ vπ ⊗ vπ ) ∂t

(1)

with σ π the stress tensor, ρπ the apparent mass density, and vπ the absolute velocity of constituent π. As in the remainder of this paper, π = s, f , with s and f denoting the solid and ﬂuid phases, respectively. Further, g is the ˆ π is the source of momentum for constituent π gravity acceleration and p from the other constituent, which takes into account the possible local drag interaction between the solid and the ﬂuid. Evidently, the latter source terms must satisfy the momentum production constraint: ˆπ = 0 (2) p π=s,f

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

57

We now neglect convective terms and the gravity acceleration, so that the momentum balances reduce to: ˆ π = ρπ ∇ · σπ + p

∂vπ ∂t

(3)

Adding both momentum balances, and taking into account Eq.(2), one obtains the momentum balance for the mixture: ∇ · σ s + ∇ · σ f − ρs

∂vs ∂vf − ρf =0 ∂t ∂t

(4)

where σ f = −αpI

(5)

with p the ﬂuid pressure, I the second–order identity tensor, and α the Biot coeﬃcient, cf. [19]. Substitution of Eq.(5) into the momentum balance of the mixture gives: ∂vs ∂vf − ρf =0 (6) ∇ · σ s − α∇p − ρs ∂t ∂t In a similar fashion as for the balances of momentum, one can write the balance of mass for each phase as: ∂ρπ + ∇ · (ρπ vπ ) = 0 ∂t

(7)

Again neglecting convective terms, the mass balances can be simpliﬁed to give: ∂ρπ + ρπ ∇ · vπ = 0 (8) ∂t We multiply the mass balance for each constituent π by its volumic ratio nπ , add them and utilise the constraint nπ = 1 (9) π=s,f

to give: ∇ · vs + nf ∇ · (vf − vs ) +

nf ∂ρf ns ∂ρs + =0 ρs ∂t ρf ∂t

(10)

The change in the mass density of the solid material is related to its volume change by: Ks nf ∂ρs (11) ∇ · vs = − Kt ρs ∂t with Ks the bulk modulus of the solid material and Kt the overall bulk modulus of the porous medium. Using the deﬁnition of the Biot coeﬃcient, 1 − α = Kt /Ks [19], this equation can be rewritten as (α − 1)∇ · vs =

nf ∂ρs ρs ∂t

(12)

58

Ren´e de Borst and Marie-Ang`ele Abellan

For the ﬂuid phase, a phenomenological relation is assumed between the incremental changes of the apparent ﬂuid mass density and of the ﬂuid pressure [19]: nf 1 dp = dρf (13) Q ρf with the overall compressibility, or Biot modulus α − nf 1 nf = + Q Ks Kf

(14)

where Kf is the bulk modulus of the ﬂuid. Inserting relations (12) and (13) into the balance of mass of the total medium, Eq.(10), gives: α∇ · vs + nf ∇ · (vf − vs ) +

1 ∂p =0 Q ∂t

(15)

The governing equations, i.e. the balance of momentum of the saturated medium, Eq.(6), that of the ﬂuid, Eq.(3) with π = f , and the balance of mass, Eq.(15), are complemented by the kinematic relation, s = ∇s us

(16)

with us , s the displacement and strain ﬁelds of the solid, respectively, the superscript s denoting the symmetric part of the gradient operator, and an incrementally linear stress–strain relation for the solid skeleton, σ˙ s = Dtan : ˙ s

(17)

tan

where D is the fourth–order tangent stiﬀness tensor of the solid material and the superimposed dot denotes diﬀerentiation with respect to a virtual time. For the pore ﬂuid ﬂow, Darcy’s relation for isotropic media is assumed to hold, (18) nf (vf − vs ) = −kf ∇p with kf the permeability coeﬃcient of the porous medium, and deﬁnes the drag force of the solid on the ﬂuid: ˆ f = −nf kf−1 (vf − vs ) p

(19)

The boundary conditions nΓ · σ = tp ,

v = vp

(20)

hold on complementary parts of the boundary ∂Ωt and ∂Ωv , with Γ = ∂Ω = ∂Ωt ∪ ∂Ωv , ∂Ωt ∩ ∂Ωv = ∅, tp being the prescribed external traction and vp the prescribed velocity, and nf (vf − vs ) = qp ,

p = pp

(21)

hold on complementary parts of the boundary ∂Ωq and ∂Ωp , with Γ = ∂Ω = ∂Ωq ∪ ∂Ωp and ∂Ωq ∩ ∂Ωp = ∅, qp and pp being the prescribed outﬂow of pore ﬂuid and the prescribed pressure, respectively.

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

59

3 Reduction of the Governing Equations Henceforth, we shall consider the problem of a uniaxially stressed homogeneous bar. Then, vsx = 0, vsy = 0, vsz = 0 and the momentum balances for the mixture and for the ﬂuid reduce to: ∂p ∂σs ∂vs ∂vf −α − ρs − ρf =0 (22) ∂x ∂x ∂t ∂t where for notational simplicity the subscript x has been dropped and σs denotes the axial stress in the solid, and ∂p ∂vf + nf kf−1 (vf − vs ) + ρf =0 (23) ∂x ∂t respectively. From Eq.(23) we observe that Eq.(19) has been used as the source of momentum for the ﬂuid from the solid phase. The mass balance of the mixture, Eq.(15) becomes: ∂vs ∂p ∂vs ∂vf + nf − + Q−1 =0 (24) α ∂x ∂x ∂x ∂t α

To allow for inelastic constitutive equations, we take the incremental format of Eqs.(22)–(24): ∂ p˙ ∂ v˙ s ∂ v˙ f ∂ σ˙ s −α − ρs − ρf =0 (25) ∂x ∂x ∂t ∂t ∂ p˙ ∂ v˙ f + nf kf−1 (v˙ f − v˙ s ) + ρf =0 (26) α ∂x ∂t and ∂ v˙ s ∂ v˙ s ∂ p˙ ∂ v˙ f α + nf − + Q−1 =0 (27) ∂x ∂x ∂x ∂t We will observe in the next section, where, using an analysis of wave dispersion in this medium, the localisation properties are derived, that the ensuing equations are rather complicated. For this reason, in [17] the pressure p was eliminated from the above equations by inserting Darcy’s relation explicitly in the balances of momentum and mass for the mixture. For the momentum balance this results in: ∂vs ∂vf ∂σs + αnf kf−1 (vf − vs ) − ρs − ρf =0 (28) ∂x ∂t ∂t The mass balance, Eq.(24) is ﬁrst diﬀerentiated with respect to x. Interchanging the order of spatial and temporal diﬀerentiation and inserting Darcy’s relation then results in: 2 ∂vs ∂ 2 vs ∂ 2 vs ∂ vf ∂vf −1 − =0 (29) − n α 2 + nf − (k Q) f f ∂x ∂x2 ∂x2 ∂t ∂t The above two equations solely have the velocity in the solid, vs , and that in the ﬂuid, vf , as unknowns. They are better amenable to analytical manipulations. However, the reduction to two equations makes that the velocity of the wave in the ﬂuid is no longer contained in the set of equations.

60

Ren´e de Borst and Marie-Ang`ele Abellan

4 Dispersion Analysis In a strain–softening medium the presence of a non-vanishing internal length scale that arises from physical properties of the system, is directly related to the well–posedness of the initial value problem. A method for the quantiﬁcation of this internal length scale is to investigate the dispersive properties of wave propagation. Wave propagation is called dispersive when harmonics propagate with diﬀerent velocities [20]. Since a wave is composed of diﬀerent harmonics, the shape of a dispersive wave can then change upon propagation. The ability to transform the shape of waves is a necessary condition for continua to properly capture localisation phenomena, since it is otherwise impossible that the shape of an arbitrary loading wave is changed into a stationary wave with for instance a sinusoidal shape in the localisation zone. On the other hand, dispersivity of loading waves in a strain–softening medium is not a suﬃcient condition for localisation to be captured in a zone of ﬁnite size, and thus, for the initial value problem to be regularised. As said, such a regularisation will only be present if, in addition to dispersivity, a non-vanishing internal length scale can be identiﬁed. To analyse the characteristics of wave propagation in the two–phase medium, a damped, harmonic wave is considered: ⎞ ⎛ ⎞ ⎛ As δ u˙ s ⎝ δ u˙ f ⎠ = ⎝ Af ⎠ exp (ikx + λt) (30) δ p˙ Ap where As , Af , Ap are the amplitudes of the perturbations for the displacement ˙ respectively, rates in the solid, u˙ s , in the ﬂuid, u˙ f , and for the pressure rate, p, while k is the wave number. The eigenvalue λ = λr −iω can have a real component λr , which characterises the damping properties of the propagating wave, and an imaginary component ω, which is the angular frequency. Substitution of the ﬁrst of these equations into the one–dimensional versions of the kinematic relation (16) and the incremental stress–strain relation (17) yields after diﬀerentiation with respect to x: ∂ σ˙ s = −E tan As k 2 exp (ikx + λt) ∂x

(31)

with E tan the tangential stiﬀness modulus of the solid. Substitution of this relation and the perturbation (30) into Eqs.(25) – (27) yields: −E tan k 2 As − iαkAp − ρs λ2 As − ρf λ2 Af = 0 iαkAp + nf kf−1 λAf − nf kf−1 λAs + ρf λ2 Af = 0 2

2

−1

(nf − α)λk As − nf λk Af + iQ

kλAp = 0

(32)

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

61

A non–trivial solution to this set of homogeneous equations exists if and only if: tan 2 E k + ρs λ2 ρf λ2 iαk −nf k −1 λ nf k −1 λ + ρf λ2 iαk = 0 (33) f f (nf − α)k −nf k iQ−1 from which the characteristic equation for the eigenvalues λ derives in a straightforward manner as: λ4 + aλ3 + bk 2 λ2 + ck 2 λ + dk 4 = 0 with a= b= c=

nf kf−1 (ρs + ρf ) ρs ρf

nf ρs αQ + ρf E tan ρs ρf

nf kf−1 (E tan + α2 Q) ρs ρf d=

nf αQE tan ρs ρf

(34)

(35a) (35b) (35c) (35d)

Decomposing Eq.(34) into real and imaginary parts leads to: λ4r + aλ3r + (bk 2 − 6ω 2 )λ2r + (ck 2 − 3aω 2 )λr + dk 4 − bω 2 k 2 + ω 4 = 0 and

(a + 4λr )ω 2 − 4λ3r − 3aλ2r − 2bk 2 λr − ck 2 = 0

(36) (37)

From the latter equation the phase velocity can formally be deduced as: ω 1 cf = = (4k −2 λ3r + 3ak −2 λ2r + 2bλr + c) (38) k a + 4λr Evidently, wave propagation is dispersive, since Eq.(38) is such that the phase velocity cf is dependent on the wave number k, cf. [10, 11, 12, 13, 14, 15, 16]. Taking the long wave–length limit in Eqs.(36) and (37) by letting k → 0, and eliminating ω yields the following sixth-order equation in λr : λ3r (8λ3r + 12aλ2r + 6a2 λr + a3 ) = 0

(39)

which has two triple roots: λr = 0 and λr = − 12 a. Substitution of the ﬁrst root in Eq.(37) gives for the long–wave limit aω 2 = ck 2 , so that with Eqs.(35–a) and (35–c), the phase velocity in the mixture is obtained as:

E tan + α2 Q (40) cf = ρs + ρf

62

Ren´e de Borst and Marie-Ang`ele Abellan

This expression is identical to that which has been found by an analysis of the reduced equations (28)–(29). The second wave speed is obtained by substituting the second independent root λr = − 21 a into Eq.(37), which results in cf = (b − c/a) − (a/2k)2 . For k → 0 this expression becomes imaginary, and harmonics with small wave numbers cannot propagate. The cut-oﬀ wave number below which harmonics cannot propagate is given by k = a3 /(ab − c). This situation is somewhat reminiscent of some gradient–enhanced plasticity models [21]. For the short wave-length limit, i.e. when k → ∞, we assume, inspired by the closed-form solution of the reduced equations (28)–(29), a general form for the damping coeﬃcient as λr ∼ −k n , n > 1. Substitution of this identity into Eq.(38) and taking k → ∞ yields that cf → k n−1 . In analogy with a single– phase, rate–dependent medium [4], an internal length scale can be deﬁned as: cf ∼ lim k −1 = 0 (41) l = lim − k→∞ k→∞ λr which indicates that the internal length scale l vanishes in the short wave– length limit. Again, this result is in agreement with earlier analyses using the reduced set of equations [17]. The observation that in a ﬂuid–saturated medium a non–vanishing physical internal length scale cannot be identiﬁed for the short–wave length limit, is diﬀerent from the situation in a rate–dependent single–phase medium [4]. The lack of a non–vanishing physical internal length scale in the present case causes that in numerical analyses the grid spacing takes the role of the internal length scale and localisation necessarily occurs between two neighbouring grid points. Evidently, this leads to a dependence of the solution on the discretisation, as is the case for localisation in the underlying strain–softening, single–phase continuum.

5 Numerical Examples To verify and elucidate the theoretical results of the preceding section, a ﬁnite diﬀerence analysis has been carried out. The spatial derivatives in Eqs.(28) and (29) have been approximated with a second–order accurate ﬁnite diﬀerence scheme. Explicit forward ﬁnite diﬀerences have been used to approximate the temporal derivatives, which is ﬁrst-order accurate. The choice for a fully explicit time integration scheme was motivated by the analysis of Benallal and Comi [16], in which they showed that in this case no numerical length scale was introduced in the analysis, apart from the grid spacing. As implied in Eqs.(28) and (29) the velocities vs and vf of the solid skeleton and the ﬂuid have been taken as fundamental unknowns and the displacements have been obtained by integration. This scheme may not be the most accurate, but it suﬃces to provide the numerical evidence needed to support the analytical ﬁndings of the preceding section.

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

σ

σ

σ0

σy

εu ε

t

t0

63

Fig. 1. Applied stress as function of time (left) and local stress–strain diagram (right)

strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 2. Strain profiles along the bar for 101 grid points and time step ∆t = 0.5·10−3 s

All calculations have been carried out for a bar with a length L = 100 m. For the solid material, a Young’s modulus E = 20 GP a and an absolute mass density ρs = ρs /ns = 2000 kg/m3 have been assumed. For the ﬂuid, an absolute mass density ρf = ρf /nf = 1000 kg/m3 was adopted and a compressibility modulus Q = 5 GP a was assumed. As regards the porosity, a value nf = 0.3 was adopted and in the reference calculations α = 0.6 and the permeability kf = 10−10 m3 /N s. In all cases, the external compressive stress was applied according to the scheme shown in Fig. 1, with a rise time t0 = 0.05 s to reach the peak level σ0 = 1.5 M P a. In the reference calculations a time step ∆t = 0.5 · 10−3 s was adopted, which is about half the critical time step for this explicit scheme. The results of the reference calculation are shown in Fig. 2 in terms of the strain proﬁle along the bar for t = 0.1, 0.2, 0.3, 0.4, 0.5, 0.6, 0.7, 0.8, 0.9, 0.95 s. For the above set of parameters, the phase velocity for the long wave– length limit is captured exactly. In line with this expression, a variation of the permeability kf does not inﬂuence the phase velocity. Also, the inﬂuence of α according to Eq.(40) was correctly reproduced, as was veriﬁed by varying

64

Ren´e de Borst and Marie-Ang`ele Abellan strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 3. Strain profiles along the bar for 126 grid points and time step ∆t = 0.5·10−3 s

α between 0 and 1. In all cases the maximum error with respect to the phase velocity remained within 3%. Upon reﬂection at the right boundary, the stress intensity doubles and the stress in the solid exceeds the yield strength σy = 2.5 M P a and enters a linear descending branch with an ultimate strain u = 1.125 · 10−3 , see Fig. 1. Figure 2 shows that a Dirac–like strain distribution develops immediately upon wave reﬂection. This is logical, since a two–phase medium with neither constituent being equipped with viscosity in its constitutive model, does not have regularising properties. To further strengthen this observation the analysis was repeated with a slightly reﬁned mesh (126 grid points), which resulted in a marked increase of the localised strain (Fig. 3, which has been plotted on the same scale as the results of the original discretisation in Fig. 2). In dynamic calculations of softening media without regularisation, not only the spatial discretisation strongly inﬂuences the results, but also the time discretisation [16]. This is exempliﬁed in Fig. 4 for a time step that is only 20% smaller than the time step used in the reference calculation.

6 Concluding Remarks In two–phase media waves propagation is dispersive. However, in the short wave–length limit, the physical internal length scale disappears. Since this limiting case governs the development of localisation in a zone of ﬁnite width after the onset of strain softening, regularising properties, which are directly related to the existence of a non–vanishing internal length scale, are absent. This conclusion is corroborated by the results of numerical analyses of wave propagation in a ﬁnite one–dimensional bar, which show that, upon the introduction of a softening stress–strain relation for the solid constituent, strain

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

65

strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 4. Strain profiles along the bar for 101 grid points and time step ∆t = 0.4·10−3 s

localisation develops in the smallest possible size, i.e. between two neighbouring grid points. Additional computations with a diﬀerent spatial resolution and with a diﬀerent time step conﬁrm this observation. Regularisation can be introduced in a two–phase medium, but this necessitates the introduction of rate or gradient dependence in the solid constituent, or explicitly taking into account the eﬀect of grain rotations.

References 1. M¨ uhlhaus HB, Vardoulakis I (1987) The thickness of shear bands in granular materials. G´eotechnique 37: 271–283 2. de Borst R, Sluys LJ (1991) Localisation in a Cosserat continuum under static and dynamic loading conditions. Comp Meth Appl Mech Eng 90: 805–827 3. Needleman A (1987) Material rate dependence and mesh sensitivity in localization problems. Comp Meth Appl Mech Eng 67: 68–85 4. Sluys LJ, de Borst R (1992) Wave propagation and localisation in a ratedependent cracked medium — Model formulation and one-dimensional examples. Int J Solids Struct 29: 2945–2958 5. Aifantis EC (1984) On the microstructural origin of certain inelastic models. ASME J Eng Mater Technol 106: 326–330 6. Pijaudier-Cabot G, Bazant ZP (1987) Nonlocal damage theory. ASCE J Eng Mech 113: 1512–1533 7. de Borst R, M¨ uhlhaus HB (1992) Gradient-dependent plasticity: Formulation and algorithmic aspects. Int J Num Meth Eng 35: 521–539 8. Peerlings RHJ, de Borst R, Brekelmans WAM, de Vree JHP (1996) Gradient enhanced damage modelling for quasi–brittle materials. Int J Num Meth Eng 39: 3391–3403 9. Ehlers W, Volk W (1997) On shear band localization phenomena in liquid– saturated granular elastoplastic porous solid materials accounting for fluid viscosity and micropolar solid rotations. Mech Coh-frict Mat 2: 301–330

66

Ren´e de Borst and Marie-Ang`ele Abellan

10. Biot MA (1956) Theory of propagation of elastic waves in a fluid-saturated porous solid. I. Low-frequency range. J Acoust Soc America 28: 168–178 11. Rizzi E, Loret B (1999) Strain localization in fluid–saturated anisotropic elastic– plastic porous media. Int J Eng Sci f37: 235–251 12. Simoes FMF, Martins JAC, Loret B (1999) Instabilities in elastic-plastic saturated porous media: harmonic wave versus acceleration wave analysis. Int J Solids Struct 36: 1277–1295 13. Zhang HW, Sanavia L, Schrefler BA (1999) An internal length scale in dynamic strain localization of multiphase porous media. Mech Coh-frict Mat 4: 445–460 14. Zhang HW, Schrefler BA (2004) Particular aspects of internal length scales in strain localisation analysis of multiphase porous materials. Comp Meth Appl Mech Eng 193: 2867–2884 15. Benallal A, Comi C (2002) Material instabilities in inelastic saturated porous media under dynamic loadings. Int J Sol Struct 39: 3693–3716 16. Benallal A, Comi C (2003) On numerical analyses in the presence of unstable saturated porous materials. Int J Num Meth Eng 56: 883–910 17. Abellan MA, de Borst R (2006) Wave propagation and localisation in a softening two–phase medium. Comp Meth Appl Mech Eng, doi: 10.1016/j.cma.2005.05.056 18. Jouanna P, Abellan MA (1995) Generalized approach to heterogeneous media. In: Gens A, Jouanna P, Schrefler B (eds) Modern Issues in Non-Saturated Soils, 1–128. Springer, Berlin Heidelberg New York 19. Lewis RW, Schrefler BA (1998) The Finite Element Method in the Static and Dynamic Deformation and Consolidation of Porous Media, Second Edition. John Wiley & Sons, Chichester 20. Whitham GB (1974) Linear and Nonlinear Waves. Wiley-Interscience, New York 21. Sluys LJ, de Borst R, M¨ uhlhaus HB (1993) Wave propagation and dispersion in a gradient-dependent medium. Int J Solids Struct 30: 1153–1171

New Developments in Surface-to-Surface Discretization Strategies for Analysis of Interface Mechanics Tod A. Laursen and Bin Yang Computational Mechanics Laboratory Department of Civil and Environmental Engineering Duke University, Durham, NC 27708-0287, USA [email protected] Summary. This article summarizes recent results pertaining to the implementation of mortar-based contact formulations in nonlinear computational solid mechanics. In particular, the authors discuss extension of the mortar framework to encompass large sliding, searching algorithms, treatment of self-contact phenomena, and use of the mortar framework to treat problems of lubricated contact.

1 Introduction This paper describes recent progress in the development of mortar-based methods for analysis of contact mechanics problems using ﬁnite elements. The mortar element method was ﬁrst conceived as a domain decomposition method, whereby possibly distinct meshes may be joined across interfaces such that optimal convergence results expected from the underlying ﬁnite element method can be obtained (the reader may consult [4, 2, 3, 15] for early descriptions of the idea, as well as useful overviews). In the context of nonlinear mechanics, one of the appealing applications of this idea is “mesh tying.” In such an application, separate meshes can be generated for subcomponents of an assembly to be analyzed, and then the mortar formulation can be used to “join” these parts by enforcing compatibility of the solution across the interfaces where they meet. Using this approach, accurate results can be obtained even for nonconforming meshes, as long is there is not too large a discrepancy in mesh ﬁneness across each interface. In mortar methods in general, the key idea is that the kinematic constraints between neighboring domains are enforced in an integral sense, rather than locally at each of a ﬁnite set of collocation points. Since contact problems frequently feature nonconforming meshes in contact regions, the potential applicability of mortar techniques to such problems

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 67–86. © 2007 Springer. Printed in the Netherlands.

68

Tod A. Laursen and Bin Yang

is not hard to imagine. Several early authors recognized this fact and proposed mortar-based formulations for kinematically linear applications with considerable success (see [1, 9, 10, 6]). In extending such methods to the large deformation, large sliding regime, however, one is confronted with the need to not only reformulate the constraint deﬁnitions to reﬂect changing connectivity during relative sliding, but also to provide robust algorithmic implementations of these deﬁnitions such that (for example) Newton-Raphson or similar iterative schemes for solution of the nonlinear equations will be eﬀective. In a set of recent papers [12, 13, 17], such large deformation formulations have been thoroughly described, and have been shown to be robust for large deformation applications in both two and three dimensions, and under either dynamic or quasistatic circumstances. In this paper, we review some of the key constructs of mortar-based contact algorithms, starting by looking at the mesh tying problem as a template and brieﬂy discussing the extension to truly large sliding contact. After this review, the emphasis will be on recent extensions of the mortar methodology, which allow it to encompass a much broader set of applications. Speciﬁcally, the self-contact problem and the lubricated contact problem will be examined. Generally speaking, the mortar framework allows us to put the spatial discretization of contact phenomena on a much ﬁrmer theoretical basis, opening up a large range of interfacial phenomena that can be reliably simulated. In addition to the accuracy exhibited by these approaches, they also lend considerable robustness to a nonlinear equation solving strategy as compared to traditional contact descriptions, due to the nonlocal nature of the constraints produced by the formulation.

2 Background: Mortar Projection in Contact Mechanics 2.1 The Mesh Tying Problem The key conceptual concept behind mortar projection is illuminated by taking the mesh tying application as a ﬁrst example. To ﬁx ideas, we consider the large deformation response of two bodies (i), with an eye toward approximately computing the deformation mappings ϕ(i) ∈ H 1 (Ω (i) ), describing the current positions of reference conﬁgurations Ω (i) . As per a common procedure, the surfaces of the bodies ∂Ω (i) are assumed to be decomposed into prescribed traction, displacement and contact regions via ∂Ω (i) = Γσ(i) ∪ Γu(i) ∪ Γc(i) Γσ(i) ∩ Γu(i) = Γu(i) ∩ Γc(i) = Γσ(i) ∩ Γc(i) = ∅

(1)

and boundary conditions are summarized as (J)

(i)

(i)

PiJ NJ = t¯i (i)

(i)

ϕi = ϕ¯i

on Γσ(i) on Γu(i)

(2)

Surface-to-Surface Discretization Strategies for Interface Mechanics

69

(1) h

Γc

(2) h

Γc

Fig. 1. Simple two dimensional illustration of how dissimilar polynomial interpola(1) h (2) h tion of the same surface causes Γc = Γc . The dark curve indicates the surface to be approximated

In (2), PiJ denotes the components of the ﬁrst Piola-Kirchhoﬀ stress, NJ represents the components of the outward normal to the reference conﬁguration, (i) (i) and t¯i and ϕ¯i are the prescribed tractions and displacements, respectively. The summation convention is applied, where uppercase Roman indices refer to reference quantities, while lowercase counterparts are spatial. We leave unspeciﬁed the speciﬁc constitutive law governing PiJ ; in fact, the formulations we propose in this paper for treatment of interfaces are conceived independently of the material laws used to describe the contacting continua. The mortar method is to be applied over the tied regions, which are de(i) noted here by Γc , i = 1, 2, such that the mesh tying constraint becomes ϕ(1) = ϕ(2) on Γc(1) = Γc(2) .

(3)

In the continuum setting, the reference positions of the tied regions coincide, so that one could equivalently require U (1) = U (2) on Γc(1) = Γc(2) ,

(4)

where U (i) = ϕ(i) − X (i) is the Lagrangian displacement. In a numerical ap(i)h proximation, the discretized versions of the surfaces (denoted Γc , i = 1, 2) are no longer coincident; indeed, it is easy to show that discretizations of the same (curved) surface will in general produce areas of unintended overlap and void (see Fig. 1). This fact is important in practice (see for example [11]), and means that quite often reference geometries must be corrected after mesh generation so that the initial conﬁguration obeys the mortar-based constraints. This is particularly true if the continuity constraints are written in terms of (3) rather than (4), which are not equivalent in the spatially discrete case. To simplify our discussion here, however, we neglect this subtlety.

70

Tod A. Laursen and Bin Yang

By convention, we introduce a mortar multiplier ﬁeld λh , deﬁned over the (1)h non-mortar (sometimes termed slave) surface Γc . This ﬁeld is written in (1)h

terms of the shape functions NA describing Γc ns

λh =

A=1

, such that

(1)

λ A NA ,

(5)

(1)

where ns is the set of all nodes comprising Γc . A mortar method enforcing compatibility of the two bodies’ responses over the tying region is deﬁned by enforcing: ∗h ∗h (6) 0 = Gint,ext (ϕh , ϕ ) + Gc (ϕh , ϕ ) ∗ (1)

h

∗ (2)

which must hold for all admissible variations {ϕ ,ϕ h h 0= q h · (U (1) − U (2) ) dΓ h

h

}, and (7)

(1)

Γc

which must hold for all q h ∈ Mh , where Mh is the space of admissible variations of the multiplier ﬁeld λh . In (6), Gint,ext is the usual virtual work of the internal stresses and applied loads, while Gc denotes the contact virtual work, given here as h h ∗h ∗ (1) ∗ (2) Gc (ϕh , ϕ ) = − λh · (ϕ −ϕ ) dΓ. (8) h (1) Γc

Equation (6) is recognized as the usual expression of global equilibrium, while the constraints implied by (7) weakly enforce compatibility between h h U (1) and U (2) . Weighting functions associated with the constraint equation are given as ns (1) q A NA . (9) qh = A=1

Writing the Lagrangian displacements on both surfaces as h

U (1) =

ns A=1

(1)

h

U A NA , U (2) =

nm C=1

(2)

U C NC ,

(10)

(2)h

where nm is the number of nodes C that comprise Γc (the mortar surface), we ﬁnd that substitution into (7) renders ns ns nm (1) (2) qA · NA U B NB − U C NC dΓ . (11) 0= h A=1

(1)

Γc

B=1

C=1

Equation (11) must hold for arbitrary q A , so that a vector-valued constraint

Surface-to-Surface Discretization Strategies for Interface Mechanics (1)h

is implied at each node A in Γc 0 = cA = =

(1)h

Γc

ns B=1

(1)

:

(1) NA

(1) nAB U B

71

ns

U B NB −

B=1 nm

−

ˆ B=1

nm C=1

(2) U C NC

dΓ (12)

(2) nAC U C .

(2)

In (12), nAB and nAC are given by (1) (1) (1) nAB = NA NB dΓ , and h (1) Γc

(2)

nAC =

(1)h Γc

(1)

(2)

NA NC dΓ.

(13)

h

One may readily see that (12) forces U (1) to equal a least squares projection h

(1)

h

(1)

of Γc . The multiplier ﬁeld λh deﬁned in of U (2) onto the discretization Γc (5) enforces these discrete constraints, and may be understood as the surface tractions distribution appearing in the contact virtual work, as given in (8). 2.2 Generalization to Sliding Contact In extending the mortar idea to true contact-impact interaction, one must recognize that the deﬁnition of the mortar operators (as summarized above in (13)) is now aﬀected by changing connectivity as sliding occurs. This suggests that it is now more natural (in contrast to (8)) to represent the contact virtual work Gc in terms of spatial conﬁguration quantities, via (1) ∗ ∗ ∗ (2) X ) − ϕ (Y¯ ) dγ, Gc (ϕ, ϕ) = − λ · ϕ (X (14) (1) γc

(1)

where γc is the current conﬁguration of the (non-mortar) contact surface (1) on Γc , the mortar multiplier λ now denotes the Cauchy contact traction, and where ϕ(2) (Y¯ ) is the current position of the contact point for X . Superscript h’s have been omitted in (14) to simplify notation. The notation Y¯ has (2) been used to denote the contact point on Γc corresponding to each point (1) X ∈ Γc . In traditional contact implementations, this point is typically explicitly determined for each point at which which contact constraints are to be enforced. Here we will employ a spatial integration procedure which will only indirectly deﬁne pairings between points X and Y¯ . Another important distinction between the contact problem and the mesh tying problem is that inequality constraints now govern the Lagrange multipliers (tractions) and associated kinematics. We may deﬁne a gap function X , t) as g(X

X , t) − ϕ(2) Y¯ , t X , t) = n · ϕ(1) (X (15) g(X

72

Tod A. Laursen and Bin Yang (1)

X , t). The where n denotes the outward unit normal to γc at x = ϕ(1) (X Kuhn-Tucker conditions governing the normal part of the contact interaction are then written as X , t) ≤ 0 g(X X , t) ≥ 0 λN (X (16) X , t)g(X X , t) = 0 λN (X X , t) = −λ · n is the Cauchy contact pressure at material point X where λN (X on the slave surface. Equation (162 ) implies that only compressive interaction is allowed, while (163 ) allows the contact pressure to be non-zero only when X , t) = 0. g(X The frictional response can be characterized by isolating the relative tangential velocity v T via

X , t) v=ϕ ˙ (2) Y¯ , t − ϕ ˙ (1) (X (17) = vN + vT where v T is that part of the relative velocity in the tangent plane associated with n. The contact traction λ is similarly resolved, λ = λ N + λT .

(18)

With these notions in hand, the conditions for Coulomb friction can be written as: λT

v T − γ˙

=0

λT

(19) Φ := λT − µ λN ≤ 0 γ˙ ≥ 0 Φγ˙ = 0, where, as can be seen, the frictional traction λT is forced to oppose the tangential velocity v T . A discrete version of the contact problem is achieved through substitution of ﬁnite dimensional approximations for deformation mappings, variations, and Lagrange multipliers. This results in the following mortar approximation to the contact virtual work, denoted as Gcm : ns ns nm ∗h (1) ∗ (1) (2) ∗ (2) λA · nAB ϕB − nAC ϕC . Gcm (ϕh , ϕ ) = − (20) A

(1) nAB

B

(2) nAC

C

and are similar to those given in the tying The expressions for problem (see (13), but now live in the spatial conﬁguration: (1) (1) X ) NB(1) ξ (1) (X X ) dγ, NA ξ (1) (X nAB = γ (1)h (21)

(2) (1) X ) NC(2) ξ (2) Y¯ (X X ) dγ. nAC = NA ξ (1) (X γ (1)h

Surface-to-Surface Discretization Strategies for Interface Mechanics

73

The normal and tangential portions of the contact operator are now exposed by splitting each nodal λA into normal and frictional parts: λA = λNA + λTA .

(22)

The normal part of the contact traction may be represented as (see [12]) λNA = −λNA n A (no sum)

(23)

where λNA represents the contact pressure at node A. It is subject to KuhnTucker conditions via λNA ≥ 0 gA ≤ 0 (24) λNA gA = 0 where the mortar projected gap gA at slave node A is deﬁned as gA = n A · g A , ns nm (1) (1) (2) (2) nAB ϕ B − nAC ϕ C , g A = κA B

(25)

C

where κA is a scale factor deﬁned as 1 κA = (1,ref ) , n D AD (1,ref ) (1) (1) X ) ND X ) dΓ. ξ (1) (X = NA ξ (1) (X nAD

(26)

Γ (1)h

The scaling deﬁned in (26), while not by any means unique, is performed so that the gap function g A is dimensionally correct; this feature is of crucial importance when implementing penalty methods in particular. Equation (25) is written in terms of a nodal normal nA associated with each slave node A. Although other implementations of mortar-based frictional contact are possible, we consider here a penalty regularization of conditions (19). This may be expressed via ⎤ ⎡ λT ⎦

Lv λT = T ⎣v T − γ˙

λT

Φ := λT − µ λN ≤ 0

(27)

γ˙ ≥ 0 Φγ˙ = 0 where T is the frictional penalty parameter. The frictional conditions in (19) are recovered in the limit as T → ∞. Lv λT is the Lie derivative of the

74

Tod A. Laursen and Bin Yang

frictional traction, and may be deﬁned (for example) in a two dimensional context via (28) Lv λT = λ˙ T τ where τ is a tangential base vector. Equation (28) contains material time derivatives of the components of λT only; the absence of derivatives of base vectors assures its frame indiﬀerence. Correspondingly, as shown in [17], the appropriate notion of tangential velocity to use in a mortar projected framework is nm ns (2) (2) (1) (1) n˙ AC ϕ C − n˙ AB ϕ B · (I − n ⊗ n) v TA = −κA (29) C

(2) n˙ AC

B

(1) n˙ AB

and are time derivatives of the mortar integrals (holding node where A constant). Note that the scaling factors κA have again been introduced to retain dimensional consistency. Since the mortar integral time derivatives are invariant with respect to any rigid body motion relative to the original spatial frame, v TA is frame indiﬀerent. With these deﬁnitions in hand, a trial state-return map strategy is employed to determine the Coulomb frictional tractions in an algorithmic, time stepping procedure. The algorithm begins by computation of a trial state, assuming no slip during the increment: nm (2) (2) (2) trial nACn+1 − nACn ϕ C = λTAn − T κA λTA n+1

−

C

ns B

(1) nABn+1

−

(1) nABn

(1) ϕB

(30) · (I − nA ⊗ nA ),

with a corresponding trial value for the slip function

trial Φtrial An+1 = λTAn+1 − µ|λNAn |. A return map is then used to deﬁne the ﬁnal frictional traction via ⎧ trial ⎪ if Φtrial ⎨λTAn+1 An+1 ≤ 0 (stick), trial λT λTAn+1 = An+1 ⎪ otherwise (slip). ⎩µ|λNAn | λtrial T

(31)

(32)

An+1

In these expressions, the subscript n + 1 means a state associated with the current iteration for the unknown solution at tn+1 , while n is associated with the last (converged) time level.

3 An Extension of the Framework: Mortar-Based Self-Contact In many applications, such as are encountered in post-buckling analysis, a surface may fold upon itself such that so-called self contact takes place. A two

Surface-to-Surface Discretization Strategies for Interface Mechanics

75

γσ Γσ (1,1)

γc ϕ

(3,1)

γc

(1,2)

γc

(3,2)

γc

(2,1) γc

Γc

(2,2)

Ω

γc

γu

Γu

Y

X

Fig. 2. Notation for a large deformation self-contact problem

dimensional self-contact problem, with large deformation and large sliding, is shown schematically in Fig. 2. Recent work shows that the mortar framework can be extended to such settings, and we highlight some of the key steps here in accomplishing that extension. In writing the virtual work for such a system, the expression given originally in (8) must be generalized not only to account for the possibility of sliding, but also to account for the possibility of multiple contact patches which can be generated as the surface folds over on itself. We therefore replace (8) by c

∗

G (ϕ, ϕ) := −

k i=1

(i,1)

γc

(i,1) ∗ ∗ (i,2) ¯ X , t) · ϕ X , t) − ϕ λ(i,1) (X (X (Y , t) dγ,

(33) where ϕ(i,2) (Y¯ ) is the current position of the contact point for X . Indices i refer to the multiple contact patches which might be identiﬁed at any instant in the simulation, with k being the number of these patches. As before, the (i,1) is the nonmortar surface where the Lagrange multipliers will be surface γc (i,2) is the mortar surface. As summarized earlier in (22), interpolated, and γc the contact traction λ can be resolved into normal and tangential components, and the conditions of normal contact are given by (24), and the frictional conditions by (19), just as in the frictional contact case. The contact searching

76

Tod A. Laursen and Bin Yang

Fig. 3. Mortar segments in (a) two dimensions; (b) three dimensions. A segment is shown in green

algorithm for mortar contact, however, must be considerably generalized to deal with the phenomenon of self-contact. As discussed in [17] and [12] for general mortar contact formulations, we (1) need to ﬁnd all the mortar segments to compute the mortar integrals, nAB (2) and nAC , deﬁned in (21). For example, in three dimensional problems, the mortar integrals are computed as: (i,1)

nAB = (i,1) tri,seg

nAB

(i,2)

nAC = (i,2) tri,seg nAC

seg

(i,1) seg

nAB

seg

(1)

γctri,seg,i (i,2) seg

nAC

=

γctri,seg,i

seg tri

=

=

NA

=

ξ

, i = 1, ..., k,

X ) NB(1) ξ (1) (X X ) dγ ξ (1) (X

seg tri

(1) NA

(i,1) tri,seg

nAB

(1)

(i,2) tri,seg

nAC

(34)

, i = 1, ..., k,

X ) dγ X ) NC(2) ξ (2) Y¯ (X (X

(35)

In these equations, the superscript seg refers to a mortar segment , which is constructed such that each segment is deﬁned by the mutual projection of a single slave element surface with a single master element surface, as shown in Fig. 3. The polygonal intersections of element surfaces, shown in green in Fig. 3(b), are in turn divided into triangles for numerical evaluation of the integrals, giving rise to the superscripts tri above. The segments change dynamically during a simulation of sliding contact, and the dependence of the method on the determination of the segments is why we refer to the contact algorithms in this work as being surface to surface algorithms. Given a discretized contact surface, an eﬃcient contact algorithm depends crucially on eﬃcient determination of these mortar segments. In our implementation, we recursively split the surface into subsurfaces to build a tree

Surface-to-Surface Discretization Strategies for Interface Mechanics

1

77

1

2

4 6

5

7

5

4

8

8

3

2

3

6

7

9

9

Fig. 4. A bounding volume tree for a 2D surface

structure; the approach has been extensively described in [16] and will only be brieﬂy recounted here. The subsurfaces related to leaf tree nodes are the elements of the surface. Each node of the tree will be termed a T-node, to differentiate from a ﬁnite element node. Each subsurface is deﬁned and stored in terms of an inﬂated bounding volume (speciﬁcally, a k-DOP), which is saved in its corresponding T-nodes. Binary trees are used in this work so each nonleaf T-node has exactly two children, a left child and right child. A typical bounding volume hierarchy is shown in Fig. 4. If there are n elements for a contact surface, the number of T-nodes in bounding volume tree is 2n − 1. The storage space for a bounding volume tree is then O(n). In [16], two methods for building bounding volume trees are discussed: top-down and bottom-up approaches. A top-down approach, which is used to build the bounding volume trees for multi-body contact problems, starts with one T-node (a root T-node) which is related to the entire surface. The surface is then recursively split into subsurfaces and each of them is saved in a newly created T-node. The bottom-up approach, by contrast, begins with the input elements as the leaves of the bounding volume tree and applies some algorithms to group elements recursively. Usually, by this approach, the subsurface corresponding to a T-node is a connected surface so it is a more appropriate way than the top-down approach to build the bounding volume trees for self-contact problems. In this work, we apply the surface clustering algorithm introduced in [14, 7] to build bounding volume trees. In the face clustering algorithm, one ﬁrst creates a dual graph for the mesh of the contact surface. A dual graph is constructed by mapping each element of the surface mesh to a dual node and connecting every two dual nodes by a dual edge if the corresponding elements are adjacent and share an element edge. An example of a dual graph is shown in Fig. 5, where dashed lines are

78

Tod A. Laursen and Bin Yang

Dual Edge

Dual Node

Finite Element Edge Finite Element Node Fig. 5. Dual graph for a surface mesh. Each dual node represents an element or subsurface in the ﬁnite element mesh

ﬁnite element edges, solid lines are dual edges, grey dots are ﬁnite element nodes, and black dots are dual nodes. By contracting a dual edge (i.e., removing the dual edge and collapsing its two dual nodes into a new dual node) one can group two elements into an element cluster (or a subsurface) which corresponds to a new dual node in the dual graph, as seen in Fig. 6. Basically, this contraction will group two contiguous elements or subsurfaces into a new subsurface, which will be their parent in the bounding volume hierarchy. One may also notice that each dual node in the dual graph corresponds to a T-node in the bounding volume tree. By doing this contraction iteratively, one can ﬁnally build a hierarchical structure of the surface mesh, as shown in Fig. 7. To control the quality of the bounding volume hierarchy, i.e. the balance of the bounding volume tree and the shape and tightness of the bounding volumes, one has to follow a carefully designed rule to contract the dual edges. This rule identiﬁes which edge should be contracted ﬁrst and which should be contracted later. To do this, a cost function is assigned to each dual edge; the cost function applied in this work is similar with that was used by [14]. All dual edges are saved in a heap data structure (see [5] for an introduction) and the key values of the heap entries are the contraction costs of the corresponding dual edges. Thus, the dual edge with the least cost is saved on the top of the heap. The procedure to construct a bounding volume hierarchy with the face clustering algorithm can be summarized as: 1. Build the initial dual graph for the ﬁnite element mesh, compute cost functions of all dual edges, and save all the dual edges in a heap.

Surface-to-Surface Discretization Strategies for Interface Mechanics

Contract This Dual Edge

79

New Subsurface

Surface Mesh Dual Graph

(a)

(b)

Fig. 6. Contraction of a dual edge to construct a new subsurface (i.e. removal of a dual edge and collapsing of its two dual nodes): (a) initial dual graph, and (b) new dual graph. The bigger dot on (b) denotes the new generated dual node by this contraction, and the new dual node corresponds to a new constructed subsurface denoted by the shaded area

2. Remove a dual edge from the top of the heap and contract it to construct a new subsurface. 3. Generate a new T-node for the new subsurface. The two children of the new T-node are the two T-nodes corresponding to two dual nodes (subsurfaces or elements) connected by the dual edge. 4. Update all cost functions of dual edges that are connected with the two dual nodes of the contracted dual edge. 5. Update the heap. 6. Repeat 2 through 5 iteratively until the whole tree is constructed. From this procedure, one can see that the bounding volume tree is built in a bottom-up manner. For each node of the tree, the bounding volume of its corresponding subsurface is computed. For large deformation contact problems, the updating of the bounding volume trees is required after each iteration since the bounding volumes are dependent on deformation. Finally, after the contact detection has been accomplished, it is necessary to do some post processing after the searching, to avoid the situation where the contact traction ﬁelds on each contact patch could be deﬁned on discontinuous surfaces, as shown in Fig. 8. As can be seen, without some type of intervention, an element can be a slave element in one contact pair and a master element in another, and there may be a mixture of slave and master elements on a continuous contact element patch (the lower or upper solid line in Fig. 8). A

80

Tod A. Laursen and Bin Yang

(a)

(b)

(c)

(d)

(e)

Fig. 7. A hierarchy (tree) structure from the bottom level to the top level

M M S

S

S

M M

S M

S

S − Slave

M − Master

Fig. 8. Discontinuous deﬁnition of slave and master elements (a double arrow denotes a contact element pair) which should be avoided

simple sorting procedure is applied so that each side of each contact patch retains its own identity as master or slave. As an example of the type of problem to which this self-contact approach is applicable, we consider the rolling of a highly loaded tire which is nearly ﬂat. In this problem, the part of the surface in self-contact (inside the tire) continually changes due to the rolling, placing a signiﬁcant demand for robustness on the searching algorithm and Newton-Raphson iterative scheme. Deformed conﬁgurations of the nearly ﬂat tire at diﬀerent load steps are shown in Fig. 9, where (c) and (d) only show a quarter of the tire to demonstrate self-contact

Surface-to-Surface Discretization Strategies for Interface Mechanics

81

Fig. 9. Deformed conﬁgurations of the tire rolling problem at diﬀerent load steps; parts (c) and (d) only show a quarter of the tire

inside the tire. Signiﬁcant deformation and sliding are seen to occur in this problem. Notably, it is diﬃcult if not impossible to perform this situation using node-to-surface contact discretization strategies.

4 Mortar Formulation of Lubricated Contact Another recent extension of the mortar formalism involves its use to describe lubricated contact, such as might occur for example in many metal forming applications, or underneath a tire rolling on wet pavement. Such a problem, with two deformable solid bodies and a thin ﬂuid ﬁlm between them, is shown (1) (2) in Fig. 10. The two solid bodies occupy the open sets Ωs and Ωs , where a subscript s represents the solid phase. The solid phase of a lubricated contact problem is governed by the usual solid continuum mechanics equations. Here we assume inﬁnitesimal deformations for the solid phase for simplicity, although it is possible to extend the formulation to large deformation cases with proper treatments of geometric nonlinearities. No assumptions are made for the constitutive laws: the material response may be either elastic or inelastic, rate dependent or independent.

82

Tod A. Laursen and Bin Yang

(1)

Γsu (1) Γsσ

Fluid phase

(1) Ωs (1)

Γsc

(2)

Γsc

(2)

Ωs (2)

Γsu

(2)

Γsσ

Fig. 10. Notation for two body lubricated contact problems

In the problems considered here, the through-the-thickness dimension of the ﬂuid ﬁlm is assumed to be much smaller than the size of the contact patch in surface coordinates. Under such conditions, the ﬂuid phase of a lubricated contact problem is governed by the Reynolds equation, which can be derived from the Navier-Stokes and continuity equations based on the thinﬁlm assumption (see, e.g., [8]). The Reynolds equation is deﬁned on a surface domain, which considered to be parameterized by the slave side of a contact surface in this formulation. As shown in Fig. 11, the contact domain Ωf , cor(1) responding to the slave surface Γsc less the dry contact region Ωd , is divided into two diﬀerent subdomains, Ωfl and Ωfc . Ωfl is the subdomain where the lubricant is continuous and has positive pressure, while Ωfc is the subdomain where the lubricant has cavitations and is ruptured (the ﬂuid ﬁlm is assumed to support only a negligible amount of tension before rupture). ΓfD is the surface where the Dirichlet boundary conditions are prescribed for the Reynolds equation, while ΓfN is the boundary between the dry contact domain and the lubrication domain and where Neumann boundary conditions are prescribed. ΓfR , which is called the Reynolds boundary, is the boundary between Ωfl and Ωfc . Based on these deﬁnitions, \ Ωd , Ωf = Γs(1) c

(36)

Ωf = Ω f l ∪ Ω f c .

(37)

and

Surface-to-Surface Discretization Strategies for Interface Mechanics

Ωd

ΓfN

ΓfR

83

Ωfc

Ωfl

ΓfD Fig. 11. Notation for the lubrication domain

The virtual work for the solid phase can be written in the usual way via (1) ∗ ∗ ∗ (2) c u u t(1) (X X ) · u (X X ) − u (Y¯ ) dΓ, G (u , p, ) := − (38) (1) Γsc

where Y¯ is the position of the contact point for X , with the understanding that the contact traction t is now inherited from the traction ﬁeld prevailing in the intervening ﬂuid, consisting in general of a ﬂuid pressure p in the normal direction and a viscous tangential component. It is the ﬂuid part of the formulation that makes the mortar approach attractive in this case, since the pressure distribution in the thin ﬁlm is subject to a governing diﬀerential equation (the Reynolds equation). The fact that the mortar approach produces a consistent surface discretization gives an ideal way to not only approximate this diﬀerential equation, but also to couple it to the solid response. As presented by [8], the general Reynolds equation which governs the ﬂuid pressures within Ωfl is ∂ (ρh) ˜· +∇ ∂t

(1) (2) ρh3 ˜ ρ(V˜ + V˜ ) − ∇p + h 12µ 2

= 0,

(39)

where ρ is the current mass density of the lubricant, h is the ﬂuid ﬁlm thickness (1) (negative of the gap function g), µ is the viscosity of the lubricant, V˜ and

84

Tod A. Laursen and Bin Yang

Fig. 12. Finite element mesh of the three dimensional lubricated contact problem with two diﬀerent perspectives (2) V˜ are projections of slave and master surface velocity vectors onto the slave surface, and p is the ﬂuid pressure (the primary unknown of Equation (39)). ˜ indicate divergence and gradient operators in reduced (surface) Operators ∇ coordinates. The ﬂuid viscosity may be dependent on the ﬂuid pressure; both constant viscosity cases and exponential pressure dependence of viscosity have been tested in our early work. We have implemented a mortar-based monolithic strategy to solve the coupled Reynolds equations and global equilibrium equations, with the solid phase displacement coupling to the ﬂuid equations through the ﬁlm thickness h and the ﬂuid equations coupling to the solid mechanics equations through generation of the pressure ﬁeld p and the viscous shear stresses. Although the full numerical formulation is too involved to recount in detail here, we present a simple three dimensional example to demonstrate the type of simulation for which the technique has been tested. The problem is depicted in Fig. 12, where the relative rotation of two cylinders with a lubricant-ﬁlled interface is considered. A quasi-static rotation is applied to the inner surface of the inside cylinder, corresponding to an angular speed of ω = 500. Figure 12 presents the ﬁnite element mesh for the two cylinders. The inside surface of the outer cylinder is chosen as the slave surface and the outside surface of the inner cylinder is chosen as the master surface. Only one load step is applied for this problem. The computed pressure distribution in the ﬂuid ﬁlm is plotted in Fig. 13.

5 Conclusion This paper has discussed the mortar method as an underlying spatial discretization technique for large deformation contact problems, and has empha-

Surface-to-Surface Discretization Strategies for Interface Mechanics

85

Fig. 13. Computed pressure distribution for the three dimensional lubricated contact problem

sized two promising recent extensions of this idea: incorporation of self-contact phenomena, and consideration of lubricated contact problems. Contact formulations based on mortar concepts have been seen not only to be extremely accurate in comparison with more traditional node-to-surface strategies, but are also extremely robust numerically, particularly within the implicit dynamic and quasistatic applications of primary interest here.

Acknowledgment This work was supported through a research contract by Michelin Americas Research Corporation. This support, as well as the collaboration of Drs. Stephane Cohade, Ali Rezgui, and Mike Andrews, is greatly appreciated.

References 1. Belgacem FB, Hild P, Laborde P (1997) Approximation of the unilateral contact problem by the mortar ﬁnite element method. Comptes Rendus De L’Academie Des Sciences 324:123–127 2. Belgacem FB, Maday Y (1994) A spectral element methodology tuned to parallel implementations. Computer Methods in Applied Mechanics and Engineering 116:59–67 3. Belhachmi Z, Bernardi C (1994) Resolution of fourth order problems by the mortar element method. Computer Methods in Applied Mechanics and Engineering 116:53–58

86

Tod A. Laursen and Bin Yang

4. Bernardi C, Maday Y, Patera AT (1992) A new nonconforming approach to domain decomposition: The mortar element method. In H. Brezia and J.L. Lions (Eds.) Nonlinear Partial Diﬀerential Equations and Their Applications pp 13–51. Pitman and Wiley 5. Cormen TH, Leiserson CE, Rivest RL, Stein C (2001) Introduction to Algorithms, Second Edition. The MIT Press 6. El-Abbasi N, Bathe K-J (2001) Stability and patch test performance of contact discretizations and a new solution algorithm. Computers and Structures 79:1473–1486 7. Garland M, Willmott AJ, Heckbert PS (2001) Hierarchical face clustering on polygonal surfaces. In SI3D, pp 49–58 8. Hamrock BJ (1991) Fundamentals of Fluid Film Lubrication. NASA, Washington, D.C. 9. Hild P (2000) Numerical implementation of two nonconforming ﬁnite element methods for unilateral contact. Computer Methods in Applied Mechanics and Engineering 184:99–123 10. McDevitt TW, Laursen TA (2000) A mortar-ﬁnite element formulation for frictional contact problems. International Journal for Numerical Methods in Engineering 48:1525–1547 11. Puso MA (2004) A 3d mortar method for solid mechanics. International Journal for Numerical Methods in Engineering 59:315–336 12. Puso MA, Laursen TA (2004) A mortar segment-to-segment contact method for large deformation solid mechanics. Computer Methods in Applied Mechanics and Engineering 193:601–629 13. Puso MA, Laursen TA (2004) A mortar segment-to-segment frictional contact method for large deformations. Computer Methods in Applied Mechanics and Engineering 193:4891–4913 14. Willmott AJ (2000) Hierarchical Radiosity with Multiresolution Meshes. PhD thesis, Carnegie Mellon University 15. Wohlmuth BI (2001) Discretization Methods and Iterative Solvers Based on Domain Decomposition. Springer-Verlag, Heidelberg 16. Yang B, Laursen TA (2006) A contact searching algorithm for large deformation mortar formulation. Computational Mechanics, (submitted) 17. Yang B, Laursen TA, Meng XN (2005) Two dimensional mortar contact methods for large deformation frictional sliding. International Journal for Numerical Methods in Engineering 62:1183–1225

Particle Finite Element Methods in Solid Mechanics Problems J. Oliver, J.C. Cante, R. Weyler, C. Gonz´ alez and J. Hernandez E.T.S. Enginyers de Camins, Canals I Ports de Barcelona E.T.S. d’Enginyer´ıa Industrial i Aeron´ autica de Terrassa Universitat Polit´ecnica de Catalunya (UPC) Campus Nord UPC, Ediﬁci C-1, c/ Jordi Girona 1-3, 08034 Barcelona, Spain [email protected] Summary. The paper examines the possibilities of extending the Particle ﬁnite element methods (PFEM), which have been successfully applied in ﬂuid mechanics, to solid mechanics problems. After a review of the fundamentals of the method, their speciﬁc features in solid mechanics are presented. A methodology to face contact problems, the anticipating contact interface mesh, is presented on the basis of a penalty-like constitutive models for imposing the contact and friction conditions. Finally, the PFEM is applied to same representative solid mechanics problems to display the capabilities of the method and some ﬁnal conclusions are obtained.

1 Introduction Particle ﬁnite element methods (PFEM) have received considerable attention in the recent years due to their modeling capabilities for same speciﬁc problems. So far, most of the research and applications of PFEM can be found in the context of computational ﬂuid dynamics (CFD) to tackle ﬂuid mechanics problems in typical solid mechanics settings: i.e. using Lagrangean descriptions of the motion of the continuum medium (Onate et al., 1996; Lohner et al., 2002; Idelsohn et al., 2003a, 2003b, 2004). Their main advantages are found in modeling conﬁned ﬂuids exhibiting moving free surfaces. There, the limited character of the particle displacement makes suitable a Lagrangean description which, in turn, facilitates the tracking and modeling of the existing free surfaces. On the other hand, Lagrangean descriptions are the natural way of describing motion of solids, and, therefore, there is a long solid mechanics tradition in this sense. However in certain processes, of considerable practical interest, the material undergoes very large deformations, rapidly changing boundaries are involved and the motion resembles that of ﬂuids. Metal forming and machining processes, or manufacturing processes involving powder and granular Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 87–103. © 2007 Springer. Printed in the Netherlands.

88

J. Oliver et al.

materials are typical cases where the border between solid and ﬂuid behaviors becomes fuzzy. Therefore, the application of PFEM to solid mechanics problems appears as a new research ﬁeld deserving to be explored. The purpose of this work is precisely investigating the possibilities oﬀered by the particle ﬁnite element methods in some representative solid mechanics problems involving large deformations, multiple contacts, new boundaries generation, etc., thus providing some insights on the future developments in that ﬁeld.

2 Fundamentals: The Particle Finite Element Method Particle ﬁnite element methods emerged as a natural result of previous explorations in the context of the meshless methods (Belytschko et al., 1994, 1996; Onate et al., 1998). They can be characterized by the following ingredients: 1. The use of a Lagrangean format for describing the motion (Malvern, 1969). A selected cloud of particles of inﬁnitesimal size (material points) are tracked along the motion to describe the continuum medium properties evolution (position, displacement, velocities, strain, stresses, internal variables, etc.). When necessary, the properties of the remaining particles of the continuum medium are obtained by interpolation of the properties at points of that cloud. Numerical computations are done on the basis of a ﬁnite element mesh that is constructed at every time step on the basis of the particle positions. Then, Delaunay triangulations, allowing the construction of a ﬁnite element mesh for a given sets of nodes, emerge as a suitable meshing procedure (George, 1991; Calvo et al., 2003). 2. The use of a boundary recognition procedure to identify what particles of the cloud deﬁne an external (or internal) boundary. The so-called alphashape method (Calvo et al., 2003; Xu et al., 2003) constitutes a suitable strategy for this purpose (see Figure 1). It essentially consists of identifying those sides/segments of the cloud that can be inserted into an empty circle/ball (not including other particles of the cloud) of size larger than a given parameter (the alpha-shape parameter). The vertices/particles of those segments are then identiﬁed as boundary particles. Large values of the alpha-shape parameter result in a boundary which is the convex hull of the cloud. Small values of the alpha-shape parameter return a boundary constituted of all the particles of the cloud.1 2.1 Equations of Motion. Boundary Value Problem Let us consider a solid body B experiencing a deformation ϕ(X, t) : B × [0, T ] → R2 , where [0, T ] is the time interval of interest. Let us also consider a 1 For a uniformly distributed cloud of particles (with typical separation h) alphashape values of 1.1h − 1.5h are recommended for a good estimation of the actual boundary.

Particle Finite Element Methods in Solid Mechanics Problems

89

Fig. 1. The alpha-shape method for recognizing boundaries of a cloud of particles

Fig. 2. Incremental non-linear problem at time step [tn , tn+1 ]

ﬁnite set of particles of B ⊃ P := {P1 , P2 , . . . , Pnpart }, occupying, at a speciﬁc ¯ i = [X1 , X2 ]T , which time interval t ∈ [0, T ], spatial points with coordinates X ¯ ¯ P2 , . . . , X ¯ Pn } (see deﬁne the particle reference conﬁguration Ωt := {XP1 , X part Figure 2). Let us assume, at time t, a Delaunay triangulation, with all its vertices, i, ¯ i , of the particle conﬁguration Ωt , thus placed at corresponding positions, X

90

J. Oliver et al.

deﬁning an open set, Vt , at the Euclidean 2D space, with boundary ∂Vt . ˜ ⊂B The particles of B belonging to the material volume Vt deﬁne a body B approaching B as npart → ∞. Let us also consider a time discretization of [0, T ] in time intervals and a speciﬁc time slice [tn , tn+1 ] ⊂ [0, T ] characterizing the time interval/step n+1 of length ∆t = tn+1 −tn . The boundary value problem at the material domain during the time interval can be written as: Given vn , an , σ n , qn , u∗n+1 , t∗n+1 Find un+1 ≡ ϕn+1 (Xn )

such that:

∇ · σ n+1 + bn+1 = ρn+1 an+1

(momentum equation) ⎫ σ n+1 = σ n + Σ(en+1 , σ n+1 , qn+1 ) ⎪ ⎪ ⎪ ⎬ ∆σ n+1 (constitutive equations) qn+1 = qn + Q(en+1 , σ n+1 , qn+1 ) ⎪ ⎪ ⎪ ⎭

(1)

∆qn+1

en+1 = E(un+1 ) (kinematic equation) σ n+1 , nn+1 = t∗n+1

(natural boundary condition)

un+1 = u∗n+1

(essential boundary condition) at ∂u Vn+1

at ∂σ Vn+1

where vn , an , σ n , qn are, respectively, the velocities, accelerations, stresses and internal variable values at the beginning of the interval, u∗n+1 , t∗n+1 are the prescribed values of displacements and tractions, respectively, at the boundary ∂Vn+1 with outward normal nn+1 , un+1 = Xn+1 − Xn are the interval displacements and en+1 is a suitable measure of the interval strains. 2.2 Time Marching Scheme The problem described in Section 2.1 allows considering the motion of the ˜ as a sequence of discrete (in time) boundary value approximating body B problems ruled by equations (1). Then, at every time step the corresponding problem is solved according to the following strategy: Step I: Finite element discretization: Spatial discrete problem Let us now consider a ﬁnite element discretization of Vn , on the basis of the existing triangularization, so that the nodes match the vertices (therefore, ˜ is evaluated nnode = npart ), and that every property, µ, of the particles of B via interpolation of the corresponding property at the vertices/nodes as: µ(X) =

n node

Ni (X)¯ µi

∀X ∈ Vn

(2)

1

¯i stand for the shape/interpolation function and the nodal where Ni and µ value of the property, respectively, at node i.

Particle Finite Element Methods in Solid Mechanics Problems

91

Then, using standard Galerkin’s procedures, and a Newmark’s time integration scheme (Hughes, 2000), the discrete counterpart of the continuum boundary value problem in equations (1) at the space-time slice Vn ×[tn , tn+1 ] ⊂ R2 × [0, T ] reads, in matrix form: ¯n+1 + Fint Mn+1 · a un+1 ) − Fext un+1 ) = 0 n+1 (¯ n+1 (¯ ¯ n+1 = u ¯ n + ∆t¯ u vn +

1 2

∆t2 [(1 − 2β)¯ an + 2β¯ an+1 ]

(3)

¯ n+1 = v ¯ n + ∆t[(1 − γ)¯ v an + γ¯ an+1 ] ext where Mn+1 , Fint n+1 and Fn+1 are, respectively, the mass-matrix, the internal ¯ n+1 , v ¯ n+1 and a ¯n+1 are, reforces vector and the external forces vector, u spectively, the nodal displacement, velocities and accelerations and β and γ are the classical Newmark’s integration parameters. Equations (3) are a set ¯ n+1 and a ¯ n+1 . ¯ n+1 , v of non-linear equations that can be solved for u Combining interpolations, according to equation (2), and substitution in equations (1) allows determining the stresses and the internal variables σ n+1 (X), qn+1 (X) at points X ∈ Vn as required in next step.

Step II: Spatial information transfer All the information necessary in subsequent time steps has now to be transferred to the nodes/particles of Ωn . This is achieved by standard extrapolation (smoothing) procedures (Zienkiewicz et al., 2000) from the element Gauss ¯ n+1 , to be ¯ n+1 and q points to the nodes. For instance, the nodal values, σ considered as initial values for the next time step, n + 1, are computed as:

¯ n+1 = σ ¯ n + [Mσn ]−1 · σ Nσn · ∆σ n+1 dV ¯ n + [Mqn ]−1 · ¯ n+1 = q q

Vn

Vn

Nqn · ∆qn+1 dV

(4)

where Mσn and Mqn are standard “mass-like matrices”, and Nσn and Nqn are “transfer” matrices, with dimensions appropriated to the set of variables, σ and q, computed in terms of the interpolation functions Ni of the ﬁnite element mesh on the domain Vn , and ∆σ n+1 and ∆qn+1 (X) are the point-wise corresponding increments computed at the present time step [tn , tn+1 ]. Step III: Update Finally the set of particles of Ωn are updated to the new positions according to: ¯ Pi )n + (¯ ¯ Pi )n+1 = (X uPi )n+1 ∀Pi ∈ P (5) (X and the new particle conﬁguration is determined as: ¯ Pi )n+1 , (X ¯ P2 )n+1 , . . . , (X ¯ Pn )n+1 } Ωn+1 := {(X part

(6)

92

J. Oliver et al.

Fig. 3. Anticipating contact interface strategy

Then, the boundary of the new cloud of positions of the set of particles P is recognized via de corresponding alpha-shape strategy, and a new triangularization, determining the new spatial domain Vn+1 , is performed. The algorithm proceeds to Step I of the next time step.

3 Contact Strategy: Anticipating Interface Mesh One of the main diﬃculties found in standard contact algorithms in solid mechanics, is the identiﬁcation of the interacting parts of two contacting bodies (master-slave based algorithms). The previously described PFEM setting provides a very interesting feature to be exploited in this sense: the possibility of anticipating the contact boundaries and of imposing the corresponding contact constraints in a diﬀuse manner, without the necessity of a precise identiﬁcation of the contact topologies. Let us consider, for illustration purposes, a forming process characterized by a forming material and some (elastic) tooling, amenable to experience mutual contact (see Figure 3). We can consider each of them as a speciﬁc class, constituted by its own cloud of particles. At every time step, a Delaunay triangularization is performed for every class and its boundary (in terms of the boundary particles) is recognized as indicated in Section 2 by the alpha-shape procedure. Then, an additional triangularization is performed: the particles of the identiﬁed boundaries are deﬁned as a new class (the contact interface class) and sent to the mesher that returns an interface mesh, which connects anticipating contacting particles of diﬀerent classes. The value of the supplied alpha-shape value determines the maximum size of the resulting interface elements and, therefore, rules the degree of anticipation of the contacts. The contact interface mesh constructed in this way, enjoys some speciﬁc properties: •

It is an interface mesh in the sense that there is no interior node (all the nodes are placed at the boundary). In consequence, all the computations done in that ﬁnite element are naturally condensed out to the boundary nodes.

Particle Finite Element Methods in Solid Mechanics Problems

93

Fig. 4. Penalty strategy at the contact interface

• •

•

Typical properties of the Delaunay tessellation procedure ensure that the contact interface connects nearest particles in the contacting bodies. The identiﬁcation of the contact topologies is trivially done via the mesh topology: potentially contacting nodes are those belonging to the same element of the mesh. This overcomes many of the diﬃculties and computational challenges found in classical contact recognition procedures. The contact condition, imposing that nodal gaps should be positive (no penetration), can be fulﬁlled in weak form in terms of strain measures deﬁned at the elements of the interface mesh (see Section 3.1).

Generalization of this procedure to multiple contacting bodies is trivial. As for the imposition of the contact conditions there are several options. In next sections, a penalty strategy for this purpose is presented. 3.1 A Penalty Strategy at the Contact Interface (1)

Let us consider the time step [tn , tn+1 ] and two contacting boundaries, ∂Bn+1 (2) and ∂Bn+1 , and the resulting interface mesh (see Figure 4) deﬁning the interface Bint n+1 . We realize that every element of Bint n+1 has one node (node P) placed on one of the contacting bodies, and two nodes, Q1 and Q2 , on the other (see Figure 4b), which can be trivially identiﬁed. The signed distance of P to the segment Q1 − Q2 , according to the normal2 n of the boundary corresponding to this segment, is deﬁned as the initial elemental normal gap: 2 Information about the normals corresponding to the boundary segments is generated, during the boundary recognition procedure, for every body and transmitted to the boundary interface class.

94

J. Oliver et al. (e)(0)

gn+1 = (XP − XQ1 ) · n = (XP − XQ2 ) · n ∀e ∈ Bint n+1

(7)

(e)(0)

Notice that gn+1 ≥ 0 corresponds to no initial penetration of node P on the opposite boundary. Therefore, negative values of the gap correspond to boundary penetrations. Let us now deﬁne the current normal gap for the element e, at the iteration i of the linearization procedure, as: (e)(i)

(e)(0)

(i)

(e)(i)

gn+1 (un+1 = gn+1 + ∆gn+1 (e)(0) (e)(0) (e)(i) = gn+1 + gn+1 (n · ∇S un+1 · n)

∀e ∈ Bint n+1

(8)

(i)

∆gn+1 (e)(i)

which involves the iterative displacements3 un+1 at the element e. Now, let us deﬁne a strain measure associated to that gap as: (e)

(e)

ε˜n+1 =

gn+1

(9)

where stands for the typical local particle distance (see Figure 4). The con(1) (2) tact condition for boundaries, ∂Bn+1 and ∂Bn+1 , can be immediately written as the positive character of the strain measure ε˜(un+1 ): (e)

(e)

gn+1 ≥ 0 ⇔ ε˜n+1 ≥ 0 ∀e ∈ Bint n+1

(10)

In a variational context, condition (10) can be imposed via a Lagrange multiplier procedure:

λn+1 ε˜(un+1 ) dΩ Π(un+1 , λn+1 ) = ΠB(1) (un+1 ) + ΠB(2) (un+1 ) + n+1

δΠ(un+1 , λn+1 ) = 0;

n+1

g(un+1 ) ≥ 0;

Bint n+1

λn+1 ≥ 0;

λn+1 g(un+1 ) = 0 (11)

where ΠB(1) (un+1 ) and ΠB(2) (un+1 ) stand for the original minimizing funcn+1

n+1

(1)

(2)

tionals for the contacting bodies Bn+1 and Bn+1 , and λn+1 are the corresponding Lagrange multipliers. Now, all the typical strategies for solving the problem in equations (11) can be used. In particular, penalty-based strategies will be recovered by imposing a speciﬁc format to the Lagrange multipliers as: (e)

λn+1 = E 3

int

=

1 2

(e)

E int ε˜n+1 (e)

0 for ε˜n+1 ≥ 0 (e)

K for ε˜n+1 < 0

∀e ∈ Bint n+1

Superindex (·)S stands for the symmetric part of (·).

(12)

Particle Finite Element Methods in Solid Mechanics Problems

95

where K > 0 is the penalty parameter. The resulting problem is formally equivalent to the introduction of an elastic-type constitutive law, σ − ε˜, in the normal direction, deﬁned in terms of the parameter, E int , as a pseudo-elastic modulus: (e)

(e)

˜n+1 n ⊗ n σ n+1 = σ

contact stress

(e)

(e)

σ ˜n+1 = E int ε˜n+1

∀e ∈ Bint n+1

(13)

and extending the boundary value problem in equations (1) to the interface domain Bint n+1 . Inclusion of Frictional Eﬀects Frictional eﬀects can be now included in a very simple manner. For instance, on the basis of a simple Coulomb model, additional tangential stresses can be considered in the constitutive model for every element of the interface (see Figure 5): (e)

(e)

(e)

σ n+1 = σ ˜n+1 n ⊗ n + 2˜ τn+1 (t ⊗ n)S contact stress

(e)

(e)

σ ˜n+1 = E int ε˜n+1 (e)

frictional stress

∀e ∈ Bint n+1

(e)

(e)

(14) (e)

(e)

τ˜n+1 = µ|˜ σn+1 | sign(˜ γn+1 ) (˜ γn+1 = 2t · ∇S un+1 · n) where t stands for the tangent vector associated to the normal n in anticlockwise sense. Numerical Treatment Resolution of the variational problem (11), in the context of the ﬁnite element method, leads to the following expression for the equivalent nodal forces, Fcont , at the nodes i of the interface mesh, due to contact/friction actions: i δΠ = 0 ⇒ =− Fcont i

Bint n+1

(1)

∇Ni · σ n+1 dΩ

(2)

∀i ∈ ∂Bn+1 ∪ ∂Bn+1

(15) (e)

, Besides, it can be readily proven that the elemental counterparts, Fcont i of those contact/friction forces in a given element e, constitute a set of selfequilibrated forces: i=3 i=1

Fcont i

(e)

=−

(e) Bint n+1

(e)

∇Ni

(e)

· σ n+1 dΩ = 0

(16)

96

J. Oliver et al.

Fig. 5. Contact/friction eﬀects: interface constitutive model

which proves the self-equilibrated character of those forces as action-reactions (1) (2) at the contacting boundaries ∂Bn+1 and ∂Bn+1 , i.e.: (1) j∈∂Bn+1

Fcont + j

Fcont = j

(2) j∈∂Bn+1

i=3 e∈Bint n+1

Fcont i

(e)

=0

(17)

i=1

Finally, in view of the structure of the problem in equations (11), the con, once computed at every node of the interface tact/friction nodal forces, Fcont i mesh Bint according to equation (15), can be formally added to the original n+1 problem (1), for every contacting body, as external prescribed point forces acting on the boundary ∂σ Vn+1 . In this way, the contact/friction problem gets reduced to computing nodal/friction forces at all the generated interface meshes, and incorporating them, as external point forces, at the boundaries of the contacting classes. No additional degrees of freedom are involved.

4 Representative Examples In order to illustrate the modeling capacities of the methodology described so far, in next sections some applications to solid mechanics problems are presented. 4.1 Flexible Spring with Multiple Self-contacts In Figure 6 an elastic ﬂexible spring (Figure 6a) is pushed down vertically as to impose multiple contacts, as displayed in Figures 6b and 6c. In the ﬁgures,

Particle Finite Element Methods in Solid Mechanics Problems

97

Fig. 6. Flexible spring: (a) initial conﬁguration, (b) and (c) shrunk deformed conﬁgurations displaying the contact interfaces

the contact interface mesh is artiﬁcially ampliﬁed, for visualization purposes, and the contacting bodies are shrunk in correspondence.4 The actual contacts, keep very little gaps that would not allow that visualization. Two facts should be noticed there: •

The contact interface mesh only aﬀects a limited part of the boundary. This is ruled by the value of the alpha shape parameter precluding interface elements larger than the speciﬁed size.

4 This criterion will be kept from now on, to allow visualizing the contact interface mesh.

98

J. Oliver et al.

Fig. 7. Rivet forming. Top: Riveting parts. Bottom: (a), (b) and (c) deformed ﬁnite element mesh at diﬀerent stages of the forming process. At every stage: actual mesh (left) and shrunk mesh (right), showing the contact interface is displayed

•

Only few elements of the contact interface mesh are active in the sense that (e) (e) gn+1 = 0 ⇔ ε˜n+1 = 0 and, therefore, there is a positive reaction at the contact points according to equations (12) and (13). They are displayed in grey in Figure 6.

This example displays that multiple self-contacts, as the ones occurring in this problem, are trivially solved by the proposed procedure. 4.2 Riveting Process In Figure 7, the geometrical description of a metallic rivet, and the deformation of the ﬁnite element mesh (axisymmetric cross-section) for diﬀerent stages of the forming simulation process, are presented. This is a very representative example of application of the proposed methodology to a variety of metal forming processes.5 It is remarkable the capacity of the method to handle large strains in the deformed body, minimizing the angular distortions of the resulting ﬁnite element mesh. This is an advantageous property of the Delaunay triangulation based meshing procedure. 5 Certainly, the reliability of the simulation requires the use of appropriate constitutive models, typically J2 plasticity models and large strain kinematics.

Particle Finite Element Methods in Solid Mechanics Problems

99

Fig. 8. Machining process: (a) chip forming process, (b)–(e) particle conﬁgurations (left: actual particle conﬁgurations, right: shrunk ﬁnite element meshes displaying the anticipating contact interfaces)

100

J. Oliver et al.

Fig. 9. Filling of a two-stepped cavity with powder material: ﬁnite element meshes displaying the contact interfaces at diﬀerent stages

4.3 Machining Process In Figure 8, simulation of an orthogonal cutting process on a metallic part is considered. This is, again, a very illustrative example of the proposed methodology potential to handle challenging solid mechanics problems. In this case, the formation of the chip, very relevant for the quality of the mechanical process, generates a new boundary at the cutting tool edge. The alpha shape method automatically generates the new boundary as the deformed size at the elements, close to the cutting edge, exceeds the alpha-shape tolerance. The contact/friction model allows sliding the formed chip on the upper surface of the machined part. Both the boundary recognition and the imposition of the dynamic contacts are automatically done by the mesher. 4.4 Powder Filling Process There are many interesting solid mechanics processes, involving ﬂows of granular materials, where PFEM methods can be advantageously applied. Powder metallurgy manufacturing processes or casting processes are typical examples. In Figure 9 the numerical simulation of a powder ﬁlling process is presented using a speciﬁc solid-type constitutive model (Oliver et al., 1996; Cante

Particle Finite Element Methods in Solid Mechanics Problems

101

et al., 2005). The feeder moves horizontally, from left to right, dropping the powder into a two steps cavity. The goal of the analysis is to obtain, through a physically meaningful simulation of the process, the density distribution of the powder at the end of the process. This type of powder ﬁlling processes has been often modelled by the so called discrete element methods, on the basis of models made of a ﬁnite number of interacting balls or cylinders representing the powder grains (Wu et al., 2004; Coube et al., 2005). However, the large number of particles involved in the physical process translates into unaﬀordable computations when a realistic modelling is intended. Here, the powder is treated as a continuum medium, ruled by an elastoplastic constitutive model, and modelled via the PFEM by tracking a limited number of the constituent particles. In the ﬁgure it can be observed as the powder/tool contact conditions are correctly imposed by the contact interface (also displayed in the ﬁgure). In addition, the alpha shape method allows reproducing the complex dynamics of the generated free surface of the powder during the ﬁlling process.

5 Concluding Remarks In the previous sections, PFEM techniques applied to solid mechanics problems have been explored. In addition to their appealing properties, already explored for ﬂuid mechanics problems, some additional advantages can be obtained when they are applied to solids i.e.: •

•

•

Delaunay tessellation techniques, for constructing ﬁnite element meshes on the basis of the selected cloud of points, minimize the angular distortion eﬀects of the resulting elements, thus providing additional robustness to the modelling in problems dominated by large strains. The relatively low computational cost (Calvo et al., 2003) of those techniques allows frequent remeshing without leading to unaﬀordable computational costs. Alpha-shape techniques for boundary recognition purposes, constitute a powerful tool in those solid problems where new physical boundaries are generated (for instance, cutting processes) or when there is a continuous creation and disappearance of boundaries, as a natural part of the physics of the problem (i.e. powder ﬁlling processes). Contacting boundaries problems can be solved by constructing anticipating contact interfaces as it is presented in Section 3. Construction of those contact interfaces becomes an easy and automatic task by using, Delaunay tessellation techniques on the basis of particles of the contacting boundaries. Typical highly computationally demanding techniques, for recognizing point/segment contacts, can then be overcome by imposing the contact conditions on the generated contact interfaces by using, for instance, penalty techniques (Section 3.1). Then, friction eﬀects can be trivially implemented (Section 3.1.1). This confers larger computational eﬃciency and robustness to simulation of problems involving a large number of contacts.

102

J. Oliver et al.

Although the formulation, and the corresponding examples, has been here restricted to 2D cases, extension to 3D problems seems straightforward and in essence the beneﬁts of PFEM should be similar to the ones mentioned above.

Acknowledgements Financial support from the Spanish Ministry of Science and Technology trough grants DPI203-00629 and DPI2004-07666-C02-02 and the Catalan Department of Universities, Research and Society of Information (DURSI) through grant 2005SGR0084 are gratefully acknowledged.

References 1. Belytschko T, Krongauz Y, Organ D, Fleming M, Krysl P (1996) Meshless methods: An overview and recent developments. Comput. Meth. in Appl. Mech. Engng. 139:3-47 2. Belytschko T, Lu YY, Gu L (1994) Element-Free Galerkin Methods. International Journal for Numerical Methods in Engineering 37:229-256 3. Calvo N, Idelsohn SR, Onate E (2003) The extended Delaunany tessellation. Engineering Computations 20:583-600 4. Cante JC, Oliver J, Gonzalez C, Calero JA, Benitez F (2005) On numerical simulation of powder compaction processes: powder transfer modelling and characterisation. Powder Metallurgy 48:85-92 5. Coube O, Cocks ACF, Wu CY (2005) Experimental and numerical study of die ﬁlling, powder transfer and die compaction. Powder Metallurgy 48:68-76 6. George PL (1991) Automatic Mesh Generation, Applications to Finite Methods, New York, Wiley 7. Hughes TJR (2000) The Finite Element Method: Linear Static and Dynamic Finite Element Analysis, Mineola, NY, Dover Publications Inc 8. Idelsohn SR, Onate E, Calvo N, Del Pin F (2003a) The meshless ﬁnite element method. Int. J. Num. Meth. Engng. 58:893-912 9. Idelsohn SR, Onate E, Del Pin F (2003b) A Lagrangian meshless ﬁnite element method applied to ﬂuid-structure interaction problems. Computers & Structures 81:655-671 10. Idelsohn SR, Onate E, Del Pin F (2004) The particle ﬁnite element method: a powerful tool to solve incompressible ﬂows with free-surfaces and breaking waves. Int. J. Num. Meth. Engng. 61:964-989 11. Lohner R, Sacco C, Onate E, Idelsohn SR (2002) A ﬁnite point method for compressible ﬂow. Int. J. Num. Meth. Engng. 53:1765-1779 12. Malvern L (1969) Introduction to the Mechanics of a Continuous Medium. Englewood Cliﬀs, New Jersey, USA, Prentice-Hall 13. Oliver J, Oller S, Cante JC (1996) A plasticity model for simulation of industrial powder compaction processes. Int. J. Solids and Structures 33:3161-3178 14. Onate E, Idelsohn S (1998) A mesh-free ﬁnite point method for advectivediﬀusive transport and ﬂuid ﬂow problems. Comput. Mechanics 21: 283-292.

Particle Finite Element Methods in Solid Mechanics Problems

103

15. Onate E, Idelsohn SR, Zienkiewicz OC, Taylor RL (1996) A ﬁnite point method in computational mechanics. Applications to convective transport and ﬂuid ﬂow. Int. J. Num. Meth. Engng 39:3839-3866 16. Wu CY, Cocks ACF (2004) Flow behaviour of powders during die ﬁlling. Powder Metallurgy 47:127-136 17. Xu XL, Harada K (2003) Automatic surface reconstruction with alpha-shape method. Visual Computer.19:431-443 18. Zienkiewicz OC, Taylor RL (2000) The Finite Element Method. Oxford UK, Butterworth-Heinemann

Micro-Meso-Macro Modelling of Composite Materials P. Wriggers and M. Hain Institute of Mechanics and Computational Mechanics University of Hannover, Appelstr. 9a, 30167 Hannover, Germany [email protected] Summary. Multi-scale models can be helpful in the understanding of complex materials used in engineering practice. Applications related to this class of problems covers diﬀerent length scales in the range from µm to m. Using the concept of representative volume elements (RVE), the theoretical background is discussed in this contribution as well as the numerical treatment of the resulting three-dimensional RVEs. The developed methodology is applied to a speciﬁc engineering material which is concrete. This construction material has to be investigated on three diﬀerent scales: the hardened cement paste (hcp), the mortar and ﬁnally the concrete. Here, a successive two-stage approach is followed in which ﬁrst the multi-scale model of hcp and mortar is applied. The resulting homogenization can then be used in the next step for a multi-scale mortar-concrete model. At the micro-scale of hcp, a ﬁnite element mesh based on a three-dimensional computer-tomography with diﬀerent constitutive equations for the three parts unhydrated residual clinker, pores and hydrated products is introduced. With respect to the ﬁnite element solution, homogenization techniques are used in order to calculate eﬀective elastic material properties. The constitutive equations at the micro-scale contain inelastic parameters, which cannot be obtained through experimental testings. Therefore, one has to solve an inverse problem which yields the identiﬁcation of these properties. For computational eﬃciency and robustness, a combination of the stochastic genetic algorithm and the deterministic Levenberg-Marquardt method is used. In order to speedup the computation time signiﬁcantly, all calculations are distributed automatically within a network environment. Inelastic behavior occurs when the micro-structure hcp is ﬁlled partly with water and a freezing process takes place. A constitutive model for ice is applied to the water ﬁlled parts of the micro-structure. The expansion of the ice leads to damage in the hcp which is associated with inelastic material behavior. If such a calculation is performed for diﬀerent moisture and temperatures, a correlation between moisture, temperature and the inelastic material behavior can be obtained. The eﬀective constitutive equation of hcp will serve as a basis for a multi-scale mortar-concrete model.

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 105–122. © 2007 Springer. Printed in the Netherlands.

106

P. Wriggers and M. Hain

1 Introduction A deeper understanding of the constitutive behavior of complex materials such as concrete can be achieved on one hand by experimental investigations and on the other hand by numerical simulations. While the experimental techniques are applied successfully since several decades, the use of numerical simulation techniques is quite young. This is due to the fact that the underlying threedimensional models are very complex and need considerable computer power which only in the last decade has reached a suﬃcient state. The advantage of a numerical simulation is that one can look inside a specimen during the loading process and also is able to resolve fast processes on a diﬀerent time scale. Figure 1 depicts the multi-scale modeling process which can be used for a material like concrete. The underlying nano-scale is not considered in this contribution.

Fig. 1. Multi-scale model of concrete

Within the above mentioned multi-scale approach, diﬀerent three-dimensional mechanical models are applied on each length scale in order to describe the constitutive behavior on that scale. These are called representative volume elements (RVEs). Normally, the material on a speciﬁc length scale consists of diﬀerent phases which have to be taken into account in order to characterize the material with suﬃcient accuracy. The RVE is then subjected to diﬀerent loading conditions which lead to a material response. Based on these results a homogenization process can be initiated to describe the material behavior averaged over the whole RVE. The resulting homogenized constitutive equation is then applied within the the next scale to model the constituents of the RVE belonging to that scale.

Micro-Meso-Macro Modelling of Composite Materials

107

Fig. 2. Cut through of a CT-scan (1750 × 1750µm)

In this contribution, a multi-scale model for hardened cement paste (hcp) is introduced. The scale of the superior system is denoted meso-scale, the underlying microscopic system of hcp micro-scale [17], [5]. The homogenized properties of hcp serves as a basis for the constitutive model of mortar at the meso-scale.

2 Micro-structure of Hardened Cement Paste (hcp) The FE-analysis of hcp requires the discretization of the micro-structure. Here, the geometry on the micro-scale is obtained from a three-dimensional computer tomography (CT) which provides a spatial resolved distribution of the density. In this contribution, CT-scans of several specimens with an edge length of 1750µm and a resolution of 1µm have been performed by the Bundesanstalt f¨ ur Materialforschung und -pr¨ ufung in Berlin, Germany. The CT-scans have been applied for a hcp with the water-cement ratio of wc = 0.45 and a degree of hydration of h = 0.945. In Fig. 2 a cut through of such a CT-scan is shown. The unhydrated residual clinker is black and the hydrated part is middle gray colored. One can see the accumulation of pores, which are marked in light gray. Each CT-ﬁle contains 17503 data points (each corresponds to 1µm3 ) and allocates totally 5GB of memory. For the mechanical analysis, the surrounding synthetic tube is not relevant. Hence, only the interior part of the CT-scan is used for further mechanical simulations which contains 10083 data points (see Fig. 3). Due to noise, a median ﬁlter has to be applied to the raw data. Based on the theory of Powers and coworkers [13], [12] the fractional volume of the pores cp and the unhydrated residual clinker cu are calculated cp =

wc − 0.36h , wc + 0.32

cu =

0.32(1 − cp ) . wc + 0.32

(1)

108

P. Wriggers and M. Hain

Fig. 3. Cut through of the raw data (1008 × 1008µm)

N (d) 350000

pores

unhydr. residual clinker

300000 250000 200000 150000 100000 50000 0

50

100

150

200

Fig. 4. Histogram of the raw data

250

d

In order to distinguish unhydrated residual clinker, hydration products and porosity a histogram is generated, where N (d) describes the number of voxels at a speciﬁc density d (see Fig. 4). Threshold values for the pores and the unhydrated residual clinker are calculated with respect to (1). Hence, the raw data can be segmented in the hydrated part, unhydrated residual clinker and porosity. In Fig. 5 a cross section of the ﬁltered data is shown which is obtained from the raw data (see Fig. 3). The hydrated part has a volume fracture of 84Vol.%, the pores of approximately 14Vol.% and the unhydrated residual clinker of roughly 2Vol.%. The micro-structure of hcp can also be generated by simulating the chemical reactions of the hydration. Result of such a simulation is an artiﬁcial micro-structure with diﬀerent phases. The chemical reaction of the hydration can be simulated with respect to a cellular automata, as the programme from NIST does [6]. Herein, the whole micro-structure is divided into topological, geometrical and physical uniform cells. Each cell has an individual state, corresponding to its current property. A set of rules calculate the new state for each cell at time n + 1. The result of this calculation depends on the state at time n, the states of the neighbors and a random part. The rules are applied at the same time to all cells.

Micro-Meso-Macro Modelling of Composite Materials

109

Fig. 5. Cross section of the ﬁltered data (1008 × 1008µm)

Fig. 6. Simulated microstructure (128 × 128µm)

Fig. 7. CT-based microstructure (128 × 128µm)

If the hydration is simulated with the above mentioned cellular automata, one obtains a diﬀerent geometry as those obtained from CT-scans, compare Figs. 6 and 7. Due to the random based rules of the programme, the porosity is evenly distributed. There are no accumulations of pores as the corresponding CT-scan depicts, but for a reliable simulation of frost heave a proper geometry of the pores is necessary. Therefore, only CT-based micro-structures are applied within the further calculations.

3 Constitutive Equations Numerical results on the micro-scale are obtained by use of the ﬁnite element method which is applied to discretize the representative volume elements (RVEs). The RVEs are generated directly from the ﬁltered CT-data and have diﬀerent material properties for each phase. In this contribution RVEs with an edge length of 64µm are used. Since each voxel is represented by one ﬁnite element this leads to a 643 ﬁnite element mesh. Hence each RVE has about 800 000 degrees of freedoms (DOFs).

110

P. Wriggers and M. Hain

Fig. 8. Embedded RVE

Due to the diﬀerent properties classical constant strain boundary conditions – leading to Voigt bounds – will cause problems at the boundary. Constant stress boundary conditions – leading to Reuss bounds – are also not be used. Instead the RVEs are embedded in a matrix of average stiﬀness, see Fig. 8. This corresponds to the self-consistency method from analytical micro-mechanics and is sometimes referred to as window-technique. Material properties for the elastic behavior of the diﬀerent phases from hcp can directly be taken from the literature [1], [2], [3]. To avoid numerical problems and further mechanical inﬂuences the pores are described using an elastic material of negligible stiﬀness. With respect to the minor volume fraction, averaged properties can be chosen for the unhydrated phase. Table 1. Elastic properties of the phases E

phase

unhydrated phase hydrated phase pores

N mm2

ν −

≈ 132 700 20 000 1

0.30 0.21 0.00

Experimental tests of hcp show that the inelastic eﬀects of hcp are related to damage behavior combined with visco-plastic eﬀects. Due to that a model for the hydrated phase is selected which consists of a visco-plastic constitutive relation of the classical Perzyna-type combined with a damage model. Due to mechanical loading, cracks occur at the nano-scale. These nanocracks are statistically distributed and oriented, thus isotropic damage can be chosen for the micro-structure. Stress-strain relations for isotropic damage can be found in [9], here we select σ = (1 − D)C : .

(2)

Micro-Meso-Macro Modelling of Composite Materials

111

The scalar variable D describes the damage and C refers to the material tensor of the undamaged elastic material. An evolution law for the damage variable ∂S(eq ) (3) D˙ = ∆ξ ∂eq and a damage surface S(eq ) are introduced. The damage surface determines, whether the damage increases or not. It is deﬁned by an exponential relation and depends on the equivalent strain eq . The parameter a, b and c constitute the material properties of this model c eq −a S(eq ) := 1 − exp − −D 0. (4) b For the visco-plastic part, a penalty formulation P is introduced, see e.g. [14], based on the second fundamental theorem of thermodynamics. Here, the scalar variable η describes the viscosity, φ(f ) denotes a penalty-function of power type P = σ : ˙ pl + η1 φ(f ) , 0 ;f ≤ 0 . φ(f ) = 1 m+1 f ;f > 0 m+1

(5)

In order to keep the constitutive model at the micro-scale as simple as possible, a Drucker-Prager model with the yield surface f is chosen. Therefore, diﬀerent behavior of hcp in compression and tension can be described (6) f := αtr σ + dev σ − 23 kf ≤ 0 . Within the associated theory of visco-plasticity, the evolution equation for ∂f has to be integrated. Here we apply an the inelastic strains ˙pl = ∆λ˙ ∂σ Euler backward integration leading to ∂f pl pl n+1 = n + ∆λ . (7) ∂σ n+1 The increment ∆λ = Newton-scheme

∆t + η φ

is locally, at every Gauss point, calculated by a

∆λk+1 = ∆λk −

∂Gk ∂∆λk

−1

Gk ,

(8)

where Gk describes the nonlinear equation resulting from the evaluation of (5) and (6) m η∆λk ! − f trial − 9α2 κ∆λk − 2µ∆λk =0. (9) Gk = ∆t For computational eﬃciency, the above mentioned set of constitutive equations is linearized consistently.

112

P. Wriggers and M. Hain

4 Homogenization In order to determine eﬀective elastic material properties for each RVE, homogenization is needed and the eﬀective material tensor has to be calculated. The eﬀective material tensor C eﬀ maps the average of the strains (eﬀective strains) onto the average of the stress σ (eﬀective stresses) by σ = C eﬀ : ,

(10)

where • denotes the volume average within the RVE, Ω being the volume of the RVE. 1 • dΩ . (11) • = |Ω| Ω

In order to calculate the eﬀective stresses and strains, one has to deﬁne boundary conditions and solve the boundary value problem on the micro-scale. The latter will be performed by using ﬁnite elements. Since the application of a pure stress ﬁeld to the RVE leads to some diﬃculties regarding the suppression of rigid body modes, we apply here only pure displacement boundary conditions (constant stress state). Subsequently, the volume average of the strain can be evaluated from the ﬁnite element solution of the RVE by ne 1 h dΩ (12) = Ωe e=1 Ωe

where h is the strain computed from the ﬁnite element solution, Ωe the volume of a ﬁnite element and ne the total number of ﬁnite elements of the RVE. The same relation holds for the computation average of the stresses. Once the eﬀective strains and stresses are known the eﬀective material tensor C eﬀ can be computed within the homogenization step. In this this step a linear elastic eﬀective material of σ() = λeﬀ tr 1 + 2µeﬀ is chosen. A least square functional is introduced to ﬁt the averaged stresses with those obtained from the eﬀective constitutive equation σ() Π := σ − σ() → min .

(13)

The diﬀerentiation of this relation with respect to the eﬀective material properties yields a symmetric linear equation for the two Lame constants λeﬀ and µeﬀ 2 λeﬀ 2tr tr σ 6tr 4tr 2 · = . (14) µeﬀ 4σ : 4tr 2 8 : Due to the randomly distributed phases within the micro-structure of hcp, a Monte Carlo method was selected to compute the average values for the constitutive parameters. Hence a suﬃciently large number of diﬀerent RVEs has

Micro-Meso-Macro Modelling of Composite Materials W

113

W

0.8 0.8 0.6 0.6 0.4 0.4 0.2 0.2 80

10

12

14

16

18

20

22

24 eﬀ kN E mm2

Fig. 9. Probability density of Eeﬀ

0.2

0.205

0.21

0.215

0.22

0.225

ν eﬀ [−]

Fig. 10. Probability density of µeﬀ

to be investigated. Each homogenization yields the eﬀective material properties λeﬀ and µeﬀ of the speciﬁc RVE. Therefore, one obtains statistical distributed eﬀective parameters, e.g. a probability density. The probability density W of the eﬀective Young‘s modulus Eeﬀ and effective Poisson‘s ratio µeﬀ are shown in Figs. 9 and 10 for a set of 9200 RVEs, respectively. Both are close to a Gaussian distribution (dashed lines). Furthermore, the above mentioned numerical results are in excellent agreement with results obtained from experimental tests of hcp, see Table 2. Table 2. Experimental versus numerical results test

numerical experimental series 1 experimental series 2

med Eeﬀ

med νeﬀ

N mm2

−

17 665 17 455 17 727

0.211 0.210 0.210

By applying loading in diﬀerent directions one can test whether the material response of a RVE is isotropic or anisotropic. For loadings only in the x-direction (constant strain xx ), the above mentioned homogenization procedure yields nearly the same results as for simultaneously loading in x, y and z-direction (full strain tensor). The same holds for loadings only in the y or z-direction (see Table 3). This depicts clearly that the response of the micro-structure (RVE) is isotropic. This result corresponds to the irregular geometry of the phases and the large number of ﬁnite elements for each RVE. The above mentioned homogenization is a result from a real multi-scale approach. The geometry has been obtained from CT-scans of hcp. The material properties of the diﬀerent phases of the RVE were taken directly from the literature, without any modiﬁcation. The accuracy of this procedure is very good since the eﬀective properties, obtained numerically, agree excellently with results from experimental tests.

114

P. Wriggers and M. Hain Table 3. Results for diﬀerent loadings loading direction

every direction only x-direction only y-direction only z-direction

Eeﬀ

νeﬀ

N mm2

−

17 665 17 952 17 779 17 740

0.2107 0.2108 0.2110 0.2100

5 Parameter Identification The inelastic material model on the micro-scale described in Section 3 contains constitutive parameters κ, which neither can be found in the literature, nor obtained through experimental testing. Therefore, one has to compute these by parameter identiﬁcation. The displacement of the micro-structure u(κ) depends, under a given loading, upon the unknown material properties. For an assumed constitutive model, see Section 3, the material parameters can be identiﬁed. The identiﬁcation of these parameters is carried out, such that the displacements u(κ) from the numerical simulation ﬁt with the displacements d from an experimental test. This yields an ill-posed inverse problem which cannot be solved directly. Instead, an optimization problem is carried out. The material parameters of the constitutive model presented in Section 3 have to be calculated, such that an objective function is minimized. The objective function A is deﬁned by a least-square sum between each numerical and experimental value A(κ) =

n

u(κ)i − di

2

→ min .

(15)

i=1

The identiﬁcation is obtained by solving the above mentioned optimization problem. For computational eﬃciency and robustness, a combination of the stochastic genetic algorithm [16], [15] and the deterministic LevenbergMarquardt method is used [4]. Here, the gradient information of the objective function is obtained numerically from a central diﬀerence quotient A(κ + ei ) − A(κ − ei ) . (16) 2 In a ﬁrst step a pre-optimization with a genetic algorithm is performed in order to get close to the global minimum. Once the value of the objective function falls below a certain threshold value, the optimization procedure switches to the more eﬃcient Levenberg-Marquardt method. Due to the complex micro-structure, the inelastic material behavior and the large number of loading steps, each examination of the objective function A(κ) needs approximately 12 hours on a standard PC computer system. ∇κ A(κ)i ≈

σ33

N mm2

Micro-Meso-Macro Modelling of Composite Materials

−10 −20

115

experimental curve numerical fit

−30 −40 −50 −60 −70 −80 −0.006

−0.005

−0.004

−0.003

−0.002

−0.001 33 [−]

Fig. 11. Numerical ﬁt of the experimental data

Therefore, a typical parameter identiﬁcation with 120 evaluations requires roughly two month CPU time on a modern standard computer. In order to keep the overall computing time within reasonable bounds, the calculations, which can be performed stand alone, are distributed within a network environment. A client-server based system has been implemented, a detailed introduction of those systems can be found in [11]. For the optimization procedure, a client is started. This client does not evaluate the objective function itself, but distributes the computation to the compute-servers via a network connection. The evaluation of the objective function A(κ) is performed on those servers. Once the necessary output data is produced on the servers, it is transported back to the client automatically. The results are then used on the client for the next iteration step of the optimization procedure. Within the network environment using 11 standard computers, the identiﬁcation can be completed within six days. This yields a speed-up factor of approximately 10. In Fig. 11 a result of the parameter identiﬁcation is shown. One can see a satisfying accuracy between the experimental and the numerical results. The experimental load-deﬂection curve varies with respect to diﬀerent specimens, therefore it is not reasonable to ﬁt the experimental data more exactly. The identiﬁed parameters are presented in the subsequent table. The properties marked with • have not been identiﬁed, but were chosen in advance. They describe the exponent of the equivalent strain and the penalty function, respectively. For their deﬁnition see Section 3. A real multi-scale approach cannot be set up for the inelastic behavior since there do not exist experimental tests which yield values for the constitutive behaviour of the diﬀerent phases within the micro-structure. Only eﬀective load-deﬂection curves can be obtained through experiments. In order to get the desired inelastic properties of the micro-structure, one has to solve the inverse problem via parameter identiﬁcation. Hence, the experimental eﬀective behavior is used to calculate the inelastic properties at the micro-scale which

116

P. Wriggers and M. Hain Table 4. Identiﬁed parameters parameter value a b c α kf m η

0.488 0.1 3.0 0.538 48.27 3 84 650

is not a multi-scale approach. However, the obtained inelastic constitutive data for the micro-structure are needed within the next step which then is related to a multi-scale approach.

6 Thermo-mechanical Coupling Hardened cement past is a part of mortar which in itself is part of concrete. Concrete structures are often subjected to ﬂuids such as rain. When this water permeates into the concrete, it actually ﬁlls the pores of the hcp to a certain degree. In freezing condition this water changes its phase to ice and with it expands. This expansion process may lead to damage in some parts of hcp. This process will be investigated in this section. For that we have to know the water contents of the hcp, its constitutive behaviour, see last section, and the constitutive behaviour of the ice which depends on temperature. A numerical simulation of this process has to take into account thermal eﬀects besides the mechanical ones. Considerable work related to the simulation of water permeability and water vapor diﬀusion in hcp has been performed in [8]. These results are used in the further calculations to obtain a realistic distribution of water on the micro-structural level. In Figs. 12-15 cuts through the RVE with diﬀerent moisture contents wh are shown. The water ﬁlled parts of the micro-structure are colored in blue. As expected the water prefers the boundaries of a pore. For the coupled thermo-mechanical simulation, transient thermal conduction is introduced. The mechanical and the thermal behavior is coupled in a weak sense. We assume that cooling down of hcp leads to strains, but strains due to mechanical loading do not change the temperature. The strains are separated into a mechanical part u and a thermal part in an additive way (17) = u + αt (Θ − Θ0 )1 . The parameter αt denotes the coeﬃcient of thermal expansion. With respect to the above mentioned split, the weak form of the internal part of the

Micro-Meso-Macro Modelling of Composite Materials

117

Fig. 12. Cut through of a RVE, wh = 80% (64 × 64µm)

Fig. 13. Cut through of a RVE, wh = 85% (64 × 64µm)

Fig. 14. Cut through of a RVE, wh = 90% (64 × 64µm)

Fig. 15. Cut through of a RVE, wh = 95% (64 × 64µm)

mechanical equilibrium is given by

Gu = grad η u : C : − αt (Θ − Θ0 )1 dΩ . int

(18)

Ω

Hence, the mechanical equilibrium depends both on the temperature Θ and the displacement u (19) Gu = Gu (Θ, u) while the thermal weak form only depends on the temperature GΘ = GΘ (Θ) .

(20)

The linearization and subsequent discretization of the thermal and mechanical weak yields the tangential stiﬀness matrix for the ﬁnite element method. It contains of the sub-matrices of the thermal and of the mechanical problem K uu K uΘ ∆u Gu =− (21) 0 K ΘΘ GΘ ∆Θ The thermo-mechanical coupling is described by the couple-matrix K uΘ .

118

P. Wriggers and M. Hain

In general it is possible to subject the RVE to thermal and mechanical loading conditions which leads to a speciﬁc material response. For this analysis a constitutive model for ice has to be introduced and applied to the water ﬁlled parts of the micro-structure. In this contribution, the micro-structural ice is assumed to have the same properties as macroscopic ice. The material model for ice is chosen as visco-plastic model of Perzyna type (see section 3) and is coupled thermo-mechanically. The previously mentioned expansion of ice is described through a negative coeﬃcient of thermal expansion αt . In this contribution Young‘s modulus of ice is assumed to depend on the current temperature. The other constitutive parameters µ, kf , α and ν are assumed to be constant. It is well known that water ﬁlled pores with a hydraulic diameter of r < 0.5µm freeze at temperatures of Θ ≈ −20◦ C. The pores in the micro-structure of hcp have this size. Hence Young‘s modulus of ice reaches a certain limiting value E∞ which is kept constant below this temperature E∞ ; Θ ≤ −20◦ C E= . (22) ≈ 0 ; Θ ≥ 0◦ C In order to describe this experimental evidence an equation is introduced in which Young’s modulus depends upon the temperature and the four constitutive parameters E0 , E∞ , e and f . E ∞ − E0 Θ−f E(Θ) := E0 + exp 1 − exp . (23) e e The parameter E0 describes the stiﬀness of unfrozen ice (respectively water) and has a negligible value. E∞ denotes the stiﬀness of ice. The parameters e and f eﬀect the development of Young‘s modulus and are selected such that the stiﬀness E∞ is reached at a temperature of Θ ≈ −20◦ C (see Fig. 16). Within the analysis of the damage due to frost within the hcp the constitutive equation for ice is applied to the water ﬁlled pores of hcp. The material properties of ice are given in the Table 5. They are taken directly from the literature, see e.g. [7]. The properties indicated with • are chosen in order to describe the temperature dependency of Young‘s modulus using (23). Within the numerical simulations thermal loading is increased linearly such that the temperature inside the micro-structure reaches Θ ≈ −20◦ C. Mechanical loadings are not applied within this investigation. However they are present e.g. due to dead loads and have to be considered for a determination of damage within hcp in a real structure. Here we want to compare with experiments of hcp in which we can neglect these loads. For the mechanical properties of hcp the identiﬁed parameters from Section 5 are used. The principal stress due to thermal expansion is depicted in Fig. 17. Compression stress is marked in dark gray and tension stress in light gray. Obviously, the water ﬁlled pores are in compression state due to the expansion of ice.

E

N mm2

Micro-Meso-Macro Modelling of Composite Materials

119

3000 2500 2000 1500 1000 500 0

−25

−20

−15

−10

−5

0

5 Θ[◦ C]

Fig. 16. Temperature dependency of Young‘s modulus (e = 2.5, f = −5.0)

Table 5. Material properties for ice parameter value E0 E∞ ν kf α η m e f

1.0 3 500 0.35 1.633 0.333 1.0 0 2.5 -5.0

The thermal loading (freezing) leads to damage in the micro-structure and hence is related to an inelastic material response. For the given loading, one can observe damage zones in Fig. 6. The undamaged material is marked in light gray and the damaged material in dark gray. As one can expect, damage occurs between the water ﬁlled pores and will reduce the load carrying capacity of the hcp and thus the mortar. So far these simulations have only be performed for one sample related to the degree of water ﬁlling. Hence these results can be used to understand the mechanical behaviour of the freezing process, but not for quantitative evaluations leading to new constitutive relations for the eﬀective material properties. For this purpose statistical computations have to be made with diﬀerent samples as performed in section 4. Based on such statistical evaluations we will compare the numerical results with those obtained from experimental tests of frozen hcp in future research.

120

P. Wriggers and M. Hain

Fig. 17. Principal stress due to frost

Fig. 18. Damage due to frost

When the above mentioned numerical simulations are performed for different moisture and temperatures states, a correlation between moisture, temperature and inelastic material behavior is obtained. In order to describe such inelastic mechanical phenomena at the meso-scale, an eﬀective material model has to be constructed. In such meso-scale model the constitutive parameters have to depend now upon the mechanical strains, the moisture and the temperature. Results for two diﬀerent degrees of moisture are depicted in Fig. 19. From such numerical simulation one obtains the development of the eﬀective damage variable D as a function of the eﬀective temperature Θ. The eﬀective values are computed within the RVE by volume averaging of the local damage and local temperature using the procedure described in equation (12). Such curves have now to be computed for diﬀerent degrees of moisture in order to get a function on meso-scale which relates the state of eﬀective damage to temperature and moisture.

7 Outlook On the next length scale, a model for mortar will be introduced. This model consists of an eﬀective material for hcp, aggregates, pores and the cohesive zone around the aggregates. The geometry of mortar will be based on CTscans. But additionally, a generated structure of mortar is also used. A particle generator has been implemented, which shuﬄes spherical particles in order to get close to a given sieve curve (see Fig. 20). With respect to this particle distribution, one obtains an artiﬁcial mortar. Further comparisons with CTscans will prove, if such an artiﬁcial structure is realistically. A corresponding FE-mesh is generated using the hanging nodes technique. The hanging node technique leads to a more accurate mesh without any dis-

Micro-Meso-Macro Modelling of Composite Materials

121

Fig. 19. Damage evolution due to frost

Fig. 20. Generated particle distribution

Fig. 21. Damage in artiﬁcial mortar

torted elements. In a ﬁrst approach the aggregates are described with an elastic constitutive equation and the cohesive zone is neglected. Further research will prove, if these assumptions yield reliable results. Due to mechanical loading, damage zones occur between the aggregates. A ﬁrst result was calculated in [10] and is shown in Fig. 21. As expected, damage zones occur around the particles. Further research will compare those numerical results with accompanying experimental tests of mortar.

Acknowledgments Financial support from the Deutsche Forschungsgemeinschaft (German Research Council) DFG is gratefully appreciated. All experimental results of hcp

122

P. Wriggers and M. Hain

were performed by the Institut f¨ ur Bauforschung (director Prof. Brameshuber) at Aachen, Germany. The Bundesanstalt f¨ ur Materialforschung und -pr¨ ufung in Berlin, Germany provides the CT-scans of hcp.

References 1. Acker P (2001) Micromechanical analysis of creep and shrinkage mechanisms. Creep, Shrinkage and Durability Mechanics of Concrete and other Quasi-Brittle materials: proceedings of the sixth international conference 1:15–25 2. Bernard O, Ulm F-J, Lemarchand E (2003) A multiscale micromechanicshydration model for the early-age elastic properties of cement-based materials. Cement and Concrete Research 33:1293–1309 3. Constantinides G, Ulm F-J (2004) The eﬀect of two types of csh on the elasticity of cement-based materials: Results from nanoindentation and micromechanical modeling. Cement and Concrete Research 34:67–80 4. Geiger C, Kanzow C (1999) Numerische Verfahren zur L¨ osung unrestringierter Optimierungsaufgaben. Springer Verlag 5. Gross D, Seelig T (2001) Bruchmechanik. Springer Verlag 6. Internetlink. National institute of standards and technology; http://ﬁre.nist.gov/bfrlpubs/build00/art060.html. 7. Kolari K, Kouhia R, K¨ arn¨ a T (2002) Ice failure simulation–softening material model. Proceedings of the 16th IAHR International Symposium on Ice, Dunedin, New Zealand, pages 154–159 8. Koster M, Hannawald J, Brameshuber W (2006) Simulation of water permeability and water vapor diﬀusion through hardened cement paste. Computational Mechanics 37(2):163–172 9. Lemaitre J (1996) A course on damage mechanics. Springer Verlag 10. L¨ ohnert S (2004) Computational homogenization of microheterogeneous materials at ﬁnite strains including damage. PhD thesis, Universit¨ at Hannover 11. Pollakowski M (2004) Grundkurs Socketprogrammierung mit C unter Linux. Vieweg Verlag 12. Powers TC (1962) Physical properties of cement paste. Proceedings of the Fourth International Symposium on the Chemistry of Cement; Paper V-1: Physical Properties of Cement Paste 2(43):577–613 13. Powers TC, Brownyard TL (1948) Studies of the physical properties of hardened portland cement paste. Research Laboratories of the Portland Cement Association Bulletin 22:101–992 14. Simo JC, Hughes TJR (1998) Computational Inelasticity. Springer, New York, Berlin 15. Thielecke F (1997) Parameteridentiﬁzierung von Simulationsmodellen f¨ ur das viskoplastische Verhalten von Metallen -Theorie, Numerik, Anwendung-. PhD thesis, Technische Universit¨ at Braunschweig 16. Wedemeier K (1990) Beitr¨ age zur Theorie und Numerik von Materialien mit innerer Reibung am Beispiel des Werkstoﬀes Beton. PhD thesis, Universit¨ at Hannover 17. Zohdi TI, Wriggers P (2004) An Introduction to Computational Micromechanics. Springer Verlag, New York

Numerical Modeling of Transient Impact Processes with Large Deformations and Nonlinear Material Behavior Ekkehard Ramm1 , Tobias Erhart2 and Wolfgang A. Wall3 1

2 3

Institute of Structural Mechanics, University of Stuttgart, Pfaﬀenwaldring 7, 70569 Stuttgart, Germany [email protected] DYNAmore GmbH, Industriestr. 2, 70565 Stuttgart, Germany [email protected]e Chair for Computational Mechanics, Technical University of Munich, Boltzmannstr. 15, 85748 Garching, Germany [email protected]

Summary. A robust computational approach for transient dynamic impact processes will be presented. Main focus will be on an adaptive remeshing strategy and constitutive models for metals and geomaterials under impact loading. Practical relevant numerical examples will complete this contribution. Key words: Impact, Large Deformations, Adaptive Remeshing, Metals, Geomaterials

1 Introduction The present study is concerned with a special case of solid mechanics, where structures are exposed to short-time, highly concentrated loading. Such transient impact processes appear in civil and military security technology, dynamic soil compaction, vehicle crash or fastening and demolition technology. They are characterized by varying non-linearities, as e.g. large deformations and strains, highly non-linear material behavior, frictional contact between multiple bodies and stress wave propagation. Development and combination of diﬀerent methods in the ﬁelds of adaptivity, constitutive modeling, element technology, eﬃcient time discretization and contact are essential for reliable computations and predictions in engineering practice. Accuracy, robustness and eﬃciency are mandatory requirements for the solution of those complex problems. In this contribution, we will mainly focus on two issues, namely adaptive remeshing and constitutive modeling of metals and geomaterials especially Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 123–144. © 2007 Springer. Printed in the Netherlands.

124

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

elaborated for impact loading. The proposed methods are tested for model problems and their performance in relevant industrial applications is veriﬁed.

2 Class of Problems The speciﬁc class of problems focussed in this study excel themselves through a large complexity. Essentially these are fast transient plane strain or axisymmetric problems that are treated in an explicit way. Adopted material models range from simple elastic up to large strain thermo-elastic-viscoplastic models. The problems exhibit large deformations and may even include severe mesh distortion. Frictional contact is an essential feature of the related physical processes.

3 Adaptive Remeshing Since large deformations occur in impact simulations and a Lagrangean description is used, repeated remeshing of individual domains is necessary [6] [21]. To achieve a quality controlled solution and an optimal deployment of used computational resources at the same time, an adaptive strategy is applied [12]. The essential ingredients of an adaptive remeshing strategy in this highly nonlinear regime are (i) a mesh quality check for triggering automatic remeshing, (ii) a reasonable assessment of discretization errors and derivation of a corresponding mesh density distribution, (iii) an automatic mesh generation tool for graded meshes and (iv) methods for the transfer of state variables from old to new discretization. The core of this strategy is the assessment of discretization errors by adequate indicators. Diﬀerent indicators are presented and new methods are developed, which are especially suited for the simulation of transient impact processes. Theoretical deﬁnitions and numerical treatment of these aspects are dealt with. 3.1 Mesh Quality Check In our approach, mesh quality is evaluated for each element by a combination of two geometrical criteria, the so-called ’corner angle criterion’ and the ratio of the radius of the inscribed circle to the radius of the circumscribed circle [12]. If the combination of these two measures, e.g. the mean value falls below a prescribed threshold value for a prescribed number of elements, the remeshing procedure starts automatically. With this mesh quality check, it is guaranteed, that the FE solution is prevented from occurence of a negative Jacobian. 3.2 Error Assessment and Mesh Density Distribution In our approach, three categories of error indicators, gradient-based, local quantity-based as well as geometric, are used for adaptive remeshing [12]. In the following, all indicators that have been studied and implemented are

Numerical Modeling of Transient Impact Processes

125

presented in more detail along with their associated reﬁnement strategy, i.e. the determination of a corresponding mesh density distribution. Gradient-Based Indicators Gradient-based indicators use the fact that there is a connection between the size of local gradients and the quality of solution. Here, ’gradients’ not only mean stresses, but local variations of arbitrary quantitites like strains, plastic work, etc.. The corresponding adaptive remeshing strategy is characterized by an equi-distribution - with respect to the element length - of those gradients in the domain of solution. This leads to a reﬁnement in high gradient zones on the one hand and to a coarsening in low gradient areas on the other hand. Now the question is, which relevant quantities for the gradient calculation should be used to indicate a meaningful error and subsequently govern the mesh density? We have chosen two diﬀerent elastic and one plastic variable, whose gradients are tightly connected to some of the speciﬁc physical phenomena or processes occurring in complex problems like in our applications, depending on the speciﬁc example at hand. The ﬁrst quantity is the von Mises stress (1) ψ1 := µ 2(dev(e ) : dev(e )) which especially tracks elastic shape changing behavior, whereas the second one, the hydrostatic stress (2) ψ2 := κ tr(e ) mainly grasps elastic volumetric changes. Plastic regions in a structure, e.g. localization zones, can be detected with the third quantity ’plastic work’ t ψ3 := J −1 τ : ˙ p dt (3) t0

Gradients of these quantities need to be calculated at all nodes of the old mesh. Therefore, the superconvergent patch recovery technique in an element patch [31] is used to get information about the local gradient at the particular assembly node, i.e. the central node of the patch. According to this method, a least square ﬁt between a polynomial approximation and discrete values (e.g. at quadrature points) leads to a minimization problem. After solution of the corresponding system of linear equations, the norm of the gradient can be calculated at the position of node N (central node of patch) gk := ∇ψk (xN ) = (∇ψk (xN ) · ∇ψk (xN ))

1/2

(4)

The local element size of the new mesh has to be inversely proportional to the size of the local gradient due to the above mentioned reasons. In addition, the magnitude of reﬁnement needs to be controlled in order to adapt the element sizes to the diﬀerent indicator and/or examples. This can be achieved

126

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

by scaling the gradient with a prescribed value ∆ψk , which describes the maximal allowed change of the considered quantity ψk per element. At the end the new element size hnew e,k results in hnew e,k =

∆ψk gk

(5)

Local Quantity Indicators On the basis of pure physical considerations, local reﬁnement indicators can be developed that control the mesh density in the interior mesh. For this purpose, a physically relevant quantity is calculated for each element in the old mesh. The new mesh is then generated provided that this quantity becomes equi-distributed so that every element experiences roughly the same ’physical action’. This obviously results in reﬁnement for high values and in coarsening for small values of this quantity per old element. For these indicators, no gradients need to be calculated. In the following we sketch some of these local quantity indicators that are given in the literature and that we adopted for our study. For problems of strain localization, Ortiz and Quigley [19] proposed an adaptive strategy, which is based on the equi-distribution of variation of the velocity ﬁeld v over the elements of the mesh. Such localization problems can be characterized by large diﬀerences between the mechanical behavior of the global structure and a local zone, e. g. shear bands, bringing along a loss of ellipticity of the governing equations. For a two-dimensional element, this indicator can be expressed as the maximum deviation for the velocity vi of two nodes a and b e e − vib |} (6) φ1 := max{max |via i

a,b

This is a suitable indicator for the analysis of transient processes with wave propagation as well as localization. It is however restricted to dynamic calculations. Singularities in quasi-static zones of transient problems or poor approximations of quasi-static quantities are not treated appropriately. Another physical indicator was used by Batra and Ko [2] for shear bands in plane strain compression and by Camacho and Ortiz [6] for diﬀerent impact and penetration calculations. The intention of this indicator is that the integral of the second invariant of the deviatoric strain-rate tensor over an element 1 dev˙ : dev˙ dv (7) φ2 := 2 ϕ(Ωe ) is the same for all elements. This indicator is capable of resolving strain localizations in dynamic calculations. A third indicator, based on the equi-distribution of plastic power, was developed by Marusich and Ortiz [17] for simulation of high-speed machining: p ˙ J −1 τ : ˙ p dv (8) W dv = φ3 := ϕ(Ωe )

ϕ(Ωe )

Numerical Modeling of Transient Impact Processes

127

This indicator is especially suited for nonlinear, highly dynamic problems with large plastic deformations, since it leads to reﬁnement in high strain rate regions. In order to be able to combine diﬀerent indicators later, we adopt here a similar strategy as before. At ﬁrst, the elementwise calculated quantities φl are related to the respective old element size hold e g˜l =

φl hold e

(9)

Now we use the same reﬁnement strategy as we did for the gradient-based error indicators, i.e. the new element size is inversely proportional to the ’variation per element’ g˜l and it is scaled by a prescribed value ∆φl hnew e,l =

∆φl g˜l

(10)

Geometric Indicator Strongly curved surfaces have to be discretized with suﬃciently small elements to avoid signiﬁcant ’geometrical errors’. This is especially important with respect to mass conservation and in contact situations. The curvature of the boundary is used as a geometric indicator to control this problem. However, this indicator is only activated if it suggests reﬁnement of the ’mechanical’ indicator driven mesh density. In case of a discrete boundary description, e.g. the polygonal boundary of a ﬁnite element mesh, the discrete curvature κh at the position of a ﬁnite element node is given as κh :=

2ϑ s1 + s2

(11)

where ϑ is the smaller angle between two boundary segments with lengths s1 and s2 , respectively. If this measure is calculated for boundary nodes of the old mesh, the element size in the new mesh results in hnew e,g =

ϑadm κh

(12)

where ϑadm is a prescribed value, which can be interpreted as admissible angle between two adjacent boundary segments. A similar indicator was used by Camacho and Ortiz [9]. In general, through application of this indicator, there is no connection between internal element size and boundary element size. In such cases, a mesh smoothing technique is used to avoid large diﬀerences between element sizes in the interior and at the boundary. Selection of Indicators and Final Mesh Density Distribution The objective of the diﬀerent indicators and possible application areas have been given above. For real and complex applications the question of the ﬁnal selection of indicator remains. Which speciﬁc indicator or combination of

128

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

diﬀerent indicators should be used? The answer is both trivial and diﬃcult at the same time. It should be rather clear from the above discussion which indicators are not suited in which cases. The ﬁnal selection however can only be based on engineering intuition and on a deep insight into the physics of the problem or the class of problems. It is crucial to know what the governing phenomena and the dominating processes are. One should be aware that the answers not only depend on the problem itself but also on the respective quantities of interest of a speciﬁc simulation. To obtain the ﬁnal mesh density, two further steps are needed. As already pointed out it is in some cases useful to combine diﬀerent error indicators. For this purpose, the minimum of the diﬀerent element sizes hnew e,k (which be(which belong to the three long to the ﬁve gradient-based indicators), hnew e,l (the geometric indicator for the boundary) local quantity indicators) and hnew e,g has to be chosen as ﬁnal element size new new = min{hnew hnew e e,k , he,l , he,g }

(13)

On the other hand, the element size has to be restricted by some prescribed threshold values, because undesirably small elements (time step size in explicit scheme!) or large elements (approximation quality!) should be avoided: ≤ hnew ≤ hmax hmin e e e

(14)

3.3 Mesh Generation Generating a graded mesh needs two sources of information: the boundary of the domain and the mesh density inside the domain mostly given on a background mesh. In our case of large deformations and changing topologies the background mesh is preferably the old mesh of the preceding time step, for which the error assessment is done and the mesh density distribution is calculated. Secondly, a polygonal description of the boundary has to be provided. Boundary nodes must be generated adaptively, i.e. subject to the calculated mesh density. Special care has to be taken of boundaries in contact situations. The re-ordering of nodes on convexly curved boundaries during remeshing can result in sudden gaps between contacting bodies, which results in socalled ’remeshing shocks’: oscillations induced by unphysically high contact forces. This is remedied by a smooth contact formulation combined with a procedure for precise surface recovery [9]. After that, a new ’almost-all-quad’ mesh is generated inside the domain by an ’advancing front method’ starting from these previously generated boundary nodes and based on the given mesh density found at the nodes of the old mesh [16] [20]. In exceptional cases, e.g. for sharp corners, triangular elements (e.g. CST - constant strain triangles) are also allowed. This has the advantage, that no ’bad quads’ have to be generated and therefore the time span until next remeshing is increased.

Numerical Modeling of Transient Impact Processes

129

3.4 Transfer of State Variables Since results are determined in an iterative or in an incremental process for nonlinear or transient problems, a transfer of state variables between old and new spatial discretization is essential [21] [6]. Examples of variables, which have to be ’mapped’ are strains, stresses, velocities, boundary conditions, etc., i.e. a mapping strategy for both nodal and integration point data is needed. The location and number of nodes and integration points changes totally in case of complete remeshing of a domain. Therefore, the location of new points in the old mesh has to be determined by an intelligent search algorithm, e.g. directional search [20], and thereafter, state variables have to be transfered by a suitable mapping method like inter/extrapolation [21], inverse distance weighting [8] or moving least square techniques [31] [26]. Especially in the context of explicit time integration the quality of the mapping scheme is crucial. Since mapping cannot be supplemented by equilibrium iterations in these cases mapping errors may propagate and pollute the whole simulation. Other aspects like minimization of diﬀusion should be met as in implicit situations.

4 Constitutive Modeling Based on the theory of ﬁnite plasticity, constitutive models for thermoviscoplastic metals and cohesive as well as non-cohesive frictional materials are presented and developed. One focus will be on a formulation for loose, granular media under high pressure loadings. For this a Drucker-Prager-Cap model is modiﬁed and enhanced. The properties and eﬀects of the developing powder will be examined. Our implementation of ﬁnite strain plasticity is based on the multiplicative split of the deformation gradient into elastic and plastic parts F = Fe Fp and an isotropic Eulerian formulation in eigenvalues [24] [23] [18]. Using a spectral decomposition of the Finger-tensor b = FFT and the Kirchhoﬀ stress tensor τ = Jσ, a general return mapping scheme with elastic predictor and closest point projection algorithm formulated in principal logarithmic strains = 1/2 ln(b) = [1 , 2 , 3 ]T and in principal Kirchhoﬀ stresses τ = [τ1 , τ2 , τ3 ]T is applied. With this approach, which is valid for isotropic materials, the functional form of the return mapping is identical to the algorithm of the inﬁnitesimal theory [23]. Therefore, the whole scheme with elastic predictor, plastic corrector etc. is not shown here, but only the most important parts of our models are presented brieﬂy. 4.1 Metals The mechanical behavior of metals under transient impact loadings is mainly aﬀected through strain rate and temperature. Therefore, a Johnson-Cook plasticity model [15] is used, where the yield limit is a function of eﬀective plastic

s y ) B(å p)

k1

plastic strain

ǒ

.p

1 ) C ln 1 ) å. å0 plastic strain rate

Ǔ

yield limit

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

yield limit

yield limit

130

1 * (T *) k2

temperature

Fig. 1. Qualitative inﬂuence of strain, strain rate and temperature on yield limit in Johnson-Cook plasticity model p strain ¯p , eﬀective plastic strain rate ¯˙ and absolute temperature T : 2 p p q(¯ , ¯˙ , T ) ≤ 0 f (τ , q) = s − 3

with norm of stress deviator s = dev(τ ) and yield limit p ¯˙ p k 1 + C ln 1 + 1 − (T ∗ )k2 q(¯ p , ¯˙ , T ) = σy + B(¯ p ) 1 ¯˙ 0

(15)

(16)

σy indicates the static yield limit and material parameters B and k1 describe the strain hardening behavior (see Fig. 1). The increase of strength due to high strain rates, i.e. the viscosity, is considered through the second term of eq. (16). Factor C quantiﬁes the strain rate dependency, whereas the rate of plasp tic strain ¯˙ is normalized by ¯˙ = 1.0 [1/s]. With the last part in (16), the eﬀect of decreasing strength for high temperatures is reproduced: The homologous temperature T ∗ = (T − T0 )/(Tm − T0 ) is a measure for the mobility of crystal grid components and is modeled as a function of current temperature T , room temperature T0 and melting temperature Tm . This non-dimensional variable ranges from 0 (current = room temp.) to 1 (current = melt. temp.). Thermal softening is controlled by exponent k2 . Since transient impact and penetration processes are of very short duration, adiabatic temperature changes are assumed in our study. In addition, for the local temperature evolution, the empirical assumption is used, that most (90-100 percent) of the plastic work W p is transformed into heat ηd −1 T p ηd ˙ p W = J τ ˙ , 0.9 ≤ ηd ≤ 1.0 T˙ = cv cv

(17)

with density , grade of dissipation ηd and speciﬁc heat capacity cv . The return mapping algorithm ends up in a local Newton iteration, where plastic strain and plastic strain rate are the implicitely considered unknowns, whereas the temperature is accounted for in an explicit manner, i.e. it is computed from previous time step values.

Numerical Modeling of Transient Impact Processes

131

Fig. 2. Failure modes of geomaterial under impact loading (left) and typical compaction behavior of powder (right)

4.2 Geomaterials A constitutive model for cohesive and non-cohesive frictional materials will be presented, which is especially suited for dynamic impact processes. During a high velocity impact acting on cohesive frictional material (e.g. sandstone), a crushed zone appears directly under the impactor nose. In this region of highly conﬁned loading, the intact material disintegrates and loose, granular or powder-like media develops. Realistic description of this powderization and the material modeling of powder itself are important topics of our study. Characterization of Geomaterials Under Impact Loading Considering a solid structure made of intact, cohesive frictional material (e.g. concrete, sandstone, rock) under transient impact loading, diﬀerent states of stress and therefore diﬀerent states of failure can be observed, which we divided into three zones (Fig. 2): (i) high-pressure driven crushing (or powderization) directly under the impactor, (ii) moderate compaction due to mixed compression/shear loading and (iii) tensile fracture with low shearing. As already stated above, our main focus will be on the ﬁrst part, where compact cohesive frictional material is going to be totally disintegrated to loose, granular powder. The material will obviously change its mechanical properties during this crushing process. Due to comminution, a higher density can be achieved than with the original material. This densiﬁcation reserve leads to a temporary decrease of hardening behavior and an increase of maximal density. Additionally, crushing causes total loss of internal cohesion due to particle and matrix breaking, which results in full decrease of cohesion and tensile strength on macroscopic level. The eﬀect becomes obvious, when the evolved powder gets unloaded and loaded in the opposite direction (i.e. tension): Without tensile strength and cohesive capability, unlimited motion of powder particles is possible and dilatant loosening of the material will be observed. Since powder-like materials are distinctly compressible, depending

132

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

on the initial density, they can have severe damping and energy absorbing eﬀects in dynamic impact processes that are of interest in a number of different applications. Herein, the kinetic energy of a system is transformed into internal energy by a relative volume change of the powder (Fig. 2). A better understanding of this phenomenon is needed to extenuate or to intensify the damping and energy absorbing inﬂuence of powder in a quantitative and predictable way. In our investigations, the powder material of interest is of dry ﬁne sand type. In this study, a continuum cap model for the numerical simulation of geomaterials under quasi-static as well as dynamic loading is presented. A nonsmooth multisurface plasticity model with tension cutoﬀ, Drucker-Prager failure envelope and strain hardening cap provides the reproduction of the relevant phenomena: tensile failure, material ﬂow under shearing and compaction under pressure. For the comminution process, i.e. the transition from intact, cohesive frictional material to loose, granular media, this model will be enhanced. It includes a criterion for the powder development, diﬀerent evolution laws for material parameters like tensile strength, cohesion and compressibility and a modiﬁed hardening law. Modified Drucker-Prager-Cap Model The original multi-surface plasticity model consists of a nonlinear DruckerPrager cone for shear failure, an elliptical cap for compressive strain hardening and a limit in the tension region for tensile failure [22] [7] [13]. Therefore, the elastic region is bounded by following three yield criteria: f1 (τ ) := s − Fe (I1 ) ≤ 0 f2 (τ , q) := Fc (s , I1 , q) − Fe (q) ≤ 0

(18)

f3 (τ ) := I1 − T ≤ 0 These yield surfaces f1 = 0, f2 = 0 and f3 = 0 (see Fig. 3) are functions of stress invariants I1 = tr(τ ) and s = dev(τ ) as well as functions Fe (I1 ) := α − λ exp(βI1 ) − θI1

and

(19)

1 2 (q − I1 ) (20) R2 Fe deﬁnes the nonlinear Drucker-Prager cone and Fc describes the elliptical cap. The transitions between yield surfaces is discontinuous with two so-called corner regions. At the position, where cap and shear failure envelope intersect, we have q − X(q) (21) Fe (I1 = q) = R Fc (s , I1 , q) :=

2

s +

Numerical Modeling of Transient Impact Processes

133

Fig. 3. Yield surfaces of Drucker-Prager Cap plasticity in meridian plane

with hydrostatic compressive strength X(q) = q − R(α − λ exp(βq) − θq)

(22)

Material parameters of this formulation are the Drucker-Prager parameters α, λ, β and θ, the cap ellipticity R, the initial hydrostatic compressive strength X0 and the hydrostatic tensile limit T . Internal variable q < 0 is a function of volumetric plastic strain and it is responsible for the position and movement of the cap (hardening). The original Drucker-Prager-Cap (DPC) model of Hofstetter et al. [13] comes with associated ﬂow rules for all three failure surfaces. However, we will use non-associated ﬂow rules for the Drucker-Prager cone section and the tensile region to get rid of discontinuous ﬂow directions in both corners and to receive less dilatant behavior for shear failure, which seems to be more realistic from an experimental point of view [25]. Finally, our three ﬂow directions m1 , m2 and m3 are given by: −q ∂Fe (I1 ) I1 −q s s − IT1−q 1 = + (λβ exp(βI ) + θ) m1 := s 1 ∂I1 s T −q 1 m2 :=

s s Fc (s,I1 ,q) s

m3 :=

s s Fe (T ) s

−

q−I1 R2 Fc (s,I1 ,q)

+ 1− 1+

∂Fe (T ) ∂I1

1 s Fe (T )

(23) 1

A comparison between associated and non-associated ﬂow directions for the DPC model is shown in Fig. 4. Assuming that the relation between pressure and volume change is known from triaxial experiments, a strain hardening law can be deﬁned, which describes the dependence of internal variable q from volumetric plastic strain pvol = tr(p ). Here, two similar functions for that relation are provided. The

134

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Fig. 4. Flow directions of DPC model: associated and non-associated

ﬁrst one was proposed by Sandler and Rubin [22], whereas the second one was developed for better agreement with our experimental results for dry ﬁne sand type: ⎧ ⎨ W (exp (D(X(q) − X0 )) − 1) Sandler and Rubin [22] p vol = (24) ⎩ X(q)−X0 DW 1−D(X(q)−X Erhart et al. [11] 0) In Fig. 5 both hardening functions are shown. It can be observed, that the second curve (representing the second hardening law [11]) approaches the asymptote at pvol = −W in a more moderate way. In triaxial experiments, cohesive as well as non-cohesive geomaterials show a dependence from third invariant of stress deviator J3 = det(s) when it comes to failure. To reproduce this behavior in simulations, we scale all three yield surfaces with the Willam-Warnke function [28] 2(1 − e2 ) cos υ + (2e − 1) 4(1 − e2 ) cos2 υ + 5e2 − 4e (25) r(υ, e) = 2 4(1 − e2 ) cos2 υ + (2e − 1) with Lode angle 1 υ = arccos 3

√ 3 3 J3 2 (J2 )1.5

(26)

In our algorithm, the third stress invariant is considered in an explicit sense, i.e. Lode angle υ is calculated at tn and then yield surfaces are scaled with the Willam-Warnke function r(υ, e) at tn+1 . Therefore, the stress update algorithm is not aﬀected here. Powderization Under High Pressure With the plasticity model presented above, it is possible to reproduce the mechanical behavior of compact, cohesive geomaterials (sandstone, concrete,

Numerical Modeling of Transient Impact Processes

135

hydrostatic pressure

* X(q) Sandler & Rubin (1979):

ǒ

X(q) + X 0 )

å

p vol

p

p DW ǒ1 ) å vol ńWǓ

1ńD X0

Ǔ

å vol X(q) + X 0 ) 1 ln 1 ) D W

Erhart et al. (2005):

volumetric plastic strain

p * å vol

hydrostatic compression test

W

Fig. 5. Strain hardening laws for modiﬁed DPC model

mortar, etc.) as well as loose, granular media (sand, powder, etc.). The distinction between them is achieved by appropriate choice of material parameters. Now, this model will be enhanced in order to describe the transition from compact to loose material, i.e. the powderization under high pressure. At ﬁrst, a criterion is needed, which indicates the beginning of powder formation. On the other hand, a consistent transition from ’compact’ to ’loose’ is necessary. Therefore, a strategy is developed, where a new internal variable is used to modify the material parameters tensile strength (T ) and cohesion (α, λ). Additionally, hardening response is modiﬁed in loading and unloading to grasp the diﬀerent behavior of cohesive and non-cohesive material. In our approach, a stress dependent criterion is used as ’powderization indicator’ 1 − 2ν δ < δcrush 1+ν

and

I1 < I1,crush

(27)

where δcrush and I1,crush are material parameters and factor δ (’triaxiality’) is a function of stress invariants [14]: I1 δ=− √ √ 2 3 J2 cosυ

(28)

With this criterion, beginning of crushing is detected for very high pressures and highly conﬁned material (e.g. under impactor nose). If the criterion is fulﬁlled, tensile strength and cohesion will decrease, which is reproduced by softening in tension and shear regime in our constitutive model. Therefore, material parameters α, λ and T are now functions of new internal crushing variable qc . Following the hardening law (section 4.3), this history variable is chosen in such a way that it is identical with the 1/D-scaled volumetric plastic strain, which develops after the beginning of powderization: ⎧ 1 p p p ⎨ D ˙vol if ˙vol > ˙vol,crush (29) q˙c = ⎩ 0 else

136

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Shear strength α − λ at I1 = 0 is reduced by modiﬁcation of the nonlinear Drucker-Prager yield surface with following exponential softening (given in incremental form) q λn+1 = αn − (αn − λ0 ) exp − qc,n cu (30) αn+1 = αn + (λn+1 − λn ) exp(βqn ) with material parameter qcu controlling the reduction intensity. With these two equations it is guaranteed, that the position of the cap is not changed in the current time step. To receive the same amount of softening for the tensile limit, following nonlinear equation has to be solved for unknown Tn Fe (T0 ) Fe (Tn ) = Tn T0

(31)

The increase of hydrostatic compressive strength X(q) with increasing plastic compression (i.e. the expansion of the cap) is controlled by hardening law (24). On the other hand, the contraction of the cap due to dilatant plastic ﬂow in shear or tension depends on the material at hand. Loose, granular media like sand or powder is able to break up quite easily due to missing cohesion, whereas for intact cohesive geomaterials like concrete this phenomenon is not very distinct. We incorporated this observation in our model by allowing cap contraction only for powder-like materials (see Fig. 6). As already mentioned above, comminution of initially compact material has the consequence that a higher compaction is possible, clearly depending on the initial density. This phenomenon was observed in experiments [30] [29] and is incorporated in our model by modiﬁcation of the original hardening law. In Fig. 7, this modiﬁed hardening/loosening behavior is shown schematically. At point A, the intact material begins to deform plastically under hydrostatic pressure. Further increase of loading leads to an increase of density (contraction). At point B, powderization begins and hardening slope is less than before. Now, the material is crushed and condensed and therefore, higher compaction is possible (C) compared to a load path without powderization (C’). The transition from B to C is deﬁned analog to the usual hardening law øsø

øsø

loose material: loosening (cap contracts)

intact material: no loosening (cap remains) I1

Fig. 6. Diﬀerent cap treatment for dilatant plastic ﬂow

I1

Numerical Modeling of Transient Impact Processes pressure * X(q)

start of powderization

137

extra compression C’

C

dense powder

densification

B intact material loose powder E

loosening

A

D dilatation

contraction

p * å vol volumetric plastic strain

Fig. 7. Modiﬁed hardening for geomaterials with powderization

with two new material parameters Wcrush and Dcrush . If the highly condensed powder is now loaded in shear or tensile direction (dilatant plastic ﬂow), loosening of the material and a decrease of hydrostatic compressive strength can be observed (C → D). Further reduction of powder density is achieved with nearly no eﬀort, i.e. unlimited ﬂow of the material is possible.

5 Numerical Examples Practical relevant applications will demonstrate the performance of our overall approach. In Sec. 5.1, adaptive simulations with high-speed deformations of metals will be presented, followed by several geomaterial computations with our modiﬁed DPC model in Sec. 5.2. 5.1 Adaptive Computations To demonstrate the eﬀectiveness of our adaptive strategy and to examine the suitability of diﬀerent error indicators for large deformation transient problems, three numerical examples will be presented: Taylor bar impact, highstrain rate compression of WHA block and penetration of a steel cylinder by WHA long rod. For a detailed description of model settings, material parameters, etc. we refer to [12]. Here, only short descriptions of most interesting results are given. Taylor Bar Impact A cylindrical rod made of soft metal hits a rigid wall with high velocity [27] [6]. During the impact, elastic and slower plastic waves are initiated, propagating

138

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

t + 20ms

t + 40ms

smooth changes in time

t + 80ms

Fig. 8. Taylor bar impact with indicator ’gradient of plastic work’: Adaptive meshes and plastic energy (0–1500 Nmm)

t + 20ms

t + 40ms

t + 80ms

propagating plastic wave

Fig. 9. Taylor bar impact with indicator ’plastic power’: Adaptive meshes and plastic strain rates (0-75000 1/s)

in axial direction and reﬂecting at the bar tails. Therefore, the initial kinetic energy is transformed into internal energy and large plastic deformations can be observed. In our analysis, we compared diﬀerent error indicators. In Figs. 8 and Fig.9 the interrelation between adaptive meshes and choice of indicators is illustrated. The indicator ’gradient of plastic work’ causes a smooth and continuous growth of ﬁne mesh regions being consistent with the evolving plastic zone (Fig. 8). The indicator ’rate of plastic work’ also depicts the connection between adaptive discretizations and the corresponding physical/mechanical process: Reﬁnement occurs where rate of plastic strain is very high, i.e. where current material ﬂow takes place. Therefore, the propagating plastic wave is accompanied by a shift of ﬁne mesh region (Fig. 9).

Numerical Modeling of Transient Impact Processes

139

Fig. 10. WHA block: Adaptive meshes and temperature distribution

High-Strain Rate Compression of WHA Block In the second example, a prismatic metal block undergoes highly dynamic compression, which causes large plastic strains, which again eﬀects signiﬁcant temperature rise [3]. The involved thermal softening ﬁnally results in adiabatic shear bands, i.e. strain localization in consequence of heat. Figure 10 shows the evolution of shear bands represented by temperature distributions and appropriate adaptive meshes. For error assessment, the local quantity indicator ’variation of velocity’ was used as reﬁnement indicator. This indicator is well suited here, since dynamically developing strain localizations are detected automatically. The development of localizations results in expedient mesh reﬁnements, which again provide high resolutions in corresponding regions. Penetration of a Steel Cylinder by WHA Long Rod A cylindrical rod made of tungsten heavy alloy (WHA) hits an externally clamped cylindrical block made of high-strength steel at high velocity [6] [1]. Figure 11 shows deformed meshes and appropriate equivalent plastic strain distributions at time instances 20 µs and 40 µs with a logarithmic spectrum. The physical process gets obvious: The impactor penetrates the steel cylinder and produces a deep crater. At the same time, the melted tungsten is pressed outwards and the bar almost completely erodes. Plastic deformations are very high in both parts. These phenomena can be observed in experiments [1] and in corresponding simulations [6] in the same way. In our calculation with repeated remeshings, the spatial discretization adaptively follows the transient process. At the beginning, strong reﬁnement in the process zone under the impactor is ascertained. Beyond this area of high plastic deformation, the material behaves elastically and therefore the mesh density is relatively low. The ﬁne mesh region increases with proceeding penetration depth. The error indicator

140

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Fig. 11. Adapive meshes and equivalent plastic strains of WHA long rod penetration

’gradient of plastic work’ is apparently well suited to follow the physics of this problem in an intelligent way. 5.2 Geomechanical computations In this section, we present some results from numerical simulations with our enhanced DPC model for geomaterials. More detailed descriptions of these examples can be found in [11] and [10]. Quasi-Static Tests First, veriﬁcation and evaluation was done on diﬀerent quasi-static tests like conﬁned or hydrostatic compression for several geomaterials [4] [5] [29]. After identiﬁcation of appropriate material parameters good correlation with experimental results can be achieved (see Fig. 12). Here, especially the third diagram of a hydrostatic compression test on sandstone [29] has to be pointed out, since the distinct change of hardening behavior due to powderization is well captured by our modiﬁed DPC model. Triple Impact on Microconcrete A steel rod with spherical tail hits the surface of a ﬁne grade concrete [10]. Due to the impacts, the material powderizes in a small zone directly under the impactor, which is kept in our model through the criterion described in Sect. 4.2: In Fig. 13, ’powderized elements’ are represented by dark grey coloring. Additionally, the evolution of the hydrostatic compressive stress is shown for point A: The densiﬁcation and loosening of the comminuted material leads to increasing strength followed by decreasing strength for every single impact. On the other hand, this behavior is not discovered for the intact microconcrete

Numerical Modeling of Transient Impact Processes axial stress [N/mm2]

concrete

mortar

axial stress [N/mm2]

effective stress [N/mm2] experiment

1250

2000

141

1000

simulation

600 powderi– zation

450

1500 750

300

1000

500

500

150

250

0

0 0

0,05

0,10

0,15

0,20

0 0

0,05

axial strain [-]

0,10

0,15

0,20

0

axial strain [-]

0,04

0,08

0,12

volume change [-]

Fig. 12. Conﬁned compression and hydrostatic tests [4] [5] [29] hydrostatic compressive strength X(q) 0 A

–1000 powder (Point A)

intact microconcrete (Point B)

B

–2000

increase of strength

3rd impact

–3000 1st impact

2nd impact

time t [ms]

–4000 0

0,5

1,0

1,5

2,0

decrease of strength

Fig. 13. Results from triple impact on ﬁne grade concrete

(point B). Hence it follows that part of the kinetic energy is dissipated by the arised powder layer. Further inspection of this phenomenon will be done in our last example. Dynamic Compaction of Powder This example could be deemed to be a ’dynamic oedometer test’, i.e. we carried out dynamic compression (with several impacts) of conﬁned dry ﬁne sand type powder measuring penetration depth and contact force [11]. In the penetration-time diagram (Fig. 14), the periodical indentation for three diﬀerent layer heights can be observed as well as the decrease of penetration depth after a maximum compression was reached. As gets obvious from Fig. 14 the experimental and numerical results are in good agreement for all three thicknesses. The time dependent behavior of the contact force shows the damping eﬀect of powder (Fig. 14). The periodical impact causes peak loads at the

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall force [kN]

142

penetration [mm] 0,0

1 mm

-0,2

45 30

0

5 mm

force [kN]

-0,4

simulation

time [ms]

0

3 mm

-0,6

1 mm

15

-1,0 0

0,2

0,4

0,6

time [ms]

0,8

1,0

1,2

force [kN]

experiment

0,4

0,6

0,8

1,0

1,2

45 30

3 mm

15 0 0

-0,8

0,2

0,2

0,4

0,6

0,8

1,0

1,2

0,6

0,8

1,0

1,2

45 30

5 mm

15 0 0

0,2

0,4

Fig. 14. Evolution of penetration and contact force in dynamic compression of powder

same instances but they are diﬀerent in size depending on the layer thickness. Also the time of maximum contact force is delayed with increasing height. The amount of absorbed energy, i.e. the grade of damping by powder depends on layer thickness and initial density.

6 Conclusion High-velocity impact problems are physically extremely complex and therefore numerically very demanding. The speciﬁc challenge is due to the interaction of several areas like large deformations exhibiting large strains needing eﬃcient adaptive schemes, dynamic frictional contact algorithms avoiding nonphysically oscillations of contact forces and in particular distinct non-linear material models. It was found that the applied explicit formulation was very successful. It came along with time step control and continuous updates of the FE meshes based on physically motivated error indicators. Impact automatically drives the constitutive response into the highly non-linear range. Despite this fact macroscopic continuum based material models turned out to be sufﬁcient for a realistic simulation of the structural response, both for metals as well as for geomaterials. It is remarkable that one constitutive model, namely the Drucker-Prager-Cap plasticity model, is rich enough to represent the material disintegration of geomaterials from the intact phase via a powderization stage with a subsequent hardening to a potential loosening after unloading. It opens a large variety of applications from soil compaction to fasting problems, demolition techniques, crash simulations and other impact problems in civil and military engineering.

Numerical Modeling of Transient Impact Processes

143

References 1. Anderson Jr CE, Hohler V, Walker JD, Stilp AJ (1995) Time-resolved penetration of long rods into steel targets. Int J Imp Engrg 16:1–18 2. Batra RC, Ko KI (1992) An adaptive mesh reﬁnement technique for the analysis of shear bands in plane strain compression of thermoviscoplastic solid. Comput Mech 10:369–379 3. Batra RC, Peng Z (1995) Development of shear bands in dynamic plane strain compression of depleted uranium and tungsten blocks. Int J Imp Engrg 16:375– 395 4. Bazant ZP, Bishop FC, Chang TP (1986) Conﬁned compression tests of cement paste and concrete up to 300 ksi. J Amer Conc Inst 83:553–560 5. Burlion N, Pijaudier-Cabot G, Dahan N (2001) Experimental analysis of compaction of concrete and mortar. Int J Num Anal Meth Geomech 25:291–308 6. Camacho GT, Ortiz M (1997) Adaptive Lagrangian modelling of ballistic penetration of metallic targets. Comput Meth Appl Mech Engrg 142:269–301 7. Chen WF, Baladi GY (1985) Soil plasticity – Theory and implementation. McGraw Hill, New York 8. Dyduch M, Habraken AM, Cescotto S (1992) Automatic adaptive remeshing for numerical simulation of metalforming. Comput Meth Appl Mech Engrg 101:283–298 9. Erhart T, Taenzer L, Diekmann R, Wall WA (2001) Adaptive remeshing issues for fast transient, highly nonlinear processes. In Waszczyszyn Z, Pamin J (eds) Proceedings of ECCM 2001. Cracow, Poland 10. Erhart T (2004) Strategien zur numerischen Modellierung transienter Impaktvorgaenge bei nichtlinearem Materialverhalten. PhD Thesis, Institute of Structural Mechanics, University of Stuttgart, Germany 11. Erhart T, Wall WA, Ramm E (2005) A robust computational approach for dry powders under quasi-static and transient impact loadings. Comput Meth Appl Mech Engrg 194:4115–4134 12. Erhart T, Wall WA, Ramm E (2006) Robust adaptive remeshing strategy for large deformation, transient impact simulations. Int J Num Meth Engrg 65:2139–2166 13. Hofstetter G, Simo JC, Taylor RL (1993) A modiﬁed cap model: Closest point solution algorithms. Comput Struct 46:203–214 14. Hofstetter G, Mang HA (1995) Computational mechanics of reinforced concrete structures. Vieweg & Sohn, Braunschweig/Wiesbaden 15. Johnson GR, Cook WH (1985) Fracture characteristics of three metals subjected to various strains, strain rates, temperatures and pressures. Engrg Fract Mech 21:31–48 16. Lo SH (1985) A new mesh generation scheme for arbitrary planar domains. Int J Num Meth Engrg 21:1403–1426 17. Marusich TD, Ortiz M (1995) Modelling and simulation of high-speed machining. Int J Num Meth Engrg 38:3675–3694 18. Miehe C (1998) A formulation of ﬁnite elastoplasticity based on dual co- and contravariant eigenvector triads normalized with respect to a plastic metric. Comput Meth Appl Mech Engrg 159:223–260 19. Ortiz M, Quigley JJ (1991) Adaptive mesh reﬁnement in strain localization problems. Comput Meth Appl Mech Engrg 90:781–804

144

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

20. Peraire J, Vahdati M, Morgan K, Zienkiewicz OC (1987) Adaptive remeshing for compressible ﬂow simulations. J Comp Phys 72:449–466 21. Peric D, Vaz Jr. M, Owen DRJ (1999) On adaptive strategies for large deformations of elasto-plastic solids at ﬁnite strains: Computational issues and industrial applications. Comp Meth Appl Mech Engrg 176:279–312 22. Sandler IS, Rubin D (1979) An algorithm and a modular subroutine for the cap model. Int J Num Anal Meth Geomech 3:173–186 23. Simo JC (1992) Algorithms for static and dynamic multiplicative plasticity that preserve the classical return mapping schemes of the inﬁnitesimal theory. Comput Meth Appl Mech Engrg 99:61–112 24. Simo JC, Miehe C (1992) Associative coupled thermoplasticity at ﬁnite strains: Formulation, numerical analysis and implementation. Comput Meth Appl Mech Engrg 98:41–104 25. Smith SS, Willam KJ, Gerstle KH, Sture S (1989) Concrete over the top, or: Is there life after peak? ACI Mat J 86:491–497 26. Tabbara M, Blacker T, Belytschko T (1994) Finite element derivative recovery by moving least square interpolants. Comput Meth Appl Mech Engrg 117:211– 223 27. Taylor G (1948) The use of ﬂat-ended projectiles for determining dynamic yield stress. I. Theoretical considerations. Proc Roy Soc London, Series A, Math Phys Sci 194:289–299 28. Willam KJ, Warnke E (1975) Constitutive model for triaxial behavior of concrete. In: Proc. Concrete structures subjected to triaxial stresses, International Association for Bridge and Structural Engineering, Section III: 1–30 29. Wong TF, Szeto H, Zhang J (1992) Eﬀect of loading path and porosity on the failure mode of porous rocks. Appl Mech Rev 45:281–293 30. Zhang J, Wong TF, Davis DM (1990) Micromechanics of pressure-induced grain crushing in porous rocks. J Geophys Res 95:341–352 31. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. Part 1: The recovery technique. Int J Num Meth Engrg 33:1331–1364

A Computational Model For Viscoplasticity Coupled with Damage Including Unilateral Eﬀects D.R.J. Owen1 , F.M. Andrade Pires2 and E.A. de Souza Neto1 1

2

Civil and Computational Engineering Centre, School of Engineering University of Wales Swansea, Singleton Park, Swansea SA2 8PP, UK [email protected], [email protected] DEMEGI – Department of Mechanical Engineering and Industrial Management, Faculty of Engineering, Oporto University, Rua Dr. Roberto Frias, s/n, 4200-465 Porto, Portugal [email protected]

Summary. This contribution is concerned with the numerical modelling of nonlinear solid material behaviour in the presence of ductile damage. The description of the complex inelastic material behaviour is accomplished by coupling the elastoviscoplastic constitutive model, discussed by Peri´c (1993)[1], with a ductile damage evolution law, introduced by Ladev`eze & Lemaitre (1984) [2]. The evolution of the damage internal variable includes the important eﬀect of micro-crack closure, which may dramatically decrease the rate of damage growth under compression [3]. The theoretical basis of the material model and the computational treatment, within the framework of a ﬁnite element solution procedure, are presented. The resulting integration algorithm reduces to the solution of only one scalar non-linear equation and generalizes the standard return mapping procedures of the inﬁnitesimal theory. Numerical tests of the integration algorithm, which rely in the analysis of iso-error maps, are provided.

1 Introduction The numerical treatment of diﬀerent material phenomena, in the context of ﬁnite element simulations, has been addressed in several publications (see [4, 5, 6, 7, 8, 9, 10, 11] and references therein) during the last three decades or so. As a result, a wide range of material models, incorporating elastic, viscoelastic and elasto-plastic material behaviour is currently available in standard commercial ﬁnite-element codes. The computational algorithms that model the inelastic material behaviour have achieved a high degree of maturity. This is particularly true for the isotropic material response and situations

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 145–164. © 2007 Springer. Printed in the Netherlands.

146

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

in which diﬀerent rheological phenomena (elasticity, viscoelasticity, plasticity) can be considered independently of each other. Despite such developments, it is often necessary to enhance the constitutive description to describe noticeable features of the material behaviour and also to formulate models with greater predictive capability. Here, we are particularly interested in the inelastic constitutive description of materials subjected to forming operations. These processes are usually characterised by the presence of extreme deformations and strains, often resulting in localised material deterioration with possible fracture nucleation and growth. Rate sensitivity and strain rate eﬀects are also known to have a signiﬁcant role in the constitutive description. In many relevant practical problems, even when the material is initially isotropic, plastic ﬂow is usually responsible for inducing anisotropy. In this case, the experimental identiﬁcation of material parameters becomes a very diﬃcult and complicated task, with very few examples in the published literature. Bearing in mind that a model intended to represent such phenomena should be simple enough to allow eﬃcient numerical treatment and easy experimental veriﬁcation of material parameters, this work is restricted to situations in which the overall behaviour can be regarded as isotropic. Therefore, a scalar damage variable is chosen to represent the material internal degradation. The assumption of isotropic damage in many cases is not too far from reality, as a result of the random shapes and distribution of the included particles that trigger damage initiation and growth. The purpose of this contribution is the formulation and numerical implementation of a phenomenological constitutive model for elasto-viscoplastic solids, capable of handling regions of high rate-sensitivity to rate independent conditions in the presence of ductile damage. The description of the complex inelastic material behaviour is accomplished by coupling a power-law elasto-viscoplastic constitutive model [1, 12], which is widely accepted for the description of rate-dependent deformations of solids, with a ductile damage evolution law [2, 13]. The damage growth is inﬂuenced by the hydrostatic stress state and includes the important eﬀect of micro-crack closure. The introduction of unilateral damage eﬀects allows for a clear distinction between states of identical triaxiality but stresses of opposite sign (tension and compression) in the damage evolution. This eﬀect may dramatically decrease the rate of damage growth under compression, which was highlighted by numerical tests carried out by the authors [3]. The chapter is organized as follows: Section 2 discusses the essential assumptions of the model and outlines the set of constitutive equations that govern the coupled elasto-viscoplastic damage behaviour. The algorithm for numerical integration of the model is described in detail in Section 3 and the closed form of the consistent tangent operator is presented. An assessment of the accuracy and stability of the elastic predictor-viscoplastic corrector algorithm is carried out relying on the analysis of iso-error maps in Section 4. The chapter ends with the concluding remarks presented in Section 5.

Computational Model For Viscoplasticity Coupled with Damage

147

2 Elasto-Viscoplastic Damage Constitutive Model In this section, the constitutive relations, represented by a set of equations in time, which govern the elasto-viscoplastic damage model with crack closure eﬀects are presented. The undamaged phenomenological behaviour of the material is modelled by a von Mises type power-law elasto-viscoplastic model described in Section 2.1. The important concept of eﬀective stress [14] is recalled in Section 2.2. In Section 2.3 the principle of strain equivalence is used to derive eﬀective constitutive equations for the damaged material. The damage evolution law, which includes the important eﬀect of crack closure, is presented in Section 2.4. 2.1 Viscoplastic Model It is well known that the phenomenological behaviour of real materials is generally time-dependent in the sense that the stress response always depends on the rate of loading and/or the time scale considered. The eﬀects of time dependent mechanisms are particularly visible at higher temperatures. Several diﬀerent visco-plasticity models have been proposed in the past and, in practice, a particular choice should be dictated by its ability to model the dependency of the plastic strain rate on the state of stress for the material under consideration. This section provides a brief review of the equations governing the undamaged material. The elasto-viscoplastic model described is based on a von Mises yield criterion and a power-law isotropic hardening [1]. The model is deﬁned by an elastic constitutive equation, i.e., a linear elastic relation between the stress tensor, σ, and the elastic strain, εe : σ = De : εe

(1)

where the symbol : denotes double contraction and De is the standard isotropic elasticity fourth order tensor given by (2) De = 2G I − 13 I ⊗ I + K I ⊗ I where I, is the fourth order identity tensor. The material constants G and K are, respectively, the shear and bulk moduli. The conventional additive ˙ into an elastic contribution, ε˙ e , and decomposition of the total strain rate, ε, vp an inelastic contribution, ε˙ : ε˙ = ε˙ e + ε˙ vp

(3)

is assumed. Furthermore, an associative plastic ﬂow rule is adopted: ε˙ vp = γ˙

∂Φ(σ, σy ) , ∂σ

(4)

148

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

where γ˙ is the plastic multiplier whose expression is deﬁned later. In the above, Φ is the von Mises yield function (5) Φ(σ, σy ) ≡ q (s (σ)) − σy = 3 J2 (s) − σy , where s ≡ σ − 13 (trσ) I, with I the identity tensor, is the stress deviator, and σy = σy (¯ ε vp )

(6)

is the stress-like variable associated with isotropic hardening. In the present case (isotropic strain hardening), σy is an experimentally determined function of the equivalent plastic strain, ε¯ vp , whose evolution is deﬁned by the rate equation: vp ε¯˙ = 23 ε˙ vp . (7) The yield function Φ deﬁnes an elastic domain such that the material behaviour is purely elastic (no viscoplastic ﬂow) whenever q < σy . Among the various possibilities for the deﬁnition of γ, ˙ here, the following form of a power-type law is adopted [1]: 1/ 1 q −1 , (8) γ˙ = µ σy where µ and are the viscosity and rate-sensitivity, respectively. These material parameters are, generally, temperature-dependent and can only assume positive values. The symbol · represents the ramp function deﬁned as x = (x + |x|)/2.

(9)

The evolution problem described by the set of constitutive equations (1)– (8), has a ﬁrm experimental basis and is widely accepted as a description of rate-dependent deformations of solids. Remark 1. The elasto-viscoplastic model contains, as special limiting cases, two important models[1]: (i) When µ → 0 (no viscosity) and/or → 0 (no rate-sensitivity), the standard rate-independent von Mises elasto-plastic model is recovered. (ii) When µ → ∞ a form of viscoelastic model is recovered. 2.2 Concept of Eﬀective Stress An important step in the formulation of damage models is the introduction of damage eﬀects without loosing the properties of well established models of

Computational Model For Viscoplasticity Coupled with Damage

149

elasto-plasticity and elasto-viscoplaticity. Therefore, several diﬀerent concepts and postulates have been introduced in the literature in order to account for the material progressive internal deterioration. The most frequently used concept, which is crucial to the deﬁnition of the theory, is the concept of eﬀective stress [15, 16]. Due to the diversity of forms in which internal damage manifests itself at the microscopic level, variables of diﬀerent mathematical nature (scalars, vectors, tensors) possessing diﬀerent physical meaning (reduction of load bearing area, loss of stiﬀness, distribution of voids) have been employed in the description of damage under various circumstances. Here, only one single scalar variable, D, will be used, representing the simplest possible isotropic formulation. According with the concept of eﬀective stress an eﬀective stress tensor is introduced as 1 ˜ ≡ σ. (10) σ 1−D The damage variable assumes values between 0 (for the undamaged material) and 1 (for the completely damaged material). In practice, a critical value Dc < 1 usually deﬁnes the onset of a macro-crack (i.e., complete loss of load carrying capacity at a point). Continuum damage mechanics relies on the postulate of strain equivalence, which states that ”the strain behaviour of a damaged material is represented by constitutive equations of the virgin material (without damage) in the potential of which the stress is simply replaced by the eﬀective stress” [14, 17]. This principle can be used to derive eﬀective constitutive equations for the damaged material based on the equations which govern the undamaged material response, simply by replacing the stress tensor σ in these equations by ˜ according to (10). the eﬀective stress tensor σ 2.3 Elasto-Viscoplasticity Coupled with Damage A coupled elasto-viscoplastic model can be obtained by including the eﬀect of damage in the power-law viscoplastic model described in Section 2.1. This can be accomplished by simply substituting Equation (10) in the deﬁnition of the von Mises yield function: 3 J2 (s) q − σy = − σy (¯ ε vp ) . (11) Φ (σ, σy , D) ≡ 1−D 1−D It should be noted that (11) accounts for two competing eﬀects: damaging, which shrinks (isotropically) the elastic domain (deﬁned as the subset of stress space for which Φ ≤ 0) as D grows; and hardening, which can expand the elastic domain (also isotropically) with the growth of σy . The von Mises yield function can be rewritten as ε vp ) . (12) Φ (σ, σy , D) ≡ q − (1 − D) σy = 3 J2 (s) − (1 − D)σy (¯

150

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

If this particular form is used, the associative plastic ﬂow rule (4) remains unchanged, i.e., is not directly aﬀected by the introduction of damage. This equation is more convenient and will be used later for the computational implementation. In addition to Equation (12), damage eﬀects will also be included in the deﬁnition of the viscoplastic multiplier:

1/ q 1 −1 , (13) γ˙ = µ (1 − D)σy or equivalently, ⎧ 1/ 1 q ⎪ ⎨ −1 (1 − D)σy γ˙ = µ ⎪ ⎩ 0

if

Φ (σ, σy , D) > 0

if

Φ (σ, σy , D) ≤ 0 .

(14)

Note that the eﬀect of internal damage on the elastic behaviour of the material is ignored in the present model. That is, the elasticity tensor is not a function of the damage variable or in other words, elasticity and damage are assumed to be decoupled. This simpliﬁcation can be justiﬁed if the elastic strain remains truly inﬁnitesimal in the type of problems addressed with this model. Remark 2. The damage variable ranges between 0 and 1, with D = 0 corresponding to the sound (undamaged) material and D = 1 to the fully damaged state with complete loss of load carrying capacity. Note that damage growth induces softening, i.e., shrinkage of the yield surface deﬁned by Φ = 0. For D = 0 the yield surface reduces to that of the (pressure insensitive) von Mises type power-law elasto-viscoplastic model. In the presence of damage, i.e., for D = 0 the yield surface shrinks and its size reduces to zero for D = 1. 2.4 Damage Evolution Law The damage evolution law should reﬂect the nucleation and growth of voids and microcracks which accompany viscoplastic ﬂow. Damage and viscoplasticity are undoubtedly coupled, as the presence of internal deterioration introduces local stress concentrations which may in turn drive viscoplastic deformation. The evolution of the damage internal variable is assumed to be governed by the relation: ⎧ vp 0 if ε¯ vp ≤ ε¯D ⎪ ⎨ s (15) D˙ = γ˙ −Y vp ⎪ ⎩ if ε¯ vp > ε¯D , 1−D r

Computational Model For Viscoplasticity Coupled with Damage

151

vp are material constants. In the nucleation phase, experimenwhere r, s and ε¯D tal evidence reveals that there is no noticeable eﬀect of damage on the mechanvp is the so-called damage threshold, ical properties, therefore the constant ε¯D i.e., the value of accumulated plastic strain below which no damage evolution is observed. The quantity

Y =

−1 2 [(1 + ν)σ+ : σ+ − ν trσ ] 2E(1 − D)2 −

h 2 [(1 + ν)σ− : σ− − ν −trσ ] , 2E(1 − hD)2

(16)

is the damage energy release rate, with E and ν denoting, respectively, the Young’s modulus and the Poisson’s ratio of the undamaged material. The tensors σ+ and σ+ are, respectively, the tensile and compressive components of σ, deﬁned as: 3 σi ei ⊗ ei (17) σ+ = i=1

and σ− =

3

−σi ei ⊗ ei ,

(18)

i=1

with {σi } and {ei } denoting, respectively, the eigenvalues and an orthonormal basis of eigenvectors of σ. The crack closure parameter, h, is an experimentally determined coeﬃcient which satisﬁes: 0 ≤ h ≤ 1.

(19)

This coeﬃcient characterizes the closure of microcracks and micro-cavities and depends upon the density and the shape of the defects. It is a material dependent parameter and, for simplicity, h is considered as constant. A value h ≈ 0.2 is typically observed in many experiments [18]. This deﬁnition of the energy release rate (16) was introduced by Ladev`eze (1983)[13] and Ladev`eze & Lemaitre (1984) [2]. Note that, for a state of purely tensile principal stresses, the damage energy release rate (16), can be simpliﬁed and rewritten as −1 (1 + ν) σ : σ − ν (tr σ)2 2 2E(1 − D) 2 2 −q 2 p (1 + ν) + 3(1 − 2ν) . = 2E(1 − D)2 3 q

Y =

(20)

For states with purely compressive principal stresses, (16) will give absolute values of Y smaller than those produced by (20), resulting in a decrease of damage growth rates. Also note that the limit h = 1 corresponds to no crack closure eﬀect whereas the other extreme, h = 0, corresponds to a total crack closure, with no damage evolution under compression. Any other value of h describes a partial crack closure eﬀect.

152

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

Remark 3. The particular form of the energy release rate (20), was initially proposed by Lemaitre (1983) [19] in order to describe the inﬂuence of stress triaxiality ratio, p/q, on the rate of damage growth. The inclusion of the hydrostatic component of σ in the deﬁnition of Y implies that D˙ increases (decreases) with increasing (decreasing) triaxiality ratio. One important feature of damage growth is the clear distinction between rates of damage growth observed for states of stress with identical triaxiality but stresses of opposite sign (tension and compression). Such a distinction stems from the fact that, under a compressive state, voids and micro-cracks that would grow under tension will partially close, reducing (possibly dramatically) the damage growth rate. This phenomenon can be crucially important in the simulation of forming operations, particularly under extreme strains. It is often the case that, in such operations, the solid (or parts of it) undergoes extreme compressive straining followed by extension or vice-versa [3].

3 Integration Algorithm In this section the derivation of an integration algorithm for the elasto-viscoplastic damage constitutive model, described in the previous section is carried out in detail. Operator split algorithms are particularly suitable for numerical integration of constitutive equations and are widely used in the context of elasto-plasticity and also elasto-viscoplasticity [20, 21, 22, 1, 7]. Let us consider a typical time step over the time interval [tn , tn+1 ], where the time and strain increments are deﬁned in the usual way as ∆t = tn+1 + tn ,

∆ε ≡ εn+1 − εn .

(21)

In addition, all variables of the problem, given by the set {σn , εen , εnvp , ε¯nvp , Dn }, are assumed to be known at tn . The operator split algorithm should obtain vp ¯n+1 , Dn+1 } of variables at tn+1 consisthe updated set {σn+1 , εen+1 , εvp n+1 , ε tently with the evolution equations of the model. The algorithm comprises the standard elastic predictor and the visco-plastic return mapping which, for the present model, has the following format. Elastic Predictor The ﬁrst step in the algorithm is the evaluation of the elastic trial state where the increment is assumed purely elastic with no evolution of internal variables (internal variables frozen at tn ). The elastic trial strain and trial accumulated viscoplastic strain are given by: εe trial = εen + ∆ε;

ε¯ vp trial = ε¯nvp .

(22)

Computational Model For Viscoplasticity Coupled with Damage

153

The corresponding elastic trial stress tensor is computed: σtrial = De : εe trial ,

(23)

e

where D is the standard isotropic elasticity tensor. Equivalently, in terms of stress deviator and hydrostatic pressure, we have:

where

strial = 2G ee trial ,

ptrial = K v e trial ,

(24)

ee trial = een + ∆e,

v e trial = vne + ∆v .

(25)

The material constants G and K are, respectively, the shear and bulk moduli, s and p stand for the deviatoric and hydrostatic stresses. The strain deviator and the volumetric strain are denoted, respectively, by e and v. The trial yield stress is simply ε vp ). (26) σytrial = σy (¯ The next step of the algorithm is to check whether σtrial lies inside or outside of the trial yield surface. With variables ε¯ vp and D frozen at time tn we compute: ε vp ) Φtrial := q trial − (1 − Dn )σy (¯ (27) ε vp ) . = 32 strial − (1 − Dn )σy (¯ If Φtrial ≤ 0, the process is indeed elastic within the interval and the elastic trial state coincides with the updated state at tn+1 . In other words, there is no viscoplastic ﬂow or damage evolution within the interval and εen+1 = εe trial ;

σn+1 = σtrial ;

σy n+1 = σytrial ;

Dn+1 = D trial .

vp ε¯n+1 = ε¯ vp trial ;

(28)

Otherwise, we apply the viscoplastic corrector algorithm described in the following. Visco-plastic corrector (or return mapping algorithm) At this stage, we solve the evolution equations of the model with the elastic trial state as the initial condition. With the adoption of a backward Euler discretisation, the viscoplastic corrector is given by the following set of algebraic equations: ∂Φ σn+1 = σtrial − ∆γ D : ∂σ n+1 vp ε¯n+1 = ε¯nvp + ∆γ

⎧ ⎨0 Dn+1 =

⎩D + n

∆γ 1−Dn+1

−Yn+1 r

s

vp vp if ε¯n+1 ≤ ε¯D vp vp if ε¯n+1 > ε¯D ,

(29)

154

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

where the incremental multiplier , ∆γ, is given by:

1/ q(σn+1 ) ∆t −1 , ∆γ = vp µ (1 − Dn+1 ) σy (¯ εn+1 )

(30)

with ∆t denoting the time increment within the considered interval. After solving (29), we can update: ∂Φ ∂Φ vp e e trial = ε + ∆γ ε = ε − ∆γ . (31) εvp n n+1 n+1 ∂σ n+1 ∂σ n+1 The visco-plastic corrector can be more eﬃciently implemented by reducing (29) to a single non-linear equation for the incremental multiplier ∆γ. 3.1 Single-Equation Corrector As we shall see in what follows, analogously to what happens to the classical von Mises model, the above system can be reduced by means of simple algebraic substitutions to a single non-linear equation having the incremental plastic multiplier, ∆γ, as a variable. Firstly, we observe that the plastic ﬂow vector: ∂Φ 3 s = 2 (32) ∂σ s is deviatoric. The stress update equation (29)1 can then be split as: n+1 sn+1 = strial − ∆γ 2G 32 s sn+1 pn+1 = ptrial ,

(33)

where p denotes the hydrostatic pressure and G is the shear modulus. Further, simple inspection of (33)1 shows that sn+1 is a scalar multiple of strial so that, trivially, we have the identity: strial sn+1 = trial , sn+1 s which allows us to re-write (33)1 as: ∆γ 2G ∆γ 3G trial 3 = 1 − trial strial sn+1 = 1 − 2 trial s s q where q trial is the elastic trial von Mises equivalent stress: q trial = q(strial ) = 32 strial . Equation (35) results in the following update formula for q:

(34)

(35)

(36)

Computational Model For Viscoplasticity Coupled with Damage qn+1 = q trial − 3G ∆γ .

155 (37)

With the substitution of the above formula together with (29)2 into (30) we obtain the following scalar algebraic equation for the incremental multiplier, ∆γ:

1/ q trial − 3G ∆γ ∆t − 1 = 0, (38) ∆γ − vp µ (1 − Dn+1 ) σy (¯ εn+1 ) or, equivalently, after a straightforward rearrangement, 3 trial − 3G ∆γ ∆t 2 s Dn+1 = D(∆γ) ≡ 1 − , σy0 + R(¯ εnvp + ∆γ) µ ∆γ + ∆t

(39)

which expresses Dn+1 as an explicit function of ∆γ. Finally, by introducing the damage explicit function (39) into the discretised damage evolution equation (29)3 , the viscoplastic corrector is reduced to the solution of a single algebraic equation for the incremental multiplier, ∆γ: ⎧ vp p if ε¯n+1 ≤ ε¯D ⎨ D(∆γ) = 0 s (40) F (∆γ) ≡ −Y (∆γ) vp vp ∆γ ⎩ D(∆γ) − D − = 0 if ε¯n+1 > ε¯D . n 1−D(∆γ) r In (40)2 , the dependency of Y on ∆γ originates from its dependency on the updated values of D and σ: Y (∆γ) =

−1 2 [(1 + ν)σ+ (∆γ) : σ+ (∆γ) − ν trσ(∆γ) ] 2E[1 − D(∆γ)]2

h 2 [(1 + ν)σ− (∆γ) : σ− (∆γ) − ν −trσ(∆γ) ] , 2E[1 − hD(∆γ)]2 (41) The updated stress tensor, σn+1 , whose tensile and compressive components take part in the calculation of Yn+1 , is obtained as: −

σn+1 = sn+1 + pn+1 I ,

(42)

where I is the second order identity tensor and sn+1 is obtained from the standard implicit return mapping as a function of ∆γ according to update formula (35): ∆γ 3G strial ; pn+1 = ptrial . (43) sn+1 = 1 − trial q The single-equation viscoplastic corrector comprises the solution of the above equation for ∆γ, followed by the straightforward update of the relevant variables. The solution of the equation for ∆γ is, as usual, undertaken by the Newton-Raphson iterative scheme. The overall algorithm for the numerical integration of the elasto-viscoplastic damage model, which includes the eﬀect of crack closure, is summarised in Box 1 in pseudo-code format.

156

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto (i) Elastic predictor. Given ∆ε, ∆t and the state variables at tn , compute the elastic trial state: εe trial = εen + ∆ε; etrial = dev[εe trial ]; v trial = tr[εe trial ] ε¯ vp trial = ε¯nvp ;

Dtrial = Dn

strial = 2G etrial ; ptrial = K v trial q trial = 32 strial , (ii) Check for viscoplastic ﬂow. First compute: εnvp )] , Φtrial = q trial − (1 − Dn ) [σy0 + R(¯ IF Φtrial ≤ εtol THEN (elastic step) Update (·)n+1 = (·)trial and EXIT ELSE GOTO (iii) (iii)Visco-plastic corrector . Solve the return mapping equation ⎧ vp vp if ε¯n+1 ≤ ε¯D ⎨ D(∆γ) = 0 s F (∆γ) ≡ −Y (∆γ) vp vp ∆γ ⎩ D(∆γ)−Dn − = 0 if ε¯n+1 > ε¯D 1−D(∆γ)

r

with D(∆γ) deﬁned by (39) and Y (∆γ) deﬁned through (16), (39) (42) and (43). (iv) Update the variables: 3G strial ; pn+1 = ptrial ; sn+1 = 1 − ∆γ q trial σn+1 = sn+1 + pn+1 I ; e εn+1 =

1 2G

sn+1 +

1 3K

vp ε¯n+1 = ε¯nvp + ∆γ ;

pn+1 I ; Dn+1 = D(∆γ).

(v) EXIT Box 1: Elastic predictor/visco-plastic return mapping integration algorithm for the elasto-viscoplastic damage model with crack closure eﬀect (over time interval [tn , tn+1 ])

Remark 4. (computational implementation aspects) In the computer implementation of the model (as shown in Box 1), it is important to specify the damage function D(∆γ), as expressed in equation (39). The reason for this lies in the fact that, for low rate-sensitivity, i.e., small values of , the NewtonRaphson scheme for solution of (38) becomes unstable as its convergence bowl is sharply reduced with decreasing . The reduction of the convergence bowl stems from the fact that large exponents 1/ can easily produce numbers

Computational Model For Viscoplasticity Coupled with Damage

157

which are computationally intractable. This fact has been recognised by Peri´c (1993) [1] in the context of a more general visco-plastic algorithm. In equation (39), on the other hand, the term to the power on the left hand side can only assume values within the interval [0, 1] and causes no numerical problems within practical ranges of material constants. 3.2 Consistent Tangent Operator To obtain the consistent tangent operator for the case of a strain-driven problem, all variables of the problem are considered as functions of the strain ε. The exact linearization of the algorithm described in Box 1 is performed by a systematic application of the concept of directional derivative. In the elastic case, the elastic consistent tangent at tn+1 , is simply the standard elasticity operator ˆ = De = 2G I − 1 I ⊗ I + K I ⊗ I (44) D 3 where I, is the fourth order identity tensor. In the elasto-viscoplastic damage case, i.e., when it is assumed that viscoplastic ﬂow occurs within the step, the tangent operator is called the elastoˆ vp . For the present viscoplastic damage consistent tangent and is denoted by D model it is possible to obtain a closed form expression for the tangent operator. The details of derivation, which is rather lengthy, will be omitted here and we shall limit ourselves to show only its ﬁnal expression which is given by: ¯n+1 + a3 s ¯n+1 ⊗ s ¯n+1 ⊗ I + K I ⊗ I , (45) Dvp = a1 I − 13 I ⊗ I + a2 s ¯n+1 is the normalised stress deviator: where s ¯n+1 = s

sn+1 , sn+1

(46)

and the scalars a1 , a2 , a3 , are given by: 3G a1 = 2G 1 − ∆γ trial q ∂F ∂F a2 = 6G2 q∆γ trial + ∂ (q trial ) / ∂ (∆γ)

a3 = 2G

2 3

K

∂F / ∂F ∂ (ptrial ) ∂ (∆γ)

(47)

.

In the deﬁnition of constants a2 and a3 , the scalars ∂F /∂ (∆γ), ∂F /∂ (q trial ) and ∂F /∂ (ptrial ), correspond to the derivatives of the return mapping residual

158

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

function deﬁned by (40): ∂F ∂ (∆γ)

=

∂D ∂ (∆γ)

s + 1−D1n+1 − Yn+1 r ∂Y − ∂ ∂D ∆γ − 1 / (1−D ) − s / Y n+1 n+1 (∆γ) ∂ (∆γ) s 2 − Yn+1 − ∆γ ∂ (q∂D trial ) /(1−Dn+1 ) r s−1 s ∆γ ∂Y − Yn+1 − r (1−D r ∂ (q trial ) n+1 )

∂F ∂ (q trial )

=

∂D ∂ (q trial )

∂F ∂ (ptrial )

=

s ∆γ r (1−Dn+1 )

− Yn+1 r

s

(48)

∂Y . ∂ (ptrial )

where the scalars ∂Y /∂ (∆γ), ∂Y /∂ (q trial ) and ∂Y /∂ (ptrial ), represent the derivatives of the energy release rate function, deﬁned by (16): √3 ∂D ∂D h2 ∂ (∆γ) 2G ∂ (∆γ) ∂Y 2 ¯ = − b + ∂ (∆γ) E (1−Dn+1 )3 + E (1−Dn+1 )2 C+ : sn+1 − E (1−h Dn+1 )3 b− √

+ ∂Y ∂ (q trial )

¯n+1 C− : s

∂D ∂ (q trial )

= − E (1−Dn+1 )3 b+ − +

∂Y ∂ (ptrial )

3 2G 2 h E (1−h Dn+1 )2

√2

3 h E (1−h Dn+1 )2

√2 3

E (1−Dn+1 )2

¯n+1 − C+ : s

h2

∂D ∂ (q trial )

E (1−h Dn+1 )3

b−

¯n+1 C− : s

1 = − E (1−D 2 C+ : I − n+1 )

h E (1−h Dn+1 )2

C− : I

(49) furthermore, the scalars b+ and b− and the second order tensors C+ and C− introduced in (49), are given by 2

b+ = (1 + ν) σ+ : σ+ − ν tr σ

b− = (1 + ν) σ− : σ− − ν −tr σ

2

C+ = (1 + ν) ∂∂σσ+ : σ+ − ν tr σ I

(50)

C− = (1 + ν) ∂∂σσ− : σ− − ν −tr σ I Here, one should note that the tensors C+ and C− deﬁned in (50)3 and (50)4 , respectively, contain the terms: ∂σ+ , ∂σ

and

∂σ− . ∂σ

Computational Model For Viscoplasticity Coupled with Damage

159

To compute such derivatives, we ﬁrst note that (17) and (18) deﬁne σ+ and σ− as isotropic tensor-valued functions of σ. Such functions are particular cases of the families of functions discussed by Chadwick & Ogden (1971)[23] and Carlson & Hoger(1986) [24] and their derivatives are promptly available in closed form. Finally, the scalars ∂D/∂ (∆γ) and ∂D/∂ (q trial ), which are the outcome of the derivation of the damage function (39) are deﬁned by trial H(q trial −3G∆γ) µ q −3G∆γ ∂D ∆t 3G = + + vp vp vp 2 ∂ (∆γ) µ ∆γ+∆t µ ∆γ+∆t σy (¯ ε ) σy (¯ ε ) σy (¯ ε ) n+1

∂D ∂ (q trial )

= − σy (¯ε1vp

n+1

)

∆t µ ∆γ+∆t

n+1

n+1

(51) In the above, H denotes the derivative of the hardening function evaluated at tn+1 : dσy H= . (52) d¯ ε vp ε¯ vp n+1

Remark 5. It is important to note that, the resulting elasto-viscoplastic tangent operator Dep is generally unsymmetric so that, within the context of ﬁnite element computations, an unsymmetric solver is required in the global Newton-Raphson scheme.

4 Accuracy Analysis of the Integration Algorithm To illustrate the accuracy of the integration algorithm in practical situations, this section presents some iso-error maps, produced with material constants covering a range of high rate-sensitivity to rate-independency. Iso-error maps have long been accepted as an eﬀective and reliable (if not the only) tool for assessing the accuracy of constitutive integration algorithms under realistic ﬁnite time/strain steps [25, 26, 20]. The maps have been generated in the standard fashion. Using the threedimensional implementation of the model, we start from a stress point at time tn , σn , lying on the yield surface (refer to Fig. 1) and apply a sequence of strain increments (within the interval [tn , tn+1 ]), corresponding to linear combinations of trial stress increments of the form ∆σtrial =

∆σN ∆σT T+ N, q q

(53)

where N and T are, respectively, the unit normal and tangent vectors to the yield surface and q is the von Mises equivalent stress. For each increment of trial stress, we obtain a numerical solution, σnum n+1 , with the above described algorithm in one step. In addition, a solution assumed to be ‘exact’, σexact n+1 , is obtained with the same algorithm by dividing the corresponding strain (and time) increment into 1000 sub-increments of equal size. For each point in

160

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto ∆σT tria

N

∆σ

T

σn

l

σtrial ∆σN

Fig. 1. Isoerror map. Trial stress increment directions Table 1. Material data for aluminium alloy Description

Symbol

Elastic Modulus Poisson’s ratio Initial yield stress Hardening curve

E 69004 [M N/m2 ] ν 0.3 80.559 [M P a] σ y0 ε vp ) 589 · (10−4 + ε¯ vp )0.216 σy (¯

Damage data (exponent) Damage data (denominator)

s r

Value

1.0 2.8 [M P a]

which a numerical and ‘exact’ solution is obtained, the error is computed as: ERROR =

num σexact n+1 − σn+1 × 100 . σexact n+1

The resulting iso-error map is the contour plot of the error ﬁeld. The material properties adopted in the present analysis, are listed in Table 1. These parameters were taken from Reference [27] for an aluminium alloy, except for the value of the damage denominator, r. The value of this material constant has been calibrated by performing several numerical tests with a single axisymmetric ﬁnite element, such that critical value of damage (D = 1) is attained, for the same applied displacement. To preserve the constant rate of total strain ∆ε/∆t for the iso-error map under consideration, the time increment ∆t is appropriately scaled. Figure 2 shows iso-error maps obtained at low and high strain rates with the non-dimensional rate ˙ µ ε set respectively to 1 and 1000. For each non-dimensional rate, three values of rate-sensitivity parameter, , have been used: 100 , 10−1 and 0. For = 0 virtually identical maps are obtained for the two rates [see Figs. 2 (a)3 and 2 (b)3 ] and the algorithm recovers the rate-independent solution.

Computational Model For Viscoplasticity Coupled with Damage

163

5 Concluding Remarks A computational model for elasto-viscoplastic solids, capable of handling regions of high rate-sensitivity to rate independent conditions in the presence of ductile damage, has been presented in this contribution. The material constitutive model is derived by coupling a power-law elasto-viscoplastic constitutive model, with a ductile damage evolution law. The evolution of the damage internal variable includes the important eﬀect of micro-crack closure. The model can describe diﬀerent concurrent physical phenomena and implicitly contains, as limit cases, simpler constitutive descriptions. The resulting integration algorithm generalizes the standard return mapping procedures of the inﬁnitesimal theory, and quite remarkably requires the solution of only one scalar non-linear equation.

References 1. Peri´c D (1993) On a class of constitutive equations in viscoplasticity: Formulation and computational issues. Int J Num Meth Engng 36:1365– 1393 2. Ladev`eze P, Lemaitre J (1984) Damage eﬀective stress in quasi unilateral conditions. In: 16th Int. Congress Theor Appl Mech, Lyngby, Denmark 3. Andrade Pires FM , de Souza Neto EA, Owen DRJ (2004) On the ﬁnite element prediction of damage growth and fracture initiation in ﬁnitely deforming ductile materials. Comp Meth Appl Mech 193:5223–5256 4. Owen DRJ, Hinton E (1980) Finite Elements in Plasticity: Theory and Practice. Pineridge Press, Swansea 5. Bathe K-J (1996) Finite Element Procedures. Prentice-Hall, Englewood Cliﬀs, New Jersey 6. Crisﬁeld MA (1991) Non-linear Finite Element Analysis of Solids and Structures. Vol.1: Essentials. John Wiley & Sons, Chichester 7. Crisﬁeld MA (1997) Non-linear Finite Element Analysis of Solids and Structures. Vol.2: Advanced Topics. John Wiley & Sons, Chichester 8. Simo, JC, Hughes, TJR (1998) Computational Inelasticity. SpringerVerlag, New York 9. Belytschko T, Liu WK, Moran B (2000) Nonlinear Finite Elements for Continua and Structures. Wiley, New York 10. Zienkiewicz OC, Taylor, RL, Zhu, JZ (2005) The Finite Element Method – Its Basis & Fundamentals. Butterworth-Heinemann, 6th edition 11. Zienkiewicz OC, Taylor, RL (2005) The Finite Element Method for Solid and Structural Mechanics. Butterworth-Heinemann, 6th edition 12. Perzyna P (1971) Thermodynamic Theory of Viscoplasticity. Academic Press, New York

164

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

13. Lad`eveze P (1983) On an anisotropic damage theory. In: J.P. Boehler, editor, Proc CNRS Int Coll 351 – Failure Criteria of Structured Media 355–363. Villars-de-Lans 14. Lemaitre J (1985) Coupled elasto-plasticity and damage constitutive equations. Comp Meth Appl Mech Engng 51:31–49 15. Odqvist FKG, Hult J (1961) Some aspects of creep rupture. Arkiv f¨ or fysik 19(26):379-382 16. Rabotnov YN (1969) Creep rupture. In: M. Het´enyi and W.G. Vincenti (eds), Proc of the Twelfth International Congress of Applied Mechanics XII 342–349. Springer, Berlin, Germany 17. Lemaitre J, Chaboche JL (1990) Mechanics of Solid Materials. Cambridge Univ Press 18. Lemaitre J (1996) A Course on Damage Mechanics. Springer, 2nd edition 19. Lemaitre J (1983) A three-dimensional ductile damage model applied to deep-drawing forming limits. In: ICM 4 Stockholm Vol.2 1047–1053 20. Simo JC, Taylor RL (1985) Consistent tangent operators for rateindependent elastoplasticity. Comp Meth Appl Mech Engng 48:101–118 21. Ortiz M, Simo JC (1986) An analysis of a new class of integration algorithms for elastoplastic constitutive relations. Int J Num Meth Engng 23:353–366 22. Simo JC, Govindjee, S (1991) Non-linear b-stability and symmetry preserving return mapping algorithms for plasticity and viscoplasticity. Int J Num Meth Engng 31:151–176 23. Chadwick P, Ogden RW (1971) A theorem in tensor calculus and its application to isotropic elasticity. Arch Rat Mech Anal 44:54–68 24. Carlson DE, Hoger A (1986) The derivative of a tensor-valued function of a tensor. Quart Appl Math 44(3):409–423 25. Krieg RD, Krieg DB (1977) Accuracies of numerical solution methods for the elastic-perfectly plastic model. J Pressure Vessel Tech ASME 99:510– 515 26. Ortiz M, Popov EP (1985) Accuracy and stability of integration algorithms for elastoplastic constitutive relations. Int J Num Meth Engng 21:1561–1576 27. Vaz Jr. M, Owen DRJ (2001) Aspects of ductile fracture and adaptive mesh reﬁnement in damaged elasto-plastic materials. Int J Num Meth Engng 50:29–54, 2001.

On Multiscale Analysis of Heterogeneous Composite Materials: Implementation of Micro-to-Macro Transitions in the Finite Element Setting D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi Centre for Civil and Computational Engineering School of Engineering, Swansea SA2 8PP, UK [email protected] Summary. This paper describes a multiscale homogenization procedure required for computation of material response of non-linear microstructures undergoing small strains. Such procedures are important for computer modelling of heterogeneous materials when the length-scale of heterogeneities is small compared to the dimensions of the body. The described homogenization procedure is based on the standard ﬁnite element discretisation of both macro- and micro-structure. The attention is restricted to two dimensional problem and the deformation-driven microstructures. Two classical types of boundary conditions are imposed over the unit cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. These boundary conditions satisfy the fundamental averaging condition, which equates microscopic and macroscopic virtual work. Numerical simulations, performed for an elasto-plastic material with micro-cavities, illustrate the scope and beneﬁts of the described computational strategy.

1 Introduction The ever increasing requirements in high-performance applications have provided a constant stimulus for the design of new materials. Often, this has been achieved by appropriately manipulating microstructure, for instance, by adding certain material component to the matrix phase, thus tailoring the overall material properties to speciﬁc applications. The added material phase is typically at a scale that is much smaller than the overall structural size, hence making the direct modelling of the material behaviour impractical. In many situations scales remain tightly coupled and the traditional phenomenological approach does not provide suﬃciently general predictive modelling capability. Therefore a means of continuous interchange of information be-

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 165–185. © 2007 Springer. Printed in the Netherlands.

166

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

tween scales is needed if predictive modelling of material behaviour is to be attempted. Since the basic principles for the micro-macro modelling of heterogeneous materials were introduced (see Suquet [12, 13]), this technique has proved to be a very eﬀective way to deal with arbitrary physically non-linear and time dependent material behaviour at micro-level. A number of recent works has been concerned with various approaches and techniques for the micromacro simulation of heterogeneous materials. Among these we highlight the contributions by Moulinec and Suquet [10], Smit et al. [11], Miehe and coworkers [7, 8, 9], Kouznetsova et al. [5], Terada and Kikuchi [15] and Zohdi and Wriggers [16]. The present article discusses some issues related to computational strategy for homogenisation of microstructures with non-linear material behaviour undergoing small strains. Since the aim is to provide the basic ingredients of the computational strategy allowing for the concurrent simulation at diﬀerent scales of the model, a simple model is considered comprising two scales arising, for instance, in modelling of heterogeneous composite materials. The focus of this article is on computational aspects; more speciﬁcally on the computational technique for prescribing the boundary conditions at the micro-scale and calculation of the macro-scale tangent moduli characterising relations between the macroscopic stress and strain tensors. The attention is restricted to the deformation-driven microstructures, which have been proven to provide a convenient computational format [14]. Two types of boundary conditions are imposed over the unit micro-cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. These boundary conditions satisfy the fundamental Hill-Mandel averaging condition, which equates microscopic and macroscopic virtual work [4]. The resulting computational strategy is characterised by the Newton-Raphson solution of the discrete boundary value problem, and incorporates the appropriate tangent operators. Numerical examples of both micro-scale and two-scale ﬁnite element simulations are presented in order to illustrate the scope and the beneﬁts of the described computational strategy.

2 Continuum Model at Small Strains 2.1 Preliminaries A homogenized macro-continuum B ⊂ R3 with locally attached microstructures B ⊂ R3 is visualized in Fig. 1. A point x ∈ B of the homogenized macromedium B ⊂ R3 is represented as a microstructure B ⊂ R3 . The tensors σ and σµ denote the macro and micro Cauchy stress tensor at x ∈ B and y ∈ B, respectively. The representative volume element (RVE) of the microstructure V ⊂ R3 represents the part of the heterogeneous material consisting of the solid part B and the hole H, i.e. V = B ∪ H and ∂B = ∂V ∪ ∂H.

On Multiscale Analysis of Heterogeneous Materials

167

Fig. 1. Micro to macro transition

It is assumed that the traction ﬁeld on the surface of the holes in the interior of RVE vanishes, i.e. t(y , t) = 0 at y ∈ ∂H, where t ≡ σµ n on ∂B is the traction ﬁeld vector on the surface with outward normal n at y ∈ ∂B. 2.2 Basic Microvariables Microscopic small strain tensor µ is deﬁned as the symmetric part of the displacement gradient tensor, µ ≡ sym{∇(u)}

(1)

where u is the displacement ﬁeld at a material point y ∈ B. Microequilibrium state is assumed in the presence of body forces per unit of mass b, (2) div(σµ ) + ρ b = 0 in B , where symmetric stress tensor σµ is assumed to be related to the strain tensor µ by some constitutive law ˆ µ ; α ; y ) in B, σµ = σ(

(3)

where α is the set of internal variables. 2.3 Basic Macrovariables and Averaging Theorem Within the described homogenization technique no constitutive assumptions have been assumed at the macrolevel. Overall macrostress σM of microstructure V is deﬁned as an average of the microstresses over the unit cell. By applying the Gauss theorem and microquilibrium (2), σM is given by the expression 1 1 1 σM ≡ σ = σµ dV = sym[t ⊗ y ] dA + ρ sym[b ⊗ y ] dV |V| V |V| ∂V |V| V (4)

168

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

in terms of the traction t at y ∈ ∂V and body force vector ﬁeld b at y ∈ V. By applying Green’s Lemma in similar way, overall macrostrain M is deﬁned, 1 1 µ dV = sym[u ⊗ n] dA (5) M ≡ = |V| V |V| ∂V in terms of the displacement u at y ∈ ∂V. Overall tangent modulus C relates the variations of overall macrostress σ and the macrostrain in the form C ≡

dσ d

(6)

The computation of these fourth-order tensors, in their discrete FE form, is an important aspect of this work. The Hill-Mandel Principle The Hill-Mandel principle or averaging theorem [4], demands that macroscopic stress work (or power) must equal the volume average of the microscopic stress work (or power) over the RVE associated with the macroscopic point, that is 1 σ: = σ : dV (7) |V| V Using (1) and integrating by parts the right hand side of (7) and then applying microequlibrium (2), the averaging theorem can be expressed in the following form 1 1 σ: = t · u dA + ρ b · u dV (8) |V| ∂V |V| V 2.4 Deﬁnition of the Boundary Conditions for the Small Scale The boundary conditions for the displacement u and traction t at the microstructure, are chosen such that condition (7) is satisﬁed. Two classical types of boundary conditions that satisfy these conditions are prescribed on the unit cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. A crucial aspect is the formulation in deformation-driven context, where the macroscopic strain is prescribed as averaged over the microstructure. The deformation-driven format has proved more convenient than the stress driven format [14]. The displacement ﬁeld is divided in two parts: (y ) = y + u (y ), u(y ) = u∗ (y ) + u

(9)

where u∗ is the Taylor displacement, which deﬁnes a constant deformation over the unit cell as (10) u∗ ≡ y .

On Multiscale Analysis of Heterogeneous Materials

169

∂V

V

Fig. 2. Microstructure for linear b.c.

is known as the displacement ﬂuctuation, which is conThe component u sidered to be unknown. Insertion of (9) into the averaging theorem (8) yields in the following new form of the Hill-Mandel principle 1 1 dA + dV = 0 t·u ρb · u (11) |V| ∂V |V| V Linear displacements on the boundary In this state, the deﬁnition of the linear deformation boundary constraint over the microstructure RVE shown in Fig. 2 assumes the following form (y ) = 0 u

at y ∈ ∂V.

(12)

This condition deﬁnes a linear deformation on the boundary ∂V of the RVE. Insertion of the above condition (12) into the new averaging condition form (11) conﬁrms that this model satisﬁes the averaging theorem only when body force eﬀect is negligible. Periodic deformation and antiperiodic traction on the boundary Another possibility consists of applying periodic deformation and antiperiodic traction on the boundary of the RVE ∂V, which can be represented as (y − ) and t(y + ) = −t(y − ). (y + ) = u u

(13)

In order to apply these conditions the boundary of the unit cell is decomposed in two parts as indicated in Fig. 3. Thus ∂V = ∂V + ∪ ∂V − with outwards normals n+ = −n− which are associated with the points y + ∈ ∂V + and y − ∈ ∂V − . The body force eﬀect is not taken into consideration so that this condition satisﬁes the averaging theorem. This can be proved easily by inserting (13)1 and (13)2 into (11).

170

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

∂V + V

∂V −

Fig. 3. Microstructure for periodic b.c.

V B

B H

Fig. 4. Micro to macro transition

3 Discretised Model at Small Strains 3.1 Introduction The discretisation of the continuum multi-scale problem described in Section 2 is based on ﬁnite element formulation. A representative ﬁnite element dicretisations of the macro and microstructure are depicted in Fig. 4. One can notice that at every integration Gauss point of the macrostructure, a discrete RVE microstructure is considered as representation of a Gauss point at the macro-level. The present approach is based on the deformation-driven microstructures, in which the value of the overall macroscopic deformation is prescribed on the discretised RVE. The goal is then to develop a numerical procedure for computing macroscopic average stress σ and the overall tangent moduli C at each macroscopic integration point with locally attached microstructure.

On Multiscale Analysis of Heterogeneous Materials

171

3.2 Displacement Field Partition and Matrix Notation Following the previous Section 2.4, where the continuum displacement ﬁeld partition (9) was established, the displacement ﬁeld is divided in two parts: u = u∗ + u

(14)

where the Taylor displacement u∗ (previously deﬁned in the continuum form (10)) is expressed in its discrete form u∗j ≡ y j

j = 1 ··· n

(15)

for the n nodes of the discretised microstructure RVE. The displacement ﬂuc is the unknown for every node of the discretised microstructure. tuation u In what follows the standard ﬁnite element matrix notation will be used, where the tensor entities so far used, can be expressed in the matrix form as ⎧ ⎧ ⎫ ⎫

⎨ ε11 ⎬ ⎨σ 11 ⎬ u1 f1 ε22 , uj ≡ ≡ , σ ≡ σ 22 and fj ≡ . (16) u f2 j ⎩ ⎩ ⎭ ⎭ 2 j 2 ε12 σ 12 Here is the matrix representation of the macrostrain tensor, uj is the displacement ﬁeld at the node j of the discretised unit cell V, σ is the averaged stress ﬁeld while fj denotes the force vector associated with the microcell node j. The Taylor displacement u∗j of the node j is computed in the following matrix form j = 1 · · · n. (17) u∗j = DT j , where Dj is the coordinate matrix at node j of the microstructure deﬁned in [9]. 3.3 Discretised Micro-equilibrium State and Solution Procedure Following standard procedure, the discrete boundary value problem is formulated as follows: Find the nodal displacements global vector u, such that r(u) ≡ f int (u) − f ext = 0

(18)

where f int and f ext are, respectively, the internal and external global force vectors, and r is the residual (or out-of-balance force) vector. An iterative Newton-type procedure for the solution of the Non-linear microscopic equilibrium (18) is considered here. Each iteration determines the current ﬂuctuation ﬁeld assuming frozen macroscopic strain . At the end of the procedure, when microequilibrium is reached, the averaged macroscopic stress over the microstructure RVE can be updated.

172

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

3.4 General Average Stress and Overall Tangent Modulus Computation Average Stress Computation Assuming no body forces in the expression for the average stress (4), in the discrete setting, t dA → f ext j , that is the inﬁnitesimal force t dA becomes the ﬁnite force f ext at position y j on the boundary ∂V. Therefore (4) degenerates j into the discrete sum σ =

nb 1 sym[f ext ⊗ yj] j |V| j = 1

(19)

where nb is the number of nodes on the boundary ∂V. Using matrix representation this expression becomes σ =

nb 1 Dj f ext j |V| j = 1

(20)

where Dj is the coordinate matrix evaluated at node j on the boundary of the discretised microstructure RVE. The above expression can be rearranged in the following global expression σ =

1 Db f ext , b |V|

(21)

where f ext is the external nodal force vector of the boundary nodes, and Db b is the boundary coordinate matrix deﬁned by:

Db ≡ Db1 Db2 . . . Dbnb . (22) Overall Tangent Modulus Computation In the computational homogenization approach no explicit form of the constitutive behavior on the macrolevel is assumed a priori, so that the tangent modulus has to be determined numerically by relations between variations of the macroscopic stress and variations of the macroscopic strain at such integration point. This can be accomplished by numerical diﬀerentiation of the numerical macroscopic stress strain relation, for instance, by using forward diﬀerence approximations as suggested in [8]. An alternative approach is to condense the microstructural stiﬀness matrix to the macroscopic matrix tangent modulus. This task is achieved by reducing the total RVE system of equations to the relation between the forces acting on the boundary ∂V and the displacement on the boundary. This procedure has been used in [5], [6], and also in [9], in combination with the Lagrange multiplier method to impose the boundary constraints. A similar scheme have been used in this work

On Multiscale Analysis of Heterogeneous Materials

173

whereby the direct condensation is employed to obtain a relation between the forces acting on the boundary ∂V and the Taylor displacement on the boundary nodes array u∗ which depends linearly on the macroscopic strain . The total microstructural system of equations that gives the relation between the iterative nodal displacement du and iterative nodal external force vectors is (23) K du = df ext With the displacement partition (14) the system can be rearranged as u = df ext ⇒ K d u = df ext − K du∗ ⇒ K du∗ + K d

(24)

The boundary constraints are then applied to this system in the following sections to condense the system. This procedure gives the expression that against the variation relates the variation of boundary external forces df ext b of the Taylor displacement du∗ . 3.5 Linear Displacements on the Boundary Assumption In view of the discrete formulation of the boundary conditions outlined before in section 2.4, the nodes of the mesh are partitioned into those on the surface ∂V of RV and those in the interior of V. In this mesh nb boundary nodes and ni internal nodes are distinguished. More details of the discrete form of this linear constraint are given in [1]. Partitioning of Algebraic Equations Partitioning of the current nodal displacements and internal forces is given as

Li u Li f fi ui ≡ ≡ and f = . (25) u= ub fb Lb u Lb f Here Li and Lb are the connectivity matrices [2], which deﬁne the contributions of the interior and boundary nodes, respectively. These are Boolean matrices, i.e. they consist of integers 0 and 1. Displacements ui and ub are arranged as shown in (25). In line with (25) the tangent stiﬀness matrix is rearranged as df int Li K LT Li K LT kii kib i b = ≡ K= T kbi kbb Lb K LT du i Lb K Lb

(26)

into contributions associated with internal nodes and nodes on the surface of the RVE.

174

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Linear Displacement At each node j of the boundary ∂V the condition (12) induces the discrete constraint j = 0, j = 1 · · · nb . u (27) According to the matrix notation introduced in Section 3.2, we deﬁne the global coordinate matrix

(28) Dglobal,l ≡ Di Db,l , where Di and Db are the interior coordinate matrix and the boundary coordinate matrix, respectively, given as

and Db,l ≡ Db1 Db2 . . . Dbnb . (29) Di ≡ Di1 Di2 . . . Dini Matrices Di and Db are deﬁned in terms of the node coordinate matrices of the interior and boundary nodes, as discussed in Section 3.2. The Taylor displacement u∗ deﬁned in (17), is now represented in global form as u∗ = DT global,l , where is the matrix representation of the prescribed macroscopic strain (16). In this model the variation of the Taylor displacement vector du∗ is represented as (30) du∗ = DT global,l d, that is, as a function of the variation of the macroscopic average strain vector d. Tangent Modulus of Linear Displacements on the Boundary Constraint Using Partitioning of the algebraic equations (25) and (26), the system (23) = 0. can be rewritten for the case when df ext i The general procedure explained in Section 3.4, where the rearranged system (24) was obtained, is followed. By applying linear displacement constraint in discrete form (27) and by using the Taylor displacement variation du∗ given by (30), after some algebraic manipulation, a variation for the external nodal force vector at the boundary nodes is obtained as B T df ext b = K lin Dglobal,l d

(31)

in terms of the global coordinate matrix (28) and the overall averaged macrostrain. The overall tangent moduli deﬁned in (6), can be computed in its discretised matrix form, using previous averaged stress expression (21), in the following way 1 dσ df ext b = Db (32) Cl = d |V| d

On Multiscale Analysis of Heterogeneous Materials

175

Substituting (31) into (32), the overall tangent modulus representation is obtained as 1 T Db,l K B Cl = (33) lin Dglobal,l . |V| Clearly the modulus C l is given as a function of the boundary coordinate matrix Db,l deﬁned in (29), the condensed stiﬀness matrix K B lin and the global coordinate matrix DT global,l outlined in (28). Finally we remark that using (33) the tangent moduli can be computed for heterogeneous material with arbitrary microstructures. When using this tangent modulus the quadratic rate of convergence is attained at the macroscopic level. 3.6 Periodic Displacements and Antiperiodic Traction on the Boundary In order to discretise the continuum model of the periodic boundary conditions described in 2.4, the nodes of the mesh are partitioned in four groups: 1) ni interior nodes, 2) np positive boundary nodes which are located at the top and right of the microstructure boundary ∂V of the RVE, 3) np negative boundary nodes which are located at the bottom and left of the microstructure boundary ∂V of the RVE, and 4) nc = 4 node at the corners. More details on these discrete constraints are given in [1]. Partitioning of Algebraic Equations The partition of the nodal displacements and internal forces for the periodic boundary condition is as follows ⎫ ⎧ ⎫ ⎧ ⎫ ⎫ ⎧ ⎧ fi ⎪ Li u ⎪ Li f ⎪ ui ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎬ ⎨ ⎬ ⎨ ⎬ ⎬ ⎨ ⎨ fp up Lp u Lp f u= ≡ ≡ and f = (34) un ⎪ Ln f ⎪ f ⎪ ⎪ ⎪ Ln u ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎭ ⎪ ⎭ ⎪ ⎭ ⎭ ⎩ ⎩ ⎩ n⎪ ⎩ uc Lc u Lc f fc Here Li , Lp , Ln and Lc are the connectivity matrices which deﬁne respectively: the interior contribution, the contribution of positive boundary nodes, the one from their corresponding negative boundary nodes, and ﬁnally the contribution from the nodes at the corners. In correspondence to (34), the tangent stiﬀness matrix is partitioned in the following way ⎡ ⎤ ⎡ ⎤ T T T Li K LT kii kip kin kic i Li K Lp Li K Ln Li K Lc T T T T⎥ ⎢ df int ⎢ kpi kpp kpn kpc ⎥ ⎥≡⎢ Lp K LiT Lp K LpT Lp K LnT Lp K LcT ⎥ . =⎢ K= ⎣kni knp knn knc ⎦ ⎣ Ln K Li Ln K Lp Ln K Ln Ln K Lc ⎦ du T T T kci kcp kcn kcc Lc K LT i Lc K Lp Lc K Ln Lc K Lc (35)

176

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Periodic Displacements and Antiperiodic Tractions At each node pair j on the boundary ∂V + ∪ ∂V − , the continuum conditions (13)1 and (13)2 induce discrete constraints at boundary nodes of the discretised RVE. The displacement ﬂuctuation at the corners is prescribed to zero in order to avoid the solid rigid body motion. Using the matrix notation introduced in Section 3.2, we redeﬁne the global coordinate matrix for the periodic b.c. assumption as

(36) Dglobal,p ≡ Di Db,p where Di is the interior coordinate matrix deﬁned in (29) and the Db,p is the boundary coordinate matrix for periodic assumption deﬁned this time as

(37) Db,p = Dp Dn Dc where Dp , Dn , Dc are the positive boundary coordinate matrix, negative boundary coordinate matrix and corner coordinate matrix, respectively. The Taylor displacement u∗ deﬁned as a constant for each node in (17), is given in a compact form as u∗ = DT global,p , where Dglobal,p is the global coordinate matrix for periodic assumption and is the matrix representation of the prescribed macroscopic strain tensor. In this model the variation of the Taylor displacement vector du∗ is considered as follows du∗ = DT global,p d ,

(38)

i.e. the displacement du∗ is a function of the variation of the macroscopic average strain vector d. Tangent Modulus of Periodic Displacements and Antiperiodic Traction on the Boundary Constraints After rearranging the displacement nodal vector u, the external nodal force vector f ext and the stiﬀness matrix K, as deﬁned in (34) and (35), respectively, the general system (23) that relates the variations du and df ext can be obtained. Again the general procedure of Section 3.4 is followed to rearrange the system in the way described in (24). The variation of the Taylor displacement du∗ is given by (38). In this system the displacement ﬂuctuation variation vector d u is considered as unknown. The application of the periodic displacement and antiperiodic external force in its discrete form, after some algebraic operations, gives the variation of the external force vector as B T df ext b = K per Dglobal,p d

(39)

where the Taylor displacement variation (38) has been inserted into the above

On Multiscale Analysis of Heterogeneous Materials

177

equation (39). Therefore the desired expression is obtained as df ext b T = KB per Dglobal,p d

(40)

in terms which gives the sensitivity of external boundary force vector df ext b of the macroscopic average strain matrix d. The overall tangent moduli deﬁned in (6), can be computed in its discretised F.E. matrix form, using previous averaged stress expression (21), in the following way 1 df ext dσ b = Db,p (41) Cp = d |V| d Inserting (40) into (41), the overall tangent modulus matrix form for periodic deformation and antiperiodic traction on the boundary of RVE is ﬁnally obtained as 1 T Db,p K B Cp = (42) per Dglobal,p . |V| Clearly the modulus Cp is a function of the boundary coordinate matrix Db,p deﬁned in (37), the condensed periodic stiﬀness matrix K B per and the global coordinate matrix Dglobal,p outlined in (36). Finally we remark that with the above expression (42), the tangent moduli can be computed for heterogeneous materials with arbitrary microstructures of the RVE. This results in the desired quadratic rate of convergence of the Newton-type solution procedure applied to solve the homogenized nonlinear macrostructure under periodic deformation and antiperiodic traction on the boundary of the RVE.

4 Numerical Examples In this section numerical examples are presented in order to illustrate the scope and beneﬁts of the described computational strategy. First set of numerical simulations focuses on microstructure simulations and discusses some important issues regarding numerical analysis at the micro-level such as the effect of boundary conditions, topology and distribution of heterogeneities, etc. Second numerical example considers a full two-scale simulation of a boundary value problem and incorporates all computational ingredients described in this paper. This example also includes a comparison with a detailed single scale analysis. 4.1 Study of the Eﬀect of Topology of Cavities on the Properties of the RVE Problem Speciﬁcations A square unit cell is considered representing an RVE at the micro-level. The cell is composed of an elasto-plastic material with heterogeneity being induced

178

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 5. Regular cavity model

by cavities. Two models are considered: (i) a regular cell with a single circular hole embedded in a soft matrix depicted in Fig. 5, (ii) randomly generated distribution of cavities surrounded by soft matrix given in Fig. 7. For both models the void volume fraction of the unit cell is taken as 15%. Two types of ﬁnite elements are employed: linear 3-noded triangle element and 8-noded quadrilateral element with 4-Gauss points. The matrix in all models is assumed to be composed of the von Mises elasto-plastic material with linear strain hardening. The material properties assigned are: Young’s modulus E = 70 GP a, Poisson’s ratio ν = 0.2, the initial yield stress σY0 = 0.243 GP a and the strain hardening modulus H = 0.2 GP a. Analysis Approach All simulations in this section have been performed by employing the computational homogenisation under the plane-stress assumption in small strain regime. The average stress is obtained by imposing the macro-strain over the unit cell and solving the problem for deﬁned boundary condition over the RVE. The generic imposed macro-strain tensor is expressed by: ε12 ] = [0.001, 0.001, 0.0034] . [¯ ε11 , ε¯22 , 2¯ To obtain the load step at each load increment, the generic strain tensor is multiplied by the relevant load factor. The analysis is performed under two diﬀerent boundary conditions: (i) linear displacement boundary condition, and (ii) periodic displacement boundary condition. Study of the Regular Cavity Model An 8-node quadrilateral element with 4-Gauss points is employed in this simulation. Figure 5 depicts a ﬁnite element mesh containing 350 elements and 1158 nodes. Figures 6 (a) and (b) show, respectively, the deformed mesh and the equivalent plastic strain distribution for the linear displacement boundary condition. This plastic zone is clearly positioned along the diagonal side of the unit

On Multiscale Analysis of Heterogeneous Materials

179

Fig. 6. Regular cavity model under linear displacement boundary condition and periodic condition. a) Deformed mesh. b)Eﬀective plastic strain contour plot

cell in direction of the imposed shear. The corresponding results for the periodic boundary condition are given in Figs. 6 (c) and (d). From Fig. 6, it can be seen that the plastic zone has a distinctively diﬀerent pattern under periodic boundary condition. The overall stress-strain response is presented in terms of the Euclidean norm of the average stress and strain, given, respectively as 2 +σ 2 +σ 2 , ¯11 ¯22 ¯12 ¯ ε = ε¯211 + ε¯222 + ε¯212 . ¯ σ = σ Figure 9 shows the resulting average stress - strain curves for this model. The obtained results show that under linear displacement boundary condition the overall response of the regular cavity model shows signiﬁcantly stiﬀer behaviour with respect to the overall response under periodic boundary condition. The RVE with Randomly Generated Voids In this study a unit cell at the micro-level with a randomly generated distribution of void placements and sizes is considered (see Fig. 7). A standard 3-node linear triangular element is employed in this simulation. Again planestress conditions are prescribed and two boundary conditions at the micro-

180

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 7. Unit cell with randomly generated voids

level are considered: (i) linear displacement boundary condition, and (ii) periodic boundary condition. The imposed macro-strain and material properties for this model are identical to the previous examples in this section. Figure 8 shows the equivalent plastic strain distribution for both linear displacement boundary condition and periodic boundary conditions. The occurrence of localised bands with signiﬁcant plastic straining can be observed on both contour plots. Signiﬁcantly, unlike in the case of the single cavity model both boundary conditions give similar distribution of the plastic strain indicating the convergence of the results at the micro-level with the increase of the statistical sample of heterogeneities. Figure 9 shows the average stress - strain curves for this model. It can be observed that the micro-cell with randomly generated void distribution results in the stress-strain behaviour that shows small diﬀerence between the two diﬀerent boundary conditions imposed at the micro-level. This clearly indicates the convergence of the average properties with the increase of the statistical sample representing the heterogeneities at the micro-level. 4.2 Two-scale Analysis of Stretching of an Elasto-plastic Perforated Plate In this section a full two-scale analysis of a perforated plate is performed. This is a classical example often used as a veriﬁcation problem in computational plasticity. The plate is composed of an elasto-plastic material and contains regularly distributed voids. The plate has width 10 mm, length 18 mm and

On Multiscale Analysis of Heterogeneous Materials

181

Fig. 8. Eﬀective plastic strain contours for the unit cell with randomly generated voids under two boundary conditions

Fig. 9. Stress-Strain norm curves for dense model under two boundary conditions

uniform thickness of 1 mm (see Fig. 10). For obvious symmetry reasons only one-quarter of the specimen is considered (see Fig. 10). The simulation is performed by imposing uniform displacement along the upper boundary. The elasto-plastic material is assumed to follow the standard von Mises model with linear isotropic hardening. Material properties are: Young modulus E = 70 GP a, Poisson’s ration ν = 0.2, yield stress σY0 = 0.243 GP a and hardening modulus H = 0.2 GP a. Both two-scale analysis and a single scale analysis of this problem are performed.

182

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

R=

Fig. 10. Plane-stress strip with a circular hole. Geometry and boundary conditions

Single-scale Analysis Single scale analysis is used for comparative purposes and is performed on a detailed ﬁnite element mesh of the problem given in Fig. 11 (a). The mesh is composed of 11216 4-node quadrilateral elements and 12147 nodes. Figure 11 (b) illustrates distribution of an equivalent plastic strain at latter stages of the simulation. Two-scale Analysis For the multi-scale ﬁnite element analysis the perforated plate is deﬁned as a homogeneous structure at the macro-level, while at the micro-level a unit cell is deﬁned with side length equal to 1 mm and a single void in the centre of the micro-cell giving the volume fraction of 50%. Linear 3-noded triangle element is employed at both macro and micro-level (see Fig. 12). The mesh at the macro-level number is composed of 25 elements and 21 nodes, while at the micro-level the FE mesh is composed of 603 elements and 352 nodes. Multi-scale analysis has been performed under three diﬀerent boundary conditions at the micro-level: (i) Taylor assumption, (ii) linear displacement boundary condition and (iii) periodic boundary condition. As can be seen from Fig. 13, which gives reaction force against the prescribed displacement, diﬀerent boundary conditions result in markedly diﬀerent force-displacement diagrams. As expected, the results obtained for the Taylor assumption show substantially stiﬀer behaviour with comparison to the other two boundary assumptions. Periodic boundary assumption generates the softest response, and signiﬁcantly the resulting overall behaviour shows very good correspondence with the results obtained by the detailed single-scale analysis.

On Multiscale Analysis of Heterogeneous Materials

a)

183

b)

Fig. 11. Single-scale analysis of an elasto-plastic perforated plate: (a) Finite element mesh, and (b) distribution of equivalent plastic strain

Fig. 12. FE meshes at macro- and micro-level for multi-scale analysis

5 Conclusions A multiscale computational strategy for homogenisation of material behaviour of heterogeneous composites has been described. The presented numerical tests have conﬁrmed the successful implementation of the computational procedure and eﬃcient solution of the discrete multiscale problem.

184

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 13. Reaction along Y direction against the applied displacement

The ongoing research is concerned with the analysis of more general nonlinear material behaviour at the microscale and incorporation of the ﬁnite strain kinematics. This work will be reported in future publications.

References 1. Carneiro Molina AJ, de Souza Neto EA and Peri´c D (2005) Homogenized tangent moduli for heterogeneous materials. In: Crouch P (ed) Proceedings of the 13th ACME Conference. Sheﬃeld UP, Sheﬃeld 2. Belytschko T, Liu WK, Moran B (2000) Nonlinear Finite Element for Continua and Structures. Wiley, New York 3. de Souza Neto EA, Peri´c D, Owen DRJ (to be published) Computational Plasticity: Small and Large Strain Finite Element Analisys of Elastic and Inelastic Solids. 4. Hill R (1972) On constitutive macro-variables for heterogeneous solids at ﬁnite strain. Proc Roy Soc London 326:131-147 5. Kouznetsova VG, Brekelmans WAM, Baaijens FPT (2001) An Approach to micro-macro modelling of heterogeneous materials. Comput Mech 27:37-48 6. Kouznetsova VG (2002) Computational homogenization for multiscale analysis of multi-phase materials PhD Thesis, TU University Eindhoven, Eindhoven 7. Miehe C, Schotte J and Schr¨ oder J (1999) Computational micro-macro transitions and overall moduli in the analysis of polycrystals at large strains. Comput Material Sci 16:372-382 8. Miehe C, Schr¨ oder J and Schotte J (1999) Computational homogenization analysis in ﬁnite plasticity - Simulation of texture development in polycrystalline materials. Comp Meth Appl Mech Engng 171:387-418 9. Miehe C and Koch A (2002) Computational micro-to-macro transitions of discretized microstructures undergoing small strains. Arch Appl Mech 72:300-317 10. Moulinec H and Suquet P (1998) A numerical method for computing the overall response of nonlinear composites with complex microstructure. Comp Meth Appl Mech Engng 157:69-94

On Multiscale Analysis of Heterogeneous Materials

185

11. Smit RJM, Brekelmans WAM and Meijer HEH (1998) Prediction of the mechanichal behaviour of nonlinear heterogeneous syatems by multi-level ﬁnite element modeling. Comp Meth Appl Mech Engng 155:181-192 12. Suquet PM (1985) Local and global aspects in the mathematical theory of plasticity. In: Sawczuk A (ed) Plasticity today: modelling methods and applications. Elsevier Applied Science Publishers, Amsterdam 13. Suquet PM (1987) Elements of homogenization for inelastic solid mechanics. In: Sanchez-Palencia E and Zaoui A (eds) Homogenization Techniques for Composite Media. Springer-Verlag, Berlin 14. Swan CC (1994) Techniques for stress-controlled and strain-controlled homogenization of inelastic periodic composites. Comp Meth Appl Mech Engng 117:249-267 15. Terada K and Kikuchi N (2001) A class of general algorithms for multi-scale analyses of heterogeneous media. Comp Meth Appl Mech Engng 190:5427-5464 16. Zohdi TI and Wriggers P (2005) Introduction to Computational Micromechanics. Springer, Berlin

Assessment of Protection Systems for Gravel-Buried Pipelines Considering Impact and Recurrent Shear Loading Caused by Thermal Deformations of the Pipe B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang Institute for Mechanics of Materials and Structures Vienna University of Technology Karlsplatz 13/202, A-1040 Vienna, Austria e-mail: [email protected] Summary. Two safety topics in pipeline engineering are considered: (1) rockfall onto gravel-buried steel pipes and (2) protection of the outer anti-corrosion coating of soil-covered steel pipelines. For both cases, eﬀective protection systems are identiﬁed, based on the results of non-linear elasto-plastic Finite Element analyses.

Introduction Two safety topics in pipeline engineering will be treated: (i) rockfall onto gravel-buried steel pipes and (ii) protection of the outer anti-corrosion coating of soil-covered steel pipelines. In both cases non-linear elasto-plastic Finite Element (FE) analyses provide insight into the structural behavior, as needed for the design of eﬀective protection systems. For rockfall, a two-component protection system is recommended. It consists of an impact damping layer and of a buried load-distributing and load-carrying structure. As regards wear of the anti-corrosion coating, two well-established means of protection are considered to be most eﬀective: (i) burying pipelines by sand and (ii) covering pipelines by (ﬁbre-)reinforced concrete.

1 Protection Systems for Gravel-Buried Pipelines Subjected to Rockfall Recent increase of rockfall activities in the European Alps has raised the need for designing impact protection systems for pipelines in Alpine valleys. This section deals with the assessment of diﬀerent protection systems including

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 187–206. © 2007 Springer. Printed in the Netherlands.

188

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

surface of structure gravel H. . . height of overburden s = 11.13 mm sand 90 cm

d=1016 mm 50 cm

150 cm soil/rock Fig. 1. Geometric dimensions of the gravel-buried steel pipeline in a section perpendicular to the axis of the pipe

sandy gravel as an energy-absorbing and load-distributing structural component. In Subsection 1.1, the development of a FE model allowing for prediction of the loading of a gravel-buried steel pipe subjected to rockfall is described. In Subsection 1.2, results from a real-scale impact experiment of a boulder onto a buried steel pipe are used for an assessment of this model. To ensure the signiﬁcance of this validation procedure, the identiﬁcation of the model parameters is based on experiments which are independent of the real-scale impact test. Finally, in Subsection 1.3 and 1.4, respectively, the structural model is used to study the performance of two diﬀerent rockfall-protection systems covering a steel pipe. 1.1 Development of a Structural Model Geometric Dimensions of the Considered Problem A pipeline with an outer diameter d = 1016 mm and a wall thickness s = 11.13 mm is considered. It is buried in the middle of a trench of 3 m width, resting on a 50 cm thick layer of sand. The tube is laterally buried up to a height of 40 cm by sand. The rest of the trench is ﬁlled by sandy gravel, see Fig. 1. Impact Scenario and Mode of Analysis Single boulders impacting vertically, directly above the axis of the steel pipe, are considered as typical rockfall events. Making use of symmetries, it is sufﬁcient to discretize one fourth of the entire structure, see Fig. 2 (a). The material beside and beneath the trench is represented by a Winkler foundation modeled by bar elements representing linear springs, see Figs. 1 and 2 (a).

Protection Systems for Gravel-Buried Pipelines

189

Fig. 2. (a) FE discretization used for the validation of the structural model; (b) axisymmetric analysis performed to obtain the distribution of surface loads applied to the 3D FE model

Dead load results in stresses in the pipe, which are by two orders of magnitude smaller than the stresses caused by the investigated types of impact. Therefore, dead load is not taken into account and, hence, the overburden of the pipe is only discretized to simulate the load distribution. Since the impact stresses in the backﬁll material above the pipe occur only in the vicinity of the impact axis, the discretization of the overburden of the pipe is restricted to a longitudinal distance of 3.4 m from the impact axis, see Fig. 2 (a). Outside this domain, only the backﬁll material beside and beneath the tube is discretized. The penetration process is not modeled in detail. Instead, the height of the overburden H is reduced by the penetration depth W at which the maximum impact force occurs, see Fig. 2 (a). Both dynamic and static 2D plain strain analyses delivered approximately the same maximum stresses in the pipe [18]. Therefore, the maximum impact force is applied quasistatically onto the surface of the FE model. This mode of modeling requires estimates of (i) the maximum impact force and the penetration depth at maximum impact force, both as a function of the mass m and the impact velocity v0 of an impacting boulder, and (ii) the distribution of stresses corresponding to the maximum impact force, which are prescribed as stress boundary conditions for the FE analysis. Estimates of the Maximum Impact Force and the Penetration Depth at Maximum Impact Force The ﬁnal penetration depth X, i.e. the penetration depth after the end of the impact, is estimated based on the dimensionless formula [16] X m v2 1 + k π/4 N 4k X = I for ≤ k , with I = 3 0 , (1) d (1 + I/N ) π d d R where d denotes the characteristic size of the boulder, N is a geometry function characterizing the “sharpness” of the boulder nose, k stands for the dimen-

190

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

sionless depth of a surface crater, and R denotes the indentation resistance of the hit material. For cubic granite boulders with a volume V and a mass density equal to 2700 kg/m3 , impacting with a tip onto gravel with a mass density equal to 1800 kg/m3 , the following relationships were obtained based on a hybrid experimental-analytical approach [16] √ 3 (2) N = 2.385 , k = 1.257 , d = 1.050 V , and R = 9.22 MPa . Relations between X and the maximum impact force F , and between X and the penetration depth at maximum impact force, W , were derived on the basis of a model for the impact kinematics which was deduced from experimental acceleration measurements [16, 17] as m v02 W X 4 π2 = = . (3) d Fd d 3 π2 + 4 Computation of the Distribution of Stresses Corresponding to the Maximum Impact Force In order to perform a 3D FE analysis of rockfall onto gravel as described previously, the stress distribution corresponding to the maximum impact force must be speciﬁed. Herein, this stress distribution is computed by means of an axisymmetric linear-elastic FE model. It comprises the gravel and the tip of the granite boulder approximated as a conical indenter at a penetration depth W , see Fig. 2 (b). The maximum impact force F is applied to the conical indenter as a spatially constant surface stress σ. The material parameters for gravel and granite are taken from Table 1. The vertical stresses obtained for the axisymmetric FE model in a horizontal section through the model at the tip of the boulder, see Fig. 2 (b), serve as surface loads for the 3D FE model. Material Modeling of Steel, Gravel and Sand The material behavior of steel is modeled by small-strain von Mises elastoplasticity, see e.g. [10, 22] and Table 1 for Young’s modulus E, Poisson’s ratio ν, and the uniaxial yield strength σy . The material behavior of gravel is represented by the elasto-plastic Cap Model [3, 5, 19]. The elastic domain follows the isotropic generalized Hooke’s law [12]: σ = C : (ε − εp ) , where σ denotes the Cauchy stress tensor, and ε and εp stand for the linearized strain tensor and the plastic strain tensor, respectively. C represents the isotropic constitutive elasticity tensor which can be expressed as a function of the bulk modulus K and the shear modulus G, reading C = K 1I ⊗ 1I + 2G(II − 13 1I ⊗ 1I) , where 1I and II denote the 2nd-order unity tensor and the 4th-order unity tensor, respectively. In the principal stress space the elastic domain is bounded by three surfaces, (i) a tension cutoﬀ accounting for tensile failure, (ii) a Drucker-Prager surface deﬁning shear failure under pronounced deviatoric stress states, and (iii) an ellipsoidal cap

Protection Systems for Gravel-Buried Pipelines ||s||, ||ep||

f3 (σ, ζ) = 0 dεp

f2 (σ) = 0 √ dεpvol / 3

dεp √ RFe (ζ)/ 3

f1 (σ) = 0

√ 1/ 3 elastic α domain √ ζ/ 3

Fe (ζ)

√ dεpvol / 3

191

ϑ

√ X(ζ)/ 3

√ p dεp dεvol / 3 √

T/ 3

√ √ I1 / 3, εpvol / 3

Fig. 3. Cap model for gravel: elastic domain and direction of plastic ﬂow, respectively, in a meridional plane of the principal stress and the plastic-strain space, respectively

representing the hardening of the material associated with compaction, see Fig. 3. In mathematical terms, these functions read [8, 9] = I1 − T = 0 , f1 (σ) = s−Fe (I1 ) = 0 for T ≥ I1 ≥ ζ , f2 (σ) f3 (σ, ζ) = Fc (s, I1 , ζ) − Fe (ζ) = 0 for ζ ≥ I1 ≥ X(ζ) Fe (ξ) = α − ϑξ, 2 s + ([I1 − L(ζ)]/R)2 Fc (s, I1 , ζ) =

and

L(ζ) =

ζ 0

(4) with if if

ζ < 0, ζ ≥ 0,

where I1 and s denote the ﬁrst invariant of the stress tensor and the deviatoric stress tensor, respectively. The direction of plastic ﬂow is given by the associated ﬂow rule [7] ∂fα , (5) dλα dεp = ∂σ α∈Jact

where the consistency parameters are denoted as dλα , whereas Jact stands for the set of active yield surfaces, deﬁned as Jact = {α ∈ [1, 2, 3] | fα (σ, ζ) = 0}. Activation of the cap mode leads to compaction, whereas activation of the failure-surface mode or the tension cut-oﬀ mode results in plastic volume dilatation, see Fig. 3. The tension cut-oﬀ and the Drucker-Prager surface are ﬁxed in the stress space. The ellipsoidal cap, however, expands if it is activated, reﬂecting material compaction described by εpvol = −W (1 − exp[D X(ζ)]) ,

with

X(ζ) = ζ + R Fe (ζ) ,

(6)

where ζ denotes the hardening state variable. Algorithmic issues of this model as well as the expressions for the consistent tangent moduli can be found in [5, 8, 9, 22].

192

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Parameter Identiﬁcation The parameters K and G of the backﬁll material are identiﬁed on the basis of the theory of elastic waves from a series of small strain acoustic experiments on unloaded sandy gravel [15], see Table 1. The tested material (mass density of 1800 kg/m3 ) consisted to 60–80 % of particles with diameters < 70 mm, and to 20–40 % of edged stones with diameters from 70 mm – 200 mm. The loading surfaces of the Cap Model are deﬁned by seven material parameters (see Fig. 2 (b)): T , α, ϑ, W , D, R, and ζini , denoting the initial value of the hardening state variable ζ. Identiﬁcation of the parameters α, ϑ, W , and D was based on triaxial tests on gravel [14, 15, 18], where cylindrical specimens were subjected to hydrostatic compression up to diﬀerent conﬁning pressures p. While p was subsequently kept constant, the specimens were subjected to additional uniaxial loading in the direction of the cylinder axis, up to shear failure. The parameters α and ϑ (Table 1) were identiﬁed from the stress states at failure. W and D were identiﬁed such that measured relationships between the mean normal stress and the volumetric strain are well predicted for p ≤ 0.9 MPa, see (Table 1). The initial size and the shape of the cap were determined from constant volume tests, R = 4.4 and ζini = 0 kPa, see [8]. For numerical reasons, the material parameter referring to tensile failure of gravel, T , was set equal to a very small positive value (100 Pa). Since, in a ﬁrst approximation, material parameters of dense sand are comparable to the material parameters of the investigated type of gravel [20], no distinction between sand and gravel was made in the numerical simulation. Table 1. Material parameters of steel, gravel, sand, granite, and concrete Material parameters of steel: E = 210 GPa , ν = 0.3 , σy = 514 MPa Material parameters of sandy gravel (also valid for dense sand) K = 244 MPa , G = 72 MPa , α = 149 kPa , ϑ = 0.40 , W = 0.28 , D = 0.05 MPa−1 , R = 4.4 , ζini = 0 kPa , T = 0.1 kPa ≈ 0 Material parameters of granite: E = 50 GPa , ν = 0.17 Material parameters of concrete E = 26.2 GPa , ν = 0.3 , α = 21.74 MPa , ϑ = 0.099 , T = 0.1 kPa ≈ 0

1.2 Validation of the Developed Structural Model Real-scale Impact Experiment The assessment of the developed structural model is based on a real-scale impact experiment, which is independent from all experiments related to the development of the structural model. In an area of a quarry, used for disposal of wet clay, a 22 m long steel pipe was buried with sandy gravel as illustrated in Fig. 1. The height of the overburden H was equal to 2 m. A granite boulder

Protection Systems for Gravel-Buried Pipelines

193

of approximately cubic shape with a mass m = 18260 kg (V = 6.76 m3 , d = 1.99 m) was dropped from a height hf = 18.85 m (v0 = 19.23 m/s) onto the buried pipeline such that it impacted with a tip. The impact of the boulder caused a crater with a depth of X = 0.85 m. The cross-section of the pipe containing the impact axis was equipped with four strain gauge rosettes. The strain histories measured during the impact were converted into stress histories by means of ideal elasto-plasticity of von Mises type, see e. g. [10], assuming plane-stress conditions. The obtained maximum von Mises stresses at the locations of the strain gauge rosettes are listed in Table 2. Table 2. Von Mises stresses and second invariant of the strain tensor referring to the maximum loading of the pipe subjected to rockfall: experimental results, numerical results, and relative errors position

experimental result

FE result

relative error∗

exp FE 12h σvM = 514 MPa = σy σvM = 514 MPa = σy exp FE 3h σvM = 5386 MPa σvM = 357 MPa exp FE 6h σvM = 5204 MPa σvM = 305 MPa exp FE 12h J2,ε = −3.4761 · 10−6 J2,ε = −3.1754 · 10−6 exp exp exp exp ∗ FE FE evaluated as |σvM − σvM |/σvM and |J2,ε − J2,ε |/J2,ε ,

0.0 % 7.5 % 49.5 % 8.7 % respectively

Comparison between Model-predicted and Experimentally Determined Stress Distribution in the Steel Pipe The real-scale impact experiment was simulated by means of the developed 3D FE model. The maximum impact force and the penetration depth at maximum impact force were calculated from Eqs. (3) as F = 7.94 MN , and W = 0.72 m . The values for F and W served as input for modeling of the impact as described in Subsection 1.1. The coeﬃcient for the sub-grade reaction, ks , characterizing the elastic foundation of the trench, was set equal to 18 MN/m3 , which is the mean value of the interval [12 MN/m3 ; 24 MN/m3 ] recommended for soft clay in [6]. Finite elements with trilinear shape functions for the displacements were used. The nonlinear elasto-plastic FE simulation was performed in an incremental-iterative manner, based on consistent tangent moduli [5, 8, 9]. The computed stresses in the pipe were compared to the corresponding experimental results, see Table 2. For a graphical representation of the obtained von Mises stresses along the inner surface of the pipe, see the thick solid line in Fig. 4 (a). In general, the simulated behavior of the steel pipe reﬂects the experimentally observed behavior of the tube satisfactorily, both qualitatively and quantitatively. At the positions 12h and 3h, good agreement between the numerical predictions and the experimental results is observed. Since the steel

194

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang von Mises stress σvM [ MPa ]

500

σy

400

von Mises stress σvM [ MPa ] 12h

ks =

18 MN/m3 6h

500 s 3h

400

300

300

200

200

100 k = 100 MN/m3 s

100

0 12h

1h

2h

3h (a)

ks = 500 MN/m3 4h

5h

σy

6h s

0 12h

12h

H = 2.0 m

H = 3.0 m 1h

2h

3h (b)

4h

s 3h

6h

H = 2.5 m

5h

6h s

Fig. 4. Prognoses of the distribution of the von Mises stress along the inner surface of the pipe in the cross-section beneath the impact as a function of (a) the coeﬃcient of the sub-grade reaction and (b) the height of overburden

yielded at the top of the pipe, also strain measurements and FE-predictions are compared at the position 12h, based on the second invariant of the strain deviator, J2ε =

1 (εxx − εϑϑ )2 + (εϑϑ − εrr )2 + (εrr − εxx )2 + ε2xϑ + ε2ϑr + ε2rx . (7) 6

Also this comparison yields a discrepancy of less than 10 %, see Table 2. The largest relative error between the numerical simulation and the experiment is obtained at the position 6h. There, the numerically predicted loading of the pipe is 49.5 % greater than the experimentally obtained value. Nevertheless, in regions where the highest loading of the steel pipe occurs, the developed structural model yields satisfactory results. Consequently, this model possesses predictive capabilities, i. e., the model is successfully validated. 1.3 Prognoses of Structural Behavior Prognoses Considering a Change of the Boundary Conditions The trench in which pipelines in Alpine valleys are buried by gravel is usually surrounded by rock rather than by soft clay. This provides the motivation to study the inﬂuence of diﬀerent coeﬃcients of sub-grade reaction on the loading of the pipe. In order to model the behavior of weathered rock, ks is set equal to 100 MN/m3 , as recommended for dense sand in [6]. Secondly, ks is set equal to 500 MN/m3 in order to investigate an (almost) rigid bedding, as encountered with unweathered rock. In both cases, the height of the overburden and the intensity of the impact are the same as in the FE simulation described in Subsection 1.2. For increased values of the coeﬃcient of sub-grade reaction, the FE-predicted maximum von Mises stress of the pipe does not reach the

Protection Systems for Gravel-Buried Pipelines

195

yield stress, see Fig. 4 (a). An increase of ks from 18 MN/m3 to 100 MN/m3 and 500 MN/m3 results in a reduction of the loading of the pipe by approximately 25 % and 30 %, respectively. Prognoses Considering a Change of the Structural Dimensions In order to assess the capability of gravel layers to serve as a protection system for steel pipes endangered by rockfall, the inﬂuence of diﬀerent heights of overburden (H = 2.5 m and 3.0 m) on the loading of the pipe is studied. In these two simulations, the coeﬃcient of sub-grade reaction and the intensity of the impact are the same as in the FE simulation which allowed for validation of the model, see the Subsection 1.2. For increased heights of the overburden, the maximum von Mises stress of the pipe, predicted by the FE simulation, does not reach the yield stress, see Fig. 4 (b). An increase of H from 2.0 m to 2.5 m and 3.5 m results in a reduction of the loading by approximately 20 % and 30 %, respectively. However, this decrease is less than linear. Therefore, in order to eﬀectively increase the safety of a gravel-buried pipeline subjected to rockfall, the burying depth must be increased signiﬁcantly. Prognoses Considering a Change of the Boundary Conditions and of the Structural Dimensions In the two previous parameter studies the inﬂuence of the increasing height of the overburden and the one of the increasing coeﬃcient of sub-grade reaction on the loading of the pipe were investigated separately. In order to investigate the synergism of both modiﬁcations, H and ks are increased simultaneously in an additional numerical analysis. The height of overburden is set equal to 3 m and the coeﬃcient of sub-grade reaction equal to 500 MN/m3 , whereas the intensity of the impact remains unchanged. Results from this FE analysis show a further reduction of the loading of the pipe (compare the thick line in Fig. 6 with the results illustrated in Figs. 4 (a) and (b)). The maximum von Mises stress encountered along the inner surface of the pipe is equal to 33.5 % of the yield stress. 1.4 Assessment of an Enhanced Protection System Consisting of Gravel and, Additionally, of Buried Load-Carrying Structural Elements A protection system for a steel pipe subjected to rockfall must satisfy two requirements: (i) damping of the impact, in order to keep the forces arising from rockfall reasonably small and (ii) load distribution and load-carrying capacity, in order to reduce the loading of the steel pipe. As for the protection system investigated so far, both tasks are accomplished by the layer of gravel. However, the ﬂexibility of gravel required for the damping of the impact is opposed to the stiﬀness of the material required for distribution and carrying of the load.

196

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

B

A

surface of structure gravel Section A–A steel plate t=1.5 cm concrete wall 200 cm

surface of structure gravel Section B–B steel plate t=1.5 cm concrete wall 200 cm

sand 17 cm 100 cm soil/rock B

sand soil/rock

132 cm A

Fig. 5. Alternative protection system consisting of gravel as an energy-absorbing and impact-damping system and a buried steel plate supported by concrete walls as a load-carrying structural component

In order to further improve the eﬀectiveness of a protection system for a steel pipe subjected to rockfall, the aforementioned two tasks should be performed by two separate structural elements. Such an enhanced protection system is investigated subsequently. Buried Steel Plate Resting on Concrete Walls The investigated protection system consists of (i) gravel as an energy-absorbing and impact-damping system and (ii) a buried steel plate supported by concrete walls, representing a load-carrying structural component, as illustrated in Figs. 5 (a) and (b). Length, width, and thickness of the steel plate are equal to 264 cm, 234 cm, and 1.5 cm, respectively. It consists of the same steel as used for the pipe (Table 1). The boundary conditions at the interface between the steel plate and the concrete walls are chosen such that only compressive forces can be transmitted to the concrete walls. For the description of the material behavior of concrete, the Cap Model is employed, with the ellipsoidal failure surface being removed. The considered type of concrete is characterized by the uniaxial compressive strength fcu = −30.3 MPa (σ11 = fcu , σ22 = σ33 = σ12 = σ23 = σ31 = 0) and the biaxial compressive strength fcb = −35.15 MPa (σ11 = σ22 = fcb , σ33 = σ12 = σ23 = σ31 = 0). These two strength values are the basis for calculating the material parameters α and ϑ of the Drucker-Prager failure criterion

2 fcu −fcb 2 fcu fcb = 0.099 , α = = 21.74 MPa . (8) ϑ= 3 fcu −2 fcb 3 fcu −2 fcb

Protection Systems for Gravel-Buried Pipelines

197

von-Mises stress σvM [ MPa ]

200

without steel plate and concrete wall 160

12h

s 3h

6h

120 80

reduction of pipe loading

40

with steel plate and concrete wall 0 12h 1h 2h 3h 4h 5h 6h s

Fig. 6. Prognoses of the distribution of the von Mises stress along the inner surface of the pipe in the cross-section beneath the impact for a height of overburden H = 3 m and a coeﬃcient of sub-grade reaction ks = 500 MN/m3 with and without the additional construction consisting of a steel plate and concrete walls

Young’s modulus E, Poisson’s ratio ν and the parameter T referring to the tension cut-oﬀ are listed in Table 1. Assessment of the Enhanced Protection System The performance of the enhanced protection system is assessed considering the same rockfall scenario as previously investigated, i.e., the mass and the height of fall of the boulder are equal to 18260 kg and 18.85 m, respectively, the coeﬃcient of sub-grade reaction is set equal to 500 MN/m3 , the height of overburden equal to 3 m, and F and W again equal to 7.94 MN and 0.72 m, respectively. Results from the FE analysis show that the additional structural elements result in a further signiﬁcant reduction of the loading of the pipe, see Fig. 6. 1.5 Conclusions It was shown that a protection system for a steel pipe subjected to rockfall must satisfy two requirements: (i) damping of the impact, in order to keep the forces arising from rockfall reasonably small and (ii) load distribution and load-carrying capacity, in order to reduce the loading of the steel pipe. In case of a purely gravel-based protection system, both tasks must be performed by gravel. Thereby, the ﬂexibility of gravel required for the damping of the impact is opposed to the stiﬀness of the material required for the task of load distribution and carrying of the load. This was the motivation to investigate an enhanced protection system consisting of (i) gravel as an energy-absorbing and impact-damping system

198

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

and (ii) a buried steel plate supported by concrete walls as a load-carrying structural component. This analysis showed that buried load-carrying structural elements can signiﬁcantly increase the safety of pipelines endangered by rockfall.

2 Protection Systems Against Abrasive Shear Loading Caused by Thermal Deformation of Soil-Covered Pipelines Oil and gas pipelines are commonly bedded in and covered with sand. The transport of sand to the construction site may be expensive. Therefore, the replacement of sand by a (coarse) ﬁlling material which is directly available at the construction site (e.g. possibly sharp-edged stones with dimensions up to ≈ 10 × 10 × 10 cm) could prove proﬁtable. However, such a construction method would result in larger contact forces exerted from relatively large, sharp-edged stones onto the pipelines. This is particularly disadvantageous in combination with motions of the pipeline relative to the backﬁll material, resulting from temperature-induced displacements of the pipeline in longitudinal direction: Recurrent abrasive shear loading by tips of stones may damage the anti-corrosion ﬁlm at the outer surface of the pipeline. This section deals with the protection of the anti-corrosion ﬁlm against such shear forces, discussing the role of geosynthetics and steel-ﬁbre reinforced concrete. 2.1 Assessment of Static Forces Exerted by Single Stone Tips onto Soil-Covered Pipelines Loading Scenario The magnitude of forces acting onto soil-covered pipelines depends on the height of the cover, on the mechanical properties and the speciﬁc weight of the ﬁlling material, and on the settlements of the pipeline and the ﬁlling material. If no settlements occur, the force acting onto the pipeline is equal to the weight of the ﬁlling material directly above the pipeline. If, however, the settlements of the ﬁlling material beside the pipeline are greater than the ones of the pipeline, the forces acting onto the pipeline increase because of signiﬁcant load re-arrangement processes in the soil [21]. The extent of this re-arrangement depends on the shear resistance of the ﬁlling material. It increases with decreasing shear resistance. Structural Model The relevant force acting on a soil-covered pipeline follows from the combination of a ﬁlling material of low shear resistance, piled up to a standard maximum cover height of 1.5 m, with an adverse settlement scenario. We consider

Protection Systems for Gravel-Buried Pipelines

199

Fig. 7. Structural model of the soil body above and lateral of the pipeline

uniform settlements of the ﬁlling material on both sides of a ﬁxed pipeline. Consequently, no longitudinal displacements occur and displacements in a plane orthogonal to the pipe axis do not change along the longitudinal direction. This corresponds to a plane state of strain, and allows for the use of a plane structural model [12] (see Fig. 7). Steel pipes for oil and gas pipelines are so stiﬀ that the displacements resulting from a soil cover of 1.5 m height are negligibly small as compared to typical soil settlements of several centimeters. Hence, the pipe does not have to be considered explicitly in the structural model. Instead, the contact surface between the pipe and the ﬁlling material is spatially ﬁxed in the structural model. Since both the structure and the settlements are symmetric, investigation of half the structure is suﬃcient. Thereby, the axis of symmetry (left boundary in Fig. 7) and the boundary opposite to the axis of symmetry (right boundary in Fig. 7) are ﬁxed in the x-direction. The upper boundary, corresponding to the ground surface, is stress-free. At the lower boundary, settlements, i.e. displacements in the y-direction, are prescribed (see Fig. 7). The boundary opposite to the axis of symmetry is suﬃciently far from this axis so to exert no inﬂuence on the stress state around the pipe. Determination of this stress state requires a realistic consideration of the nonlinear material behavior of the ﬁlling material. Therefore, the Cap Model described in Subsection 1.1 is adopted. Aiming at determination of the relevant forces that are acting on a soil-covered pipeline embedded in a material with low shear resistance, the subsequent calculations are based on a cohesionless material, i.e. we use the parameters of sandy gravel listed in Table 1, setting, however, α equal to 0.5 kPa.

200

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Finite Element Simulation The structural problem, involving elasto-plastic material behavior, is solved numerically for three standard diameters of oil or gas pipelines (d = 500, 1000 and 1500 mm), by means of nonlinear FE simulations [21], which are performed in an incremental-iterative manner, based on consistent tangent moduli [5, 8, 9]. For determination of forces exerted by single stone tips onto a pipeline, the distribution of the radial stresses along the pipeline perimeter must be computed. Prior to settlements on both sides of the pipeline, radial compression stresses amount to 25 kPa – 35 kPa, depending on the pipeline diameter [see Fig. 8(a)–(c)]. After completion of the re-arrangement of the loading, caused by the settlements, release occurs in the vicinity of the vertex of the pipeline. In the lateral regions of the upper half of the pipeline the radial stresses are increasing signiﬁcantly (see Figs. 8). The increase of the maximum load is the larger, the smaller the pipeline diameter [see Fig. 8(d)]. Relevant Forces of Tips of Single Stone Acting on Soil-covered Pipelines, as a Function of the Pipe Diameter These forces can be determined through integration of the maximum radial stresses over parts of the surface associated with a characteristic distribution of stone tips. For the sake of simplicity, a quadratic grid of stone tips with distances a is assumed (see Fig. 9). Thus, forces exerted by one stone tip read as ⎧ ⎨ −106 kPa for d = 500 mm, −69 kPa for d = 1000 mm, (9) F = a2 · max σrr,∆s with max σrr,∆s = ⎩ −63.4 kPa for d = 1500 mm. Assuming a uniformly granulated ﬁlling material, the stone tip distance a can be set equal to the grain size of the ﬁlling material. Thus, following from Eq. (91 ), the force exerted by one tip of a stone for a given pipeline diameter is a quadratic function of the grain size of the ﬁlling material (see Fig. 10). 2.2 Identiﬁcation of Wear Protection Strategies Archard’s Wear Law Using Archard’s wear law [2], the maximum contact forces determined in Subsection 2.1 allow for calculation of the service life of the protection layer serving as an envelope of the pipe. In order to carry out this calculation, the wear resistance must be determined experimentally (see Fig. 11). Archard’s wear law reads as [2] Fv . (10) V˙ = KA H

Protection Systems for Gravel-Buried Pipelines

201

Fig. 8. Distribution of radial stresses resulting from the dead load of the ﬁlling material (speciﬁc weight γ of covering soil 20.0 kN/m3 and cover height 1.5 m) along the perimeter of a soil-covered pipeline before (◦, σrr,DL ) and after (, σrr,∆s ) settlement-induced load re-arrangement for (a) d = 500 mm, (b) d = 1000 mm, and (c) d = 1500 mm; and (d) settlement-induced increase of maximum radial stresses in the pipe

Fig. 9. Deﬁnition of distance a between stone tips and stress integration area A of a single stone tip: stone tips exert contact force F in a regular grid (a × a) on the pipeline surface

202

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Fig. 10. Relevant forces of single stone tips as function of the distance between stone tips, and of pipeline diameter (speciﬁc weight γ of covering soil 20.0 kN/m3 , cover height 1.5 m)

Fig. 11. Deﬁnition of the term ’shear cycle’ in context with wear tests conducted on specimens representing the protection layer of the outer anti-corrosion layer of soil-covered steel pipelines: per shear cycle, twice the shear distance, 2l, is covered

In Eq. (10), V˙ is the abrasion rate (abrased volume per time), F is the compressive force, v denotes the velocity of the abrasion-inducing body, H represents the hardness of the loaded body, and KA is a dimensionless parameter, related to the probability of (microscopic) abrasion phenomena depending on characteristics of the abrased and the abrasive body (e.g. mineralogical hardness, viscosity, stiﬀness) [11, 13].

Protection Systems for Gravel-Buried Pipelines

203

Since time-dependent eﬀects play no role in the considered wear tests, the integration of Eq. (10) is trivial, V = KA

Fs , H

(11)

where V is the abrased volume along the total shear path length s. V can be expressed as the product of the tip width w of the abrasion-inducing body, the shear distance l, and the cutting depth t. The total shear path length can be expressed as the product of the shear cycle number n and twice the shear distance covered during one shear cycle, 2l (see Fig. 11), s = n · 2l. Thus, following from Eq. (11), w · l · t = KA

F · n · 2l H

⇒

t=

2KA · F · n. wH

(12)

According to Eq. (12), the cutting depth t depends on the compressive force F , on the number of conducted shear cycles n, on KA , on the metal tip width w, and on the hardness H of the specimen. Notably, the shear distance l has no inﬂuence on the cutting depth. Protection Performance of Geosynthetics The wear resistance of common geosynthetics was determined by means of shear tests (see Fig. 11) on 6 mm thick geosynthetic specimens of the type Polyfelt AR 20 [4] (a = 21 cm, b = 14.85 cm). For this purpose, a metal tip was used, similar to the cone-shaped tip described in [1]. It was attached to the geosynthetic specimen, loaded by a compressive force of approximately 50 N, acting perpendicular to the specimen. In two independent tests the specimens were completely transected after ≈ 50 shear cycles. Evaluation of Eq. (12) for the tests (t = 6 mm; n = 50; F = 50 N) yields (2KA )/(wH) = 2.4 · 10−6 m/N. This value, together with Eq. (12), allows for estimation of the cutting depth t into a geosynthetic specimen of the aforementioned type, as a function of the compressive force F and the shear cycle number n. The order of magnitude of the shear cycle number which leads to a transection of a geosynthetic of 6 mm thickness can be assessed through insertion of t = 6 mm, (2KA )/(wH) = 2.4 · 10−6 m/N, and Eq. (9) into Eq. (12), ⎧ ⎨ 60/90/100 for a = 2 cm , 7/10/11 for a = 6 cm , nd=500/1000/1500 mm = (13) ⎩ 2/4/4 for a = 10 cm . For common pipe diameters (500 – 1500 mm) and grain sizes (distance between stone tips) of 2 – 10 cm, the 6 mm geosynthetic investigated herein resists 2 – 100 shear cycles, until being completely transected.

204

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Given a typical service life of n = 5000 shear cycles for oil and gas pipelines, the above results [see Eq. (13)] reveal that a 6 mm geosynthetic of the considered type protects the outer anti-corrosion ﬁlm of the pipeline for only ≈ 1/2500 to 1/50 of the service life. The stone tip force which results in transection of the 6 mm geosynthetic of the type Polyfelt AR 20 after 5000 shear cycles can be assessed through insertion of t = 6 mm, (2KA )/(wH) = 2.4 · 10−6 m/N, and n = 5000 into Eq. (12). This force amounts to olyf elt = 6 mm) = 0.5 N . F (n = 5000, tP AR 20

(14)

The maximum admissible distance a between stone tips exerting a force of F = 0.5 N, can be determined by means of Eqs. (9) as a function of the outer pipe diameter, ⎧ ⎨ 2.2 mm for d = 500 mm , a = 2.7 mm for d = 1000 mm , (15) ⎩ 2.8 mm for d = 1500 mm . Hence, when covered by sand grains, the 6 mm geosynthetic investigated herein resists 5000 shear cycles before being transected. Eﬀective Means of Protection The results of the previous paragraph suggest two strategies for providing a suﬃcient protection of the outer anti-corrosion ﬁlm of soil-covered pipelines for oil and gas transport against abrasive shear loading exerted by coarse ﬁlling material, caused by temperature-induced displacements of the pipeline in the longitudinal direction: (a) Increase of the hardness H and the thickness t, respectively, of the protective layer subjected to wear: e.g. by coating the pipeline by steel-ﬁbre reinforced concrete (SFRC) [see Fig. 12(a)]. (b) Decrease of the abrasion force by reducing the distance a between the stone tips, as the pipeline is embedded in and buried by sand. Thereby, leaching of sand can be avoided by enveloping the sand body with a ﬁltration layer which separates the sand body and the coarse ﬁlling material from each other. Preferably, geosynthetics are attached as ﬁltration layer [see Fig. 12(b)].

2.3 Conclusions The resistivity of geosynthetics of a type similar to ones tested herein against abrasion through sharp-edged stones larger than 2 mm, is too low as to provide, during the entire service life, suﬃcient protection of the outer anticorrosion ﬁlm of the pipeline. Hence, sand cannot be replaced by coarser

Protection Systems for Gravel-Buried Pipelines

205

Fig. 12. Strategies for protecting the outer anti-corrosion ﬁlm of soil-covered steel pipelines in case a mixture of sandy gravel and square-edged stones is used as ﬁlling material: (a) increase of hardness and thickness of the protective layer, e.g. made of steel-ﬁbre reinforced concrete (SFRC) or (b) decrease of the abrasion force through use of sandy material around the pipe

ﬁlling material together with an envelope of the steel pipe by geosynthetics comparable to ones investigated herein. However, when subjected to shear loading exerted by sand grains, failure (transection) of Polyfelt AR 20 -type geosynthetics can indeed be excluded prior to 5000 shear cycles, i.e. within the entire service life of such a pipe. Hence, two strategies can be recommended for protecting the outer anti-corrosion ﬁlm of soil-covered steel pipelines against abrasive shear loading: On the one hand, the wear resistance of the protection layer can be improved by increasing its hardness and thickness, e.g. through the use of steel-ﬁbre reinforced concrete. On the other hand, encasing the pipeline with sand minimizes the abrasion force, which can be withstood by the outer anti-corrosion ﬁlm of the pipeline without any additional means of protection. Leaching of sand can be avoided by an envelope of the sand body by geosynthetics.

References ¨ 1. ONORM EN 14574 (2005) Geokunststoﬀe – Bestimmung des Pyramidendurchdr¨ uckwiderstandes von Geokunststoﬀen auf harter Unterlage [Geosynthetics – Determination of the Pyramid Puncture Resistance of Geosynthetics on ¨ Hard Underlay]. Osterreichisches Normungsinstitut In German. 2. Archard JF (1953) Contact and rubbing of ﬂat surfaces. Journal of Applied Physics 24(8):981–988 3. DiMaggio FL, Sandler IS (1971) Material models for granular soils. Journal of Engineering Mechanics (ASCE) 97(3):935–950 4. Polyfelt Geosynthetics (2006) Technical data polyfelt.AR – 500 917 | 02.2002. www.polyfelt.com. 5. Hofstetter G, Simo JC, Taylor RL (1993) A modiﬁed cap model: closest point solution algorithms. Computers & Structures 46(2):203–214 6. JDAAF (1983) Soils and Geology Procedures for Foundation Design of Buildings and Other Structures (Except Hydraulic Structures): Technical Manual 5-818-

206

7. 8.

9. 10. 11. 12. 13. 14. 15. 16.

17.

18.

19.

20. 21.

22.

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang 1, Air Force Manual 88-3. Joint Departments of the Army and the Air Force, Washington, DC, USA Koiter WT (1960) General theorems for elastic-plastic solids, volume I, Chapter IV, pp 167–218. North-Holland Publishing Company, Amsterdam Kropik Ch (1994) Three-dimensional elasto-viscoplastic ﬁnite element analysis of deformations and stresses resulting from the excavation of shallow tunnels. PhD thesis, Vienna University of Technology, Vienna, Austria Kropik Ch, Mang HA (1996) Computational mechanics of the excavation of tunnels. Engineering Computations 13(7):49–69 Lubliner J (1990) Plasticity Theory. Macmillan Publishing Company, New York Magne´e A (1993) Modelization of damage by abrasion. Wear 162–164:848–855 Mang H, Hofstetter G (2000) Festigkeitslehre [Strength of Materials]. Springer, Wien, NewYork. In German Olofsson U, Telliskivi T (2003) Wear, plastic deformation and friction of two rail steels – a full scale test and a laboratory study. Wear 254:80–93 Penumadu D, Zhao R (1999) Triaxial compression behavior of sand and gravel using artiﬁcial neural networks (ANN). Computers & Geotechnics 24:207–230 Pichler B (2003) Parameter identiﬁcation as the basis for prognoses in geotechnical engineering. PhD thesis, Vienna University of Technology, Vienna, Austria Pichler B, Hellmich Ch, Mang HA (2005) Impact of rocks onto gravel - design and evaluation of experiments. International Journal of Impact Engineering 31:559–578. Available online at www.sciencedirect.com. Pichler B, Hellmich Ch, Mang HA, Eberhardsteiner J (2005) Assessment of protection systems for buried steel pipelines endangered by rockfall. ComputerAided Civil and Infrastructure Engineering 20:331–342 Pichler B, Hellmich Ch, Mang HA, Eberhardsteiner J (2006) Gravel-buried steel pipe subjected to rockfall: Development and veriﬁcation of a structural model. Journal of Geotechnical and Geoenvironmental Engineering (ASCE) 132(11):1465–1473 Sandler IS, Rubin D (1979) An algorithm and a modular subroutine for the cap model. International Journal for Numerical and Analytical Methods in Geomechanics 3:173–186 ´ Sawicki A, Swidzi´ nski W (1998) Elastic moduli of non-cohesive particulate materials. Powder Technology 96:24–32 Scheiner St, Pichler B, Hellmich Ch, Eberhardsteiner J (2006) Loading of soil-covered oil and gas pipelines due to adverse soil settlements – protection against thermal dilatation-induced wear, involving geosynthetics. Computers and Geotechnics 33(8):371–380 Simo JC, Taylor RL (1985) Consistent tangent operators for rate independent elasto–plasticity. Computer Methods in Applied Mechanics and Engineering 48:101–118

Enriched Free Mesh Method: An Accuracy Improvement for Node-based FEM Genki Yagawa1 and Hitoshi Matsubara2 1

2

Center for Computational Mechanics Research, Toyo University, 2-36-5, Hakusan, Bunkyo-ku, Tokyo, Japan, 112-8611 [email protected] Center for Computational Science and Engineering, Japan Atomic Energy Agency, 6-9-3 Higashi-Ueno, Taito-ku, Tokyo, Japan, 110-0015 [email protected]

Summary. In the present paper, we discuss the accuracy improvement for the free mesh method: a node based ﬁnite element technique. We propose here a scheme where the strain ﬁeld is deﬁned over clustered local elements in addition to the standard ﬁnite element displacement ﬁeld. In order to determine the unknown parameter, the least square method or the Hellinger-Reissner Principle is employed. Through some bench mark examples, the proposed technique has shown excellent performances.

1 Introduction Recent advances in computer technology have enabled a number of complicated natural phenomena to be accurately simulated, which were ever only observed by experiments. Among various computer simulation techniques, the ﬁnite element method (hereinafter referred to as ”FEM”) has been most widely used due to the capability of analyzing an arbitrary domain, and results, accurate enough for engineering purposes, are obtainable at reasonable cost[1][2]. However, mesh generation for ﬁnite element analysis becomes very diﬃcult and time consuming if the degree of freedom of the analysis model is extremely large, for example exceeding 100-million, and the geometries of the model are complex. In order to overcome the above shortcoming of the standard FEM, the so called mesh-free methods[3][4] have been studied. The Element-Free Galerkin Method (EFGM)[5][6] is among them with the use of integration by background-cells instead of by elements, based on the moving least square and diﬀuses element methods. The Reproducing Kernel Particle Method (RKPM)[7][8] is another mesh-free scheme, which is based on a particle method and wavelets. The general feature of these mesh-free methods is that, contrary to the standard FEM, the connectivity information between Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 207–219. © 2007 Springer. Printed in the Netherlands.

208

Genki Yagawa and Hitoshi Matsubara

nodes and elements is not required explicitly, since the evaluation of the total stiﬀness matrix is performed generally by the node-wise calculations instead of the element-wise calculations. On the other hand, a virtually mesh-free approach called the free mesh method (hereinafter referred to as ”FMM”)[9][10] is based on the usual FEM, having a cluster of local meshes and equations constructed in a node-by-node manner. In other word, the FMM is a node-based FEM, which still keeps the well-known excellent features of the standard FEM. Through the nodewise manner of the FMM, a seamless ﬂow in simulation procedures from local mesh generation to visualization of the results without user’s consciousness is realized. The method has been applied to solid/ﬂuid dynamics [11], crack problems[12], concrete problems[13], and so on. In addition, in order to achieve a high accuracy, the FMM with vertex rotations has been studied[14][15]. In this paper, we discuss another high accurate FMM: the Enriched FMM (hereinafter referred to as ”EFMM”). In the following section, the fundamental concept of the original FMM is reviewed, and the third section deals with two EFMMs, one is ”EFMM based on the localized least square method” and the other ”EFMM based on the Hellinger-Reissner principle”. In the fourth section, some numerical examples are presented, and concluding remarks are given in the ﬁnal section.

2 Basic Concept of Free Mesh Method (FMM) The FMM starts with only the nodes distributed in the analysis domain (Ω), without the global mesh data, as following equation. pi (xi , yi , ri ) ∀i ∈ {1, 2, · · · , m}

(1)

where m is the number of node, pi (xi , yi ) are the Cartesian coordinates, and ri is the nodal density information, which is used to generate appropriate nodes as illustrated in Fig. 1(a). From above nodal information, a node is selected as a central node and nodes within a certain distance from the central node are selected as candidate nodes. This distance is usually decided from the prescribed density of the distribution of nodes. Then, satellite nodes are selected from the candidate nodes, which generate the local elements around the central node (shown in Fig. 1(b)). For each local element, the element stiﬀness matrix is constructed in the same way as the FEM, however in FMM, only the row vector of stiﬀness matrix for each local element is necessary. The local stiﬀness matrix of each temporary element is given by kei = [ kpi kSj kSk ]

(2)

where kei is the row vector of the stiﬀness matrix for element ei and kpi , kSi and kSk are components for node of pi , Si and Sk (j and k are number

Enriched Free Mesh Method S3 e3

S4

e2

e4

Other nodes S2

Central node

e1

pi e6 e

S5

5

Local elements S1

S6

(a) Domain of analysis

pi S1

pi S1 S2

pi

…

S2

209

Satellite nodes

(b) Clustered local elements

pi S6 S1 Assembling

S6

pi S1 S2 S3 S4 S5 S6

S1

Stiffness matrix for e1

Stiffness matrix for e2

Stiffness matrix for Pi

(c) Stiﬀness matrix for central node Fig. 1. Concept of Free Mesh Method

of current satellite nodes). Through the above procedures are carried out for all local elements, the stiﬀness matrix for a central node is given by kpi =

ne

k ei

(3)

i=1

where kpi is the stiﬀness matrix for central node pi , and ne the number of local elements. Through the above procedures for all nodes is carried out, the global stiﬀness matrix is given by assembling kpi which are computed by node-wise manner: ⎡ ⎤ kp1 ⎢ kp2 ⎥ ⎢ ⎥ K=⎢ . ⎥ (4) ⎣ .. ⎦ kpm Brief of the nodal stiﬀness matrix is shown in Fig. 1(c). After the construction of the global stiﬀness matrix, a derivation of the solution is processed. The great advantage of the FMM is that the global stiﬀness matrix can be evaluated in parallel with respect to each node through the node-wise manner, and only satellite node information is required with each nodal calculation. Finally, a derivation of the solution is performed as the usual FEM. Thus, the FMM is a node-wise FEM, which still keeps the well-known excellent features of the usual FEM. The features of FMM are summarized as follows, (1) Easy to generate a large-scale mesh automatically (2) Processed without being conscious of mesh generation (3) The result being equivalent to that of the FEM

210

Genki Yagawa and Hitoshi Matsubara

Mixed

Element-wise displacement fields

Node-wise strain field

Fig. 2. Concept of enriched free mesh method

3 Enriched Free Mesh Method (EFMM) 3.1 Outline of EFMM ”Assumed strain on the clustered local elements” is the concept of EFMM as shown in Fig. 2. In the EFMM, the strain ﬁeld on the clustered local elements and the displacement ﬁeld of each local element are assumed independently. Relating these independent ﬁelds, we propose here two approaches, one is the localized least square method and the other is the method based on the Hellinger-Reissner principle. 3.2 EFMM Based on the Localized Least Square Method The EFMM based on the localized least square method (hereinafter referred to as ”EFMM-LS”) assumes the strain ﬁeld on the clustered local elements as {ε(x)} = [Nε ]{a}

(5)

where {ε(x)} = {εxx , εyy , γxy } is the strain ﬁeld deﬁned on the clustered local elements and each component of {εxx , εyy , γxy } is assumed independently, and [Nε ] is a matrix, which consists of arbitrary polynomials as follows, ⎤ ⎡ t p (x) 0 0 (6) [Nε ] = ⎣ 0 pt (x) 0 ⎦ 0 0 pt (x) where pt (x) is given on the clustered local elements as linear basis pt (x) = 1 x y quadratic basis pt (x) = 1 x y x2 xy y 2 pt (x) = 1 x y x2 xy y 2 x3 x2 y xy 2 y 3 cubic basis ···

(7)

Enriched Free Mesh Method

211

In this paper, pt (x) is assumed to be linear or quadratic basis polynomial. The coeﬃcients vector {a} in Eq. (5) is determined by minimizing the discrete L2 norm as follows, p ne 2 [{ε(x)} − {εci }] (8) J= c=1 i=1

where ne is the number of local elements with c(= 1, 2, · · · , ne ) being current local element, p the number of points, which are called as the ”strain monitoring points” on the clustered local elements with i(= 1, 2, · · · , p) being the current strain monitoring point and {εci }the strain vector of i-th strain monitoring point on the c-th local element, which is called as the ”mother element”. The stationary condition of Eq. (8) is δJ = 2{a}T

p ne εT ε [Ni ] [Ni ]{a} − [Nεi ]T {εci } = 0

(9)

c=1 i=1

which yields the coeﬃcients vector {a} as follows, {a} =

p ne

T [Nεi ]

−1

[Nεi ]

T [Nεi ]

{εci }

(10)

c=1 i=1

Let us consider a simple Constant Strain Triangle as the mother element in which the displacement ﬁeld of each local element is deﬁned by {u} =

3

{ui }ζi

(11)

i=1

where {u} is the displacement ﬁeld of the local element, {ui } is the nodal displacement, and ζi is the area-coordinate[16]. Thus, the strain value on the strain monitoring points is given by {εci } = [Bci ]{ui } where

[Bci ] = [B1 ] [B2 ] [B3 ] with ⎡ ⎤ ∂ζj /∂x 0 ∂ζj /∂y ⎦ [Bj ] = ⎣ 0 ∂ζj /∂y ∂ζj /∂x

(12)

(13) , j = 1, 2, 3

By substituting Eq. (12) into Eq. (10), the unknown coeﬃcient {a} is determined as

p ne −1 T T [Nεi ] [Nεi ] [Nεi ] [Bci ] {ui } (14) {a} = c=1 i=1

212

Genki Yagawa and Hitoshi Matsubara

Substituting Eq. (14) into Eq. (15), we obtain {ε(x)} = [Nε ]

p ne ε T ε −1 ε T c [[Ni ] [Ni ]] [Ni ] [Bi ]{ui } = [A]{ui }

(15)

e=1 i=1

where [A] = [Nε ]

p ne

[[Nεi ]T [Nεi ]]−1 [Nεi ]T [Bci ]

(16)

e=1 i=1

In the elasticity problem, the stress vector {σ} and the strain vector {ε} have the relation as follows, {σ} = [D]{ε}

(17)

where [D] is a symmetric matrix of material stiﬀness. With [D] given by Eq. (16), the stiﬀness matrix based on the localized least square method is computed on the clustered local elements as [A]T [D][A]dΩ (18) [kLS ] = Ω

where Ω is area of the clustered local elements. It is important to say that the above stiﬀness matrix is computed in a node-wise manner. It is noted that the present EFMM-LS is closely related to the superconvergent patch recovery proposed by Zienkiewicz and Zhu[17][18]. In an adaptive ﬁnite element method[19][20], the Z-Z error estimator has been most widely used to estimate the error. The error estimator requires an exact solution, but generally it is impossible to compute the exact value because the exact solution is not available in general. The Z-Z technique then obtains the recovered solution in a post processing stage. The clustered local elements in the present method are equivalent to the superconvergent patch used in the Z-Z technique. The diﬀerence lies in that the recovering procedure in the EFMM-LS is in a main process stage when computing element stiﬀness matrices. The use of the assumed strain is therefore, in some sense, equivalent to the ”post-process” of the Z-Z superconvergent patch recovery. 3.3 EFMM Based on Hellinger-Reissner Principle In the EFMM based on the Hellinger-Reissner principle [1][21] (hereinafter referred to as ”EFMM-HR”), the Hellinger-Reissner (hereinafter referred to as ”HR”) principle is employed to obtain better accuracy. Let the HR principle of a linear elastic body be deﬁned on the clustered local elements by 1 {ε}T [D]{∂u}dΩ − {ε}T [D]{ε}dΩ (ε, u) = 2 Ω Ω T − {u} {b}dΩ − {u}T {˜ t}dS (19) Ω

Sσ

Enriched Free Mesh Method

where

ε} {∂u} = [B]{¯ u} , {ε} = [Nε ]{¯

213

(20)

with {b} being the applied body force per unit mass, and {t˜} the applied traction on boundary Sσ . {¯ u} is the unknown nodal displacement and {¯ ε} the unknown nodal strain. The unknown values (¯ u, ε¯) of the HR principle satisfy the following equations in a weak manner, δ{ε}T [D] ([B]{¯ u} − [N]{¯ ε}) dΩ = 0 (21) Ω

Ω

δ{u} [B] [D][N]{¯ u}dΩ − T

T

δ{u} {b}dΩ − T

Ω

Sσ

δ{u}T {˜ t}dS = 0 (22)

It is noted here that the strain ﬁeld is deﬁned on the clustered local elements by node-wise manner, where the displacement ﬁeld is deﬁned on each element by element-wise manner. Equations (21) and (22) yields the following linear matrix equation,

ε¯ f1 −A C = (23) u ¯ f2 CT 0 where

⎧ A = Ω [Nε ]T [D][Nε ]dΩ ⎪ ⎪ ⎨ C = Ω [Nε ]T [D][B]dΩ f1 = 0 ⎪ ⎪ ⎩ f2 = Ω [Nu ]T {b}dΩ + Γ [Nu ]T {t˜}dΓ

(24)

By condensing the coeﬃcient matrix of Eq. (23), we obtain the following equation, u = f2 (25) CT A−1 C¯ where the condensation should be executed on the clustered local elements. Thus, the stiﬀness matrix based on the HR principle is computed on the clustered local elements as follows, [kHR ] = CT A−1 C

(26)

It is noted here that we can obtain the enriched stiﬀness matrix without increasing the number of nodal degrees of freedom.

4 Examples 4.1 Convergence Study: Displacement To study the convergence characters of the present methods, a cantilever model is solved as shown Fig. 3, where the three diﬀerent mesh patterns are prepared and the mesh division in the x direction is varied. As shown in the ﬁgure, a beam of length L = 10, height D = 1 and thickness t = 1

214

Genki Yagawa and Hitoshi Matsubara y

D=1

P

E = 1000, v = 0.25

x

L = 10

(a) Cantilever beam model

(b) One layer mesh

(c) Two layers mesh

(d) Three layers mesh Fig. 3. Mesh patterns for cantilever beam model

is subjected to a shear load in plane stress condition. The material parameters are given as the Young’s modulus E = 1000.0 and the Poisson’s ratio ν = 0.25. The displacements at the loaded edge normalized by the exact value are plotted against the degrees of freedom (see Fig. 4). From the comparison of displacement results among the six diﬀerent solutions, it can be observed that (a) The accuracy of the FEM with the three noded linear element of constant strain is the worst, whereas that with the six noded quadratic element is the best irrespective of the mesh patterns. (b) As the number of layers in the thickness direction increase, the accuracy of EFMMs approaches that of the quadratic FEM. (c) Regarding the comparisons among the EFMMs, the accuracy of the EFMM-HR and the EFMM-LS with the linear strain ﬁeld are the best, whereas, for the ﬁner meshes (see Fig. 4(c)), the results of EFMMs with the quadratic strain ﬁeld are almost equivalent to those of the formers. 4.2 Convergence Study: Error Norms As another convergence measures, two kinds of error norms for the beam problems as shown Fig. 5 [22] are employed, which are, respectively, given as

E2 =

Ω

exact T

u−u

exact

u−u

1/2 dΩ

(27)

Enriched Free Mesh Method

215

0.8 1

0.75 0.7 Displacement

Displacement

0.8 0.6 0.4

0.65 0.6 0.55 0.5

0.2

0.45 0

0.4 0

25

50

75

100 125 150 175 200

0

25

50

75

DOFs

100 125 150 175 200 DOFs

(a) One layer mesh 1

0.8

Displacement

Displacement

1

0.6 0.4

0.95

0.9

0.85

0.2 0

0.8

0

50

100

150

200

250

300

0

50

DOFs

100

150

200

250

300

DOFs

(b) Two layer mesh 1

0.8

Displacement

Displacement

1

0.6 0.4

0.95

0.9

0.85

0.2 0

0.8

0

50

100 150 200 250 300 350 400

0

DOFs

50

100 150 200 250 300 350 400 DOFs

(c) Three layer mesh FEM (linear) EFMM-LS (linear) EFMM-HR (linear)

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

Fig. 4. Normalized displacements at the loaded edge vs. DOFs (The ﬁgures in the right hand side are zoomed ones)

216

Genki Yagawa and Hitoshi Matsubara

10

2

y

E = 1000.0, v = 0.25

P

x P/2 Constrained in both the x and y directions Constrained in the x direction only Fig. 5. Cantilever beam model for error norm study; only the case of mesh is shown as examples

Ee =

Ω

T 1 ε − εexact σ − σ exact dΩ 2

1/2 (28)

where E2 is the displacement error norm and Ee that of the energy error. u, ε and σ are, respectively, the numerical results of displacement, strain and stress, whereas uexact , εexact and σ exact are the exact solutions. A beam of length L = 10, height D = 2 and thickness t = 1 is subjected to a shear load in plane stress condition. The material parameters are given by the Young’s modulus E = 1000.0 and the Poisson’s ratio ν = 0.25. The above displacement and energy convergence norms are plotted against the DOFs in Figs. 6 and 7, respectively, where the meshes are, respectively, 1 × 1, 2 × 2, 4 × 4, 16 × 16, 32 × 32, and 64 × 64. It can be seen from these ﬁgures that (a) Again, the error norms of the displacement of the EFMMs are between those of the linear and the quadratic FEMs (see Fig. 6). However, the convergence slopes of the EFMMs are almost equal to that of the quadratic FEM. (b) The error norms of the energy of the quadratic EFMMs are almost the same as that of the quadratic FEM and those of the linear EFMMs are between the linear and the quadratic FEMs. 4.3 Patch Test The patch test is performed using the three models of patch as shown in Fig. 8, where the displacement ﬁeld u(x) 0.2x = (29) v(y) −0.6y is applied at the boundary. Table 1 shows the test results for the FEMs and the EFMMs. As illustrated in the table, all the method passes the patch test for the Model A, which is a regular mesh division model. However, for the Model B and C, which are irregular ones, the EFMM-LSs do not pass the

Enriched Free Mesh Method FEM (linear) EFMM-LS (linear) EFMM-HR (linear) 0.5

217

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

0 0

1

2

3

4

Log ||E||2

-0.5 -1 -1.5 -2 -2.5 Log(DOFs)

Fig. 6. L2 error norms of displacement vs. DOFs FEM (linear) EFMM-LS (linear) 0.5 EFMM-HR (linear)

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

0 0

1

2

3

4

Log ||E||e

-0.5 -1

-1.5 -2 -2.5 Log(DOFs)

Fig. 7. Energy error norms vs. DOFs

M1

(a) Model A

M1

(b) Model B

M1

M2

(c) Model C

Fig. 8. Models for patch tests

test. Here, ”Pass” means that the displacement of the internal node (M 1 or M 2) satisﬁes Eq. (29). This means that the EFMM-LSs are nonconforming for irregular mesh, which is an open question.

218

Genki Yagawa and Hitoshi Matsubara Table 1. Displacements at internal nodes M 1 and M 2

Model A u(M 1) v(M 1) FEM(linear) 0.900 -2.400 0.900 -2.400 FEM(quadratic) 0.900 -2.400 EFMM-LS(linear) EFMM-LS(quadratic) 0.900 -2.400 0.900 -2.400 EFMM-HR(linear) EFMM-HR(quadratic) 0.900 -2.400 Exact 0.900 -2.400

Model B u(M 1) v(M 1) 1.200 -3.000 1.200 -3.000 1.198 -3.170 1.198 -3.141 1.200 -3.000 1.200 -3.000 1.200 -3.000

u(M 1) 0.600 0.600 0.611 0.611 0.600 0.600 0.600

Model C v(M 1) u(M 2) -2.400 1.300 -2.400 1.300 -2.372 1.285 -2.368 1.290 -2.400 1.300 -2.400 1.300 -2.400 1.300

v(M 2) -1.800 -1.800 -1.899 -1.859 -1.800 -1.800 -1.800

5 Concluding remarks A new Free Mesh Method called ”Enriched Free Mesh Method” is proposed in this paper, in which a high accuracy can be obtained without explicitly increasing the degree of freedoms. The work is summarized as follows, (1) The key idea of the proposed method is that the strain ﬁeld is assumed on clustered local elements, in addition to the usual displacement ﬁeld on each element. To relate the above two ﬁelds, the localized least square method or the Hellinger-Reissner principle are, respectively, employed. (2) The convergence characteristics of the displacement L2 error norms in the cantilever problem are between that of the FEM with the linear displacement ﬁeld and that with the quadratic one, whereas that of the energy error norms with the quadratic strain ﬁeld for the clustered elements is equivalent to that of the FEM with the quadratic displacement ﬁeld. (3) The EFMM based on the Hellinger-Reissner principle passes the patch test, whereas, for irregular nodal arrangements, the EFMM based on the localized least square method does not. This would be an open question and there is a room for future research.

References 1. Zienkiewicz OC, Taylor RL (2000) The ﬁnite element method. Fifth edition, Butterworth Heinemann 2. Cook RD, Malkus DS, Plesha ME (1989) Concepts and applications of ﬁnite element analysis. Third edition, Wiley 3. Barth TJ, Griebel M, Keyes DE, Nieminen RM, Roose D, Schlick T (2003) Meshfree methods for partial diﬀerential equation. Springer-Verlag Berlin Heidelberg 4. Liu GR, Liu MB (2003) Smoothed Particle Hydrodynamics a meshfree particle method. World Scientiﬁc publishing 5. Belytschko T, Lu YY, Gu L (1994) Element-free Galerkin methods. Int J Num Meth Engng 37:229–256 6. Lu YY, Belytschko T, Gu L (1994) A new implementation of the element-free Galerkin Method. Comput Meth Appl Mech Engng 113:397–414

Enriched Free Mesh Method

219

7. Liu WK, Jun S, Adee J, Belytischko T (1995) Reproducing kernel particle methods for structural dynamics. Int J Num Meth Engng 38:1655–1680 8. Liu WK, Li S, Belytschko T (1997) Moving least square kernel particle method Part 1: methodology and convergence. Comput Meth Appl Mech Engng 143:113–154 9. Yagawa G, Yamada T (1996) Free mesh method: a new meshless ﬁnite element method. Computational Mechanics 18:383–386 10. Yagawa G, Furukawa T (2000) Recent developments approaches for accurate free mesh method. Int J Num Meth Engng 47:1445–1462 11. Fujisawa T, Inaba M, Yagawa G (2003) Parallel computing of high-speed compressible ﬂows using a node-based ﬁnite-element method. Int J Num Meth Engng 58:481–511 12. J. Imasato, Y. Sakai (2002) Application of 2-dimentional crack propagation problem using FMM. Advances in Meshfree and X-FEM Methods, Liu GR, editor, World-Scientiﬁc 13. Matsubara H, Iraha S, Tomiyama J, Yagawa G (2002) Application of 3D free mesh method to fracture analysis of concrete. Advances in Meshfree and XFEM Methods, Liu GR, editor, World-Scientiﬁc 14. Matsubara H, Iraha S, Tomiyama J, Yamashiro T, Yagawa G (2004) Free mesh method using a tetrahedral element including vertex rotations. JSCE J of Structural Mechanics and Earthquake Engineering 766(I-68):97–107 15. Tian R, Matsubara H, Yagawa G, Iraha S, Tomiyama J (2004) Accuracy improvement on free mesh method: a high performance quadratic tetrahedral/triangular element with only corners. Proc of the 2004 Sixth World Congress on Computational Mechanics (WCCM VI) 16. O.C. Zienkiewicz, K. Morgan (1983), Finite element and approximation, John Wiley & Sons 17. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. PART 1: The recovery technique. Int J Num Meth Engng 33:1331–1364 18. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. PART 2: Error estimates and adaptivity. Int J Num Meth Engng 33:1365–1382 19. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery (SPR) and adaptive ﬁnite element reﬁnement. Comput Meth Appl Mech Engng 101:207– 224 20. Babuska I, Rheinboldt WC (1978) A-posteriori error estimates for the ﬁnite element method. Int J Num Meth Engng 12:1597–1615 21. Washizu K (1968) Variational methods in elasticity and plasticity. Pergamon Press, New York 22. Timoshenko SP, Goodier JN (1987) Theory of elasticity. McGraw-Hill

Modelling of Metal Forming Processes and Multi-Physic Coupling J.-L. Chenot and F. Bay Center for Material Forming (CEMEF) Ecole des Mines de Paris - UMR CNRS 7635 BP 207, F-06904 Sophia-Antipolis Cedex, France [email protected] Summary. The main physical phenomena which can be coupled with the mechanical computation of metal forming processes are analyzed. Recalling the classical thermal coupling, it is shown that a stronger numerical coupling is necessary when localization of the deformation occurs. Several situations where we have mechanical solid and liquid interactions with thermal coupling are brieﬂy mentioned. A more complete description of electro magnetic and thermal coupling is given in view of induction heating. Finally the case of multi scale coupling for metallurgic microstructure evolution is introduced. Key words: Computational Plasticity, Forming Process, Thermal Coupling, Induction Heating, Micro-Structure.

1 Introduction Since about thirty years ago, numerical modeling of metal forming processes was starting to be developed in laboratories [1] to [4] and later in software companies as well, using mostly the ﬁnite element method. To-day, with the help of powerful modern computers and parallel computation, it is possible to predict accurately several important technical parameters, for complex 3-D forming processes such as forging, rolling or extrusion. On the other hand, several physical phenomena still remain very approximately known, either during the forming process itself, or during the heating or cooling process, and in heat treatment operations. It is an industrial demand to predict with the same software the material evolution during the whole process. This particularly important if one wants to predict the microstructure evolution. The objective of the paper is to review some of the most important physical evolutions, which are coupled with the mechanical working process, keeping in mind that the ﬁnal microstructure is responsible for the ﬁnal properties of the work-piece. Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 221–238. © 2007 Springer. Printed in the Netherlands.

222

J.-L. Chenot and F. Bay

2 Mechanical Approach of Metal Forming Processes For a detailed account of the ﬁnite element modeling of metal forming processes, the reader is referred to [5]. 2.1 Constitutive Modeling Despite rigid plastic or rigid viscoplastic laws are still widely used in many research teams, the elastic plastic or viscoplastic laws must be preferred. The later ones are intrinsically more realistic; they allow the user to model properly unloading after forming, to predict spring back and the associated residual stresses. The elastic viscoplastic laws are also compulsory when small deformation processes are simulated such as during cooling, heat treatment, stretching, etc. In the literature, several degrees of sophistication can be found. The most widely used approximation, which reveals accurate enough in most forming processes is the additive decomposition of the strain rate tensor ε˙ into the elastic and plastic parts. It is usually written: ε˙ = ε˙ e + ε˙ p

(1)

Introduction of an objective derivative of the stress tensor; which is necessary when large rotations take place: dj σ = λe trace(˙ε e ) + 2µeε˙ e dt

(2)

The relatively general Perzyna formalism is often retained for the plastic component of the strain rate tensor: 1 −1 1 σeq − R m σ ε˙ p = (3) k K where σ is the deviatoric stress tensor, σeq the equivalent stress, R the yield stress, K the consistency and m the strain rate sensitivity index. At the interface between part and tool the friction shear stress can be modelled by : τ = αf (σn )K|∆v|q−1 ∆v

(4)

where αf is the friction coeﬃcient, σn function of the normal stress and ∆v is the tangential velocity. For an incompressible or quasi incompressible ﬂow, it is desirable to utilize a mixed formulation. In the domain Ω of the part, this formulation is written for any virtual velocity and pressure ﬁelds v ∗ , p∗ as: ∗ σ˙ : ε˙ ∗ dV − τ˙ · v ∗ dS − pdiv(v ˙ )dV = 0 (5) Ω

Ω

∂Ωc

Ω

∗ (div(v) + p/κ)p ˙ dV = 0

(6)

Modelling of Metal Forming Processes and Multi-Physic Coupling

223

2.2 Finite Element Approximation Many diﬀerent ﬁnite element formulations were proposed, and developed at the laboratory level, but it is now realized that the discretization scheme must be compatible with other numerical and computational constraints, among which we can quote: • • • • •

Remeshing and adaptive remeshing, Unilateral contact analysis, Iterative solving of non linear and linear systems; Domain decomposition and parallel computing; Easy transfer of physical internal parameters, when multi physic coupling must be taken into account.

Today a satisfactory compromise is based on a mixed velocity and pressure formulation using tetrahedral elements, and a bubble function to stabilize the solution for incompressible or quasi incompressible materials. The velocity ﬁeld is discretized with shape functions Nn , in term of nodal velocity vectors Vn : Vn Nn (ξ) (7) v= n

Using isoparametric elements the mapping between the physical space with coordinates x and the reference space, with coordinate ξ is: x= Xn Nn (ξ) (8) n

The strain rate tensor can be computed with the help of the conventional B discretized linear operator: ε˙ = Vn Bn (ξ) (9) n

The discretized mixed integral formulation for the mechanical problem is: √ RnV = ργNn dV + dK( 3ε¯˙)m−1 ε˙ : Bn dV Ω

Ω

p−1

αf K|∆v|

+ ∂Ωc

P Rm =

∆vNn dS −

ptr(Bn )dV = 0

(10)

Ω

Mm (div(v) + 3αd T˙ )dV = 0

(11)

Ω

The most widely used integration method remains the simple Euler one step scheme. It was recognized that a two levels Runge and Kutta method leads to a considerable improvement of the solution, which is particularly desirable when the work-piece undergoes a large rotation, such as in ring rolling.

224

J.-L. Chenot and F. Bay

2.3 Numerical Issues The non-linear equations resulting from the mechanical behaviour are linearized with the Newton-Raphson method. The resulting linear systems are often solved now with iterative methods, which appear faster and require much less CPU memory than the direct ones. Prediction of possible formation of folding defects during forging is based on the analysis of the contact of the part with itself, so providing a similar problem like the coupling with tools. Automatic dynamic remeshing during the simulation of the whole forming process is almost always necessary, as elements undergo very high strain which could produce degeneracy. Before this catastrophic event, decrease of element quality must be evaluated and a remeshing module must be launched periodically to recover a satisfactory element quality. The global mesh can be completely regenerated, using a Delaunay or any front tracing method, but the method of iterative improvement of the mesh, with a possible local change of element structure and connectivity, seems to be much more eﬀective. For industrial, complicated applications with short delays, the computing time can be decreased dramatically using several or several tens of processors. This requires to use an iterative solver and to deﬁne a partition of the domain, each sub domain being associated with a processor. But the parallelization is made more complex due to remeshing and the remeshing process itself must be parallelized. In order to avoid the necessity for the user to perform several computations, with diﬀerent meshes to check the accuracy, an error estimation can be developed using for example the generalization of the method proposed by Zienckiewicz and Zhu. Then, if the rate of convergence of the computation is known, the local mesh reﬁnement necessary to achieve a prescribed tolerance can be computed, and the meshing modules are improved to be able to respect the reﬁnement when generating the new mesh.

3 Thermal and Fluid-Solid Coupling 3.1 Classical Thermal and Mechanical Coupling The classical heat equation for deformable bodies is written simply: ρc

√ dT = div(kgrad(T )) + fw ( 3ε¯˙)m+1 dt

(12)

where the last term is a fraction fw of the viscoplastic heat dissipation. The constitutive law depends on temperature. For example we have the equations: K = K0 (ε0 + ε¯)n exp(β/T ),

m = m0 + m1 T

(13)

Modelling of Metal Forming Processes and Multi-Physic Coupling

225

The radiation condition on the free surface ∂Ωs is written: −k

∂T = εr σr (T 4 − T04 ) ∂n

(14)

where εr is the emissivity parameter, σr the Stephan constant and T0 the outside temperature. The conduction with the tools on ∂Ωc , is modeled by: −k

b ∂T = hcd (T − Ttool ) + αf K|∆v|q+1 ∂n b + btool

(15)

where Ttool is the tool temperature, b and btool are the eﬀuvisity parameters of the part and of the tool respectively. The thermal integral formulation can be written, for any test function w: dT ρc wdV + kgrad(T ) · grad(w)dV − q˙V wdV + εr σr (T 4 − T04 )wdS+ dt

Ω

Ω

+ ∂Ωc

Ω

∂Ωf

b q+1 αK|∆v| hcd (T − Ttool ) + wdS = 0 b + btool (16)

The previous equations are discretized with ﬁnite element, generally similar to those for the mechanical problem: Tn Nn (ξ) (17) T = n

so that the discretized form of the equations is: ˙ ρcT Nn dV + kgrad(T ) · grad(Nn )dV − q˙V wNn dV Ω

+

4

εr σr (T −

∂Ωf

T04 )Nn dS

Ω

+ hcd (T − Ttool ) − ∂Ωc

Ω

b τf ∆v Nn dS = 0 b + btool (18)

Diﬀerent time discretization schemes can be used, which allow to compute the temperature ﬁeld at time t + ∆t, knowing it at time t and t − ∆t, using an explicit scheme which avoids solving a non linear thermal equations. In most codes, coupling between mechanical and thermal equations is not performed at the increment level, as the scheme consists in computing ﬁrst the thermal ﬁeld, then the mechanical ﬁeld (without a ﬁxed point iteration algorithm).

226

J.-L. Chenot and F. Bay

3.2 Localization When the thermal and mechanical coupling is strong enough, such as in processes where localization in narrow shear bands can occur (e. g. in high speed machining), the previous method is not satisfactory and a ﬁxed point algorithm may not converge. In this case it is desirable to solve simultaneously the mechanical and thermal equations. Therefore we have a non linear problem with the following unknowns nodal unknowns at time t+∆t: temperature Tt+∆t , velocity Vt+∆t , and pressure Pt+∆t when a mixed formulation is used. A Newton-Raphson method must be utilized, where the unknowns are the same and the stiﬀness matrix must contain all the derivatives of the residual equation, including the coupling terms. 3.3 Fluid Solid Coupling During Heating or Heat Treatment Fluid solid coupling is an important issue in several industrial processes. During heating in a furnace, we must take into account the ﬂow of the surrounding gas and heat exchange between the gas and the preforms, in order to determine precisely the temperature ﬁeld inside the work-pieces which will be formed. The problem is even more complicated when one wants to predict the quenching process with water which will be vaporized at the contact of a hot work piece. The prediction of the temperature evolution in the part is again important, as it will be responsible for the geometric change of the part and the microstructure evolution. An analogous situation arises in casting of large work pieces during the cooling process, when a solid fraction interacts with a moving ﬂuid with complicated thermal and mechanical evolutions. An eﬃcient frame for this coupling is to use an ALE formulation for the liquid phase where the material velocity v is diﬀerent from the mesh velocity vg , which will be deﬁned by a smoothing operator, such as: div(grad(vg )) = 0

(19)

and boundary conditions preserving the geometry of the free surface: (vg − v) · n = 0. With the ALE scheme, the grid derivative of any parameter a will be evaluated in term if the material derivative according to: da dg a = + (vg − v) · grad(a) dt dt

(20)

4 Electro Magnetic Coupling 4.1 The Induction Heating Process Many industrial processes are based on an eﬃcient use of coupling between electromagnetic, thermal and mechanical phenomena. They generally use direct or induced currents to generate heat inside a work piece in order to get

Modelling of Metal Forming Processes and Multi-Physic Coupling

227

Fig. 1. Induction heating setup

either a prescribed temperature ﬁeld or some given mechanical or metallurgical properties through an accurate control of temperature evolution with respect to time. The basic induction setup [6] consists of one or several inductors and metallic work pieces to be heated (see Fig. 1). The inductors are supplied with alternating current with frequencies ranging from ﬁfty to several hundred thousand cycles per second. A rapidly oscillating magnetic ﬁeld is generated and in turn induces eddy currents in the work piece due to the Joule eﬀect. These currents generate ohmic heat losses inside the work piece. Moreover, for ferromagnetic materials, alternating magnetization and hysteresis eﬀect also contribute to heat generation. Most of the heat is produced in a thin layer under the surface of the work piece; the skin depth - deﬁned as the depth at which the magnitude of the ﬁeld drops to a value of e−1 of its surface value: 1 (21) δ= πf σµ where f is the frequency, σ the electrical conductivity and µ the magnetic permeability. High frequencies are used to achieve surface heating, while low frequencies generate a more uniform heating. 4.2 The Direct Electro-Thermal Formulation The electromagnetic model is classically based on the set of Maxwell equations: div(B) = 0 (22) div(D) = 0

(23)

228

J.-L. Chenot and F. Bay

rot(E) = −

∂B ∂t

(24)

∂D (25) ∂t where H is the magnetic ﬁeld, B the magnetic induction, E the electric ﬁeld, D the electric ﬂux density, and J the electric current density associated with free charges. We also have the following relations which for the intrinsic material properties: D = εE (26) rot(H) = J +

B = µ(|H|)H

(27)

J = σE

(28)

where ε is the dielectric constant, µ the magnetic permeability, and σ the electrical conductivity. They all depend on temperature and the magnetic permeability µ depends also on H. The range of frequencies dealt with in induction heating (less than 106 Hz) enables us to neglect the displacement currents in the Maxwell-Ampere equation (magneto-quasi-static approximation). A combination of the previous relations leads us to the following equation where the unknown is the electric ﬁeld. 1 ∂JS ∂E + rot rot(E) = − (29) σ ∂t µ ∂t with σ = σ(T ) and µ = µ(T, H). We deal here with axisymmetrical cases, in which the electric ﬁeld will only have a non-zero component in the θ direction: E = (0, Eθ (r, z), 0)

(30)

Temperature evolution in the work piece is governed by the classical heat transfer equation: ∂T − div(kgrad (T )) = Q˙ em (31) ρC ∂t where ρ denotes the material density, C and k respectively the speciﬁc heat and thermal conductivity, all temperature dependent. Q˙ em denotes the local heat rate, generated by the eddy currents, and integrated over one period: 1 ¯˙ Q em = T

T

σ|E|2 dt

(32)

0

The boundary conditions can be of various kinds: prescribed heat ﬂux or temperature, convection or radiation.

Modelling of Metal Forming Processes and Multi-Physic Coupling

229

4.3 Finite Element Numerical Approximation We deﬁne Ω as being a two-dimensional axisymmetrical domain which covers the part to be heated Ωpart , the inductor Ωinductor and a ﬁnite volume of air air surrounding the inductor and the part. We have chosen here to carry out coupling between the part and the inductor for the electromagnetic computations using ﬁnite elements rather than boundary elements; the air domain thus needs to be wide enough in order to model accurately electromagnetic wave propagation. The domain is discretized using second order triangular ﬁnite elements (6nodes triangles). The unknown ﬁelds - electric ﬁeld Eθ for the electromagnetic computations, temperature ﬁeld T for the thermal computations and velocity ﬁeld V for the mechanical computations - can thus be approximated over the whole domain by the classical ﬁnite element approximation: En (t)Nn (ξ) (33) E(t, r, z) = n

where E : n(t) denotes the approximated value of the θ-component of the electric ﬁeld at the node n and at time t. The discretized expression of the variational formulation is: ∂E (34) [C em ] + [K em ] {E(t)} = {B em } ∂t The temperature distribution is discretized according in the same way as in Eq.(18). Numerical models in induction heating often solve a harmonic model. This assumption is quite restrictive when one deals with non-linear magnetic materials. We have thus chosen to solve the time-dependent model. We need therefore to integrate numerically in time the electromagnetic and thermal equations. We detail here the selected time integration scheme for the electromagnetic equation. The procedure is the same for the thermal equation. We use a second-order two time step ﬁnite diﬀerence scheme: Step 1: the system is solved at time t∗ such that t < t∗ < t + δt2 with: t∗ = α1 (t − δt1 ) + α2 t + α3 (t + δt2 )

(35)

with α1 + α2 + α3 = 0. The electric ﬁeld E ∗ at time t∗ and its time derivative write: E ∗ = α1 E t−δt1 + α2 E t + α3 E t+δt2

(36)

E t+δt2 ∂E ∗ E t−δt2 − E t =γ + (γ − 1) ∂t δt2 δt1

(37)

230

J.-L. Chenot and F. Bay

The following system Eq.(38) is written at time t∗ . E ∗ and its derivative are replaced by Eqs.(36) and (37) and the system are solved for the unknown variable E ∗ : γ ∗ em ∗ em ∗ [C ] + [K ] E ∗ = {B em } + c1 [C em ]∗ E t + c0 [C em ]∗ E t−δt1 (38) α3 δt2 γ γ−1 γα2 γα1 γ−1 + + , c2 = − . δt2 δt1 α3 δt2 α3 δt2 δt1 The two time steps scheme we have requires the solving of a non-linear equation, as the matrix [C] is dependant on the magnetic ﬁeld. In order to avoid an additional non-linearity, the matrix is linearized and is approximated using its values at time t and t − δt1 : δt2 δt2 ∗ (39) [C]t−δt1 + α2 + α3 1 + [C]t−δt1 [C] = α1 − α3 δt1 δt1 where c1 =

Step 2: computation of: {E}

t+δt2

=

1

∗ t−δt1 t − α2 {E} {E} − α1 {E} α3

(40)

4.4 The Electromagnetic/Thermal Coupling Procedure Physical problems arising from heat transfer and electromagnetism have in common the fact that they are both time-dependent. Their speciﬁc timescales are however very diﬀerent. The speciﬁc time scale of an electromagnetic problem is related to the wave-associated period –typically 102 s for a 100 Hz frequency down to 108 s for a 100 MHz frequency– whereas the speciﬁc time scale for heat transfer averages normally one second. A direct model based on ﬁnite elements has been developed in our laboratory to cope with these speciﬁcities. The model includes a speciﬁc coupling procedure for solving: •

the Maxwell equations - in order to access the electromagnetic ﬁelds giving the eddy currents dissipated in the material (main source term for the heat transfer equation), • the heat transfer equation - leading to temperature evolution in the material. The coupling between the electromagnetic and thermal computations relies on a convergence test over the mean heating power and on tests over the variations of the magnetic parameters that determine respectively the passage from an electrical to thermal resolution or inversely from a thermal to an electric one. Once the electromagnetic ﬁeld has been calculated, the rate of heat generation Q˙ em for the heat equation needs to be evaluated at every integration

Modelling of Metal Forming Processes and Multi-Physic Coupling

231

points. As the electromagnetic time step is far smaller than the thermal one, we do not consider the instantaneous Joule power calculated at a given time at every integration points. We rather consider a mean Joule power averaged over one period of the electromagnetic ﬁeld: 1 Qem (nT, int) = T

nT

σ(int, t)|E(int, t)|2 dt

(41)

(n−1)T

where int is the considered integration point, T is the period of the power supply currents, n is number of periods considered and Eθ (int, t) is the value at time t of the electric ﬁeld interpolated at the integration point int. At the end of each electromagnetic period, the newly calculated mean power is compared to the one calculated at the previous period until it stabilizes. Thermal computations are started with the stabilized thermal source power calculated at (n + 1) T if the following convergence test (33) is conducted at every integration points: ¯ em (nT ) ¯ em ((n + 1)T ) − Q Q <ε ¯ Qem (nT )

(42)

where ε is the user-supplied convergence parameter. These thermal computations are valid as long as the variation of the physical magnetic parameters such as the magnetic permeability and the electric conductivity do not exceed 5%. Their variations with temperature are tested after each new thermal computation. The following criteria are tested for every mesh element: n+1 n ) − σ(Tmax ) σ(Tmax < 5% n ) σ(Tmax (43) n+1 n µ(Tmax ) − µ(Tmax ) < 5% n ) µ(Tmax n+1 where Tmax is the maximum value of the temperature ﬁeld in a given element n is the maximum value of the temperature ﬁeld at time t + dtther and Tmax in the same given element at current time t. When the maximum relative variations reach the threshold of 5%, the previously calculated mean heat power is assumed to be irrelevant, and a new electromagnetic calculation is carried out. For their part, mechanical computations are carried out at the same time steps than thermal computations.

4.5 Results The ﬁrst case deals with a static long inductor in ferromagnetic EN3 mild steel annealed at 930 ◦ C. In this case, the work piece is heated by an inductor of the same length as the work piece. The geometry consists in a cylindrical

232

J.-L. Chenot and F. Bay

Fig. 2. a) Finite element mesh; b) Electric ﬁeld; c) Temperature ﬁeld

EN3 part surrounded with Kaowool insulation, a ceramic tube and ﬁnally a three-layer coil. The mesh used for this case is displayed in Fig. 2a. The multiturn coil is modeled as a continuous single coil with a uniform initial current density. Two thermocouples have been placed: the ﬁrst one on the surface on the middle of the part and the second one in a hole bored in the center of the part so as to measure temperature inside the part. Process parameters are: • frequency: 500Hz • current density: 8.108 Amps/m2 • electromagnetic time step: T/64=3.125 10−5 s • thermal time step: 0.5s In order to enable a visualization of the dissipated joule power, an eﬀective electrical ﬁeld has been deﬁned at a given node as the integration over an electromagnetic period of the square of the real instantaneous electrical ﬁeld:

(n+1)T

1 E 2 (t)dt (44) Eef f = T nT

This eﬀective electrical ﬁeld is also proportional to the amplitude of the electric ﬁeld in a harmonic complex formulation. Figure 2b shows the eﬀective electric ﬁelds isovalues. Due to the high value of the permeability, we can notice the concentration of the magnetic ﬁeld along the work piece surface; this is a well-known physical eﬀect since magnetic ﬁeld lines tend to concentrate on material surface when the magnetic permeability gets high. We can see on Fig. 2c how the heat propagates here rather uniformly from the surface towards the centre. This is typical of a global homogeneous heating application.

Modelling of Metal Forming Processes and Multi-Physic Coupling

233

Fig. 3. Experimental validation

Figure 3 shows the excellent agreement between experimental and computed temperatures on the surface and inside the work piece. On one hand, the computed temperatures on the surface provide a good way to validate the dissipated heat due to eddy currents inside the work piece - and thus the electric ﬁeld computation and the whole electromagnetic procedure. On the other hand, the good agreement observed between the experimental and numerically computed delay on heat propagation to the internal part of the work piece validates the heat transfer diﬀusion model and the thermal coupling procedure. This case deals with a moving short inductor - a case representative of what takes place in an induction heat treatment process. The inductor displacement is modeled through a continuous variation of physical properties of the mesh. Figure 4 shows the geometry and the initial location of the inductor in the mesh. Figure 5 shows an example of electric ﬁeld distribution at a given time step; in this case, the electric ﬁeld is non-symmetric since the inductor location changes continuously. The numerical model presented here is described more in detail in [7]. Extension to parallel computations is detailed in [8]. This model has also been used for magnetic parameters identiﬁcation as detailed in [9]. A global optimization procedure has also been developed to achieve better control of induction heating processes. This strategy can be extended to various multiphysics coupled problems; it is detailed in [10].

234

J.-L. Chenot and F. Bay

Fig. 4. Moving inductor case: geometry and initial mesh

Fig. 5. Moving inductor case: electric ﬁeld isovalues

5 Coupling with Microstructure Evolution 5.1 Introduction The microstructure of the materials changes signiﬁcantly during forming operations. For instance in metals, dynamic or static recovery and recrystallization can take place. These evolutions need to be modeled when the ﬁnal microstructure is to be optimized, or when the behavior of the metal must be described accurately during forming. Several strategies can be developed to compute microstructure evolutions in forming processes with large spatial

Modelling of Metal Forming Processes and Multi-Physic Coupling

235

heterogeneity of strain rate, strain and temperature ﬁelds. The ﬁnite element method allows to model microstructure evolutions in complementary ways. 5.2 Macroscopic Approach In a ﬁrst classical way, one can assume that each node covers a material volume suﬃciently large to be summarized by a Homogeneous Equivalent Medium (HEM). Laws for microstructure evolution of homogeneous media are then applied. This strategy is adequate for modeling a large volume of material, for instance at the scale of a component. A well-known example of a microstructure model is the Avrami equation [11]. It is typically used in an integrated form to describe the recrystallization phenomena for metals as a function of time t: k t (45) X = 1 − exp − ln t0.5 where X is the state variable describing the recrystallized volume fraction, t0.5 is the half recrystallization time, and k the Avrami exponent. Such microstructure evolution laws are typically obtained from isothermal experiments. However, a typical forming process induces signiﬁcant temperature evolutions. It is assumed that non isothermal path can be divided into a number of isothermal steps. Using the results of isothermal tests to calculate the microstructure evolution for any thermal path implies that an integration rule can be applied. Additivity rules are often used in recrystallization studies, the procedure uses a ﬁctitious time method [12], [22] to discretize the microstructure evolution equation. Using for instance the Avrami equation, the algorithm is as follows: at step i of the computation, the recrystallized volume fraction Xi at time ti has been computed; the ﬁctitious time t∗i+1 is calculated as the total time needed to obtain a recrystallized volume fraction Xi at constant temperature Ti+1 . In order to calculate the next recrystallized volume fraction Xi+1 , Avrami equation is used for temperature Ti+1 and time (t∗i+1 + ti+1 − ti ). R for This strategy has been used with the 3D Finite Element code Forge3 forging simulations. Figure 6 illustrates the case of a 316L austenitic stainless steel part deformed at 1273K and annealed at 1373K during 50 seconds. The simulation allows us to take into account both the strain and temperature variations throughout the part, leading to a complex map of statically recrystallized volume fractions, ranging from 10 to 100%, as shown in Fig. 6. The challenge is now to model microstructure evolutions over multiple interpass and forming steps; this requires to go back and reﬁne the description of the physical phenomena integrated in the macroscopic evolution laws. 5.3 Multi-Scale Coupling and the Digital Material A second approach may be taken at a smaller scale, within a HEM. It consists in meshing a heterogeneous microstructure, possibly of complex topology and

236

J.-L. Chenot and F. Bay

Fig. 6. Recrystallized volume fraction maps of a forged 316l part

geometry, for studying the detailed relationships between the microstructure and its evolution, or even the associated constitutive law. This is the case for instance when dealing with the plastic deformation of a steel during phase transformation (e.g. [13]). An austenite and ferrite composite is in fact a two-phase HEM which needs to be analyzed in order to determine the mechanical behavior of the steel and the strain distribution within each phase. Analytical bounds and estimates for the mechanical behavior of a two-phase aggregate imply strong topological assumptions. The calculation of the mechanical response of these composite materials can be calculated using the F. E. M. with a representative description of the microstructure, and well posed boundary conditions. The HEM must contain enough grains so that the global behavior is statistically representative of material response. Predictions of such FEM simulations can then be compared with analytical models. An example of a two-phase topology is shown in Fig. 7 with the corresponding 3D ﬁnite element discretization. A calculation of strain distribution for this two-phase ensemble is presented in Fig. 8. The F.E. discretization allows us to capture strong strain gradients at the interface between the two phases. Such digital multiphase volume calculations can ﬁrst be used to validate appropriate analytical models. These simpler models can be used as constitutive laws in large scale ﬁnite element simulations and coupled with the phase transformation diagram to calculate local percentage of each phase. This complete numerical model allows us to calculate thermal, mechanical and metallurgical evolutions in forming processes inducing large strain such as forging or rolling.

Modelling of Metal Forming Processes and Multi-Physic Coupling

237

Fig. 7. Austenite-ferrite topology and corresponding 3d ﬁnite element mesh

Fig. 8. Strain ﬁeld calculated for the two-phase material volume of Fig. 7

This digital material approach can be further reﬁned to integrate the crystallographic textures. A statistically representative ﬁnite element polycrystal can be created by considering each ﬁnite element as a single crystal. Such a strategy proves to be very eﬃcient when the mechanical response is dictated by the heterogeneity of the elastic-plastic behavior throughout a polycrystal, as in fatigue [14].

6 Conclusions We have reviewed several coupling problems where the classical mechanical treatment must be completed in order to take also into account other physical phenomenons: thermal behavior with possible localization of the strain rate, ﬂuid-solid coupling, electro magnetic heating and microstructure evolution. The simple examples which are presented show that the domain is still under

238

J.-L. Chenot and F. Bay

development, and that much eﬀort must be devoted to these ﬁelds before it can be used routinely in industry for any metallic material.

References 1. Cornﬁeld GC, Johnson RH (1973) Theoretical prediction of plastic ﬂow in hot rolling including the eﬀect of various temperature distribution. J Iron Steel Inst 211:567 2. Lee CH, Kobayashi S (1973) New solutions to rigid plastic deformation problems using a matrix method. Trans ASME, J Eng Ind 95:865 3. Zienkiewicz OC, Valliapan S, King IP (1969) Elasto-solution of engineering problems: initial stress, ﬁnite element approach. Int J Num Meth Engng 1:75– 100 4. Surdon G., Chenot J-L (1986) Finite element calculations of three-dimensional hot forging. International Conference on Numerical Methods in Industrial Forming Processes Numiform’86, ed. by Mattiasson K et al., Balkema AA, Rotterman, 287–292 5. Wagoner, RH, Chenot J-L (2001) Metal forming analysis. Cambridge University Press, Cambridge 6. Davies EJ (1990) Conduction and Induction Heating, P. Peregrinus Ltd., London 7. Bay F, Labbe V, Favennec Y, Chenot J-L (2000) A numerical model for induction heating processes coupling electromagnetism and thermomechanics. Int J Num Meth Engng 58:839–867 8. Labbe V, Favennec Y, Bay F (2002) Numerical modeling of heat treatment with induction heating processes using a parallel ﬁnite element software. 5th Conf. World Congress on Computational Mechanics, Vienna, Austria 9. Favennec Y, Labbe V, Tillier Y, Bay F (2000) Identiﬁcation of magnetic parameters through inverse analysis coupled with ﬁnite element modeling. IEEE Transactions on Magnetics 38(6):3607–3619 10. Favennec Y, Labbe V, Bay F (2004) The ultraweak time coupling in nonlinear modeling and related optimization problems. Int J Num Meth Engng 60:3 11. Avrami M (1939) Kinetics of phase change. I. General theory, Journal of Chemical Physics 7:1103–1112; (1940) II. Transformation-time relations for random distribution of nuclei. Journal of Chemical Physics 8:212–224; (1941) III, Granulation, phase change and microstructure. Journal of Chemical Physics 9:177–18 12. Pumphrey WI, Jones FW (1948) Inter-relation of hardenability and isothermal transformation data. ISIJ 159:137–144 13. Thibaux P (2001) Comportement m´ecanique d’un acier C-Mn microalli´e lors du laminage intercritique. PhD Thesis, Ecole des Mines de Paris, CEMEF, Sophia Antipolis, France 14. Turkmen HS, Log´e RE, Dawson PR, Miller MP (2003) On the mechanical behavior of AA 7075-T6 during cyclic loading. International Journal of Fatigue 25(4):267–281

Enhanced Rotation-Free Basic Shell Triangle. Applications to Sheet Metal Forming Eugenio O˜ nate1 , Fernando G. Flores2 and Laurentiu Neamtu3 1

2

3

International Center for Numerical Methods in Engineering (CIMNE) Technical University of Catalonia (UPC) Ediﬁcio C1 Gran Capit´ an s/n, 08034 Barcelona, Spain [email protected] National University of Cordoba Casilla de Correo 916 5000 C´ ordoba, Argentina [email protected] Quantech ATZ SA Gran Capit´ an 2–4, 08034 Barcelona, Spain [email protected]

Summary. An enhanced rotation-free three node triangular shell element (termed EBST) is presented. The element formulation is based on a quadratic interpolation of the geometry in terms of the six nodes of a patch of four triangles associated to each triangular element. This allows to compute an assumed constant curvature ﬁeld and an assumed linear membrane strain ﬁeld which improves the in-plane behaviour of the element. A simple and economic version of the element using a single integration point is presented. The implementation of the element into an explicit dynamic scheme is described. The eﬃciency and accuracy of the EBST element and the explicit dynamic scheme are demonstrated in many examples of application including the analysis of a cylindrical panel under impulse loading and sheet metal stamping problems.

1 Introduction Triangular shell elements are very useful for the solution of large scale shell problems occurring in many practical engineering situations. Typical examples are the analysis of shell roofs under static and dynamic loads, sheet stamping processes, vehicle dynamics and crash-worthiness situations. Many of these problems involve high geometrical and material non linearities and time changing frictional contact conditions. These diﬃculties are usually increased by the need of discretizing complex geometrical shapes. Here the use of shell triangles and non-structured meshes becomes a critical necessity. Despite recent advances in the ﬁeld [1]–[6] there are not so many simple shell

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 239–265. © 2007 Springer. Printed in the Netherlands.

240

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

triangles which are capable of accurately modelling the deformation of a shell structure under arbitrary loading conditions. A promising line to derive simple shell triangles is to use the nodal displacements as the only unknowns for describing the shell kinematics. This idea goes back to the original attempts to solve thin plate bending problems using ﬁnite diﬀerence schemes with the deﬂection as the only nodal variable [7]–[9]. In past years some authors have derived a number of thin plate and shell triangular elements free of rotational degrees of freedom (d.o.f.) based on Kirchhoﬀ’s theory [10]–[26]. In essence all methods attempt to express the curvatures ﬁeld over an element in terms of the displacements of a collection of nodes belonging to a patch of adjacent elements. O˜ nate and Cervera [14] proposed a general procedure of this kind combining ﬁnite element and ﬁnite volume concepts for deriving thin plate triangles and quadrilaterals with the deﬂection as the only nodal variable and presented a simple and competitive rotation-free three d.o.f. triangular element termed BPT (for Basic Plate Triangle). These ideas were extended in [20] to derive a number of rotationfree thin plate and shell triangles. The basic ingredients of the method are a mixed Hu-Washizu formulation, a standard discretization into three node triangles, a linear ﬁnite element interpolation of the displacement ﬁeld within each triangle and a ﬁnite volume type approach for computing constant curvature and bending moment ﬁelds within appropriate non-overlapping control domains. The so called “cell-centered” and “cell-vertex” triangular domains yield diﬀerent families of rotation-free plate and shell triangles. Both the BPT plate element and its extension to shell analysis (termed BST for Basic Shell Triangle) can be derived from the cell-centered formulation. Here the “control domain” is an individual triangle. The constant curvatures ﬁeld within a triangle is computed in terms of the displacements of the six nodes belonging to the four elements patch formed by the chosen triangle and the three adjacent triangles. The cell-vertex approach yields a diﬀerent family of rotation-free plate and shell triangles. Details of the derivation of both rotation-free triangular shell element families can be found in [20]. An extension of the BST element to the non linear analysis of shells was implemented in an explicit dynamic code by O˜ nate et al. [25] using an updated Lagrangian formulation and a hypo-elastic constitutive model. Excellent numerical results were obtained for non linear dynamics of shells involving frictional contact situations and sheet stamping problems [17,18,19,25]. A large strain formulation for the BST element using a total Lagrangian description was presented by Flores and O˜ nate [23]. A recent extension of this formulation is based on a quadratic interpolation of the geometry of the patch formed by the BST element and the three adjacent triangles [26]. This yields a linear displacement gradient ﬁeld over the element from which linear membrane strains and constant curvatures can be computed within the BST element.

Enhanced Rotation-Free Basic Shell Triangle

241

In this chapter an enhanced version of the BST element (termed EBST element) is derived using an assumed linear ﬁeld for the membrane strains and an assumed constant curvature ﬁeld. Both assumed ﬁelds are obtained from the quadratic interpolation of the patch geometry following the ideas presented in [26]. Details of the element formulation are given. An eﬃcient version of the EBST element using one single quadrature point for integration of the tangent matrix is presented. An explicit scheme adequate for dynamic analysis is brieﬂy described. The eﬃciency and accuracy of the EBST element is validated in a number of examples of application including the non linear analysis of a cylindrical shell under an impulse loading and practical sheet stamping problems.

2 Basic Thin Shell Equations Using a Total Lagrangian Formulation 2.1 Shell Kinematics A summary of the most relevant hypothesis related to the kinematic behaviour of a thin shell are presented. Further details may be found in the wide literature dedicated to this ﬁeld [8,9]. Consider a shell with undeformed middle surface occupying the domain Ω 0 in R3 with a boundary Γ 0 . At each point of the middle surface a thickness h0 is deﬁned. The positions x0 and x of a point in the undeformed and the deformed conﬁgurations can be respectively written as a function of the coordinates of the middle surface ϕ and the normal t3 at the point as x0 (ξ1 , ξ2 , ζ) = ϕ0 (ξ1 , ξ2 ) + λt03 x (ξ1 , ξ2 , ζ) = ϕ (ξ1 , ξ2 ) + ζλt3

(1) (2)

where ξ1 , ξ2 are arc-length curvilinear principal coordinates deﬁned over the middle surface of the shell and ζ is the distance from the point to the middle surface in the undeformed conﬁguration. The product ζλ is the distance from the point to the middle surface measured on the deformed conﬁguration. The parameter λ relates the thickness at the present and initial conﬁgurations as: h (3) h0 This approach implies a constant strain in the normal direction. Parameter λ will not be considered as an independent variable and will be computed from purely geometrical considerations (isochoric behaviour) via a staggered iterative update. Besides this, the usual plane stress condition of thin shell theory will be adopted. A convective system is computed at each point as λ=

gi (ξ) =

∂x ∂ξi

i = 1, 2, 3

(4)

242

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

∂ (ϕ ϕ (ξ1 , ξ2 ) + ζλt3 ) = ϕ α + ζ (λt3 ) α ∂ξα ∂ (ϕ ϕ (ξ1 , ξ2 ) + ζλt3 ) = λt3 g3 (ξ) = ∂ζ

gα (ξ) =

α = 1, 2

(5) (6)

This can be particularized for the points on the middle surface as aα = gα (ζ = 0) = ϕ α

(7)

a3 = g3 (ζ = 0) = λt3

(8)

The covariant (ﬁrst fundamental form) metric tensor of the middle surface is aαβ = aα · aβ = ϕ α · ϕ β

(9)

The Green-Lagrange strain vector of the middle surface points (membrane strains) is deﬁned as (10) εm = [εm11 , εm12 , εm12 ]T with

1 (aij − a0ij ) (11) 2 The curvatures (second fundamental form) of the middle surface are obtained by εmij =

καβ =

1 ϕ α · t3 β + ϕ β · t3 α = −t3 · ϕαβ 2

,

α, β = 1, 2

The deformation gradient tensor is F =[x1 , x2 , x3 ] = ϕ 1 + ζ (λt3 ) 1 ϕ 2 + ζ (λt3 ) 2 λt3

(12)

(13)

The product FT F = U2 = C (where U is the right stretch tensor, and C the right Cauchy-Green deformation tensor) can be written as ⎤ ⎡ a11 + 2κ11 ζλ a12 + 2κ12 ζλ 0 (14) U2 = ⎣ a12 + 2κ12 ζλ a22 + 2κ22 ζλ 0 ⎦ 0 0 λ2 In the derivation of expression (14) the derivatives of the thickness ratio λ a and the terms associated to ζ 2 have been neglected. Equation (14) shows that U2 is not a unit tensor at the original conﬁguration for curved surfaces (κ0ij = 0). The changes of curvature of the middle surface are computed by (15) χij = κij − κ0ij Note that δχij = δκij .

Enhanced Rotation-Free Basic Shell Triangle

243

For computational convenience the following approximate expression (which is exact for initially ﬂat surfaces) will be adopted ⎤ ⎡ a11 + 2χ11 ζλ a12 + 2χ12 ζλ 0 (16) U2 = ⎣ a12 + 2χ12 ζλ a22 + 2χ22 ζλ 0 ⎦ 0 0 λ2 This expression is useful to compute diﬀerent Lagrangian strain measures. An advantage of these measures is that they are associated to material ﬁbres, what makes it easy to take into account material anisotropy. It is also useful to compute the eigen decomposition of U as U=

3

λα rα ⊗ rα

(17)

α=1

where λα and rα are the eigenvalues and eigenvectors of U. The resultant stresses (axial forces and moments) are obtained by integrating across the original thickness the second Piola-Kirchhoﬀ stress vector σ using the actual distance to the middle surface for evaluating the bending moments. This gives

σ dζ (18) σ m ≡ [N11 , N22 , N12 ]T = σ b ≡ [M11 , M22 , M12 ]T =

h0

h0

σ λζ dζ

With these values the virtual work can be written as

T δεεmσ m + δκ κT σ b dA = δuT tdA A0

(19)

(20)

A0

where δu are virtual displacements, δεεm is the virtual Green-Lagrange membrane strain vector, δκ κ are the virtual curvatures and t are the surface loads. Other load types can be easily included into (20). 2.2 Constitutive Models In order to treat plasticity at ﬁnite strains an adequate stress-strain pair must be used. The Hencky measures will be adopted here. The (logarithmic) strains are deﬁned as ⎤ ⎡ 3 ε11 ε21 0 ln (λα ) rα ⊗ rα (21) Eln = ⎣ ε12 ε22 0 ⎦ = α=1 0 0 ε33 For the type of problems dealt within the paper we use an elastic-plastic material associated to thin rolled metal sheets.

244

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

In the case of metals, where the elastic strains are small, the use of a logarithmic strain measure reasonably allows to adopt an additive decomposition of elastic and plastic components as Eln = Eeln + Epln

(22)

A linear relationship between the (plane) Hencky stresses and the logarithmic elastic strains is chosen giving T = H Eeln

(23)

where H is the constitutive matrix. The constitutive equations are integrated using a standard return algorithm. The following Mises-Hill [30] yield function with non-linear isotropic hardening is chosen n

2 2 2 + (F + H) T22 − 2H T11 T22 + 2N T12 = σ0 (e0 + ep ) (G + H) T11

(24)

where F, G, H and N deﬁne the non-isotropic shape of the yield surface and the parameters σ0 , e0 and n deﬁne its size as a function of the eﬀective plastic strain ep . The simple Mises-Hill yield function allows, as a ﬁrst approximation, to treat rolled thin metal sheets with planar and transversal anisotropy. The Hencky stress tensor T can be easily particularized for the plane stress case. We deﬁne the rotated Hencky and second Piola-Kirchhoﬀ stress tensors as TL = RTL T RL

(25)

RTL

(26)

SL =

S RL

where RL is the rotation tensor obtained from the eigenvectors of U given by (27) RL = r1 , r2 , r3 The relationship between the rotated Hencky and Piola-Kirchhoﬀ stresses is (α, β = 1, 2) 1 [TL ]αα λ2α ln (λα /λβ ) [TL ]αβ = 1 2 − λ2 λ α β 2

[SL ]αα = [SL ]αβ

(28)

The second Piola-Kirchhoﬀ stress tensor can be computed by S=

2 2 α=1 β=1

[SL ]αβ rα ⊗ rβ

(29)

The second Piola-Kirchhoﬀ stress vector σ used in Eqs.(18–19) can be readily extracted from the S tensor.

Enhanced Rotation-Free Basic Shell Triangle

245

3 Enhanced Basic Shell Triangle The main features of the element formulation (termed EBST for Enhanced Basic Shell Triangle) are the following: 1. The geometry of the patch formed by an element and the three adjacent elements is quadratically interpolated from the position of the six nodes in the patch (Fig. 1). 2. The membrane strains are assumed to vary linearly within the central triangle and are expressed in terms of the (continuous) values of the deformation gradient at the mid side points of the triangle. 3. An assumed constant curvature ﬁeld within the central triangle is chosen. This is computed in terms of the values of the (continuous) deformation gradient at the mid side points. Details of the derivation of the EBST element are given below. 3.1 Definition of the Element Geometry and Computation of Membrane Strains A quadratic approximation of the geometry of the four elements patch is chosen using the position of the six nodes in the patch. It is useful to deﬁne the patch in the isoparametric space using the nodal positions given in the Table 1 (see also Fig. 1). Table 1. Isoparametric coordinates of the six nodes in the patch of Fig. 1 1234 5 6 ξ 0 1 0 1 -1 1 η 0 0 1 1 1 -1

The quadratic interpolation is deﬁned by ϕ=

6

Ni ϕ i

(30)

i=1

with (ζ = 1 − ξ − η) N1 = ζ + ξη N4 = N2 = ξ + ηζ N5 = N3 = η + ζξ N6 =

ζ 2 ξ 2 η 2

(ζ − 1) (ξ − 1) (η − 1)

(31)

This interpolation allows to computing the displacement gradients at selected points in order to use an assumed strain approach. The computation of the gradients is performed at the mid side points of the central element of the patch denoted by G1 , G2 and G3 in Fig. 1. This choice has the following advantages.

246

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

η 5

4

2

M

2

G1

G2

1

4

.. .

1 3

3

2

1

3

G3

2

ξ

3 1

5

6

(a)

6 (b)

Fig. 1. (a) Patch of three node triangular elements including the central triangle (M) and three adjacent triangles (1, 2 and 3); (b) Patch of elements in the isoparametric space

•

Gradients at the three mid side points depend only on the nodes belonging to the two elements adjacent to each side. This can be easily veriﬁed by sampling the derivatives of the shape functions at each mid-side point. • When gradients are computed at the common mid-side point of two adjacent elements, the same values are obtained, as the coordinates of the same four points are used. This in practice means that the gradients at the mid-side points are independent of the element where they are computed. A side-oriented implementation of the ﬁnite element will therefore lead to a unique evaluation of the gradients per side. The Cartesian derivatives of the shape functions are computed at the original conﬁguration by the standard expression

Ni,ξ Ni,1 = J−1 (32) Ni,2 Ni,η

where the Jacobian matrix at the original conﬁguration is

0 ϕ · t1 ϕ0 η · t1 J = 0ξ ϕ ξ · t2 ϕ0 η · t2

(33)

The deformation gradients on the middle surface, associated to an arbitrary spatial Cartesian system and to the material cartesian system deﬁned on the middle surface are related by [ϕ ϕ 1 , ϕ 2 ] = ϕ ξ , ϕ η J−1 (34) The membrane strains within the central triangle are obtained using a linear assumed strain ﬁeld εˆm , i.e. εm = εˆm

(35)

Enhanced Rotation-Free Basic Shell Triangle

with εˆm = (1 − 2ζ)εε1m + (1 − 2ξ)εε2m + (1 − 2η)εε3m =

3

¯i ε i N m

247

(36)

i=1

where εim are the membrane strains computed at the three mid side points Gi ¯1 = (1 − 2ζ), etc. (i = 1, 2, 3 see Fig. 1). In Eq.(36) N The gradient at each mid side point is computed from the quadratic interpolation (30): ⎤ ⎡ 3 i i Nj,α ϕj ⎦ + Ni+3,α ϕi+3 , α = 1, 2 , i = 1, 2, 3 (ϕ ϕ α )Gi = ϕi α = ⎣ j=1

(37) Substituting Eq.(11) into (36) and using Eq.(9) gives the membrane strain vector as ⎧ i ⎫ 3 ϕ · ϕi − 1 ⎬ 1 ¯ ⎨ i1 i1 Ni ϕ · ϕ − 1 (38) εm = 2 ⎩ 2ϕi 2 i ⎭ i=1 2ϕ 1 · ϕ 2 and the virtual membrane strains as ⎧ ⎫ 3 ϕi 1 ϕi 1 · δϕ ⎨ ⎬ ¯i ϕi 2 ϕi2 · δϕ N δεεm = ⎩ i ⎭ ϕ 1 · ϕi 2 + ϕi 1 · δϕ ϕi2 i=1 δϕ

(39)

We note that the gradient at each mid side point Gi depends only on the coordinates of the three nodes of the central triangle and on those of an additional node in the patch, associated to the side i where the gradient is computed. Combining Eqs.(39), (37) and (30) gives δεεm = Bm δap with

δap 18×1

= [δuT1 , δuT2 , δuT3 , δuT4 , δuT5 , δuT6 ]T

(40a) (40b)

where δap is the patch displacement vector and Bm is the membrane strain matrix. An explicit form of this matrix is given in [26]. Note that the membrane strains within the EBST element are a function of the displacements of the six patch nodes. 3.2 Computation of Curvatures We will assume the following constant curvature ﬁeld within each element ˆ αβ καβ = κ

(41)

248

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

where κ ˆ αβ is the assumed constant curvature ﬁeld deﬁned by

1 t3 · ϕ βα dA0 κ ˆ αβ = − 0 AM A0M

(42)

where A0M is the area (in the original conﬁguration) of the central element in the patch. Substituting Eq.(42) into (41) and integrating by parts the area integral gives the curvature vector within the element in terms of the following line integral ⎫ ⎧ ⎡ ⎤

−n1 0 ⎨ κ11 ⎬ 1 t3 · ϕ 1 ⎣ ⎦ κ22 0 −n2 dΓ (43) = κ= t3 · ϕ 2 ⎭ A0M ΓM ⎩ 0 2κ12 −n2 −n1 where ni are the components (in the local system) of the normals to the 0 . The integration by parts of element sides in the initial conﬁguration ΓM Eq.(42) is typical in ﬁnite volume methods for computing second derivatives over volumes by line integrals of gradient terms [28,29]. For the deﬁnition of the normal vector t3 , the linear interpolation over the central element is used. In this case the tangent plane components are ϕ α =

3

LM i,α ϕ i

,

α = 1, 2

(44a)

i=1

t3 =

ϕ1 × ϕ2 = λ ϕ1 × ϕ2 |ϕ ϕ1 × ϕ2 |

(44b)

From these expressions it is also possible to compute in the original coni ﬁguration the element area A0M , the outer normals (n1 , n2 ) at each side and M the side lengths li . Equation (44b) also allows to evaluate the thickness ratio λ in the deformed conﬁguration and the actual normal t3 . The numerical evaluation of the line integral in Eq.(43) results in a sum over the integration points at the element boundary which are, in fact, the same points used for evaluating the gradients when computing the membrane strains. As one integration point is used over each side, it is not necessary to distinguish between sides (i) and integration points (Gi ). In this way the curvatures can be computed by ⎡ ⎤

3 −n1 0 1 M⎣ t3 · ϕ 1 ⎦ 0 −n2 dΓ (45) l κ= 0 t3 · ϕ 2 AM i=1 i −n2 −n1 Eq.(45) is now expressed in terms of the shape functions of the 3-noded triangle LM i (which coincide with the area coordinates [4]). Noting the property of the area coordinates

i

M liM Li,x nx M =− (46) ∇Li = LM 2AM niy i,y

Enhanced Rotation-Free Basic Shell Triangle

the expression for the curvature can be expressed as ⎡ M ⎤

Li,1 0 3 i M ⎦ t3 · ϕ 1 ⎣ 0 L κ=2 i,2 t3 · ϕi 2 M i=1 LM i,2 Li,1

249

(47)

The gradient ϕiα is evaluated at each side Gi from the quadratic interpolation ⎡ ⎤ ϕ1

i i i i i ⎢ ϕ2 ⎥ N1,1 N2,1 N3,1 Ni+3,1 ϕ1 ⎢ ⎥ = (48) i i i i ϕi2 N1,2 N2,2 N3,2 Ni+3,2 ⎣ ϕ3 ⎦ ϕi+3 This is a basic diﬀerence with respect of the computation of the curvature ﬁeld in the original Basic Shell Triangle (BST) where the gradient at the side mid-point is computed as the average value between the values at two adjacent elements [20, 23, 26, 27]. Note again than at each side the gradients depend only on the positions of the three nodes of the central triangle and of an extra node (i + 3), associated precisely to the side (Gi ) where the gradient is computed. Direction t3 in Eq.(47) can be seen as a reference direction. If a diﬀerent direction than that given by Eq.(44b) is chosen at an angle θ with the former, this has an inﬂuence of order θ2 in the projection. This justiﬁes Eq.(44b) for the deﬁnition of t3 as a function exclusively of the three nodes of the central triangle, instead of using the 6-node isoparametric interpolation. The variation of the curvatures can be obtained as ⎡ M ⎤ i Li,1 0 3 3 i Nj,1 Ni+3,1 (t3 · δui+3 ) (t3 · δuj ) M ⎦ ⎣ 0 Li,2 κ=2 + − δκ i i (t3 · δuj ) (t3 · δui+3 ) Nj,2 Ni+3,2 M i=1 i=1 LM L i,2 i,1 ⎤ ⎡ M 1 M 2 (L 3 i,1 ρ11 + Li,2 ρ11 ) 1 M 2 ⎦ (t3 · δui ) = Bb δap ⎣ (LM − (49) i,1 ρ22 + Li,2 ρ22 ) M 1 M 2 i=1 (Li,1 ρ12 + Li,2 ρ12 ) In Eq.(49) Bb = [Bb1 , Bb2 , · · · , Bb6 ]

(50)

Details of the derivation of the curvature matrix Bb are given in [26, 27]. 3.3 The EBST1 Element A simpliﬁed and yet very eﬀective version of the EBST element can be obtained by using one point quadrature for the computation of all the element integrals. This element is termed EBST1. Note that this only aﬀects the membrane stiﬀness matrices and it is equivalent to using a assumed constant membrane strain ﬁeld deﬁned by an average of the metric tensors computed at each side. Numerical experiments have shown that both the EBST and the EBST1 elements are free of spurious energy modes.

250

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

4 Boundary Conditions Elements at the domain boundary, where an adjacent element does not exist, deserve a special attention. The treatment of essential boundary conditions associated to translational constraints is straightforward, as they are the natural degrees of freedom of the element. The conditions associated to the normal vector are crucial in the bending formulation. For clamped sides or symmetry planes, the normal vector t3 must be kept ﬁxed (clamped case), or constrained to move in the plane of symmetry (symmetry case). The former case can be seen as a special case of the latter, so we will consider symmetry planes only. This restriction can be imposed through the deﬁnition of the tangent plane at the boundary, including the normal to the plane of symmetry ϕ0 n that does not change during the process. The tangent plane at the boundary (mid-side point) is expressed in terms of two orthogonal unit vectors referred to a local-to-the-boundary Cartesian system (see Fig. 2) deﬁned as 0 ¯ s (51) ϕ n , ϕ ¯ s emerges from where vector ϕ0 n is ﬁxed during the process while direction ϕ the intersection of the symmetry plane with the plane deﬁned by the central element (M ). The plane (gradient) deﬁned by the central element in the selected original convective Cartesian system (t1 , t2 ) is M ϕ 1 , ϕM (52) 2 the intersection line (side i) of this plane with the plane of symmetry can be written in terms of the position of the nodes that deﬁne the side (j and k) and the original length of the side liM , i.e. ϕi s =

1 ϕk − ϕj

(53)

liM

T

T

That together with the outer normal to the side ni = [n1 , n2 ] = [n · t1 , n · t2 ] (resolved in the selected original convective Cartesian system) leads to

iT iT ϕ 1 n1 −n2 ϕ n = (54) n2 n1 ϕiT ϕiT 2 s

where, noting that λ is the determinant of the gradient, the normal component of the gradient ϕi n can be approximated by ϕi n =

ϕ0 n ϕi s | λ|ϕ

(55)

For a simple supported (hinged) side, the problem is not completely deﬁned. The simplest choice is to neglect the contribution to the side rotations

Enhanced Rotation-Free Basic Shell Triangle symmetry plane

t0i3

i

t3 0

0

n=

ι =ϕ ’n ϕ ’n

ϕ ’n 0

s= k

251

j

ϕ ’s

M t1 t2 j

j Μ

i

ϕ ’s

k Z

k

i

Y

original

X

Μ

ϕ ’2

ϕ ’1 i deformed

Fig. 2. Local Cartesian system for the treatment of symmetry boundary conditions

from the adjacent element missing in the patch in the evaluation of the curvatures via Eq.(43) [20, 23, 26]. This is equivalent to assume that the gradient at the side is equal to the gradient in the central element, i.e. i M (56) ϕ 1 , ϕi 2 = ϕM 1 , ϕ 2 More precise changes can be however introduced to account for the diﬀerent natural boundary conditions. One may assume that the curvature normal to the side is zero, and consider a contribution of the missing side to introduce this constraint. As the change of curvature parallel to the side is also zero along the hinged side, this obviously leads to zero curvatures in both directions. We note ﬁnally that for the membrane formulation of element EBST, the gradient at the mid-side point of the boundary is assumed equal to the gradient of the main triangle. More details on the speciﬁcation of the boundary conditions on the EBST element can be found in [26, 27].

5 Explicit Solution Scheme For simulations including large non-linearities, such as those occuring in sheet metal forming processes involving frictional contact conditions on complex geometries or large instabilities, convergence is diﬃcult to achieve with implicit schemes. In those cases an explicit solution algorithm is typically most advantageous. This scheme provides the solution for dynamic problems and also for quasi-static problems if an adequate damping is chosen. The dynamic equations of motion to solve are of the form r(u) + Du˙ + M¨ u=0

(57)

where M is the mass matrix, D is the damping matrix and the dot means the time derivative. The solution is performed using the central diﬀerence method.

252

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

To make the method competitive a diagonal (lumped) M matrix is typically used and D is taken proportional to M. As usual, mass lumping is performed by assigning one third of the triangular element mass to each node in the central element. The explicit solution scheme can be summarized as follows. At each time step n where displacements have been computed: 1. Compute the internal forces rn . This follows the steps described in Box 1. 2. Compute the accelerations at time tn n ˙ n−1/2 ] ¨ n = M−1 u d [r − Du

(58)

where Md is the diagonal (lumped) mass matrix. 3. Compute the velocities at time tn+1/2 ¨ n δt u˙ n+1/2 = u˙ n−1/2 + u

(59)

4. Compute the displacements at time tn+1 un+1 = un + u˙ n+1/2 δt

(60)

5. Update the shell geometry 6. Check frictional contact conditions

6 Example 1. Cylindrical Panel under Impulse Loading The geometry of the cylinder and the material properties are shown in Fig. 3. A prescribed initial normal velocity of vo = −5650 in/sec is applied to the points in the region shown modelling the eﬀect of the detonation of an explosive layer. The panel is assumed to be clamped along all the boundary. One half of the cylinder is discretized only due to symmetry conditions. Three diﬀerent meshes of 6 × 12, 12 × 32 and 18 × 48 triangles were used for the analysis. The deformed conﬁgurations for time = 1msec are shown for the three meshes in Fig. 3. The analysis was performed assuming an elastic-perfect plastic material behaviour (σy = ky ky = 0). A study of the convergence of the solution with the number of thickness layers showed again that four layers suﬃce to capture accurately the non linear material response [25]. A comparison of the results obtained with the BST and EBST1 elements using the coarse mesh and the ﬁner mesh is shown in Fig. 4 where experimental results reported in [32] have also been plotted for comparison purposes. Good agreement between the numerical and experimental results is obtained. Figs. 4 show the time evolution of the vertical displacement of two reference points along the center line located at y = 6.28in and y = 9.42in, respectively. For the ﬁner mesh results between both elements are almost identical. For the coarse mesh it can been seen that the BST element is more ﬂexible than the EBST1.

Enhanced Rotation-Free Basic Shell Triangle

253

1. Generate the actual configuration ϕn+1 = ϕn + ∆un n+1 2. Compute the metric tensor an+1 αβ and the curvatures καβ . Then at each layer k compute the (approximate) right Cauchy-Green tensor. From Eq.(14) Cn+1 = an+1 + zk χn+1 (61) k 3. Compute the total (21) and elastic (22) deformations at each layer k εn+1 = k

1 ln Cn+1 k 2

(62)

n+1 n − [εεp ]k [εεe ]k = εn+1 k

4. Compute the trial Hencky elastic stresses (23) at each layer k n+1

Tn+1 = H [εεe ]k k

(63)

5. Check the plasticity condition and return to the plasticity surface. If necn+1 essary correct the plastic strains [εεp ]k at each layer 6. Compute the second Piola-Kirchhoff stress vector σ n+1 and the generalk ized stresses σ n+1 = m

NL h0 X σ n+1 wk k NL k=1

σ n+1 = b

NL h0 X σ n+1 zk wk k NL

(64)

k=1

Where wk is the weight of the through-the-thickness integration point. Recall that zk is the current distance of the layer to the mid-surface and not the original distance. However, for small strain plasticity this distinction is not important. This computation of stresses is exact for an elastic problem. 7. Compute the residual force vector from ZZ ZZ Li t dA − (BTmi σ m + BTbi σ b )dA (65) rei = A

A◦

Box 1. Computation of the internal forces vector

254

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3.0

10 .2 r v egio 03 0= n 36 w i n 50 it in h /s ec

h = 0.125 in

8 6

12.56

ky = 44 000 lb/in2 k’y = 0 lb/in2

R=2.9375 Z

2

E = 10.5 x 10 lb/in ρ = 2.5 x 104 lb sec2/in4 ν = 0.33

Y

X Z

Y X

Fig. 3. Cylindrical panel under impulse loading. Geometry and material properties. Deformed meshes for time = 1msec

1.4

1.2

Deflection [in]

1

0.8

0.6

0.4 Experimental BST mesh 3 EBST1 mesh 3 BST mesh 1 EBST1 mesh 1

0.2

0

0

0.2

0.4 0.6 Time [msec.]

0.8

1

Fig. 4. Cylindrical panel under impulse loading. Time evolution of the displacement of two points along the crown line. Upper lines y = 6.28in. Lower lines y = 9.42 in. Comparison of results obtained with BST and EBST1 elements (mesh 1: 6 × 12 elements and mesh 3: 18 × 48 elements) and experimental values

Enhanced Rotation-Free Basic Shell Triangle

255

The numerical values of the vertical displacement at the two reference points obtained with the BST and EBST1 elements after a time of 0.4 ms using the 16 × 32 mesh are compared in Table 2 with a numerical solution obtained by Stolarski et al. [31] using a curved triangular shell element and the 16 × 32 mesh. Experimental results reported in [32] are also given for comparison. It is interesting to note the reasonable agreement of the results for y = 6.28in. and the discrepancy of present and other published numerical solutions with the experimental value for y = 9.42in. Table 2. Cylindrical panel under impulse load. Comparison of vertical displacement values of two central points for t = 0.4 ms Vertical displacement (in.) element/mesh y = 6.28in y = 9.42in BST (6 × 12 el.) -1.310 -0.679 BST (18 × 48 el.) -1.181 -0.587 EBST1 (6 × 12 el.) -1.147 -0.575 EBST1 (18 × 48 el.) -1.171 -0.584 Stolarski et al. [31] -1.183 -0.530 Experimental [32] -1.280 -0.700

The deformed shapes of the transverse section for y = 6.28in. and the longitudinal section for x = 0 obtained with the both elements for the coarse and the ﬁne meshes after 1ms. are compared with the experimental results in Figs. 5 and 6. Excellent agreement is observed for the ﬁne mesh for both elements.

7 Application to Sheet Metal Forming Problems The features of tghe EBST1 element make it ideal for analysis of sheet metal stamping processes. A number of examples of simulations of practical problems of this kind are presented. Numerical results have been obtained with the sheet stamping simulation code STAMPACK where the EBST1 element has been implemented [35]. 7.1 S-rail Sheet Stamping The next problem corresponds to one of the sheet stamping benchmark tests proposed in NUMISHEET’96 [33]. The analysis comprises two parts, namely, simulation of the stamping of a S-rail sheet component and springback computations once the stamping tools are removed. Figure 7 shows the deformed sheet after springback.

256

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3

Z [in]

2

Original Experimental EBST1 mesh 1 BST mesh 1 EBST1 mesh 3 BST mesh 3

1

0

1

2

X [in]

Fig. 5. Cylindrical panel under impulse loading. Final deformation (t = 1msec) of the panel at the cross section y = 6.28in. Comparison with experimental values

Z-direction [in]

3

2

Experimental BST mesh 3 EBST1 mesh 3 BST mesh 1 EBST1 mesh 1

1

0

0

2

4

6

8

10

12

Y-direction [in]

Fig. 6. Cylindrical panel under impulse loading. Final deformation (t = 1msec) of the panel at the crown line (x = 0.00in). Comparison with experimental values

The detailed geometry and material data can be found in the proceedings of the conference [33] or in the web [34]. The mesh used for the sheet has 6000 triangles and 3111 points (Fig. 7). The tools are treated as rigid bodies.

Enhanced Rotation-Free Basic Shell Triangle

G"

257

Z

X

Y

B"

Fig. 7. Stamping of a S-rail. Final deformation of the sheet after springback obtained in the simulation. The triangular mesh of the deformed sheet is also shown

The meshes used for the sheet and the tools are those provided by the benchmark organizers. The material considered here is a mild steel (IF) with Young Modulus E = 2.06GP a and Poisson ratio ν = 0.3. Mises yield criterion was used for plasticity behaviour with non-linear isotropic hardening deﬁned by σy (ep ) = 545(0.13 + ep )0.267 [M P a]. A uniform friction of 0.15 was used for all the tools. A low (10kN) blank holder force was considered in this simulation. Figure 8 compares the punch force during the stamping stage obtained with both BST and EBST1 elements for the simulation and experimental values. Also for reference the average values of the simulations presented in the conference are included. Explicit and implicit simulations are considered as diﬀerent curves. There is a remarkable coincidence between the experimental values and the results obtained with both the BST and EBST1 elements. Figure 9 plots the Z coordinate along line B”–G” after springback. The top surface of the sheet does not remain plane due to some instabilities due to the low blank holder force used. Results obtained with the simulations compare very well with the experimental values. 7.2 Stamping of Industrial Automotive Part Figure 10 shows the geometry of the lateral panel of a car and the mesh of 457760 EBST1 elements used for the computation. Results of the stamping simulation are shown in Fig. 11. Note that the outpus of the simulation have been translated into graphical plots indicating the quality of the stamping process and the risk of failure in the diﬀerent zones of the panel. This helps designers to taking decissions on the adequacy of the stamping process and for introducing changes in the design of the stamping tools (dies, punch, blankholders, etc.) and the process parameters if needed. Figure 12 shows the geometry mesh and results of the stamping of a front fender part of an automotive. The initial mesh had 121960 EBST1 elements.

258

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

40

Punch Force [kN]

30

20

Experimental Explicit (average) Implicit (average) BST EBST1

10

0

0

10

20

30

40

Punch Travel [mm]

Fig. 8. Stamping of a S-rail. Punch force versus punch travel. Average of explicit and implicit results reported at the benchmark conference are also shown

Adaptive mesh reﬁnement was used along the simulation process leading to a ﬁnal mesh of 389870 elements. Finally, Figs. 13 and 14 show the same type of information for the stamping of a car tail gate. The initial and ﬁnal meshes (after adaptive mesh reﬁnement) had 186528 and 489560 EBST1 elements, respectively. The simulation results are displayed in both problems with an “engineering insight” in order to help the design and manufacturing of the stamping tools and the deﬁnition of the stamping process as previously mentioned.

8 Concluding Remarks An enhanced rotation-free shell triangle (termed EBST) is obtained by using a quadratic interpolation of the geometry in terms of the six nodes belonging to the four elements patch associated to each triangle. This allows to computing an assumed constant curvature ﬁeld and an assumed linear membrane strain ﬁeld which improves the in-plane behaviour of the original element. A simple and economic version of the element using a single integration point has been presented. The eﬃciency of the rotation-free shell triangle has been demonstrated in examples of application including the analysis of a cylinder under impulse loading and practical sheet stamping problems.

Enhanced Rotation-Free Basic Shell Triangle

259

Z coordinate[mm]

39

38

37 Experimental Explicit (average) Implicit (average) BST EBST1 36

0

50

100

150

200

250

distance [mm]

Fig. 9. Stamping of a S-rail. Z-coordinate along line B”—G” after springback. Average of explicit and implicit results reported at the benchmark conference are also shown

Fig. 10. Lateral panel of an automotive. Finite element mesh of 457760 triangles used for the simulation

260

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

Fig. 11. Lateral panel of a car. Results of the stamping analysis

The enhanced rotation-free basic shell triangle element with a single integration point (the EBST1 element) is an excellent candidate for solving practical sheet metal stamping problems and other non linear shell problems in engineering involving complex geometry, dynamics, material and geometrical non linearities and frictional contact conditions.

Enhanced Rotation-Free Basic Shell Triangle

261

Fig. 12. Front fender. Results of the stamping analysis using an initial mesh of 121960 EBST1 elements. The ﬁnal adapted mesh had 389870 elements

262

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

Fig. 13. Car tail gate. Geometry and ﬁnal adapted mesh of 489560 EBST1 elements used for the stamping simulation

ACKNOWLEDGEMENTS The support of the company QUANTECH (www.quantech.es) providing the code STAMPACK [35] is gratefully acknowledged. This research was partially supported by project SEDUREC of the Consolider Programme of the Ministerio de Educaci´ on y Ciencia of Spain.

Enhanced Rotation-Free Basic Shell Triangle

263

Fig. 14. Car tail gate. Map of relative thickness distribution and forming zones on the stamped part

References 1. O˜ nate E (1994) A review of some ﬁnite element families for thick and thin plate and shell analysis. Publication CIMNE N. 53, May 2. Flores FG, O˜ nate E, Z´ arate F (1995) New assumed strain triangles for non-linear shell analysis. Computational Mechanics 17:107–114

264

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3. Argyris JH, Papadrakakis M, Apostolopoulou C, Koutsourelakis S (2000) The TRIC element. Theoretical and numerical investigation. Comput Meth Appl Mech Engrg 182:217–245 4. Zienkiewicz OC, Taylor RL (2005) The ﬁnite element method. Solid Mechanics. Vol II, Elsevier 5. Stolarski H, Belytschko T, Lee S-H (1995) A review of shell ﬁnite elements and corotational theories. Computational Mechanics Advances vol. 2 (2), NorthHolland 6. Ramm E, Wall WA (2002) Shells in advanced computational environment. In V World Congress on Computational Mechanics, Eberhardsteiner J, Mang H, Rammerstorfer F (eds), Vienna, Austria, July 7–12. http://wccm.tuwien.ac.at. 7. Bushnell D, Almroth BO (1971) Finite diﬀerence energy method for non linear shell analysis. J Computers and Structures 1:361 8. Timoshenko SP (1971) Theory of Plates and Shells, McGraw Hill, New York 9. Ugural AC (1981) Stresses in Plates and Shells, McGraw Hill, New York 10. Nay RA, Utku S (1972) An alternative to the ﬁnite element method. Variational Methods Eng vol. 1 11. Hampshire JK, Topping BHV, Chan HC (1992) Three node triangular elements with one degree of freedom per node. Engng Comput 9:49–62 12. Phaal R, Calladine CR (1992) A simple class of ﬁnite elements for plate and shell problems. I: Elements for beams and thin plates. Int J Num Meth Engng 35:955–977 13. Phaal R, Calladine CR (1992) A simple class of ﬁnite elements for plate and shell problems. II: An element for thin shells with only translational degrees of freedom. Int J Num Meth Engng 35:979–996 14. O˜ nate E, Cervera M (1993) Derivation of thin plate bending elements with one degree of freedom per node. Engineering Computations 10:553–561 15. Brunet M, Sabourin F (1994) Prediction of necking and wrinkles with a simpliﬁed shell element in sheet forming. Int Conf of Metal Forming Simulation in Industry II:27–48, Kr¨ oplin B (ed) 16. Rio G, Tathi B, Laurent H (1994) A new eﬃcient ﬁnite element model of shell with only three degrees of freedom per node. Applications to industrial deep drawing test. In Recent Developments in Sheet Metal Forming Technology, Barata Marques MJM (ed), 18th IDDRG Biennial Congress, Lisbon 17. Rojek J, O˜ nate E (1998) Sheet springback analysis using a simple shell triangle with translational degrees of freedom only. Int J of Forming Processes 1(3):275– 296 18. Rojek J, O˜ nate E, Postek E (1998) Application of explicit FE codes to simulation of sheet and bulk forming processes. J of Materials Processing Technology 8081:620–627 19. Jovicevic J, O˜ nate E (1999) Analysis of beams and shells using a rotation-free ﬁnite element-ﬁnite volume formulation, Monograph 43, CIMNE, Barcelona 20. O˜ nate E, Z´ arate F (2000) Rotation-free plate and shell triangles. Int J Num Meth Engng 47:557–603 21. Cirak F, Ortiz M (2000) Subdivision surfaces: A new paradigm for thin-shell ﬁnite element analysis. Int J Num Meths in Engng 47:2039-2072 22. Cirak F, Ortiz M (2001) Fully C 1 -conforming subdivision elements for ﬁnite deformations thin-shell analysis. Int J Num Meths in Engng 51:813-833 23. Flores FG, O˜ nate E (2001) A basic thin shell triangle with only translational DOFs for large strain plasticity. Int J Num Meths in Engng 51:57–83

Enhanced Rotation-Free Basic Shell Triangle

265

24. Engel G, Garikipati K, Hughes TJR, Larson MG, Mazzei L, Taylor RL (2002). Continuous/discontinuous ﬁnite element approximation of fourth-order elliptic problems in structural and continuum mechanics with applications to thin beams and plates, and strain gradient elasticity. Comput Methods Appl Mech Engrg 191:3669–3750 25. O˜ nate E, Cendoya P, Miquel J (2002) Non linear explicit dynamic analysis of shells using the BST rotation-free triangle. Engineering Computations 19(6):662–706 26. Flores FG, O˜ nate E (2005) Improvements in the membrane behaviour of the three node rotation-free BST shell triangle using an assumed strain approach. Comput Meth Appl Mech Engng 194(6-8):907–932 27. O˜ nate E, Flores FG (2005) Advances in the formulation of the rotation-free basic shell triangle. Comput Meth Appl Mech Engng 194(21–24):2406–2443 28. Zienkiewicz OC, O˜ nate E (1991) Finite Elements vs. Finite Volumes. Is there really a choice?. Nonlinear Computational Mechanics. State of the Art. Wriggers P, Wagner R (eds), Springer Verlag, Heidelberg 29. O˜ nate E, Cervera M, Zienkiewicz OC (1994) A ﬁnite volume format for structural mechanics. Int J Num Meth Engng 37:181–201 30. Hill R (1948) A Theory of the Yielding and Plastic Flow of Anisotropic Metals. Proc Royal Society London A193:281 31. Stolarski H, Belytschko T, Carpenter N (1984) A simple triangular curved shell element. Eng Comput 1:210–218 32. Balmer HA, Witmer EA (1964) Theoretical experimental correlation of large dynamic and permanent deformation of impulsively loaded simple structures. Air force ﬂight Dynamic Lab Rep FDQ-TDR-64-108, Wright-Patterson AFB, Ohio, USA 33. NUMISHEET’96 Third International Conference and Workshop on Numerical Simulation of 3D Sheet Forming Processes, Lee EH, Kinzel GL, Wagoner RH (eds), Dearbon-Michigan, USA, 1996 34. http://rclsgi.eng.ohio-state.edu/%7Elee-j-k/numisheet96/ 35. STAMPACK. A General Finite Element System for Sheet Stamping and Forming Problems, Quantech ATZ, Barcelona, Spain, 2007. (www.quantech.es)

Computational Methods in Applied Sciences 1. 2. 3. 4. 5. 6.

7.

J. Holnicki-Szulc and C.A.M. Soares (eds.): Advances in Smart Technologies in Structural Engineering. 2004 ISBN 3-540-22331-2 J.A.C. Ambrósio (ed.): Advances in Computational Multibody Systems. 2005 ISBN 1-4020-3392-3 E. Oñate and B. Kröplin (eds.): Textile Composites and Inflatable Structures. 2005 ISBN 1-4020-3316-8 J.C. García Orden, J.M. Goicolea and J. Cuadrado (eds.): Multibody Dynamics. Computational Methods and Applications. 2007 ISBN 1-4020-5683-4 V.M.A. Leitão, C.J.S. Alves and C.A. Duarte (eds.): Advances in Meshfree Techniques. 2007 ISBN 1-4020-6094-6 C.A.M. Soares, J.A.C. Martins, H.C. Rodrigues and J.A.C. Ambrósio (eds.): Computational Mechanics. Solids, Structures and Coupled Problems. 2006 ISBN 978-1-4020-4978-1 E. Oñate and R. Owen (eds.): Computational Plasticity. 2007 ISBN 978-1-4020-6576-7

www.springer.com

Computational Methods in Applied Sciences Volume 7

Series Editor E. Oñate International Center for Numerical Methods in Engineering (CIMNE) Technical University of Catalunya (UPC) Edificio C-1, Campus Norte UPC Gran Capitán, s/n 08034 Barcelona, Spain [email protected] www.cimne.com

Computational Plasticity Edited by

Eugenio Oñate Universitat Politècnica de Catalunya, Barcelona, Spain and

Roger Owen University of Wales, Swansea, United Kingdom

A C.I.P. Catalogue record for this book is available from the Library of Congress.

ISBN 978-1-4020-6576-7 (HB) ISBN 978-1-4020-6577-4 (e-book) Published by Springer, P.O. Box 17, 3300 AA Dordrecht, The Netherlands. www.springer.com

Printed on acid-free paper

All Rights Reserved © 2007 Springer No part of this work may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, microfilming, recording or otherwise, without written permission from the Publisher, with the exception of any material supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work.

Table of Contents

Preface . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . vii A Multi-Scale Continuum Theory for Heterogeneous Materials F. Vernerey, C. McVeigh, W.K. Liu and B. Moran . . . . . . . . . . . . . . . . . . . . .1 Towards a Model for Large Strain Anisotropic Elasto-Plasticity F.J. Mont´ ans and K.J. Bathe . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 13 Localized and Diﬀuse Bifurcations in Porous Rocks Undergoing Shear Localization and Cataclastic Flow R.I. Borja . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 37 Dispersion and Localisation in a Strain-Softening Two-Phase Medium R. de Borst and M.-A. Abellan . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 55 New Developments in Surface-to-Surface Discretization Strategies for Analysis of Interface Mechanics T.A. Laursen and B. Yang . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 67 Particle Finite Element Methods in Solid Mechanics Problems J. Oliver, J.C. Cante, R. Weyler, C. Gonz´ alez and J. Hern´ andez . . . . . . 87 Micro-Meso-Macro Modelling of Composite Materials P. Wriggers and M. Hain . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 105 Numerical Modeling of Transient Impact Processes with Large Deformations and Nonlinear Material Behavior E. Ramm, T. Erhart and W.A. Wall . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 123 A Computational Model For Viscoplasticity Coupled with Damage Including Unilateral Eﬀects D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto . . . . . . . . . 145

v

vi

Table of Contents

On Multiscale Analysis of Heterogeneous Composite Materials: Implementation of Micro-to-Macro Transitions in the Finite Element Setting D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .165 Assessment of Protection Systems for Gravel-Buried Pipelines Impact and Recurrent Shear Loading Caused by Considering Thermal Deformations of the Pipe B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 187 Enriched Free Mesh Method: An Accuracy Improvement for Node-based FEM G. Yagawa and H. Matsubara . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .207 Modelling of Metal Forming Processes and Multi-Physic Coupling J.-L. Chenot and F. Bay . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 221 Enhanced Rotation-Free Basic Shell Triangle. Applications to Sheet Metal Forming E. O˜ nate, F.G. Flores and L. Neamtu . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 239

Preface

This book contains state of the art contributions in the ﬁeld of computational plasticity. This topic encompasses a wide spectrum of areas in non-linear computational solid mechanics and modelling of materials and their industrial applications. Despite the apparent activity in the ﬁeld, the ever increasing rate of development of new engineering materials required to meet advanced technological needs poses fresh challenges in the ﬁeld of constitutive modelling. The complex behaviour of such materials demands a closer interaction between numerical analysts and material scientists in order to produce thermodynamically consistent models which provide a response in keeping with fundamental micromechanical principles and experimental observations. This necessity for collaboration is further highlighted by the continuing remarkable developments in computer hardware which makes the numerical simulation of complex deformation responses increasingly possible. The book contains 14 invited contributions written by distinguished authors who participated in the VIII International Conference on Computational Plasticity held at CIMNE/UPC (www.cimne.com), Barcelona, Spain, from 5th to 8th September 2005. The meeting was one of the Thematic Conferences of the European Community on Computational Methods in Applied Sciences (ECCOMAS, www.eccomas.org). The diﬀerent chapters of this book present recent progress and future research directions in the ﬁeld of computational plasticity. A common line of many contributions is that a stronger interaction between the phenomenological and micromechanical modelling of plasticity behaviour is apparent and the use of inverse identiﬁcation techniques is also more prominent. The development of adaptive strategies for plasticity problems continues to be a challenging goal, while it is interesting to note the permanence of element modelling as a research issue. Industrial forming processes, geomechanics, steel and concrete structures form the core of the applications of the diﬀerent numerical methods presented in the book. The book includes contributions sent directly by the authors and the editors cannot accept responsibility for any inaccuracies and opinions contained in the text. vii

viii

Preface

The editors would like to take this opportunity for thanking all authors for submitting their contributions. We also express our gratitude to Maria Jes´ us Samper from CIMNE for her excellent work in the edition of this volume. Many thanks ﬁnally to ECCOMAS and Springer for accepting the publication of this book. Eugenio O˜ nate Universitat Polit`ecnica de Catalunya Barcelona, Spain

Roger Owen University of Wales Swansea, United Kingdom

A Multi-Scale Continuum Theory for Heterogeneous Materials Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran Department of mechanical engineering, Northwestern University, 2145 Sheridan Road, Evanston, IL 60208-3111, USA [email protected]

Summary. For the design of materials, it is important to faithfully model the physics due to interactions at the microstructural scales [18, 17, 19]. While bruteforce modeling of all the details of the microstructure is too costly, current homogenized continuum models suﬀer from their inability to suﬃciently capture the correct physics - especially where localization and failure are concerned. To overcome this limitation, a multi-scale continuum theory is proposed so that kinematic variables representing the deformation at various scales are incorporated. The method of virtual power is then used to derive a system of coupled governing equations, each equation representing a particular scale and its interactions with the macro-scale. A constitutive relation is then introduced to preserve the underlying physics associated with each scale. The inelastic behavior is represented by multiple yield functions, each representing a particular scale of microstructure, but collectively coupled through the same set of internal variables. The proposed theory is applied to model porous metals and high strength steel. For the high strength steel the microstructure of interest consists of two populations of inclusions at distinct scales, in an alloy matrix.

1 Multi-Physics Multi-Scale Material Model 1.1 Kinematics and Virtual Power In the spririt of the work performed by Cosserat [2], Mindlin [11] and Germain [10], the building blocks of the multi-scale continuum theory are a set of kinematic variables which represent the motion within the material’s microstructure. These variables can capture the heterogeneous deformation due to the micro-mechanisms occuring at each scale. For an N-scale material, in addition to the macro-velocity ﬁeld v we introduce N-1 independent micro velocity gradients LI 1≤I≤N −1 . In the context of a ﬁrst gradient theory, the internal virtual power density is written as a linear combination of the various

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 1–11. © 2007 Springer. Printed in the Netherlands.

2

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

kinetic variables and their gradients. Integrating over the body Ω, the virtual internal power is written as:

N −1 I. I − I I← . σ : δD + β : δL − δL + β . δL ∇ δPint = dΩ. (1) Ω

I=1 I

I

where σ is the Cauchy stress, β is the Ith micro-stress and β is the Ith microstress couple. The Ith micro-stresses are interpreted as a stress redistribution arising from the presence of heterogeneities within the Ith microstructure. The kinetic virtual power, external virtual power, governing equations and boundary conditions can be found here [4]. 1.2 Constitutive Relation For convenience, we introduce the generalized stress Σ and strain D measures in a vector form containing the components of the macroscopic quantities as well as the various microscopic quantities deﬁned in the previous section. Hence, we write: 1 N −1 . Σ = σ β 1 β · · · β N −1 β

1 1←

N −1 − ← − D = D L − L L ∇ ··· L − L LN −1 ∇ . The generalized rate of deformation D is decomposed into an elastic part De and a plastic part Dp : (2) D = De + Dp . In the elastic regime, it is possible to introduce a generalized elastic matrix C such that the generalized stress increment Σ is related to the elastic part of the rate of deformation De as follows: Σ = C · De

(3)

where Σ is an objective stress rate. The plastic response is written in a multi-physics plastic potential framework. We introduce a yield function φI with the Ith micro-scale of interest. The plastic ﬂow at each scale is determined from the corresponding yield function in the context of associative plasticity.

2 Application to Porous metals Substantial eﬀort has been dedicated to the study and development of micromechanical models applicable to the plastic deformation and failure of porous metals. Two distinct mechanisms contribute to failure. The ﬁrst stage involves the independent growth of voids subject to a remote hydrostatic stress. The

A Multi-Scale Continuum Theory for Heterogeneous Materials

3

Fig. 1. Multi-scale decomposition for a two-scale porous material

second occurs when the voids a large enough to trigger a necking instability of the inter-void ligament. The second stage of failure is therefore characterized by an acceleration in the loss of load carrying capacity of the material as void coalescence occurs. The use of traditional continuum methods to treat failure of porous metals is limited due to their inability to handle localization problems. To overcome this problem, the outlined multi-scale continuum theory is used to describe the response of porous metals after the onset of localization. The additional degrees of freedom introduced through the microﬁelds can represent the inhomogeneous strains arising due to void interactions and coalescence. 2.1 Multi-Scale Model The multiscale description of porous metal is based on the deﬁnition of two domains, representing the micro- and macro-scales, respectively (Fig. 1) The kinematics are expressed in terms of the velocity v associated with the macro-scale and the rate of micro-deformation D1 . The generalized stress and rate of deformation for the two-scale porous metal can therefore be written as: 1 1 1 ← − D= D D −D D1 ∇ , (4) Σ= σ β β , where D is the symmetric part of the macro-velocity gradient, σ is the macro1

1

stress, and β and β are the micro-stress and micro-stress couple, respectively. From (1), the internal power is written as: 1. 1 ← − σ : δD + β : δD1 − δD + β .. δD1 ∇ dΩ. (5) δPint = Ω

4

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

A physical interpretation is provided as follows: the macro-stress σ represents the macroscopic response that undergoes a loss of load carrying capacity due 1 to void growth and coalescence. The presence of the micro-stress β represents the stress redistributions around voids as they grow. It provides a resistance of the matrix material to highly localized deformations. 2.2 Constitutive Relation 1

1

A two-potential plasticity model with yield functions Φ(σ) and Φ1 (β , β ) is employed to represent the material plastic behavior at the macro and microscale, respectively. Homogenization is performed over two averaging domains (macro and meso) as described. The macro-stress σ is determined by an av¯ (macro domain). The macroscopic plastic eraging operation over the RVE Ω deformation is based on an extension of the von-Mises plasticity model that incorporates the eﬀects of the porosity f . A standard yield function accounting for softening mechanisms due to void growth is given as follows: Φ = Φ (σ, f, ε) = 0,

(6)

where the material constants which appear in the function Φ are determined through cell modeling computer simulations. Microscopic plastic deformation is deﬁned as the plastic deformation of the matrix material after the onset of void coalescence. The plastic model is taken in the form of J2 ﬂow plasticity modiﬁed to account for the eﬀects of higher order stress. The microscopic yield function Φ1 is given by: 1

1

Φ1 = Φ1 (β , β , E 1 )

(7)

where E 1 is the microscopic eﬀective plastic strain. 2.3 Numerical Results We multi-scale model is now implemented and compared to a direct numerical sumilation (DNS) of a porous metal bar loaded in tension. In the DNS, the explicit microstructure is represented by a periodic distribution of circular voids of diameter 1µm and volume fraction 3%. An imperfection is introduced by making the void in the center of the specimen slightly larger than others. As localization is expected to occur around the imperfection, voids are only modeled in the central region. For the two-scale continuum simulation, the ﬁnite element discretisation is ﬁne enough to capture size eﬀects at the scale of the voids. An imperfection, in the form of a higher initial average porosity, is introduced in the center of the specimen to initiate localization. The comparison of the macroscopic plastic strain distribution for the DNS and the two-scale continuum is depicted in Fig. 2. The results are displayed at four diﬀerent times t1 , t2 , t3 and t4 . At time t = t1 , the material response reaches

A Multi-Scale Continuum Theory for Heterogeneous Materials

5

Fig. 2. Snapshots of the distribution of equivalent plastic strain in a specimen in tension for (a) the explicit microstructure (b) the equivalent two-scale continuum

Fig. 3. Comparison of the distribution of plastic strain for (a) the explicit microstructure (b) the two-scale material (c) conventional continuum model (one-scale porous model)

the macroscopic instability point (softening of the macroscopic constitutive relation due to void growth), and deformation localizes in a shear band at 45 1

1

degrees to the tensile direction. The micro-stresses β and β act to stabilize the void growth at time t = t2 . The onset of void coalescence occurs at time t = t3 in a plane perpendicular to the loading direction. This mechanism is modeled by a yielding of the micro-stresses and therefore a decrease in resistance to micro-deformation. Consequently, a plane of highly localized plastic

6

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

strain arises in the horizontal direction as shown at time t4 . The behavior of the two-scale continuum compares well with the behavior of the explicit microstructure. The main attraction of the two-scale continuum resides in the gain of computational time. For instance, the typical element size for the twoscale model is ten times as large as that used for the DNS (1 µm and 0.1 µm respectively).

3 Three-scale Model of High-Strength Steels In the previous example, two scales of analysis where considered. Physically speaking, these were the average macroscale behavior of a population of voids and the microscale behavior deﬁned by the coalescence between neighboring voids. We now consider a material in which three distinct scales can be considered. In high strength steels, previously examined within the hierarchical methodology [14, 12, 13, 15, 16, 3], the embedded particles are divided into two groups: the primary particles with the diameter around microns and the secondary particles in the range of 10 to 100 nanometers. By adding alloys during metallurgical processes, the desirable dispersed secondary particles, such as M2C carbides, are formed through precipitation or dissolved from primary particles, which blocks the dislocation path; thus, the strength of steel rise. Whereas the primary particles, such as nitrides, usually have lower toughness as compared with the iron matrix. The formation of primary particles is inevitable during manufacture process. A key-issue in steel design is to establish the relationships between the micro/nano-structures of steel and its macro-scale mechanical properties. To this end, we use the proposed multiscale continuum theory. Three mechanisms are considered here: (i)the failure at the level of primary particles, (ii) the failure at the level of secondary particles and (iii) the failure by necking of the ligaments between micro-voids [1]. 3.1 Multi-Scale Model The three levels of microstructure are shown in Fig. 4. The macro-scale contains primary particles (large square particles) and secondary particles (small circular particles). The micro-scale contains only secondary particles and the sub-micro scale represents the matrix material. Following the framework described before, we introduce the macro-velocity v, the micro-velocity gradient D1 and the sub-micro velocity gradient D2 . The internal power for a three scale material is written as: 1. 1 ← − δPint = σ : δD + β : δD1 − δD + β .. δD1 ∇ Ω 2. 2 ← − (8) + β : δD2 − δD + β .. δD2 ∇ dΩ.

A Multi-Scale Continuum Theory for Heterogeneous Materials

7

Fig. 4. Proposed multi-scale framework for the modelling of high strength steel

A physical interpretation of the various terms can be given as follows. The quantity D1 − D is the inhomogeneous deformation resulting from the localization that occurs from the nucleation of large voids (from primary particles) and the inhomogeneous deformation D2 − D is the result of the localization that occurs from nucleation of micro-voids (from secondary particles). The micro-stress at a scale is interpreted as the stress exerted by the microstructure to redistribute plastic deformation around the voids at that scale. 3.2 Constitutive Relation The failure of High Strength Steels involves mechanisms which involve the microstructure at each scale. Three yield functions are introduced: the macro1

1

potential Φ(σ) and the ﬁrst and second micro-potential Φ1 (β , β ) and 2

2

Φ2 (β , β ), respectively. Each of the above functions is associated with a failure mechanism summarized as follows: (i) void nucleation and growth at primary particles followed by strain localization of width approximately equal to the diameter of a ’primary’ void. (ii) void nucleation and growth at primary particles followed by strain localization of width approximately equal to the diameter of a ’secondary’ void. (iii) secondary-void coalescence by necking of the inter-void ligament and localization of the deformation in the neck. The macroscopic yield function Φ describes the evolution of the macro-stress and plastic strains. It represents the plastic deformation and response of the RVE and can be derived within the hierarchical methodology. The form of the constitutive relation at the macro-scale is such that: Φ = Φ (σ, f, ε)

(9)

where f and ε are the porosity and eﬀective plastic strain, respectively. This function accounts for the loss of load carrying capacity of the material due to

8

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

the cumulative eﬀects of void nucleation, growth and coalescence from both the primary and secondary particles. 1

1

The micro-stresses (β , β ) are the local stress and moment generated in the matrix by larger voids as they grow. When the matrix material fails, the microcouple and micro-stress can no longer be sustained to the same extent i.e. they yield. The yielding point of the micro-stress is controlled by the degradation and strain localization in the material between the primary particles, which is driven by the formation of a void sheet mechanism originating at the scale of the secondary particles. The microscopic plastic deformation is therefore a function of the nucleation and growth of secondary particle nucleated voids (void sheet). As such, volumetric deformation must be accounted for. A simple model can be developed in the form of a Drucker-Prager plasticity model, modiﬁed to account for the eﬀects of higher order stress. It is written in the form: 1 1 (10) Φ1 = Φ1 (β , β , E 1 ) where E 1 is the microscopic eﬀective plastic strain. The submicro-stresses provide a measure of the local stress distribution around the secondary particle nucleated voids during void growth. This mechanism is similar to that described in the previous section for porous materials. The yielding point of the submicro-stresses corresponds to the inability of the matrix material to transmit stress moments after ligament instability. Submicroscopic plastic deformation is subsequently deﬁned as the plastic deformation of the matrix material after the onset of void coalescence (necking of the ligament). The yield function is written in the form of a plasticity model modiﬁed to account for the eﬀects of higher order stress: 2

2

Φ2 = Φ2 (β , β , E 2 )

(11)

where E 2 is the sub-microscopic eﬀective plastic strain. 3.3 Numerical Results A two-dimensional plane strain analysis of a shear test was employed to evaluate the performance of the three-scale material model in shear. The behavior of high strength steel in pure shear has been investigated experimentally by Cowie et al. [5]. Two computations are performed here: (a) direct numerical simulation (DNS) of the shear test with explicit modeling of particles and (b) a computation of the same model using the three-scale steel model. A comparison is then drawn between the two simulations. The stages of shear failure are explained as follows. (a) Debonding of primary particles, and strain localization between the primary particle nucleated voids. In the multi-scale model this corresponds to the yielding of the macro-stress and the formation of a shear band of

A Multi-Scale Continuum Theory for Heterogeneous Materials

9

Fig. 5. Contours of eﬀective plastic strain at diﬀerent stages of deformation

width related to the primary particle size. During this stage the microstress remains in the elastic regime and is responsible for sustaining the observed size eﬀect. (b) Shear driven nucleation and growth at the scale of the secondary particles leads to a terminal shear instability. In the multi-scale simulation this mechanism is modeled through the yielding of the micro-stress. The size eﬀect resulting from the micro-stress can no longer be sustained. The formation of a shear band of width related to the secondary particle size is then observed. This size eﬀect arises from the existence of a sub-microstress that remains in the elastic regime. (c) As deformation increases, coalsecence of secondary particle nucleated voids will occur, leading to a rapid decrease in the load carrying capacity of the material. In the multiscale model this is captured through a yielding of the sub-microstress. No size eﬀect is then captured. This is consistent with the ﬁnal failure of a material.

4 Conclusion The outlined multiscale model oﬀers several advantages over traditional continuum theory. It can be used to model a material which contains an arbitrary number of scales of microstructure. The internal interactions in the microstructure and the resulting size eﬀects can be accounted for at each scale within the mathematical framework. The mechanisms resulting in heterogeneous deformation at each scale are modeled individually through the

10

Franck Vernerey, Cahal McVeigh, Wing Kam Liu and Brian Moran

introduction of mutliple plastic potentials, while being coupled through the internal state variables. This theory has been successfully applied to describe the behavior of a porous metal and a high strength steel. This multi-scale framework has been successfully used in [4] to capture the fracture toughness of a high strength steel in terms of the underlying microstructure. Improvements in eﬃcency may be possible by employing the Bridging Scale Method [7, 8, 9, 6].

Acknowledgements The authors gratefully acknowledge the support of the ONR D3D Digital Structure Consortium (award N00014-05-C-0241) and the National Science Foundation.

References 1. McVeigh C, Vernerey F, Liu WK, Moran B and Olson GB (2006) An interactive microvoid shear localization mechanism in high strength steels. Submitted to Journal of Mechanics and Physics of Solids 2. Cosserat E and Cosserat F (1909) Theorie des corps deformables. Paris: A Hermann et Fils 3. Horstemeyer MF, Lathrop J, Gokhale AM and Dighe M (2000) Modeling stress state dependent damage evolution in a cast al-si-mg aluminium ally. Theoretical and applied fracture mechanics 33:31–47 4. Vernerey FJ (2006) Multi-Scale Continuum theory for material with microstructure. PhD thesis, Northwestern University 5. Cowie JG, Azrin M and Olson GB (1989) Microvoid formation during shear deformation of ultrahigh strength steels. Metallurgical transactions 20A:143– 153 6. Wagner G, Karpov EG and Liu Wing Kam (2004) Molecular dynamics boundary conditions for regular crystal lattices. Computer Method in Applied Mechanics and Engineering 193:1579–1601 7. Kadowaki H and Liu WK (2004) Bridging multi-scale method for localization problems. Computer Methods in Applied Mechanics and Engineering 193:3267– 3302 8. Kadowaki H and Liu WK (2005) A multiscale approach for the micropolar continuum model. Computer modeling in Engineering and Science 7:269–282 9. Wagner GJ and Liu WK (2003) Coupling of atomistic and continuum simulations using a bridging scale decomposition. Journal of Computational Physics 190:249–274 10. Germain P (1973) The method of virtual power in continuum mechanics. part 2 microstructure. SIAM Journal of Applied Mathematics 25:556–575 11. Mindlin RD (1964) Micro-structure in linear elasticity. Arch. Ration. Mech. Anal 16:15–78

A Multi-Scale Continuum Theory for Heterogeneous Materials

11

12. Hao S, Moran B, Liu WK and Olson GB (2003) A hierarchical multi-physics constitutive model for steels design. Journal of Computer-Aided Materials Design 10:99–142 13. Hao S, Liu WK and Chang CT (2000) Computer implementation of damage models by ﬁnite element and meshfree methods. Computer methods in Applied Mechanics and Engineering 187:401–440 14. Hao S, Liu WK, Moran B, Vernerey F and Olson GB (2004) Multiple-scale constitutive model and computational framework for the design of ultra-high strength, high toughness steels. Comput. Methods Appl. Mech. Engrg 193(1720):1865–1908 15. Tvergaard V (1982) Ductile fracture by cavity nucleation between larger voids. J. Mech. Pys. Solids 30:265–286 16. Tvergaard V (1988) 3d-analysis of localization failure in a ductile material containing two size-scales of spherical particles. Engineering Fracture Mechanics 31:421–436 17. Liu WK, Karpov EG and Park HS (2005) Nano Mechanics and Materials: Theory, Multiscale Methods and Applications, Wiley 18. Liu WK, Karpov EG, Zhang S and Park HS (2004) An introduction to computational nanomechanics and materials. Computer Methods in Applied Mechanics and Engineering 193:1529–1578 19. Liu WK, Hao S, Vernerey FJ, Kadowaki H, Park H and Qian D (2003) Multiscale analysis and design in heterogeneous system. VII International Conference on Computational Plasticity (COMPLAS VII) 7

Towards a Model for Large Strain Anisotropic Elasto-Plasticity F.J. Mont´ ans1 and K.J. Bathe2 1

2

Universidad de Castilla-La Mancha. E.T.S. de Ingenieros Industriales C/ Camilo Jos´e Cela s/n. 13071-Ciudad Real. Spain. [email protected] Massachusetts Institute of Technology. Dept. of Mechanical Engineering 77 Massachusetts Avenue. Cambridge, U.S.A. [email protected]

Summary. The modeling of large strain anisotropic elasto-plasticity requires that the elastic response can be anisotropic, the yielding is governed by anisotropic yield functions, the hardening is anisotropic and the principal anisotropic elastic and yield directions can align themselves to more favorable stress directions during the response. For general ﬁnite element analysis, the model also needs to be macroscopically-based and computationally eﬀective. We have worked towards such a model based on using the decomposition of the deformation gradient into elastic and plastic parts, logarithmic strains, exponential mapping and the plastic spin as an internal variable. The objective of this presentation is to give basic theoretical considerations and a computational framework for this anisotropic elasto-plasticity model. We also present some numerical results.

1 Introduction Computational large strain plasticity is now well established for the case of isotropic elasto-plasticity, see for example References [1–4]. In these formulations, the use of hyperelasticity [5] was important both conceptually —to not dissipate energy during elastic cycles, see Reference [6]— and algorithmically —to avoid the integration of objective stress rates. Also, the use of the Lee multiplicative decomposition of the deformation gradient into an elastic and a plastic part [7, 8] —previously used by Bilby et al. [9]— and the formulation of the incremental equations in terms of logarithmic strains and Kirchhoﬀ stresses resulted into a remarkable simplicity for the computational return mapping algorithm [10, 11]. Indeed, the backward integration of the rate equation, via the exponential product formula, rendered the incremental algorithm in the logarithmic strain space identical to the small strain return mapping algorithm. This simplicity allowed for an extension of both the theory and the algorithm to anisotropic mixed hardening [11]. Both “unrotated” [10, 11] and spatial formulations and algorithms followed, sometimes formulated in the principal stress/strain space [12, 13]. Of course, all these formulations are Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 13–36. © 2007 Springer. Printed in the Netherlands.

14

F.J. Mont´ ans and K.J. Bathe

completely equivalent, see Reference [14]. However, if kinematic hardening is considered, special care must be used because some plastic spin eﬀects may be inadvertently introduced, resulting in completely diﬀerent response predictions, see Reference [15]. Alternatively, a special but not standard type of kinematic hardening may be considered [16]. Computational plasticity formulations based on logarithmic strains and work-conjugate stresses have now been used extensively and have also been extended successfully to applications in soil mechanics, see Reference [17]. Common to the diﬀerent formulations are the following ingredients: isotropic hyperelasticity, exponential mapping and the additive return in the logarithmic strain space. In this framework, the algorithm of Eterovi´c and Bathe [11] seems to be the ﬁrst implicit algorithm to allow for some anisotropy. This anisotropy is given by the kinematic hardening rule. The algorithm is consistently linearized in Reference [15], where it is noted that anisotropic yield functions may be directly employed in the formulation. However, all the large strain computational plasticity algorithms based on logarithmic strains are using one hypothesis: the elastic strains and the work-conjugate stress measures commute. This property only holds in isotropic elasticity and hence the previous formulations are not applicable in anisotropic elasticity. While some publications appeared recently on computational anisotropic plasticity, see for example [18–21], the published algorithms are not developed following the successful framework of using the deformation gradient decomposition into an elastic and a plastic part, logarithmic strains and exponential mapping. In many cases the eﬀect of the elastic anisotropy is considerably smaller than the eﬀect of the plastic anisotropy and, hence, elastic isotropy is assumed with an anisotropic yield function, see for example Reference [22]. The algorithm presented in [15] is then directly applicable. An important observation discussed in this reference is that, then, the plastic spin does not enter in the dissipation equation and as a consequence, any plastic rotation is possible. Hence, a constitutive hypothesis may be chosen. However, for general anisotropic elasto-plasticity the plastic spin requires special attention. In order to understand the nature and practical eﬀects of the plastic spin, researchers have proposed several ad-hoc constitutive equations, see for example [23–31]. A possible eﬀect of the plastic spin is to cause rotations of the elastic and plastic anisotropy directions during loading. These rotations take place at diﬀerent strain levels depending on the type of material considered [22], as observed and measured experimentally, see References [32–36]. Some materials preserve an almost isotropic elastic behaviour as aluminum [37, 38], and also only show a small rotation of the preferred plasticity orthotropy directions [22, 34, 35]. In these References, approximately 5o of rotation is measured for 20% of strains. Other metals such as steel contain both a substantial elastic and plastic anisotropy and show a signiﬁcant rotation of the orthotropy directions, see References [32, 33, 36]. In these works a realignment of the anisotropy

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

15

directions in steel sheets to new directions during the loading is experimentally observed for strain levels of about 10%. Considering a thermodynamical framework of continua, it seems natural to relate the development of these rotations to the plastic ﬂow and to a decrease of the stored energy. In the following sections we present a model and an algorithm to describe the plastic behaviour of metals with both elastic and plastic anisotropies, and consider the rotation of the elastic and plastic anisotropy directions. This theory is an extension of the formulation presented in References [11] and [15]. The theory employs the multiplicative decomposition of the deformation gradient, logarithmic strain measures, the exponential mapping formula and the plastic spin to govern the rotations of the elastic and plastic anisotropy directions.

2 Kinematics and Incremental Integrations In the derivation of the continuum formulation and the algorithm for the stress calculation we follow the notation used in References [1], [2] and [39]. We include in this section both the continuum and algorithmic formulations since they are closely related. 2.1 Kinematics of Deformation: Multiplicative Decomposition and Strain Rate Tensors The Lee decomposition yields the following multiplicative decomposition for the deformation gradient t 0X

=

p(t) t 0 X p(t) X

:=

e t p t 0X 0X

(1)

where, conceptually, p (t) is a conﬁguration with the elastic strains relaxed p(t) t X ≡ t0 X e and 0 X ≡ t0 X p . Of course (stress-free conﬁguration). Hence, p(t) the decomposition of Equation (1) is unique if t0 X p is known, for example, via the integration of the plastic path. The spatial velocity gradient t l = ∂ t v/∂ t x, where t v ( t x) is the time derivative of the displacements, is t

l=

−1 t ˙ t 0X 0X

(2)

and its symmetric part, the spatial deformation rate tensor, is t T t d = 12 t0 X˙ 0 X −1 + t0 X −T t0 X˙

(3)

In view of Eq.(1), Eq.(2) can be decomposed as p e −1 −1 −1 l = le + lp = X˙ (X e ) + X e X˙ (X p ) (X e )

(4)

16

F.J. Mont´ ans and K.J. Bathe

In the equations to follow we frequently omit the time left-indices when a confusion is hardly possible. The tensor p

−1

Lp := X˙ (X p )

(5)

is the modiﬁed plastic velocity gradient. The tensor Lp operates in the intermediate stress-free conﬁguration. The symmetric part of Lp is the modiﬁed plastic deformation rate tensor p pT −1 −T (6) D p := 12 X˙ (X p ) + (X p ) X˙ while its skew part is the modiﬁed plastic spin. p pT −1 −T W p := 12 X˙ (X p ) − (X p ) X˙

(7)

On the other hand, if we deﬁne L, the modiﬁed velocity gradient as the pull-back of l to the intermediate conﬁguration, we arrive at L = Le + C e Lp

(8)

where C e ≡ X e T X e is the right Cauchy-Green deformation tensor in the stress-free conﬁguration. Note that some of our deﬁnitions diﬀer from those sometimes found in the literature. For example D p is sometimes deﬁned as D p = sym (C e Lp ), see for example [40–42]. 2.2 Integration of the Plastic Deformation Gradient This section follows the same procedure presented in Reference [15]. From Equation (5), the evolution of the plastic deformation gradient tensor is given by the diﬀerential equation t ˙p 0X

= t Lp t0 X p

(9)

whose backward-Euler exponential solution is given by t p p t+∆t t+∆t p L (10) 0X 0 X = exp ∆t where the exponentialfunction of a matrix exp ∆t t+∆t Lp for small steps such that ∆t t+∆t Lp 1 can be approximated by (11) exp ∆t t+∆t Lp I + ∆t t+∆t Lp Using ∆t

t+∆t

Lp = ∆t

t+∆t

D p + ∆t

t+∆t

Wp

we have that for small steps the following property holds exp ∆t t+∆t Lp exp ∆t t+∆t D p exp ∆t t+∆t W p

(12)

(13)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

yielding the following update formulas: p −1 t+∆t = t0 X p −1 exp −∆t t+∆t W p exp −∆t t+∆t D p 0X e e t+∆t t+∆t W p exp −∆t t+∆t D p 0 X = X ∗ exp −∆t

17

(14) (15)

where the tensor X e∗ := t+∆tt X t0 X e is the trial elastic deformation gradient (i.e. with the plastic state frozen). The polar decomposition theorem applied to the trial elastic deformation gradient yields e X e∗ = Re∗ ← U −∗

(16)

e e where ← U −∗ is the trial (elastic) right stretch tensor and R∗ is the trial rotation tensor. We now deﬁne the following incremental (“plastic”) rotation t+∆t w t+∆t (17) Wp t R = exp ∆t e e Using (15) and deﬁning ← C −∗ := X ∗ deformation tensor) we obtain

e C ← −∗ =

t+∆t wT tR

exp ∆t

t+∆t

Dp

T

X e∗ (the trial right Cauchy-Green

t+∆t e 0C

exp ∆t

t+∆t

Dp

t+∆t w tR

(18)

We now deﬁne the logarithmic strains by t+∆t e 0E

:=

1 2

log

t+∆t e 0C

e E ← −∗ :=

and

1 2

e log ← C −∗

(19)

The following tensors are the measures updated to the stress-free conﬁguration C e∗ :=

t+∆t w tR

E e∗ :=

t+∆t w tR

e C ← −∗

t+∆t wT tR

(20)

e t+∆t wT E (21) tR ← −∗ For future expressions we note that (·) are the quantities (·) rotated to the ← − rotationally-frozen conﬁguration (deﬁned below), i.e.

(·) = ← −

t+∆t wT tR

(·)

t+∆t w tR

(22)

Using Equations (11) and (19), Equation (18) may be written as E e∗

t+∆t e 0E

+ ∆t

t+∆t

Dp

(23)

with the additional restriction that E e∗ 1, i.e. the elastic strains and incremental steps are only moderately large. This restriction is typically fulﬁlled in metal plasticity. Alternatively, expression (23) may be written as t+∆t e E 0← −

e E ← −∗ − ∆t

known

t+∆t

p D ← −

(24)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

19

conﬁguration is given by t+∆t0 ReT , only known after integration. Fortunately, Equations (24) and (25) show that the additive algorithm also holds in the conﬁguration in which the plastic rotation t+∆tt Rw has not been applied yet. From a continuum perspective, using the following deﬁnitions e p e ˙ e eT ˙ w wT and wp = Re W p ReT we∗ = R˙ ∗ ReT ∗ , w =R R , W =R R (30) performing the time derivative of Equation (27) and multiplying by ReT ∗ = RwT ReT to transfer the Equation to the spatial conﬁguration, we obtain

i.e.

e ˙ e eT + Re R˙ w RwT ReT R˙ ∗ ReT ∗ = R R

(31)

we∗ = we + wp

(32)

3 Free Energy Function and Dissipation Inequality The global free energy ψ is assumed to admit the additive decomposition into a stored energy function W and a hardening potential H ψ X e , X i , X i -history = W X e , X i -history + H X i , X i -history (33) where X i are internal variables which can be deﬁned by a gradient of some local internal displacements. Obviously, by objectivity, the stored energy function should depend only on the stretch part of X e , since it must remain unaﬀected by rigid body motions. We assume that the solid deforms in such a way that the total potential energy is minimum and that the dissipation energy is maximum including the eﬀect of plastic spin. We assume that the rotation of the anisotropy directions is also related to a change of the potential energy. Hence, special considerations arise for the stored energy function and the hardening potential. We incorporate these considerations in the energy function and hardening potential proposed below. 3.1 Stored Energy Function: Orthotropic Hyperelasticity Based on Logarithmic Strain Measures In the case of isotropic elasticity, the right Cauchy deformation tensor C e and the second Piola-Kirchhoﬀ stress tensor S commute. Then, the Mandel stress tensor Ξ := C e S and the symmetric part of the Mandel stress tensor, Ξ s , results in (34) Ξ s = Ξ = 12 (C e S + SC e ) = U e SU e which in terms of the spatial Kirchhoﬀ stress tensor τ may be written as Ξ s = U e X e−1 τ X e−T U e = ReT τ Re = τ¯

(35)

20

F.J. Mont´ ans and K.J. Bathe

where τ¯ is the rotated Kirchhoﬀ stress tensor [2]. Assuming isotropic elasticity, the governing strain energy function can be expressed as W = U (J) + µ E ed : E ed = U (J) + µ E e : P : E e

(36)

where E e := ln U e are the logarithmic strains, E ed := P : E e are the deviatoric logarithmic strains, P := I − 13 I ⊗ I is the deviatoric projector tensor and I and I are, respectively, the fourth and second order identity tensors. The two terms in Equation (36) represent the volumetric and deviatoric strain energies respectively. The rotated Kirchhoﬀ stress tensor is obtained as (see for example Reference [15]) Ξ ≡ Ξ s ≡ τ¯ =

∂W = JU (J) + 2µ P : E e ∂E e

(37)

whereas the skew-symmetric part of the Mandel stress tensor, Ξ w , vanishes. As also mentioned in the introduction, in anisotropic plasticity, the elastic properties are frequently considered as isotropic given that experimentally much smaller deviations from isotropy are observed for elastic properties than for plastic properties. In this work we wish to relax the assumption of isotropy for the elastic properties and allow moderate anisotropic elasticity, and hence we use the following function: t W = U t J + µ t E e : t Ad : t E e (38) where t Ad is the orthotropy structural tensor which has the same characteristic space as P (commutes with P) and is, in general, close to P. Note that in this case the volumetric component is assumed as isotropic reducing the number of independent constants to seven. Of course, a general anisotropic tensor t A (with nine constants) may also be employed with the logarithmic strain. In this case the stored energy function is of the type t

W=

1 t e 2 E

: tA : tEe

(39)

where t A−1 in the principal material orthotropy axes { t P i , i = 1, 2, 3}, may be written as —see for example Reference [1]— ⎤ ⎡ 0 0 1/Ea −νba /Eb −νca /Ec 0 ⎢ −νab /Ea 1/Eb −νcb /Ec 0 0 0 ⎥ ⎥ ⎢ ⎢ /E −ν /E 1/E 0 0 0 ⎥ −ν ac a bc b c t −1 ⎥ ⎢ A =⎢ (40) 0 ⎥ 0 0 0 1/Gab 0 ⎥ ⎢ ⎣ 0 0 0 0 1/Gbc 0 ⎦ 0 0 0 0 0 1/Gca { t P } i

where Ea , Eb , Ec are the Young’s moduli in the principal directions, νba , νca , νcb , νab , νac , νbc are the Poisson ratios and Gab , Gbc , Gca are the shear moduli. These constants need to satisfy certain conditions, see e.g. [1].

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

21

In Equations (38) and (39), the strain tensor, and thus also the elastic anisotropy tensor, are deﬁned in the unrotated conﬁguration (i.e. with the elastic rotations given by Re removed). Between time t and time t + ∆t, this conﬁguration and all objects deﬁned in this conﬁguration rotate by the amount t+∆tt Rw due to the plastic spin—see Equation (28). And during the plastic ﬂow, also the lattice rotation takes place, resulting in an additional rotation t+∆tt RA for the anisotropy directions. For example, the resulting energy of Equation (39) at t + ∆t is t+∆t

W= = =

t

t t+∆t e 1 t+∆t e E E 2 ← − : A: ← − t+∆t t+∆t e 1 t+∆t e E : A : E 2 ← − ← − ← − t+∆t t+∆t e 1 t+∆t e E : A : E 2

(41)

t+∆t A A tR ← − we imply that the tensor has rotated by t+∆t A t with respect to A. The rotation tensor t R represents the rotation of the elastic anisotropy tensors. Therefore, the energy expression in the stress-free conﬁguration is obtained by the rotation t+∆tt Rw and the rotation t+∆tt RA . The derivative of the stored energy function in absence of plastic rotations is e ˙ ˙e W = ← E A E (42) − :← −: ← − apr

where by

A =:

t+∆t

e L = Ee : A : ← −E

(43)

e e The tensor ← T = ∂W / ∂ E A E − ← − apr = ← − : ← − is deﬁned as the symmetric logarithmic stress tensor (or generalized Kirchhoﬀ stress tensor) in the rotation-free conﬁguration. If the lattice structure is not ﬁxed, the variation of the strain energy function in the rotation-free conﬁguration is ˙ = T : E˙ e + 1 E e : A˙ : E e W 2← ← − ← − − ← − ← −

(44)

The second term in Equation (44) is the work variation due to a rotation of the lattice, which after plastic ﬂow will be in a more favorable orientation. Hence A ˙ A A T as the structural this term must be negative. Deﬁning ← W − := R R t+∆t t+∆t e T A E anisotropy spin tensor and using t+∆t ← − = ← − : ← − , the second term of Equation (44) can be written in symbolic notation as 1 2

e A A e W − W E E T − ← − ← − :← ← − ← −+ e A A e = ← T : E W − W E − ← − ← − ← − ← −

e e ˙ E A E ← − :← −: ← − =

1 2

A =← T −w : W ← −

1 2

e A A e T : E W − W E ← − ← − ← − ← − ← −

(45)

22

F.J. Mont´ ans and K.J. Bathe

where ← T −w is a skew tensor deﬁned as e e T E T T E (46) ← −w := ← − ← −−← −← − Of course we can deﬁne equivalent measures in the unrotated conﬁguration: t+∆t wT T = A : E e and T w := E e T − T E e tR ← − or in the spatial conﬁguration

T :=

t+∆t

t :=

t+∆t w tR

t+∆t e t+∆t T t+∆t0 ReT 0R

(47)

eT e e = Re∗ ← T − R∗ and tw := e t − te (48)

where ee := ln V e and V e is the stretch tensor obtained from the left polar decomposition theorem. Finally we obtain ˙ = T : E˙ e + T w : W A W ← − ← − ← − ← −

(49)

˙ = T : L Ee + T w : W A W ← −

(50)

Here T w is determined once T and E e are known, i.e., it is not an independent or internal variable. The second term in the variation of the stored energy function is the variation due to the rotation of the anisotropy axes, and depends on the non-coaxiality of stresses and elastic strains. Figure 1 refers to the diﬀerent rotations and conﬁgurations used. The spatial conﬁguration for strains is known from the material conﬁguration by t+∆t 0 X. From this spatial conﬁguration we can directly obtain the trial unrotated conﬁguration (rotationally frozen) by the rotation ReT ∗ , obtained from the polar decomposition Eq.(16) of the trial elastic gradient (292 ). Then, as shown below, we obtain the plastic correction t+∆tt Rw for the trial unrotated conﬁguration, which has the ﬁnal value given by Equation (28). Due to the rotation t+∆tt Rw the preferred elastic and plastic anisotropy directions rotate by the additional amount t+∆tt RA in the form given below. Since we are assuming moderate incremental steps, both t+∆tt Rw and t+∆tt RA may be considered to commute. 3.2 Hardening Potential Consider a hardening potential of a similar form to that of the stored energy function H = Hkin +Hiso +Hw = 12 h¯ (1 − M ) 32 E i : H : E i + M ζ 2 + 12 Kw ξ 2 =

1¯ 2h

(1 − M )

3 2

i

i

E H E ← − : ← −:← − +M ζ

2

(51)

+

2 1 2 Kw ξ

(52)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity a principal orthotropy direction in the trial unrotated configuration

23

a principal strain direction in the trial unrotated configuration a principal strain direction or principal orthotropy direction in the final unrotated configuration

a principal strain direction or principal orthotropy direction in the final spatial configuration

Fig. 1. Conﬁgurations involved in the stress-integration algorithm

¯ (1 − M ) is the eﬀecwhere M is the mixed hardening parameter, 23 H := h ¯ tive kinematic hardening modulus and K := hM is the isotropic hardening ¯ plays the role of eﬀective hardening modulus. The modulus. The parameter h parameter Kw is a hardening for couple-stresses. Eq.(51) corresponds to a ¯ it SPM description of hardening, see Reference [43]. However, for constant h coincides with the SPS method. In (51) we have included the possibility of anisotropic kinematic hardening through the use of an anisotropy tensor H, H similar to Ad . The tensor ← −, rotates at the speed given by the internal spin tensor W H for similar reasons as those given for the stored energy function. We deﬁne the internal overstresses as κ :=

∂ψ and ∂ζ

κw :=

∂ψ ∂ξ

(53)

Hence, κ=

∂ψ ∂H = = Kζ ∂ζ ∂ζ

and

∂H ∂ψ = = Kw ξ ∂ξ ∂ξ

(54)

∂2ψ ˙ ∂2H ˙ ξ= ξ = Kw ξ˙ ∂ξ 2 ∂ξ 2

(55)

κw =

or κ˙ =

∂2ψ ˙ ∂2H ˙ ζ= ζ = K ζ˙ ∂ζ 2 ∂ζ 2

and

κ˙ w =

We define the internal backstress as ∂ψ ∂H i = = H← H E B i −:← − ← −s = ∂ E i ∂ E ← − apr ← − apr

(56)

Then, the derivative of the hardening potential is ˙ E i + κζ˙ + κw ξ˙ ˙ i 1 Ei : H E H˙ = ← B − + 2H ← − ← −:← − −s : ←

(57)

24

F.J. Mont´ ans and K.J. Bathe

and following the same steps as for the stored energy function 1 2H

i i H ˙ E H E B ← − :← −: ← − =← −w : W ← −

(58)

where ← B −w is a skew tensor deﬁned as i i B E B B E ← −w := ← − ← −s − ← −s ← −

(59)

Finally we have ˙ i B w : W H + κζ˙ + κw ξ˙ E H˙ = ← B − +← − ← − −s : ← i H ˙ ˙ = Bs : ← L −E + B w : W + κζ + κw ξ

(60)

However, we note that equations (51), (54) and (56) may not be formally adequate because they are deﬁned in terms of total internal strains and, as the plastic strains, they are path dependent. Hence directly assuming (60), (55) and the rate form of (56) is more appropriate, and (51) should be taken just for motivation purposes. Furthermore, Equation (33) should formally be assumed in rate form, and in the derivations to follow only the rate form will be used.

4 Mapping Tensors from Quadratic to Logarithmic Strain Space In large strain plasticity, logarithmic strain measures frequently yield simple and natural descriptions. Of course, these strains may be used in any conﬁguration simply using the proper stretch tensor to obtain them. The following relationship holds: E e = Re T ee Re

with

E e = ln U e , ee = ln V e

(61)

Hence, it is noted that for logarithmic strain tensors, the push-forward and pull-back operations are performed with the rotation part of the deformation gradient alone. One may say that the stress-free conﬁguration and the “unrotated” conﬁguration are coincident in the logarithmic strain space. Obviously, since the logarithmic strain tensors and the Almansi and Green strains are all unique for a given deformation gradient, there exist a one-to-one mapping between them. For example e E e = ME A:A

(62)

where if the spectral forms of the strain tensors are Ee =

3 i=1

ln λei N i ⊗ N i ,

Ae =

3 e 1 2 λi i=1

2

− 1 Ni ⊗ Ni

(63)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

25

ME A can be written as ME A=

3 2 ln λei Ni ⊗ Ni ⊗ Ni ⊗ Ni λe 2 − 1 i=1 i

(64)

as it is straightforward to verify. Conversely MA E=

3 λe i=1

2

−1 Ni ⊗ Ni ⊗ Ni ⊗ Ni 2 ln λei i

(65)

e is such that Ae = MA E : E . In a similar way, there is a one-to-one mapping between the deformation rate tensor and the time-derivative of the logarithmic strains. These mapping tensors may be found to be (see Reference [51]) 3 3 ln λej − ln λei s 1 ∂E e ˙ = M ⊗ M + 2 M i M j (66) ME = i i e e 2 e 2 e 2 D ∂A λ λj − λi i=1 i i=1 j=i

and 3 3 λej 2 − λei 2 s ∂Ae e 2 D 1 λi M i ⊗ M i + M˙ = e = e − ln λe M i M j 2 E ∂E ln λ j i i=1 i=1

(67)

j=i

where M i := N i ⊗ N i s

M i M j :=

1 4

(68) s

(N i ⊗ N j + N j ⊗ N i ) ⊗ (N i ⊗ N j + N j ⊗ N i ) ≡ M j M i (69)

These tensors have major and minor symmetries and represent the one-to-one mappings relating deformation rates as e ˙ e E˙ = ME D:D

e and D e = MD : E˙ E˙

(70)

respectively. Furthermore, in the rotation-frozen conﬁguration ˙ e ME˙ : D e and D e = MD : E˙ e E −D ← ← − ← −E˙ ← ← − =← − −

(71)

Also, in the stress-free conﬁguration e E˙ L Ae and L Ae = MD : L E e L ← − − − ← −E = MD : ← E˙ ←

For future use, we deﬁne two fourth order mapping tensors 1 M e3 E˙ − C e 4· ME˙ := · M W C −D ← −D ← − − ← − ← 2 ←

(72)

(73)

26

F.J. Mont´ ans and K.J. Bathe

and

1 S M := ← − 2

e3 e4 E˙ E˙ M M C C −D + ← −D ← − ·← − ·←

(74)

n where by · we imply the contraction of the n − index of the fourth order tensor with the second index of the second order tensor. Then, it can be shown that if we deﬁne D E˙ K S M S M (75) ← − := ← −:← −E˙ so that ← − =: K ← −:← −D we obtain

and

e e E˙ = K : S M + WM S = C K : M Ξ := C − ← − ← ← − − ← −D ← − ← − ← − ← − ← M e e E E K ← −:W ← − =← − K ← −−K ← −← − ≡ Ξw ← −w := K Ξ SM ← −s = K ← −:← −

(76)

(77) (78)

The tensor K is actually the generalized K irchhoff stress tensor T , see also below, and hence the conversion to the symmetric part of the Mandel stress tensor Ξ s is given by Equation (78).

5 Dissipation Inequality The stress power in the reference volume may be expressed in the intermediate conﬁguration as P ≡ S : L = S : (Le + C e Lp ) = S : (D e + W e ) + S : C e (D p + W p )

(79) (80)

where S is the pull-back of the Kirchhoﬀ stress τ to the stress-free conﬁguration. Since S is symmetric the product S : W e = 0, i.e. the modiﬁed elastic spin (which also contains the rigid-body spin) produces no work. Thus, in a rotationally-frozen conﬁguration we are left with ˙ e + S : C e Dp + W p (81) P≡← S : L = K : E ← − ← − ← ← − − − ← − ← − ← − where we used (71) and (75). Alternatively, in the stress-free conﬁguration e e p p S:L = K:← L −E + S : C (D + W ) e e p p = K:← L −E + C S : (D + W )

(82) (83)

Using Ξ = C e S, the stress power can be written as e p p S:L =K:← L −E + (Ξ s + Ξ w ) : (D + W ) e p p =K:← L −E + Ξ s : D + Ξ w : W

(84)

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

27

Thus, the symmetric Mandel stress tensor produces power on the modiﬁed plastic strain rate, whereas the skew-symmetric Mandel tensor produces power on the modiﬁed plastic spin. This last work is due to the kinematic coupling produced by the Lee decomposition and the possible rotation of elastic anisotropy axes. In the case of isotropy or deformation through the orthotropy axes, the term vanishes. Neglecting the eﬀect of temperature, the dissipation inequality from the second law of the thermodynamics is D˙ = P − ψ˙ ≥ 0

(85)

˙ + H. ˙ Thus where ψ˙ is the free energy function rate, assumed to be ψ˙ = W using (49) and (60) e A i H ˙ ˙ L ψ˙ = T : ← L −E + B w : W + κζ + κw ξ −E + T w : W + B s : ←

and

(86)

e p p D˙ = (K − T ) : ← L −E + Ξ s : D + Ξ w : W

i H ˙ ˙ −T w : W A − B s : ← L −E − B w : W − κζ − κw ξ ≥ 0

(87)

Since the equality must hold for pure elastic deformations, T =K

(88)

T w = Kw ≡ Ξw

(89)

and, in consequence, The reduced (plastic) dissipation inequality is now i H ˙ ˙ D˙ p = Ξ s : D p + Ξ w : W d − B s : ← L −E − B w : W − κζ − κw ξ ≥ 0 (90)

where we deﬁned the dissipative spin tensor in the unrotated conﬁguration as W d := W p − W A

(91)

We note that if W p = W A then the skew part of the Mandel stress tensor does not contribute to the dissipation function. On the other hand, since W A is assumed to be a function of W p , if W p = 0 then W A = 0 and no dissipation takes place either due to the skew part of the Mandel stress tensor. We will assume that the following relationship holds W A = ρW p

(92)

where ρ is a material scalar parameter. Then W d = (1 − ρ) W p

(93)

We assume now –without loss of generality– that the elastic region is enclosed by two yield functions fs (Ξ s , B s , κ) and fw (Ξ w , B w , κw ), the La˙ s − γf ˙ w , where t˙ and γ˙ grangian for the constrained problem is L = D˙ p − tf

28

F.J. Mont´ ans and K.J. Bathe

i i are the consistency parameter increments. Note also that ← L −E ≡ D . If we claim that the principle of maximum dissipation holds, the stress and other internal variables are such that ∇L = 0, i.e. for the yield function expressions given ⎧ ∂L ∂fs ∂L ∂fw ⎪ = 0 ⇒ D p = t˙ and = 0 ⇒ W d = γ˙ ⎪ ⎪ ∂Ξ s ∂Ξ s ∂Ξ w ∂Ξ w ⎪ ⎪ ⎪ ⎪ ⎨ ∂L ∂fs ∂L ∂fw = 0 ⇒ L E i = −t˙ and = 0 ⇒ W H = −γ˙ ∇L = 0 ⇒ ← − ∂B ∂B ∂B ∂B ⎪ s s w w ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ∂fw ⎩ ∂L ˙ ˙ ˙ ∂fs

∂κ

= 0 ⇒ ζ = −t

∂κ

and

ξ = −γ˙

∂κw

(94) These expressions are the associated ﬂow and hardening rules for general elastoplasticity at ﬁnite strains. It is noted that if, as usual, the enclosure of the elastic region for the symmetric part is expressed in the form of fs (Ξ s − B s ...) then for associative plasticity the following relationship is automatically enforced i i p (95) L ← −E ≡ D = D Furthermore, W i does not aﬀect the dissipation function and can be freely prescribed. In view of Equation (95), and assuming that internal variables rotate as the plastic variables, we will set

and, as a consequence

Wi = Wp

(96)

Xi = Xp

(97)

The loading/unloading (complementary) Kuhn-Tucker conditions are, as usual ˙ s≡0 t˙ ≥ 0, fs ≤ 0 and tf (98) γ˙ ≥ 0,

fw ≤ 0

and γf ˙ w≡0

(99)

and the consistency conditions are t˙f˙s ≡ 0

and γ˙ f˙w ≡ 0

(100)

The formulations presented herein and in Reference [44] show some similarities with some other works, see for example References [18, 20, 45–48], but there are also some signiﬁcant diﬀerences; in particular we are using logarithmic strains in an incremental form.

6 Yield Functions There is still much experimental work needed to establish the elastic domain and yield functions for the symmetric and skew parts of the Mandel stress tensor. From the current experimental evidence it is diﬃcult to infer sound

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

29

data about a macroscopic (continuum) elastic domain for the skew part of the Mandel stress tensor, and for the plastic spin evolution. Hence, at this point a “reasonable” proposition is necessary. An ad hoc extension of the small strains theory without plastic spin follows. 6.1 Yield Function for the Symmetric Part For the symmetric part of the Mandel stress tensor the well-known Hill’s quadratic yield criterion is assumed to hold, i.e. the yield function for Ξ s is given by the expression (see for example Reference [1]) fs :=

3 (Ξ s − B s ) : Aps : (Ξ s − B s ) − 1 = 0 2κ2

(101)

where Aps is the plastic anisotropy tensor which in this work we assume to have the same preferred anisotropy directions as the elastic anisotropy tensor. Given this function, the speciﬁc values of the internal variable increments are obtained from Equations (94) and (95) as ∂fs 3 = 2 Aps : (Ξ s − B s ) t˙ D i = D p = t˙ ∂Ξ s κ

(102)

The internal isotropic variable rate is obtained as 2 ∂fs = (fs + 1) t˙ ζ˙ = −t˙ ∂κ κ

(103)

which, at the yield condition (fs = 0) takes the value ζ˙ = 2t˙ /κ. The physical meaning of ζ˙ is the eﬀective plastic strain rate, see Reference [1]. 6.2 Yield Function for the Skew Part For the skew part, in this work we consider the simplest possible yield function, of the Mises type √ (104) fw = Ξ w − 2κw where κw is the allowed yield value, which may take the value of zero. From Equation (94), the speciﬁc ﬂow variables take the form W d = γ˙

∂fw ˆw = γ˙ Ξ ∂Ξ w

(105)

√ ∂fw ξ˙ = −γ˙ = 2γ˙ (106) ∂κw ˆ w := Ξ w / Ξ w . The physical meaning of where we deﬁned the “direction” Ξ ξ˙ is the eﬀective dissipative rotation rate. Using Equations (92) and (93) we obtain 1 ρ ˆ w and W A = ˆw γ˙ Ξ γ˙ Ξ (107) Wp = (1 − ρ) (1 − ρ)

30

F.J. Mont´ ans and K.J. Bathe

One important consequence of the function fw deﬁned in Equation (104) and the expression (1072 ) is that if 1 > ρ > 0 then W A and Ξ w ≡ T w have the same direction. But as noted just after Equation (44), the term T w : W A should be negative. Hence possible values are ρ > 1 and ρ < 0. If ρ > 1 then the term T w : W A is negative and W p and W A have the same direction. If ρ < 0 then the term T w : W A is also negative and W p and W A have opposite direction. The actual rotation direction is not only determined by ρ, but also by the elastic anisotropy tensor because its shape may change the direction of Ξ w . 6.3 Coupling of Symmetric and Skew Parts The yield function Equation (104)√would mean an instantaneous rotation once Ξ w is over the allowed value 2κw . However this is not consistent with experiments, in which progressive rotations are observed. Aside, in mechanics of single crystals this rotation is not independent of the ordinary (symmetric) plastic ﬂow (Schmid’s law). Hence, in this work we propose a viscoplasticitylike ﬂow for the skew part in which the eﬀective plastic strain plays the role of the time variable. This proposed expression is m ˙ξ = < fw > ζ˙ (108) η where < · > is the Macauley bracket function, η is the “viscosity” material parameter with units of (couple-)stress and m is another material parameter. Hence, fw may have values greater than zero which relax with plastic ﬂow. In terms of consistency parameters, Equation (108) may be written as √ m 2 < fw > t˙ (109) γ˙ = κ η Hence, γ˙ is zero if either fw ≤ 0 or t˙ = 0.

7 Numerical Example In order to test the capabilities of the present theory in modelling the rotation of the anisotropy directions, we have carried out some numerical experiments. In these numerical tests, we aim for predictions of the experimental results reported in Reference [32]. In these experiments, a rotation of the material symmetry was observed when a steel sheet is strained in a direction that forms an angle θ with the rolling or prestrain direction. Details of the experiments are given in Reference [32]. Only small changes in the shape of the yield function were observed and hence the shape of the yield function can be assumed to remain constant, see also Reference [33].

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

31

However, unfortunately, in Reference [32] only the measured plastic anisotropy and its evolution are reported. Since our theory includes and indeed uses elastic anisotropy, we need to assume elastic anisotropy parameters. In a uniaxial test, a relevant degradation of Young’s modulus and a variation of Poisson’s ratio in the test direction has been reported [49]. Elastic anisotropy has also been measured in rolled steel, brass and aluminum, see for example [50]. We therefore assume the following elastic (only slightly anisotropic) material parameters: Ea = 2.04×1011 Pa, Eb = 2.03×1011 Pa, Ec = 2.10×1011 Pa, νab = 0.3, νac = 0.3, νbc = 0.3, and Gab = 0.82 × 1011 Pa. The yield stress κ0 and Hill’s yield function parameters have been reported in Reference [32], i.e. f = 0.3613, h = 0.4957, g = 0.3535 and we used N = 1.175 and κ0 = 23 × 107 Pa. The hardening has been considered as isotropic according ¯ for which the constants to the formula κ = κ∞ − (κ∞ − κ0 ) exp (−δζ) + hζ, ¯ have been deduced from the experimental data, h = 3.5 × 108 Pa, κ∞ = 1.2κ0 , δ = 30. We also used the parameters κw = 0, m = 2, ρ = −2 and η = 600 Pa. All these parameters should really be chosen based on experimental results. However, we used the mentioned values and only adjusted η to match the experimental data. Details of the numerical implementation of the theory may be found in Reference [51]. The Young’s modulus and the yield stress in the diﬀerent directions, as well as their evolution are shown in Figure 2. In this ﬁgure we also compare the predicted yield stresses with the experimental data for the case of the applied load at θ = 30o to the rolling direction. Figure 3 compares experimental data and computed results for θ = 30o , 45o and 60o . Of course, diﬀerent elastic anisotropy constants (obtained experimentally) would change the predictions, but then also the material parameters η, ρ and m should be based on experimental results. An important feature of our formulation is that diﬀerent rotation rates are obtained for diﬀerent angles, and the predictions may not be symmetric for 30 and 60 degrees —in accordance with experimental results— even though the yield function is almost symmetric about the direction 44.7 degrees with the rolling direction. This is due to the selected shape for the anisotropy tensors.

8 Conclusions We presented our research towards a model for anisotropic elasto-plasticity. The model shall represent possible anisotropic elasticity, anisotropic yield surfaces, hardening and the rotation of the elastic and plastic orthotropy directions during plastic ﬂow. Both the continuum and time integration incremental formulations are simultaneously derived since incremental formulations give some insight into the continuum formulation. The model and the integration algorithm are derived using the multiplicative Lee decomposition of the total deformation gradient into an elastic and a plastic part. However, no total plas-

32

F.J. Mont´ ans and K.J. Bathe (a)

0 2.1

11

20

40

60

80

a

100

120

140

160

180

x 10 Young's modulus E [Pa]

2.09 2.08 2.07 2.06

Prediction:

2.05 2.04 2.03 2.02

120

e = 0% x e = 2% x e = 5% x ex = 10% 140

Y

(b)

Kim & Yin exp.:

Pred. & exp.

a

ex = 0% ex = 2% ex = 5% ex = 10%

x

b (c)

q

3.6 8

(RD)

x 10

Yield stress k [Pa]

3.4 3.2 3 2.8 2.6 2.4 2.2 0

20

40

60

80

a

100

120

140

160

180

Fig. 2. (a) Prediction of the evolution of the Young’s modulus proﬁle at diﬀerent spatial strains ex for a uniaxial load at an angle of θ = 30o with respect to the rolling direction (RD). (b) Angles involved in the example. Angle of the uniaxial load with the rolling direction (θ), angle of the principal direction a with the uniaxial load (β) —initially β = θ—, angle of the Young’s modulus and yield stress shown in the curves with the uniaxial load (α). (c) Comparison of the experimental data of [32] with the prediction of the evolution of the yield stress proﬁle at diﬀerent spatial strains ex for a plane stress load at an angle of θ = 30o with respect to the rolling direction

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

33

(a) 100

80 Kim & Yin experiments, q = 30º, q = 45º, q = 60º Prediction for q = 30º Prediction for q = 45º Prediction for q = 60º

b

60

40

20

0 0

0.01

0.02

0.03

0.04

0.05

0.06

0.07

0.08

0.09

0.1

0.06

0.07

0.08

0.09

0.1 10

ex 0

0.01

0.02

0.03

0.04

0.05

3.2 8

3

3

x 10

x 10

8

tx [Pa ]

2.8

6

2.6

4 2.4

|| tw || [Pa ]

(b)

2

2.2 2

0.1

0.09

0.08

0.07

0.06

0.05

0.04

0.03

0.02

0.01

0

ex

Fig. 3. (a) Prediction for the evolution of the principal orthotropy directions and comparison with the experimental values of Reference [32]. (b) Uniaxial stress and couple-stress evolutions

tic deformation measure is used. Plastic deformations and plastic rotations are considered only incrementally. The stresses are directly obtained from the logarithmic elastic strains, with the model assuming linear elastic anisotropy and moderate elastic strains, but accounting for possible large plastic strains. The model presented oﬀers, in particular, possibilities to simulate the rotation of the material axes observed in experiments on anisotropic elasto-plastic materials, and as an example good correlation to the experimental data of Kim and Yin has been obtained. However, clearly, the model must be studied much more. The sensitivity of the model predictions with respect to the model parameters needs to be identiﬁed, and comparisons of computed solutions with test data for many more and varied material tests need to be obtained. These studies will also identify the limitations of the model and whether the model could be simpliﬁed without signiﬁcant loss of predictive capability.

34

F.J. Mont´ ans and K.J. Bathe

References 1. Koji´c M, Bathe KJ (2005) Inelastic analysis of solids and structures. SpringerVerlag, New York 2. Bathe KJ (1996) Finite element procedures. Prentice-Hall, New Jersey 3. Sim´ o JC (1988) A framework for ﬁnite strain elastoplasticity based on maximum plastic dissipation and the multiplicative decomposition. Part I: Continuum formulation. Comp Meth Appl Mech Engrng 66: 199-219. Part II: Computational aspects. Comp Meth Appl Mech Engrng 68: 1-31 4. Sim´ o JC, Hughes TJR (1998) Computational inelasticity. Springer-Verlag, New York 5. Bathe KJ, Ramm E, Wilson EL (1975) Finite element formulations for large deformation dynamic analysis. Int J Num Meth Engrg 9: 353-386 6. Koji´c M, Bathe KJ (1987) Studies of ﬁnite element procedures—Stress solution of a closed elastic strain path with stretching and shearing using the updated Lagrangian Jaumann formulation. Comp Struct 26: 175-179 7. Lee EH (1969) Elastic-plastic deformations at ﬁnite strains. J Appl Mech ASME 36: 1-6 8. Lee EH, Liu DT (1967) Finite-strain elastic-plastic theory with application to plane wave analysis. J Appl Phys 38: 19-27 9. Bilby BA, Bullough R, Smith E (1955) Continuous distributions of dislocations: A new application of the methods of Non-Riemannian Geometry. Proc Roy Soc London Ser A 231: 263-273 10. Weber G, Anand L (1990) Finite deformation constitutive equations and a time integration procedure for isotropic hyperelastic-viscoplastic solids. Comp Meth Appl Mech Engrg 79: 173-202 11. Eterovi´c AL, Bathe KJ (1990) A hyperelastic-based large strain elasto-plastic constitutive formulation with combined isotropic-kinematic hardening using the logarithmic stress and strain measures. Int J Num Meth Engrg 30: 1099-1114 12. Sim´ o JC (1992) Algorithms for multiplicative plasticity that preserve the form of the return mappings of the inﬁnitesimal theory. Comp Meth Appl Mech Engrg 99: 61-112 13. Peri´c D, de Souza EA (1999) A new model for Tresca plasticity at ﬁnite strains with an optimal parametrization in the principal space. Comp Meth Appl Mech Engrg 171: 463-489 14. Mont´ ans FJ, Bathe KJ (2003) On the stress integration in large strain elastoplasticity. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2003. Elsevier, Oxford 15. Mont´ ans FJ, Bathe KJ (2005) Computational issues in large strain elastoplasticity: An algorithm for mixed hardening and plastic spin. Int J Num Meth Engrg 63: 159-196 16. Cuiti˜ no A, Ortiz M (1992) A material-independent method for extending stress update algorithms from small strain plasticity to ﬁnite plasticity with multiplicative kinematics. Engrg Comp 9: 437-451 17. Borja RI, Tamagnini C (1998) Cam–Clay plasticity, Part III: Extension of the inﬁnitesimal model to include ﬁnite strains. Comp Meth Appl Mech Engrg 155, 77-95 18. Papadopoulus P, Lu J (1998) A general framework for the numerical solution of problems in ﬁnite elasto-plasticity. Comp Meth Appl Mech Engrg 159: 1-18

Towards a Model for Large Strain Anisotropic Elasto-Plasticity

35

19. Car E, Oller S, O˜ nate E (2001) A large strain plasticity model for anisotropic materials—composite material application. Int J Plasticity 17: 1537-1463 20. Miehe C, Apel N, Lambrecht M (2002) Anisotropic additive plasticity in the logarithmic strain space: modular kinematic formulation and implementation based on incremental minimization principles for standard materials. Comp Meth Appl Mech Engrg 191: 5383-5426 21. Eidel B, Gruttmann F (2003) On the theory and numerics of orthotropic elastoplasticity at ﬁnite plastic strains. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2003. Elsevier, Oxford 22. Han CS, Lee MG, Chung K, Wagoner RH (2003) Integration algorithms for planar anisotropic shells with isotropic and kinematic hardening at ﬁnite strains. Comm Num Meth Engrg 19: 473-490 23. Loret B (1983) On the eﬀects of plastic rotation in the ﬁnite deformation of anisotropic elastoplastic materials. Mech Mater 2: 287-304 24. Dafalias YF (1985) The plastic spin. J Appl Mech ASME 52: 865-871 25. Dafalias YF (1990) On the microscopic origin of the plastic spin. Acta Mech 82: 31-48 26. Anand L (1983) Elasto-viscoplasticity: Constitutive modelling and deformation processing. In Teodosiu C, Raphanel JL, Sidoroﬀ F (eds) Large plastic deformations. AA Balkema, Rotterdam 27. Dafalias YF (1998) The plastic spin: necessity or redundancy? Int J Plasticity 14: 909-931 28. Kuroda M, Tvergaard V (2001) Plastic spin associated with a non-normality theory of plasticity. Eur J Mech A/Solids 20: 893-905 29. Khan AS, Huang S (1995) Continuum theory of plasticity. John Wiley & Sons, New York 30. Levitas V (1998) A new look at the problem of plastic spin based on stability analysis. J Mech Phys Solids 46: 557-590 31. Tong W, Tao H, Jiang X (2004) Modeling the rotation of orthotropic axes of sheet metals subjected to oﬀ-axis uniaxial tension. J Appl Mech ASME 71: 521-531 32. Kim KH, Yin JJ (1997) Evolution of anisotropy under plane stress. J Mech Phys Solids 45: 841-851 33. Kowalewski ZL, Sliwowski M (1997) Eﬀect of cyclic loading on the yield surface evolution of 18G2A low-alloy steel. Int J Mech Sci 39: 51-68 34. Bunge HJ, Nielsen I (1997) Experimental determination of plastic spin in polycrystalline materials. Int J Plasticity 13: 435-446 35. Truong Qui HK, Lippmann H. (2001) Plastic spin and evolution of an anisotropic yield condition. Int J Mech Sci 43: 1969-1983 36. Boheler JP, Koss S (1991) Evolution of anisotropy in sheet steels subjected fo oﬀ-axes large deformation. In Brueler O, Mannl V, Najar J (eds) Advances in continuum mechanics. Springer, Berlin 37. R.H. Randal, C. Zener (1940) Internal friction of aluminum. Phys Rev 58: 472-473 38. Tam AC, Leung WP (1984) Measurement of small elastic anisotropy in solids using laser-induced ultrasonic pulses. Appl Phys L 45: 1040-1042 39. Dvorkin EN, Goldschmit MB (2006) Nonlinear continua. Springer-Verlag, New York

36

F.J. Mont´ ans and K.J. Bathe

40. Mor´ an B, Ortiz M, Shih CF (1990) Formulation of implicit ﬁnite element methods for multiplicative ﬁnite deformation plasticity. Int J Num Meth Engrg 29: 483-514 41. Anand L (1985) Constitutive equations for hot-working of metals. Int J Plasticity 1: 213-231 42. Sim´ o JC (1986) On the computational signiﬁcance of the intermediate conﬁguration and hyperelastic relations in ﬁnite deformation elastoplasticity. Mech Mat 4: 439-451 43. Bathe KJ, Mont´ ans FJ (2004) On modelling mixed hardening in computational plasticity. Comp Struct 82: 535-539 44. Mont´ ans FJ, Bathe KJ (2005) Large strain anisotropic plasticity including effects of plastic spin. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2005. Elsevier, Oxford 45. Tsakmakis Ch (2004) Description of plastic anisotropy eﬀects at large deformations—part I: restrictions imposed by the second law and the postulate of Il’iushin. Int J Plasticity 20: 167-198 46. Eidel B, Gruttmann F (2005) Anisotropic pile-up pattern at spherical indentation into a fcc single crystal—ﬁnite element analysis versus experiment. In: Bathe KJ (ed) Computational ﬂuid and solid mechanics 2005. Elsevier, Oxford 47. Han C-S, Choi Y, Lee J-K, Wagoner RH (2002) A FE formulation for elastoplastic materials with planar anisotropic yield functions and plastic spin. Int J Solids Struct 39: 5123-5141 48. Han C-S, Chung K, Wagoner RH, S-I Oh (2003) A multiplicative ﬁnite elastoplastic formulation with anisotropic yield functions. Int J Plasticity 19: 197-211 49. Luo L, Ghosh AK (2003) Elastic and inelastic recovery after plastic deformation of DQSK steel sheet. J Engrg Mater Tech ASME 125: 237-246 50. Lauwagie T, Sol H, Roebben G, Heylen W, Shi Y (2002) Validation of the Resonalyser method: an inverse method for material identiﬁcation. Proc Int Conf Noise Vibration Engrg, ISMA2002, Leuven, Belgium 51. Mont´ ans FJ, Bathe KJ (in preparation) A framework for computational large strain plasticity—anisotropic elasticity, anisotropic yield functions and mixed hardening

Localized and Diﬀuse Bifurcations in Porous Rocks Undergoing Shear Localization and Cataclastic Flow Ronaldo I. Borja Department of Civil and Environmental Engineering, Stanford University, Stanford, CA 94305, USA [email protected] Summary. Under normal temperature porous rocks can fail either by shear strain localization or cataclastic ﬂow. Shear localization results from the coalescence of microcracks leading to a tabular deformation band, whereas cataclastic ﬂow is characterized by grain crushing and pore collapse resulting in a severely damaged but macroscopically homogeneous compacted continuum. In this paper we view the two types of instability as arising from two distinct bifurcation modes. The ﬁrst mode, predicted from the singularity of the acoustic tensor, produces a strain rate jump tensor of rank one and deﬁnes a deformation band. The second mode, predicted from the singularity of the tangent constitutive operator, is diﬀuse and produces a full-rank strain rate jump tensor. After identifying the relevant bifurcation mode, we present a framework for capturing post-failure responses through constitutive branching. The post-collapse constitutive response features a cohesion softeningfriction hardening applied either to an emerging fault for shear localization or to the bulk constitutive theory for diﬀuse pore collapse instability.

1 Introduction Under normal laboratory testing conditions porous rocks tested under triaxial compression can fail either by shear strain localization or by cataclastic ﬂow [1–4]. The relevant mode of failure depends on the conﬁning pressure and temperature under which the rock sample is tested. Trends are depicted pictorially in Figs. 1 and 2 for the case of triaxial compression testing of Adamswiller sandstone (the details of the testing are given in [4]). At lower conﬁning pressures (5 and 20 MPa) the rock sample ﬁrst compacts and then dilates until it forms a well-deﬁned shear band. This is characteristic of brittle failure. The specimen tested at 40 MPa exhibits multiple bands representing transition from localized to cataclastic failure. Multiple compaction bands are not atypical at this transition pressure, with the axial strain increasing in Fig. 1 due to porosity reduction as the thickness of the compaction bands increases (Wong, personal communication). Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 37–53. © 2007 Springer. Printed in the Netherlands.

Ronaldo I. Borja

POROSITY CHANGE (%)

STRESS DIFFERENCE, MPA

38

240

150 MPa 100 MPa

180 60 MPa

120

40 MPa 20 MPa

60

5 MPa

0 0

5 MPa 20 MPa

2

40 MPa 60 MPa

4 6

100 MPa 150 MPa

8 10

0

3

6

9

12

15

AXIAL STRAIN (%)

Fig. 1. Mechanical data for Adamswiller sandstone from six triaxial compression tests under diﬀerent eﬀective pressures as indicated. Samples tested at 5 and 20 MPa failed by shear localization; sample tested at 40 MPa exhibited multiple bands; samples tested at higher conﬁning pressures failed by cataclastic ﬂow. Figure reproduced from [4]

At higher conﬁning pressures (60, 100, and 150 MPa) the sample compacts throughout as the mean normal stress increases up to a knee in the stress-strain curve (Fig. 2b), after which an accelerated volume compaction occurs with some hardening in the principal stress diﬀerence (Fig. 1) and mild increase in the mean normal stress (Fig. 2). The micromechanical processes may be considered brittle in all specimens due to the pervasive grain-scale microcracking. However, on a macroscopic scale the modes of failure may be described very diﬀerently in that shear localization manifests a brittle mode whereas cataclastic ﬂow appears much more ductile. Though not reported for this particular sandstone, Hirth and Tullis [1] observed that cataclastic ﬂow in a porous quartzite is only a transient behavior in that when the pores have collapsed any subsequent deformation could become more localized into a shear band. This typically occurs at much higher strains, of the order 25%, and subsequent volume deformation could eventually become dilative. In this paper we employ classical bifurcation analysis to predict shear localization and cataclastic ﬂow failure modes in rocks at macroscale. Shear localization is predicted from the singularity of the acoustic tensor as described by Rudnicki and Rice [5]. The upshot of the prediction is a planar band across

Localized and Diﬀuse Bifurcations

39

EFFECTIVE MEAN STRESS (MPA)

125

(a) 100

ISOTROPIC 40 MPa

75 20 MPa

50 5 MPa

25

0 −1

0

1

3

2

4

5

EFFECTIVE MEAN STRESS (MPA)

POROSITY CHANGE (%)

(b)

500 400

ISOTROPIC

300 150 MPa

200

100 MPa 60 MPa

100

0

0

2

4

6

8

10

12

14

POROSITY CHANGE (%)

Fig. 2. Shear-induced dilation and compaction in Adamswiller sandstone: (a) samples tested at 5 and 20 MPa conﬁning pressures localized in shear across a single band, sample tested at 40 MPa exhibited multiple bands; (b) samples tested at higher conﬁning pressures failed by cataclastic ﬂow. Figure reproduced from [4]

which the velocity gradient exhibits a uniform jump while the nominal traction rate vector remains continuous. In this case the jump in the velocity gradient is a rank-one tensor. Cataclastic ﬂow does not involve a deformation band, so we predict the occurrence of this mode from the singularity of the tangent constitutive operator as described by Borja [6]. In this case the jump in the velocity gradient is a full-rank tensor obtained from the condition that the nominal stress rate remain continuous. We term a full-rank velocity gradient jump tensor as diﬀuse bifurcation, in contrast to ‘global bifurcation’ as used, for example, in [7]. A comparison of rank-one and full-rank velocity gradient tensors is shown in Fig. 3.

40

Ronaldo I. Borja

ISOTROPIC IMPLOSION

STRICT IMPLOSION

IMPLOSION

ISOCHORIC MODE

PURE COMPACTION BAND

COMPACTIVE SHEAR BAND

SIMPLE SHEAR BAND

(b)

(a)

Fig. 3. Eigenmodes for bifurcations leading to pore collapse for: (a) singular tangent constitutive operator; (b) singular tangent acoustic tensor, see Reference [6]

Grain crushing and pore collapse in rocks lead to a drastically diﬀerent material. For rocks experiencing shear localization, these processes are limited to a narrow zone called deformation band [8, 9]. In cataclastic ﬂow, on the other hand, grain crushing and pore collapse are pervasive throughout the entire volume. Deformation at post-collapse is dominated by continued grain fracturing, as well as by rigid body rotation and relative translation of the fractured grains and fragments. Eﬀectively, the ‘new’ material now behaves as a dense particulate medium possessing much diﬀerent constitutive properties than those of the intact rock. In this paper we also present a framework for constitutive branching to allow the constitutive model to capture the new material properties in both shear localization and cataclastic ﬂow failure regimes. Notations and symbols used in this paper are as follows: bold-faced letters denote tensors and vectors; the symbol ‘·’ denotes an inner product of two vectors (e.g. a · b = ai bi ), or a single contraction of adjacent indices of two tensors (e.g. c · d = cij djk ); the symbol ‘:’ denotes an inner product of two second-order tensors (e.g. c : d = cij dij ), or a double contraction of adjacent indices of tensors of rank two and higher (e.g. C : e = Cijkl ekl ); the symbol ‘⊗’ denotes a juxtaposition, e.g., (a ⊗ b)ij = ai bj . Finally, for any symmetric second order tensors α and β, (α ⊗ β)ijkl = αij βkl , (α ⊕ β)ijkl = αjl βik , and (α β)ijkl = αil βjk .

2 Shear Localization 2.1 E-mode for Shear Localization The condition for shear localization is given by Aep · m = 0 ,

ep Aep ij = NA AiAjB NB ,

(1)

where Aep is the elastoplastic acoustic tensor, Aep = ∂P /∂F is the ﬁrst tangential elastoplastic moduli tensor, P is the ﬁrst Piola-Kirchhoﬀ stress

Localized and Diﬀuse Bifurcations

41

tensor, F is the deformation gradient, m is the unit vector in the direction of velocity jump across the band, and N (with component NA ) is the unit normal vector to the band in the undeformed conﬁguration, see [10]. Determining the eigenmode (e-mode) provides an insight into the volume change response at bifurcation. Let J = det(F ) > 0 denote the Jacobian of the motion, with material time derivative J˙ = Jdiv v. The jump in J˙ induced by a non-unique velocity ﬁeld is given by ˙ = J˙ − J˙∗ = J div [[v]] = J tr [[l]] = J tr([[F˙ ]] · F −1 ) . [[J]]

(2)

Accordingly, we characterize the appropriate volume change mode from the following criteria: ˙ = (−) =⇒ contraction/implosion; sgn [[J]] (3) (+) =⇒ dilation/explosion. ˙ = 0 denotes an isochoric mode. The transition condition [[J]] For condition (1) to provide a non-trivial solution we must have inf{D(N ) ∈ |D(N ) = det(Aep )} = 0 ,

(4)

where we view the ﬁeld of determinants of Aep as a set function of N and we want the inﬁmum of this set to vanish at a critical orientation deﬁned by the band normal N . At this critical orientation the tensor Aep is singular and the vector m deﬁnes its e-mode. We determine the correct algebraic sign of this e-mode from the conditions described in [9, 10]. For shear localization the form of the jump tensor [[F˙ ]] is given by [[F˙ ]] = ϕm ⊗ N ,

(5)

where ϕ denotes the magnitude of the jump. Noting from Nanson’s formula that (6) n = (h/h0 )N · F −1 , where h and h0 are the band thicknesses in the deformed and undeformed conﬁgurations, respectively, then we get ˙ =J [[J]]

h h tr(m ⊗ n) = J (m · n) . h0 h0

(7)

The shear band mode is then classiﬁed as either compactive or dilative depending on the sign of the vector dot product m · n. Following [9], we classify a deformation band according to the following criteria: ⎧ ⎪ m·n=1: pure dilation band; ⎪ ⎪ ⎪ ⎪ ⎪0 < m · n < 1 : dilatant shear band; ⎨ (8) m·n=0: simple shear band; ⎪ ⎪ ⎪ −1 < m · n < 0 : compactive shear band; ⎪ ⎪ ⎪ ⎩m · n = −1 : pure compaction band.

42

Ronaldo I. Borja

Note that the above deﬁnitions only pertain to the speciﬁc mode at bifurcation. 2.2 Constitutive Branching for Shear Localization Slip weakening, a process describing the mechanical response of rocks from the onset of shear localization to the beginning of the residual state, provides a critical link between pre-localization and residual state behaviors. Developing a constitutive framework for this initial stage of slip instability requires knowledge of the residual state to which the slip weakening model will branch. For a shear band that is deforming by tangential frictional sliding we consider the classical Mohr-Coulomb friction law formulated in the Lagrangian description. Following [11], we take the nominal traction vector at material point X on the band as t = P · N , where N deﬁnes the unit band normal in the reference conﬁguration (determined from the bifurcation analysis). We can resolve this traction into normal and tangential components at the current conﬁguration as (9) t(X, t) = tN (X, t)n + tT (X, t)ξ , where n = N · F −1 /N · F −1 , and tN and tT are normal and tangential components obtained from tN = n · P · N ,

tT = tT ,

ξ = tT /tT ,

tT = t − t N n ,

(10)

assuming planar sliding (some metric transformation may be required for sliding along curvilinear surfaces). Note that tN (negative for compression) and tT are resolved nominal stresses representing forces in the current conﬁguration per unit undeformed area. Next we write the Mohr-Coulomb friction law at residual state using the format of classical plasticity. Let µ denote the coeﬃcient of friction; then we have ˙ , [[v]] = ζξ ζ˙ ≥ 0 , Φζ˙ = 0 . (11) Φ = tT + µtN ≤ 0 , In the above expressions Φ takes the role of the yield function at residual state, [[v]] is the velocity jump across the band (evaluated from a non-associative ﬂow rule), ζ˙ is the nonnegative slip rate, and the fourth expression is the ˙ = J tr[[l]] = 0, since Kuhn-Tucker condition. The band kinematics yields [[J]] [[v]] · n = 0 for a band that moves by tangential sliding. Furthermore, the ﬂow rule suggests that the velocity jump [[v]] across the band is fully plastic, consistent with results obtained for strong discontinuity kinematics [12, 13]. We can also accommodate a variable coeﬃcient of friction with this framework. For small slips and slow slip velocities the variation of the coeﬃcient of friction µ may be described by the Dieterich-Ruina law [14–16] ˙ ∗ ) + B ln(θ/θ∗ ) µ = µ∗ + A ln(ζ/V ˙ c, θ˙ = 1 − θζ/D

(12) (13)

Localized and Diﬀuse Bifurcations

43

where ζ˙ is the magnitude of [[v]], θ is a state variable, and A, B, µ∗ , V ∗ , θ∗ , and Dc are material parameters. The state variable θ has been linked to the changing set of frictional contacts and wear on the materials [16], and Dc is a characteristic slip required to replace a contact population representative of a previous sliding condition with a contact population created under a new sliding condition. For zero and near-zero slip velocities, such as what occurs near the tip of a nucleating fault, the expression for µ as given by the above logarithmic function becomes singular. To circumvent this problem we view frictional sliding as a rate process and add backward jumps in the spirit of the Arrhenius law to obtain the regularized form [17] µ = A sinh−1

ζ˙ µ∗ + B ln(θ/θ∗ ) . exp ∗ 2V A

(14)

This equation then predicts a zero coeﬃcient of friction at zero slip velocity. The above variable friction model has been implemented in the context of strong discontinuity ﬁnite elements [18, 19]. Note that for large slips and high slip velocities, such as those encountered in earthquake fault nucleation

(a)

(b)

(c) Fig. 4. Model for fault nucleation and propagation in rock: (a) fault nucleates (dashed line) over a characteristic distance; (b) slip weakening takes place over characteristic slip ζ ∗ ; (c) initially dilatant shear band becomes isochoric over a characteristic slip ζ

44

Ronaldo I. Borja (a)

(b)

Fig. 5. Slip weakening models for rocks during fault nucleation: (a) linear slip weakening resulting from a combined cohesion softening-friction hardening on an emerging fault; (b) nonlinear slip weakening. Shaded area GII represents shear fracture energy that has been correlated with the magnitude of an earthquake for regionalscale faulting, see [20]

processes, a much lower coeﬃcient of friction may be activated by additional weakening mechanisms such as ﬂash heating [17]. The concept of slip weakening leading to the above rate- and statedependent residual friction model was motivated by the cohesive zone models for tensile fracture and extended to the shear fracture problem by Ida [20] and Palmer and Rice [21]. To better understand this process we consider a rock through which a shear band (or fault) is nucleating and propagating, as shown in Fig. 4. At the bifurcation point we assume that slip begins to accumulate, as deﬁned by the integral

(15) ζ = ζ˙ dt , t

where the integration is taken over the slip path, see Fig. 4a. Figure 4b shows the resolved nominal shear stress tT decaying to a residual state value away from the tip of a propagating band, where the cumulative slip ζ has exceeded a value ζ ∗ ≈ 0.5 mm for most rocks (Rice, personal communication, see also [22]). Figure 5 further depicts this narrow region of slip weakening [20], in which tT decreases either linearly or nonlinearly with ζ (Figs. 5a and 5b, respectively). The shaded area GII represents the shear fracture energy that has been correlated by many authors with the magnitude of an earthquake. Figure 6 portrays the notion of constitutive branching during slip weakening in the context of classical elastoplasticity. Prior to bifurcation, plastic deformation of an intact rock is described by the yield function F = 0, which is assumed isotropic on the π-plane and dependent on all three principal Kirchhoﬀ stresses. A deformation band-type bifurcation is detected at point A, and consequently the constitutive theory branches to the slip weakening law Φ = tT − c + µtN = 0 .

(16)

Localized and Diﬀuse Bifurcations

45

A

B

Fig. 6. Slip weakening on the π-plane in principal Kirchhoﬀ stress space. Yield surface for intact rock F = 0 branches at the bifurcation stress point A to the Mohr-Coulomb failure criterion Φ = 0 for a planar fault; at residual state B the cohesion decays to zero and the failure criterion passes through the origin

This equation plots as a straight line on the π-plane. However, the slip velocity is zero at the bifurcation point, so µ = 0 initially, and the shear resistance is then purely cohesive. As slip accumulates the coeﬃcient of friction µ quickly increases while the cohesion c decays to zero. During this time tN may also vary, and the slip weakening law then plots as a fan of straight lines on the π-plane. At the conclusion of slip weakening the cohesion is zero and the shear resistance is purely frictional; hence, the straight line passes through the origin of the π-plane. This interplay between the cohesive and frictional resistances is also shown in Fig. 5a. Assuming the shear resistance on the band is purely frictional and the slipweakening constitutive law is linear, we can write an ‘eﬀective yield function’ of the form ζ ζ ∈ [ 0, ζ ∗ ] , (17) Φ = tT − t◦T − (t◦T + µt∗N ) ∗ ≤ 0 , ζ where Φ = 0 now describes a linear slip weakening. However, the condition Φ = 0 is not a trivial linear constraint to impose since t∗N is unknown during the slip weakening process. A ﬁrst-order approximation may be obtained by assuming t∗N ≈ tN [18], in which case (17) reduces to the form ζ Φ = tT − t◦T − (t◦T + µtN ) ∗ ≤ 0 , ζ

ζ ∈ [ 0, ζ ∗ ] .

(18)

This equation predicts a nonlinear slip weakening similar to Fig. 5b for the case of a variable tN , and recovers a linear slip weakening for the case of a constant tN , see [18, 19] for further details.

46

Ronaldo I. Borja

3 Cataclastic Flow 3.1 E-mode for Cataclastic Flow The condition for stationary stress rate is given by [[P˙ ]] = Aep : [[F˙ ]] = 0 .

(19)

For a non-trivial solution [[F˙ ]] = 0 to exist, we must have det(Aep ) = 0 .

(20)

The e-mode in this case is the jump tensor [[F˙ ]]. Borja [6] provides details on how the correct sign of this e-mode may be determined. To further characterize the e-mode associated with condition (19), we write τ = P · Ft ,

(21)

where τ is the symmetric Kirchhoﬀ stress tensor. Taking the jumps in the rates gives (22) [[τ˙ ]] = P · [[F˙ ]]t + [[P˙ ]] · F t . Noting that [[P˙ ]] = 0 and [[F˙ ]] = [[l]] · F at bifurcation, we get [[τ˙ ]] = (τ 1) : [[l]] ,

(23)

where (τ 1)ijkl = τil δjk and δjk is the Kronecker delta. Now, consider a rate constitutive equation of the form [10] τ˙ = αep : l ,

(24)

where αep is a rank-four spatial elastoplastic tangential moduli tensor with minor symmetry on its ﬁrst two indices. This yields an eigenvalue problem aep : [[l]] = 0 ,

aep = αep − τ 1 .

(25)

Thus, Aep is singular whenever aep is singular. The singularity of aep is of three types [23], and here we shall consider only the one relevant to pore collapse instability. We recall the polar decomposition of the deformation gradient F and spectral decomposition of the left stretch tensor V , 3 λA m(A) , (26) F = V ·R, V = A=1 (A)

(A)

(A)

where m = n ⊗ n , R is a proper orthogonal rotation tensor, λA are the principal stretches, and n(A) are the principal directions of V . Taking the time derivative gives ˙ , F˙ = V˙ · R + V · R (27)

Localized and Diﬀuse Bifurcations

where V˙ =

3

λ˙ A m(A) +

A=1

3

ωAB (λB − λA )m(AB) ,

47

(28)

A=1 B=A

m(AB) = n(A) ⊗ n(B) , and ωAB is the spin of the (Eulerian) principal axes of V. The velocity gradient can be expressed in the form l = F˙ · F −1 = V˙ · V −1 + V · Ω · V −1 ,

˙ · Rt . Ω=R

(29)

Using the spectral forms and taking the jumps gives [[l]] =

3

[[ε˙A ]]m(A)

(30)

A=1

+

3 λA (AB) λA , + [[wAB ]] m [[ωAB ]] 1 − λB λB

(31)

A=1 B=A

where wAB = Ω : m(AB) and εA = ln λA is the principal logarithmic stretch. Note that wAB arises from the ﬁnite rotation of the stretch tensor V whereas ωAB describes the spin of the principal axes of V ; the former vanishes in the inﬁnitesimal theory whereas the latter generally does not. The particular e-mode of interest is characterized by [[ωAB ]] = [[wAB ]] = 0, where the volume simply implodes at ﬁxed principal directions. In this case the jump in the velocity gradient [[l]] is equal to the jump in the rate of deformation [[d]] (since the spins are ‘frozen’), and the relevant jump tensor becomes 3 [[ε˙A ]]m(A) . (32) [[l]] = [[d]] = A=1

By a simple tensor manipulation the jumps in the principal logarithmic stretch rates, characterizing the e-mode at bifurcation, may be obtained from the eigenvalue problem 3 aep (33) AB [[ε˙B ]] = 0 , A=1

where

(A) aep : aep : m(B) AB = m

(34)

is a 3 × 3 matrix of elastoplastic moduli, which also includes the initial stress terms arising from ﬁnite deformation eﬀects. Pore collapse is characterized by the condition 3 [[ε˙A ]] < 0 . (35) A=1

Note that the e-mode predicted above is diﬀuse in the sense that it does not entail the formation of a deformation band.

48

Ronaldo I. Borja

3.2 Constitutive Branching for Cataclastic Flow As in classical continuum plasticity we consider yield and plastic potential functions, Φ and Ψ , respectively, representing yield behavior of the compacted material at the conclusion of cataclastic ﬂow. We assume that these functions depend on the Kirchhoﬀ stress tensor τ and some plastic internal variable κ. By multiplicative plasticity we write the velocity gradient as the sum of elastic and plastic parts, (36) l = le + lp , where and

le = F˙ e · F e−1 p Lp = F˙ · F p−1 .

lp = F e · Lp · F e−1 , p

(37)

p

(38)

p

Ignoring plastic spin, we have l = sym(l ) := d , and the ﬂow rule thus gives ˙ , dp = λq

q=

∂Ψ . ∂τ

(39)

Φ(τ , κ)λ˙ = 0 ,

(40)

Subject to the usual Kuhn-Tucker conditions Φ(τ , κ) ≤ 0 ,

λ˙ ≥ 0 ,

along with an appropriate hardening law, we have thus formulated a constitutive model appropriate for the ‘new’ material at post-cataclasis. It has been reported [1] that cataclastic ﬂow is only a transient behavior. When the pores have collapsed and the compacted material is loaded further, any subsequent deformation could result in a net dilatancy leading to strain localization. For porous quartzite this occurs at nominal axial strains greater than about 25%. This suggests that constitutive models for a porous but intact rock, initially exhibiting compactive tendencies, should branch to a model exhibiting dilative tendencies at the conclusion of cataclastic ﬂow. During this time the eﬀective cohesion exhibited by the intact rock decays to a near-zero value while the eﬀective frictional strength increases with increased compaction. Interestingly, these features are analogs of those encountered in the development of the slip weakening model of the previous section, with the exception that they now apply to the bulk response of the material. For a more concrete illustration, we assume the following form of the yield function to which the constitutive response branches at the onset of cataclastic ﬂow: f1 = I 13 /I 3 , (41) Φ = (f1 − 27)(I 1 /pa )m − κ ≤ 0 , where I1 = τ 1 + τ 2 + τ 3 ,

I 3 = τ 1τ 2τ 3

(42)

Localized and Diﬀuse Bifurcations

49

q

p A

B Fig. 7. Yield surface for intact rock F = 0 branches at the bifurcation stress point A into yield surface Φ(τ , κ) = 0 signifying onset of cataclastic ﬂow. Post-bifurcation yield surface undergoes cohesion softening-friction hardening. Transient cataclastic ﬂow concludes at stress point B where the compacted continuum can now potentially undergo shear localization with plastic dilatancy

are, respectively, the ﬁrst and third invariants of the translated principal Kirchhoﬀ stresses τ 1 = τ1 − a ,

τ 2 = τ2 − a ,

τ 3 = τ3 − a ,

(43)

a > 0 is a stress shift on the hydrostatic axis to account for cohesion, and pa is the atmospheric pressure (a normalizing constant). The exponent m is a given parameter describing the curvature of the surface on a meridian plane (straight line for m = 0), and κ is the slope that varies with the frictional yield strength. Lade [24] utilizes this function to characterize yielding of dense sands. The yield function described above has the shape of an asymmetric bullet with the pointed apex initially on the tensile side of the hydrostatic axis (Fig. 7) and initially coinciding with the apex of the yield surface for the intact rock, which is represented in the same ﬁgure by the boundary of the region with a compression cap. Cataclastic ﬂow-type bifurcation occurs at point A, and by requiring that Φ = 0 for this given stress state we obtain the initial value κ0 of the frictional parameter κ. Cohesion softening during cataclastic ﬂow is simulated by a degrading value of a, while friction hardening is captured by an increasing value of κ.

4 Transient Plastic Flow During slip weakening and cataclastic ﬂow, the directions of plastic ﬂow evolve from those predicted at bifurcation to those attained at residual state. To capture the evolution during these ‘transient’ conditions we can interpolate these

50

Ronaldo I. Borja

plastic ﬂow directions to satisfy the initial (bifurcation) and ﬁnal (residual) states. 4.1 Slip Weakening The region of interest is 0 ≤ ζ ≤ ζ , as shown in Fig. 4c. Inside this region the velocity jump [[v]] evolves from being parallel to m at bifurcation to being parallel to ξ when the fault begins to deform by pure tangential sliding. Interpolating linearly with ζ (as a ﬁrst-order approximation), we get ˙ ⊗N, [[F˙ ]] = ζb

(44)

where

ζ ζ β , β = 1 − m + ξ. β ζ ζ The corresponding jump in velocity gradient is b=

h0 [[l]] = [[F˙ ]] · F −1 = ζ˙ b ⊗ n . h It follows that the jump in the Jacobian rate is ˙ = Jtr[[l]] = ζ˙ J h0 1 − ζ m · n . [[J]] β h ζ

(45)

(46)

(47)

˙ = 0 when ζ = ζ , so at this level of deformation any initial This yields [[J]] dilation or compaction of the band will cease and subsequent motion will be characterized by pure tangential sliding. 4.2 Cataclastic Flow The region of interest is J1 ≤ J ≤ J0 , where J0 is the value of the Jacobian at the bifurcation point and J1 is the value at the conclusion of cataclastic ﬂow. It is ﬁtting that in this case we select J as our parameter since we are concerned with pore collapse instability and J is a measure of volume change. At the bifurcation stress we take the e-mode as the instantaneous plastic ﬂow direction, 3 p ˙ [[ε˙A ]]m(A) , J = J0 . (48) d0 = λ A=1

At the conclusion of cataclastic ﬂow the plastic ﬂow direction is given by the ﬂow rule ∂Ψ , J = J1 . (49) dp1 = λ˙ ∂τ A linear interpolation gives dp =

J − J1 p J0 − J p d + d , J0 − J1 0 J0 − J1 1

J1 ≤ J ≤ J0 .

(50)

Localized and Diﬀuse Bifurcations

51

Of course, other forms of interpolation are possible provided they satisfy the two end conditions. We emphasize that both slip weakening and cataclastic ﬂow are micromechanical processes. The plastic ﬂow theory presented in this section should thus be interpreted simply as a rough approximation of the micromechanical phenomena and not as a faithful description of the grain-scale ﬂow processes taking place during these transient periods of instability.

5 Closure We have presented a framework for mathematical modeling of shear localization and cataclastic ﬂow in porous rocks. Classical bifurcation theory provides conditions for the occurrence of these two instability modes, in which shear localization is equated to a singular acoustic tensor whereas cataclastic ﬂow is equated to a singular tangent constitutive operator. For general 3D kinematics, the corresponding e-modes are given by velocity gradient jump tensors of ranks one and three, respectively. We have also proposed a framework for constitutive branching to allow the model to capture post-bifurcation responses. Slip weakening provides a critical link to modeling post-shear localization in rocks. The process is captured by a cohesion softening-friction hardening law applied to the nucleating fault plane. A similar cohesion softening-friction hardening law has been proposed for bifurcation leading to cataclastic ﬂow, except that the law is applied to the bulk constitutive response.

Acknowledgements The author is grateful to Professor James R. Rice of Harvard University and Professor Teng-fong Wong of State University of New York at Stony Brook for discussions on the basic issues of slip weakening and cataclastic ﬂow addressed in this paper, as well as for providing numerous references relevant to this work. Discussions with Professors David Pollard and Atilla Aydin of Stanford University also helped elucidate the processes and mechanisms of rock deformation addressed in this work. Graduate student Joshua White assisted in the preparation of the manuscript. This work has been supported in part by the U.S. National Science Foundation, Grant No. CMG-0417521 (Collaborations in Mathematical Geosciences) and the U.S. Department of Energy Grant No. DE-FG02-03ER15454.

References [1] Hirth G, Tullis J (1989) The eﬀects of pressure and porosity on the micromechanics of the brittle-ductile transition in quartzite. Journal of Geophysical Research 94:17825–17838

52

Ronaldo I. Borja

[2] Men´endez B, Zhu W, Wong TF (1996) Micromechanics of brittle faulting and cataclastic ﬂow in Berea sandstone. Journal of Structural Geology 18:1–16 [3] Tullis J, Yund R (1992) The brittle-ductile transition in feldspar aggregates: An experimental study. In B. Evans and T.F. Wong, editors, Fault mechanics and transport properties of rocks. Cambridge University Press, United Kingdom, [4] Wong TF, David C, Zhu W (1997). The transition from brittle faulting to cataclastic ﬂow in porous sandstones: Mechanical deformation. Journal of Geophysical Research 102:3009–3025 [5] Rudnicki JW, Rice JR (1975) Conditions for localization of deformation in pressure-sensitive dilatant materials. Journal of the Mechanics and Physics of Solids 23:371394 [6] Borja RI (2006) Conditions for instabilities in collapsible solids including volume implosion and compaction banding. Acta Geotechnica, in press [7] Chau K, Rudnicki JW (1990) Bifurcations of compressible pressuresensitive materials in plane strain tension and compression. Journal of the Mechanics and Physics of Solids 38:875–898 [8] Aydin A, Borja RI, Eichnubl P (2006) Geological and mathematical framework for failure modes in granular rock. Journal of Structural Geology 28:83–98 [9] Borja RI, Aydin A (2004) Computational modeling of deformation bands in granular media. I. Geological and mathematical framework. Computer Methods in Applied Mechanics and Engineering 193:26672698 [10] Borja RI (2002) Bifurcation of elastoplastic solids to shear band mode at ﬁnite strains. Computer Methods in Applied Mechanics and Engineering 191:52875314 [11] Laursen TA, Simo JC (1993) A continuum-based ﬁnite element formulation for the implicit solution of multibody, large deformation frictional contact problems. International Journal for Numerical Methods in Engineering 36:3451-3485 [12] Borja RI (2000) A ﬁnite element model for strain localization analysis of strongly discontinuous ﬁelds based on standard Galerkin approximations. Computer Methods in Applied Mechanics and Engineering 190:1529–1549 [13] Borja RI (2002) Finite element simulation of strain localization with large deformation: Capturing strong discontinuity using a Petrov-Galerkin multiscale formulation. Computer Methods in Applied Mechanics and Engineering 191:2949–2978 [14] Dieterich JH (1979) Modeling of rock friction 1. Experimental results and constitutive equations. Journal of Geophysical Research 84:2161–2168 [15] Ruina AL (1983) Slip instability and state variable friction laws. Journal of Geophysical Research 88:10359–10370

Localized and Diﬀuse Bifurcations

53

[16] Dieterich JH, Kilgore BD (1996) Imaging surface contacts: Power law contact distributions and contact stresses in quartz, calcite, glass and acrylic plastic. Tectonophysics 256:219–239 [17] Lapusta N, Rice JR, Ben-Zion Y, Zheng G (2000) Elastodynamic analysis for slow tectonic loading with spontaneous rupture episodes on faults with rate- and state-dependent friction. Journal of Geophysical Research 105:23765–23789 [18] Borja RI, Foster CD (2006) Continuum mathematical modeling of slip weakening in geological systems. Journal of Geophysical Research, in review. [19] Foster CD, Borja RI, Regueiro RA (2006) Embedded strong discontinuity ﬁnite elements for fractured geomaterials with variable friction. International Journal for Numerical Methods in Engineering, in review. [20] Ida Y (1972) Cohesive force across the tip of a longitudinal shear crack and Griﬃth’s speciﬁc surface energy. Journal of Geophysical Research 77:3796–3805 [21] Palmer AC, Rice JR (1973) The growth of slip surfaces in the progressive failure of overconsolidated clay. In Proceedings of the Royal Society of London Ser. A332, pp. 527–548 [22] Wong TF (1982) Shear fracture energy of Westerly granite from postfailure behavior. Journal of Geophysical Research 87:990–1000 [23] Ogden RW (1984) Nonlinear Elastic Deformations. Chichester, Ellis Horwood [24] Lade PV (1977) Elasto-plastic stress-strain theory for cohesionless soil with curved yield surfaces. International Journal of Solids and Structures 13:1019–1035

Dispersion and Localisation in a Strain–Softening Two–Phase Medium Ren´e de Borst1,2 and Marie-Ang`ele Abellan3 1

2 3

Delft University of Technology, Faculty of Aerospace Engineering, Kluyverweg 1, Delft, The Netherlands [email protected] LaMCoS, UMR CNRS 5514, INSA de Lyon, 69621 Villeurbanne, France LTDS-ENISE, UMR CNRS 5513, ENISE, 42023 Saint-Etienne, France

Summary. In fluid–saturated media wave propagation is dispersive, but the associated internal length scale vanishes in the short wave–length limit. Accordingly, upon the introduction of softening, localisation in a zero width will occur and no regularisation is present. This observation is corroborated by numerical analyses of wave propagation in a finite one–dimensional bar.

1 Introduction Strain softening and the ensuing phenomenon of localisation have been the subject of profound investigations in the past two decades. While, initially, the incorporation of strain softening in constitutive equations was considered to be a straightforward exercise, it soon appeared that the use of strain-softening models led to an excessive dependency of the solution on the discretisation in numerical analyses. At ﬁrst, deﬁciencies in the numerical methods were believed to cause this severe mesh dependency. However, it was demonstrated that the underlying cause was the local change of character of the partial diﬀerential equations that govern the initial/boundary value problem: from elliptic to hyperbolic for quasi–static problems and from hyperbolic to elliptic in dynamic problems. This local change of character renders the initial/boundary value ill–posed, unless special interface conditions are imposed between both regimes. For ill–posed problems, numerical methods, including ﬁnite element methods, still try to capture ‘the best possible’ solution, but this solution changes for every other discretisation. To repair this ill–posedness, several proposals have been put forward. Invariably, the aim is to enrich the continuum description to include more of the underlying physical properties of the material, such as grain rotations in granular materials — the Cosserat continuum approach, e.g. [1, 2] —, the incorporation of viscosity or rate–dependency, e.g. [3, 4], or nonlocal approaches which reﬂect medium and long–range forces which emerge in materials where Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 55–66. © 2007 Springer. Printed in the Netherlands.

56

Ren´e de Borst and Marie-Ang`ele Abellan

the heterogeneity is in the same order of magnitude as the fracture process zone [5, 6, 7, 8]. While these ideas have been suggested and elaborated for single–phase media, they are also eﬀective for multi–phase media, such as ﬂuid–saturated porous solids, e.g. [9]. The question has arisen whether the diﬀusive character of the movement of the ﬂuid in such a medium already provides a physically based regularisation mechanics. Indeed, it has already been shown by Biot [10], see also Loret and co-workers [11, 12] that wave propagation in such a medium is dispersive, and, accordingly, that an internal length scale must exist. This issue has been debated intensely in recent years [13, 14, 15, 16, 17]. In a previous contribution [17], we have demonstrated that stability in a ‘standard’ two–phase medium is assured until the tangent modulus ceases to be positive, at least in a one–dimensional medium and for a normal range of material parameters. Thus, the stability condition coincides with that of a single–phase medium. Moreover, it was shown by an analysis of dispersive waves that the length scale associated with wave dispersion vanishes in the short wave–length limit. In this contribution, we supplement the previous analysis by a more comprehensive study in which the momentum balance in the ﬂuid is kept explicitly in the analysis, which enables the identiﬁcation of the second wave speed in the mixture. The main conclusion of the previous study, namely that the length scale associated with wave dispersion vanishes in the short wave–length limit, so that no regularisation exists, is corroborated by the present analysis, and therefore put on a solid basis.

2 Governing Equations We consider a two–phase medium subject to the restriction of small displacement gradients and small variations in the concentrations [18]. Furthermore, the assumptions are made that there is no mass transfer between the constituents and that the processes which we consider, occur isothermally. With these assumptions, the balances of linear momentum for the solid and the ﬂuid phases read: ˆ π + ρπ g = ∇ · σπ + p

∂(ρπ vπ ) + ∇(ρπ vπ ⊗ vπ ) ∂t

(1)

with σ π the stress tensor, ρπ the apparent mass density, and vπ the absolute velocity of constituent π. As in the remainder of this paper, π = s, f , with s and f denoting the solid and ﬂuid phases, respectively. Further, g is the ˆ π is the source of momentum for constituent π gravity acceleration and p from the other constituent, which takes into account the possible local drag interaction between the solid and the ﬂuid. Evidently, the latter source terms must satisfy the momentum production constraint: ˆπ = 0 (2) p π=s,f

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

57

We now neglect convective terms and the gravity acceleration, so that the momentum balances reduce to: ˆ π = ρπ ∇ · σπ + p

∂vπ ∂t

(3)

Adding both momentum balances, and taking into account Eq.(2), one obtains the momentum balance for the mixture: ∇ · σ s + ∇ · σ f − ρs

∂vs ∂vf − ρf =0 ∂t ∂t

(4)

where σ f = −αpI

(5)

with p the ﬂuid pressure, I the second–order identity tensor, and α the Biot coeﬃcient, cf. [19]. Substitution of Eq.(5) into the momentum balance of the mixture gives: ∂vs ∂vf − ρf =0 (6) ∇ · σ s − α∇p − ρs ∂t ∂t In a similar fashion as for the balances of momentum, one can write the balance of mass for each phase as: ∂ρπ + ∇ · (ρπ vπ ) = 0 ∂t

(7)

Again neglecting convective terms, the mass balances can be simpliﬁed to give: ∂ρπ + ρπ ∇ · vπ = 0 (8) ∂t We multiply the mass balance for each constituent π by its volumic ratio nπ , add them and utilise the constraint nπ = 1 (9) π=s,f

to give: ∇ · vs + nf ∇ · (vf − vs ) +

nf ∂ρf ns ∂ρs + =0 ρs ∂t ρf ∂t

(10)

The change in the mass density of the solid material is related to its volume change by: Ks nf ∂ρs (11) ∇ · vs = − Kt ρs ∂t with Ks the bulk modulus of the solid material and Kt the overall bulk modulus of the porous medium. Using the deﬁnition of the Biot coeﬃcient, 1 − α = Kt /Ks [19], this equation can be rewritten as (α − 1)∇ · vs =

nf ∂ρs ρs ∂t

(12)

58

Ren´e de Borst and Marie-Ang`ele Abellan

For the ﬂuid phase, a phenomenological relation is assumed between the incremental changes of the apparent ﬂuid mass density and of the ﬂuid pressure [19]: nf 1 dp = dρf (13) Q ρf with the overall compressibility, or Biot modulus α − nf 1 nf = + Q Ks Kf

(14)

where Kf is the bulk modulus of the ﬂuid. Inserting relations (12) and (13) into the balance of mass of the total medium, Eq.(10), gives: α∇ · vs + nf ∇ · (vf − vs ) +

1 ∂p =0 Q ∂t

(15)

The governing equations, i.e. the balance of momentum of the saturated medium, Eq.(6), that of the ﬂuid, Eq.(3) with π = f , and the balance of mass, Eq.(15), are complemented by the kinematic relation, s = ∇s us

(16)

with us , s the displacement and strain ﬁelds of the solid, respectively, the superscript s denoting the symmetric part of the gradient operator, and an incrementally linear stress–strain relation for the solid skeleton, σ˙ s = Dtan : ˙ s

(17)

tan

where D is the fourth–order tangent stiﬀness tensor of the solid material and the superimposed dot denotes diﬀerentiation with respect to a virtual time. For the pore ﬂuid ﬂow, Darcy’s relation for isotropic media is assumed to hold, (18) nf (vf − vs ) = −kf ∇p with kf the permeability coeﬃcient of the porous medium, and deﬁnes the drag force of the solid on the ﬂuid: ˆ f = −nf kf−1 (vf − vs ) p

(19)

The boundary conditions nΓ · σ = tp ,

v = vp

(20)

hold on complementary parts of the boundary ∂Ωt and ∂Ωv , with Γ = ∂Ω = ∂Ωt ∪ ∂Ωv , ∂Ωt ∩ ∂Ωv = ∅, tp being the prescribed external traction and vp the prescribed velocity, and nf (vf − vs ) = qp ,

p = pp

(21)

hold on complementary parts of the boundary ∂Ωq and ∂Ωp , with Γ = ∂Ω = ∂Ωq ∪ ∂Ωp and ∂Ωq ∩ ∂Ωp = ∅, qp and pp being the prescribed outﬂow of pore ﬂuid and the prescribed pressure, respectively.

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

59

3 Reduction of the Governing Equations Henceforth, we shall consider the problem of a uniaxially stressed homogeneous bar. Then, vsx = 0, vsy = 0, vsz = 0 and the momentum balances for the mixture and for the ﬂuid reduce to: ∂p ∂σs ∂vs ∂vf −α − ρs − ρf =0 (22) ∂x ∂x ∂t ∂t where for notational simplicity the subscript x has been dropped and σs denotes the axial stress in the solid, and ∂p ∂vf + nf kf−1 (vf − vs ) + ρf =0 (23) ∂x ∂t respectively. From Eq.(23) we observe that Eq.(19) has been used as the source of momentum for the ﬂuid from the solid phase. The mass balance of the mixture, Eq.(15) becomes: ∂vs ∂p ∂vs ∂vf + nf − + Q−1 =0 (24) α ∂x ∂x ∂x ∂t α

To allow for inelastic constitutive equations, we take the incremental format of Eqs.(22)–(24): ∂ p˙ ∂ v˙ s ∂ v˙ f ∂ σ˙ s −α − ρs − ρf =0 (25) ∂x ∂x ∂t ∂t ∂ p˙ ∂ v˙ f + nf kf−1 (v˙ f − v˙ s ) + ρf =0 (26) α ∂x ∂t and ∂ v˙ s ∂ v˙ s ∂ p˙ ∂ v˙ f α + nf − + Q−1 =0 (27) ∂x ∂x ∂x ∂t We will observe in the next section, where, using an analysis of wave dispersion in this medium, the localisation properties are derived, that the ensuing equations are rather complicated. For this reason, in [17] the pressure p was eliminated from the above equations by inserting Darcy’s relation explicitly in the balances of momentum and mass for the mixture. For the momentum balance this results in: ∂vs ∂vf ∂σs + αnf kf−1 (vf − vs ) − ρs − ρf =0 (28) ∂x ∂t ∂t The mass balance, Eq.(24) is ﬁrst diﬀerentiated with respect to x. Interchanging the order of spatial and temporal diﬀerentiation and inserting Darcy’s relation then results in: 2 ∂vs ∂ 2 vs ∂ 2 vs ∂ vf ∂vf −1 − =0 (29) − n α 2 + nf − (k Q) f f ∂x ∂x2 ∂x2 ∂t ∂t The above two equations solely have the velocity in the solid, vs , and that in the ﬂuid, vf , as unknowns. They are better amenable to analytical manipulations. However, the reduction to two equations makes that the velocity of the wave in the ﬂuid is no longer contained in the set of equations.

60

Ren´e de Borst and Marie-Ang`ele Abellan

4 Dispersion Analysis In a strain–softening medium the presence of a non-vanishing internal length scale that arises from physical properties of the system, is directly related to the well–posedness of the initial value problem. A method for the quantiﬁcation of this internal length scale is to investigate the dispersive properties of wave propagation. Wave propagation is called dispersive when harmonics propagate with diﬀerent velocities [20]. Since a wave is composed of diﬀerent harmonics, the shape of a dispersive wave can then change upon propagation. The ability to transform the shape of waves is a necessary condition for continua to properly capture localisation phenomena, since it is otherwise impossible that the shape of an arbitrary loading wave is changed into a stationary wave with for instance a sinusoidal shape in the localisation zone. On the other hand, dispersivity of loading waves in a strain–softening medium is not a suﬃcient condition for localisation to be captured in a zone of ﬁnite size, and thus, for the initial value problem to be regularised. As said, such a regularisation will only be present if, in addition to dispersivity, a non-vanishing internal length scale can be identiﬁed. To analyse the characteristics of wave propagation in the two–phase medium, a damped, harmonic wave is considered: ⎞ ⎛ ⎞ ⎛ As δ u˙ s ⎝ δ u˙ f ⎠ = ⎝ Af ⎠ exp (ikx + λt) (30) δ p˙ Ap where As , Af , Ap are the amplitudes of the perturbations for the displacement ˙ respectively, rates in the solid, u˙ s , in the ﬂuid, u˙ f , and for the pressure rate, p, while k is the wave number. The eigenvalue λ = λr −iω can have a real component λr , which characterises the damping properties of the propagating wave, and an imaginary component ω, which is the angular frequency. Substitution of the ﬁrst of these equations into the one–dimensional versions of the kinematic relation (16) and the incremental stress–strain relation (17) yields after diﬀerentiation with respect to x: ∂ σ˙ s = −E tan As k 2 exp (ikx + λt) ∂x

(31)

with E tan the tangential stiﬀness modulus of the solid. Substitution of this relation and the perturbation (30) into Eqs.(25) – (27) yields: −E tan k 2 As − iαkAp − ρs λ2 As − ρf λ2 Af = 0 iαkAp + nf kf−1 λAf − nf kf−1 λAs + ρf λ2 Af = 0 2

2

−1

(nf − α)λk As − nf λk Af + iQ

kλAp = 0

(32)

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

61

A non–trivial solution to this set of homogeneous equations exists if and only if: tan 2 E k + ρs λ2 ρf λ2 iαk −nf k −1 λ nf k −1 λ + ρf λ2 iαk = 0 (33) f f (nf − α)k −nf k iQ−1 from which the characteristic equation for the eigenvalues λ derives in a straightforward manner as: λ4 + aλ3 + bk 2 λ2 + ck 2 λ + dk 4 = 0 with a= b= c=

nf kf−1 (ρs + ρf ) ρs ρf

nf ρs αQ + ρf E tan ρs ρf

nf kf−1 (E tan + α2 Q) ρs ρf d=

nf αQE tan ρs ρf

(34)

(35a) (35b) (35c) (35d)

Decomposing Eq.(34) into real and imaginary parts leads to: λ4r + aλ3r + (bk 2 − 6ω 2 )λ2r + (ck 2 − 3aω 2 )λr + dk 4 − bω 2 k 2 + ω 4 = 0 and

(a + 4λr )ω 2 − 4λ3r − 3aλ2r − 2bk 2 λr − ck 2 = 0

(36) (37)

From the latter equation the phase velocity can formally be deduced as: ω 1 cf = = (4k −2 λ3r + 3ak −2 λ2r + 2bλr + c) (38) k a + 4λr Evidently, wave propagation is dispersive, since Eq.(38) is such that the phase velocity cf is dependent on the wave number k, cf. [10, 11, 12, 13, 14, 15, 16]. Taking the long wave–length limit in Eqs.(36) and (37) by letting k → 0, and eliminating ω yields the following sixth-order equation in λr : λ3r (8λ3r + 12aλ2r + 6a2 λr + a3 ) = 0

(39)

which has two triple roots: λr = 0 and λr = − 12 a. Substitution of the ﬁrst root in Eq.(37) gives for the long–wave limit aω 2 = ck 2 , so that with Eqs.(35–a) and (35–c), the phase velocity in the mixture is obtained as:

E tan + α2 Q (40) cf = ρs + ρf

62

Ren´e de Borst and Marie-Ang`ele Abellan

This expression is identical to that which has been found by an analysis of the reduced equations (28)–(29). The second wave speed is obtained by substituting the second independent root λr = − 21 a into Eq.(37), which results in cf = (b − c/a) − (a/2k)2 . For k → 0 this expression becomes imaginary, and harmonics with small wave numbers cannot propagate. The cut-oﬀ wave number below which harmonics cannot propagate is given by k = a3 /(ab − c). This situation is somewhat reminiscent of some gradient–enhanced plasticity models [21]. For the short wave-length limit, i.e. when k → ∞, we assume, inspired by the closed-form solution of the reduced equations (28)–(29), a general form for the damping coeﬃcient as λr ∼ −k n , n > 1. Substitution of this identity into Eq.(38) and taking k → ∞ yields that cf → k n−1 . In analogy with a single– phase, rate–dependent medium [4], an internal length scale can be deﬁned as: cf ∼ lim k −1 = 0 (41) l = lim − k→∞ k→∞ λr which indicates that the internal length scale l vanishes in the short wave– length limit. Again, this result is in agreement with earlier analyses using the reduced set of equations [17]. The observation that in a ﬂuid–saturated medium a non–vanishing physical internal length scale cannot be identiﬁed for the short–wave length limit, is diﬀerent from the situation in a rate–dependent single–phase medium [4]. The lack of a non–vanishing physical internal length scale in the present case causes that in numerical analyses the grid spacing takes the role of the internal length scale and localisation necessarily occurs between two neighbouring grid points. Evidently, this leads to a dependence of the solution on the discretisation, as is the case for localisation in the underlying strain–softening, single–phase continuum.

5 Numerical Examples To verify and elucidate the theoretical results of the preceding section, a ﬁnite diﬀerence analysis has been carried out. The spatial derivatives in Eqs.(28) and (29) have been approximated with a second–order accurate ﬁnite diﬀerence scheme. Explicit forward ﬁnite diﬀerences have been used to approximate the temporal derivatives, which is ﬁrst-order accurate. The choice for a fully explicit time integration scheme was motivated by the analysis of Benallal and Comi [16], in which they showed that in this case no numerical length scale was introduced in the analysis, apart from the grid spacing. As implied in Eqs.(28) and (29) the velocities vs and vf of the solid skeleton and the ﬂuid have been taken as fundamental unknowns and the displacements have been obtained by integration. This scheme may not be the most accurate, but it suﬃces to provide the numerical evidence needed to support the analytical ﬁndings of the preceding section.

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

σ

σ

σ0

σy

εu ε

t

t0

63

Fig. 1. Applied stress as function of time (left) and local stress–strain diagram (right)

strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 2. Strain profiles along the bar for 101 grid points and time step ∆t = 0.5·10−3 s

All calculations have been carried out for a bar with a length L = 100 m. For the solid material, a Young’s modulus E = 20 GP a and an absolute mass density ρs = ρs /ns = 2000 kg/m3 have been assumed. For the ﬂuid, an absolute mass density ρf = ρf /nf = 1000 kg/m3 was adopted and a compressibility modulus Q = 5 GP a was assumed. As regards the porosity, a value nf = 0.3 was adopted and in the reference calculations α = 0.6 and the permeability kf = 10−10 m3 /N s. In all cases, the external compressive stress was applied according to the scheme shown in Fig. 1, with a rise time t0 = 0.05 s to reach the peak level σ0 = 1.5 M P a. In the reference calculations a time step ∆t = 0.5 · 10−3 s was adopted, which is about half the critical time step for this explicit scheme. The results of the reference calculation are shown in Fig. 2 in terms of the strain proﬁle along the bar for t = 0.1, 0.2, 0.3, 0.4, 0.5, 0.6, 0.7, 0.8, 0.9, 0.95 s. For the above set of parameters, the phase velocity for the long wave– length limit is captured exactly. In line with this expression, a variation of the permeability kf does not inﬂuence the phase velocity. Also, the inﬂuence of α according to Eq.(40) was correctly reproduced, as was veriﬁed by varying

64

Ren´e de Borst and Marie-Ang`ele Abellan strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 3. Strain profiles along the bar for 126 grid points and time step ∆t = 0.5·10−3 s

α between 0 and 1. In all cases the maximum error with respect to the phase velocity remained within 3%. Upon reﬂection at the right boundary, the stress intensity doubles and the stress in the solid exceeds the yield strength σy = 2.5 M P a and enters a linear descending branch with an ultimate strain u = 1.125 · 10−3 , see Fig. 1. Figure 2 shows that a Dirac–like strain distribution develops immediately upon wave reﬂection. This is logical, since a two–phase medium with neither constituent being equipped with viscosity in its constitutive model, does not have regularising properties. To further strengthen this observation the analysis was repeated with a slightly reﬁned mesh (126 grid points), which resulted in a marked increase of the localised strain (Fig. 3, which has been plotted on the same scale as the results of the original discretisation in Fig. 2). In dynamic calculations of softening media without regularisation, not only the spatial discretisation strongly inﬂuences the results, but also the time discretisation [16]. This is exempliﬁed in Fig. 4 for a time step that is only 20% smaller than the time step used in the reference calculation.

6 Concluding Remarks In two–phase media waves propagation is dispersive. However, in the short wave–length limit, the physical internal length scale disappears. Since this limiting case governs the development of localisation in a zone of ﬁnite width after the onset of strain softening, regularising properties, which are directly related to the existence of a non–vanishing internal length scale, are absent. This conclusion is corroborated by the results of numerical analyses of wave propagation in a ﬁnite one–dimensional bar, which show that, upon the introduction of a softening stress–strain relation for the solid constituent, strain

Dispersion and Localisation in a Strain–Softening Two–Phase Medium

65

strain [x 0.0001]

6

5

4

3

2

1

0

10

20

30

40

50

60

70

80

x [m]

90

100

Fig. 4. Strain profiles along the bar for 101 grid points and time step ∆t = 0.4·10−3 s

localisation develops in the smallest possible size, i.e. between two neighbouring grid points. Additional computations with a diﬀerent spatial resolution and with a diﬀerent time step conﬁrm this observation. Regularisation can be introduced in a two–phase medium, but this necessitates the introduction of rate or gradient dependence in the solid constituent, or explicitly taking into account the eﬀect of grain rotations.

References 1. M¨ uhlhaus HB, Vardoulakis I (1987) The thickness of shear bands in granular materials. G´eotechnique 37: 271–283 2. de Borst R, Sluys LJ (1991) Localisation in a Cosserat continuum under static and dynamic loading conditions. Comp Meth Appl Mech Eng 90: 805–827 3. Needleman A (1987) Material rate dependence and mesh sensitivity in localization problems. Comp Meth Appl Mech Eng 67: 68–85 4. Sluys LJ, de Borst R (1992) Wave propagation and localisation in a ratedependent cracked medium — Model formulation and one-dimensional examples. Int J Solids Struct 29: 2945–2958 5. Aifantis EC (1984) On the microstructural origin of certain inelastic models. ASME J Eng Mater Technol 106: 326–330 6. Pijaudier-Cabot G, Bazant ZP (1987) Nonlocal damage theory. ASCE J Eng Mech 113: 1512–1533 7. de Borst R, M¨ uhlhaus HB (1992) Gradient-dependent plasticity: Formulation and algorithmic aspects. Int J Num Meth Eng 35: 521–539 8. Peerlings RHJ, de Borst R, Brekelmans WAM, de Vree JHP (1996) Gradient enhanced damage modelling for quasi–brittle materials. Int J Num Meth Eng 39: 3391–3403 9. Ehlers W, Volk W (1997) On shear band localization phenomena in liquid– saturated granular elastoplastic porous solid materials accounting for fluid viscosity and micropolar solid rotations. Mech Coh-frict Mat 2: 301–330

66

Ren´e de Borst and Marie-Ang`ele Abellan

10. Biot MA (1956) Theory of propagation of elastic waves in a fluid-saturated porous solid. I. Low-frequency range. J Acoust Soc America 28: 168–178 11. Rizzi E, Loret B (1999) Strain localization in fluid–saturated anisotropic elastic– plastic porous media. Int J Eng Sci f37: 235–251 12. Simoes FMF, Martins JAC, Loret B (1999) Instabilities in elastic-plastic saturated porous media: harmonic wave versus acceleration wave analysis. Int J Solids Struct 36: 1277–1295 13. Zhang HW, Sanavia L, Schrefler BA (1999) An internal length scale in dynamic strain localization of multiphase porous media. Mech Coh-frict Mat 4: 445–460 14. Zhang HW, Schrefler BA (2004) Particular aspects of internal length scales in strain localisation analysis of multiphase porous materials. Comp Meth Appl Mech Eng 193: 2867–2884 15. Benallal A, Comi C (2002) Material instabilities in inelastic saturated porous media under dynamic loadings. Int J Sol Struct 39: 3693–3716 16. Benallal A, Comi C (2003) On numerical analyses in the presence of unstable saturated porous materials. Int J Num Meth Eng 56: 883–910 17. Abellan MA, de Borst R (2006) Wave propagation and localisation in a softening two–phase medium. Comp Meth Appl Mech Eng, doi: 10.1016/j.cma.2005.05.056 18. Jouanna P, Abellan MA (1995) Generalized approach to heterogeneous media. In: Gens A, Jouanna P, Schrefler B (eds) Modern Issues in Non-Saturated Soils, 1–128. Springer, Berlin Heidelberg New York 19. Lewis RW, Schrefler BA (1998) The Finite Element Method in the Static and Dynamic Deformation and Consolidation of Porous Media, Second Edition. John Wiley & Sons, Chichester 20. Whitham GB (1974) Linear and Nonlinear Waves. Wiley-Interscience, New York 21. Sluys LJ, de Borst R, M¨ uhlhaus HB (1993) Wave propagation and dispersion in a gradient-dependent medium. Int J Solids Struct 30: 1153–1171

New Developments in Surface-to-Surface Discretization Strategies for Analysis of Interface Mechanics Tod A. Laursen and Bin Yang Computational Mechanics Laboratory Department of Civil and Environmental Engineering Duke University, Durham, NC 27708-0287, USA [email protected] Summary. This article summarizes recent results pertaining to the implementation of mortar-based contact formulations in nonlinear computational solid mechanics. In particular, the authors discuss extension of the mortar framework to encompass large sliding, searching algorithms, treatment of self-contact phenomena, and use of the mortar framework to treat problems of lubricated contact.

1 Introduction This paper describes recent progress in the development of mortar-based methods for analysis of contact mechanics problems using ﬁnite elements. The mortar element method was ﬁrst conceived as a domain decomposition method, whereby possibly distinct meshes may be joined across interfaces such that optimal convergence results expected from the underlying ﬁnite element method can be obtained (the reader may consult [4, 2, 3, 15] for early descriptions of the idea, as well as useful overviews). In the context of nonlinear mechanics, one of the appealing applications of this idea is “mesh tying.” In such an application, separate meshes can be generated for subcomponents of an assembly to be analyzed, and then the mortar formulation can be used to “join” these parts by enforcing compatibility of the solution across the interfaces where they meet. Using this approach, accurate results can be obtained even for nonconforming meshes, as long is there is not too large a discrepancy in mesh ﬁneness across each interface. In mortar methods in general, the key idea is that the kinematic constraints between neighboring domains are enforced in an integral sense, rather than locally at each of a ﬁnite set of collocation points. Since contact problems frequently feature nonconforming meshes in contact regions, the potential applicability of mortar techniques to such problems

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 67–86. © 2007 Springer. Printed in the Netherlands.

68

Tod A. Laursen and Bin Yang

is not hard to imagine. Several early authors recognized this fact and proposed mortar-based formulations for kinematically linear applications with considerable success (see [1, 9, 10, 6]). In extending such methods to the large deformation, large sliding regime, however, one is confronted with the need to not only reformulate the constraint deﬁnitions to reﬂect changing connectivity during relative sliding, but also to provide robust algorithmic implementations of these deﬁnitions such that (for example) Newton-Raphson or similar iterative schemes for solution of the nonlinear equations will be eﬀective. In a set of recent papers [12, 13, 17], such large deformation formulations have been thoroughly described, and have been shown to be robust for large deformation applications in both two and three dimensions, and under either dynamic or quasistatic circumstances. In this paper, we review some of the key constructs of mortar-based contact algorithms, starting by looking at the mesh tying problem as a template and brieﬂy discussing the extension to truly large sliding contact. After this review, the emphasis will be on recent extensions of the mortar methodology, which allow it to encompass a much broader set of applications. Speciﬁcally, the self-contact problem and the lubricated contact problem will be examined. Generally speaking, the mortar framework allows us to put the spatial discretization of contact phenomena on a much ﬁrmer theoretical basis, opening up a large range of interfacial phenomena that can be reliably simulated. In addition to the accuracy exhibited by these approaches, they also lend considerable robustness to a nonlinear equation solving strategy as compared to traditional contact descriptions, due to the nonlocal nature of the constraints produced by the formulation.

2 Background: Mortar Projection in Contact Mechanics 2.1 The Mesh Tying Problem The key conceptual concept behind mortar projection is illuminated by taking the mesh tying application as a ﬁrst example. To ﬁx ideas, we consider the large deformation response of two bodies (i), with an eye toward approximately computing the deformation mappings ϕ(i) ∈ H 1 (Ω (i) ), describing the current positions of reference conﬁgurations Ω (i) . As per a common procedure, the surfaces of the bodies ∂Ω (i) are assumed to be decomposed into prescribed traction, displacement and contact regions via ∂Ω (i) = Γσ(i) ∪ Γu(i) ∪ Γc(i) Γσ(i) ∩ Γu(i) = Γu(i) ∩ Γc(i) = Γσ(i) ∩ Γc(i) = ∅

(1)

and boundary conditions are summarized as (J)

(i)

(i)

PiJ NJ = t¯i (i)

(i)

ϕi = ϕ¯i

on Γσ(i) on Γu(i)

(2)

Surface-to-Surface Discretization Strategies for Interface Mechanics

69

(1) h

Γc

(2) h

Γc

Fig. 1. Simple two dimensional illustration of how dissimilar polynomial interpola(1) h (2) h tion of the same surface causes Γc = Γc . The dark curve indicates the surface to be approximated

In (2), PiJ denotes the components of the ﬁrst Piola-Kirchhoﬀ stress, NJ represents the components of the outward normal to the reference conﬁguration, (i) (i) and t¯i and ϕ¯i are the prescribed tractions and displacements, respectively. The summation convention is applied, where uppercase Roman indices refer to reference quantities, while lowercase counterparts are spatial. We leave unspeciﬁed the speciﬁc constitutive law governing PiJ ; in fact, the formulations we propose in this paper for treatment of interfaces are conceived independently of the material laws used to describe the contacting continua. The mortar method is to be applied over the tied regions, which are de(i) noted here by Γc , i = 1, 2, such that the mesh tying constraint becomes ϕ(1) = ϕ(2) on Γc(1) = Γc(2) .

(3)

In the continuum setting, the reference positions of the tied regions coincide, so that one could equivalently require U (1) = U (2) on Γc(1) = Γc(2) ,

(4)

where U (i) = ϕ(i) − X (i) is the Lagrangian displacement. In a numerical ap(i)h proximation, the discretized versions of the surfaces (denoted Γc , i = 1, 2) are no longer coincident; indeed, it is easy to show that discretizations of the same (curved) surface will in general produce areas of unintended overlap and void (see Fig. 1). This fact is important in practice (see for example [11]), and means that quite often reference geometries must be corrected after mesh generation so that the initial conﬁguration obeys the mortar-based constraints. This is particularly true if the continuity constraints are written in terms of (3) rather than (4), which are not equivalent in the spatially discrete case. To simplify our discussion here, however, we neglect this subtlety.

70

Tod A. Laursen and Bin Yang

By convention, we introduce a mortar multiplier ﬁeld λh , deﬁned over the (1)h non-mortar (sometimes termed slave) surface Γc . This ﬁeld is written in (1)h

terms of the shape functions NA describing Γc ns

λh =

A=1

, such that

(1)

λ A NA ,

(5)

(1)

where ns is the set of all nodes comprising Γc . A mortar method enforcing compatibility of the two bodies’ responses over the tying region is deﬁned by enforcing: ∗h ∗h (6) 0 = Gint,ext (ϕh , ϕ ) + Gc (ϕh , ϕ ) ∗ (1)

h

∗ (2)

which must hold for all admissible variations {ϕ ,ϕ h h 0= q h · (U (1) − U (2) ) dΓ h

h

}, and (7)

(1)

Γc

which must hold for all q h ∈ Mh , where Mh is the space of admissible variations of the multiplier ﬁeld λh . In (6), Gint,ext is the usual virtual work of the internal stresses and applied loads, while Gc denotes the contact virtual work, given here as h h ∗h ∗ (1) ∗ (2) Gc (ϕh , ϕ ) = − λh · (ϕ −ϕ ) dΓ. (8) h (1) Γc

Equation (6) is recognized as the usual expression of global equilibrium, while the constraints implied by (7) weakly enforce compatibility between h h U (1) and U (2) . Weighting functions associated with the constraint equation are given as ns (1) q A NA . (9) qh = A=1

Writing the Lagrangian displacements on both surfaces as h

U (1) =

ns A=1

(1)

h

U A NA , U (2) =

nm C=1

(2)

U C NC ,

(10)

(2)h

where nm is the number of nodes C that comprise Γc (the mortar surface), we ﬁnd that substitution into (7) renders ns ns nm (1) (2) qA · NA U B NB − U C NC dΓ . (11) 0= h A=1

(1)

Γc

B=1

C=1

Equation (11) must hold for arbitrary q A , so that a vector-valued constraint

Surface-to-Surface Discretization Strategies for Interface Mechanics (1)h

is implied at each node A in Γc 0 = cA = =

(1)h

Γc

ns B=1

(1)

:

(1) NA

(1) nAB U B

71

ns

U B NB −

B=1 nm

−

ˆ B=1

nm C=1

(2) U C NC

dΓ (12)

(2) nAC U C .

(2)

In (12), nAB and nAC are given by (1) (1) (1) nAB = NA NB dΓ , and h (1) Γc

(2)

nAC =

(1)h Γc

(1)

(2)

NA NC dΓ.

(13)

h

One may readily see that (12) forces U (1) to equal a least squares projection h

(1)

h

(1)

of Γc . The multiplier ﬁeld λh deﬁned in of U (2) onto the discretization Γc (5) enforces these discrete constraints, and may be understood as the surface tractions distribution appearing in the contact virtual work, as given in (8). 2.2 Generalization to Sliding Contact In extending the mortar idea to true contact-impact interaction, one must recognize that the deﬁnition of the mortar operators (as summarized above in (13)) is now aﬀected by changing connectivity as sliding occurs. This suggests that it is now more natural (in contrast to (8)) to represent the contact virtual work Gc in terms of spatial conﬁguration quantities, via (1) ∗ ∗ ∗ (2) X ) − ϕ (Y¯ ) dγ, Gc (ϕ, ϕ) = − λ · ϕ (X (14) (1) γc

(1)

where γc is the current conﬁguration of the (non-mortar) contact surface (1) on Γc , the mortar multiplier λ now denotes the Cauchy contact traction, and where ϕ(2) (Y¯ ) is the current position of the contact point for X . Superscript h’s have been omitted in (14) to simplify notation. The notation Y¯ has (2) been used to denote the contact point on Γc corresponding to each point (1) X ∈ Γc . In traditional contact implementations, this point is typically explicitly determined for each point at which which contact constraints are to be enforced. Here we will employ a spatial integration procedure which will only indirectly deﬁne pairings between points X and Y¯ . Another important distinction between the contact problem and the mesh tying problem is that inequality constraints now govern the Lagrange multipliers (tractions) and associated kinematics. We may deﬁne a gap function X , t) as g(X

X , t) − ϕ(2) Y¯ , t X , t) = n · ϕ(1) (X (15) g(X

72

Tod A. Laursen and Bin Yang (1)

X , t). The where n denotes the outward unit normal to γc at x = ϕ(1) (X Kuhn-Tucker conditions governing the normal part of the contact interaction are then written as X , t) ≤ 0 g(X X , t) ≥ 0 λN (X (16) X , t)g(X X , t) = 0 λN (X X , t) = −λ · n is the Cauchy contact pressure at material point X where λN (X on the slave surface. Equation (162 ) implies that only compressive interaction is allowed, while (163 ) allows the contact pressure to be non-zero only when X , t) = 0. g(X The frictional response can be characterized by isolating the relative tangential velocity v T via

X , t) v=ϕ ˙ (2) Y¯ , t − ϕ ˙ (1) (X (17) = vN + vT where v T is that part of the relative velocity in the tangent plane associated with n. The contact traction λ is similarly resolved, λ = λ N + λT .

(18)

With these notions in hand, the conditions for Coulomb friction can be written as: λT

v T − γ˙

=0

λT

(19) Φ := λT − µ λN ≤ 0 γ˙ ≥ 0 Φγ˙ = 0, where, as can be seen, the frictional traction λT is forced to oppose the tangential velocity v T . A discrete version of the contact problem is achieved through substitution of ﬁnite dimensional approximations for deformation mappings, variations, and Lagrange multipliers. This results in the following mortar approximation to the contact virtual work, denoted as Gcm : ns ns nm ∗h (1) ∗ (1) (2) ∗ (2) λA · nAB ϕB − nAC ϕC . Gcm (ϕh , ϕ ) = − (20) A

(1) nAB

B

(2) nAC

C

and are similar to those given in the tying The expressions for problem (see (13), but now live in the spatial conﬁguration: (1) (1) X ) NB(1) ξ (1) (X X ) dγ, NA ξ (1) (X nAB = γ (1)h (21)

(2) (1) X ) NC(2) ξ (2) Y¯ (X X ) dγ. nAC = NA ξ (1) (X γ (1)h

Surface-to-Surface Discretization Strategies for Interface Mechanics

73

The normal and tangential portions of the contact operator are now exposed by splitting each nodal λA into normal and frictional parts: λA = λNA + λTA .

(22)

The normal part of the contact traction may be represented as (see [12]) λNA = −λNA n A (no sum)

(23)

where λNA represents the contact pressure at node A. It is subject to KuhnTucker conditions via λNA ≥ 0 gA ≤ 0 (24) λNA gA = 0 where the mortar projected gap gA at slave node A is deﬁned as gA = n A · g A , ns nm (1) (1) (2) (2) nAB ϕ B − nAC ϕ C , g A = κA B

(25)

C

where κA is a scale factor deﬁned as 1 κA = (1,ref ) , n D AD (1,ref ) (1) (1) X ) ND X ) dΓ. ξ (1) (X = NA ξ (1) (X nAD

(26)

Γ (1)h

The scaling deﬁned in (26), while not by any means unique, is performed so that the gap function g A is dimensionally correct; this feature is of crucial importance when implementing penalty methods in particular. Equation (25) is written in terms of a nodal normal nA associated with each slave node A. Although other implementations of mortar-based frictional contact are possible, we consider here a penalty regularization of conditions (19). This may be expressed via ⎤ ⎡ λT ⎦

Lv λT = T ⎣v T − γ˙

λT

Φ := λT − µ λN ≤ 0

(27)

γ˙ ≥ 0 Φγ˙ = 0 where T is the frictional penalty parameter. The frictional conditions in (19) are recovered in the limit as T → ∞. Lv λT is the Lie derivative of the

74

Tod A. Laursen and Bin Yang

frictional traction, and may be deﬁned (for example) in a two dimensional context via (28) Lv λT = λ˙ T τ where τ is a tangential base vector. Equation (28) contains material time derivatives of the components of λT only; the absence of derivatives of base vectors assures its frame indiﬀerence. Correspondingly, as shown in [17], the appropriate notion of tangential velocity to use in a mortar projected framework is nm ns (2) (2) (1) (1) n˙ AC ϕ C − n˙ AB ϕ B · (I − n ⊗ n) v TA = −κA (29) C

(2) n˙ AC

B

(1) n˙ AB

and are time derivatives of the mortar integrals (holding node where A constant). Note that the scaling factors κA have again been introduced to retain dimensional consistency. Since the mortar integral time derivatives are invariant with respect to any rigid body motion relative to the original spatial frame, v TA is frame indiﬀerent. With these deﬁnitions in hand, a trial state-return map strategy is employed to determine the Coulomb frictional tractions in an algorithmic, time stepping procedure. The algorithm begins by computation of a trial state, assuming no slip during the increment: nm (2) (2) (2) trial nACn+1 − nACn ϕ C = λTAn − T κA λTA n+1

−

C

ns B

(1) nABn+1

−

(1) nABn

(1) ϕB

(30) · (I − nA ⊗ nA ),

with a corresponding trial value for the slip function

trial Φtrial An+1 = λTAn+1 − µ|λNAn |. A return map is then used to deﬁne the ﬁnal frictional traction via ⎧ trial ⎪ if Φtrial ⎨λTAn+1 An+1 ≤ 0 (stick), trial λT λTAn+1 = An+1 ⎪ otherwise (slip). ⎩µ|λNAn | λtrial T

(31)

(32)

An+1

In these expressions, the subscript n + 1 means a state associated with the current iteration for the unknown solution at tn+1 , while n is associated with the last (converged) time level.

3 An Extension of the Framework: Mortar-Based Self-Contact In many applications, such as are encountered in post-buckling analysis, a surface may fold upon itself such that so-called self contact takes place. A two

Surface-to-Surface Discretization Strategies for Interface Mechanics

75

γσ Γσ (1,1)

γc ϕ

(3,1)

γc

(1,2)

γc

(3,2)

γc

(2,1) γc

Γc

(2,2)

Ω

γc

γu

Γu

Y

X

Fig. 2. Notation for a large deformation self-contact problem

dimensional self-contact problem, with large deformation and large sliding, is shown schematically in Fig. 2. Recent work shows that the mortar framework can be extended to such settings, and we highlight some of the key steps here in accomplishing that extension. In writing the virtual work for such a system, the expression given originally in (8) must be generalized not only to account for the possibility of sliding, but also to account for the possibility of multiple contact patches which can be generated as the surface folds over on itself. We therefore replace (8) by c

∗

G (ϕ, ϕ) := −

k i=1

(i,1)

γc

(i,1) ∗ ∗ (i,2) ¯ X , t) · ϕ X , t) − ϕ λ(i,1) (X (X (Y , t) dγ,

(33) where ϕ(i,2) (Y¯ ) is the current position of the contact point for X . Indices i refer to the multiple contact patches which might be identiﬁed at any instant in the simulation, with k being the number of these patches. As before, the (i,1) is the nonmortar surface where the Lagrange multipliers will be surface γc (i,2) is the mortar surface. As summarized earlier in (22), interpolated, and γc the contact traction λ can be resolved into normal and tangential components, and the conditions of normal contact are given by (24), and the frictional conditions by (19), just as in the frictional contact case. The contact searching

76

Tod A. Laursen and Bin Yang

Fig. 3. Mortar segments in (a) two dimensions; (b) three dimensions. A segment is shown in green

algorithm for mortar contact, however, must be considerably generalized to deal with the phenomenon of self-contact. As discussed in [17] and [12] for general mortar contact formulations, we (1) need to ﬁnd all the mortar segments to compute the mortar integrals, nAB (2) and nAC , deﬁned in (21). For example, in three dimensional problems, the mortar integrals are computed as: (i,1)

nAB = (i,1) tri,seg

nAB

(i,2)

nAC = (i,2) tri,seg nAC

seg

(i,1) seg

nAB

seg

(1)

γctri,seg,i (i,2) seg

nAC

=

γctri,seg,i

seg tri

=

=

NA

=

ξ

, i = 1, ..., k,

X ) NB(1) ξ (1) (X X ) dγ ξ (1) (X

seg tri

(1) NA

(i,1) tri,seg

nAB

(1)

(i,2) tri,seg

nAC

(34)

, i = 1, ..., k,

X ) dγ X ) NC(2) ξ (2) Y¯ (X (X

(35)

In these equations, the superscript seg refers to a mortar segment , which is constructed such that each segment is deﬁned by the mutual projection of a single slave element surface with a single master element surface, as shown in Fig. 3. The polygonal intersections of element surfaces, shown in green in Fig. 3(b), are in turn divided into triangles for numerical evaluation of the integrals, giving rise to the superscripts tri above. The segments change dynamically during a simulation of sliding contact, and the dependence of the method on the determination of the segments is why we refer to the contact algorithms in this work as being surface to surface algorithms. Given a discretized contact surface, an eﬃcient contact algorithm depends crucially on eﬃcient determination of these mortar segments. In our implementation, we recursively split the surface into subsurfaces to build a tree

Surface-to-Surface Discretization Strategies for Interface Mechanics

1

77

1

2

4 6

5

7

5

4

8

8

3

2

3

6

7

9

9

Fig. 4. A bounding volume tree for a 2D surface

structure; the approach has been extensively described in [16] and will only be brieﬂy recounted here. The subsurfaces related to leaf tree nodes are the elements of the surface. Each node of the tree will be termed a T-node, to differentiate from a ﬁnite element node. Each subsurface is deﬁned and stored in terms of an inﬂated bounding volume (speciﬁcally, a k-DOP), which is saved in its corresponding T-nodes. Binary trees are used in this work so each nonleaf T-node has exactly two children, a left child and right child. A typical bounding volume hierarchy is shown in Fig. 4. If there are n elements for a contact surface, the number of T-nodes in bounding volume tree is 2n − 1. The storage space for a bounding volume tree is then O(n). In [16], two methods for building bounding volume trees are discussed: top-down and bottom-up approaches. A top-down approach, which is used to build the bounding volume trees for multi-body contact problems, starts with one T-node (a root T-node) which is related to the entire surface. The surface is then recursively split into subsurfaces and each of them is saved in a newly created T-node. The bottom-up approach, by contrast, begins with the input elements as the leaves of the bounding volume tree and applies some algorithms to group elements recursively. Usually, by this approach, the subsurface corresponding to a T-node is a connected surface so it is a more appropriate way than the top-down approach to build the bounding volume trees for self-contact problems. In this work, we apply the surface clustering algorithm introduced in [14, 7] to build bounding volume trees. In the face clustering algorithm, one ﬁrst creates a dual graph for the mesh of the contact surface. A dual graph is constructed by mapping each element of the surface mesh to a dual node and connecting every two dual nodes by a dual edge if the corresponding elements are adjacent and share an element edge. An example of a dual graph is shown in Fig. 5, where dashed lines are

78

Tod A. Laursen and Bin Yang

Dual Edge

Dual Node

Finite Element Edge Finite Element Node Fig. 5. Dual graph for a surface mesh. Each dual node represents an element or subsurface in the ﬁnite element mesh

ﬁnite element edges, solid lines are dual edges, grey dots are ﬁnite element nodes, and black dots are dual nodes. By contracting a dual edge (i.e., removing the dual edge and collapsing its two dual nodes into a new dual node) one can group two elements into an element cluster (or a subsurface) which corresponds to a new dual node in the dual graph, as seen in Fig. 6. Basically, this contraction will group two contiguous elements or subsurfaces into a new subsurface, which will be their parent in the bounding volume hierarchy. One may also notice that each dual node in the dual graph corresponds to a T-node in the bounding volume tree. By doing this contraction iteratively, one can ﬁnally build a hierarchical structure of the surface mesh, as shown in Fig. 7. To control the quality of the bounding volume hierarchy, i.e. the balance of the bounding volume tree and the shape and tightness of the bounding volumes, one has to follow a carefully designed rule to contract the dual edges. This rule identiﬁes which edge should be contracted ﬁrst and which should be contracted later. To do this, a cost function is assigned to each dual edge; the cost function applied in this work is similar with that was used by [14]. All dual edges are saved in a heap data structure (see [5] for an introduction) and the key values of the heap entries are the contraction costs of the corresponding dual edges. Thus, the dual edge with the least cost is saved on the top of the heap. The procedure to construct a bounding volume hierarchy with the face clustering algorithm can be summarized as: 1. Build the initial dual graph for the ﬁnite element mesh, compute cost functions of all dual edges, and save all the dual edges in a heap.

Surface-to-Surface Discretization Strategies for Interface Mechanics

Contract This Dual Edge

79

New Subsurface

Surface Mesh Dual Graph

(a)

(b)

Fig. 6. Contraction of a dual edge to construct a new subsurface (i.e. removal of a dual edge and collapsing of its two dual nodes): (a) initial dual graph, and (b) new dual graph. The bigger dot on (b) denotes the new generated dual node by this contraction, and the new dual node corresponds to a new constructed subsurface denoted by the shaded area

2. Remove a dual edge from the top of the heap and contract it to construct a new subsurface. 3. Generate a new T-node for the new subsurface. The two children of the new T-node are the two T-nodes corresponding to two dual nodes (subsurfaces or elements) connected by the dual edge. 4. Update all cost functions of dual edges that are connected with the two dual nodes of the contracted dual edge. 5. Update the heap. 6. Repeat 2 through 5 iteratively until the whole tree is constructed. From this procedure, one can see that the bounding volume tree is built in a bottom-up manner. For each node of the tree, the bounding volume of its corresponding subsurface is computed. For large deformation contact problems, the updating of the bounding volume trees is required after each iteration since the bounding volumes are dependent on deformation. Finally, after the contact detection has been accomplished, it is necessary to do some post processing after the searching, to avoid the situation where the contact traction ﬁelds on each contact patch could be deﬁned on discontinuous surfaces, as shown in Fig. 8. As can be seen, without some type of intervention, an element can be a slave element in one contact pair and a master element in another, and there may be a mixture of slave and master elements on a continuous contact element patch (the lower or upper solid line in Fig. 8). A

80

Tod A. Laursen and Bin Yang

(a)

(b)

(c)

(d)

(e)

Fig. 7. A hierarchy (tree) structure from the bottom level to the top level

M M S

S

S

M M

S M

S

S − Slave

M − Master

Fig. 8. Discontinuous deﬁnition of slave and master elements (a double arrow denotes a contact element pair) which should be avoided

simple sorting procedure is applied so that each side of each contact patch retains its own identity as master or slave. As an example of the type of problem to which this self-contact approach is applicable, we consider the rolling of a highly loaded tire which is nearly ﬂat. In this problem, the part of the surface in self-contact (inside the tire) continually changes due to the rolling, placing a signiﬁcant demand for robustness on the searching algorithm and Newton-Raphson iterative scheme. Deformed conﬁgurations of the nearly ﬂat tire at diﬀerent load steps are shown in Fig. 9, where (c) and (d) only show a quarter of the tire to demonstrate self-contact

Surface-to-Surface Discretization Strategies for Interface Mechanics

81

Fig. 9. Deformed conﬁgurations of the tire rolling problem at diﬀerent load steps; parts (c) and (d) only show a quarter of the tire

inside the tire. Signiﬁcant deformation and sliding are seen to occur in this problem. Notably, it is diﬃcult if not impossible to perform this situation using node-to-surface contact discretization strategies.

4 Mortar Formulation of Lubricated Contact Another recent extension of the mortar formalism involves its use to describe lubricated contact, such as might occur for example in many metal forming applications, or underneath a tire rolling on wet pavement. Such a problem, with two deformable solid bodies and a thin ﬂuid ﬁlm between them, is shown (1) (2) in Fig. 10. The two solid bodies occupy the open sets Ωs and Ωs , where a subscript s represents the solid phase. The solid phase of a lubricated contact problem is governed by the usual solid continuum mechanics equations. Here we assume inﬁnitesimal deformations for the solid phase for simplicity, although it is possible to extend the formulation to large deformation cases with proper treatments of geometric nonlinearities. No assumptions are made for the constitutive laws: the material response may be either elastic or inelastic, rate dependent or independent.

82

Tod A. Laursen and Bin Yang

(1)

Γsu (1) Γsσ

Fluid phase

(1) Ωs (1)

Γsc

(2)

Γsc

(2)

Ωs (2)

Γsu

(2)

Γsσ

Fig. 10. Notation for two body lubricated contact problems

In the problems considered here, the through-the-thickness dimension of the ﬂuid ﬁlm is assumed to be much smaller than the size of the contact patch in surface coordinates. Under such conditions, the ﬂuid phase of a lubricated contact problem is governed by the Reynolds equation, which can be derived from the Navier-Stokes and continuity equations based on the thinﬁlm assumption (see, e.g., [8]). The Reynolds equation is deﬁned on a surface domain, which considered to be parameterized by the slave side of a contact surface in this formulation. As shown in Fig. 11, the contact domain Ωf , cor(1) responding to the slave surface Γsc less the dry contact region Ωd , is divided into two diﬀerent subdomains, Ωfl and Ωfc . Ωfl is the subdomain where the lubricant is continuous and has positive pressure, while Ωfc is the subdomain where the lubricant has cavitations and is ruptured (the ﬂuid ﬁlm is assumed to support only a negligible amount of tension before rupture). ΓfD is the surface where the Dirichlet boundary conditions are prescribed for the Reynolds equation, while ΓfN is the boundary between the dry contact domain and the lubrication domain and where Neumann boundary conditions are prescribed. ΓfR , which is called the Reynolds boundary, is the boundary between Ωfl and Ωfc . Based on these deﬁnitions, \ Ωd , Ωf = Γs(1) c

(36)

Ωf = Ω f l ∪ Ω f c .

(37)

and

Surface-to-Surface Discretization Strategies for Interface Mechanics

Ωd

ΓfN

ΓfR

83

Ωfc

Ωfl

ΓfD Fig. 11. Notation for the lubrication domain

The virtual work for the solid phase can be written in the usual way via (1) ∗ ∗ ∗ (2) c u u t(1) (X X ) · u (X X ) − u (Y¯ ) dΓ, G (u , p, ) := − (38) (1) Γsc

where Y¯ is the position of the contact point for X , with the understanding that the contact traction t is now inherited from the traction ﬁeld prevailing in the intervening ﬂuid, consisting in general of a ﬂuid pressure p in the normal direction and a viscous tangential component. It is the ﬂuid part of the formulation that makes the mortar approach attractive in this case, since the pressure distribution in the thin ﬁlm is subject to a governing diﬀerential equation (the Reynolds equation). The fact that the mortar approach produces a consistent surface discretization gives an ideal way to not only approximate this diﬀerential equation, but also to couple it to the solid response. As presented by [8], the general Reynolds equation which governs the ﬂuid pressures within Ωfl is ∂ (ρh) ˜· +∇ ∂t

(1) (2) ρh3 ˜ ρ(V˜ + V˜ ) − ∇p + h 12µ 2

= 0,

(39)

where ρ is the current mass density of the lubricant, h is the ﬂuid ﬁlm thickness (1) (negative of the gap function g), µ is the viscosity of the lubricant, V˜ and

84

Tod A. Laursen and Bin Yang

Fig. 12. Finite element mesh of the three dimensional lubricated contact problem with two diﬀerent perspectives (2) V˜ are projections of slave and master surface velocity vectors onto the slave surface, and p is the ﬂuid pressure (the primary unknown of Equation (39)). ˜ indicate divergence and gradient operators in reduced (surface) Operators ∇ coordinates. The ﬂuid viscosity may be dependent on the ﬂuid pressure; both constant viscosity cases and exponential pressure dependence of viscosity have been tested in our early work. We have implemented a mortar-based monolithic strategy to solve the coupled Reynolds equations and global equilibrium equations, with the solid phase displacement coupling to the ﬂuid equations through the ﬁlm thickness h and the ﬂuid equations coupling to the solid mechanics equations through generation of the pressure ﬁeld p and the viscous shear stresses. Although the full numerical formulation is too involved to recount in detail here, we present a simple three dimensional example to demonstrate the type of simulation for which the technique has been tested. The problem is depicted in Fig. 12, where the relative rotation of two cylinders with a lubricant-ﬁlled interface is considered. A quasi-static rotation is applied to the inner surface of the inside cylinder, corresponding to an angular speed of ω = 500. Figure 12 presents the ﬁnite element mesh for the two cylinders. The inside surface of the outer cylinder is chosen as the slave surface and the outside surface of the inner cylinder is chosen as the master surface. Only one load step is applied for this problem. The computed pressure distribution in the ﬂuid ﬁlm is plotted in Fig. 13.

5 Conclusion This paper has discussed the mortar method as an underlying spatial discretization technique for large deformation contact problems, and has empha-

Surface-to-Surface Discretization Strategies for Interface Mechanics

85

Fig. 13. Computed pressure distribution for the three dimensional lubricated contact problem

sized two promising recent extensions of this idea: incorporation of self-contact phenomena, and consideration of lubricated contact problems. Contact formulations based on mortar concepts have been seen not only to be extremely accurate in comparison with more traditional node-to-surface strategies, but are also extremely robust numerically, particularly within the implicit dynamic and quasistatic applications of primary interest here.

Acknowledgment This work was supported through a research contract by Michelin Americas Research Corporation. This support, as well as the collaboration of Drs. Stephane Cohade, Ali Rezgui, and Mike Andrews, is greatly appreciated.

References 1. Belgacem FB, Hild P, Laborde P (1997) Approximation of the unilateral contact problem by the mortar ﬁnite element method. Comptes Rendus De L’Academie Des Sciences 324:123–127 2. Belgacem FB, Maday Y (1994) A spectral element methodology tuned to parallel implementations. Computer Methods in Applied Mechanics and Engineering 116:59–67 3. Belhachmi Z, Bernardi C (1994) Resolution of fourth order problems by the mortar element method. Computer Methods in Applied Mechanics and Engineering 116:53–58

86

Tod A. Laursen and Bin Yang

4. Bernardi C, Maday Y, Patera AT (1992) A new nonconforming approach to domain decomposition: The mortar element method. In H. Brezia and J.L. Lions (Eds.) Nonlinear Partial Diﬀerential Equations and Their Applications pp 13–51. Pitman and Wiley 5. Cormen TH, Leiserson CE, Rivest RL, Stein C (2001) Introduction to Algorithms, Second Edition. The MIT Press 6. El-Abbasi N, Bathe K-J (2001) Stability and patch test performance of contact discretizations and a new solution algorithm. Computers and Structures 79:1473–1486 7. Garland M, Willmott AJ, Heckbert PS (2001) Hierarchical face clustering on polygonal surfaces. In SI3D, pp 49–58 8. Hamrock BJ (1991) Fundamentals of Fluid Film Lubrication. NASA, Washington, D.C. 9. Hild P (2000) Numerical implementation of two nonconforming ﬁnite element methods for unilateral contact. Computer Methods in Applied Mechanics and Engineering 184:99–123 10. McDevitt TW, Laursen TA (2000) A mortar-ﬁnite element formulation for frictional contact problems. International Journal for Numerical Methods in Engineering 48:1525–1547 11. Puso MA (2004) A 3d mortar method for solid mechanics. International Journal for Numerical Methods in Engineering 59:315–336 12. Puso MA, Laursen TA (2004) A mortar segment-to-segment contact method for large deformation solid mechanics. Computer Methods in Applied Mechanics and Engineering 193:601–629 13. Puso MA, Laursen TA (2004) A mortar segment-to-segment frictional contact method for large deformations. Computer Methods in Applied Mechanics and Engineering 193:4891–4913 14. Willmott AJ (2000) Hierarchical Radiosity with Multiresolution Meshes. PhD thesis, Carnegie Mellon University 15. Wohlmuth BI (2001) Discretization Methods and Iterative Solvers Based on Domain Decomposition. Springer-Verlag, Heidelberg 16. Yang B, Laursen TA (2006) A contact searching algorithm for large deformation mortar formulation. Computational Mechanics, (submitted) 17. Yang B, Laursen TA, Meng XN (2005) Two dimensional mortar contact methods for large deformation frictional sliding. International Journal for Numerical Methods in Engineering 62:1183–1225

Particle Finite Element Methods in Solid Mechanics Problems J. Oliver, J.C. Cante, R. Weyler, C. Gonz´ alez and J. Hernandez E.T.S. Enginyers de Camins, Canals I Ports de Barcelona E.T.S. d’Enginyer´ıa Industrial i Aeron´ autica de Terrassa Universitat Polit´ecnica de Catalunya (UPC) Campus Nord UPC, Ediﬁci C-1, c/ Jordi Girona 1-3, 08034 Barcelona, Spain [email protected] Summary. The paper examines the possibilities of extending the Particle ﬁnite element methods (PFEM), which have been successfully applied in ﬂuid mechanics, to solid mechanics problems. After a review of the fundamentals of the method, their speciﬁc features in solid mechanics are presented. A methodology to face contact problems, the anticipating contact interface mesh, is presented on the basis of a penalty-like constitutive models for imposing the contact and friction conditions. Finally, the PFEM is applied to same representative solid mechanics problems to display the capabilities of the method and some ﬁnal conclusions are obtained.

1 Introduction Particle ﬁnite element methods (PFEM) have received considerable attention in the recent years due to their modeling capabilities for same speciﬁc problems. So far, most of the research and applications of PFEM can be found in the context of computational ﬂuid dynamics (CFD) to tackle ﬂuid mechanics problems in typical solid mechanics settings: i.e. using Lagrangean descriptions of the motion of the continuum medium (Onate et al., 1996; Lohner et al., 2002; Idelsohn et al., 2003a, 2003b, 2004). Their main advantages are found in modeling conﬁned ﬂuids exhibiting moving free surfaces. There, the limited character of the particle displacement makes suitable a Lagrangean description which, in turn, facilitates the tracking and modeling of the existing free surfaces. On the other hand, Lagrangean descriptions are the natural way of describing motion of solids, and, therefore, there is a long solid mechanics tradition in this sense. However in certain processes, of considerable practical interest, the material undergoes very large deformations, rapidly changing boundaries are involved and the motion resembles that of ﬂuids. Metal forming and machining processes, or manufacturing processes involving powder and granular Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 87–103. © 2007 Springer. Printed in the Netherlands.

88

J. Oliver et al.

materials are typical cases where the border between solid and ﬂuid behaviors becomes fuzzy. Therefore, the application of PFEM to solid mechanics problems appears as a new research ﬁeld deserving to be explored. The purpose of this work is precisely investigating the possibilities oﬀered by the particle ﬁnite element methods in some representative solid mechanics problems involving large deformations, multiple contacts, new boundaries generation, etc., thus providing some insights on the future developments in that ﬁeld.

2 Fundamentals: The Particle Finite Element Method Particle ﬁnite element methods emerged as a natural result of previous explorations in the context of the meshless methods (Belytschko et al., 1994, 1996; Onate et al., 1998). They can be characterized by the following ingredients: 1. The use of a Lagrangean format for describing the motion (Malvern, 1969). A selected cloud of particles of inﬁnitesimal size (material points) are tracked along the motion to describe the continuum medium properties evolution (position, displacement, velocities, strain, stresses, internal variables, etc.). When necessary, the properties of the remaining particles of the continuum medium are obtained by interpolation of the properties at points of that cloud. Numerical computations are done on the basis of a ﬁnite element mesh that is constructed at every time step on the basis of the particle positions. Then, Delaunay triangulations, allowing the construction of a ﬁnite element mesh for a given sets of nodes, emerge as a suitable meshing procedure (George, 1991; Calvo et al., 2003). 2. The use of a boundary recognition procedure to identify what particles of the cloud deﬁne an external (or internal) boundary. The so-called alphashape method (Calvo et al., 2003; Xu et al., 2003) constitutes a suitable strategy for this purpose (see Figure 1). It essentially consists of identifying those sides/segments of the cloud that can be inserted into an empty circle/ball (not including other particles of the cloud) of size larger than a given parameter (the alpha-shape parameter). The vertices/particles of those segments are then identiﬁed as boundary particles. Large values of the alpha-shape parameter result in a boundary which is the convex hull of the cloud. Small values of the alpha-shape parameter return a boundary constituted of all the particles of the cloud.1 2.1 Equations of Motion. Boundary Value Problem Let us consider a solid body B experiencing a deformation ϕ(X, t) : B × [0, T ] → R2 , where [0, T ] is the time interval of interest. Let us also consider a 1 For a uniformly distributed cloud of particles (with typical separation h) alphashape values of 1.1h − 1.5h are recommended for a good estimation of the actual boundary.

Particle Finite Element Methods in Solid Mechanics Problems

89

Fig. 1. The alpha-shape method for recognizing boundaries of a cloud of particles

Fig. 2. Incremental non-linear problem at time step [tn , tn+1 ]

ﬁnite set of particles of B ⊃ P := {P1 , P2 , . . . , Pnpart }, occupying, at a speciﬁc ¯ i = [X1 , X2 ]T , which time interval t ∈ [0, T ], spatial points with coordinates X ¯ ¯ P2 , . . . , X ¯ Pn } (see deﬁne the particle reference conﬁguration Ωt := {XP1 , X part Figure 2). Let us assume, at time t, a Delaunay triangulation, with all its vertices, i, ¯ i , of the particle conﬁguration Ωt , thus placed at corresponding positions, X

90

J. Oliver et al.

deﬁning an open set, Vt , at the Euclidean 2D space, with boundary ∂Vt . ˜ ⊂B The particles of B belonging to the material volume Vt deﬁne a body B approaching B as npart → ∞. Let us also consider a time discretization of [0, T ] in time intervals and a speciﬁc time slice [tn , tn+1 ] ⊂ [0, T ] characterizing the time interval/step n+1 of length ∆t = tn+1 −tn . The boundary value problem at the material domain during the time interval can be written as: Given vn , an , σ n , qn , u∗n+1 , t∗n+1 Find un+1 ≡ ϕn+1 (Xn )

such that:

∇ · σ n+1 + bn+1 = ρn+1 an+1

(momentum equation) ⎫ σ n+1 = σ n + Σ(en+1 , σ n+1 , qn+1 ) ⎪ ⎪ ⎪ ⎬ ∆σ n+1 (constitutive equations) qn+1 = qn + Q(en+1 , σ n+1 , qn+1 ) ⎪ ⎪ ⎪ ⎭

(1)

∆qn+1

en+1 = E(un+1 ) (kinematic equation) σ n+1 , nn+1 = t∗n+1

(natural boundary condition)

un+1 = u∗n+1

(essential boundary condition) at ∂u Vn+1

at ∂σ Vn+1

where vn , an , σ n , qn are, respectively, the velocities, accelerations, stresses and internal variable values at the beginning of the interval, u∗n+1 , t∗n+1 are the prescribed values of displacements and tractions, respectively, at the boundary ∂Vn+1 with outward normal nn+1 , un+1 = Xn+1 − Xn are the interval displacements and en+1 is a suitable measure of the interval strains. 2.2 Time Marching Scheme The problem described in Section 2.1 allows considering the motion of the ˜ as a sequence of discrete (in time) boundary value approximating body B problems ruled by equations (1). Then, at every time step the corresponding problem is solved according to the following strategy: Step I: Finite element discretization: Spatial discrete problem Let us now consider a ﬁnite element discretization of Vn , on the basis of the existing triangularization, so that the nodes match the vertices (therefore, ˜ is evaluated nnode = npart ), and that every property, µ, of the particles of B via interpolation of the corresponding property at the vertices/nodes as: µ(X) =

n node

Ni (X)¯ µi

∀X ∈ Vn

(2)

1

¯i stand for the shape/interpolation function and the nodal where Ni and µ value of the property, respectively, at node i.

Particle Finite Element Methods in Solid Mechanics Problems

91

Then, using standard Galerkin’s procedures, and a Newmark’s time integration scheme (Hughes, 2000), the discrete counterpart of the continuum boundary value problem in equations (1) at the space-time slice Vn ×[tn , tn+1 ] ⊂ R2 × [0, T ] reads, in matrix form: ¯n+1 + Fint Mn+1 · a un+1 ) − Fext un+1 ) = 0 n+1 (¯ n+1 (¯ ¯ n+1 = u ¯ n + ∆t¯ u vn +

1 2

∆t2 [(1 − 2β)¯ an + 2β¯ an+1 ]

(3)

¯ n+1 = v ¯ n + ∆t[(1 − γ)¯ v an + γ¯ an+1 ] ext where Mn+1 , Fint n+1 and Fn+1 are, respectively, the mass-matrix, the internal ¯ n+1 , v ¯ n+1 and a ¯n+1 are, reforces vector and the external forces vector, u spectively, the nodal displacement, velocities and accelerations and β and γ are the classical Newmark’s integration parameters. Equations (3) are a set ¯ n+1 and a ¯ n+1 . ¯ n+1 , v of non-linear equations that can be solved for u Combining interpolations, according to equation (2), and substitution in equations (1) allows determining the stresses and the internal variables σ n+1 (X), qn+1 (X) at points X ∈ Vn as required in next step.

Step II: Spatial information transfer All the information necessary in subsequent time steps has now to be transferred to the nodes/particles of Ωn . This is achieved by standard extrapolation (smoothing) procedures (Zienkiewicz et al., 2000) from the element Gauss ¯ n+1 , to be ¯ n+1 and q points to the nodes. For instance, the nodal values, σ considered as initial values for the next time step, n + 1, are computed as:

¯ n+1 = σ ¯ n + [Mσn ]−1 · σ Nσn · ∆σ n+1 dV ¯ n + [Mqn ]−1 · ¯ n+1 = q q

Vn

Vn

Nqn · ∆qn+1 dV

(4)

where Mσn and Mqn are standard “mass-like matrices”, and Nσn and Nqn are “transfer” matrices, with dimensions appropriated to the set of variables, σ and q, computed in terms of the interpolation functions Ni of the ﬁnite element mesh on the domain Vn , and ∆σ n+1 and ∆qn+1 (X) are the point-wise corresponding increments computed at the present time step [tn , tn+1 ]. Step III: Update Finally the set of particles of Ωn are updated to the new positions according to: ¯ Pi )n + (¯ ¯ Pi )n+1 = (X uPi )n+1 ∀Pi ∈ P (5) (X and the new particle conﬁguration is determined as: ¯ Pi )n+1 , (X ¯ P2 )n+1 , . . . , (X ¯ Pn )n+1 } Ωn+1 := {(X part

(6)

92

J. Oliver et al.

Fig. 3. Anticipating contact interface strategy

Then, the boundary of the new cloud of positions of the set of particles P is recognized via de corresponding alpha-shape strategy, and a new triangularization, determining the new spatial domain Vn+1 , is performed. The algorithm proceeds to Step I of the next time step.

3 Contact Strategy: Anticipating Interface Mesh One of the main diﬃculties found in standard contact algorithms in solid mechanics, is the identiﬁcation of the interacting parts of two contacting bodies (master-slave based algorithms). The previously described PFEM setting provides a very interesting feature to be exploited in this sense: the possibility of anticipating the contact boundaries and of imposing the corresponding contact constraints in a diﬀuse manner, without the necessity of a precise identiﬁcation of the contact topologies. Let us consider, for illustration purposes, a forming process characterized by a forming material and some (elastic) tooling, amenable to experience mutual contact (see Figure 3). We can consider each of them as a speciﬁc class, constituted by its own cloud of particles. At every time step, a Delaunay triangularization is performed for every class and its boundary (in terms of the boundary particles) is recognized as indicated in Section 2 by the alpha-shape procedure. Then, an additional triangularization is performed: the particles of the identiﬁed boundaries are deﬁned as a new class (the contact interface class) and sent to the mesher that returns an interface mesh, which connects anticipating contacting particles of diﬀerent classes. The value of the supplied alpha-shape value determines the maximum size of the resulting interface elements and, therefore, rules the degree of anticipation of the contacts. The contact interface mesh constructed in this way, enjoys some speciﬁc properties: •

It is an interface mesh in the sense that there is no interior node (all the nodes are placed at the boundary). In consequence, all the computations done in that ﬁnite element are naturally condensed out to the boundary nodes.

Particle Finite Element Methods in Solid Mechanics Problems

93

Fig. 4. Penalty strategy at the contact interface

• •

•

Typical properties of the Delaunay tessellation procedure ensure that the contact interface connects nearest particles in the contacting bodies. The identiﬁcation of the contact topologies is trivially done via the mesh topology: potentially contacting nodes are those belonging to the same element of the mesh. This overcomes many of the diﬃculties and computational challenges found in classical contact recognition procedures. The contact condition, imposing that nodal gaps should be positive (no penetration), can be fulﬁlled in weak form in terms of strain measures deﬁned at the elements of the interface mesh (see Section 3.1).

Generalization of this procedure to multiple contacting bodies is trivial. As for the imposition of the contact conditions there are several options. In next sections, a penalty strategy for this purpose is presented. 3.1 A Penalty Strategy at the Contact Interface (1)

Let us consider the time step [tn , tn+1 ] and two contacting boundaries, ∂Bn+1 (2) and ∂Bn+1 , and the resulting interface mesh (see Figure 4) deﬁning the interface Bint n+1 . We realize that every element of Bint n+1 has one node (node P) placed on one of the contacting bodies, and two nodes, Q1 and Q2 , on the other (see Figure 4b), which can be trivially identiﬁed. The signed distance of P to the segment Q1 − Q2 , according to the normal2 n of the boundary corresponding to this segment, is deﬁned as the initial elemental normal gap: 2 Information about the normals corresponding to the boundary segments is generated, during the boundary recognition procedure, for every body and transmitted to the boundary interface class.

94

J. Oliver et al. (e)(0)

gn+1 = (XP − XQ1 ) · n = (XP − XQ2 ) · n ∀e ∈ Bint n+1

(7)

(e)(0)

Notice that gn+1 ≥ 0 corresponds to no initial penetration of node P on the opposite boundary. Therefore, negative values of the gap correspond to boundary penetrations. Let us now deﬁne the current normal gap for the element e, at the iteration i of the linearization procedure, as: (e)(i)

(e)(0)

(i)

(e)(i)

gn+1 (un+1 = gn+1 + ∆gn+1 (e)(0) (e)(0) (e)(i) = gn+1 + gn+1 (n · ∇S un+1 · n)

∀e ∈ Bint n+1

(8)

(i)

∆gn+1 (e)(i)

which involves the iterative displacements3 un+1 at the element e. Now, let us deﬁne a strain measure associated to that gap as: (e)

(e)

ε˜n+1 =

gn+1

(9)

where stands for the typical local particle distance (see Figure 4). The con(1) (2) tact condition for boundaries, ∂Bn+1 and ∂Bn+1 , can be immediately written as the positive character of the strain measure ε˜(un+1 ): (e)

(e)

gn+1 ≥ 0 ⇔ ε˜n+1 ≥ 0 ∀e ∈ Bint n+1

(10)

In a variational context, condition (10) can be imposed via a Lagrange multiplier procedure:

λn+1 ε˜(un+1 ) dΩ Π(un+1 , λn+1 ) = ΠB(1) (un+1 ) + ΠB(2) (un+1 ) + n+1

δΠ(un+1 , λn+1 ) = 0;

n+1

g(un+1 ) ≥ 0;

Bint n+1

λn+1 ≥ 0;

λn+1 g(un+1 ) = 0 (11)

where ΠB(1) (un+1 ) and ΠB(2) (un+1 ) stand for the original minimizing funcn+1

n+1

(1)

(2)

tionals for the contacting bodies Bn+1 and Bn+1 , and λn+1 are the corresponding Lagrange multipliers. Now, all the typical strategies for solving the problem in equations (11) can be used. In particular, penalty-based strategies will be recovered by imposing a speciﬁc format to the Lagrange multipliers as: (e)

λn+1 = E 3

int

=

1 2

(e)

E int ε˜n+1 (e)

0 for ε˜n+1 ≥ 0 (e)

K for ε˜n+1 < 0

∀e ∈ Bint n+1

Superindex (·)S stands for the symmetric part of (·).

(12)

Particle Finite Element Methods in Solid Mechanics Problems

95

where K > 0 is the penalty parameter. The resulting problem is formally equivalent to the introduction of an elastic-type constitutive law, σ − ε˜, in the normal direction, deﬁned in terms of the parameter, E int , as a pseudo-elastic modulus: (e)

(e)

˜n+1 n ⊗ n σ n+1 = σ

contact stress

(e)

(e)

σ ˜n+1 = E int ε˜n+1

∀e ∈ Bint n+1

(13)

and extending the boundary value problem in equations (1) to the interface domain Bint n+1 . Inclusion of Frictional Eﬀects Frictional eﬀects can be now included in a very simple manner. For instance, on the basis of a simple Coulomb model, additional tangential stresses can be considered in the constitutive model for every element of the interface (see Figure 5): (e)

(e)

(e)

σ n+1 = σ ˜n+1 n ⊗ n + 2˜ τn+1 (t ⊗ n)S contact stress

(e)

(e)

σ ˜n+1 = E int ε˜n+1 (e)

frictional stress

∀e ∈ Bint n+1

(e)

(e)

(14) (e)

(e)

τ˜n+1 = µ|˜ σn+1 | sign(˜ γn+1 ) (˜ γn+1 = 2t · ∇S un+1 · n) where t stands for the tangent vector associated to the normal n in anticlockwise sense. Numerical Treatment Resolution of the variational problem (11), in the context of the ﬁnite element method, leads to the following expression for the equivalent nodal forces, Fcont , at the nodes i of the interface mesh, due to contact/friction actions: i δΠ = 0 ⇒ =− Fcont i

Bint n+1

(1)

∇Ni · σ n+1 dΩ

(2)

∀i ∈ ∂Bn+1 ∪ ∂Bn+1

(15) (e)

, Besides, it can be readily proven that the elemental counterparts, Fcont i of those contact/friction forces in a given element e, constitute a set of selfequilibrated forces: i=3 i=1

Fcont i

(e)

=−

(e) Bint n+1

(e)

∇Ni

(e)

· σ n+1 dΩ = 0

(16)

96

J. Oliver et al.

Fig. 5. Contact/friction eﬀects: interface constitutive model

which proves the self-equilibrated character of those forces as action-reactions (1) (2) at the contacting boundaries ∂Bn+1 and ∂Bn+1 , i.e.: (1) j∈∂Bn+1

Fcont + j

Fcont = j

(2) j∈∂Bn+1

i=3 e∈Bint n+1

Fcont i

(e)

=0

(17)

i=1

Finally, in view of the structure of the problem in equations (11), the con, once computed at every node of the interface tact/friction nodal forces, Fcont i mesh Bint according to equation (15), can be formally added to the original n+1 problem (1), for every contacting body, as external prescribed point forces acting on the boundary ∂σ Vn+1 . In this way, the contact/friction problem gets reduced to computing nodal/friction forces at all the generated interface meshes, and incorporating them, as external point forces, at the boundaries of the contacting classes. No additional degrees of freedom are involved.

4 Representative Examples In order to illustrate the modeling capacities of the methodology described so far, in next sections some applications to solid mechanics problems are presented. 4.1 Flexible Spring with Multiple Self-contacts In Figure 6 an elastic ﬂexible spring (Figure 6a) is pushed down vertically as to impose multiple contacts, as displayed in Figures 6b and 6c. In the ﬁgures,

Particle Finite Element Methods in Solid Mechanics Problems

97

Fig. 6. Flexible spring: (a) initial conﬁguration, (b) and (c) shrunk deformed conﬁgurations displaying the contact interfaces

the contact interface mesh is artiﬁcially ampliﬁed, for visualization purposes, and the contacting bodies are shrunk in correspondence.4 The actual contacts, keep very little gaps that would not allow that visualization. Two facts should be noticed there: •

The contact interface mesh only aﬀects a limited part of the boundary. This is ruled by the value of the alpha shape parameter precluding interface elements larger than the speciﬁed size.

4 This criterion will be kept from now on, to allow visualizing the contact interface mesh.

98

J. Oliver et al.

Fig. 7. Rivet forming. Top: Riveting parts. Bottom: (a), (b) and (c) deformed ﬁnite element mesh at diﬀerent stages of the forming process. At every stage: actual mesh (left) and shrunk mesh (right), showing the contact interface is displayed

•

Only few elements of the contact interface mesh are active in the sense that (e) (e) gn+1 = 0 ⇔ ε˜n+1 = 0 and, therefore, there is a positive reaction at the contact points according to equations (12) and (13). They are displayed in grey in Figure 6.

This example displays that multiple self-contacts, as the ones occurring in this problem, are trivially solved by the proposed procedure. 4.2 Riveting Process In Figure 7, the geometrical description of a metallic rivet, and the deformation of the ﬁnite element mesh (axisymmetric cross-section) for diﬀerent stages of the forming simulation process, are presented. This is a very representative example of application of the proposed methodology to a variety of metal forming processes.5 It is remarkable the capacity of the method to handle large strains in the deformed body, minimizing the angular distortions of the resulting ﬁnite element mesh. This is an advantageous property of the Delaunay triangulation based meshing procedure. 5 Certainly, the reliability of the simulation requires the use of appropriate constitutive models, typically J2 plasticity models and large strain kinematics.

Particle Finite Element Methods in Solid Mechanics Problems

99

Fig. 8. Machining process: (a) chip forming process, (b)–(e) particle conﬁgurations (left: actual particle conﬁgurations, right: shrunk ﬁnite element meshes displaying the anticipating contact interfaces)

100

J. Oliver et al.

Fig. 9. Filling of a two-stepped cavity with powder material: ﬁnite element meshes displaying the contact interfaces at diﬀerent stages

4.3 Machining Process In Figure 8, simulation of an orthogonal cutting process on a metallic part is considered. This is, again, a very illustrative example of the proposed methodology potential to handle challenging solid mechanics problems. In this case, the formation of the chip, very relevant for the quality of the mechanical process, generates a new boundary at the cutting tool edge. The alpha shape method automatically generates the new boundary as the deformed size at the elements, close to the cutting edge, exceeds the alpha-shape tolerance. The contact/friction model allows sliding the formed chip on the upper surface of the machined part. Both the boundary recognition and the imposition of the dynamic contacts are automatically done by the mesher. 4.4 Powder Filling Process There are many interesting solid mechanics processes, involving ﬂows of granular materials, where PFEM methods can be advantageously applied. Powder metallurgy manufacturing processes or casting processes are typical examples. In Figure 9 the numerical simulation of a powder ﬁlling process is presented using a speciﬁc solid-type constitutive model (Oliver et al., 1996; Cante

Particle Finite Element Methods in Solid Mechanics Problems

101

et al., 2005). The feeder moves horizontally, from left to right, dropping the powder into a two steps cavity. The goal of the analysis is to obtain, through a physically meaningful simulation of the process, the density distribution of the powder at the end of the process. This type of powder ﬁlling processes has been often modelled by the so called discrete element methods, on the basis of models made of a ﬁnite number of interacting balls or cylinders representing the powder grains (Wu et al., 2004; Coube et al., 2005). However, the large number of particles involved in the physical process translates into unaﬀordable computations when a realistic modelling is intended. Here, the powder is treated as a continuum medium, ruled by an elastoplastic constitutive model, and modelled via the PFEM by tracking a limited number of the constituent particles. In the ﬁgure it can be observed as the powder/tool contact conditions are correctly imposed by the contact interface (also displayed in the ﬁgure). In addition, the alpha shape method allows reproducing the complex dynamics of the generated free surface of the powder during the ﬁlling process.

5 Concluding Remarks In the previous sections, PFEM techniques applied to solid mechanics problems have been explored. In addition to their appealing properties, already explored for ﬂuid mechanics problems, some additional advantages can be obtained when they are applied to solids i.e.: •

•

•

Delaunay tessellation techniques, for constructing ﬁnite element meshes on the basis of the selected cloud of points, minimize the angular distortion eﬀects of the resulting elements, thus providing additional robustness to the modelling in problems dominated by large strains. The relatively low computational cost (Calvo et al., 2003) of those techniques allows frequent remeshing without leading to unaﬀordable computational costs. Alpha-shape techniques for boundary recognition purposes, constitute a powerful tool in those solid problems where new physical boundaries are generated (for instance, cutting processes) or when there is a continuous creation and disappearance of boundaries, as a natural part of the physics of the problem (i.e. powder ﬁlling processes). Contacting boundaries problems can be solved by constructing anticipating contact interfaces as it is presented in Section 3. Construction of those contact interfaces becomes an easy and automatic task by using, Delaunay tessellation techniques on the basis of particles of the contacting boundaries. Typical highly computationally demanding techniques, for recognizing point/segment contacts, can then be overcome by imposing the contact conditions on the generated contact interfaces by using, for instance, penalty techniques (Section 3.1). Then, friction eﬀects can be trivially implemented (Section 3.1.1). This confers larger computational eﬃciency and robustness to simulation of problems involving a large number of contacts.

102

J. Oliver et al.

Although the formulation, and the corresponding examples, has been here restricted to 2D cases, extension to 3D problems seems straightforward and in essence the beneﬁts of PFEM should be similar to the ones mentioned above.

Acknowledgements Financial support from the Spanish Ministry of Science and Technology trough grants DPI203-00629 and DPI2004-07666-C02-02 and the Catalan Department of Universities, Research and Society of Information (DURSI) through grant 2005SGR0084 are gratefully acknowledged.

References 1. Belytschko T, Krongauz Y, Organ D, Fleming M, Krysl P (1996) Meshless methods: An overview and recent developments. Comput. Meth. in Appl. Mech. Engng. 139:3-47 2. Belytschko T, Lu YY, Gu L (1994) Element-Free Galerkin Methods. International Journal for Numerical Methods in Engineering 37:229-256 3. Calvo N, Idelsohn SR, Onate E (2003) The extended Delaunany tessellation. Engineering Computations 20:583-600 4. Cante JC, Oliver J, Gonzalez C, Calero JA, Benitez F (2005) On numerical simulation of powder compaction processes: powder transfer modelling and characterisation. Powder Metallurgy 48:85-92 5. Coube O, Cocks ACF, Wu CY (2005) Experimental and numerical study of die ﬁlling, powder transfer and die compaction. Powder Metallurgy 48:68-76 6. George PL (1991) Automatic Mesh Generation, Applications to Finite Methods, New York, Wiley 7. Hughes TJR (2000) The Finite Element Method: Linear Static and Dynamic Finite Element Analysis, Mineola, NY, Dover Publications Inc 8. Idelsohn SR, Onate E, Calvo N, Del Pin F (2003a) The meshless ﬁnite element method. Int. J. Num. Meth. Engng. 58:893-912 9. Idelsohn SR, Onate E, Del Pin F (2003b) A Lagrangian meshless ﬁnite element method applied to ﬂuid-structure interaction problems. Computers & Structures 81:655-671 10. Idelsohn SR, Onate E, Del Pin F (2004) The particle ﬁnite element method: a powerful tool to solve incompressible ﬂows with free-surfaces and breaking waves. Int. J. Num. Meth. Engng. 61:964-989 11. Lohner R, Sacco C, Onate E, Idelsohn SR (2002) A ﬁnite point method for compressible ﬂow. Int. J. Num. Meth. Engng. 53:1765-1779 12. Malvern L (1969) Introduction to the Mechanics of a Continuous Medium. Englewood Cliﬀs, New Jersey, USA, Prentice-Hall 13. Oliver J, Oller S, Cante JC (1996) A plasticity model for simulation of industrial powder compaction processes. Int. J. Solids and Structures 33:3161-3178 14. Onate E, Idelsohn S (1998) A mesh-free ﬁnite point method for advectivediﬀusive transport and ﬂuid ﬂow problems. Comput. Mechanics 21: 283-292.

Particle Finite Element Methods in Solid Mechanics Problems

103

15. Onate E, Idelsohn SR, Zienkiewicz OC, Taylor RL (1996) A ﬁnite point method in computational mechanics. Applications to convective transport and ﬂuid ﬂow. Int. J. Num. Meth. Engng 39:3839-3866 16. Wu CY, Cocks ACF (2004) Flow behaviour of powders during die ﬁlling. Powder Metallurgy 47:127-136 17. Xu XL, Harada K (2003) Automatic surface reconstruction with alpha-shape method. Visual Computer.19:431-443 18. Zienkiewicz OC, Taylor RL (2000) The Finite Element Method. Oxford UK, Butterworth-Heinemann

Micro-Meso-Macro Modelling of Composite Materials P. Wriggers and M. Hain Institute of Mechanics and Computational Mechanics University of Hannover, Appelstr. 9a, 30167 Hannover, Germany [email protected] Summary. Multi-scale models can be helpful in the understanding of complex materials used in engineering practice. Applications related to this class of problems covers diﬀerent length scales in the range from µm to m. Using the concept of representative volume elements (RVE), the theoretical background is discussed in this contribution as well as the numerical treatment of the resulting three-dimensional RVEs. The developed methodology is applied to a speciﬁc engineering material which is concrete. This construction material has to be investigated on three diﬀerent scales: the hardened cement paste (hcp), the mortar and ﬁnally the concrete. Here, a successive two-stage approach is followed in which ﬁrst the multi-scale model of hcp and mortar is applied. The resulting homogenization can then be used in the next step for a multi-scale mortar-concrete model. At the micro-scale of hcp, a ﬁnite element mesh based on a three-dimensional computer-tomography with diﬀerent constitutive equations for the three parts unhydrated residual clinker, pores and hydrated products is introduced. With respect to the ﬁnite element solution, homogenization techniques are used in order to calculate eﬀective elastic material properties. The constitutive equations at the micro-scale contain inelastic parameters, which cannot be obtained through experimental testings. Therefore, one has to solve an inverse problem which yields the identiﬁcation of these properties. For computational eﬃciency and robustness, a combination of the stochastic genetic algorithm and the deterministic Levenberg-Marquardt method is used. In order to speedup the computation time signiﬁcantly, all calculations are distributed automatically within a network environment. Inelastic behavior occurs when the micro-structure hcp is ﬁlled partly with water and a freezing process takes place. A constitutive model for ice is applied to the water ﬁlled parts of the micro-structure. The expansion of the ice leads to damage in the hcp which is associated with inelastic material behavior. If such a calculation is performed for diﬀerent moisture and temperatures, a correlation between moisture, temperature and the inelastic material behavior can be obtained. The eﬀective constitutive equation of hcp will serve as a basis for a multi-scale mortar-concrete model.

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 105–122. © 2007 Springer. Printed in the Netherlands.

106

P. Wriggers and M. Hain

1 Introduction A deeper understanding of the constitutive behavior of complex materials such as concrete can be achieved on one hand by experimental investigations and on the other hand by numerical simulations. While the experimental techniques are applied successfully since several decades, the use of numerical simulation techniques is quite young. This is due to the fact that the underlying threedimensional models are very complex and need considerable computer power which only in the last decade has reached a suﬃcient state. The advantage of a numerical simulation is that one can look inside a specimen during the loading process and also is able to resolve fast processes on a diﬀerent time scale. Figure 1 depicts the multi-scale modeling process which can be used for a material like concrete. The underlying nano-scale is not considered in this contribution.

Fig. 1. Multi-scale model of concrete

Within the above mentioned multi-scale approach, diﬀerent three-dimensional mechanical models are applied on each length scale in order to describe the constitutive behavior on that scale. These are called representative volume elements (RVEs). Normally, the material on a speciﬁc length scale consists of diﬀerent phases which have to be taken into account in order to characterize the material with suﬃcient accuracy. The RVE is then subjected to diﬀerent loading conditions which lead to a material response. Based on these results a homogenization process can be initiated to describe the material behavior averaged over the whole RVE. The resulting homogenized constitutive equation is then applied within the the next scale to model the constituents of the RVE belonging to that scale.

Micro-Meso-Macro Modelling of Composite Materials

107

Fig. 2. Cut through of a CT-scan (1750 × 1750µm)

In this contribution, a multi-scale model for hardened cement paste (hcp) is introduced. The scale of the superior system is denoted meso-scale, the underlying microscopic system of hcp micro-scale [17], [5]. The homogenized properties of hcp serves as a basis for the constitutive model of mortar at the meso-scale.

2 Micro-structure of Hardened Cement Paste (hcp) The FE-analysis of hcp requires the discretization of the micro-structure. Here, the geometry on the micro-scale is obtained from a three-dimensional computer tomography (CT) which provides a spatial resolved distribution of the density. In this contribution, CT-scans of several specimens with an edge length of 1750µm and a resolution of 1µm have been performed by the Bundesanstalt f¨ ur Materialforschung und -pr¨ ufung in Berlin, Germany. The CT-scans have been applied for a hcp with the water-cement ratio of wc = 0.45 and a degree of hydration of h = 0.945. In Fig. 2 a cut through of such a CT-scan is shown. The unhydrated residual clinker is black and the hydrated part is middle gray colored. One can see the accumulation of pores, which are marked in light gray. Each CT-ﬁle contains 17503 data points (each corresponds to 1µm3 ) and allocates totally 5GB of memory. For the mechanical analysis, the surrounding synthetic tube is not relevant. Hence, only the interior part of the CT-scan is used for further mechanical simulations which contains 10083 data points (see Fig. 3). Due to noise, a median ﬁlter has to be applied to the raw data. Based on the theory of Powers and coworkers [13], [12] the fractional volume of the pores cp and the unhydrated residual clinker cu are calculated cp =

wc − 0.36h , wc + 0.32

cu =

0.32(1 − cp ) . wc + 0.32

(1)

108

P. Wriggers and M. Hain

Fig. 3. Cut through of the raw data (1008 × 1008µm)

N (d) 350000

pores

unhydr. residual clinker

300000 250000 200000 150000 100000 50000 0

50

100

150

200

Fig. 4. Histogram of the raw data

250

d

In order to distinguish unhydrated residual clinker, hydration products and porosity a histogram is generated, where N (d) describes the number of voxels at a speciﬁc density d (see Fig. 4). Threshold values for the pores and the unhydrated residual clinker are calculated with respect to (1). Hence, the raw data can be segmented in the hydrated part, unhydrated residual clinker and porosity. In Fig. 5 a cross section of the ﬁltered data is shown which is obtained from the raw data (see Fig. 3). The hydrated part has a volume fracture of 84Vol.%, the pores of approximately 14Vol.% and the unhydrated residual clinker of roughly 2Vol.%. The micro-structure of hcp can also be generated by simulating the chemical reactions of the hydration. Result of such a simulation is an artiﬁcial micro-structure with diﬀerent phases. The chemical reaction of the hydration can be simulated with respect to a cellular automata, as the programme from NIST does [6]. Herein, the whole micro-structure is divided into topological, geometrical and physical uniform cells. Each cell has an individual state, corresponding to its current property. A set of rules calculate the new state for each cell at time n + 1. The result of this calculation depends on the state at time n, the states of the neighbors and a random part. The rules are applied at the same time to all cells.

Micro-Meso-Macro Modelling of Composite Materials

109

Fig. 5. Cross section of the ﬁltered data (1008 × 1008µm)

Fig. 6. Simulated microstructure (128 × 128µm)

Fig. 7. CT-based microstructure (128 × 128µm)

If the hydration is simulated with the above mentioned cellular automata, one obtains a diﬀerent geometry as those obtained from CT-scans, compare Figs. 6 and 7. Due to the random based rules of the programme, the porosity is evenly distributed. There are no accumulations of pores as the corresponding CT-scan depicts, but for a reliable simulation of frost heave a proper geometry of the pores is necessary. Therefore, only CT-based micro-structures are applied within the further calculations.

3 Constitutive Equations Numerical results on the micro-scale are obtained by use of the ﬁnite element method which is applied to discretize the representative volume elements (RVEs). The RVEs are generated directly from the ﬁltered CT-data and have diﬀerent material properties for each phase. In this contribution RVEs with an edge length of 64µm are used. Since each voxel is represented by one ﬁnite element this leads to a 643 ﬁnite element mesh. Hence each RVE has about 800 000 degrees of freedoms (DOFs).

110

P. Wriggers and M. Hain

Fig. 8. Embedded RVE

Due to the diﬀerent properties classical constant strain boundary conditions – leading to Voigt bounds – will cause problems at the boundary. Constant stress boundary conditions – leading to Reuss bounds – are also not be used. Instead the RVEs are embedded in a matrix of average stiﬀness, see Fig. 8. This corresponds to the self-consistency method from analytical micro-mechanics and is sometimes referred to as window-technique. Material properties for the elastic behavior of the diﬀerent phases from hcp can directly be taken from the literature [1], [2], [3]. To avoid numerical problems and further mechanical inﬂuences the pores are described using an elastic material of negligible stiﬀness. With respect to the minor volume fraction, averaged properties can be chosen for the unhydrated phase. Table 1. Elastic properties of the phases E

phase

unhydrated phase hydrated phase pores

N mm2

ν −

≈ 132 700 20 000 1

0.30 0.21 0.00

Experimental tests of hcp show that the inelastic eﬀects of hcp are related to damage behavior combined with visco-plastic eﬀects. Due to that a model for the hydrated phase is selected which consists of a visco-plastic constitutive relation of the classical Perzyna-type combined with a damage model. Due to mechanical loading, cracks occur at the nano-scale. These nanocracks are statistically distributed and oriented, thus isotropic damage can be chosen for the micro-structure. Stress-strain relations for isotropic damage can be found in [9], here we select σ = (1 − D)C : .

(2)

Micro-Meso-Macro Modelling of Composite Materials

111

The scalar variable D describes the damage and C refers to the material tensor of the undamaged elastic material. An evolution law for the damage variable ∂S(eq ) (3) D˙ = ∆ξ ∂eq and a damage surface S(eq ) are introduced. The damage surface determines, whether the damage increases or not. It is deﬁned by an exponential relation and depends on the equivalent strain eq . The parameter a, b and c constitute the material properties of this model c eq −a S(eq ) := 1 − exp − −D 0. (4) b For the visco-plastic part, a penalty formulation P is introduced, see e.g. [14], based on the second fundamental theorem of thermodynamics. Here, the scalar variable η describes the viscosity, φ(f ) denotes a penalty-function of power type P = σ : ˙ pl + η1 φ(f ) , 0 ;f ≤ 0 . φ(f ) = 1 m+1 f ;f > 0 m+1

(5)

In order to keep the constitutive model at the micro-scale as simple as possible, a Drucker-Prager model with the yield surface f is chosen. Therefore, diﬀerent behavior of hcp in compression and tension can be described (6) f := αtr σ + dev σ − 23 kf ≤ 0 . Within the associated theory of visco-plasticity, the evolution equation for ∂f has to be integrated. Here we apply an the inelastic strains ˙pl = ∆λ˙ ∂σ Euler backward integration leading to ∂f pl pl n+1 = n + ∆λ . (7) ∂σ n+1 The increment ∆λ = Newton-scheme

∆t + η φ

is locally, at every Gauss point, calculated by a

∆λk+1 = ∆λk −

∂Gk ∂∆λk

−1

Gk ,

(8)

where Gk describes the nonlinear equation resulting from the evaluation of (5) and (6) m η∆λk ! − f trial − 9α2 κ∆λk − 2µ∆λk =0. (9) Gk = ∆t For computational eﬃciency, the above mentioned set of constitutive equations is linearized consistently.

112

P. Wriggers and M. Hain

4 Homogenization In order to determine eﬀective elastic material properties for each RVE, homogenization is needed and the eﬀective material tensor has to be calculated. The eﬀective material tensor C eﬀ maps the average of the strains (eﬀective strains) onto the average of the stress σ (eﬀective stresses) by σ = C eﬀ : ,

(10)

where • denotes the volume average within the RVE, Ω being the volume of the RVE. 1 • dΩ . (11) • = |Ω| Ω

In order to calculate the eﬀective stresses and strains, one has to deﬁne boundary conditions and solve the boundary value problem on the micro-scale. The latter will be performed by using ﬁnite elements. Since the application of a pure stress ﬁeld to the RVE leads to some diﬃculties regarding the suppression of rigid body modes, we apply here only pure displacement boundary conditions (constant stress state). Subsequently, the volume average of the strain can be evaluated from the ﬁnite element solution of the RVE by ne 1 h dΩ (12) = Ωe e=1 Ωe

where h is the strain computed from the ﬁnite element solution, Ωe the volume of a ﬁnite element and ne the total number of ﬁnite elements of the RVE. The same relation holds for the computation average of the stresses. Once the eﬀective strains and stresses are known the eﬀective material tensor C eﬀ can be computed within the homogenization step. In this this step a linear elastic eﬀective material of σ() = λeﬀ tr 1 + 2µeﬀ is chosen. A least square functional is introduced to ﬁt the averaged stresses with those obtained from the eﬀective constitutive equation σ() Π := σ − σ() → min .

(13)

The diﬀerentiation of this relation with respect to the eﬀective material properties yields a symmetric linear equation for the two Lame constants λeﬀ and µeﬀ 2 λeﬀ 2tr tr σ 6tr 4tr 2 · = . (14) µeﬀ 4σ : 4tr 2 8 : Due to the randomly distributed phases within the micro-structure of hcp, a Monte Carlo method was selected to compute the average values for the constitutive parameters. Hence a suﬃciently large number of diﬀerent RVEs has

Micro-Meso-Macro Modelling of Composite Materials W

113

W

0.8 0.8 0.6 0.6 0.4 0.4 0.2 0.2 80

10

12

14

16

18

20

22

24 eﬀ kN E mm2

Fig. 9. Probability density of Eeﬀ

0.2

0.205

0.21

0.215

0.22

0.225

ν eﬀ [−]

Fig. 10. Probability density of µeﬀ

to be investigated. Each homogenization yields the eﬀective material properties λeﬀ and µeﬀ of the speciﬁc RVE. Therefore, one obtains statistical distributed eﬀective parameters, e.g. a probability density. The probability density W of the eﬀective Young‘s modulus Eeﬀ and effective Poisson‘s ratio µeﬀ are shown in Figs. 9 and 10 for a set of 9200 RVEs, respectively. Both are close to a Gaussian distribution (dashed lines). Furthermore, the above mentioned numerical results are in excellent agreement with results obtained from experimental tests of hcp, see Table 2. Table 2. Experimental versus numerical results test

numerical experimental series 1 experimental series 2

med Eeﬀ

med νeﬀ

N mm2

−

17 665 17 455 17 727

0.211 0.210 0.210

By applying loading in diﬀerent directions one can test whether the material response of a RVE is isotropic or anisotropic. For loadings only in the x-direction (constant strain xx ), the above mentioned homogenization procedure yields nearly the same results as for simultaneously loading in x, y and z-direction (full strain tensor). The same holds for loadings only in the y or z-direction (see Table 3). This depicts clearly that the response of the micro-structure (RVE) is isotropic. This result corresponds to the irregular geometry of the phases and the large number of ﬁnite elements for each RVE. The above mentioned homogenization is a result from a real multi-scale approach. The geometry has been obtained from CT-scans of hcp. The material properties of the diﬀerent phases of the RVE were taken directly from the literature, without any modiﬁcation. The accuracy of this procedure is very good since the eﬀective properties, obtained numerically, agree excellently with results from experimental tests.

114

P. Wriggers and M. Hain Table 3. Results for diﬀerent loadings loading direction

every direction only x-direction only y-direction only z-direction

Eeﬀ

νeﬀ

N mm2

−

17 665 17 952 17 779 17 740

0.2107 0.2108 0.2110 0.2100

5 Parameter Identification The inelastic material model on the micro-scale described in Section 3 contains constitutive parameters κ, which neither can be found in the literature, nor obtained through experimental testing. Therefore, one has to compute these by parameter identiﬁcation. The displacement of the micro-structure u(κ) depends, under a given loading, upon the unknown material properties. For an assumed constitutive model, see Section 3, the material parameters can be identiﬁed. The identiﬁcation of these parameters is carried out, such that the displacements u(κ) from the numerical simulation ﬁt with the displacements d from an experimental test. This yields an ill-posed inverse problem which cannot be solved directly. Instead, an optimization problem is carried out. The material parameters of the constitutive model presented in Section 3 have to be calculated, such that an objective function is minimized. The objective function A is deﬁned by a least-square sum between each numerical and experimental value A(κ) =

n

u(κ)i − di

2

→ min .

(15)

i=1

The identiﬁcation is obtained by solving the above mentioned optimization problem. For computational eﬃciency and robustness, a combination of the stochastic genetic algorithm [16], [15] and the deterministic LevenbergMarquardt method is used [4]. Here, the gradient information of the objective function is obtained numerically from a central diﬀerence quotient A(κ + ei ) − A(κ − ei ) . (16) 2 In a ﬁrst step a pre-optimization with a genetic algorithm is performed in order to get close to the global minimum. Once the value of the objective function falls below a certain threshold value, the optimization procedure switches to the more eﬃcient Levenberg-Marquardt method. Due to the complex micro-structure, the inelastic material behavior and the large number of loading steps, each examination of the objective function A(κ) needs approximately 12 hours on a standard PC computer system. ∇κ A(κ)i ≈

σ33

N mm2

Micro-Meso-Macro Modelling of Composite Materials

−10 −20

115

experimental curve numerical fit

−30 −40 −50 −60 −70 −80 −0.006

−0.005

−0.004

−0.003

−0.002

−0.001 33 [−]

Fig. 11. Numerical ﬁt of the experimental data

Therefore, a typical parameter identiﬁcation with 120 evaluations requires roughly two month CPU time on a modern standard computer. In order to keep the overall computing time within reasonable bounds, the calculations, which can be performed stand alone, are distributed within a network environment. A client-server based system has been implemented, a detailed introduction of those systems can be found in [11]. For the optimization procedure, a client is started. This client does not evaluate the objective function itself, but distributes the computation to the compute-servers via a network connection. The evaluation of the objective function A(κ) is performed on those servers. Once the necessary output data is produced on the servers, it is transported back to the client automatically. The results are then used on the client for the next iteration step of the optimization procedure. Within the network environment using 11 standard computers, the identiﬁcation can be completed within six days. This yields a speed-up factor of approximately 10. In Fig. 11 a result of the parameter identiﬁcation is shown. One can see a satisfying accuracy between the experimental and the numerical results. The experimental load-deﬂection curve varies with respect to diﬀerent specimens, therefore it is not reasonable to ﬁt the experimental data more exactly. The identiﬁed parameters are presented in the subsequent table. The properties marked with • have not been identiﬁed, but were chosen in advance. They describe the exponent of the equivalent strain and the penalty function, respectively. For their deﬁnition see Section 3. A real multi-scale approach cannot be set up for the inelastic behavior since there do not exist experimental tests which yield values for the constitutive behaviour of the diﬀerent phases within the micro-structure. Only eﬀective load-deﬂection curves can be obtained through experiments. In order to get the desired inelastic properties of the micro-structure, one has to solve the inverse problem via parameter identiﬁcation. Hence, the experimental eﬀective behavior is used to calculate the inelastic properties at the micro-scale which

116

P. Wriggers and M. Hain Table 4. Identiﬁed parameters parameter value a b c α kf m η

0.488 0.1 3.0 0.538 48.27 3 84 650

is not a multi-scale approach. However, the obtained inelastic constitutive data for the micro-structure are needed within the next step which then is related to a multi-scale approach.

6 Thermo-mechanical Coupling Hardened cement past is a part of mortar which in itself is part of concrete. Concrete structures are often subjected to ﬂuids such as rain. When this water permeates into the concrete, it actually ﬁlls the pores of the hcp to a certain degree. In freezing condition this water changes its phase to ice and with it expands. This expansion process may lead to damage in some parts of hcp. This process will be investigated in this section. For that we have to know the water contents of the hcp, its constitutive behaviour, see last section, and the constitutive behaviour of the ice which depends on temperature. A numerical simulation of this process has to take into account thermal eﬀects besides the mechanical ones. Considerable work related to the simulation of water permeability and water vapor diﬀusion in hcp has been performed in [8]. These results are used in the further calculations to obtain a realistic distribution of water on the micro-structural level. In Figs. 12-15 cuts through the RVE with diﬀerent moisture contents wh are shown. The water ﬁlled parts of the micro-structure are colored in blue. As expected the water prefers the boundaries of a pore. For the coupled thermo-mechanical simulation, transient thermal conduction is introduced. The mechanical and the thermal behavior is coupled in a weak sense. We assume that cooling down of hcp leads to strains, but strains due to mechanical loading do not change the temperature. The strains are separated into a mechanical part u and a thermal part in an additive way (17) = u + αt (Θ − Θ0 )1 . The parameter αt denotes the coeﬃcient of thermal expansion. With respect to the above mentioned split, the weak form of the internal part of the

Micro-Meso-Macro Modelling of Composite Materials

117

Fig. 12. Cut through of a RVE, wh = 80% (64 × 64µm)

Fig. 13. Cut through of a RVE, wh = 85% (64 × 64µm)

Fig. 14. Cut through of a RVE, wh = 90% (64 × 64µm)

Fig. 15. Cut through of a RVE, wh = 95% (64 × 64µm)

mechanical equilibrium is given by

Gu = grad η u : C : − αt (Θ − Θ0 )1 dΩ . int

(18)

Ω

Hence, the mechanical equilibrium depends both on the temperature Θ and the displacement u (19) Gu = Gu (Θ, u) while the thermal weak form only depends on the temperature GΘ = GΘ (Θ) .

(20)

The linearization and subsequent discretization of the thermal and mechanical weak yields the tangential stiﬀness matrix for the ﬁnite element method. It contains of the sub-matrices of the thermal and of the mechanical problem K uu K uΘ ∆u Gu =− (21) 0 K ΘΘ GΘ ∆Θ The thermo-mechanical coupling is described by the couple-matrix K uΘ .

118

P. Wriggers and M. Hain

In general it is possible to subject the RVE to thermal and mechanical loading conditions which leads to a speciﬁc material response. For this analysis a constitutive model for ice has to be introduced and applied to the water ﬁlled parts of the micro-structure. In this contribution, the micro-structural ice is assumed to have the same properties as macroscopic ice. The material model for ice is chosen as visco-plastic model of Perzyna type (see section 3) and is coupled thermo-mechanically. The previously mentioned expansion of ice is described through a negative coeﬃcient of thermal expansion αt . In this contribution Young‘s modulus of ice is assumed to depend on the current temperature. The other constitutive parameters µ, kf , α and ν are assumed to be constant. It is well known that water ﬁlled pores with a hydraulic diameter of r < 0.5µm freeze at temperatures of Θ ≈ −20◦ C. The pores in the micro-structure of hcp have this size. Hence Young‘s modulus of ice reaches a certain limiting value E∞ which is kept constant below this temperature E∞ ; Θ ≤ −20◦ C E= . (22) ≈ 0 ; Θ ≥ 0◦ C In order to describe this experimental evidence an equation is introduced in which Young’s modulus depends upon the temperature and the four constitutive parameters E0 , E∞ , e and f . E ∞ − E0 Θ−f E(Θ) := E0 + exp 1 − exp . (23) e e The parameter E0 describes the stiﬀness of unfrozen ice (respectively water) and has a negligible value. E∞ denotes the stiﬀness of ice. The parameters e and f eﬀect the development of Young‘s modulus and are selected such that the stiﬀness E∞ is reached at a temperature of Θ ≈ −20◦ C (see Fig. 16). Within the analysis of the damage due to frost within the hcp the constitutive equation for ice is applied to the water ﬁlled pores of hcp. The material properties of ice are given in the Table 5. They are taken directly from the literature, see e.g. [7]. The properties indicated with • are chosen in order to describe the temperature dependency of Young‘s modulus using (23). Within the numerical simulations thermal loading is increased linearly such that the temperature inside the micro-structure reaches Θ ≈ −20◦ C. Mechanical loadings are not applied within this investigation. However they are present e.g. due to dead loads and have to be considered for a determination of damage within hcp in a real structure. Here we want to compare with experiments of hcp in which we can neglect these loads. For the mechanical properties of hcp the identiﬁed parameters from Section 5 are used. The principal stress due to thermal expansion is depicted in Fig. 17. Compression stress is marked in dark gray and tension stress in light gray. Obviously, the water ﬁlled pores are in compression state due to the expansion of ice.

E

N mm2

Micro-Meso-Macro Modelling of Composite Materials

119

3000 2500 2000 1500 1000 500 0

−25

−20

−15

−10

−5

0

5 Θ[◦ C]

Fig. 16. Temperature dependency of Young‘s modulus (e = 2.5, f = −5.0)

Table 5. Material properties for ice parameter value E0 E∞ ν kf α η m e f

1.0 3 500 0.35 1.633 0.333 1.0 0 2.5 -5.0

The thermal loading (freezing) leads to damage in the micro-structure and hence is related to an inelastic material response. For the given loading, one can observe damage zones in Fig. 6. The undamaged material is marked in light gray and the damaged material in dark gray. As one can expect, damage occurs between the water ﬁlled pores and will reduce the load carrying capacity of the hcp and thus the mortar. So far these simulations have only be performed for one sample related to the degree of water ﬁlling. Hence these results can be used to understand the mechanical behaviour of the freezing process, but not for quantitative evaluations leading to new constitutive relations for the eﬀective material properties. For this purpose statistical computations have to be made with diﬀerent samples as performed in section 4. Based on such statistical evaluations we will compare the numerical results with those obtained from experimental tests of frozen hcp in future research.

120

P. Wriggers and M. Hain

Fig. 17. Principal stress due to frost

Fig. 18. Damage due to frost

When the above mentioned numerical simulations are performed for different moisture and temperatures states, a correlation between moisture, temperature and inelastic material behavior is obtained. In order to describe such inelastic mechanical phenomena at the meso-scale, an eﬀective material model has to be constructed. In such meso-scale model the constitutive parameters have to depend now upon the mechanical strains, the moisture and the temperature. Results for two diﬀerent degrees of moisture are depicted in Fig. 19. From such numerical simulation one obtains the development of the eﬀective damage variable D as a function of the eﬀective temperature Θ. The eﬀective values are computed within the RVE by volume averaging of the local damage and local temperature using the procedure described in equation (12). Such curves have now to be computed for diﬀerent degrees of moisture in order to get a function on meso-scale which relates the state of eﬀective damage to temperature and moisture.

7 Outlook On the next length scale, a model for mortar will be introduced. This model consists of an eﬀective material for hcp, aggregates, pores and the cohesive zone around the aggregates. The geometry of mortar will be based on CTscans. But additionally, a generated structure of mortar is also used. A particle generator has been implemented, which shuﬄes spherical particles in order to get close to a given sieve curve (see Fig. 20). With respect to this particle distribution, one obtains an artiﬁcial mortar. Further comparisons with CTscans will prove, if such an artiﬁcial structure is realistically. A corresponding FE-mesh is generated using the hanging nodes technique. The hanging node technique leads to a more accurate mesh without any dis-

Micro-Meso-Macro Modelling of Composite Materials

121

Fig. 19. Damage evolution due to frost

Fig. 20. Generated particle distribution

Fig. 21. Damage in artiﬁcial mortar

torted elements. In a ﬁrst approach the aggregates are described with an elastic constitutive equation and the cohesive zone is neglected. Further research will prove, if these assumptions yield reliable results. Due to mechanical loading, damage zones occur between the aggregates. A ﬁrst result was calculated in [10] and is shown in Fig. 21. As expected, damage zones occur around the particles. Further research will compare those numerical results with accompanying experimental tests of mortar.

Acknowledgments Financial support from the Deutsche Forschungsgemeinschaft (German Research Council) DFG is gratefully appreciated. All experimental results of hcp

122

P. Wriggers and M. Hain

were performed by the Institut f¨ ur Bauforschung (director Prof. Brameshuber) at Aachen, Germany. The Bundesanstalt f¨ ur Materialforschung und -pr¨ ufung in Berlin, Germany provides the CT-scans of hcp.

References 1. Acker P (2001) Micromechanical analysis of creep and shrinkage mechanisms. Creep, Shrinkage and Durability Mechanics of Concrete and other Quasi-Brittle materials: proceedings of the sixth international conference 1:15–25 2. Bernard O, Ulm F-J, Lemarchand E (2003) A multiscale micromechanicshydration model for the early-age elastic properties of cement-based materials. Cement and Concrete Research 33:1293–1309 3. Constantinides G, Ulm F-J (2004) The eﬀect of two types of csh on the elasticity of cement-based materials: Results from nanoindentation and micromechanical modeling. Cement and Concrete Research 34:67–80 4. Geiger C, Kanzow C (1999) Numerische Verfahren zur L¨ osung unrestringierter Optimierungsaufgaben. Springer Verlag 5. Gross D, Seelig T (2001) Bruchmechanik. Springer Verlag 6. Internetlink. National institute of standards and technology; http://ﬁre.nist.gov/bfrlpubs/build00/art060.html. 7. Kolari K, Kouhia R, K¨ arn¨ a T (2002) Ice failure simulation–softening material model. Proceedings of the 16th IAHR International Symposium on Ice, Dunedin, New Zealand, pages 154–159 8. Koster M, Hannawald J, Brameshuber W (2006) Simulation of water permeability and water vapor diﬀusion through hardened cement paste. Computational Mechanics 37(2):163–172 9. Lemaitre J (1996) A course on damage mechanics. Springer Verlag 10. L¨ ohnert S (2004) Computational homogenization of microheterogeneous materials at ﬁnite strains including damage. PhD thesis, Universit¨ at Hannover 11. Pollakowski M (2004) Grundkurs Socketprogrammierung mit C unter Linux. Vieweg Verlag 12. Powers TC (1962) Physical properties of cement paste. Proceedings of the Fourth International Symposium on the Chemistry of Cement; Paper V-1: Physical Properties of Cement Paste 2(43):577–613 13. Powers TC, Brownyard TL (1948) Studies of the physical properties of hardened portland cement paste. Research Laboratories of the Portland Cement Association Bulletin 22:101–992 14. Simo JC, Hughes TJR (1998) Computational Inelasticity. Springer, New York, Berlin 15. Thielecke F (1997) Parameteridentiﬁzierung von Simulationsmodellen f¨ ur das viskoplastische Verhalten von Metallen -Theorie, Numerik, Anwendung-. PhD thesis, Technische Universit¨ at Braunschweig 16. Wedemeier K (1990) Beitr¨ age zur Theorie und Numerik von Materialien mit innerer Reibung am Beispiel des Werkstoﬀes Beton. PhD thesis, Universit¨ at Hannover 17. Zohdi TI, Wriggers P (2004) An Introduction to Computational Micromechanics. Springer Verlag, New York

Numerical Modeling of Transient Impact Processes with Large Deformations and Nonlinear Material Behavior Ekkehard Ramm1 , Tobias Erhart2 and Wolfgang A. Wall3 1

2 3

Institute of Structural Mechanics, University of Stuttgart, Pfaﬀenwaldring 7, 70569 Stuttgart, Germany [email protected] DYNAmore GmbH, Industriestr. 2, 70565 Stuttgart, Germany [email protected]e Chair for Computational Mechanics, Technical University of Munich, Boltzmannstr. 15, 85748 Garching, Germany [email protected]

Summary. A robust computational approach for transient dynamic impact processes will be presented. Main focus will be on an adaptive remeshing strategy and constitutive models for metals and geomaterials under impact loading. Practical relevant numerical examples will complete this contribution. Key words: Impact, Large Deformations, Adaptive Remeshing, Metals, Geomaterials

1 Introduction The present study is concerned with a special case of solid mechanics, where structures are exposed to short-time, highly concentrated loading. Such transient impact processes appear in civil and military security technology, dynamic soil compaction, vehicle crash or fastening and demolition technology. They are characterized by varying non-linearities, as e.g. large deformations and strains, highly non-linear material behavior, frictional contact between multiple bodies and stress wave propagation. Development and combination of diﬀerent methods in the ﬁelds of adaptivity, constitutive modeling, element technology, eﬃcient time discretization and contact are essential for reliable computations and predictions in engineering practice. Accuracy, robustness and eﬃciency are mandatory requirements for the solution of those complex problems. In this contribution, we will mainly focus on two issues, namely adaptive remeshing and constitutive modeling of metals and geomaterials especially Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 123–144. © 2007 Springer. Printed in the Netherlands.

124

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

elaborated for impact loading. The proposed methods are tested for model problems and their performance in relevant industrial applications is veriﬁed.

2 Class of Problems The speciﬁc class of problems focussed in this study excel themselves through a large complexity. Essentially these are fast transient plane strain or axisymmetric problems that are treated in an explicit way. Adopted material models range from simple elastic up to large strain thermo-elastic-viscoplastic models. The problems exhibit large deformations and may even include severe mesh distortion. Frictional contact is an essential feature of the related physical processes.

3 Adaptive Remeshing Since large deformations occur in impact simulations and a Lagrangean description is used, repeated remeshing of individual domains is necessary [6] [21]. To achieve a quality controlled solution and an optimal deployment of used computational resources at the same time, an adaptive strategy is applied [12]. The essential ingredients of an adaptive remeshing strategy in this highly nonlinear regime are (i) a mesh quality check for triggering automatic remeshing, (ii) a reasonable assessment of discretization errors and derivation of a corresponding mesh density distribution, (iii) an automatic mesh generation tool for graded meshes and (iv) methods for the transfer of state variables from old to new discretization. The core of this strategy is the assessment of discretization errors by adequate indicators. Diﬀerent indicators are presented and new methods are developed, which are especially suited for the simulation of transient impact processes. Theoretical deﬁnitions and numerical treatment of these aspects are dealt with. 3.1 Mesh Quality Check In our approach, mesh quality is evaluated for each element by a combination of two geometrical criteria, the so-called ’corner angle criterion’ and the ratio of the radius of the inscribed circle to the radius of the circumscribed circle [12]. If the combination of these two measures, e.g. the mean value falls below a prescribed threshold value for a prescribed number of elements, the remeshing procedure starts automatically. With this mesh quality check, it is guaranteed, that the FE solution is prevented from occurence of a negative Jacobian. 3.2 Error Assessment and Mesh Density Distribution In our approach, three categories of error indicators, gradient-based, local quantity-based as well as geometric, are used for adaptive remeshing [12]. In the following, all indicators that have been studied and implemented are

Numerical Modeling of Transient Impact Processes

125

presented in more detail along with their associated reﬁnement strategy, i.e. the determination of a corresponding mesh density distribution. Gradient-Based Indicators Gradient-based indicators use the fact that there is a connection between the size of local gradients and the quality of solution. Here, ’gradients’ not only mean stresses, but local variations of arbitrary quantitites like strains, plastic work, etc.. The corresponding adaptive remeshing strategy is characterized by an equi-distribution - with respect to the element length - of those gradients in the domain of solution. This leads to a reﬁnement in high gradient zones on the one hand and to a coarsening in low gradient areas on the other hand. Now the question is, which relevant quantities for the gradient calculation should be used to indicate a meaningful error and subsequently govern the mesh density? We have chosen two diﬀerent elastic and one plastic variable, whose gradients are tightly connected to some of the speciﬁc physical phenomena or processes occurring in complex problems like in our applications, depending on the speciﬁc example at hand. The ﬁrst quantity is the von Mises stress (1) ψ1 := µ 2(dev(e ) : dev(e )) which especially tracks elastic shape changing behavior, whereas the second one, the hydrostatic stress (2) ψ2 := κ tr(e ) mainly grasps elastic volumetric changes. Plastic regions in a structure, e.g. localization zones, can be detected with the third quantity ’plastic work’ t ψ3 := J −1 τ : ˙ p dt (3) t0

Gradients of these quantities need to be calculated at all nodes of the old mesh. Therefore, the superconvergent patch recovery technique in an element patch [31] is used to get information about the local gradient at the particular assembly node, i.e. the central node of the patch. According to this method, a least square ﬁt between a polynomial approximation and discrete values (e.g. at quadrature points) leads to a minimization problem. After solution of the corresponding system of linear equations, the norm of the gradient can be calculated at the position of node N (central node of patch) gk := ∇ψk (xN ) = (∇ψk (xN ) · ∇ψk (xN ))

1/2

(4)

The local element size of the new mesh has to be inversely proportional to the size of the local gradient due to the above mentioned reasons. In addition, the magnitude of reﬁnement needs to be controlled in order to adapt the element sizes to the diﬀerent indicator and/or examples. This can be achieved

126

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

by scaling the gradient with a prescribed value ∆ψk , which describes the maximal allowed change of the considered quantity ψk per element. At the end the new element size hnew e,k results in hnew e,k =

∆ψk gk

(5)

Local Quantity Indicators On the basis of pure physical considerations, local reﬁnement indicators can be developed that control the mesh density in the interior mesh. For this purpose, a physically relevant quantity is calculated for each element in the old mesh. The new mesh is then generated provided that this quantity becomes equi-distributed so that every element experiences roughly the same ’physical action’. This obviously results in reﬁnement for high values and in coarsening for small values of this quantity per old element. For these indicators, no gradients need to be calculated. In the following we sketch some of these local quantity indicators that are given in the literature and that we adopted for our study. For problems of strain localization, Ortiz and Quigley [19] proposed an adaptive strategy, which is based on the equi-distribution of variation of the velocity ﬁeld v over the elements of the mesh. Such localization problems can be characterized by large diﬀerences between the mechanical behavior of the global structure and a local zone, e. g. shear bands, bringing along a loss of ellipticity of the governing equations. For a two-dimensional element, this indicator can be expressed as the maximum deviation for the velocity vi of two nodes a and b e e − vib |} (6) φ1 := max{max |via i

a,b

This is a suitable indicator for the analysis of transient processes with wave propagation as well as localization. It is however restricted to dynamic calculations. Singularities in quasi-static zones of transient problems or poor approximations of quasi-static quantities are not treated appropriately. Another physical indicator was used by Batra and Ko [2] for shear bands in plane strain compression and by Camacho and Ortiz [6] for diﬀerent impact and penetration calculations. The intention of this indicator is that the integral of the second invariant of the deviatoric strain-rate tensor over an element 1 dev˙ : dev˙ dv (7) φ2 := 2 ϕ(Ωe ) is the same for all elements. This indicator is capable of resolving strain localizations in dynamic calculations. A third indicator, based on the equi-distribution of plastic power, was developed by Marusich and Ortiz [17] for simulation of high-speed machining: p ˙ J −1 τ : ˙ p dv (8) W dv = φ3 := ϕ(Ωe )

ϕ(Ωe )

Numerical Modeling of Transient Impact Processes

127

This indicator is especially suited for nonlinear, highly dynamic problems with large plastic deformations, since it leads to reﬁnement in high strain rate regions. In order to be able to combine diﬀerent indicators later, we adopt here a similar strategy as before. At ﬁrst, the elementwise calculated quantities φl are related to the respective old element size hold e g˜l =

φl hold e

(9)

Now we use the same reﬁnement strategy as we did for the gradient-based error indicators, i.e. the new element size is inversely proportional to the ’variation per element’ g˜l and it is scaled by a prescribed value ∆φl hnew e,l =

∆φl g˜l

(10)

Geometric Indicator Strongly curved surfaces have to be discretized with suﬃciently small elements to avoid signiﬁcant ’geometrical errors’. This is especially important with respect to mass conservation and in contact situations. The curvature of the boundary is used as a geometric indicator to control this problem. However, this indicator is only activated if it suggests reﬁnement of the ’mechanical’ indicator driven mesh density. In case of a discrete boundary description, e.g. the polygonal boundary of a ﬁnite element mesh, the discrete curvature κh at the position of a ﬁnite element node is given as κh :=

2ϑ s1 + s2

(11)

where ϑ is the smaller angle between two boundary segments with lengths s1 and s2 , respectively. If this measure is calculated for boundary nodes of the old mesh, the element size in the new mesh results in hnew e,g =

ϑadm κh

(12)

where ϑadm is a prescribed value, which can be interpreted as admissible angle between two adjacent boundary segments. A similar indicator was used by Camacho and Ortiz [9]. In general, through application of this indicator, there is no connection between internal element size and boundary element size. In such cases, a mesh smoothing technique is used to avoid large diﬀerences between element sizes in the interior and at the boundary. Selection of Indicators and Final Mesh Density Distribution The objective of the diﬀerent indicators and possible application areas have been given above. For real and complex applications the question of the ﬁnal selection of indicator remains. Which speciﬁc indicator or combination of

128

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

diﬀerent indicators should be used? The answer is both trivial and diﬃcult at the same time. It should be rather clear from the above discussion which indicators are not suited in which cases. The ﬁnal selection however can only be based on engineering intuition and on a deep insight into the physics of the problem or the class of problems. It is crucial to know what the governing phenomena and the dominating processes are. One should be aware that the answers not only depend on the problem itself but also on the respective quantities of interest of a speciﬁc simulation. To obtain the ﬁnal mesh density, two further steps are needed. As already pointed out it is in some cases useful to combine diﬀerent error indicators. For this purpose, the minimum of the diﬀerent element sizes hnew e,k (which be(which belong to the three long to the ﬁve gradient-based indicators), hnew e,l (the geometric indicator for the boundary) local quantity indicators) and hnew e,g has to be chosen as ﬁnal element size new new = min{hnew hnew e e,k , he,l , he,g }

(13)

On the other hand, the element size has to be restricted by some prescribed threshold values, because undesirably small elements (time step size in explicit scheme!) or large elements (approximation quality!) should be avoided: ≤ hnew ≤ hmax hmin e e e

(14)

3.3 Mesh Generation Generating a graded mesh needs two sources of information: the boundary of the domain and the mesh density inside the domain mostly given on a background mesh. In our case of large deformations and changing topologies the background mesh is preferably the old mesh of the preceding time step, for which the error assessment is done and the mesh density distribution is calculated. Secondly, a polygonal description of the boundary has to be provided. Boundary nodes must be generated adaptively, i.e. subject to the calculated mesh density. Special care has to be taken of boundaries in contact situations. The re-ordering of nodes on convexly curved boundaries during remeshing can result in sudden gaps between contacting bodies, which results in socalled ’remeshing shocks’: oscillations induced by unphysically high contact forces. This is remedied by a smooth contact formulation combined with a procedure for precise surface recovery [9]. After that, a new ’almost-all-quad’ mesh is generated inside the domain by an ’advancing front method’ starting from these previously generated boundary nodes and based on the given mesh density found at the nodes of the old mesh [16] [20]. In exceptional cases, e.g. for sharp corners, triangular elements (e.g. CST - constant strain triangles) are also allowed. This has the advantage, that no ’bad quads’ have to be generated and therefore the time span until next remeshing is increased.

Numerical Modeling of Transient Impact Processes

129

3.4 Transfer of State Variables Since results are determined in an iterative or in an incremental process for nonlinear or transient problems, a transfer of state variables between old and new spatial discretization is essential [21] [6]. Examples of variables, which have to be ’mapped’ are strains, stresses, velocities, boundary conditions, etc., i.e. a mapping strategy for both nodal and integration point data is needed. The location and number of nodes and integration points changes totally in case of complete remeshing of a domain. Therefore, the location of new points in the old mesh has to be determined by an intelligent search algorithm, e.g. directional search [20], and thereafter, state variables have to be transfered by a suitable mapping method like inter/extrapolation [21], inverse distance weighting [8] or moving least square techniques [31] [26]. Especially in the context of explicit time integration the quality of the mapping scheme is crucial. Since mapping cannot be supplemented by equilibrium iterations in these cases mapping errors may propagate and pollute the whole simulation. Other aspects like minimization of diﬀusion should be met as in implicit situations.

4 Constitutive Modeling Based on the theory of ﬁnite plasticity, constitutive models for thermoviscoplastic metals and cohesive as well as non-cohesive frictional materials are presented and developed. One focus will be on a formulation for loose, granular media under high pressure loadings. For this a Drucker-Prager-Cap model is modiﬁed and enhanced. The properties and eﬀects of the developing powder will be examined. Our implementation of ﬁnite strain plasticity is based on the multiplicative split of the deformation gradient into elastic and plastic parts F = Fe Fp and an isotropic Eulerian formulation in eigenvalues [24] [23] [18]. Using a spectral decomposition of the Finger-tensor b = FFT and the Kirchhoﬀ stress tensor τ = Jσ, a general return mapping scheme with elastic predictor and closest point projection algorithm formulated in principal logarithmic strains = 1/2 ln(b) = [1 , 2 , 3 ]T and in principal Kirchhoﬀ stresses τ = [τ1 , τ2 , τ3 ]T is applied. With this approach, which is valid for isotropic materials, the functional form of the return mapping is identical to the algorithm of the inﬁnitesimal theory [23]. Therefore, the whole scheme with elastic predictor, plastic corrector etc. is not shown here, but only the most important parts of our models are presented brieﬂy. 4.1 Metals The mechanical behavior of metals under transient impact loadings is mainly aﬀected through strain rate and temperature. Therefore, a Johnson-Cook plasticity model [15] is used, where the yield limit is a function of eﬀective plastic

s y ) B(å p)

k1

plastic strain

ǒ

.p

1 ) C ln 1 ) å. å0 plastic strain rate

Ǔ

yield limit

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

yield limit

yield limit

130

1 * (T *) k2

temperature

Fig. 1. Qualitative inﬂuence of strain, strain rate and temperature on yield limit in Johnson-Cook plasticity model p strain ¯p , eﬀective plastic strain rate ¯˙ and absolute temperature T : 2 p p q(¯ , ¯˙ , T ) ≤ 0 f (τ , q) = s − 3

with norm of stress deviator s = dev(τ ) and yield limit p ¯˙ p k 1 + C ln 1 + 1 − (T ∗ )k2 q(¯ p , ¯˙ , T ) = σy + B(¯ p ) 1 ¯˙ 0

(15)

(16)

σy indicates the static yield limit and material parameters B and k1 describe the strain hardening behavior (see Fig. 1). The increase of strength due to high strain rates, i.e. the viscosity, is considered through the second term of eq. (16). Factor C quantiﬁes the strain rate dependency, whereas the rate of plasp tic strain ¯˙ is normalized by ¯˙ = 1.0 [1/s]. With the last part in (16), the eﬀect of decreasing strength for high temperatures is reproduced: The homologous temperature T ∗ = (T − T0 )/(Tm − T0 ) is a measure for the mobility of crystal grid components and is modeled as a function of current temperature T , room temperature T0 and melting temperature Tm . This non-dimensional variable ranges from 0 (current = room temp.) to 1 (current = melt. temp.). Thermal softening is controlled by exponent k2 . Since transient impact and penetration processes are of very short duration, adiabatic temperature changes are assumed in our study. In addition, for the local temperature evolution, the empirical assumption is used, that most (90-100 percent) of the plastic work W p is transformed into heat ηd −1 T p ηd ˙ p W = J τ ˙ , 0.9 ≤ ηd ≤ 1.0 T˙ = cv cv

(17)

with density , grade of dissipation ηd and speciﬁc heat capacity cv . The return mapping algorithm ends up in a local Newton iteration, where plastic strain and plastic strain rate are the implicitely considered unknowns, whereas the temperature is accounted for in an explicit manner, i.e. it is computed from previous time step values.

Numerical Modeling of Transient Impact Processes

131

Fig. 2. Failure modes of geomaterial under impact loading (left) and typical compaction behavior of powder (right)

4.2 Geomaterials A constitutive model for cohesive and non-cohesive frictional materials will be presented, which is especially suited for dynamic impact processes. During a high velocity impact acting on cohesive frictional material (e.g. sandstone), a crushed zone appears directly under the impactor nose. In this region of highly conﬁned loading, the intact material disintegrates and loose, granular or powder-like media develops. Realistic description of this powderization and the material modeling of powder itself are important topics of our study. Characterization of Geomaterials Under Impact Loading Considering a solid structure made of intact, cohesive frictional material (e.g. concrete, sandstone, rock) under transient impact loading, diﬀerent states of stress and therefore diﬀerent states of failure can be observed, which we divided into three zones (Fig. 2): (i) high-pressure driven crushing (or powderization) directly under the impactor, (ii) moderate compaction due to mixed compression/shear loading and (iii) tensile fracture with low shearing. As already stated above, our main focus will be on the ﬁrst part, where compact cohesive frictional material is going to be totally disintegrated to loose, granular powder. The material will obviously change its mechanical properties during this crushing process. Due to comminution, a higher density can be achieved than with the original material. This densiﬁcation reserve leads to a temporary decrease of hardening behavior and an increase of maximal density. Additionally, crushing causes total loss of internal cohesion due to particle and matrix breaking, which results in full decrease of cohesion and tensile strength on macroscopic level. The eﬀect becomes obvious, when the evolved powder gets unloaded and loaded in the opposite direction (i.e. tension): Without tensile strength and cohesive capability, unlimited motion of powder particles is possible and dilatant loosening of the material will be observed. Since powder-like materials are distinctly compressible, depending

132

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

on the initial density, they can have severe damping and energy absorbing eﬀects in dynamic impact processes that are of interest in a number of different applications. Herein, the kinetic energy of a system is transformed into internal energy by a relative volume change of the powder (Fig. 2). A better understanding of this phenomenon is needed to extenuate or to intensify the damping and energy absorbing inﬂuence of powder in a quantitative and predictable way. In our investigations, the powder material of interest is of dry ﬁne sand type. In this study, a continuum cap model for the numerical simulation of geomaterials under quasi-static as well as dynamic loading is presented. A nonsmooth multisurface plasticity model with tension cutoﬀ, Drucker-Prager failure envelope and strain hardening cap provides the reproduction of the relevant phenomena: tensile failure, material ﬂow under shearing and compaction under pressure. For the comminution process, i.e. the transition from intact, cohesive frictional material to loose, granular media, this model will be enhanced. It includes a criterion for the powder development, diﬀerent evolution laws for material parameters like tensile strength, cohesion and compressibility and a modiﬁed hardening law. Modified Drucker-Prager-Cap Model The original multi-surface plasticity model consists of a nonlinear DruckerPrager cone for shear failure, an elliptical cap for compressive strain hardening and a limit in the tension region for tensile failure [22] [7] [13]. Therefore, the elastic region is bounded by following three yield criteria: f1 (τ ) := s − Fe (I1 ) ≤ 0 f2 (τ , q) := Fc (s , I1 , q) − Fe (q) ≤ 0

(18)

f3 (τ ) := I1 − T ≤ 0 These yield surfaces f1 = 0, f2 = 0 and f3 = 0 (see Fig. 3) are functions of stress invariants I1 = tr(τ ) and s = dev(τ ) as well as functions Fe (I1 ) := α − λ exp(βI1 ) − θI1

and

(19)

1 2 (q − I1 ) (20) R2 Fe deﬁnes the nonlinear Drucker-Prager cone and Fc describes the elliptical cap. The transitions between yield surfaces is discontinuous with two so-called corner regions. At the position, where cap and shear failure envelope intersect, we have q − X(q) (21) Fe (I1 = q) = R Fc (s , I1 , q) :=

2

s +

Numerical Modeling of Transient Impact Processes

133

Fig. 3. Yield surfaces of Drucker-Prager Cap plasticity in meridian plane

with hydrostatic compressive strength X(q) = q − R(α − λ exp(βq) − θq)

(22)

Material parameters of this formulation are the Drucker-Prager parameters α, λ, β and θ, the cap ellipticity R, the initial hydrostatic compressive strength X0 and the hydrostatic tensile limit T . Internal variable q < 0 is a function of volumetric plastic strain and it is responsible for the position and movement of the cap (hardening). The original Drucker-Prager-Cap (DPC) model of Hofstetter et al. [13] comes with associated ﬂow rules for all three failure surfaces. However, we will use non-associated ﬂow rules for the Drucker-Prager cone section and the tensile region to get rid of discontinuous ﬂow directions in both corners and to receive less dilatant behavior for shear failure, which seems to be more realistic from an experimental point of view [25]. Finally, our three ﬂow directions m1 , m2 and m3 are given by: −q ∂Fe (I1 ) I1 −q s s − IT1−q 1 = + (λβ exp(βI ) + θ) m1 := s 1 ∂I1 s T −q 1 m2 :=

s s Fc (s,I1 ,q) s

m3 :=

s s Fe (T ) s

−

q−I1 R2 Fc (s,I1 ,q)

+ 1− 1+

∂Fe (T ) ∂I1

1 s Fe (T )

(23) 1

A comparison between associated and non-associated ﬂow directions for the DPC model is shown in Fig. 4. Assuming that the relation between pressure and volume change is known from triaxial experiments, a strain hardening law can be deﬁned, which describes the dependence of internal variable q from volumetric plastic strain pvol = tr(p ). Here, two similar functions for that relation are provided. The

134

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Fig. 4. Flow directions of DPC model: associated and non-associated

ﬁrst one was proposed by Sandler and Rubin [22], whereas the second one was developed for better agreement with our experimental results for dry ﬁne sand type: ⎧ ⎨ W (exp (D(X(q) − X0 )) − 1) Sandler and Rubin [22] p vol = (24) ⎩ X(q)−X0 DW 1−D(X(q)−X Erhart et al. [11] 0) In Fig. 5 both hardening functions are shown. It can be observed, that the second curve (representing the second hardening law [11]) approaches the asymptote at pvol = −W in a more moderate way. In triaxial experiments, cohesive as well as non-cohesive geomaterials show a dependence from third invariant of stress deviator J3 = det(s) when it comes to failure. To reproduce this behavior in simulations, we scale all three yield surfaces with the Willam-Warnke function [28] 2(1 − e2 ) cos υ + (2e − 1) 4(1 − e2 ) cos2 υ + 5e2 − 4e (25) r(υ, e) = 2 4(1 − e2 ) cos2 υ + (2e − 1) with Lode angle 1 υ = arccos 3

√ 3 3 J3 2 (J2 )1.5

(26)

In our algorithm, the third stress invariant is considered in an explicit sense, i.e. Lode angle υ is calculated at tn and then yield surfaces are scaled with the Willam-Warnke function r(υ, e) at tn+1 . Therefore, the stress update algorithm is not aﬀected here. Powderization Under High Pressure With the plasticity model presented above, it is possible to reproduce the mechanical behavior of compact, cohesive geomaterials (sandstone, concrete,

Numerical Modeling of Transient Impact Processes

135

hydrostatic pressure

* X(q) Sandler & Rubin (1979):

ǒ

X(q) + X 0 )

å

p vol

p

p DW ǒ1 ) å vol ńWǓ

1ńD X0

Ǔ

å vol X(q) + X 0 ) 1 ln 1 ) D W

Erhart et al. (2005):

volumetric plastic strain

p * å vol

hydrostatic compression test

W

Fig. 5. Strain hardening laws for modiﬁed DPC model

mortar, etc.) as well as loose, granular media (sand, powder, etc.). The distinction between them is achieved by appropriate choice of material parameters. Now, this model will be enhanced in order to describe the transition from compact to loose material, i.e. the powderization under high pressure. At ﬁrst, a criterion is needed, which indicates the beginning of powder formation. On the other hand, a consistent transition from ’compact’ to ’loose’ is necessary. Therefore, a strategy is developed, where a new internal variable is used to modify the material parameters tensile strength (T ) and cohesion (α, λ). Additionally, hardening response is modiﬁed in loading and unloading to grasp the diﬀerent behavior of cohesive and non-cohesive material. In our approach, a stress dependent criterion is used as ’powderization indicator’ 1 − 2ν δ < δcrush 1+ν

and

I1 < I1,crush

(27)

where δcrush and I1,crush are material parameters and factor δ (’triaxiality’) is a function of stress invariants [14]: I1 δ=− √ √ 2 3 J2 cosυ

(28)

With this criterion, beginning of crushing is detected for very high pressures and highly conﬁned material (e.g. under impactor nose). If the criterion is fulﬁlled, tensile strength and cohesion will decrease, which is reproduced by softening in tension and shear regime in our constitutive model. Therefore, material parameters α, λ and T are now functions of new internal crushing variable qc . Following the hardening law (section 4.3), this history variable is chosen in such a way that it is identical with the 1/D-scaled volumetric plastic strain, which develops after the beginning of powderization: ⎧ 1 p p p ⎨ D ˙vol if ˙vol > ˙vol,crush (29) q˙c = ⎩ 0 else

136

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Shear strength α − λ at I1 = 0 is reduced by modiﬁcation of the nonlinear Drucker-Prager yield surface with following exponential softening (given in incremental form) q λn+1 = αn − (αn − λ0 ) exp − qc,n cu (30) αn+1 = αn + (λn+1 − λn ) exp(βqn ) with material parameter qcu controlling the reduction intensity. With these two equations it is guaranteed, that the position of the cap is not changed in the current time step. To receive the same amount of softening for the tensile limit, following nonlinear equation has to be solved for unknown Tn Fe (T0 ) Fe (Tn ) = Tn T0

(31)

The increase of hydrostatic compressive strength X(q) with increasing plastic compression (i.e. the expansion of the cap) is controlled by hardening law (24). On the other hand, the contraction of the cap due to dilatant plastic ﬂow in shear or tension depends on the material at hand. Loose, granular media like sand or powder is able to break up quite easily due to missing cohesion, whereas for intact cohesive geomaterials like concrete this phenomenon is not very distinct. We incorporated this observation in our model by allowing cap contraction only for powder-like materials (see Fig. 6). As already mentioned above, comminution of initially compact material has the consequence that a higher compaction is possible, clearly depending on the initial density. This phenomenon was observed in experiments [30] [29] and is incorporated in our model by modiﬁcation of the original hardening law. In Fig. 7, this modiﬁed hardening/loosening behavior is shown schematically. At point A, the intact material begins to deform plastically under hydrostatic pressure. Further increase of loading leads to an increase of density (contraction). At point B, powderization begins and hardening slope is less than before. Now, the material is crushed and condensed and therefore, higher compaction is possible (C) compared to a load path without powderization (C’). The transition from B to C is deﬁned analog to the usual hardening law øsø

øsø

loose material: loosening (cap contracts)

intact material: no loosening (cap remains) I1

Fig. 6. Diﬀerent cap treatment for dilatant plastic ﬂow

I1

Numerical Modeling of Transient Impact Processes pressure * X(q)

start of powderization

137

extra compression C’

C

dense powder

densification

B intact material loose powder E

loosening

A

D dilatation

contraction

p * å vol volumetric plastic strain

Fig. 7. Modiﬁed hardening for geomaterials with powderization

with two new material parameters Wcrush and Dcrush . If the highly condensed powder is now loaded in shear or tensile direction (dilatant plastic ﬂow), loosening of the material and a decrease of hydrostatic compressive strength can be observed (C → D). Further reduction of powder density is achieved with nearly no eﬀort, i.e. unlimited ﬂow of the material is possible.

5 Numerical Examples Practical relevant applications will demonstrate the performance of our overall approach. In Sec. 5.1, adaptive simulations with high-speed deformations of metals will be presented, followed by several geomaterial computations with our modiﬁed DPC model in Sec. 5.2. 5.1 Adaptive Computations To demonstrate the eﬀectiveness of our adaptive strategy and to examine the suitability of diﬀerent error indicators for large deformation transient problems, three numerical examples will be presented: Taylor bar impact, highstrain rate compression of WHA block and penetration of a steel cylinder by WHA long rod. For a detailed description of model settings, material parameters, etc. we refer to [12]. Here, only short descriptions of most interesting results are given. Taylor Bar Impact A cylindrical rod made of soft metal hits a rigid wall with high velocity [27] [6]. During the impact, elastic and slower plastic waves are initiated, propagating

138

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

t + 20ms

t + 40ms

smooth changes in time

t + 80ms

Fig. 8. Taylor bar impact with indicator ’gradient of plastic work’: Adaptive meshes and plastic energy (0–1500 Nmm)

t + 20ms

t + 40ms

t + 80ms

propagating plastic wave

Fig. 9. Taylor bar impact with indicator ’plastic power’: Adaptive meshes and plastic strain rates (0-75000 1/s)

in axial direction and reﬂecting at the bar tails. Therefore, the initial kinetic energy is transformed into internal energy and large plastic deformations can be observed. In our analysis, we compared diﬀerent error indicators. In Figs. 8 and Fig.9 the interrelation between adaptive meshes and choice of indicators is illustrated. The indicator ’gradient of plastic work’ causes a smooth and continuous growth of ﬁne mesh regions being consistent with the evolving plastic zone (Fig. 8). The indicator ’rate of plastic work’ also depicts the connection between adaptive discretizations and the corresponding physical/mechanical process: Reﬁnement occurs where rate of plastic strain is very high, i.e. where current material ﬂow takes place. Therefore, the propagating plastic wave is accompanied by a shift of ﬁne mesh region (Fig. 9).

Numerical Modeling of Transient Impact Processes

139

Fig. 10. WHA block: Adaptive meshes and temperature distribution

High-Strain Rate Compression of WHA Block In the second example, a prismatic metal block undergoes highly dynamic compression, which causes large plastic strains, which again eﬀects signiﬁcant temperature rise [3]. The involved thermal softening ﬁnally results in adiabatic shear bands, i.e. strain localization in consequence of heat. Figure 10 shows the evolution of shear bands represented by temperature distributions and appropriate adaptive meshes. For error assessment, the local quantity indicator ’variation of velocity’ was used as reﬁnement indicator. This indicator is well suited here, since dynamically developing strain localizations are detected automatically. The development of localizations results in expedient mesh reﬁnements, which again provide high resolutions in corresponding regions. Penetration of a Steel Cylinder by WHA Long Rod A cylindrical rod made of tungsten heavy alloy (WHA) hits an externally clamped cylindrical block made of high-strength steel at high velocity [6] [1]. Figure 11 shows deformed meshes and appropriate equivalent plastic strain distributions at time instances 20 µs and 40 µs with a logarithmic spectrum. The physical process gets obvious: The impactor penetrates the steel cylinder and produces a deep crater. At the same time, the melted tungsten is pressed outwards and the bar almost completely erodes. Plastic deformations are very high in both parts. These phenomena can be observed in experiments [1] and in corresponding simulations [6] in the same way. In our calculation with repeated remeshings, the spatial discretization adaptively follows the transient process. At the beginning, strong reﬁnement in the process zone under the impactor is ascertained. Beyond this area of high plastic deformation, the material behaves elastically and therefore the mesh density is relatively low. The ﬁne mesh region increases with proceeding penetration depth. The error indicator

140

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

Fig. 11. Adapive meshes and equivalent plastic strains of WHA long rod penetration

’gradient of plastic work’ is apparently well suited to follow the physics of this problem in an intelligent way. 5.2 Geomechanical computations In this section, we present some results from numerical simulations with our enhanced DPC model for geomaterials. More detailed descriptions of these examples can be found in [11] and [10]. Quasi-Static Tests First, veriﬁcation and evaluation was done on diﬀerent quasi-static tests like conﬁned or hydrostatic compression for several geomaterials [4] [5] [29]. After identiﬁcation of appropriate material parameters good correlation with experimental results can be achieved (see Fig. 12). Here, especially the third diagram of a hydrostatic compression test on sandstone [29] has to be pointed out, since the distinct change of hardening behavior due to powderization is well captured by our modiﬁed DPC model. Triple Impact on Microconcrete A steel rod with spherical tail hits the surface of a ﬁne grade concrete [10]. Due to the impacts, the material powderizes in a small zone directly under the impactor, which is kept in our model through the criterion described in Sect. 4.2: In Fig. 13, ’powderized elements’ are represented by dark grey coloring. Additionally, the evolution of the hydrostatic compressive stress is shown for point A: The densiﬁcation and loosening of the comminuted material leads to increasing strength followed by decreasing strength for every single impact. On the other hand, this behavior is not discovered for the intact microconcrete

Numerical Modeling of Transient Impact Processes axial stress [N/mm2]

concrete

mortar

axial stress [N/mm2]

effective stress [N/mm2] experiment

1250

2000

141

1000

simulation

600 powderi– zation

450

1500 750

300

1000

500

500

150

250

0

0 0

0,05

0,10

0,15

0,20

0 0

0,05

axial strain [-]

0,10

0,15

0,20

0

axial strain [-]

0,04

0,08

0,12

volume change [-]

Fig. 12. Conﬁned compression and hydrostatic tests [4] [5] [29] hydrostatic compressive strength X(q) 0 A

–1000 powder (Point A)

intact microconcrete (Point B)

B

–2000

increase of strength

3rd impact

–3000 1st impact

2nd impact

time t [ms]

–4000 0

0,5

1,0

1,5

2,0

decrease of strength

Fig. 13. Results from triple impact on ﬁne grade concrete

(point B). Hence it follows that part of the kinetic energy is dissipated by the arised powder layer. Further inspection of this phenomenon will be done in our last example. Dynamic Compaction of Powder This example could be deemed to be a ’dynamic oedometer test’, i.e. we carried out dynamic compression (with several impacts) of conﬁned dry ﬁne sand type powder measuring penetration depth and contact force [11]. In the penetration-time diagram (Fig. 14), the periodical indentation for three diﬀerent layer heights can be observed as well as the decrease of penetration depth after a maximum compression was reached. As gets obvious from Fig. 14 the experimental and numerical results are in good agreement for all three thicknesses. The time dependent behavior of the contact force shows the damping eﬀect of powder (Fig. 14). The periodical impact causes peak loads at the

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall force [kN]

142

penetration [mm] 0,0

1 mm

-0,2

45 30

0

5 mm

force [kN]

-0,4

simulation

time [ms]

0

3 mm

-0,6

1 mm

15

-1,0 0

0,2

0,4

0,6

time [ms]

0,8

1,0

1,2

force [kN]

experiment

0,4

0,6

0,8

1,0

1,2

45 30

3 mm

15 0 0

-0,8

0,2

0,2

0,4

0,6

0,8

1,0

1,2

0,6

0,8

1,0

1,2

45 30

5 mm

15 0 0

0,2

0,4

Fig. 14. Evolution of penetration and contact force in dynamic compression of powder

same instances but they are diﬀerent in size depending on the layer thickness. Also the time of maximum contact force is delayed with increasing height. The amount of absorbed energy, i.e. the grade of damping by powder depends on layer thickness and initial density.

6 Conclusion High-velocity impact problems are physically extremely complex and therefore numerically very demanding. The speciﬁc challenge is due to the interaction of several areas like large deformations exhibiting large strains needing eﬃcient adaptive schemes, dynamic frictional contact algorithms avoiding nonphysically oscillations of contact forces and in particular distinct non-linear material models. It was found that the applied explicit formulation was very successful. It came along with time step control and continuous updates of the FE meshes based on physically motivated error indicators. Impact automatically drives the constitutive response into the highly non-linear range. Despite this fact macroscopic continuum based material models turned out to be sufﬁcient for a realistic simulation of the structural response, both for metals as well as for geomaterials. It is remarkable that one constitutive model, namely the Drucker-Prager-Cap plasticity model, is rich enough to represent the material disintegration of geomaterials from the intact phase via a powderization stage with a subsequent hardening to a potential loosening after unloading. It opens a large variety of applications from soil compaction to fasting problems, demolition techniques, crash simulations and other impact problems in civil and military engineering.

Numerical Modeling of Transient Impact Processes

143

References 1. Anderson Jr CE, Hohler V, Walker JD, Stilp AJ (1995) Time-resolved penetration of long rods into steel targets. Int J Imp Engrg 16:1–18 2. Batra RC, Ko KI (1992) An adaptive mesh reﬁnement technique for the analysis of shear bands in plane strain compression of thermoviscoplastic solid. Comput Mech 10:369–379 3. Batra RC, Peng Z (1995) Development of shear bands in dynamic plane strain compression of depleted uranium and tungsten blocks. Int J Imp Engrg 16:375– 395 4. Bazant ZP, Bishop FC, Chang TP (1986) Conﬁned compression tests of cement paste and concrete up to 300 ksi. J Amer Conc Inst 83:553–560 5. Burlion N, Pijaudier-Cabot G, Dahan N (2001) Experimental analysis of compaction of concrete and mortar. Int J Num Anal Meth Geomech 25:291–308 6. Camacho GT, Ortiz M (1997) Adaptive Lagrangian modelling of ballistic penetration of metallic targets. Comput Meth Appl Mech Engrg 142:269–301 7. Chen WF, Baladi GY (1985) Soil plasticity – Theory and implementation. McGraw Hill, New York 8. Dyduch M, Habraken AM, Cescotto S (1992) Automatic adaptive remeshing for numerical simulation of metalforming. Comput Meth Appl Mech Engrg 101:283–298 9. Erhart T, Taenzer L, Diekmann R, Wall WA (2001) Adaptive remeshing issues for fast transient, highly nonlinear processes. In Waszczyszyn Z, Pamin J (eds) Proceedings of ECCM 2001. Cracow, Poland 10. Erhart T (2004) Strategien zur numerischen Modellierung transienter Impaktvorgaenge bei nichtlinearem Materialverhalten. PhD Thesis, Institute of Structural Mechanics, University of Stuttgart, Germany 11. Erhart T, Wall WA, Ramm E (2005) A robust computational approach for dry powders under quasi-static and transient impact loadings. Comput Meth Appl Mech Engrg 194:4115–4134 12. Erhart T, Wall WA, Ramm E (2006) Robust adaptive remeshing strategy for large deformation, transient impact simulations. Int J Num Meth Engrg 65:2139–2166 13. Hofstetter G, Simo JC, Taylor RL (1993) A modiﬁed cap model: Closest point solution algorithms. Comput Struct 46:203–214 14. Hofstetter G, Mang HA (1995) Computational mechanics of reinforced concrete structures. Vieweg & Sohn, Braunschweig/Wiesbaden 15. Johnson GR, Cook WH (1985) Fracture characteristics of three metals subjected to various strains, strain rates, temperatures and pressures. Engrg Fract Mech 21:31–48 16. Lo SH (1985) A new mesh generation scheme for arbitrary planar domains. Int J Num Meth Engrg 21:1403–1426 17. Marusich TD, Ortiz M (1995) Modelling and simulation of high-speed machining. Int J Num Meth Engrg 38:3675–3694 18. Miehe C (1998) A formulation of ﬁnite elastoplasticity based on dual co- and contravariant eigenvector triads normalized with respect to a plastic metric. Comput Meth Appl Mech Engrg 159:223–260 19. Ortiz M, Quigley JJ (1991) Adaptive mesh reﬁnement in strain localization problems. Comput Meth Appl Mech Engrg 90:781–804

144

Ekkehard Ramm, Tobias Erhart and Wolfgang A. Wall

20. Peraire J, Vahdati M, Morgan K, Zienkiewicz OC (1987) Adaptive remeshing for compressible ﬂow simulations. J Comp Phys 72:449–466 21. Peric D, Vaz Jr. M, Owen DRJ (1999) On adaptive strategies for large deformations of elasto-plastic solids at ﬁnite strains: Computational issues and industrial applications. Comp Meth Appl Mech Engrg 176:279–312 22. Sandler IS, Rubin D (1979) An algorithm and a modular subroutine for the cap model. Int J Num Anal Meth Geomech 3:173–186 23. Simo JC (1992) Algorithms for static and dynamic multiplicative plasticity that preserve the classical return mapping schemes of the inﬁnitesimal theory. Comput Meth Appl Mech Engrg 99:61–112 24. Simo JC, Miehe C (1992) Associative coupled thermoplasticity at ﬁnite strains: Formulation, numerical analysis and implementation. Comput Meth Appl Mech Engrg 98:41–104 25. Smith SS, Willam KJ, Gerstle KH, Sture S (1989) Concrete over the top, or: Is there life after peak? ACI Mat J 86:491–497 26. Tabbara M, Blacker T, Belytschko T (1994) Finite element derivative recovery by moving least square interpolants. Comput Meth Appl Mech Engrg 117:211– 223 27. Taylor G (1948) The use of ﬂat-ended projectiles for determining dynamic yield stress. I. Theoretical considerations. Proc Roy Soc London, Series A, Math Phys Sci 194:289–299 28. Willam KJ, Warnke E (1975) Constitutive model for triaxial behavior of concrete. In: Proc. Concrete structures subjected to triaxial stresses, International Association for Bridge and Structural Engineering, Section III: 1–30 29. Wong TF, Szeto H, Zhang J (1992) Eﬀect of loading path and porosity on the failure mode of porous rocks. Appl Mech Rev 45:281–293 30. Zhang J, Wong TF, Davis DM (1990) Micromechanics of pressure-induced grain crushing in porous rocks. J Geophys Res 95:341–352 31. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. Part 1: The recovery technique. Int J Num Meth Engrg 33:1331–1364

A Computational Model For Viscoplasticity Coupled with Damage Including Unilateral Eﬀects D.R.J. Owen1 , F.M. Andrade Pires2 and E.A. de Souza Neto1 1

2

Civil and Computational Engineering Centre, School of Engineering University of Wales Swansea, Singleton Park, Swansea SA2 8PP, UK [email protected], [email protected] DEMEGI – Department of Mechanical Engineering and Industrial Management, Faculty of Engineering, Oporto University, Rua Dr. Roberto Frias, s/n, 4200-465 Porto, Portugal [email protected]

Summary. This contribution is concerned with the numerical modelling of nonlinear solid material behaviour in the presence of ductile damage. The description of the complex inelastic material behaviour is accomplished by coupling the elastoviscoplastic constitutive model, discussed by Peri´c (1993)[1], with a ductile damage evolution law, introduced by Ladev`eze & Lemaitre (1984) [2]. The evolution of the damage internal variable includes the important eﬀect of micro-crack closure, which may dramatically decrease the rate of damage growth under compression [3]. The theoretical basis of the material model and the computational treatment, within the framework of a ﬁnite element solution procedure, are presented. The resulting integration algorithm reduces to the solution of only one scalar non-linear equation and generalizes the standard return mapping procedures of the inﬁnitesimal theory. Numerical tests of the integration algorithm, which rely in the analysis of iso-error maps, are provided.

1 Introduction The numerical treatment of diﬀerent material phenomena, in the context of ﬁnite element simulations, has been addressed in several publications (see [4, 5, 6, 7, 8, 9, 10, 11] and references therein) during the last three decades or so. As a result, a wide range of material models, incorporating elastic, viscoelastic and elasto-plastic material behaviour is currently available in standard commercial ﬁnite-element codes. The computational algorithms that model the inelastic material behaviour have achieved a high degree of maturity. This is particularly true for the isotropic material response and situations

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 145–164. © 2007 Springer. Printed in the Netherlands.

146

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

in which diﬀerent rheological phenomena (elasticity, viscoelasticity, plasticity) can be considered independently of each other. Despite such developments, it is often necessary to enhance the constitutive description to describe noticeable features of the material behaviour and also to formulate models with greater predictive capability. Here, we are particularly interested in the inelastic constitutive description of materials subjected to forming operations. These processes are usually characterised by the presence of extreme deformations and strains, often resulting in localised material deterioration with possible fracture nucleation and growth. Rate sensitivity and strain rate eﬀects are also known to have a signiﬁcant role in the constitutive description. In many relevant practical problems, even when the material is initially isotropic, plastic ﬂow is usually responsible for inducing anisotropy. In this case, the experimental identiﬁcation of material parameters becomes a very diﬃcult and complicated task, with very few examples in the published literature. Bearing in mind that a model intended to represent such phenomena should be simple enough to allow eﬃcient numerical treatment and easy experimental veriﬁcation of material parameters, this work is restricted to situations in which the overall behaviour can be regarded as isotropic. Therefore, a scalar damage variable is chosen to represent the material internal degradation. The assumption of isotropic damage in many cases is not too far from reality, as a result of the random shapes and distribution of the included particles that trigger damage initiation and growth. The purpose of this contribution is the formulation and numerical implementation of a phenomenological constitutive model for elasto-viscoplastic solids, capable of handling regions of high rate-sensitivity to rate independent conditions in the presence of ductile damage. The description of the complex inelastic material behaviour is accomplished by coupling a power-law elasto-viscoplastic constitutive model [1, 12], which is widely accepted for the description of rate-dependent deformations of solids, with a ductile damage evolution law [2, 13]. The damage growth is inﬂuenced by the hydrostatic stress state and includes the important eﬀect of micro-crack closure. The introduction of unilateral damage eﬀects allows for a clear distinction between states of identical triaxiality but stresses of opposite sign (tension and compression) in the damage evolution. This eﬀect may dramatically decrease the rate of damage growth under compression, which was highlighted by numerical tests carried out by the authors [3]. The chapter is organized as follows: Section 2 discusses the essential assumptions of the model and outlines the set of constitutive equations that govern the coupled elasto-viscoplastic damage behaviour. The algorithm for numerical integration of the model is described in detail in Section 3 and the closed form of the consistent tangent operator is presented. An assessment of the accuracy and stability of the elastic predictor-viscoplastic corrector algorithm is carried out relying on the analysis of iso-error maps in Section 4. The chapter ends with the concluding remarks presented in Section 5.

Computational Model For Viscoplasticity Coupled with Damage

147

2 Elasto-Viscoplastic Damage Constitutive Model In this section, the constitutive relations, represented by a set of equations in time, which govern the elasto-viscoplastic damage model with crack closure eﬀects are presented. The undamaged phenomenological behaviour of the material is modelled by a von Mises type power-law elasto-viscoplastic model described in Section 2.1. The important concept of eﬀective stress [14] is recalled in Section 2.2. In Section 2.3 the principle of strain equivalence is used to derive eﬀective constitutive equations for the damaged material. The damage evolution law, which includes the important eﬀect of crack closure, is presented in Section 2.4. 2.1 Viscoplastic Model It is well known that the phenomenological behaviour of real materials is generally time-dependent in the sense that the stress response always depends on the rate of loading and/or the time scale considered. The eﬀects of time dependent mechanisms are particularly visible at higher temperatures. Several diﬀerent visco-plasticity models have been proposed in the past and, in practice, a particular choice should be dictated by its ability to model the dependency of the plastic strain rate on the state of stress for the material under consideration. This section provides a brief review of the equations governing the undamaged material. The elasto-viscoplastic model described is based on a von Mises yield criterion and a power-law isotropic hardening [1]. The model is deﬁned by an elastic constitutive equation, i.e., a linear elastic relation between the stress tensor, σ, and the elastic strain, εe : σ = De : εe

(1)

where the symbol : denotes double contraction and De is the standard isotropic elasticity fourth order tensor given by (2) De = 2G I − 13 I ⊗ I + K I ⊗ I where I, is the fourth order identity tensor. The material constants G and K are, respectively, the shear and bulk moduli. The conventional additive ˙ into an elastic contribution, ε˙ e , and decomposition of the total strain rate, ε, vp an inelastic contribution, ε˙ : ε˙ = ε˙ e + ε˙ vp

(3)

is assumed. Furthermore, an associative plastic ﬂow rule is adopted: ε˙ vp = γ˙

∂Φ(σ, σy ) , ∂σ

(4)

148

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

where γ˙ is the plastic multiplier whose expression is deﬁned later. In the above, Φ is the von Mises yield function (5) Φ(σ, σy ) ≡ q (s (σ)) − σy = 3 J2 (s) − σy , where s ≡ σ − 13 (trσ) I, with I the identity tensor, is the stress deviator, and σy = σy (¯ ε vp )

(6)

is the stress-like variable associated with isotropic hardening. In the present case (isotropic strain hardening), σy is an experimentally determined function of the equivalent plastic strain, ε¯ vp , whose evolution is deﬁned by the rate equation: vp ε¯˙ = 23 ε˙ vp . (7) The yield function Φ deﬁnes an elastic domain such that the material behaviour is purely elastic (no viscoplastic ﬂow) whenever q < σy . Among the various possibilities for the deﬁnition of γ, ˙ here, the following form of a power-type law is adopted [1]: 1/ 1 q −1 , (8) γ˙ = µ σy where µ and are the viscosity and rate-sensitivity, respectively. These material parameters are, generally, temperature-dependent and can only assume positive values. The symbol · represents the ramp function deﬁned as x = (x + |x|)/2.

(9)

The evolution problem described by the set of constitutive equations (1)– (8), has a ﬁrm experimental basis and is widely accepted as a description of rate-dependent deformations of solids. Remark 1. The elasto-viscoplastic model contains, as special limiting cases, two important models[1]: (i) When µ → 0 (no viscosity) and/or → 0 (no rate-sensitivity), the standard rate-independent von Mises elasto-plastic model is recovered. (ii) When µ → ∞ a form of viscoelastic model is recovered. 2.2 Concept of Eﬀective Stress An important step in the formulation of damage models is the introduction of damage eﬀects without loosing the properties of well established models of

Computational Model For Viscoplasticity Coupled with Damage

149

elasto-plasticity and elasto-viscoplaticity. Therefore, several diﬀerent concepts and postulates have been introduced in the literature in order to account for the material progressive internal deterioration. The most frequently used concept, which is crucial to the deﬁnition of the theory, is the concept of eﬀective stress [15, 16]. Due to the diversity of forms in which internal damage manifests itself at the microscopic level, variables of diﬀerent mathematical nature (scalars, vectors, tensors) possessing diﬀerent physical meaning (reduction of load bearing area, loss of stiﬀness, distribution of voids) have been employed in the description of damage under various circumstances. Here, only one single scalar variable, D, will be used, representing the simplest possible isotropic formulation. According with the concept of eﬀective stress an eﬀective stress tensor is introduced as 1 ˜ ≡ σ. (10) σ 1−D The damage variable assumes values between 0 (for the undamaged material) and 1 (for the completely damaged material). In practice, a critical value Dc < 1 usually deﬁnes the onset of a macro-crack (i.e., complete loss of load carrying capacity at a point). Continuum damage mechanics relies on the postulate of strain equivalence, which states that ”the strain behaviour of a damaged material is represented by constitutive equations of the virgin material (without damage) in the potential of which the stress is simply replaced by the eﬀective stress” [14, 17]. This principle can be used to derive eﬀective constitutive equations for the damaged material based on the equations which govern the undamaged material response, simply by replacing the stress tensor σ in these equations by ˜ according to (10). the eﬀective stress tensor σ 2.3 Elasto-Viscoplasticity Coupled with Damage A coupled elasto-viscoplastic model can be obtained by including the eﬀect of damage in the power-law viscoplastic model described in Section 2.1. This can be accomplished by simply substituting Equation (10) in the deﬁnition of the von Mises yield function: 3 J2 (s) q − σy = − σy (¯ ε vp ) . (11) Φ (σ, σy , D) ≡ 1−D 1−D It should be noted that (11) accounts for two competing eﬀects: damaging, which shrinks (isotropically) the elastic domain (deﬁned as the subset of stress space for which Φ ≤ 0) as D grows; and hardening, which can expand the elastic domain (also isotropically) with the growth of σy . The von Mises yield function can be rewritten as ε vp ) . (12) Φ (σ, σy , D) ≡ q − (1 − D) σy = 3 J2 (s) − (1 − D)σy (¯

150

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

If this particular form is used, the associative plastic ﬂow rule (4) remains unchanged, i.e., is not directly aﬀected by the introduction of damage. This equation is more convenient and will be used later for the computational implementation. In addition to Equation (12), damage eﬀects will also be included in the deﬁnition of the viscoplastic multiplier:

1/ q 1 −1 , (13) γ˙ = µ (1 − D)σy or equivalently, ⎧ 1/ 1 q ⎪ ⎨ −1 (1 − D)σy γ˙ = µ ⎪ ⎩ 0

if

Φ (σ, σy , D) > 0

if

Φ (σ, σy , D) ≤ 0 .

(14)

Note that the eﬀect of internal damage on the elastic behaviour of the material is ignored in the present model. That is, the elasticity tensor is not a function of the damage variable or in other words, elasticity and damage are assumed to be decoupled. This simpliﬁcation can be justiﬁed if the elastic strain remains truly inﬁnitesimal in the type of problems addressed with this model. Remark 2. The damage variable ranges between 0 and 1, with D = 0 corresponding to the sound (undamaged) material and D = 1 to the fully damaged state with complete loss of load carrying capacity. Note that damage growth induces softening, i.e., shrinkage of the yield surface deﬁned by Φ = 0. For D = 0 the yield surface reduces to that of the (pressure insensitive) von Mises type power-law elasto-viscoplastic model. In the presence of damage, i.e., for D = 0 the yield surface shrinks and its size reduces to zero for D = 1. 2.4 Damage Evolution Law The damage evolution law should reﬂect the nucleation and growth of voids and microcracks which accompany viscoplastic ﬂow. Damage and viscoplasticity are undoubtedly coupled, as the presence of internal deterioration introduces local stress concentrations which may in turn drive viscoplastic deformation. The evolution of the damage internal variable is assumed to be governed by the relation: ⎧ vp 0 if ε¯ vp ≤ ε¯D ⎪ ⎨ s (15) D˙ = γ˙ −Y vp ⎪ ⎩ if ε¯ vp > ε¯D , 1−D r

Computational Model For Viscoplasticity Coupled with Damage

151

vp are material constants. In the nucleation phase, experimenwhere r, s and ε¯D tal evidence reveals that there is no noticeable eﬀect of damage on the mechanvp is the so-called damage threshold, ical properties, therefore the constant ε¯D i.e., the value of accumulated plastic strain below which no damage evolution is observed. The quantity

Y =

−1 2 [(1 + ν)σ+ : σ+ − ν trσ ] 2E(1 − D)2 −

h 2 [(1 + ν)σ− : σ− − ν −trσ ] , 2E(1 − hD)2

(16)

is the damage energy release rate, with E and ν denoting, respectively, the Young’s modulus and the Poisson’s ratio of the undamaged material. The tensors σ+ and σ+ are, respectively, the tensile and compressive components of σ, deﬁned as: 3 σi ei ⊗ ei (17) σ+ = i=1

and σ− =

3

−σi ei ⊗ ei ,

(18)

i=1

with {σi } and {ei } denoting, respectively, the eigenvalues and an orthonormal basis of eigenvectors of σ. The crack closure parameter, h, is an experimentally determined coeﬃcient which satisﬁes: 0 ≤ h ≤ 1.

(19)

This coeﬃcient characterizes the closure of microcracks and micro-cavities and depends upon the density and the shape of the defects. It is a material dependent parameter and, for simplicity, h is considered as constant. A value h ≈ 0.2 is typically observed in many experiments [18]. This deﬁnition of the energy release rate (16) was introduced by Ladev`eze (1983)[13] and Ladev`eze & Lemaitre (1984) [2]. Note that, for a state of purely tensile principal stresses, the damage energy release rate (16), can be simpliﬁed and rewritten as −1 (1 + ν) σ : σ − ν (tr σ)2 2 2E(1 − D) 2 2 −q 2 p (1 + ν) + 3(1 − 2ν) . = 2E(1 − D)2 3 q

Y =

(20)

For states with purely compressive principal stresses, (16) will give absolute values of Y smaller than those produced by (20), resulting in a decrease of damage growth rates. Also note that the limit h = 1 corresponds to no crack closure eﬀect whereas the other extreme, h = 0, corresponds to a total crack closure, with no damage evolution under compression. Any other value of h describes a partial crack closure eﬀect.

152

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

Remark 3. The particular form of the energy release rate (20), was initially proposed by Lemaitre (1983) [19] in order to describe the inﬂuence of stress triaxiality ratio, p/q, on the rate of damage growth. The inclusion of the hydrostatic component of σ in the deﬁnition of Y implies that D˙ increases (decreases) with increasing (decreasing) triaxiality ratio. One important feature of damage growth is the clear distinction between rates of damage growth observed for states of stress with identical triaxiality but stresses of opposite sign (tension and compression). Such a distinction stems from the fact that, under a compressive state, voids and micro-cracks that would grow under tension will partially close, reducing (possibly dramatically) the damage growth rate. This phenomenon can be crucially important in the simulation of forming operations, particularly under extreme strains. It is often the case that, in such operations, the solid (or parts of it) undergoes extreme compressive straining followed by extension or vice-versa [3].

3 Integration Algorithm In this section the derivation of an integration algorithm for the elasto-viscoplastic damage constitutive model, described in the previous section is carried out in detail. Operator split algorithms are particularly suitable for numerical integration of constitutive equations and are widely used in the context of elasto-plasticity and also elasto-viscoplasticity [20, 21, 22, 1, 7]. Let us consider a typical time step over the time interval [tn , tn+1 ], where the time and strain increments are deﬁned in the usual way as ∆t = tn+1 + tn ,

∆ε ≡ εn+1 − εn .

(21)

In addition, all variables of the problem, given by the set {σn , εen , εnvp , ε¯nvp , Dn }, are assumed to be known at tn . The operator split algorithm should obtain vp ¯n+1 , Dn+1 } of variables at tn+1 consisthe updated set {σn+1 , εen+1 , εvp n+1 , ε tently with the evolution equations of the model. The algorithm comprises the standard elastic predictor and the visco-plastic return mapping which, for the present model, has the following format. Elastic Predictor The ﬁrst step in the algorithm is the evaluation of the elastic trial state where the increment is assumed purely elastic with no evolution of internal variables (internal variables frozen at tn ). The elastic trial strain and trial accumulated viscoplastic strain are given by: εe trial = εen + ∆ε;

ε¯ vp trial = ε¯nvp .

(22)

Computational Model For Viscoplasticity Coupled with Damage

153

The corresponding elastic trial stress tensor is computed: σtrial = De : εe trial ,

(23)

e

where D is the standard isotropic elasticity tensor. Equivalently, in terms of stress deviator and hydrostatic pressure, we have:

where

strial = 2G ee trial ,

ptrial = K v e trial ,

(24)

ee trial = een + ∆e,

v e trial = vne + ∆v .

(25)

The material constants G and K are, respectively, the shear and bulk moduli, s and p stand for the deviatoric and hydrostatic stresses. The strain deviator and the volumetric strain are denoted, respectively, by e and v. The trial yield stress is simply ε vp ). (26) σytrial = σy (¯ The next step of the algorithm is to check whether σtrial lies inside or outside of the trial yield surface. With variables ε¯ vp and D frozen at time tn we compute: ε vp ) Φtrial := q trial − (1 − Dn )σy (¯ (27) ε vp ) . = 32 strial − (1 − Dn )σy (¯ If Φtrial ≤ 0, the process is indeed elastic within the interval and the elastic trial state coincides with the updated state at tn+1 . In other words, there is no viscoplastic ﬂow or damage evolution within the interval and εen+1 = εe trial ;

σn+1 = σtrial ;

σy n+1 = σytrial ;

Dn+1 = D trial .

vp ε¯n+1 = ε¯ vp trial ;

(28)

Otherwise, we apply the viscoplastic corrector algorithm described in the following. Visco-plastic corrector (or return mapping algorithm) At this stage, we solve the evolution equations of the model with the elastic trial state as the initial condition. With the adoption of a backward Euler discretisation, the viscoplastic corrector is given by the following set of algebraic equations: ∂Φ σn+1 = σtrial − ∆γ D : ∂σ n+1 vp ε¯n+1 = ε¯nvp + ∆γ

⎧ ⎨0 Dn+1 =

⎩D + n

∆γ 1−Dn+1

−Yn+1 r

s

vp vp if ε¯n+1 ≤ ε¯D vp vp if ε¯n+1 > ε¯D ,

(29)

154

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

where the incremental multiplier , ∆γ, is given by:

1/ q(σn+1 ) ∆t −1 , ∆γ = vp µ (1 − Dn+1 ) σy (¯ εn+1 )

(30)

with ∆t denoting the time increment within the considered interval. After solving (29), we can update: ∂Φ ∂Φ vp e e trial = ε + ∆γ ε = ε − ∆γ . (31) εvp n n+1 n+1 ∂σ n+1 ∂σ n+1 The visco-plastic corrector can be more eﬃciently implemented by reducing (29) to a single non-linear equation for the incremental multiplier ∆γ. 3.1 Single-Equation Corrector As we shall see in what follows, analogously to what happens to the classical von Mises model, the above system can be reduced by means of simple algebraic substitutions to a single non-linear equation having the incremental plastic multiplier, ∆γ, as a variable. Firstly, we observe that the plastic ﬂow vector: ∂Φ 3 s = 2 (32) ∂σ s is deviatoric. The stress update equation (29)1 can then be split as: n+1 sn+1 = strial − ∆γ 2G 32 s sn+1 pn+1 = ptrial ,

(33)

where p denotes the hydrostatic pressure and G is the shear modulus. Further, simple inspection of (33)1 shows that sn+1 is a scalar multiple of strial so that, trivially, we have the identity: strial sn+1 = trial , sn+1 s which allows us to re-write (33)1 as: ∆γ 2G ∆γ 3G trial 3 = 1 − trial strial sn+1 = 1 − 2 trial s s q where q trial is the elastic trial von Mises equivalent stress: q trial = q(strial ) = 32 strial . Equation (35) results in the following update formula for q:

(34)

(35)

(36)

Computational Model For Viscoplasticity Coupled with Damage qn+1 = q trial − 3G ∆γ .

155 (37)

With the substitution of the above formula together with (29)2 into (30) we obtain the following scalar algebraic equation for the incremental multiplier, ∆γ:

1/ q trial − 3G ∆γ ∆t − 1 = 0, (38) ∆γ − vp µ (1 − Dn+1 ) σy (¯ εn+1 ) or, equivalently, after a straightforward rearrangement, 3 trial − 3G ∆γ ∆t 2 s Dn+1 = D(∆γ) ≡ 1 − , σy0 + R(¯ εnvp + ∆γ) µ ∆γ + ∆t

(39)

which expresses Dn+1 as an explicit function of ∆γ. Finally, by introducing the damage explicit function (39) into the discretised damage evolution equation (29)3 , the viscoplastic corrector is reduced to the solution of a single algebraic equation for the incremental multiplier, ∆γ: ⎧ vp p if ε¯n+1 ≤ ε¯D ⎨ D(∆γ) = 0 s (40) F (∆γ) ≡ −Y (∆γ) vp vp ∆γ ⎩ D(∆γ) − D − = 0 if ε¯n+1 > ε¯D . n 1−D(∆γ) r In (40)2 , the dependency of Y on ∆γ originates from its dependency on the updated values of D and σ: Y (∆γ) =

−1 2 [(1 + ν)σ+ (∆γ) : σ+ (∆γ) − ν trσ(∆γ) ] 2E[1 − D(∆γ)]2

h 2 [(1 + ν)σ− (∆γ) : σ− (∆γ) − ν −trσ(∆γ) ] , 2E[1 − hD(∆γ)]2 (41) The updated stress tensor, σn+1 , whose tensile and compressive components take part in the calculation of Yn+1 , is obtained as: −

σn+1 = sn+1 + pn+1 I ,

(42)

where I is the second order identity tensor and sn+1 is obtained from the standard implicit return mapping as a function of ∆γ according to update formula (35): ∆γ 3G strial ; pn+1 = ptrial . (43) sn+1 = 1 − trial q The single-equation viscoplastic corrector comprises the solution of the above equation for ∆γ, followed by the straightforward update of the relevant variables. The solution of the equation for ∆γ is, as usual, undertaken by the Newton-Raphson iterative scheme. The overall algorithm for the numerical integration of the elasto-viscoplastic damage model, which includes the eﬀect of crack closure, is summarised in Box 1 in pseudo-code format.

156

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto (i) Elastic predictor. Given ∆ε, ∆t and the state variables at tn , compute the elastic trial state: εe trial = εen + ∆ε; etrial = dev[εe trial ]; v trial = tr[εe trial ] ε¯ vp trial = ε¯nvp ;

Dtrial = Dn

strial = 2G etrial ; ptrial = K v trial q trial = 32 strial , (ii) Check for viscoplastic ﬂow. First compute: εnvp )] , Φtrial = q trial − (1 − Dn ) [σy0 + R(¯ IF Φtrial ≤ εtol THEN (elastic step) Update (·)n+1 = (·)trial and EXIT ELSE GOTO (iii) (iii)Visco-plastic corrector . Solve the return mapping equation ⎧ vp vp if ε¯n+1 ≤ ε¯D ⎨ D(∆γ) = 0 s F (∆γ) ≡ −Y (∆γ) vp vp ∆γ ⎩ D(∆γ)−Dn − = 0 if ε¯n+1 > ε¯D 1−D(∆γ)

r

with D(∆γ) deﬁned by (39) and Y (∆γ) deﬁned through (16), (39) (42) and (43). (iv) Update the variables: 3G strial ; pn+1 = ptrial ; sn+1 = 1 − ∆γ q trial σn+1 = sn+1 + pn+1 I ; e εn+1 =

1 2G

sn+1 +

1 3K

vp ε¯n+1 = ε¯nvp + ∆γ ;

pn+1 I ; Dn+1 = D(∆γ).

(v) EXIT Box 1: Elastic predictor/visco-plastic return mapping integration algorithm for the elasto-viscoplastic damage model with crack closure eﬀect (over time interval [tn , tn+1 ])

Remark 4. (computational implementation aspects) In the computer implementation of the model (as shown in Box 1), it is important to specify the damage function D(∆γ), as expressed in equation (39). The reason for this lies in the fact that, for low rate-sensitivity, i.e., small values of , the NewtonRaphson scheme for solution of (38) becomes unstable as its convergence bowl is sharply reduced with decreasing . The reduction of the convergence bowl stems from the fact that large exponents 1/ can easily produce numbers

Computational Model For Viscoplasticity Coupled with Damage

157

which are computationally intractable. This fact has been recognised by Peri´c (1993) [1] in the context of a more general visco-plastic algorithm. In equation (39), on the other hand, the term to the power on the left hand side can only assume values within the interval [0, 1] and causes no numerical problems within practical ranges of material constants. 3.2 Consistent Tangent Operator To obtain the consistent tangent operator for the case of a strain-driven problem, all variables of the problem are considered as functions of the strain ε. The exact linearization of the algorithm described in Box 1 is performed by a systematic application of the concept of directional derivative. In the elastic case, the elastic consistent tangent at tn+1 , is simply the standard elasticity operator ˆ = De = 2G I − 1 I ⊗ I + K I ⊗ I (44) D 3 where I, is the fourth order identity tensor. In the elasto-viscoplastic damage case, i.e., when it is assumed that viscoplastic ﬂow occurs within the step, the tangent operator is called the elastoˆ vp . For the present viscoplastic damage consistent tangent and is denoted by D model it is possible to obtain a closed form expression for the tangent operator. The details of derivation, which is rather lengthy, will be omitted here and we shall limit ourselves to show only its ﬁnal expression which is given by: ¯n+1 + a3 s ¯n+1 ⊗ s ¯n+1 ⊗ I + K I ⊗ I , (45) Dvp = a1 I − 13 I ⊗ I + a2 s ¯n+1 is the normalised stress deviator: where s ¯n+1 = s

sn+1 , sn+1

(46)

and the scalars a1 , a2 , a3 , are given by: 3G a1 = 2G 1 − ∆γ trial q ∂F ∂F a2 = 6G2 q∆γ trial + ∂ (q trial ) / ∂ (∆γ)

a3 = 2G

2 3

K

∂F / ∂F ∂ (ptrial ) ∂ (∆γ)

(47)

.

In the deﬁnition of constants a2 and a3 , the scalars ∂F /∂ (∆γ), ∂F /∂ (q trial ) and ∂F /∂ (ptrial ), correspond to the derivatives of the return mapping residual

158

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

function deﬁned by (40): ∂F ∂ (∆γ)

=

∂D ∂ (∆γ)

s + 1−D1n+1 − Yn+1 r ∂Y − ∂ ∂D ∆γ − 1 / (1−D ) − s / Y n+1 n+1 (∆γ) ∂ (∆γ) s 2 − Yn+1 − ∆γ ∂ (q∂D trial ) /(1−Dn+1 ) r s−1 s ∆γ ∂Y − Yn+1 − r (1−D r ∂ (q trial ) n+1 )

∂F ∂ (q trial )

=

∂D ∂ (q trial )

∂F ∂ (ptrial )

=

s ∆γ r (1−Dn+1 )

− Yn+1 r

s

(48)

∂Y . ∂ (ptrial )

where the scalars ∂Y /∂ (∆γ), ∂Y /∂ (q trial ) and ∂Y /∂ (ptrial ), represent the derivatives of the energy release rate function, deﬁned by (16): √3 ∂D ∂D h2 ∂ (∆γ) 2G ∂ (∆γ) ∂Y 2 ¯ = − b + ∂ (∆γ) E (1−Dn+1 )3 + E (1−Dn+1 )2 C+ : sn+1 − E (1−h Dn+1 )3 b− √

+ ∂Y ∂ (q trial )

¯n+1 C− : s

∂D ∂ (q trial )

= − E (1−Dn+1 )3 b+ − +

∂Y ∂ (ptrial )

3 2G 2 h E (1−h Dn+1 )2

√2

3 h E (1−h Dn+1 )2

√2 3

E (1−Dn+1 )2

¯n+1 − C+ : s

h2

∂D ∂ (q trial )

E (1−h Dn+1 )3

b−

¯n+1 C− : s

1 = − E (1−D 2 C+ : I − n+1 )

h E (1−h Dn+1 )2

C− : I

(49) furthermore, the scalars b+ and b− and the second order tensors C+ and C− introduced in (49), are given by 2

b+ = (1 + ν) σ+ : σ+ − ν tr σ

b− = (1 + ν) σ− : σ− − ν −tr σ

2

C+ = (1 + ν) ∂∂σσ+ : σ+ − ν tr σ I

(50)

C− = (1 + ν) ∂∂σσ− : σ− − ν −tr σ I Here, one should note that the tensors C+ and C− deﬁned in (50)3 and (50)4 , respectively, contain the terms: ∂σ+ , ∂σ

and

∂σ− . ∂σ

Computational Model For Viscoplasticity Coupled with Damage

159

To compute such derivatives, we ﬁrst note that (17) and (18) deﬁne σ+ and σ− as isotropic tensor-valued functions of σ. Such functions are particular cases of the families of functions discussed by Chadwick & Ogden (1971)[23] and Carlson & Hoger(1986) [24] and their derivatives are promptly available in closed form. Finally, the scalars ∂D/∂ (∆γ) and ∂D/∂ (q trial ), which are the outcome of the derivation of the damage function (39) are deﬁned by trial H(q trial −3G∆γ) µ q −3G∆γ ∂D ∆t 3G = + + vp vp vp 2 ∂ (∆γ) µ ∆γ+∆t µ ∆γ+∆t σy (¯ ε ) σy (¯ ε ) σy (¯ ε ) n+1

∂D ∂ (q trial )

= − σy (¯ε1vp

n+1

)

∆t µ ∆γ+∆t

n+1

n+1

(51) In the above, H denotes the derivative of the hardening function evaluated at tn+1 : dσy H= . (52) d¯ ε vp ε¯ vp n+1

Remark 5. It is important to note that, the resulting elasto-viscoplastic tangent operator Dep is generally unsymmetric so that, within the context of ﬁnite element computations, an unsymmetric solver is required in the global Newton-Raphson scheme.

4 Accuracy Analysis of the Integration Algorithm To illustrate the accuracy of the integration algorithm in practical situations, this section presents some iso-error maps, produced with material constants covering a range of high rate-sensitivity to rate-independency. Iso-error maps have long been accepted as an eﬀective and reliable (if not the only) tool for assessing the accuracy of constitutive integration algorithms under realistic ﬁnite time/strain steps [25, 26, 20]. The maps have been generated in the standard fashion. Using the threedimensional implementation of the model, we start from a stress point at time tn , σn , lying on the yield surface (refer to Fig. 1) and apply a sequence of strain increments (within the interval [tn , tn+1 ]), corresponding to linear combinations of trial stress increments of the form ∆σtrial =

∆σN ∆σT T+ N, q q

(53)

where N and T are, respectively, the unit normal and tangent vectors to the yield surface and q is the von Mises equivalent stress. For each increment of trial stress, we obtain a numerical solution, σnum n+1 , with the above described algorithm in one step. In addition, a solution assumed to be ‘exact’, σexact n+1 , is obtained with the same algorithm by dividing the corresponding strain (and time) increment into 1000 sub-increments of equal size. For each point in

160

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto ∆σT tria

N

∆σ

T

σn

l

σtrial ∆σN

Fig. 1. Isoerror map. Trial stress increment directions Table 1. Material data for aluminium alloy Description

Symbol

Elastic Modulus Poisson’s ratio Initial yield stress Hardening curve

E 69004 [M N/m2 ] ν 0.3 80.559 [M P a] σ y0 ε vp ) 589 · (10−4 + ε¯ vp )0.216 σy (¯

Damage data (exponent) Damage data (denominator)

s r

Value

1.0 2.8 [M P a]

which a numerical and ‘exact’ solution is obtained, the error is computed as: ERROR =

num σexact n+1 − σn+1 × 100 . σexact n+1

The resulting iso-error map is the contour plot of the error ﬁeld. The material properties adopted in the present analysis, are listed in Table 1. These parameters were taken from Reference [27] for an aluminium alloy, except for the value of the damage denominator, r. The value of this material constant has been calibrated by performing several numerical tests with a single axisymmetric ﬁnite element, such that critical value of damage (D = 1) is attained, for the same applied displacement. To preserve the constant rate of total strain ∆ε/∆t for the iso-error map under consideration, the time increment ∆t is appropriately scaled. Figure 2 shows iso-error maps obtained at low and high strain rates with the non-dimensional rate ˙ µ ε set respectively to 1 and 1000. For each non-dimensional rate, three values of rate-sensitivity parameter, , have been used: 100 , 10−1 and 0. For = 0 virtually identical maps are obtained for the two rates [see Figs. 2 (a)3 and 2 (b)3 ] and the algorithm recovers the rate-independent solution.

Computational Model For Viscoplasticity Coupled with Damage

163

5 Concluding Remarks A computational model for elasto-viscoplastic solids, capable of handling regions of high rate-sensitivity to rate independent conditions in the presence of ductile damage, has been presented in this contribution. The material constitutive model is derived by coupling a power-law elasto-viscoplastic constitutive model, with a ductile damage evolution law. The evolution of the damage internal variable includes the important eﬀect of micro-crack closure. The model can describe diﬀerent concurrent physical phenomena and implicitly contains, as limit cases, simpler constitutive descriptions. The resulting integration algorithm generalizes the standard return mapping procedures of the inﬁnitesimal theory, and quite remarkably requires the solution of only one scalar non-linear equation.

References 1. Peri´c D (1993) On a class of constitutive equations in viscoplasticity: Formulation and computational issues. Int J Num Meth Engng 36:1365– 1393 2. Ladev`eze P, Lemaitre J (1984) Damage eﬀective stress in quasi unilateral conditions. In: 16th Int. Congress Theor Appl Mech, Lyngby, Denmark 3. Andrade Pires FM , de Souza Neto EA, Owen DRJ (2004) On the ﬁnite element prediction of damage growth and fracture initiation in ﬁnitely deforming ductile materials. Comp Meth Appl Mech 193:5223–5256 4. Owen DRJ, Hinton E (1980) Finite Elements in Plasticity: Theory and Practice. Pineridge Press, Swansea 5. Bathe K-J (1996) Finite Element Procedures. Prentice-Hall, Englewood Cliﬀs, New Jersey 6. Crisﬁeld MA (1991) Non-linear Finite Element Analysis of Solids and Structures. Vol.1: Essentials. John Wiley & Sons, Chichester 7. Crisﬁeld MA (1997) Non-linear Finite Element Analysis of Solids and Structures. Vol.2: Advanced Topics. John Wiley & Sons, Chichester 8. Simo, JC, Hughes, TJR (1998) Computational Inelasticity. SpringerVerlag, New York 9. Belytschko T, Liu WK, Moran B (2000) Nonlinear Finite Elements for Continua and Structures. Wiley, New York 10. Zienkiewicz OC, Taylor, RL, Zhu, JZ (2005) The Finite Element Method – Its Basis & Fundamentals. Butterworth-Heinemann, 6th edition 11. Zienkiewicz OC, Taylor, RL (2005) The Finite Element Method for Solid and Structural Mechanics. Butterworth-Heinemann, 6th edition 12. Perzyna P (1971) Thermodynamic Theory of Viscoplasticity. Academic Press, New York

164

D.R.J. Owen, F.M. Andrade Pires and E.A. de Souza Neto

13. Lad`eveze P (1983) On an anisotropic damage theory. In: J.P. Boehler, editor, Proc CNRS Int Coll 351 – Failure Criteria of Structured Media 355–363. Villars-de-Lans 14. Lemaitre J (1985) Coupled elasto-plasticity and damage constitutive equations. Comp Meth Appl Mech Engng 51:31–49 15. Odqvist FKG, Hult J (1961) Some aspects of creep rupture. Arkiv f¨ or fysik 19(26):379-382 16. Rabotnov YN (1969) Creep rupture. In: M. Het´enyi and W.G. Vincenti (eds), Proc of the Twelfth International Congress of Applied Mechanics XII 342–349. Springer, Berlin, Germany 17. Lemaitre J, Chaboche JL (1990) Mechanics of Solid Materials. Cambridge Univ Press 18. Lemaitre J (1996) A Course on Damage Mechanics. Springer, 2nd edition 19. Lemaitre J (1983) A three-dimensional ductile damage model applied to deep-drawing forming limits. In: ICM 4 Stockholm Vol.2 1047–1053 20. Simo JC, Taylor RL (1985) Consistent tangent operators for rateindependent elastoplasticity. Comp Meth Appl Mech Engng 48:101–118 21. Ortiz M, Simo JC (1986) An analysis of a new class of integration algorithms for elastoplastic constitutive relations. Int J Num Meth Engng 23:353–366 22. Simo JC, Govindjee, S (1991) Non-linear b-stability and symmetry preserving return mapping algorithms for plasticity and viscoplasticity. Int J Num Meth Engng 31:151–176 23. Chadwick P, Ogden RW (1971) A theorem in tensor calculus and its application to isotropic elasticity. Arch Rat Mech Anal 44:54–68 24. Carlson DE, Hoger A (1986) The derivative of a tensor-valued function of a tensor. Quart Appl Math 44(3):409–423 25. Krieg RD, Krieg DB (1977) Accuracies of numerical solution methods for the elastic-perfectly plastic model. J Pressure Vessel Tech ASME 99:510– 515 26. Ortiz M, Popov EP (1985) Accuracy and stability of integration algorithms for elastoplastic constitutive relations. Int J Num Meth Engng 21:1561–1576 27. Vaz Jr. M, Owen DRJ (2001) Aspects of ductile fracture and adaptive mesh reﬁnement in damaged elasto-plastic materials. Int J Num Meth Engng 50:29–54, 2001.

On Multiscale Analysis of Heterogeneous Composite Materials: Implementation of Micro-to-Macro Transitions in the Finite Element Setting D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi Centre for Civil and Computational Engineering School of Engineering, Swansea SA2 8PP, UK [email protected] Summary. This paper describes a multiscale homogenization procedure required for computation of material response of non-linear microstructures undergoing small strains. Such procedures are important for computer modelling of heterogeneous materials when the length-scale of heterogeneities is small compared to the dimensions of the body. The described homogenization procedure is based on the standard ﬁnite element discretisation of both macro- and micro-structure. The attention is restricted to two dimensional problem and the deformation-driven microstructures. Two classical types of boundary conditions are imposed over the unit cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. These boundary conditions satisfy the fundamental averaging condition, which equates microscopic and macroscopic virtual work. Numerical simulations, performed for an elasto-plastic material with micro-cavities, illustrate the scope and beneﬁts of the described computational strategy.

1 Introduction The ever increasing requirements in high-performance applications have provided a constant stimulus for the design of new materials. Often, this has been achieved by appropriately manipulating microstructure, for instance, by adding certain material component to the matrix phase, thus tailoring the overall material properties to speciﬁc applications. The added material phase is typically at a scale that is much smaller than the overall structural size, hence making the direct modelling of the material behaviour impractical. In many situations scales remain tightly coupled and the traditional phenomenological approach does not provide suﬃciently general predictive modelling capability. Therefore a means of continuous interchange of information be-

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 165–185. © 2007 Springer. Printed in the Netherlands.

166

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

tween scales is needed if predictive modelling of material behaviour is to be attempted. Since the basic principles for the micro-macro modelling of heterogeneous materials were introduced (see Suquet [12, 13]), this technique has proved to be a very eﬀective way to deal with arbitrary physically non-linear and time dependent material behaviour at micro-level. A number of recent works has been concerned with various approaches and techniques for the micromacro simulation of heterogeneous materials. Among these we highlight the contributions by Moulinec and Suquet [10], Smit et al. [11], Miehe and coworkers [7, 8, 9], Kouznetsova et al. [5], Terada and Kikuchi [15] and Zohdi and Wriggers [16]. The present article discusses some issues related to computational strategy for homogenisation of microstructures with non-linear material behaviour undergoing small strains. Since the aim is to provide the basic ingredients of the computational strategy allowing for the concurrent simulation at diﬀerent scales of the model, a simple model is considered comprising two scales arising, for instance, in modelling of heterogeneous composite materials. The focus of this article is on computational aspects; more speciﬁcally on the computational technique for prescribing the boundary conditions at the micro-scale and calculation of the macro-scale tangent moduli characterising relations between the macroscopic stress and strain tensors. The attention is restricted to the deformation-driven microstructures, which have been proven to provide a convenient computational format [14]. Two types of boundary conditions are imposed over the unit micro-cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. These boundary conditions satisfy the fundamental Hill-Mandel averaging condition, which equates microscopic and macroscopic virtual work [4]. The resulting computational strategy is characterised by the Newton-Raphson solution of the discrete boundary value problem, and incorporates the appropriate tangent operators. Numerical examples of both micro-scale and two-scale ﬁnite element simulations are presented in order to illustrate the scope and the beneﬁts of the described computational strategy.

2 Continuum Model at Small Strains 2.1 Preliminaries A homogenized macro-continuum B ⊂ R3 with locally attached microstructures B ⊂ R3 is visualized in Fig. 1. A point x ∈ B of the homogenized macromedium B ⊂ R3 is represented as a microstructure B ⊂ R3 . The tensors σ and σµ denote the macro and micro Cauchy stress tensor at x ∈ B and y ∈ B, respectively. The representative volume element (RVE) of the microstructure V ⊂ R3 represents the part of the heterogeneous material consisting of the solid part B and the hole H, i.e. V = B ∪ H and ∂B = ∂V ∪ ∂H.

On Multiscale Analysis of Heterogeneous Materials

167

Fig. 1. Micro to macro transition

It is assumed that the traction ﬁeld on the surface of the holes in the interior of RVE vanishes, i.e. t(y , t) = 0 at y ∈ ∂H, where t ≡ σµ n on ∂B is the traction ﬁeld vector on the surface with outward normal n at y ∈ ∂B. 2.2 Basic Microvariables Microscopic small strain tensor µ is deﬁned as the symmetric part of the displacement gradient tensor, µ ≡ sym{∇(u)}

(1)

where u is the displacement ﬁeld at a material point y ∈ B. Microequilibrium state is assumed in the presence of body forces per unit of mass b, (2) div(σµ ) + ρ b = 0 in B , where symmetric stress tensor σµ is assumed to be related to the strain tensor µ by some constitutive law ˆ µ ; α ; y ) in B, σµ = σ(

(3)

where α is the set of internal variables. 2.3 Basic Macrovariables and Averaging Theorem Within the described homogenization technique no constitutive assumptions have been assumed at the macrolevel. Overall macrostress σM of microstructure V is deﬁned as an average of the microstresses over the unit cell. By applying the Gauss theorem and microquilibrium (2), σM is given by the expression 1 1 1 σM ≡ σ = σµ dV = sym[t ⊗ y ] dA + ρ sym[b ⊗ y ] dV |V| V |V| ∂V |V| V (4)

168

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

in terms of the traction t at y ∈ ∂V and body force vector ﬁeld b at y ∈ V. By applying Green’s Lemma in similar way, overall macrostrain M is deﬁned, 1 1 µ dV = sym[u ⊗ n] dA (5) M ≡ = |V| V |V| ∂V in terms of the displacement u at y ∈ ∂V. Overall tangent modulus C relates the variations of overall macrostress σ and the macrostrain in the form C ≡

dσ d

(6)

The computation of these fourth-order tensors, in their discrete FE form, is an important aspect of this work. The Hill-Mandel Principle The Hill-Mandel principle or averaging theorem [4], demands that macroscopic stress work (or power) must equal the volume average of the microscopic stress work (or power) over the RVE associated with the macroscopic point, that is 1 σ: = σ : dV (7) |V| V Using (1) and integrating by parts the right hand side of (7) and then applying microequlibrium (2), the averaging theorem can be expressed in the following form 1 1 σ: = t · u dA + ρ b · u dV (8) |V| ∂V |V| V 2.4 Deﬁnition of the Boundary Conditions for the Small Scale The boundary conditions for the displacement u and traction t at the microstructure, are chosen such that condition (7) is satisﬁed. Two classical types of boundary conditions that satisfy these conditions are prescribed on the unit cell: (a) linear displacements on the boundary, and (b) periodic displacements and antiperiodic tractions on the boundary. A crucial aspect is the formulation in deformation-driven context, where the macroscopic strain is prescribed as averaged over the microstructure. The deformation-driven format has proved more convenient than the stress driven format [14]. The displacement ﬁeld is divided in two parts: (y ) = y + u (y ), u(y ) = u∗ (y ) + u

(9)

where u∗ is the Taylor displacement, which deﬁnes a constant deformation over the unit cell as (10) u∗ ≡ y .

On Multiscale Analysis of Heterogeneous Materials

169

∂V

V

Fig. 2. Microstructure for linear b.c.

is known as the displacement ﬂuctuation, which is conThe component u sidered to be unknown. Insertion of (9) into the averaging theorem (8) yields in the following new form of the Hill-Mandel principle 1 1 dA + dV = 0 t·u ρb · u (11) |V| ∂V |V| V Linear displacements on the boundary In this state, the deﬁnition of the linear deformation boundary constraint over the microstructure RVE shown in Fig. 2 assumes the following form (y ) = 0 u

at y ∈ ∂V.

(12)

This condition deﬁnes a linear deformation on the boundary ∂V of the RVE. Insertion of the above condition (12) into the new averaging condition form (11) conﬁrms that this model satisﬁes the averaging theorem only when body force eﬀect is negligible. Periodic deformation and antiperiodic traction on the boundary Another possibility consists of applying periodic deformation and antiperiodic traction on the boundary of the RVE ∂V, which can be represented as (y − ) and t(y + ) = −t(y − ). (y + ) = u u

(13)

In order to apply these conditions the boundary of the unit cell is decomposed in two parts as indicated in Fig. 3. Thus ∂V = ∂V + ∪ ∂V − with outwards normals n+ = −n− which are associated with the points y + ∈ ∂V + and y − ∈ ∂V − . The body force eﬀect is not taken into consideration so that this condition satisﬁes the averaging theorem. This can be proved easily by inserting (13)1 and (13)2 into (11).

170

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

∂V + V

∂V −

Fig. 3. Microstructure for periodic b.c.

V B

B H

Fig. 4. Micro to macro transition

3 Discretised Model at Small Strains 3.1 Introduction The discretisation of the continuum multi-scale problem described in Section 2 is based on ﬁnite element formulation. A representative ﬁnite element dicretisations of the macro and microstructure are depicted in Fig. 4. One can notice that at every integration Gauss point of the macrostructure, a discrete RVE microstructure is considered as representation of a Gauss point at the macro-level. The present approach is based on the deformation-driven microstructures, in which the value of the overall macroscopic deformation is prescribed on the discretised RVE. The goal is then to develop a numerical procedure for computing macroscopic average stress σ and the overall tangent moduli C at each macroscopic integration point with locally attached microstructure.

On Multiscale Analysis of Heterogeneous Materials

171

3.2 Displacement Field Partition and Matrix Notation Following the previous Section 2.4, where the continuum displacement ﬁeld partition (9) was established, the displacement ﬁeld is divided in two parts: u = u∗ + u

(14)

where the Taylor displacement u∗ (previously deﬁned in the continuum form (10)) is expressed in its discrete form u∗j ≡ y j

j = 1 ··· n

(15)

for the n nodes of the discretised microstructure RVE. The displacement ﬂuc is the unknown for every node of the discretised microstructure. tuation u In what follows the standard ﬁnite element matrix notation will be used, where the tensor entities so far used, can be expressed in the matrix form as ⎧ ⎧ ⎫ ⎫

⎨ ε11 ⎬ ⎨σ 11 ⎬ u1 f1 ε22 , uj ≡ ≡ , σ ≡ σ 22 and fj ≡ . (16) u f2 j ⎩ ⎩ ⎭ ⎭ 2 j 2 ε12 σ 12 Here is the matrix representation of the macrostrain tensor, uj is the displacement ﬁeld at the node j of the discretised unit cell V, σ is the averaged stress ﬁeld while fj denotes the force vector associated with the microcell node j. The Taylor displacement u∗j of the node j is computed in the following matrix form j = 1 · · · n. (17) u∗j = DT j , where Dj is the coordinate matrix at node j of the microstructure deﬁned in [9]. 3.3 Discretised Micro-equilibrium State and Solution Procedure Following standard procedure, the discrete boundary value problem is formulated as follows: Find the nodal displacements global vector u, such that r(u) ≡ f int (u) − f ext = 0

(18)

where f int and f ext are, respectively, the internal and external global force vectors, and r is the residual (or out-of-balance force) vector. An iterative Newton-type procedure for the solution of the Non-linear microscopic equilibrium (18) is considered here. Each iteration determines the current ﬂuctuation ﬁeld assuming frozen macroscopic strain . At the end of the procedure, when microequilibrium is reached, the averaged macroscopic stress over the microstructure RVE can be updated.

172

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

3.4 General Average Stress and Overall Tangent Modulus Computation Average Stress Computation Assuming no body forces in the expression for the average stress (4), in the discrete setting, t dA → f ext j , that is the inﬁnitesimal force t dA becomes the ﬁnite force f ext at position y j on the boundary ∂V. Therefore (4) degenerates j into the discrete sum σ =

nb 1 sym[f ext ⊗ yj] j |V| j = 1

(19)

where nb is the number of nodes on the boundary ∂V. Using matrix representation this expression becomes σ =

nb 1 Dj f ext j |V| j = 1

(20)

where Dj is the coordinate matrix evaluated at node j on the boundary of the discretised microstructure RVE. The above expression can be rearranged in the following global expression σ =

1 Db f ext , b |V|

(21)

where f ext is the external nodal force vector of the boundary nodes, and Db b is the boundary coordinate matrix deﬁned by:

Db ≡ Db1 Db2 . . . Dbnb . (22) Overall Tangent Modulus Computation In the computational homogenization approach no explicit form of the constitutive behavior on the macrolevel is assumed a priori, so that the tangent modulus has to be determined numerically by relations between variations of the macroscopic stress and variations of the macroscopic strain at such integration point. This can be accomplished by numerical diﬀerentiation of the numerical macroscopic stress strain relation, for instance, by using forward diﬀerence approximations as suggested in [8]. An alternative approach is to condense the microstructural stiﬀness matrix to the macroscopic matrix tangent modulus. This task is achieved by reducing the total RVE system of equations to the relation between the forces acting on the boundary ∂V and the displacement on the boundary. This procedure has been used in [5], [6], and also in [9], in combination with the Lagrange multiplier method to impose the boundary constraints. A similar scheme have been used in this work

On Multiscale Analysis of Heterogeneous Materials

173

whereby the direct condensation is employed to obtain a relation between the forces acting on the boundary ∂V and the Taylor displacement on the boundary nodes array u∗ which depends linearly on the macroscopic strain . The total microstructural system of equations that gives the relation between the iterative nodal displacement du and iterative nodal external force vectors is (23) K du = df ext With the displacement partition (14) the system can be rearranged as u = df ext ⇒ K d u = df ext − K du∗ ⇒ K du∗ + K d

(24)

The boundary constraints are then applied to this system in the following sections to condense the system. This procedure gives the expression that against the variation relates the variation of boundary external forces df ext b of the Taylor displacement du∗ . 3.5 Linear Displacements on the Boundary Assumption In view of the discrete formulation of the boundary conditions outlined before in section 2.4, the nodes of the mesh are partitioned into those on the surface ∂V of RV and those in the interior of V. In this mesh nb boundary nodes and ni internal nodes are distinguished. More details of the discrete form of this linear constraint are given in [1]. Partitioning of Algebraic Equations Partitioning of the current nodal displacements and internal forces is given as

Li u Li f fi ui ≡ ≡ and f = . (25) u= ub fb Lb u Lb f Here Li and Lb are the connectivity matrices [2], which deﬁne the contributions of the interior and boundary nodes, respectively. These are Boolean matrices, i.e. they consist of integers 0 and 1. Displacements ui and ub are arranged as shown in (25). In line with (25) the tangent stiﬀness matrix is rearranged as df int Li K LT Li K LT kii kib i b = ≡ K= T kbi kbb Lb K LT du i Lb K Lb

(26)

into contributions associated with internal nodes and nodes on the surface of the RVE.

174

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Linear Displacement At each node j of the boundary ∂V the condition (12) induces the discrete constraint j = 0, j = 1 · · · nb . u (27) According to the matrix notation introduced in Section 3.2, we deﬁne the global coordinate matrix

(28) Dglobal,l ≡ Di Db,l , where Di and Db are the interior coordinate matrix and the boundary coordinate matrix, respectively, given as

and Db,l ≡ Db1 Db2 . . . Dbnb . (29) Di ≡ Di1 Di2 . . . Dini Matrices Di and Db are deﬁned in terms of the node coordinate matrices of the interior and boundary nodes, as discussed in Section 3.2. The Taylor displacement u∗ deﬁned in (17), is now represented in global form as u∗ = DT global,l , where is the matrix representation of the prescribed macroscopic strain (16). In this model the variation of the Taylor displacement vector du∗ is represented as (30) du∗ = DT global,l d, that is, as a function of the variation of the macroscopic average strain vector d. Tangent Modulus of Linear Displacements on the Boundary Constraint Using Partitioning of the algebraic equations (25) and (26), the system (23) = 0. can be rewritten for the case when df ext i The general procedure explained in Section 3.4, where the rearranged system (24) was obtained, is followed. By applying linear displacement constraint in discrete form (27) and by using the Taylor displacement variation du∗ given by (30), after some algebraic manipulation, a variation for the external nodal force vector at the boundary nodes is obtained as B T df ext b = K lin Dglobal,l d

(31)

in terms of the global coordinate matrix (28) and the overall averaged macrostrain. The overall tangent moduli deﬁned in (6), can be computed in its discretised matrix form, using previous averaged stress expression (21), in the following way 1 dσ df ext b = Db (32) Cl = d |V| d

On Multiscale Analysis of Heterogeneous Materials

175

Substituting (31) into (32), the overall tangent modulus representation is obtained as 1 T Db,l K B Cl = (33) lin Dglobal,l . |V| Clearly the modulus C l is given as a function of the boundary coordinate matrix Db,l deﬁned in (29), the condensed stiﬀness matrix K B lin and the global coordinate matrix DT global,l outlined in (28). Finally we remark that using (33) the tangent moduli can be computed for heterogeneous material with arbitrary microstructures. When using this tangent modulus the quadratic rate of convergence is attained at the macroscopic level. 3.6 Periodic Displacements and Antiperiodic Traction on the Boundary In order to discretise the continuum model of the periodic boundary conditions described in 2.4, the nodes of the mesh are partitioned in four groups: 1) ni interior nodes, 2) np positive boundary nodes which are located at the top and right of the microstructure boundary ∂V of the RVE, 3) np negative boundary nodes which are located at the bottom and left of the microstructure boundary ∂V of the RVE, and 4) nc = 4 node at the corners. More details on these discrete constraints are given in [1]. Partitioning of Algebraic Equations The partition of the nodal displacements and internal forces for the periodic boundary condition is as follows ⎫ ⎧ ⎫ ⎧ ⎫ ⎫ ⎧ ⎧ fi ⎪ Li u ⎪ Li f ⎪ ui ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎬ ⎨ ⎬ ⎨ ⎬ ⎬ ⎨ ⎨ fp up Lp u Lp f u= ≡ ≡ and f = (34) un ⎪ Ln f ⎪ f ⎪ ⎪ ⎪ Ln u ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ ⎭ ⎪ ⎭ ⎪ ⎭ ⎭ ⎩ ⎩ ⎩ n⎪ ⎩ uc Lc u Lc f fc Here Li , Lp , Ln and Lc are the connectivity matrices which deﬁne respectively: the interior contribution, the contribution of positive boundary nodes, the one from their corresponding negative boundary nodes, and ﬁnally the contribution from the nodes at the corners. In correspondence to (34), the tangent stiﬀness matrix is partitioned in the following way ⎡ ⎤ ⎡ ⎤ T T T Li K LT kii kip kin kic i Li K Lp Li K Ln Li K Lc T T T T⎥ ⎢ df int ⎢ kpi kpp kpn kpc ⎥ ⎥≡⎢ Lp K LiT Lp K LpT Lp K LnT Lp K LcT ⎥ . =⎢ K= ⎣kni knp knn knc ⎦ ⎣ Ln K Li Ln K Lp Ln K Ln Ln K Lc ⎦ du T T T kci kcp kcn kcc Lc K LT i Lc K Lp Lc K Ln Lc K Lc (35)

176

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Periodic Displacements and Antiperiodic Tractions At each node pair j on the boundary ∂V + ∪ ∂V − , the continuum conditions (13)1 and (13)2 induce discrete constraints at boundary nodes of the discretised RVE. The displacement ﬂuctuation at the corners is prescribed to zero in order to avoid the solid rigid body motion. Using the matrix notation introduced in Section 3.2, we redeﬁne the global coordinate matrix for the periodic b.c. assumption as

(36) Dglobal,p ≡ Di Db,p where Di is the interior coordinate matrix deﬁned in (29) and the Db,p is the boundary coordinate matrix for periodic assumption deﬁned this time as

(37) Db,p = Dp Dn Dc where Dp , Dn , Dc are the positive boundary coordinate matrix, negative boundary coordinate matrix and corner coordinate matrix, respectively. The Taylor displacement u∗ deﬁned as a constant for each node in (17), is given in a compact form as u∗ = DT global,p , where Dglobal,p is the global coordinate matrix for periodic assumption and is the matrix representation of the prescribed macroscopic strain tensor. In this model the variation of the Taylor displacement vector du∗ is considered as follows du∗ = DT global,p d ,

(38)

i.e. the displacement du∗ is a function of the variation of the macroscopic average strain vector d. Tangent Modulus of Periodic Displacements and Antiperiodic Traction on the Boundary Constraints After rearranging the displacement nodal vector u, the external nodal force vector f ext and the stiﬀness matrix K, as deﬁned in (34) and (35), respectively, the general system (23) that relates the variations du and df ext can be obtained. Again the general procedure of Section 3.4 is followed to rearrange the system in the way described in (24). The variation of the Taylor displacement du∗ is given by (38). In this system the displacement ﬂuctuation variation vector d u is considered as unknown. The application of the periodic displacement and antiperiodic external force in its discrete form, after some algebraic operations, gives the variation of the external force vector as B T df ext b = K per Dglobal,p d

(39)

where the Taylor displacement variation (38) has been inserted into the above

On Multiscale Analysis of Heterogeneous Materials

177

equation (39). Therefore the desired expression is obtained as df ext b T = KB per Dglobal,p d

(40)

in terms which gives the sensitivity of external boundary force vector df ext b of the macroscopic average strain matrix d. The overall tangent moduli deﬁned in (6), can be computed in its discretised F.E. matrix form, using previous averaged stress expression (21), in the following way 1 df ext dσ b = Db,p (41) Cp = d |V| d Inserting (40) into (41), the overall tangent modulus matrix form for periodic deformation and antiperiodic traction on the boundary of RVE is ﬁnally obtained as 1 T Db,p K B Cp = (42) per Dglobal,p . |V| Clearly the modulus Cp is a function of the boundary coordinate matrix Db,p deﬁned in (37), the condensed periodic stiﬀness matrix K B per and the global coordinate matrix Dglobal,p outlined in (36). Finally we remark that with the above expression (42), the tangent moduli can be computed for heterogeneous materials with arbitrary microstructures of the RVE. This results in the desired quadratic rate of convergence of the Newton-type solution procedure applied to solve the homogenized nonlinear macrostructure under periodic deformation and antiperiodic traction on the boundary of the RVE.

4 Numerical Examples In this section numerical examples are presented in order to illustrate the scope and beneﬁts of the described computational strategy. First set of numerical simulations focuses on microstructure simulations and discusses some important issues regarding numerical analysis at the micro-level such as the effect of boundary conditions, topology and distribution of heterogeneities, etc. Second numerical example considers a full two-scale simulation of a boundary value problem and incorporates all computational ingredients described in this paper. This example also includes a comparison with a detailed single scale analysis. 4.1 Study of the Eﬀect of Topology of Cavities on the Properties of the RVE Problem Speciﬁcations A square unit cell is considered representing an RVE at the micro-level. The cell is composed of an elasto-plastic material with heterogeneity being induced

178

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 5. Regular cavity model

by cavities. Two models are considered: (i) a regular cell with a single circular hole embedded in a soft matrix depicted in Fig. 5, (ii) randomly generated distribution of cavities surrounded by soft matrix given in Fig. 7. For both models the void volume fraction of the unit cell is taken as 15%. Two types of ﬁnite elements are employed: linear 3-noded triangle element and 8-noded quadrilateral element with 4-Gauss points. The matrix in all models is assumed to be composed of the von Mises elasto-plastic material with linear strain hardening. The material properties assigned are: Young’s modulus E = 70 GP a, Poisson’s ratio ν = 0.2, the initial yield stress σY0 = 0.243 GP a and the strain hardening modulus H = 0.2 GP a. Analysis Approach All simulations in this section have been performed by employing the computational homogenisation under the plane-stress assumption in small strain regime. The average stress is obtained by imposing the macro-strain over the unit cell and solving the problem for deﬁned boundary condition over the RVE. The generic imposed macro-strain tensor is expressed by: ε12 ] = [0.001, 0.001, 0.0034] . [¯ ε11 , ε¯22 , 2¯ To obtain the load step at each load increment, the generic strain tensor is multiplied by the relevant load factor. The analysis is performed under two diﬀerent boundary conditions: (i) linear displacement boundary condition, and (ii) periodic displacement boundary condition. Study of the Regular Cavity Model An 8-node quadrilateral element with 4-Gauss points is employed in this simulation. Figure 5 depicts a ﬁnite element mesh containing 350 elements and 1158 nodes. Figures 6 (a) and (b) show, respectively, the deformed mesh and the equivalent plastic strain distribution for the linear displacement boundary condition. This plastic zone is clearly positioned along the diagonal side of the unit

On Multiscale Analysis of Heterogeneous Materials

179

Fig. 6. Regular cavity model under linear displacement boundary condition and periodic condition. a) Deformed mesh. b)Eﬀective plastic strain contour plot

cell in direction of the imposed shear. The corresponding results for the periodic boundary condition are given in Figs. 6 (c) and (d). From Fig. 6, it can be seen that the plastic zone has a distinctively diﬀerent pattern under periodic boundary condition. The overall stress-strain response is presented in terms of the Euclidean norm of the average stress and strain, given, respectively as 2 +σ 2 +σ 2 , ¯11 ¯22 ¯12 ¯ ε = ε¯211 + ε¯222 + ε¯212 . ¯ σ = σ Figure 9 shows the resulting average stress - strain curves for this model. The obtained results show that under linear displacement boundary condition the overall response of the regular cavity model shows signiﬁcantly stiﬀer behaviour with respect to the overall response under periodic boundary condition. The RVE with Randomly Generated Voids In this study a unit cell at the micro-level with a randomly generated distribution of void placements and sizes is considered (see Fig. 7). A standard 3-node linear triangular element is employed in this simulation. Again planestress conditions are prescribed and two boundary conditions at the micro-

180

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 7. Unit cell with randomly generated voids

level are considered: (i) linear displacement boundary condition, and (ii) periodic boundary condition. The imposed macro-strain and material properties for this model are identical to the previous examples in this section. Figure 8 shows the equivalent plastic strain distribution for both linear displacement boundary condition and periodic boundary conditions. The occurrence of localised bands with signiﬁcant plastic straining can be observed on both contour plots. Signiﬁcantly, unlike in the case of the single cavity model both boundary conditions give similar distribution of the plastic strain indicating the convergence of the results at the micro-level with the increase of the statistical sample of heterogeneities. Figure 9 shows the average stress - strain curves for this model. It can be observed that the micro-cell with randomly generated void distribution results in the stress-strain behaviour that shows small diﬀerence between the two diﬀerent boundary conditions imposed at the micro-level. This clearly indicates the convergence of the average properties with the increase of the statistical sample representing the heterogeneities at the micro-level. 4.2 Two-scale Analysis of Stretching of an Elasto-plastic Perforated Plate In this section a full two-scale analysis of a perforated plate is performed. This is a classical example often used as a veriﬁcation problem in computational plasticity. The plate is composed of an elasto-plastic material and contains regularly distributed voids. The plate has width 10 mm, length 18 mm and

On Multiscale Analysis of Heterogeneous Materials

181

Fig. 8. Eﬀective plastic strain contours for the unit cell with randomly generated voids under two boundary conditions

Fig. 9. Stress-Strain norm curves for dense model under two boundary conditions

uniform thickness of 1 mm (see Fig. 10). For obvious symmetry reasons only one-quarter of the specimen is considered (see Fig. 10). The simulation is performed by imposing uniform displacement along the upper boundary. The elasto-plastic material is assumed to follow the standard von Mises model with linear isotropic hardening. Material properties are: Young modulus E = 70 GP a, Poisson’s ration ν = 0.2, yield stress σY0 = 0.243 GP a and hardening modulus H = 0.2 GP a. Both two-scale analysis and a single scale analysis of this problem are performed.

182

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

R=

Fig. 10. Plane-stress strip with a circular hole. Geometry and boundary conditions

Single-scale Analysis Single scale analysis is used for comparative purposes and is performed on a detailed ﬁnite element mesh of the problem given in Fig. 11 (a). The mesh is composed of 11216 4-node quadrilateral elements and 12147 nodes. Figure 11 (b) illustrates distribution of an equivalent plastic strain at latter stages of the simulation. Two-scale Analysis For the multi-scale ﬁnite element analysis the perforated plate is deﬁned as a homogeneous structure at the macro-level, while at the micro-level a unit cell is deﬁned with side length equal to 1 mm and a single void in the centre of the micro-cell giving the volume fraction of 50%. Linear 3-noded triangle element is employed at both macro and micro-level (see Fig. 12). The mesh at the macro-level number is composed of 25 elements and 21 nodes, while at the micro-level the FE mesh is composed of 603 elements and 352 nodes. Multi-scale analysis has been performed under three diﬀerent boundary conditions at the micro-level: (i) Taylor assumption, (ii) linear displacement boundary condition and (iii) periodic boundary condition. As can be seen from Fig. 13, which gives reaction force against the prescribed displacement, diﬀerent boundary conditions result in markedly diﬀerent force-displacement diagrams. As expected, the results obtained for the Taylor assumption show substantially stiﬀer behaviour with comparison to the other two boundary assumptions. Periodic boundary assumption generates the softest response, and signiﬁcantly the resulting overall behaviour shows very good correspondence with the results obtained by the detailed single-scale analysis.

On Multiscale Analysis of Heterogeneous Materials

a)

183

b)

Fig. 11. Single-scale analysis of an elasto-plastic perforated plate: (a) Finite element mesh, and (b) distribution of equivalent plastic strain

Fig. 12. FE meshes at macro- and micro-level for multi-scale analysis

5 Conclusions A multiscale computational strategy for homogenisation of material behaviour of heterogeneous composites has been described. The presented numerical tests have conﬁrmed the successful implementation of the computational procedure and eﬃcient solution of the discrete multiscale problem.

184

D. Peri´c, E.A. de Souza Neto, A.J. Carneiro Molina and M. Partovi

Fig. 13. Reaction along Y direction against the applied displacement

The ongoing research is concerned with the analysis of more general nonlinear material behaviour at the microscale and incorporation of the ﬁnite strain kinematics. This work will be reported in future publications.

References 1. Carneiro Molina AJ, de Souza Neto EA and Peri´c D (2005) Homogenized tangent moduli for heterogeneous materials. In: Crouch P (ed) Proceedings of the 13th ACME Conference. Sheﬃeld UP, Sheﬃeld 2. Belytschko T, Liu WK, Moran B (2000) Nonlinear Finite Element for Continua and Structures. Wiley, New York 3. de Souza Neto EA, Peri´c D, Owen DRJ (to be published) Computational Plasticity: Small and Large Strain Finite Element Analisys of Elastic and Inelastic Solids. 4. Hill R (1972) On constitutive macro-variables for heterogeneous solids at ﬁnite strain. Proc Roy Soc London 326:131-147 5. Kouznetsova VG, Brekelmans WAM, Baaijens FPT (2001) An Approach to micro-macro modelling of heterogeneous materials. Comput Mech 27:37-48 6. Kouznetsova VG (2002) Computational homogenization for multiscale analysis of multi-phase materials PhD Thesis, TU University Eindhoven, Eindhoven 7. Miehe C, Schotte J and Schr¨ oder J (1999) Computational micro-macro transitions and overall moduli in the analysis of polycrystals at large strains. Comput Material Sci 16:372-382 8. Miehe C, Schr¨ oder J and Schotte J (1999) Computational homogenization analysis in ﬁnite plasticity - Simulation of texture development in polycrystalline materials. Comp Meth Appl Mech Engng 171:387-418 9. Miehe C and Koch A (2002) Computational micro-to-macro transitions of discretized microstructures undergoing small strains. Arch Appl Mech 72:300-317 10. Moulinec H and Suquet P (1998) A numerical method for computing the overall response of nonlinear composites with complex microstructure. Comp Meth Appl Mech Engng 157:69-94

On Multiscale Analysis of Heterogeneous Materials

185

11. Smit RJM, Brekelmans WAM and Meijer HEH (1998) Prediction of the mechanichal behaviour of nonlinear heterogeneous syatems by multi-level ﬁnite element modeling. Comp Meth Appl Mech Engng 155:181-192 12. Suquet PM (1985) Local and global aspects in the mathematical theory of plasticity. In: Sawczuk A (ed) Plasticity today: modelling methods and applications. Elsevier Applied Science Publishers, Amsterdam 13. Suquet PM (1987) Elements of homogenization for inelastic solid mechanics. In: Sanchez-Palencia E and Zaoui A (eds) Homogenization Techniques for Composite Media. Springer-Verlag, Berlin 14. Swan CC (1994) Techniques for stress-controlled and strain-controlled homogenization of inelastic periodic composites. Comp Meth Appl Mech Engng 117:249-267 15. Terada K and Kikuchi N (2001) A class of general algorithms for multi-scale analyses of heterogeneous media. Comp Meth Appl Mech Engng 190:5427-5464 16. Zohdi TI and Wriggers P (2005) Introduction to Computational Micromechanics. Springer, Berlin

Assessment of Protection Systems for Gravel-Buried Pipelines Considering Impact and Recurrent Shear Loading Caused by Thermal Deformations of the Pipe B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang Institute for Mechanics of Materials and Structures Vienna University of Technology Karlsplatz 13/202, A-1040 Vienna, Austria e-mail: [email protected] Summary. Two safety topics in pipeline engineering are considered: (1) rockfall onto gravel-buried steel pipes and (2) protection of the outer anti-corrosion coating of soil-covered steel pipelines. For both cases, eﬀective protection systems are identiﬁed, based on the results of non-linear elasto-plastic Finite Element analyses.

Introduction Two safety topics in pipeline engineering will be treated: (i) rockfall onto gravel-buried steel pipes and (ii) protection of the outer anti-corrosion coating of soil-covered steel pipelines. In both cases non-linear elasto-plastic Finite Element (FE) analyses provide insight into the structural behavior, as needed for the design of eﬀective protection systems. For rockfall, a two-component protection system is recommended. It consists of an impact damping layer and of a buried load-distributing and load-carrying structure. As regards wear of the anti-corrosion coating, two well-established means of protection are considered to be most eﬀective: (i) burying pipelines by sand and (ii) covering pipelines by (ﬁbre-)reinforced concrete.

1 Protection Systems for Gravel-Buried Pipelines Subjected to Rockfall Recent increase of rockfall activities in the European Alps has raised the need for designing impact protection systems for pipelines in Alpine valleys. This section deals with the assessment of diﬀerent protection systems including

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 187–206. © 2007 Springer. Printed in the Netherlands.

188

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

surface of structure gravel H. . . height of overburden s = 11.13 mm sand 90 cm

d=1016 mm 50 cm

150 cm soil/rock Fig. 1. Geometric dimensions of the gravel-buried steel pipeline in a section perpendicular to the axis of the pipe

sandy gravel as an energy-absorbing and load-distributing structural component. In Subsection 1.1, the development of a FE model allowing for prediction of the loading of a gravel-buried steel pipe subjected to rockfall is described. In Subsection 1.2, results from a real-scale impact experiment of a boulder onto a buried steel pipe are used for an assessment of this model. To ensure the signiﬁcance of this validation procedure, the identiﬁcation of the model parameters is based on experiments which are independent of the real-scale impact test. Finally, in Subsection 1.3 and 1.4, respectively, the structural model is used to study the performance of two diﬀerent rockfall-protection systems covering a steel pipe. 1.1 Development of a Structural Model Geometric Dimensions of the Considered Problem A pipeline with an outer diameter d = 1016 mm and a wall thickness s = 11.13 mm is considered. It is buried in the middle of a trench of 3 m width, resting on a 50 cm thick layer of sand. The tube is laterally buried up to a height of 40 cm by sand. The rest of the trench is ﬁlled by sandy gravel, see Fig. 1. Impact Scenario and Mode of Analysis Single boulders impacting vertically, directly above the axis of the steel pipe, are considered as typical rockfall events. Making use of symmetries, it is sufﬁcient to discretize one fourth of the entire structure, see Fig. 2 (a). The material beside and beneath the trench is represented by a Winkler foundation modeled by bar elements representing linear springs, see Figs. 1 and 2 (a).

Protection Systems for Gravel-Buried Pipelines

189

Fig. 2. (a) FE discretization used for the validation of the structural model; (b) axisymmetric analysis performed to obtain the distribution of surface loads applied to the 3D FE model

Dead load results in stresses in the pipe, which are by two orders of magnitude smaller than the stresses caused by the investigated types of impact. Therefore, dead load is not taken into account and, hence, the overburden of the pipe is only discretized to simulate the load distribution. Since the impact stresses in the backﬁll material above the pipe occur only in the vicinity of the impact axis, the discretization of the overburden of the pipe is restricted to a longitudinal distance of 3.4 m from the impact axis, see Fig. 2 (a). Outside this domain, only the backﬁll material beside and beneath the tube is discretized. The penetration process is not modeled in detail. Instead, the height of the overburden H is reduced by the penetration depth W at which the maximum impact force occurs, see Fig. 2 (a). Both dynamic and static 2D plain strain analyses delivered approximately the same maximum stresses in the pipe [18]. Therefore, the maximum impact force is applied quasistatically onto the surface of the FE model. This mode of modeling requires estimates of (i) the maximum impact force and the penetration depth at maximum impact force, both as a function of the mass m and the impact velocity v0 of an impacting boulder, and (ii) the distribution of stresses corresponding to the maximum impact force, which are prescribed as stress boundary conditions for the FE analysis. Estimates of the Maximum Impact Force and the Penetration Depth at Maximum Impact Force The ﬁnal penetration depth X, i.e. the penetration depth after the end of the impact, is estimated based on the dimensionless formula [16] X m v2 1 + k π/4 N 4k X = I for ≤ k , with I = 3 0 , (1) d (1 + I/N ) π d d R where d denotes the characteristic size of the boulder, N is a geometry function characterizing the “sharpness” of the boulder nose, k stands for the dimen-

190

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

sionless depth of a surface crater, and R denotes the indentation resistance of the hit material. For cubic granite boulders with a volume V and a mass density equal to 2700 kg/m3 , impacting with a tip onto gravel with a mass density equal to 1800 kg/m3 , the following relationships were obtained based on a hybrid experimental-analytical approach [16] √ 3 (2) N = 2.385 , k = 1.257 , d = 1.050 V , and R = 9.22 MPa . Relations between X and the maximum impact force F , and between X and the penetration depth at maximum impact force, W , were derived on the basis of a model for the impact kinematics which was deduced from experimental acceleration measurements [16, 17] as m v02 W X 4 π2 = = . (3) d Fd d 3 π2 + 4 Computation of the Distribution of Stresses Corresponding to the Maximum Impact Force In order to perform a 3D FE analysis of rockfall onto gravel as described previously, the stress distribution corresponding to the maximum impact force must be speciﬁed. Herein, this stress distribution is computed by means of an axisymmetric linear-elastic FE model. It comprises the gravel and the tip of the granite boulder approximated as a conical indenter at a penetration depth W , see Fig. 2 (b). The maximum impact force F is applied to the conical indenter as a spatially constant surface stress σ. The material parameters for gravel and granite are taken from Table 1. The vertical stresses obtained for the axisymmetric FE model in a horizontal section through the model at the tip of the boulder, see Fig. 2 (b), serve as surface loads for the 3D FE model. Material Modeling of Steel, Gravel and Sand The material behavior of steel is modeled by small-strain von Mises elastoplasticity, see e.g. [10, 22] and Table 1 for Young’s modulus E, Poisson’s ratio ν, and the uniaxial yield strength σy . The material behavior of gravel is represented by the elasto-plastic Cap Model [3, 5, 19]. The elastic domain follows the isotropic generalized Hooke’s law [12]: σ = C : (ε − εp ) , where σ denotes the Cauchy stress tensor, and ε and εp stand for the linearized strain tensor and the plastic strain tensor, respectively. C represents the isotropic constitutive elasticity tensor which can be expressed as a function of the bulk modulus K and the shear modulus G, reading C = K 1I ⊗ 1I + 2G(II − 13 1I ⊗ 1I) , where 1I and II denote the 2nd-order unity tensor and the 4th-order unity tensor, respectively. In the principal stress space the elastic domain is bounded by three surfaces, (i) a tension cutoﬀ accounting for tensile failure, (ii) a Drucker-Prager surface deﬁning shear failure under pronounced deviatoric stress states, and (iii) an ellipsoidal cap

Protection Systems for Gravel-Buried Pipelines ||s||, ||ep||

f3 (σ, ζ) = 0 dεp

f2 (σ) = 0 √ dεpvol / 3

dεp √ RFe (ζ)/ 3

f1 (σ) = 0

√ 1/ 3 elastic α domain √ ζ/ 3

Fe (ζ)

√ dεpvol / 3

191

ϑ

√ X(ζ)/ 3

√ p dεp dεvol / 3 √

T/ 3

√ √ I1 / 3, εpvol / 3

Fig. 3. Cap model for gravel: elastic domain and direction of plastic ﬂow, respectively, in a meridional plane of the principal stress and the plastic-strain space, respectively

representing the hardening of the material associated with compaction, see Fig. 3. In mathematical terms, these functions read [8, 9] = I1 − T = 0 , f1 (σ) = s−Fe (I1 ) = 0 for T ≥ I1 ≥ ζ , f2 (σ) f3 (σ, ζ) = Fc (s, I1 , ζ) − Fe (ζ) = 0 for ζ ≥ I1 ≥ X(ζ) Fe (ξ) = α − ϑξ, 2 s + ([I1 − L(ζ)]/R)2 Fc (s, I1 , ζ) =

and

L(ζ) =

ζ 0

(4) with if if

ζ < 0, ζ ≥ 0,

where I1 and s denote the ﬁrst invariant of the stress tensor and the deviatoric stress tensor, respectively. The direction of plastic ﬂow is given by the associated ﬂow rule [7] ∂fα , (5) dλα dεp = ∂σ α∈Jact

where the consistency parameters are denoted as dλα , whereas Jact stands for the set of active yield surfaces, deﬁned as Jact = {α ∈ [1, 2, 3] | fα (σ, ζ) = 0}. Activation of the cap mode leads to compaction, whereas activation of the failure-surface mode or the tension cut-oﬀ mode results in plastic volume dilatation, see Fig. 3. The tension cut-oﬀ and the Drucker-Prager surface are ﬁxed in the stress space. The ellipsoidal cap, however, expands if it is activated, reﬂecting material compaction described by εpvol = −W (1 − exp[D X(ζ)]) ,

with

X(ζ) = ζ + R Fe (ζ) ,

(6)

where ζ denotes the hardening state variable. Algorithmic issues of this model as well as the expressions for the consistent tangent moduli can be found in [5, 8, 9, 22].

192

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Parameter Identiﬁcation The parameters K and G of the backﬁll material are identiﬁed on the basis of the theory of elastic waves from a series of small strain acoustic experiments on unloaded sandy gravel [15], see Table 1. The tested material (mass density of 1800 kg/m3 ) consisted to 60–80 % of particles with diameters < 70 mm, and to 20–40 % of edged stones with diameters from 70 mm – 200 mm. The loading surfaces of the Cap Model are deﬁned by seven material parameters (see Fig. 2 (b)): T , α, ϑ, W , D, R, and ζini , denoting the initial value of the hardening state variable ζ. Identiﬁcation of the parameters α, ϑ, W , and D was based on triaxial tests on gravel [14, 15, 18], where cylindrical specimens were subjected to hydrostatic compression up to diﬀerent conﬁning pressures p. While p was subsequently kept constant, the specimens were subjected to additional uniaxial loading in the direction of the cylinder axis, up to shear failure. The parameters α and ϑ (Table 1) were identiﬁed from the stress states at failure. W and D were identiﬁed such that measured relationships between the mean normal stress and the volumetric strain are well predicted for p ≤ 0.9 MPa, see (Table 1). The initial size and the shape of the cap were determined from constant volume tests, R = 4.4 and ζini = 0 kPa, see [8]. For numerical reasons, the material parameter referring to tensile failure of gravel, T , was set equal to a very small positive value (100 Pa). Since, in a ﬁrst approximation, material parameters of dense sand are comparable to the material parameters of the investigated type of gravel [20], no distinction between sand and gravel was made in the numerical simulation. Table 1. Material parameters of steel, gravel, sand, granite, and concrete Material parameters of steel: E = 210 GPa , ν = 0.3 , σy = 514 MPa Material parameters of sandy gravel (also valid for dense sand) K = 244 MPa , G = 72 MPa , α = 149 kPa , ϑ = 0.40 , W = 0.28 , D = 0.05 MPa−1 , R = 4.4 , ζini = 0 kPa , T = 0.1 kPa ≈ 0 Material parameters of granite: E = 50 GPa , ν = 0.17 Material parameters of concrete E = 26.2 GPa , ν = 0.3 , α = 21.74 MPa , ϑ = 0.099 , T = 0.1 kPa ≈ 0

1.2 Validation of the Developed Structural Model Real-scale Impact Experiment The assessment of the developed structural model is based on a real-scale impact experiment, which is independent from all experiments related to the development of the structural model. In an area of a quarry, used for disposal of wet clay, a 22 m long steel pipe was buried with sandy gravel as illustrated in Fig. 1. The height of the overburden H was equal to 2 m. A granite boulder

Protection Systems for Gravel-Buried Pipelines

193

of approximately cubic shape with a mass m = 18260 kg (V = 6.76 m3 , d = 1.99 m) was dropped from a height hf = 18.85 m (v0 = 19.23 m/s) onto the buried pipeline such that it impacted with a tip. The impact of the boulder caused a crater with a depth of X = 0.85 m. The cross-section of the pipe containing the impact axis was equipped with four strain gauge rosettes. The strain histories measured during the impact were converted into stress histories by means of ideal elasto-plasticity of von Mises type, see e. g. [10], assuming plane-stress conditions. The obtained maximum von Mises stresses at the locations of the strain gauge rosettes are listed in Table 2. Table 2. Von Mises stresses and second invariant of the strain tensor referring to the maximum loading of the pipe subjected to rockfall: experimental results, numerical results, and relative errors position

experimental result

FE result

relative error∗

exp FE 12h σvM = 514 MPa = σy σvM = 514 MPa = σy exp FE 3h σvM = 5386 MPa σvM = 357 MPa exp FE 6h σvM = 5204 MPa σvM = 305 MPa exp FE 12h J2,ε = −3.4761 · 10−6 J2,ε = −3.1754 · 10−6 exp exp exp exp ∗ FE FE evaluated as |σvM − σvM |/σvM and |J2,ε − J2,ε |/J2,ε ,

0.0 % 7.5 % 49.5 % 8.7 % respectively

Comparison between Model-predicted and Experimentally Determined Stress Distribution in the Steel Pipe The real-scale impact experiment was simulated by means of the developed 3D FE model. The maximum impact force and the penetration depth at maximum impact force were calculated from Eqs. (3) as F = 7.94 MN , and W = 0.72 m . The values for F and W served as input for modeling of the impact as described in Subsection 1.1. The coeﬃcient for the sub-grade reaction, ks , characterizing the elastic foundation of the trench, was set equal to 18 MN/m3 , which is the mean value of the interval [12 MN/m3 ; 24 MN/m3 ] recommended for soft clay in [6]. Finite elements with trilinear shape functions for the displacements were used. The nonlinear elasto-plastic FE simulation was performed in an incremental-iterative manner, based on consistent tangent moduli [5, 8, 9]. The computed stresses in the pipe were compared to the corresponding experimental results, see Table 2. For a graphical representation of the obtained von Mises stresses along the inner surface of the pipe, see the thick solid line in Fig. 4 (a). In general, the simulated behavior of the steel pipe reﬂects the experimentally observed behavior of the tube satisfactorily, both qualitatively and quantitatively. At the positions 12h and 3h, good agreement between the numerical predictions and the experimental results is observed. Since the steel

194

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang von Mises stress σvM [ MPa ]

500

σy

400

von Mises stress σvM [ MPa ] 12h

ks =

18 MN/m3 6h

500 s 3h

400

300

300

200

200

100 k = 100 MN/m3 s

100

0 12h

1h

2h

3h (a)

ks = 500 MN/m3 4h

5h

σy

6h s

0 12h

12h

H = 2.0 m

H = 3.0 m 1h

2h

3h (b)

4h

s 3h

6h

H = 2.5 m

5h

6h s

Fig. 4. Prognoses of the distribution of the von Mises stress along the inner surface of the pipe in the cross-section beneath the impact as a function of (a) the coeﬃcient of the sub-grade reaction and (b) the height of overburden

yielded at the top of the pipe, also strain measurements and FE-predictions are compared at the position 12h, based on the second invariant of the strain deviator, J2ε =

1 (εxx − εϑϑ )2 + (εϑϑ − εrr )2 + (εrr − εxx )2 + ε2xϑ + ε2ϑr + ε2rx . (7) 6

Also this comparison yields a discrepancy of less than 10 %, see Table 2. The largest relative error between the numerical simulation and the experiment is obtained at the position 6h. There, the numerically predicted loading of the pipe is 49.5 % greater than the experimentally obtained value. Nevertheless, in regions where the highest loading of the steel pipe occurs, the developed structural model yields satisfactory results. Consequently, this model possesses predictive capabilities, i. e., the model is successfully validated. 1.3 Prognoses of Structural Behavior Prognoses Considering a Change of the Boundary Conditions The trench in which pipelines in Alpine valleys are buried by gravel is usually surrounded by rock rather than by soft clay. This provides the motivation to study the inﬂuence of diﬀerent coeﬃcients of sub-grade reaction on the loading of the pipe. In order to model the behavior of weathered rock, ks is set equal to 100 MN/m3 , as recommended for dense sand in [6]. Secondly, ks is set equal to 500 MN/m3 in order to investigate an (almost) rigid bedding, as encountered with unweathered rock. In both cases, the height of the overburden and the intensity of the impact are the same as in the FE simulation described in Subsection 1.2. For increased values of the coeﬃcient of sub-grade reaction, the FE-predicted maximum von Mises stress of the pipe does not reach the

Protection Systems for Gravel-Buried Pipelines

195

yield stress, see Fig. 4 (a). An increase of ks from 18 MN/m3 to 100 MN/m3 and 500 MN/m3 results in a reduction of the loading of the pipe by approximately 25 % and 30 %, respectively. Prognoses Considering a Change of the Structural Dimensions In order to assess the capability of gravel layers to serve as a protection system for steel pipes endangered by rockfall, the inﬂuence of diﬀerent heights of overburden (H = 2.5 m and 3.0 m) on the loading of the pipe is studied. In these two simulations, the coeﬃcient of sub-grade reaction and the intensity of the impact are the same as in the FE simulation which allowed for validation of the model, see the Subsection 1.2. For increased heights of the overburden, the maximum von Mises stress of the pipe, predicted by the FE simulation, does not reach the yield stress, see Fig. 4 (b). An increase of H from 2.0 m to 2.5 m and 3.5 m results in a reduction of the loading by approximately 20 % and 30 %, respectively. However, this decrease is less than linear. Therefore, in order to eﬀectively increase the safety of a gravel-buried pipeline subjected to rockfall, the burying depth must be increased signiﬁcantly. Prognoses Considering a Change of the Boundary Conditions and of the Structural Dimensions In the two previous parameter studies the inﬂuence of the increasing height of the overburden and the one of the increasing coeﬃcient of sub-grade reaction on the loading of the pipe were investigated separately. In order to investigate the synergism of both modiﬁcations, H and ks are increased simultaneously in an additional numerical analysis. The height of overburden is set equal to 3 m and the coeﬃcient of sub-grade reaction equal to 500 MN/m3 , whereas the intensity of the impact remains unchanged. Results from this FE analysis show a further reduction of the loading of the pipe (compare the thick line in Fig. 6 with the results illustrated in Figs. 4 (a) and (b)). The maximum von Mises stress encountered along the inner surface of the pipe is equal to 33.5 % of the yield stress. 1.4 Assessment of an Enhanced Protection System Consisting of Gravel and, Additionally, of Buried Load-Carrying Structural Elements A protection system for a steel pipe subjected to rockfall must satisfy two requirements: (i) damping of the impact, in order to keep the forces arising from rockfall reasonably small and (ii) load distribution and load-carrying capacity, in order to reduce the loading of the steel pipe. As for the protection system investigated so far, both tasks are accomplished by the layer of gravel. However, the ﬂexibility of gravel required for the damping of the impact is opposed to the stiﬀness of the material required for distribution and carrying of the load.

196

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

B

A

surface of structure gravel Section A–A steel plate t=1.5 cm concrete wall 200 cm

surface of structure gravel Section B–B steel plate t=1.5 cm concrete wall 200 cm

sand 17 cm 100 cm soil/rock B

sand soil/rock

132 cm A

Fig. 5. Alternative protection system consisting of gravel as an energy-absorbing and impact-damping system and a buried steel plate supported by concrete walls as a load-carrying structural component

In order to further improve the eﬀectiveness of a protection system for a steel pipe subjected to rockfall, the aforementioned two tasks should be performed by two separate structural elements. Such an enhanced protection system is investigated subsequently. Buried Steel Plate Resting on Concrete Walls The investigated protection system consists of (i) gravel as an energy-absorbing and impact-damping system and (ii) a buried steel plate supported by concrete walls, representing a load-carrying structural component, as illustrated in Figs. 5 (a) and (b). Length, width, and thickness of the steel plate are equal to 264 cm, 234 cm, and 1.5 cm, respectively. It consists of the same steel as used for the pipe (Table 1). The boundary conditions at the interface between the steel plate and the concrete walls are chosen such that only compressive forces can be transmitted to the concrete walls. For the description of the material behavior of concrete, the Cap Model is employed, with the ellipsoidal failure surface being removed. The considered type of concrete is characterized by the uniaxial compressive strength fcu = −30.3 MPa (σ11 = fcu , σ22 = σ33 = σ12 = σ23 = σ31 = 0) and the biaxial compressive strength fcb = −35.15 MPa (σ11 = σ22 = fcb , σ33 = σ12 = σ23 = σ31 = 0). These two strength values are the basis for calculating the material parameters α and ϑ of the Drucker-Prager failure criterion

2 fcu −fcb 2 fcu fcb = 0.099 , α = = 21.74 MPa . (8) ϑ= 3 fcu −2 fcb 3 fcu −2 fcb

Protection Systems for Gravel-Buried Pipelines

197

von-Mises stress σvM [ MPa ]

200

without steel plate and concrete wall 160

12h

s 3h

6h

120 80

reduction of pipe loading

40

with steel plate and concrete wall 0 12h 1h 2h 3h 4h 5h 6h s

Fig. 6. Prognoses of the distribution of the von Mises stress along the inner surface of the pipe in the cross-section beneath the impact for a height of overburden H = 3 m and a coeﬃcient of sub-grade reaction ks = 500 MN/m3 with and without the additional construction consisting of a steel plate and concrete walls

Young’s modulus E, Poisson’s ratio ν and the parameter T referring to the tension cut-oﬀ are listed in Table 1. Assessment of the Enhanced Protection System The performance of the enhanced protection system is assessed considering the same rockfall scenario as previously investigated, i.e., the mass and the height of fall of the boulder are equal to 18260 kg and 18.85 m, respectively, the coeﬃcient of sub-grade reaction is set equal to 500 MN/m3 , the height of overburden equal to 3 m, and F and W again equal to 7.94 MN and 0.72 m, respectively. Results from the FE analysis show that the additional structural elements result in a further signiﬁcant reduction of the loading of the pipe, see Fig. 6. 1.5 Conclusions It was shown that a protection system for a steel pipe subjected to rockfall must satisfy two requirements: (i) damping of the impact, in order to keep the forces arising from rockfall reasonably small and (ii) load distribution and load-carrying capacity, in order to reduce the loading of the steel pipe. In case of a purely gravel-based protection system, both tasks must be performed by gravel. Thereby, the ﬂexibility of gravel required for the damping of the impact is opposed to the stiﬀness of the material required for the task of load distribution and carrying of the load. This was the motivation to investigate an enhanced protection system consisting of (i) gravel as an energy-absorbing and impact-damping system

198

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

and (ii) a buried steel plate supported by concrete walls as a load-carrying structural component. This analysis showed that buried load-carrying structural elements can signiﬁcantly increase the safety of pipelines endangered by rockfall.

2 Protection Systems Against Abrasive Shear Loading Caused by Thermal Deformation of Soil-Covered Pipelines Oil and gas pipelines are commonly bedded in and covered with sand. The transport of sand to the construction site may be expensive. Therefore, the replacement of sand by a (coarse) ﬁlling material which is directly available at the construction site (e.g. possibly sharp-edged stones with dimensions up to ≈ 10 × 10 × 10 cm) could prove proﬁtable. However, such a construction method would result in larger contact forces exerted from relatively large, sharp-edged stones onto the pipelines. This is particularly disadvantageous in combination with motions of the pipeline relative to the backﬁll material, resulting from temperature-induced displacements of the pipeline in longitudinal direction: Recurrent abrasive shear loading by tips of stones may damage the anti-corrosion ﬁlm at the outer surface of the pipeline. This section deals with the protection of the anti-corrosion ﬁlm against such shear forces, discussing the role of geosynthetics and steel-ﬁbre reinforced concrete. 2.1 Assessment of Static Forces Exerted by Single Stone Tips onto Soil-Covered Pipelines Loading Scenario The magnitude of forces acting onto soil-covered pipelines depends on the height of the cover, on the mechanical properties and the speciﬁc weight of the ﬁlling material, and on the settlements of the pipeline and the ﬁlling material. If no settlements occur, the force acting onto the pipeline is equal to the weight of the ﬁlling material directly above the pipeline. If, however, the settlements of the ﬁlling material beside the pipeline are greater than the ones of the pipeline, the forces acting onto the pipeline increase because of signiﬁcant load re-arrangement processes in the soil [21]. The extent of this re-arrangement depends on the shear resistance of the ﬁlling material. It increases with decreasing shear resistance. Structural Model The relevant force acting on a soil-covered pipeline follows from the combination of a ﬁlling material of low shear resistance, piled up to a standard maximum cover height of 1.5 m, with an adverse settlement scenario. We consider

Protection Systems for Gravel-Buried Pipelines

199

Fig. 7. Structural model of the soil body above and lateral of the pipeline

uniform settlements of the ﬁlling material on both sides of a ﬁxed pipeline. Consequently, no longitudinal displacements occur and displacements in a plane orthogonal to the pipe axis do not change along the longitudinal direction. This corresponds to a plane state of strain, and allows for the use of a plane structural model [12] (see Fig. 7). Steel pipes for oil and gas pipelines are so stiﬀ that the displacements resulting from a soil cover of 1.5 m height are negligibly small as compared to typical soil settlements of several centimeters. Hence, the pipe does not have to be considered explicitly in the structural model. Instead, the contact surface between the pipe and the ﬁlling material is spatially ﬁxed in the structural model. Since both the structure and the settlements are symmetric, investigation of half the structure is suﬃcient. Thereby, the axis of symmetry (left boundary in Fig. 7) and the boundary opposite to the axis of symmetry (right boundary in Fig. 7) are ﬁxed in the x-direction. The upper boundary, corresponding to the ground surface, is stress-free. At the lower boundary, settlements, i.e. displacements in the y-direction, are prescribed (see Fig. 7). The boundary opposite to the axis of symmetry is suﬃciently far from this axis so to exert no inﬂuence on the stress state around the pipe. Determination of this stress state requires a realistic consideration of the nonlinear material behavior of the ﬁlling material. Therefore, the Cap Model described in Subsection 1.1 is adopted. Aiming at determination of the relevant forces that are acting on a soil-covered pipeline embedded in a material with low shear resistance, the subsequent calculations are based on a cohesionless material, i.e. we use the parameters of sandy gravel listed in Table 1, setting, however, α equal to 0.5 kPa.

200

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Finite Element Simulation The structural problem, involving elasto-plastic material behavior, is solved numerically for three standard diameters of oil or gas pipelines (d = 500, 1000 and 1500 mm), by means of nonlinear FE simulations [21], which are performed in an incremental-iterative manner, based on consistent tangent moduli [5, 8, 9]. For determination of forces exerted by single stone tips onto a pipeline, the distribution of the radial stresses along the pipeline perimeter must be computed. Prior to settlements on both sides of the pipeline, radial compression stresses amount to 25 kPa – 35 kPa, depending on the pipeline diameter [see Fig. 8(a)–(c)]. After completion of the re-arrangement of the loading, caused by the settlements, release occurs in the vicinity of the vertex of the pipeline. In the lateral regions of the upper half of the pipeline the radial stresses are increasing signiﬁcantly (see Figs. 8). The increase of the maximum load is the larger, the smaller the pipeline diameter [see Fig. 8(d)]. Relevant Forces of Tips of Single Stone Acting on Soil-covered Pipelines, as a Function of the Pipe Diameter These forces can be determined through integration of the maximum radial stresses over parts of the surface associated with a characteristic distribution of stone tips. For the sake of simplicity, a quadratic grid of stone tips with distances a is assumed (see Fig. 9). Thus, forces exerted by one stone tip read as ⎧ ⎨ −106 kPa for d = 500 mm, −69 kPa for d = 1000 mm, (9) F = a2 · max σrr,∆s with max σrr,∆s = ⎩ −63.4 kPa for d = 1500 mm. Assuming a uniformly granulated ﬁlling material, the stone tip distance a can be set equal to the grain size of the ﬁlling material. Thus, following from Eq. (91 ), the force exerted by one tip of a stone for a given pipeline diameter is a quadratic function of the grain size of the ﬁlling material (see Fig. 10). 2.2 Identiﬁcation of Wear Protection Strategies Archard’s Wear Law Using Archard’s wear law [2], the maximum contact forces determined in Subsection 2.1 allow for calculation of the service life of the protection layer serving as an envelope of the pipe. In order to carry out this calculation, the wear resistance must be determined experimentally (see Fig. 11). Archard’s wear law reads as [2] Fv . (10) V˙ = KA H

Protection Systems for Gravel-Buried Pipelines

201

Fig. 8. Distribution of radial stresses resulting from the dead load of the ﬁlling material (speciﬁc weight γ of covering soil 20.0 kN/m3 and cover height 1.5 m) along the perimeter of a soil-covered pipeline before (◦, σrr,DL ) and after (, σrr,∆s ) settlement-induced load re-arrangement for (a) d = 500 mm, (b) d = 1000 mm, and (c) d = 1500 mm; and (d) settlement-induced increase of maximum radial stresses in the pipe

Fig. 9. Deﬁnition of distance a between stone tips and stress integration area A of a single stone tip: stone tips exert contact force F in a regular grid (a × a) on the pipeline surface

202

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Fig. 10. Relevant forces of single stone tips as function of the distance between stone tips, and of pipeline diameter (speciﬁc weight γ of covering soil 20.0 kN/m3 , cover height 1.5 m)

Fig. 11. Deﬁnition of the term ’shear cycle’ in context with wear tests conducted on specimens representing the protection layer of the outer anti-corrosion layer of soil-covered steel pipelines: per shear cycle, twice the shear distance, 2l, is covered

In Eq. (10), V˙ is the abrasion rate (abrased volume per time), F is the compressive force, v denotes the velocity of the abrasion-inducing body, H represents the hardness of the loaded body, and KA is a dimensionless parameter, related to the probability of (microscopic) abrasion phenomena depending on characteristics of the abrased and the abrasive body (e.g. mineralogical hardness, viscosity, stiﬀness) [11, 13].

Protection Systems for Gravel-Buried Pipelines

203

Since time-dependent eﬀects play no role in the considered wear tests, the integration of Eq. (10) is trivial, V = KA

Fs , H

(11)

where V is the abrased volume along the total shear path length s. V can be expressed as the product of the tip width w of the abrasion-inducing body, the shear distance l, and the cutting depth t. The total shear path length can be expressed as the product of the shear cycle number n and twice the shear distance covered during one shear cycle, 2l (see Fig. 11), s = n · 2l. Thus, following from Eq. (11), w · l · t = KA

F · n · 2l H

⇒

t=

2KA · F · n. wH

(12)

According to Eq. (12), the cutting depth t depends on the compressive force F , on the number of conducted shear cycles n, on KA , on the metal tip width w, and on the hardness H of the specimen. Notably, the shear distance l has no inﬂuence on the cutting depth. Protection Performance of Geosynthetics The wear resistance of common geosynthetics was determined by means of shear tests (see Fig. 11) on 6 mm thick geosynthetic specimens of the type Polyfelt AR 20 [4] (a = 21 cm, b = 14.85 cm). For this purpose, a metal tip was used, similar to the cone-shaped tip described in [1]. It was attached to the geosynthetic specimen, loaded by a compressive force of approximately 50 N, acting perpendicular to the specimen. In two independent tests the specimens were completely transected after ≈ 50 shear cycles. Evaluation of Eq. (12) for the tests (t = 6 mm; n = 50; F = 50 N) yields (2KA )/(wH) = 2.4 · 10−6 m/N. This value, together with Eq. (12), allows for estimation of the cutting depth t into a geosynthetic specimen of the aforementioned type, as a function of the compressive force F and the shear cycle number n. The order of magnitude of the shear cycle number which leads to a transection of a geosynthetic of 6 mm thickness can be assessed through insertion of t = 6 mm, (2KA )/(wH) = 2.4 · 10−6 m/N, and Eq. (9) into Eq. (12), ⎧ ⎨ 60/90/100 for a = 2 cm , 7/10/11 for a = 6 cm , nd=500/1000/1500 mm = (13) ⎩ 2/4/4 for a = 10 cm . For common pipe diameters (500 – 1500 mm) and grain sizes (distance between stone tips) of 2 – 10 cm, the 6 mm geosynthetic investigated herein resists 2 – 100 shear cycles, until being completely transected.

204

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang

Given a typical service life of n = 5000 shear cycles for oil and gas pipelines, the above results [see Eq. (13)] reveal that a 6 mm geosynthetic of the considered type protects the outer anti-corrosion ﬁlm of the pipeline for only ≈ 1/2500 to 1/50 of the service life. The stone tip force which results in transection of the 6 mm geosynthetic of the type Polyfelt AR 20 after 5000 shear cycles can be assessed through insertion of t = 6 mm, (2KA )/(wH) = 2.4 · 10−6 m/N, and n = 5000 into Eq. (12). This force amounts to olyf elt = 6 mm) = 0.5 N . F (n = 5000, tP AR 20

(14)

The maximum admissible distance a between stone tips exerting a force of F = 0.5 N, can be determined by means of Eqs. (9) as a function of the outer pipe diameter, ⎧ ⎨ 2.2 mm for d = 500 mm , a = 2.7 mm for d = 1000 mm , (15) ⎩ 2.8 mm for d = 1500 mm . Hence, when covered by sand grains, the 6 mm geosynthetic investigated herein resists 5000 shear cycles before being transected. Eﬀective Means of Protection The results of the previous paragraph suggest two strategies for providing a suﬃcient protection of the outer anti-corrosion ﬁlm of soil-covered pipelines for oil and gas transport against abrasive shear loading exerted by coarse ﬁlling material, caused by temperature-induced displacements of the pipeline in the longitudinal direction: (a) Increase of the hardness H and the thickness t, respectively, of the protective layer subjected to wear: e.g. by coating the pipeline by steel-ﬁbre reinforced concrete (SFRC) [see Fig. 12(a)]. (b) Decrease of the abrasion force by reducing the distance a between the stone tips, as the pipeline is embedded in and buried by sand. Thereby, leaching of sand can be avoided by enveloping the sand body with a ﬁltration layer which separates the sand body and the coarse ﬁlling material from each other. Preferably, geosynthetics are attached as ﬁltration layer [see Fig. 12(b)].

2.3 Conclusions The resistivity of geosynthetics of a type similar to ones tested herein against abrasion through sharp-edged stones larger than 2 mm, is too low as to provide, during the entire service life, suﬃcient protection of the outer anticorrosion ﬁlm of the pipeline. Hence, sand cannot be replaced by coarser

Protection Systems for Gravel-Buried Pipelines

205

Fig. 12. Strategies for protecting the outer anti-corrosion ﬁlm of soil-covered steel pipelines in case a mixture of sandy gravel and square-edged stones is used as ﬁlling material: (a) increase of hardness and thickness of the protective layer, e.g. made of steel-ﬁbre reinforced concrete (SFRC) or (b) decrease of the abrasion force through use of sandy material around the pipe

ﬁlling material together with an envelope of the steel pipe by geosynthetics comparable to ones investigated herein. However, when subjected to shear loading exerted by sand grains, failure (transection) of Polyfelt AR 20 -type geosynthetics can indeed be excluded prior to 5000 shear cycles, i.e. within the entire service life of such a pipe. Hence, two strategies can be recommended for protecting the outer anti-corrosion ﬁlm of soil-covered steel pipelines against abrasive shear loading: On the one hand, the wear resistance of the protection layer can be improved by increasing its hardness and thickness, e.g. through the use of steel-ﬁbre reinforced concrete. On the other hand, encasing the pipeline with sand minimizes the abrasion force, which can be withstood by the outer anti-corrosion ﬁlm of the pipeline without any additional means of protection. Leaching of sand can be avoided by an envelope of the sand body by geosynthetics.

References ¨ 1. ONORM EN 14574 (2005) Geokunststoﬀe – Bestimmung des Pyramidendurchdr¨ uckwiderstandes von Geokunststoﬀen auf harter Unterlage [Geosynthetics – Determination of the Pyramid Puncture Resistance of Geosynthetics on ¨ Hard Underlay]. Osterreichisches Normungsinstitut In German. 2. Archard JF (1953) Contact and rubbing of ﬂat surfaces. Journal of Applied Physics 24(8):981–988 3. DiMaggio FL, Sandler IS (1971) Material models for granular soils. Journal of Engineering Mechanics (ASCE) 97(3):935–950 4. Polyfelt Geosynthetics (2006) Technical data polyfelt.AR – 500 917 | 02.2002. www.polyfelt.com. 5. Hofstetter G, Simo JC, Taylor RL (1993) A modiﬁed cap model: closest point solution algorithms. Computers & Structures 46(2):203–214 6. JDAAF (1983) Soils and Geology Procedures for Foundation Design of Buildings and Other Structures (Except Hydraulic Structures): Technical Manual 5-818-

206

7. 8.

9. 10. 11. 12. 13. 14. 15. 16.

17.

18.

19.

20. 21.

22.

B. Pichler, Ch. Hellmich, St. Scheiner, J. Eberhardsteiner and H.A. Mang 1, Air Force Manual 88-3. Joint Departments of the Army and the Air Force, Washington, DC, USA Koiter WT (1960) General theorems for elastic-plastic solids, volume I, Chapter IV, pp 167–218. North-Holland Publishing Company, Amsterdam Kropik Ch (1994) Three-dimensional elasto-viscoplastic ﬁnite element analysis of deformations and stresses resulting from the excavation of shallow tunnels. PhD thesis, Vienna University of Technology, Vienna, Austria Kropik Ch, Mang HA (1996) Computational mechanics of the excavation of tunnels. Engineering Computations 13(7):49–69 Lubliner J (1990) Plasticity Theory. Macmillan Publishing Company, New York Magne´e A (1993) Modelization of damage by abrasion. Wear 162–164:848–855 Mang H, Hofstetter G (2000) Festigkeitslehre [Strength of Materials]. Springer, Wien, NewYork. In German Olofsson U, Telliskivi T (2003) Wear, plastic deformation and friction of two rail steels – a full scale test and a laboratory study. Wear 254:80–93 Penumadu D, Zhao R (1999) Triaxial compression behavior of sand and gravel using artiﬁcial neural networks (ANN). Computers & Geotechnics 24:207–230 Pichler B (2003) Parameter identiﬁcation as the basis for prognoses in geotechnical engineering. PhD thesis, Vienna University of Technology, Vienna, Austria Pichler B, Hellmich Ch, Mang HA (2005) Impact of rocks onto gravel - design and evaluation of experiments. International Journal of Impact Engineering 31:559–578. Available online at www.sciencedirect.com. Pichler B, Hellmich Ch, Mang HA, Eberhardsteiner J (2005) Assessment of protection systems for buried steel pipelines endangered by rockfall. ComputerAided Civil and Infrastructure Engineering 20:331–342 Pichler B, Hellmich Ch, Mang HA, Eberhardsteiner J (2006) Gravel-buried steel pipe subjected to rockfall: Development and veriﬁcation of a structural model. Journal of Geotechnical and Geoenvironmental Engineering (ASCE) 132(11):1465–1473 Sandler IS, Rubin D (1979) An algorithm and a modular subroutine for the cap model. International Journal for Numerical and Analytical Methods in Geomechanics 3:173–186 ´ Sawicki A, Swidzi´ nski W (1998) Elastic moduli of non-cohesive particulate materials. Powder Technology 96:24–32 Scheiner St, Pichler B, Hellmich Ch, Eberhardsteiner J (2006) Loading of soil-covered oil and gas pipelines due to adverse soil settlements – protection against thermal dilatation-induced wear, involving geosynthetics. Computers and Geotechnics 33(8):371–380 Simo JC, Taylor RL (1985) Consistent tangent operators for rate independent elasto–plasticity. Computer Methods in Applied Mechanics and Engineering 48:101–118

Enriched Free Mesh Method: An Accuracy Improvement for Node-based FEM Genki Yagawa1 and Hitoshi Matsubara2 1

2

Center for Computational Mechanics Research, Toyo University, 2-36-5, Hakusan, Bunkyo-ku, Tokyo, Japan, 112-8611 [email protected] Center for Computational Science and Engineering, Japan Atomic Energy Agency, 6-9-3 Higashi-Ueno, Taito-ku, Tokyo, Japan, 110-0015 [email protected]

Summary. In the present paper, we discuss the accuracy improvement for the free mesh method: a node based ﬁnite element technique. We propose here a scheme where the strain ﬁeld is deﬁned over clustered local elements in addition to the standard ﬁnite element displacement ﬁeld. In order to determine the unknown parameter, the least square method or the Hellinger-Reissner Principle is employed. Through some bench mark examples, the proposed technique has shown excellent performances.

1 Introduction Recent advances in computer technology have enabled a number of complicated natural phenomena to be accurately simulated, which were ever only observed by experiments. Among various computer simulation techniques, the ﬁnite element method (hereinafter referred to as ”FEM”) has been most widely used due to the capability of analyzing an arbitrary domain, and results, accurate enough for engineering purposes, are obtainable at reasonable cost[1][2]. However, mesh generation for ﬁnite element analysis becomes very diﬃcult and time consuming if the degree of freedom of the analysis model is extremely large, for example exceeding 100-million, and the geometries of the model are complex. In order to overcome the above shortcoming of the standard FEM, the so called mesh-free methods[3][4] have been studied. The Element-Free Galerkin Method (EFGM)[5][6] is among them with the use of integration by background-cells instead of by elements, based on the moving least square and diﬀuses element methods. The Reproducing Kernel Particle Method (RKPM)[7][8] is another mesh-free scheme, which is based on a particle method and wavelets. The general feature of these mesh-free methods is that, contrary to the standard FEM, the connectivity information between Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 207–219. © 2007 Springer. Printed in the Netherlands.

208

Genki Yagawa and Hitoshi Matsubara

nodes and elements is not required explicitly, since the evaluation of the total stiﬀness matrix is performed generally by the node-wise calculations instead of the element-wise calculations. On the other hand, a virtually mesh-free approach called the free mesh method (hereinafter referred to as ”FMM”)[9][10] is based on the usual FEM, having a cluster of local meshes and equations constructed in a node-by-node manner. In other word, the FMM is a node-based FEM, which still keeps the well-known excellent features of the standard FEM. Through the nodewise manner of the FMM, a seamless ﬂow in simulation procedures from local mesh generation to visualization of the results without user’s consciousness is realized. The method has been applied to solid/ﬂuid dynamics [11], crack problems[12], concrete problems[13], and so on. In addition, in order to achieve a high accuracy, the FMM with vertex rotations has been studied[14][15]. In this paper, we discuss another high accurate FMM: the Enriched FMM (hereinafter referred to as ”EFMM”). In the following section, the fundamental concept of the original FMM is reviewed, and the third section deals with two EFMMs, one is ”EFMM based on the localized least square method” and the other ”EFMM based on the Hellinger-Reissner principle”. In the fourth section, some numerical examples are presented, and concluding remarks are given in the ﬁnal section.

2 Basic Concept of Free Mesh Method (FMM) The FMM starts with only the nodes distributed in the analysis domain (Ω), without the global mesh data, as following equation. pi (xi , yi , ri ) ∀i ∈ {1, 2, · · · , m}

(1)

where m is the number of node, pi (xi , yi ) are the Cartesian coordinates, and ri is the nodal density information, which is used to generate appropriate nodes as illustrated in Fig. 1(a). From above nodal information, a node is selected as a central node and nodes within a certain distance from the central node are selected as candidate nodes. This distance is usually decided from the prescribed density of the distribution of nodes. Then, satellite nodes are selected from the candidate nodes, which generate the local elements around the central node (shown in Fig. 1(b)). For each local element, the element stiﬀness matrix is constructed in the same way as the FEM, however in FMM, only the row vector of stiﬀness matrix for each local element is necessary. The local stiﬀness matrix of each temporary element is given by kei = [ kpi kSj kSk ]

(2)

where kei is the row vector of the stiﬀness matrix for element ei and kpi , kSi and kSk are components for node of pi , Si and Sk (j and k are number

Enriched Free Mesh Method S3 e3

S4

e2

e4

Other nodes S2

Central node

e1

pi e6 e

S5

5

Local elements S1

S6

(a) Domain of analysis

pi S1

pi S1 S2

pi

…

S2

209

Satellite nodes

(b) Clustered local elements

pi S6 S1 Assembling

S6

pi S1 S2 S3 S4 S5 S6

S1

Stiffness matrix for e1

Stiffness matrix for e2

Stiffness matrix for Pi

(c) Stiﬀness matrix for central node Fig. 1. Concept of Free Mesh Method

of current satellite nodes). Through the above procedures are carried out for all local elements, the stiﬀness matrix for a central node is given by kpi =

ne

k ei

(3)

i=1

where kpi is the stiﬀness matrix for central node pi , and ne the number of local elements. Through the above procedures for all nodes is carried out, the global stiﬀness matrix is given by assembling kpi which are computed by node-wise manner: ⎡ ⎤ kp1 ⎢ kp2 ⎥ ⎢ ⎥ K=⎢ . ⎥ (4) ⎣ .. ⎦ kpm Brief of the nodal stiﬀness matrix is shown in Fig. 1(c). After the construction of the global stiﬀness matrix, a derivation of the solution is processed. The great advantage of the FMM is that the global stiﬀness matrix can be evaluated in parallel with respect to each node through the node-wise manner, and only satellite node information is required with each nodal calculation. Finally, a derivation of the solution is performed as the usual FEM. Thus, the FMM is a node-wise FEM, which still keeps the well-known excellent features of the usual FEM. The features of FMM are summarized as follows, (1) Easy to generate a large-scale mesh automatically (2) Processed without being conscious of mesh generation (3) The result being equivalent to that of the FEM

210

Genki Yagawa and Hitoshi Matsubara

Mixed

Element-wise displacement fields

Node-wise strain field

Fig. 2. Concept of enriched free mesh method

3 Enriched Free Mesh Method (EFMM) 3.1 Outline of EFMM ”Assumed strain on the clustered local elements” is the concept of EFMM as shown in Fig. 2. In the EFMM, the strain ﬁeld on the clustered local elements and the displacement ﬁeld of each local element are assumed independently. Relating these independent ﬁelds, we propose here two approaches, one is the localized least square method and the other is the method based on the Hellinger-Reissner principle. 3.2 EFMM Based on the Localized Least Square Method The EFMM based on the localized least square method (hereinafter referred to as ”EFMM-LS”) assumes the strain ﬁeld on the clustered local elements as {ε(x)} = [Nε ]{a}

(5)

where {ε(x)} = {εxx , εyy , γxy } is the strain ﬁeld deﬁned on the clustered local elements and each component of {εxx , εyy , γxy } is assumed independently, and [Nε ] is a matrix, which consists of arbitrary polynomials as follows, ⎤ ⎡ t p (x) 0 0 (6) [Nε ] = ⎣ 0 pt (x) 0 ⎦ 0 0 pt (x) where pt (x) is given on the clustered local elements as linear basis pt (x) = 1 x y quadratic basis pt (x) = 1 x y x2 xy y 2 pt (x) = 1 x y x2 xy y 2 x3 x2 y xy 2 y 3 cubic basis ···

(7)

Enriched Free Mesh Method

211

In this paper, pt (x) is assumed to be linear or quadratic basis polynomial. The coeﬃcients vector {a} in Eq. (5) is determined by minimizing the discrete L2 norm as follows, p ne 2 [{ε(x)} − {εci }] (8) J= c=1 i=1

where ne is the number of local elements with c(= 1, 2, · · · , ne ) being current local element, p the number of points, which are called as the ”strain monitoring points” on the clustered local elements with i(= 1, 2, · · · , p) being the current strain monitoring point and {εci }the strain vector of i-th strain monitoring point on the c-th local element, which is called as the ”mother element”. The stationary condition of Eq. (8) is δJ = 2{a}T

p ne εT ε [Ni ] [Ni ]{a} − [Nεi ]T {εci } = 0

(9)

c=1 i=1

which yields the coeﬃcients vector {a} as follows, {a} =

p ne

T [Nεi ]

−1

[Nεi ]

T [Nεi ]

{εci }

(10)

c=1 i=1

Let us consider a simple Constant Strain Triangle as the mother element in which the displacement ﬁeld of each local element is deﬁned by {u} =

3

{ui }ζi

(11)

i=1

where {u} is the displacement ﬁeld of the local element, {ui } is the nodal displacement, and ζi is the area-coordinate[16]. Thus, the strain value on the strain monitoring points is given by {εci } = [Bci ]{ui } where

[Bci ] = [B1 ] [B2 ] [B3 ] with ⎡ ⎤ ∂ζj /∂x 0 ∂ζj /∂y ⎦ [Bj ] = ⎣ 0 ∂ζj /∂y ∂ζj /∂x

(12)

(13) , j = 1, 2, 3

By substituting Eq. (12) into Eq. (10), the unknown coeﬃcient {a} is determined as

p ne −1 T T [Nεi ] [Nεi ] [Nεi ] [Bci ] {ui } (14) {a} = c=1 i=1

212

Genki Yagawa and Hitoshi Matsubara

Substituting Eq. (14) into Eq. (15), we obtain {ε(x)} = [Nε ]

p ne ε T ε −1 ε T c [[Ni ] [Ni ]] [Ni ] [Bi ]{ui } = [A]{ui }

(15)

e=1 i=1

where [A] = [Nε ]

p ne

[[Nεi ]T [Nεi ]]−1 [Nεi ]T [Bci ]

(16)

e=1 i=1

In the elasticity problem, the stress vector {σ} and the strain vector {ε} have the relation as follows, {σ} = [D]{ε}

(17)

where [D] is a symmetric matrix of material stiﬀness. With [D] given by Eq. (16), the stiﬀness matrix based on the localized least square method is computed on the clustered local elements as [A]T [D][A]dΩ (18) [kLS ] = Ω

where Ω is area of the clustered local elements. It is important to say that the above stiﬀness matrix is computed in a node-wise manner. It is noted that the present EFMM-LS is closely related to the superconvergent patch recovery proposed by Zienkiewicz and Zhu[17][18]. In an adaptive ﬁnite element method[19][20], the Z-Z error estimator has been most widely used to estimate the error. The error estimator requires an exact solution, but generally it is impossible to compute the exact value because the exact solution is not available in general. The Z-Z technique then obtains the recovered solution in a post processing stage. The clustered local elements in the present method are equivalent to the superconvergent patch used in the Z-Z technique. The diﬀerence lies in that the recovering procedure in the EFMM-LS is in a main process stage when computing element stiﬀness matrices. The use of the assumed strain is therefore, in some sense, equivalent to the ”post-process” of the Z-Z superconvergent patch recovery. 3.3 EFMM Based on Hellinger-Reissner Principle In the EFMM based on the Hellinger-Reissner principle [1][21] (hereinafter referred to as ”EFMM-HR”), the Hellinger-Reissner (hereinafter referred to as ”HR”) principle is employed to obtain better accuracy. Let the HR principle of a linear elastic body be deﬁned on the clustered local elements by 1 {ε}T [D]{∂u}dΩ − {ε}T [D]{ε}dΩ (ε, u) = 2 Ω Ω T − {u} {b}dΩ − {u}T {˜ t}dS (19) Ω

Sσ

Enriched Free Mesh Method

where

ε} {∂u} = [B]{¯ u} , {ε} = [Nε ]{¯

213

(20)

with {b} being the applied body force per unit mass, and {t˜} the applied traction on boundary Sσ . {¯ u} is the unknown nodal displacement and {¯ ε} the unknown nodal strain. The unknown values (¯ u, ε¯) of the HR principle satisfy the following equations in a weak manner, δ{ε}T [D] ([B]{¯ u} − [N]{¯ ε}) dΩ = 0 (21) Ω

Ω

δ{u} [B] [D][N]{¯ u}dΩ − T

T

δ{u} {b}dΩ − T

Ω

Sσ

δ{u}T {˜ t}dS = 0 (22)

It is noted here that the strain ﬁeld is deﬁned on the clustered local elements by node-wise manner, where the displacement ﬁeld is deﬁned on each element by element-wise manner. Equations (21) and (22) yields the following linear matrix equation,

ε¯ f1 −A C = (23) u ¯ f2 CT 0 where

⎧ A = Ω [Nε ]T [D][Nε ]dΩ ⎪ ⎪ ⎨ C = Ω [Nε ]T [D][B]dΩ f1 = 0 ⎪ ⎪ ⎩ f2 = Ω [Nu ]T {b}dΩ + Γ [Nu ]T {t˜}dΓ

(24)

By condensing the coeﬃcient matrix of Eq. (23), we obtain the following equation, u = f2 (25) CT A−1 C¯ where the condensation should be executed on the clustered local elements. Thus, the stiﬀness matrix based on the HR principle is computed on the clustered local elements as follows, [kHR ] = CT A−1 C

(26)

It is noted here that we can obtain the enriched stiﬀness matrix without increasing the number of nodal degrees of freedom.

4 Examples 4.1 Convergence Study: Displacement To study the convergence characters of the present methods, a cantilever model is solved as shown Fig. 3, where the three diﬀerent mesh patterns are prepared and the mesh division in the x direction is varied. As shown in the ﬁgure, a beam of length L = 10, height D = 1 and thickness t = 1

214

Genki Yagawa and Hitoshi Matsubara y

D=1

P

E = 1000, v = 0.25

x

L = 10

(a) Cantilever beam model

(b) One layer mesh

(c) Two layers mesh

(d) Three layers mesh Fig. 3. Mesh patterns for cantilever beam model

is subjected to a shear load in plane stress condition. The material parameters are given as the Young’s modulus E = 1000.0 and the Poisson’s ratio ν = 0.25. The displacements at the loaded edge normalized by the exact value are plotted against the degrees of freedom (see Fig. 4). From the comparison of displacement results among the six diﬀerent solutions, it can be observed that (a) The accuracy of the FEM with the three noded linear element of constant strain is the worst, whereas that with the six noded quadratic element is the best irrespective of the mesh patterns. (b) As the number of layers in the thickness direction increase, the accuracy of EFMMs approaches that of the quadratic FEM. (c) Regarding the comparisons among the EFMMs, the accuracy of the EFMM-HR and the EFMM-LS with the linear strain ﬁeld are the best, whereas, for the ﬁner meshes (see Fig. 4(c)), the results of EFMMs with the quadratic strain ﬁeld are almost equivalent to those of the formers. 4.2 Convergence Study: Error Norms As another convergence measures, two kinds of error norms for the beam problems as shown Fig. 5 [22] are employed, which are, respectively, given as

E2 =

Ω

exact T

u−u

exact

u−u

1/2 dΩ

(27)

Enriched Free Mesh Method

215

0.8 1

0.75 0.7 Displacement

Displacement

0.8 0.6 0.4

0.65 0.6 0.55 0.5

0.2

0.45 0

0.4 0

25

50

75

100 125 150 175 200

0

25

50

75

DOFs

100 125 150 175 200 DOFs

(a) One layer mesh 1

0.8

Displacement

Displacement

1

0.6 0.4

0.95

0.9

0.85

0.2 0

0.8

0

50

100

150

200

250

300

0

50

DOFs

100

150

200

250

300

DOFs

(b) Two layer mesh 1

0.8

Displacement

Displacement

1

0.6 0.4

0.95

0.9

0.85

0.2 0

0.8

0

50

100 150 200 250 300 350 400

0

DOFs

50

100 150 200 250 300 350 400 DOFs

(c) Three layer mesh FEM (linear) EFMM-LS (linear) EFMM-HR (linear)

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

Fig. 4. Normalized displacements at the loaded edge vs. DOFs (The ﬁgures in the right hand side are zoomed ones)

216

Genki Yagawa and Hitoshi Matsubara

10

2

y

E = 1000.0, v = 0.25

P

x P/2 Constrained in both the x and y directions Constrained in the x direction only Fig. 5. Cantilever beam model for error norm study; only the case of mesh is shown as examples

Ee =

Ω

T 1 ε − εexact σ − σ exact dΩ 2

1/2 (28)

where E2 is the displacement error norm and Ee that of the energy error. u, ε and σ are, respectively, the numerical results of displacement, strain and stress, whereas uexact , εexact and σ exact are the exact solutions. A beam of length L = 10, height D = 2 and thickness t = 1 is subjected to a shear load in plane stress condition. The material parameters are given by the Young’s modulus E = 1000.0 and the Poisson’s ratio ν = 0.25. The above displacement and energy convergence norms are plotted against the DOFs in Figs. 6 and 7, respectively, where the meshes are, respectively, 1 × 1, 2 × 2, 4 × 4, 16 × 16, 32 × 32, and 64 × 64. It can be seen from these ﬁgures that (a) Again, the error norms of the displacement of the EFMMs are between those of the linear and the quadratic FEMs (see Fig. 6). However, the convergence slopes of the EFMMs are almost equal to that of the quadratic FEM. (b) The error norms of the energy of the quadratic EFMMs are almost the same as that of the quadratic FEM and those of the linear EFMMs are between the linear and the quadratic FEMs. 4.3 Patch Test The patch test is performed using the three models of patch as shown in Fig. 8, where the displacement ﬁeld u(x) 0.2x = (29) v(y) −0.6y is applied at the boundary. Table 1 shows the test results for the FEMs and the EFMMs. As illustrated in the table, all the method passes the patch test for the Model A, which is a regular mesh division model. However, for the Model B and C, which are irregular ones, the EFMM-LSs do not pass the

Enriched Free Mesh Method FEM (linear) EFMM-LS (linear) EFMM-HR (linear) 0.5

217

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

0 0

1

2

3

4

Log ||E||2

-0.5 -1 -1.5 -2 -2.5 Log(DOFs)

Fig. 6. L2 error norms of displacement vs. DOFs FEM (linear) EFMM-LS (linear) 0.5 EFMM-HR (linear)

FEM (quadratic) EFMM-LS (quadratic) EFMM-HR (quadratic)

0 0

1

2

3

4

Log ||E||e

-0.5 -1

-1.5 -2 -2.5 Log(DOFs)

Fig. 7. Energy error norms vs. DOFs

M1

(a) Model A

M1

(b) Model B

M1

M2

(c) Model C

Fig. 8. Models for patch tests

test. Here, ”Pass” means that the displacement of the internal node (M 1 or M 2) satisﬁes Eq. (29). This means that the EFMM-LSs are nonconforming for irregular mesh, which is an open question.

218

Genki Yagawa and Hitoshi Matsubara Table 1. Displacements at internal nodes M 1 and M 2

Model A u(M 1) v(M 1) FEM(linear) 0.900 -2.400 0.900 -2.400 FEM(quadratic) 0.900 -2.400 EFMM-LS(linear) EFMM-LS(quadratic) 0.900 -2.400 0.900 -2.400 EFMM-HR(linear) EFMM-HR(quadratic) 0.900 -2.400 Exact 0.900 -2.400

Model B u(M 1) v(M 1) 1.200 -3.000 1.200 -3.000 1.198 -3.170 1.198 -3.141 1.200 -3.000 1.200 -3.000 1.200 -3.000

u(M 1) 0.600 0.600 0.611 0.611 0.600 0.600 0.600

Model C v(M 1) u(M 2) -2.400 1.300 -2.400 1.300 -2.372 1.285 -2.368 1.290 -2.400 1.300 -2.400 1.300 -2.400 1.300

v(M 2) -1.800 -1.800 -1.899 -1.859 -1.800 -1.800 -1.800

5 Concluding remarks A new Free Mesh Method called ”Enriched Free Mesh Method” is proposed in this paper, in which a high accuracy can be obtained without explicitly increasing the degree of freedoms. The work is summarized as follows, (1) The key idea of the proposed method is that the strain ﬁeld is assumed on clustered local elements, in addition to the usual displacement ﬁeld on each element. To relate the above two ﬁelds, the localized least square method or the Hellinger-Reissner principle are, respectively, employed. (2) The convergence characteristics of the displacement L2 error norms in the cantilever problem are between that of the FEM with the linear displacement ﬁeld and that with the quadratic one, whereas that of the energy error norms with the quadratic strain ﬁeld for the clustered elements is equivalent to that of the FEM with the quadratic displacement ﬁeld. (3) The EFMM based on the Hellinger-Reissner principle passes the patch test, whereas, for irregular nodal arrangements, the EFMM based on the localized least square method does not. This would be an open question and there is a room for future research.

References 1. Zienkiewicz OC, Taylor RL (2000) The ﬁnite element method. Fifth edition, Butterworth Heinemann 2. Cook RD, Malkus DS, Plesha ME (1989) Concepts and applications of ﬁnite element analysis. Third edition, Wiley 3. Barth TJ, Griebel M, Keyes DE, Nieminen RM, Roose D, Schlick T (2003) Meshfree methods for partial diﬀerential equation. Springer-Verlag Berlin Heidelberg 4. Liu GR, Liu MB (2003) Smoothed Particle Hydrodynamics a meshfree particle method. World Scientiﬁc publishing 5. Belytschko T, Lu YY, Gu L (1994) Element-free Galerkin methods. Int J Num Meth Engng 37:229–256 6. Lu YY, Belytschko T, Gu L (1994) A new implementation of the element-free Galerkin Method. Comput Meth Appl Mech Engng 113:397–414

Enriched Free Mesh Method

219

7. Liu WK, Jun S, Adee J, Belytischko T (1995) Reproducing kernel particle methods for structural dynamics. Int J Num Meth Engng 38:1655–1680 8. Liu WK, Li S, Belytschko T (1997) Moving least square kernel particle method Part 1: methodology and convergence. Comput Meth Appl Mech Engng 143:113–154 9. Yagawa G, Yamada T (1996) Free mesh method: a new meshless ﬁnite element method. Computational Mechanics 18:383–386 10. Yagawa G, Furukawa T (2000) Recent developments approaches for accurate free mesh method. Int J Num Meth Engng 47:1445–1462 11. Fujisawa T, Inaba M, Yagawa G (2003) Parallel computing of high-speed compressible ﬂows using a node-based ﬁnite-element method. Int J Num Meth Engng 58:481–511 12. J. Imasato, Y. Sakai (2002) Application of 2-dimentional crack propagation problem using FMM. Advances in Meshfree and X-FEM Methods, Liu GR, editor, World-Scientiﬁc 13. Matsubara H, Iraha S, Tomiyama J, Yagawa G (2002) Application of 3D free mesh method to fracture analysis of concrete. Advances in Meshfree and XFEM Methods, Liu GR, editor, World-Scientiﬁc 14. Matsubara H, Iraha S, Tomiyama J, Yamashiro T, Yagawa G (2004) Free mesh method using a tetrahedral element including vertex rotations. JSCE J of Structural Mechanics and Earthquake Engineering 766(I-68):97–107 15. Tian R, Matsubara H, Yagawa G, Iraha S, Tomiyama J (2004) Accuracy improvement on free mesh method: a high performance quadratic tetrahedral/triangular element with only corners. Proc of the 2004 Sixth World Congress on Computational Mechanics (WCCM VI) 16. O.C. Zienkiewicz, K. Morgan (1983), Finite element and approximation, John Wiley & Sons 17. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. PART 1: The recovery technique. Int J Num Meth Engng 33:1331–1364 18. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery and a posteriori error estimates. PART 2: Error estimates and adaptivity. Int J Num Meth Engng 33:1365–1382 19. Zienkiewicz OC, Zhu JZ (1992) The superconvergent patch recovery (SPR) and adaptive ﬁnite element reﬁnement. Comput Meth Appl Mech Engng 101:207– 224 20. Babuska I, Rheinboldt WC (1978) A-posteriori error estimates for the ﬁnite element method. Int J Num Meth Engng 12:1597–1615 21. Washizu K (1968) Variational methods in elasticity and plasticity. Pergamon Press, New York 22. Timoshenko SP, Goodier JN (1987) Theory of elasticity. McGraw-Hill

Modelling of Metal Forming Processes and Multi-Physic Coupling J.-L. Chenot and F. Bay Center for Material Forming (CEMEF) Ecole des Mines de Paris - UMR CNRS 7635 BP 207, F-06904 Sophia-Antipolis Cedex, France [email protected] Summary. The main physical phenomena which can be coupled with the mechanical computation of metal forming processes are analyzed. Recalling the classical thermal coupling, it is shown that a stronger numerical coupling is necessary when localization of the deformation occurs. Several situations where we have mechanical solid and liquid interactions with thermal coupling are brieﬂy mentioned. A more complete description of electro magnetic and thermal coupling is given in view of induction heating. Finally the case of multi scale coupling for metallurgic microstructure evolution is introduced. Key words: Computational Plasticity, Forming Process, Thermal Coupling, Induction Heating, Micro-Structure.

1 Introduction Since about thirty years ago, numerical modeling of metal forming processes was starting to be developed in laboratories [1] to [4] and later in software companies as well, using mostly the ﬁnite element method. To-day, with the help of powerful modern computers and parallel computation, it is possible to predict accurately several important technical parameters, for complex 3-D forming processes such as forging, rolling or extrusion. On the other hand, several physical phenomena still remain very approximately known, either during the forming process itself, or during the heating or cooling process, and in heat treatment operations. It is an industrial demand to predict with the same software the material evolution during the whole process. This particularly important if one wants to predict the microstructure evolution. The objective of the paper is to review some of the most important physical evolutions, which are coupled with the mechanical working process, keeping in mind that the ﬁnal microstructure is responsible for the ﬁnal properties of the work-piece. Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 221–238. © 2007 Springer. Printed in the Netherlands.

222

J.-L. Chenot and F. Bay

2 Mechanical Approach of Metal Forming Processes For a detailed account of the ﬁnite element modeling of metal forming processes, the reader is referred to [5]. 2.1 Constitutive Modeling Despite rigid plastic or rigid viscoplastic laws are still widely used in many research teams, the elastic plastic or viscoplastic laws must be preferred. The later ones are intrinsically more realistic; they allow the user to model properly unloading after forming, to predict spring back and the associated residual stresses. The elastic viscoplastic laws are also compulsory when small deformation processes are simulated such as during cooling, heat treatment, stretching, etc. In the literature, several degrees of sophistication can be found. The most widely used approximation, which reveals accurate enough in most forming processes is the additive decomposition of the strain rate tensor ε˙ into the elastic and plastic parts. It is usually written: ε˙ = ε˙ e + ε˙ p

(1)

Introduction of an objective derivative of the stress tensor; which is necessary when large rotations take place: dj σ = λe trace(˙ε e ) + 2µeε˙ e dt

(2)

The relatively general Perzyna formalism is often retained for the plastic component of the strain rate tensor: 1 −1 1 σeq − R m σ ε˙ p = (3) k K where σ is the deviatoric stress tensor, σeq the equivalent stress, R the yield stress, K the consistency and m the strain rate sensitivity index. At the interface between part and tool the friction shear stress can be modelled by : τ = αf (σn )K|∆v|q−1 ∆v

(4)

where αf is the friction coeﬃcient, σn function of the normal stress and ∆v is the tangential velocity. For an incompressible or quasi incompressible ﬂow, it is desirable to utilize a mixed formulation. In the domain Ω of the part, this formulation is written for any virtual velocity and pressure ﬁelds v ∗ , p∗ as: ∗ σ˙ : ε˙ ∗ dV − τ˙ · v ∗ dS − pdiv(v ˙ )dV = 0 (5) Ω

Ω

∂Ωc

Ω

∗ (div(v) + p/κ)p ˙ dV = 0

(6)

Modelling of Metal Forming Processes and Multi-Physic Coupling

223

2.2 Finite Element Approximation Many diﬀerent ﬁnite element formulations were proposed, and developed at the laboratory level, but it is now realized that the discretization scheme must be compatible with other numerical and computational constraints, among which we can quote: • • • • •

Remeshing and adaptive remeshing, Unilateral contact analysis, Iterative solving of non linear and linear systems; Domain decomposition and parallel computing; Easy transfer of physical internal parameters, when multi physic coupling must be taken into account.

Today a satisfactory compromise is based on a mixed velocity and pressure formulation using tetrahedral elements, and a bubble function to stabilize the solution for incompressible or quasi incompressible materials. The velocity ﬁeld is discretized with shape functions Nn , in term of nodal velocity vectors Vn : Vn Nn (ξ) (7) v= n

Using isoparametric elements the mapping between the physical space with coordinates x and the reference space, with coordinate ξ is: x= Xn Nn (ξ) (8) n

The strain rate tensor can be computed with the help of the conventional B discretized linear operator: ε˙ = Vn Bn (ξ) (9) n

The discretized mixed integral formulation for the mechanical problem is: √ RnV = ργNn dV + dK( 3ε¯˙)m−1 ε˙ : Bn dV Ω

Ω

p−1

αf K|∆v|

+ ∂Ωc

P Rm =

∆vNn dS −

ptr(Bn )dV = 0

(10)

Ω

Mm (div(v) + 3αd T˙ )dV = 0

(11)

Ω

The most widely used integration method remains the simple Euler one step scheme. It was recognized that a two levels Runge and Kutta method leads to a considerable improvement of the solution, which is particularly desirable when the work-piece undergoes a large rotation, such as in ring rolling.

224

J.-L. Chenot and F. Bay

2.3 Numerical Issues The non-linear equations resulting from the mechanical behaviour are linearized with the Newton-Raphson method. The resulting linear systems are often solved now with iterative methods, which appear faster and require much less CPU memory than the direct ones. Prediction of possible formation of folding defects during forging is based on the analysis of the contact of the part with itself, so providing a similar problem like the coupling with tools. Automatic dynamic remeshing during the simulation of the whole forming process is almost always necessary, as elements undergo very high strain which could produce degeneracy. Before this catastrophic event, decrease of element quality must be evaluated and a remeshing module must be launched periodically to recover a satisfactory element quality. The global mesh can be completely regenerated, using a Delaunay or any front tracing method, but the method of iterative improvement of the mesh, with a possible local change of element structure and connectivity, seems to be much more eﬀective. For industrial, complicated applications with short delays, the computing time can be decreased dramatically using several or several tens of processors. This requires to use an iterative solver and to deﬁne a partition of the domain, each sub domain being associated with a processor. But the parallelization is made more complex due to remeshing and the remeshing process itself must be parallelized. In order to avoid the necessity for the user to perform several computations, with diﬀerent meshes to check the accuracy, an error estimation can be developed using for example the generalization of the method proposed by Zienckiewicz and Zhu. Then, if the rate of convergence of the computation is known, the local mesh reﬁnement necessary to achieve a prescribed tolerance can be computed, and the meshing modules are improved to be able to respect the reﬁnement when generating the new mesh.

3 Thermal and Fluid-Solid Coupling 3.1 Classical Thermal and Mechanical Coupling The classical heat equation for deformable bodies is written simply: ρc

√ dT = div(kgrad(T )) + fw ( 3ε¯˙)m+1 dt

(12)

where the last term is a fraction fw of the viscoplastic heat dissipation. The constitutive law depends on temperature. For example we have the equations: K = K0 (ε0 + ε¯)n exp(β/T ),

m = m0 + m1 T

(13)

Modelling of Metal Forming Processes and Multi-Physic Coupling

225

The radiation condition on the free surface ∂Ωs is written: −k

∂T = εr σr (T 4 − T04 ) ∂n

(14)

where εr is the emissivity parameter, σr the Stephan constant and T0 the outside temperature. The conduction with the tools on ∂Ωc , is modeled by: −k

b ∂T = hcd (T − Ttool ) + αf K|∆v|q+1 ∂n b + btool

(15)

where Ttool is the tool temperature, b and btool are the eﬀuvisity parameters of the part and of the tool respectively. The thermal integral formulation can be written, for any test function w: dT ρc wdV + kgrad(T ) · grad(w)dV − q˙V wdV + εr σr (T 4 − T04 )wdS+ dt

Ω

Ω

+ ∂Ωc

Ω

∂Ωf

b q+1 αK|∆v| hcd (T − Ttool ) + wdS = 0 b + btool (16)

The previous equations are discretized with ﬁnite element, generally similar to those for the mechanical problem: Tn Nn (ξ) (17) T = n

so that the discretized form of the equations is: ˙ ρcT Nn dV + kgrad(T ) · grad(Nn )dV − q˙V wNn dV Ω

+

4

εr σr (T −

∂Ωf

T04 )Nn dS

Ω

+ hcd (T − Ttool ) − ∂Ωc

Ω

b τf ∆v Nn dS = 0 b + btool (18)

Diﬀerent time discretization schemes can be used, which allow to compute the temperature ﬁeld at time t + ∆t, knowing it at time t and t − ∆t, using an explicit scheme which avoids solving a non linear thermal equations. In most codes, coupling between mechanical and thermal equations is not performed at the increment level, as the scheme consists in computing ﬁrst the thermal ﬁeld, then the mechanical ﬁeld (without a ﬁxed point iteration algorithm).

226

J.-L. Chenot and F. Bay

3.2 Localization When the thermal and mechanical coupling is strong enough, such as in processes where localization in narrow shear bands can occur (e. g. in high speed machining), the previous method is not satisfactory and a ﬁxed point algorithm may not converge. In this case it is desirable to solve simultaneously the mechanical and thermal equations. Therefore we have a non linear problem with the following unknowns nodal unknowns at time t+∆t: temperature Tt+∆t , velocity Vt+∆t , and pressure Pt+∆t when a mixed formulation is used. A Newton-Raphson method must be utilized, where the unknowns are the same and the stiﬀness matrix must contain all the derivatives of the residual equation, including the coupling terms. 3.3 Fluid Solid Coupling During Heating or Heat Treatment Fluid solid coupling is an important issue in several industrial processes. During heating in a furnace, we must take into account the ﬂow of the surrounding gas and heat exchange between the gas and the preforms, in order to determine precisely the temperature ﬁeld inside the work-pieces which will be formed. The problem is even more complicated when one wants to predict the quenching process with water which will be vaporized at the contact of a hot work piece. The prediction of the temperature evolution in the part is again important, as it will be responsible for the geometric change of the part and the microstructure evolution. An analogous situation arises in casting of large work pieces during the cooling process, when a solid fraction interacts with a moving ﬂuid with complicated thermal and mechanical evolutions. An eﬃcient frame for this coupling is to use an ALE formulation for the liquid phase where the material velocity v is diﬀerent from the mesh velocity vg , which will be deﬁned by a smoothing operator, such as: div(grad(vg )) = 0

(19)

and boundary conditions preserving the geometry of the free surface: (vg − v) · n = 0. With the ALE scheme, the grid derivative of any parameter a will be evaluated in term if the material derivative according to: da dg a = + (vg − v) · grad(a) dt dt

(20)

4 Electro Magnetic Coupling 4.1 The Induction Heating Process Many industrial processes are based on an eﬃcient use of coupling between electromagnetic, thermal and mechanical phenomena. They generally use direct or induced currents to generate heat inside a work piece in order to get

Modelling of Metal Forming Processes and Multi-Physic Coupling

227

Fig. 1. Induction heating setup

either a prescribed temperature ﬁeld or some given mechanical or metallurgical properties through an accurate control of temperature evolution with respect to time. The basic induction setup [6] consists of one or several inductors and metallic work pieces to be heated (see Fig. 1). The inductors are supplied with alternating current with frequencies ranging from ﬁfty to several hundred thousand cycles per second. A rapidly oscillating magnetic ﬁeld is generated and in turn induces eddy currents in the work piece due to the Joule eﬀect. These currents generate ohmic heat losses inside the work piece. Moreover, for ferromagnetic materials, alternating magnetization and hysteresis eﬀect also contribute to heat generation. Most of the heat is produced in a thin layer under the surface of the work piece; the skin depth - deﬁned as the depth at which the magnitude of the ﬁeld drops to a value of e−1 of its surface value: 1 (21) δ= πf σµ where f is the frequency, σ the electrical conductivity and µ the magnetic permeability. High frequencies are used to achieve surface heating, while low frequencies generate a more uniform heating. 4.2 The Direct Electro-Thermal Formulation The electromagnetic model is classically based on the set of Maxwell equations: div(B) = 0 (22) div(D) = 0

(23)

228

J.-L. Chenot and F. Bay

rot(E) = −

∂B ∂t

(24)

∂D (25) ∂t where H is the magnetic ﬁeld, B the magnetic induction, E the electric ﬁeld, D the electric ﬂux density, and J the electric current density associated with free charges. We also have the following relations which for the intrinsic material properties: D = εE (26) rot(H) = J +

B = µ(|H|)H

(27)

J = σE

(28)

where ε is the dielectric constant, µ the magnetic permeability, and σ the electrical conductivity. They all depend on temperature and the magnetic permeability µ depends also on H. The range of frequencies dealt with in induction heating (less than 106 Hz) enables us to neglect the displacement currents in the Maxwell-Ampere equation (magneto-quasi-static approximation). A combination of the previous relations leads us to the following equation where the unknown is the electric ﬁeld. 1 ∂JS ∂E + rot rot(E) = − (29) σ ∂t µ ∂t with σ = σ(T ) and µ = µ(T, H). We deal here with axisymmetrical cases, in which the electric ﬁeld will only have a non-zero component in the θ direction: E = (0, Eθ (r, z), 0)

(30)

Temperature evolution in the work piece is governed by the classical heat transfer equation: ∂T − div(kgrad (T )) = Q˙ em (31) ρC ∂t where ρ denotes the material density, C and k respectively the speciﬁc heat and thermal conductivity, all temperature dependent. Q˙ em denotes the local heat rate, generated by the eddy currents, and integrated over one period: 1 ¯˙ Q em = T

T

σ|E|2 dt

(32)

0

The boundary conditions can be of various kinds: prescribed heat ﬂux or temperature, convection or radiation.

Modelling of Metal Forming Processes and Multi-Physic Coupling

229

4.3 Finite Element Numerical Approximation We deﬁne Ω as being a two-dimensional axisymmetrical domain which covers the part to be heated Ωpart , the inductor Ωinductor and a ﬁnite volume of air air surrounding the inductor and the part. We have chosen here to carry out coupling between the part and the inductor for the electromagnetic computations using ﬁnite elements rather than boundary elements; the air domain thus needs to be wide enough in order to model accurately electromagnetic wave propagation. The domain is discretized using second order triangular ﬁnite elements (6nodes triangles). The unknown ﬁelds - electric ﬁeld Eθ for the electromagnetic computations, temperature ﬁeld T for the thermal computations and velocity ﬁeld V for the mechanical computations - can thus be approximated over the whole domain by the classical ﬁnite element approximation: En (t)Nn (ξ) (33) E(t, r, z) = n

where E : n(t) denotes the approximated value of the θ-component of the electric ﬁeld at the node n and at time t. The discretized expression of the variational formulation is: ∂E (34) [C em ] + [K em ] {E(t)} = {B em } ∂t The temperature distribution is discretized according in the same way as in Eq.(18). Numerical models in induction heating often solve a harmonic model. This assumption is quite restrictive when one deals with non-linear magnetic materials. We have thus chosen to solve the time-dependent model. We need therefore to integrate numerically in time the electromagnetic and thermal equations. We detail here the selected time integration scheme for the electromagnetic equation. The procedure is the same for the thermal equation. We use a second-order two time step ﬁnite diﬀerence scheme: Step 1: the system is solved at time t∗ such that t < t∗ < t + δt2 with: t∗ = α1 (t − δt1 ) + α2 t + α3 (t + δt2 )

(35)

with α1 + α2 + α3 = 0. The electric ﬁeld E ∗ at time t∗ and its time derivative write: E ∗ = α1 E t−δt1 + α2 E t + α3 E t+δt2

(36)

E t+δt2 ∂E ∗ E t−δt2 − E t =γ + (γ − 1) ∂t δt2 δt1

(37)

230

J.-L. Chenot and F. Bay

The following system Eq.(38) is written at time t∗ . E ∗ and its derivative are replaced by Eqs.(36) and (37) and the system are solved for the unknown variable E ∗ : γ ∗ em ∗ em ∗ [C ] + [K ] E ∗ = {B em } + c1 [C em ]∗ E t + c0 [C em ]∗ E t−δt1 (38) α3 δt2 γ γ−1 γα2 γα1 γ−1 + + , c2 = − . δt2 δt1 α3 δt2 α3 δt2 δt1 The two time steps scheme we have requires the solving of a non-linear equation, as the matrix [C] is dependant on the magnetic ﬁeld. In order to avoid an additional non-linearity, the matrix is linearized and is approximated using its values at time t and t − δt1 : δt2 δt2 ∗ (39) [C]t−δt1 + α2 + α3 1 + [C]t−δt1 [C] = α1 − α3 δt1 δt1 where c1 =

Step 2: computation of: {E}

t+δt2

=

1

∗ t−δt1 t − α2 {E} {E} − α1 {E} α3

(40)

4.4 The Electromagnetic/Thermal Coupling Procedure Physical problems arising from heat transfer and electromagnetism have in common the fact that they are both time-dependent. Their speciﬁc timescales are however very diﬀerent. The speciﬁc time scale of an electromagnetic problem is related to the wave-associated period –typically 102 s for a 100 Hz frequency down to 108 s for a 100 MHz frequency– whereas the speciﬁc time scale for heat transfer averages normally one second. A direct model based on ﬁnite elements has been developed in our laboratory to cope with these speciﬁcities. The model includes a speciﬁc coupling procedure for solving: •

the Maxwell equations - in order to access the electromagnetic ﬁelds giving the eddy currents dissipated in the material (main source term for the heat transfer equation), • the heat transfer equation - leading to temperature evolution in the material. The coupling between the electromagnetic and thermal computations relies on a convergence test over the mean heating power and on tests over the variations of the magnetic parameters that determine respectively the passage from an electrical to thermal resolution or inversely from a thermal to an electric one. Once the electromagnetic ﬁeld has been calculated, the rate of heat generation Q˙ em for the heat equation needs to be evaluated at every integration

Modelling of Metal Forming Processes and Multi-Physic Coupling

231

points. As the electromagnetic time step is far smaller than the thermal one, we do not consider the instantaneous Joule power calculated at a given time at every integration points. We rather consider a mean Joule power averaged over one period of the electromagnetic ﬁeld: 1 Qem (nT, int) = T

nT

σ(int, t)|E(int, t)|2 dt

(41)

(n−1)T

where int is the considered integration point, T is the period of the power supply currents, n is number of periods considered and Eθ (int, t) is the value at time t of the electric ﬁeld interpolated at the integration point int. At the end of each electromagnetic period, the newly calculated mean power is compared to the one calculated at the previous period until it stabilizes. Thermal computations are started with the stabilized thermal source power calculated at (n + 1) T if the following convergence test (33) is conducted at every integration points: ¯ em (nT ) ¯ em ((n + 1)T ) − Q Q <ε ¯ Qem (nT )

(42)

where ε is the user-supplied convergence parameter. These thermal computations are valid as long as the variation of the physical magnetic parameters such as the magnetic permeability and the electric conductivity do not exceed 5%. Their variations with temperature are tested after each new thermal computation. The following criteria are tested for every mesh element: n+1 n ) − σ(Tmax ) σ(Tmax < 5% n ) σ(Tmax (43) n+1 n µ(Tmax ) − µ(Tmax ) < 5% n ) µ(Tmax n+1 where Tmax is the maximum value of the temperature ﬁeld in a given element n is the maximum value of the temperature ﬁeld at time t + dtther and Tmax in the same given element at current time t. When the maximum relative variations reach the threshold of 5%, the previously calculated mean heat power is assumed to be irrelevant, and a new electromagnetic calculation is carried out. For their part, mechanical computations are carried out at the same time steps than thermal computations.

4.5 Results The ﬁrst case deals with a static long inductor in ferromagnetic EN3 mild steel annealed at 930 ◦ C. In this case, the work piece is heated by an inductor of the same length as the work piece. The geometry consists in a cylindrical

232

J.-L. Chenot and F. Bay

Fig. 2. a) Finite element mesh; b) Electric ﬁeld; c) Temperature ﬁeld

EN3 part surrounded with Kaowool insulation, a ceramic tube and ﬁnally a three-layer coil. The mesh used for this case is displayed in Fig. 2a. The multiturn coil is modeled as a continuous single coil with a uniform initial current density. Two thermocouples have been placed: the ﬁrst one on the surface on the middle of the part and the second one in a hole bored in the center of the part so as to measure temperature inside the part. Process parameters are: • frequency: 500Hz • current density: 8.108 Amps/m2 • electromagnetic time step: T/64=3.125 10−5 s • thermal time step: 0.5s In order to enable a visualization of the dissipated joule power, an eﬀective electrical ﬁeld has been deﬁned at a given node as the integration over an electromagnetic period of the square of the real instantaneous electrical ﬁeld:

(n+1)T

1 E 2 (t)dt (44) Eef f = T nT

This eﬀective electrical ﬁeld is also proportional to the amplitude of the electric ﬁeld in a harmonic complex formulation. Figure 2b shows the eﬀective electric ﬁelds isovalues. Due to the high value of the permeability, we can notice the concentration of the magnetic ﬁeld along the work piece surface; this is a well-known physical eﬀect since magnetic ﬁeld lines tend to concentrate on material surface when the magnetic permeability gets high. We can see on Fig. 2c how the heat propagates here rather uniformly from the surface towards the centre. This is typical of a global homogeneous heating application.

Modelling of Metal Forming Processes and Multi-Physic Coupling

233

Fig. 3. Experimental validation

Figure 3 shows the excellent agreement between experimental and computed temperatures on the surface and inside the work piece. On one hand, the computed temperatures on the surface provide a good way to validate the dissipated heat due to eddy currents inside the work piece - and thus the electric ﬁeld computation and the whole electromagnetic procedure. On the other hand, the good agreement observed between the experimental and numerically computed delay on heat propagation to the internal part of the work piece validates the heat transfer diﬀusion model and the thermal coupling procedure. This case deals with a moving short inductor - a case representative of what takes place in an induction heat treatment process. The inductor displacement is modeled through a continuous variation of physical properties of the mesh. Figure 4 shows the geometry and the initial location of the inductor in the mesh. Figure 5 shows an example of electric ﬁeld distribution at a given time step; in this case, the electric ﬁeld is non-symmetric since the inductor location changes continuously. The numerical model presented here is described more in detail in [7]. Extension to parallel computations is detailed in [8]. This model has also been used for magnetic parameters identiﬁcation as detailed in [9]. A global optimization procedure has also been developed to achieve better control of induction heating processes. This strategy can be extended to various multiphysics coupled problems; it is detailed in [10].

234

J.-L. Chenot and F. Bay

Fig. 4. Moving inductor case: geometry and initial mesh

Fig. 5. Moving inductor case: electric ﬁeld isovalues

5 Coupling with Microstructure Evolution 5.1 Introduction The microstructure of the materials changes signiﬁcantly during forming operations. For instance in metals, dynamic or static recovery and recrystallization can take place. These evolutions need to be modeled when the ﬁnal microstructure is to be optimized, or when the behavior of the metal must be described accurately during forming. Several strategies can be developed to compute microstructure evolutions in forming processes with large spatial

Modelling of Metal Forming Processes and Multi-Physic Coupling

235

heterogeneity of strain rate, strain and temperature ﬁelds. The ﬁnite element method allows to model microstructure evolutions in complementary ways. 5.2 Macroscopic Approach In a ﬁrst classical way, one can assume that each node covers a material volume suﬃciently large to be summarized by a Homogeneous Equivalent Medium (HEM). Laws for microstructure evolution of homogeneous media are then applied. This strategy is adequate for modeling a large volume of material, for instance at the scale of a component. A well-known example of a microstructure model is the Avrami equation [11]. It is typically used in an integrated form to describe the recrystallization phenomena for metals as a function of time t: k t (45) X = 1 − exp − ln t0.5 where X is the state variable describing the recrystallized volume fraction, t0.5 is the half recrystallization time, and k the Avrami exponent. Such microstructure evolution laws are typically obtained from isothermal experiments. However, a typical forming process induces signiﬁcant temperature evolutions. It is assumed that non isothermal path can be divided into a number of isothermal steps. Using the results of isothermal tests to calculate the microstructure evolution for any thermal path implies that an integration rule can be applied. Additivity rules are often used in recrystallization studies, the procedure uses a ﬁctitious time method [12], [22] to discretize the microstructure evolution equation. Using for instance the Avrami equation, the algorithm is as follows: at step i of the computation, the recrystallized volume fraction Xi at time ti has been computed; the ﬁctitious time t∗i+1 is calculated as the total time needed to obtain a recrystallized volume fraction Xi at constant temperature Ti+1 . In order to calculate the next recrystallized volume fraction Xi+1 , Avrami equation is used for temperature Ti+1 and time (t∗i+1 + ti+1 − ti ). R for This strategy has been used with the 3D Finite Element code Forge3 forging simulations. Figure 6 illustrates the case of a 316L austenitic stainless steel part deformed at 1273K and annealed at 1373K during 50 seconds. The simulation allows us to take into account both the strain and temperature variations throughout the part, leading to a complex map of statically recrystallized volume fractions, ranging from 10 to 100%, as shown in Fig. 6. The challenge is now to model microstructure evolutions over multiple interpass and forming steps; this requires to go back and reﬁne the description of the physical phenomena integrated in the macroscopic evolution laws. 5.3 Multi-Scale Coupling and the Digital Material A second approach may be taken at a smaller scale, within a HEM. It consists in meshing a heterogeneous microstructure, possibly of complex topology and

236

J.-L. Chenot and F. Bay

Fig. 6. Recrystallized volume fraction maps of a forged 316l part

geometry, for studying the detailed relationships between the microstructure and its evolution, or even the associated constitutive law. This is the case for instance when dealing with the plastic deformation of a steel during phase transformation (e.g. [13]). An austenite and ferrite composite is in fact a two-phase HEM which needs to be analyzed in order to determine the mechanical behavior of the steel and the strain distribution within each phase. Analytical bounds and estimates for the mechanical behavior of a two-phase aggregate imply strong topological assumptions. The calculation of the mechanical response of these composite materials can be calculated using the F. E. M. with a representative description of the microstructure, and well posed boundary conditions. The HEM must contain enough grains so that the global behavior is statistically representative of material response. Predictions of such FEM simulations can then be compared with analytical models. An example of a two-phase topology is shown in Fig. 7 with the corresponding 3D ﬁnite element discretization. A calculation of strain distribution for this two-phase ensemble is presented in Fig. 8. The F.E. discretization allows us to capture strong strain gradients at the interface between the two phases. Such digital multiphase volume calculations can ﬁrst be used to validate appropriate analytical models. These simpler models can be used as constitutive laws in large scale ﬁnite element simulations and coupled with the phase transformation diagram to calculate local percentage of each phase. This complete numerical model allows us to calculate thermal, mechanical and metallurgical evolutions in forming processes inducing large strain such as forging or rolling.

Modelling of Metal Forming Processes and Multi-Physic Coupling

237

Fig. 7. Austenite-ferrite topology and corresponding 3d ﬁnite element mesh

Fig. 8. Strain ﬁeld calculated for the two-phase material volume of Fig. 7

This digital material approach can be further reﬁned to integrate the crystallographic textures. A statistically representative ﬁnite element polycrystal can be created by considering each ﬁnite element as a single crystal. Such a strategy proves to be very eﬃcient when the mechanical response is dictated by the heterogeneity of the elastic-plastic behavior throughout a polycrystal, as in fatigue [14].

6 Conclusions We have reviewed several coupling problems where the classical mechanical treatment must be completed in order to take also into account other physical phenomenons: thermal behavior with possible localization of the strain rate, ﬂuid-solid coupling, electro magnetic heating and microstructure evolution. The simple examples which are presented show that the domain is still under

238

J.-L. Chenot and F. Bay

development, and that much eﬀort must be devoted to these ﬁelds before it can be used routinely in industry for any metallic material.

References 1. Cornﬁeld GC, Johnson RH (1973) Theoretical prediction of plastic ﬂow in hot rolling including the eﬀect of various temperature distribution. J Iron Steel Inst 211:567 2. Lee CH, Kobayashi S (1973) New solutions to rigid plastic deformation problems using a matrix method. Trans ASME, J Eng Ind 95:865 3. Zienkiewicz OC, Valliapan S, King IP (1969) Elasto-solution of engineering problems: initial stress, ﬁnite element approach. Int J Num Meth Engng 1:75– 100 4. Surdon G., Chenot J-L (1986) Finite element calculations of three-dimensional hot forging. International Conference on Numerical Methods in Industrial Forming Processes Numiform’86, ed. by Mattiasson K et al., Balkema AA, Rotterman, 287–292 5. Wagoner, RH, Chenot J-L (2001) Metal forming analysis. Cambridge University Press, Cambridge 6. Davies EJ (1990) Conduction and Induction Heating, P. Peregrinus Ltd., London 7. Bay F, Labbe V, Favennec Y, Chenot J-L (2000) A numerical model for induction heating processes coupling electromagnetism and thermomechanics. Int J Num Meth Engng 58:839–867 8. Labbe V, Favennec Y, Bay F (2002) Numerical modeling of heat treatment with induction heating processes using a parallel ﬁnite element software. 5th Conf. World Congress on Computational Mechanics, Vienna, Austria 9. Favennec Y, Labbe V, Tillier Y, Bay F (2000) Identiﬁcation of magnetic parameters through inverse analysis coupled with ﬁnite element modeling. IEEE Transactions on Magnetics 38(6):3607–3619 10. Favennec Y, Labbe V, Bay F (2004) The ultraweak time coupling in nonlinear modeling and related optimization problems. Int J Num Meth Engng 60:3 11. Avrami M (1939) Kinetics of phase change. I. General theory, Journal of Chemical Physics 7:1103–1112; (1940) II. Transformation-time relations for random distribution of nuclei. Journal of Chemical Physics 8:212–224; (1941) III, Granulation, phase change and microstructure. Journal of Chemical Physics 9:177–18 12. Pumphrey WI, Jones FW (1948) Inter-relation of hardenability and isothermal transformation data. ISIJ 159:137–144 13. Thibaux P (2001) Comportement m´ecanique d’un acier C-Mn microalli´e lors du laminage intercritique. PhD Thesis, Ecole des Mines de Paris, CEMEF, Sophia Antipolis, France 14. Turkmen HS, Log´e RE, Dawson PR, Miller MP (2003) On the mechanical behavior of AA 7075-T6 during cyclic loading. International Journal of Fatigue 25(4):267–281

Enhanced Rotation-Free Basic Shell Triangle. Applications to Sheet Metal Forming Eugenio O˜ nate1 , Fernando G. Flores2 and Laurentiu Neamtu3 1

2

3

International Center for Numerical Methods in Engineering (CIMNE) Technical University of Catalonia (UPC) Ediﬁcio C1 Gran Capit´ an s/n, 08034 Barcelona, Spain [email protected] National University of Cordoba Casilla de Correo 916 5000 C´ ordoba, Argentina [email protected] Quantech ATZ SA Gran Capit´ an 2–4, 08034 Barcelona, Spain [email protected]

Summary. An enhanced rotation-free three node triangular shell element (termed EBST) is presented. The element formulation is based on a quadratic interpolation of the geometry in terms of the six nodes of a patch of four triangles associated to each triangular element. This allows to compute an assumed constant curvature ﬁeld and an assumed linear membrane strain ﬁeld which improves the in-plane behaviour of the element. A simple and economic version of the element using a single integration point is presented. The implementation of the element into an explicit dynamic scheme is described. The eﬃciency and accuracy of the EBST element and the explicit dynamic scheme are demonstrated in many examples of application including the analysis of a cylindrical panel under impulse loading and sheet metal stamping problems.

1 Introduction Triangular shell elements are very useful for the solution of large scale shell problems occurring in many practical engineering situations. Typical examples are the analysis of shell roofs under static and dynamic loads, sheet stamping processes, vehicle dynamics and crash-worthiness situations. Many of these problems involve high geometrical and material non linearities and time changing frictional contact conditions. These diﬃculties are usually increased by the need of discretizing complex geometrical shapes. Here the use of shell triangles and non-structured meshes becomes a critical necessity. Despite recent advances in the ﬁeld [1]–[6] there are not so many simple shell

Eugenio Oñate and Roger Owen (eds.), Computational Plasticity, 239–265. © 2007 Springer. Printed in the Netherlands.

240

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

triangles which are capable of accurately modelling the deformation of a shell structure under arbitrary loading conditions. A promising line to derive simple shell triangles is to use the nodal displacements as the only unknowns for describing the shell kinematics. This idea goes back to the original attempts to solve thin plate bending problems using ﬁnite diﬀerence schemes with the deﬂection as the only nodal variable [7]–[9]. In past years some authors have derived a number of thin plate and shell triangular elements free of rotational degrees of freedom (d.o.f.) based on Kirchhoﬀ’s theory [10]–[26]. In essence all methods attempt to express the curvatures ﬁeld over an element in terms of the displacements of a collection of nodes belonging to a patch of adjacent elements. O˜ nate and Cervera [14] proposed a general procedure of this kind combining ﬁnite element and ﬁnite volume concepts for deriving thin plate triangles and quadrilaterals with the deﬂection as the only nodal variable and presented a simple and competitive rotation-free three d.o.f. triangular element termed BPT (for Basic Plate Triangle). These ideas were extended in [20] to derive a number of rotationfree thin plate and shell triangles. The basic ingredients of the method are a mixed Hu-Washizu formulation, a standard discretization into three node triangles, a linear ﬁnite element interpolation of the displacement ﬁeld within each triangle and a ﬁnite volume type approach for computing constant curvature and bending moment ﬁelds within appropriate non-overlapping control domains. The so called “cell-centered” and “cell-vertex” triangular domains yield diﬀerent families of rotation-free plate and shell triangles. Both the BPT plate element and its extension to shell analysis (termed BST for Basic Shell Triangle) can be derived from the cell-centered formulation. Here the “control domain” is an individual triangle. The constant curvatures ﬁeld within a triangle is computed in terms of the displacements of the six nodes belonging to the four elements patch formed by the chosen triangle and the three adjacent triangles. The cell-vertex approach yields a diﬀerent family of rotation-free plate and shell triangles. Details of the derivation of both rotation-free triangular shell element families can be found in [20]. An extension of the BST element to the non linear analysis of shells was implemented in an explicit dynamic code by O˜ nate et al. [25] using an updated Lagrangian formulation and a hypo-elastic constitutive model. Excellent numerical results were obtained for non linear dynamics of shells involving frictional contact situations and sheet stamping problems [17,18,19,25]. A large strain formulation for the BST element using a total Lagrangian description was presented by Flores and O˜ nate [23]. A recent extension of this formulation is based on a quadratic interpolation of the geometry of the patch formed by the BST element and the three adjacent triangles [26]. This yields a linear displacement gradient ﬁeld over the element from which linear membrane strains and constant curvatures can be computed within the BST element.

Enhanced Rotation-Free Basic Shell Triangle

241

In this chapter an enhanced version of the BST element (termed EBST element) is derived using an assumed linear ﬁeld for the membrane strains and an assumed constant curvature ﬁeld. Both assumed ﬁelds are obtained from the quadratic interpolation of the patch geometry following the ideas presented in [26]. Details of the element formulation are given. An eﬃcient version of the EBST element using one single quadrature point for integration of the tangent matrix is presented. An explicit scheme adequate for dynamic analysis is brieﬂy described. The eﬃciency and accuracy of the EBST element is validated in a number of examples of application including the non linear analysis of a cylindrical shell under an impulse loading and practical sheet stamping problems.

2 Basic Thin Shell Equations Using a Total Lagrangian Formulation 2.1 Shell Kinematics A summary of the most relevant hypothesis related to the kinematic behaviour of a thin shell are presented. Further details may be found in the wide literature dedicated to this ﬁeld [8,9]. Consider a shell with undeformed middle surface occupying the domain Ω 0 in R3 with a boundary Γ 0 . At each point of the middle surface a thickness h0 is deﬁned. The positions x0 and x of a point in the undeformed and the deformed conﬁgurations can be respectively written as a function of the coordinates of the middle surface ϕ and the normal t3 at the point as x0 (ξ1 , ξ2 , ζ) = ϕ0 (ξ1 , ξ2 ) + λt03 x (ξ1 , ξ2 , ζ) = ϕ (ξ1 , ξ2 ) + ζλt3

(1) (2)

where ξ1 , ξ2 are arc-length curvilinear principal coordinates deﬁned over the middle surface of the shell and ζ is the distance from the point to the middle surface in the undeformed conﬁguration. The product ζλ is the distance from the point to the middle surface measured on the deformed conﬁguration. The parameter λ relates the thickness at the present and initial conﬁgurations as: h (3) h0 This approach implies a constant strain in the normal direction. Parameter λ will not be considered as an independent variable and will be computed from purely geometrical considerations (isochoric behaviour) via a staggered iterative update. Besides this, the usual plane stress condition of thin shell theory will be adopted. A convective system is computed at each point as λ=

gi (ξ) =

∂x ∂ξi

i = 1, 2, 3

(4)

242

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

∂ (ϕ ϕ (ξ1 , ξ2 ) + ζλt3 ) = ϕ α + ζ (λt3 ) α ∂ξα ∂ (ϕ ϕ (ξ1 , ξ2 ) + ζλt3 ) = λt3 g3 (ξ) = ∂ζ

gα (ξ) =

α = 1, 2

(5) (6)

This can be particularized for the points on the middle surface as aα = gα (ζ = 0) = ϕ α

(7)

a3 = g3 (ζ = 0) = λt3

(8)

The covariant (ﬁrst fundamental form) metric tensor of the middle surface is aαβ = aα · aβ = ϕ α · ϕ β

(9)

The Green-Lagrange strain vector of the middle surface points (membrane strains) is deﬁned as (10) εm = [εm11 , εm12 , εm12 ]T with

1 (aij − a0ij ) (11) 2 The curvatures (second fundamental form) of the middle surface are obtained by εmij =

καβ =

1 ϕ α · t3 β + ϕ β · t3 α = −t3 · ϕαβ 2

,

α, β = 1, 2

The deformation gradient tensor is F =[x1 , x2 , x3 ] = ϕ 1 + ζ (λt3 ) 1 ϕ 2 + ζ (λt3 ) 2 λt3

(12)

(13)

The product FT F = U2 = C (where U is the right stretch tensor, and C the right Cauchy-Green deformation tensor) can be written as ⎤ ⎡ a11 + 2κ11 ζλ a12 + 2κ12 ζλ 0 (14) U2 = ⎣ a12 + 2κ12 ζλ a22 + 2κ22 ζλ 0 ⎦ 0 0 λ2 In the derivation of expression (14) the derivatives of the thickness ratio λ a and the terms associated to ζ 2 have been neglected. Equation (14) shows that U2 is not a unit tensor at the original conﬁguration for curved surfaces (κ0ij = 0). The changes of curvature of the middle surface are computed by (15) χij = κij − κ0ij Note that δχij = δκij .

Enhanced Rotation-Free Basic Shell Triangle

243

For computational convenience the following approximate expression (which is exact for initially ﬂat surfaces) will be adopted ⎤ ⎡ a11 + 2χ11 ζλ a12 + 2χ12 ζλ 0 (16) U2 = ⎣ a12 + 2χ12 ζλ a22 + 2χ22 ζλ 0 ⎦ 0 0 λ2 This expression is useful to compute diﬀerent Lagrangian strain measures. An advantage of these measures is that they are associated to material ﬁbres, what makes it easy to take into account material anisotropy. It is also useful to compute the eigen decomposition of U as U=

3

λα rα ⊗ rα

(17)

α=1

where λα and rα are the eigenvalues and eigenvectors of U. The resultant stresses (axial forces and moments) are obtained by integrating across the original thickness the second Piola-Kirchhoﬀ stress vector σ using the actual distance to the middle surface for evaluating the bending moments. This gives

σ dζ (18) σ m ≡ [N11 , N22 , N12 ]T = σ b ≡ [M11 , M22 , M12 ]T =

h0

h0

σ λζ dζ

With these values the virtual work can be written as

T δεεmσ m + δκ κT σ b dA = δuT tdA A0

(19)

(20)

A0

where δu are virtual displacements, δεεm is the virtual Green-Lagrange membrane strain vector, δκ κ are the virtual curvatures and t are the surface loads. Other load types can be easily included into (20). 2.2 Constitutive Models In order to treat plasticity at ﬁnite strains an adequate stress-strain pair must be used. The Hencky measures will be adopted here. The (logarithmic) strains are deﬁned as ⎤ ⎡ 3 ε11 ε21 0 ln (λα ) rα ⊗ rα (21) Eln = ⎣ ε12 ε22 0 ⎦ = α=1 0 0 ε33 For the type of problems dealt within the paper we use an elastic-plastic material associated to thin rolled metal sheets.

244

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

In the case of metals, where the elastic strains are small, the use of a logarithmic strain measure reasonably allows to adopt an additive decomposition of elastic and plastic components as Eln = Eeln + Epln

(22)

A linear relationship between the (plane) Hencky stresses and the logarithmic elastic strains is chosen giving T = H Eeln

(23)

where H is the constitutive matrix. The constitutive equations are integrated using a standard return algorithm. The following Mises-Hill [30] yield function with non-linear isotropic hardening is chosen n

2 2 2 + (F + H) T22 − 2H T11 T22 + 2N T12 = σ0 (e0 + ep ) (G + H) T11

(24)

where F, G, H and N deﬁne the non-isotropic shape of the yield surface and the parameters σ0 , e0 and n deﬁne its size as a function of the eﬀective plastic strain ep . The simple Mises-Hill yield function allows, as a ﬁrst approximation, to treat rolled thin metal sheets with planar and transversal anisotropy. The Hencky stress tensor T can be easily particularized for the plane stress case. We deﬁne the rotated Hencky and second Piola-Kirchhoﬀ stress tensors as TL = RTL T RL

(25)

RTL

(26)

SL =

S RL

where RL is the rotation tensor obtained from the eigenvectors of U given by (27) RL = r1 , r2 , r3 The relationship between the rotated Hencky and Piola-Kirchhoﬀ stresses is (α, β = 1, 2) 1 [TL ]αα λ2α ln (λα /λβ ) [TL ]αβ = 1 2 − λ2 λ α β 2

[SL ]αα = [SL ]αβ

(28)

The second Piola-Kirchhoﬀ stress tensor can be computed by S=

2 2 α=1 β=1

[SL ]αβ rα ⊗ rβ

(29)

The second Piola-Kirchhoﬀ stress vector σ used in Eqs.(18–19) can be readily extracted from the S tensor.

Enhanced Rotation-Free Basic Shell Triangle

245

3 Enhanced Basic Shell Triangle The main features of the element formulation (termed EBST for Enhanced Basic Shell Triangle) are the following: 1. The geometry of the patch formed by an element and the three adjacent elements is quadratically interpolated from the position of the six nodes in the patch (Fig. 1). 2. The membrane strains are assumed to vary linearly within the central triangle and are expressed in terms of the (continuous) values of the deformation gradient at the mid side points of the triangle. 3. An assumed constant curvature ﬁeld within the central triangle is chosen. This is computed in terms of the values of the (continuous) deformation gradient at the mid side points. Details of the derivation of the EBST element are given below. 3.1 Definition of the Element Geometry and Computation of Membrane Strains A quadratic approximation of the geometry of the four elements patch is chosen using the position of the six nodes in the patch. It is useful to deﬁne the patch in the isoparametric space using the nodal positions given in the Table 1 (see also Fig. 1). Table 1. Isoparametric coordinates of the six nodes in the patch of Fig. 1 1234 5 6 ξ 0 1 0 1 -1 1 η 0 0 1 1 1 -1

The quadratic interpolation is deﬁned by ϕ=

6

Ni ϕ i

(30)

i=1

with (ζ = 1 − ξ − η) N1 = ζ + ξη N4 = N2 = ξ + ηζ N5 = N3 = η + ζξ N6 =

ζ 2 ξ 2 η 2

(ζ − 1) (ξ − 1) (η − 1)

(31)

This interpolation allows to computing the displacement gradients at selected points in order to use an assumed strain approach. The computation of the gradients is performed at the mid side points of the central element of the patch denoted by G1 , G2 and G3 in Fig. 1. This choice has the following advantages.

246

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

η 5

4

2

M

2

G1

G2

1

4

.. .

1 3

3

2

1

3

G3

2

ξ

3 1

5

6

(a)

6 (b)

Fig. 1. (a) Patch of three node triangular elements including the central triangle (M) and three adjacent triangles (1, 2 and 3); (b) Patch of elements in the isoparametric space

•

Gradients at the three mid side points depend only on the nodes belonging to the two elements adjacent to each side. This can be easily veriﬁed by sampling the derivatives of the shape functions at each mid-side point. • When gradients are computed at the common mid-side point of two adjacent elements, the same values are obtained, as the coordinates of the same four points are used. This in practice means that the gradients at the mid-side points are independent of the element where they are computed. A side-oriented implementation of the ﬁnite element will therefore lead to a unique evaluation of the gradients per side. The Cartesian derivatives of the shape functions are computed at the original conﬁguration by the standard expression

Ni,ξ Ni,1 = J−1 (32) Ni,2 Ni,η

where the Jacobian matrix at the original conﬁguration is

0 ϕ · t1 ϕ0 η · t1 J = 0ξ ϕ ξ · t2 ϕ0 η · t2

(33)

The deformation gradients on the middle surface, associated to an arbitrary spatial Cartesian system and to the material cartesian system deﬁned on the middle surface are related by [ϕ ϕ 1 , ϕ 2 ] = ϕ ξ , ϕ η J−1 (34) The membrane strains within the central triangle are obtained using a linear assumed strain ﬁeld εˆm , i.e. εm = εˆm

(35)

Enhanced Rotation-Free Basic Shell Triangle

with εˆm = (1 − 2ζ)εε1m + (1 − 2ξ)εε2m + (1 − 2η)εε3m =

3

¯i ε i N m

247

(36)

i=1

where εim are the membrane strains computed at the three mid side points Gi ¯1 = (1 − 2ζ), etc. (i = 1, 2, 3 see Fig. 1). In Eq.(36) N The gradient at each mid side point is computed from the quadratic interpolation (30): ⎤ ⎡ 3 i i Nj,α ϕj ⎦ + Ni+3,α ϕi+3 , α = 1, 2 , i = 1, 2, 3 (ϕ ϕ α )Gi = ϕi α = ⎣ j=1

(37) Substituting Eq.(11) into (36) and using Eq.(9) gives the membrane strain vector as ⎧ i ⎫ 3 ϕ · ϕi − 1 ⎬ 1 ¯ ⎨ i1 i1 Ni ϕ · ϕ − 1 (38) εm = 2 ⎩ 2ϕi 2 i ⎭ i=1 2ϕ 1 · ϕ 2 and the virtual membrane strains as ⎧ ⎫ 3 ϕi 1 ϕi 1 · δϕ ⎨ ⎬ ¯i ϕi 2 ϕi2 · δϕ N δεεm = ⎩ i ⎭ ϕ 1 · ϕi 2 + ϕi 1 · δϕ ϕi2 i=1 δϕ

(39)

We note that the gradient at each mid side point Gi depends only on the coordinates of the three nodes of the central triangle and on those of an additional node in the patch, associated to the side i where the gradient is computed. Combining Eqs.(39), (37) and (30) gives δεεm = Bm δap with

δap 18×1

= [δuT1 , δuT2 , δuT3 , δuT4 , δuT5 , δuT6 ]T

(40a) (40b)

where δap is the patch displacement vector and Bm is the membrane strain matrix. An explicit form of this matrix is given in [26]. Note that the membrane strains within the EBST element are a function of the displacements of the six patch nodes. 3.2 Computation of Curvatures We will assume the following constant curvature ﬁeld within each element ˆ αβ καβ = κ

(41)

248

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

where κ ˆ αβ is the assumed constant curvature ﬁeld deﬁned by

1 t3 · ϕ βα dA0 κ ˆ αβ = − 0 AM A0M

(42)

where A0M is the area (in the original conﬁguration) of the central element in the patch. Substituting Eq.(42) into (41) and integrating by parts the area integral gives the curvature vector within the element in terms of the following line integral ⎫ ⎧ ⎡ ⎤

−n1 0 ⎨ κ11 ⎬ 1 t3 · ϕ 1 ⎣ ⎦ κ22 0 −n2 dΓ (43) = κ= t3 · ϕ 2 ⎭ A0M ΓM ⎩ 0 2κ12 −n2 −n1 where ni are the components (in the local system) of the normals to the 0 . The integration by parts of element sides in the initial conﬁguration ΓM Eq.(42) is typical in ﬁnite volume methods for computing second derivatives over volumes by line integrals of gradient terms [28,29]. For the deﬁnition of the normal vector t3 , the linear interpolation over the central element is used. In this case the tangent plane components are ϕ α =

3

LM i,α ϕ i

,

α = 1, 2

(44a)

i=1

t3 =

ϕ1 × ϕ2 = λ ϕ1 × ϕ2 |ϕ ϕ1 × ϕ2 |

(44b)

From these expressions it is also possible to compute in the original coni ﬁguration the element area A0M , the outer normals (n1 , n2 ) at each side and M the side lengths li . Equation (44b) also allows to evaluate the thickness ratio λ in the deformed conﬁguration and the actual normal t3 . The numerical evaluation of the line integral in Eq.(43) results in a sum over the integration points at the element boundary which are, in fact, the same points used for evaluating the gradients when computing the membrane strains. As one integration point is used over each side, it is not necessary to distinguish between sides (i) and integration points (Gi ). In this way the curvatures can be computed by ⎡ ⎤

3 −n1 0 1 M⎣ t3 · ϕ 1 ⎦ 0 −n2 dΓ (45) l κ= 0 t3 · ϕ 2 AM i=1 i −n2 −n1 Eq.(45) is now expressed in terms of the shape functions of the 3-noded triangle LM i (which coincide with the area coordinates [4]). Noting the property of the area coordinates

i

M liM Li,x nx M =− (46) ∇Li = LM 2AM niy i,y

Enhanced Rotation-Free Basic Shell Triangle

the expression for the curvature can be expressed as ⎡ M ⎤

Li,1 0 3 i M ⎦ t3 · ϕ 1 ⎣ 0 L κ=2 i,2 t3 · ϕi 2 M i=1 LM i,2 Li,1

249

(47)

The gradient ϕiα is evaluated at each side Gi from the quadratic interpolation ⎡ ⎤ ϕ1

i i i i i ⎢ ϕ2 ⎥ N1,1 N2,1 N3,1 Ni+3,1 ϕ1 ⎢ ⎥ = (48) i i i i ϕi2 N1,2 N2,2 N3,2 Ni+3,2 ⎣ ϕ3 ⎦ ϕi+3 This is a basic diﬀerence with respect of the computation of the curvature ﬁeld in the original Basic Shell Triangle (BST) where the gradient at the side mid-point is computed as the average value between the values at two adjacent elements [20, 23, 26, 27]. Note again than at each side the gradients depend only on the positions of the three nodes of the central triangle and of an extra node (i + 3), associated precisely to the side (Gi ) where the gradient is computed. Direction t3 in Eq.(47) can be seen as a reference direction. If a diﬀerent direction than that given by Eq.(44b) is chosen at an angle θ with the former, this has an inﬂuence of order θ2 in the projection. This justiﬁes Eq.(44b) for the deﬁnition of t3 as a function exclusively of the three nodes of the central triangle, instead of using the 6-node isoparametric interpolation. The variation of the curvatures can be obtained as ⎡ M ⎤ i Li,1 0 3 3 i Nj,1 Ni+3,1 (t3 · δui+3 ) (t3 · δuj ) M ⎦ ⎣ 0 Li,2 κ=2 + − δκ i i (t3 · δuj ) (t3 · δui+3 ) Nj,2 Ni+3,2 M i=1 i=1 LM L i,2 i,1 ⎤ ⎡ M 1 M 2 (L 3 i,1 ρ11 + Li,2 ρ11 ) 1 M 2 ⎦ (t3 · δui ) = Bb δap ⎣ (LM − (49) i,1 ρ22 + Li,2 ρ22 ) M 1 M 2 i=1 (Li,1 ρ12 + Li,2 ρ12 ) In Eq.(49) Bb = [Bb1 , Bb2 , · · · , Bb6 ]

(50)

Details of the derivation of the curvature matrix Bb are given in [26, 27]. 3.3 The EBST1 Element A simpliﬁed and yet very eﬀective version of the EBST element can be obtained by using one point quadrature for the computation of all the element integrals. This element is termed EBST1. Note that this only aﬀects the membrane stiﬀness matrices and it is equivalent to using a assumed constant membrane strain ﬁeld deﬁned by an average of the metric tensors computed at each side. Numerical experiments have shown that both the EBST and the EBST1 elements are free of spurious energy modes.

250

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

4 Boundary Conditions Elements at the domain boundary, where an adjacent element does not exist, deserve a special attention. The treatment of essential boundary conditions associated to translational constraints is straightforward, as they are the natural degrees of freedom of the element. The conditions associated to the normal vector are crucial in the bending formulation. For clamped sides or symmetry planes, the normal vector t3 must be kept ﬁxed (clamped case), or constrained to move in the plane of symmetry (symmetry case). The former case can be seen as a special case of the latter, so we will consider symmetry planes only. This restriction can be imposed through the deﬁnition of the tangent plane at the boundary, including the normal to the plane of symmetry ϕ0 n that does not change during the process. The tangent plane at the boundary (mid-side point) is expressed in terms of two orthogonal unit vectors referred to a local-to-the-boundary Cartesian system (see Fig. 2) deﬁned as 0 ¯ s (51) ϕ n , ϕ ¯ s emerges from where vector ϕ0 n is ﬁxed during the process while direction ϕ the intersection of the symmetry plane with the plane deﬁned by the central element (M ). The plane (gradient) deﬁned by the central element in the selected original convective Cartesian system (t1 , t2 ) is M ϕ 1 , ϕM (52) 2 the intersection line (side i) of this plane with the plane of symmetry can be written in terms of the position of the nodes that deﬁne the side (j and k) and the original length of the side liM , i.e. ϕi s =

1 ϕk − ϕj

(53)

liM

T

T

That together with the outer normal to the side ni = [n1 , n2 ] = [n · t1 , n · t2 ] (resolved in the selected original convective Cartesian system) leads to

iT iT ϕ 1 n1 −n2 ϕ n = (54) n2 n1 ϕiT ϕiT 2 s

where, noting that λ is the determinant of the gradient, the normal component of the gradient ϕi n can be approximated by ϕi n =

ϕ0 n ϕi s | λ|ϕ

(55)

For a simple supported (hinged) side, the problem is not completely deﬁned. The simplest choice is to neglect the contribution to the side rotations

Enhanced Rotation-Free Basic Shell Triangle symmetry plane

t0i3

i

t3 0

0

n=

ι =ϕ ’n ϕ ’n

ϕ ’n 0

s= k

251

j

ϕ ’s

M t1 t2 j

j Μ

i

ϕ ’s

k Z

k

i

Y

original

X

Μ

ϕ ’2

ϕ ’1 i deformed

Fig. 2. Local Cartesian system for the treatment of symmetry boundary conditions

from the adjacent element missing in the patch in the evaluation of the curvatures via Eq.(43) [20, 23, 26]. This is equivalent to assume that the gradient at the side is equal to the gradient in the central element, i.e. i M (56) ϕ 1 , ϕi 2 = ϕM 1 , ϕ 2 More precise changes can be however introduced to account for the diﬀerent natural boundary conditions. One may assume that the curvature normal to the side is zero, and consider a contribution of the missing side to introduce this constraint. As the change of curvature parallel to the side is also zero along the hinged side, this obviously leads to zero curvatures in both directions. We note ﬁnally that for the membrane formulation of element EBST, the gradient at the mid-side point of the boundary is assumed equal to the gradient of the main triangle. More details on the speciﬁcation of the boundary conditions on the EBST element can be found in [26, 27].

5 Explicit Solution Scheme For simulations including large non-linearities, such as those occuring in sheet metal forming processes involving frictional contact conditions on complex geometries or large instabilities, convergence is diﬃcult to achieve with implicit schemes. In those cases an explicit solution algorithm is typically most advantageous. This scheme provides the solution for dynamic problems and also for quasi-static problems if an adequate damping is chosen. The dynamic equations of motion to solve are of the form r(u) + Du˙ + M¨ u=0

(57)

where M is the mass matrix, D is the damping matrix and the dot means the time derivative. The solution is performed using the central diﬀerence method.

252

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

To make the method competitive a diagonal (lumped) M matrix is typically used and D is taken proportional to M. As usual, mass lumping is performed by assigning one third of the triangular element mass to each node in the central element. The explicit solution scheme can be summarized as follows. At each time step n where displacements have been computed: 1. Compute the internal forces rn . This follows the steps described in Box 1. 2. Compute the accelerations at time tn n ˙ n−1/2 ] ¨ n = M−1 u d [r − Du

(58)

where Md is the diagonal (lumped) mass matrix. 3. Compute the velocities at time tn+1/2 ¨ n δt u˙ n+1/2 = u˙ n−1/2 + u

(59)

4. Compute the displacements at time tn+1 un+1 = un + u˙ n+1/2 δt

(60)

5. Update the shell geometry 6. Check frictional contact conditions

6 Example 1. Cylindrical Panel under Impulse Loading The geometry of the cylinder and the material properties are shown in Fig. 3. A prescribed initial normal velocity of vo = −5650 in/sec is applied to the points in the region shown modelling the eﬀect of the detonation of an explosive layer. The panel is assumed to be clamped along all the boundary. One half of the cylinder is discretized only due to symmetry conditions. Three diﬀerent meshes of 6 × 12, 12 × 32 and 18 × 48 triangles were used for the analysis. The deformed conﬁgurations for time = 1msec are shown for the three meshes in Fig. 3. The analysis was performed assuming an elastic-perfect plastic material behaviour (σy = ky ky = 0). A study of the convergence of the solution with the number of thickness layers showed again that four layers suﬃce to capture accurately the non linear material response [25]. A comparison of the results obtained with the BST and EBST1 elements using the coarse mesh and the ﬁner mesh is shown in Fig. 4 where experimental results reported in [32] have also been plotted for comparison purposes. Good agreement between the numerical and experimental results is obtained. Figs. 4 show the time evolution of the vertical displacement of two reference points along the center line located at y = 6.28in and y = 9.42in, respectively. For the ﬁner mesh results between both elements are almost identical. For the coarse mesh it can been seen that the BST element is more ﬂexible than the EBST1.

Enhanced Rotation-Free Basic Shell Triangle

253

1. Generate the actual configuration ϕn+1 = ϕn + ∆un n+1 2. Compute the metric tensor an+1 αβ and the curvatures καβ . Then at each layer k compute the (approximate) right Cauchy-Green tensor. From Eq.(14) Cn+1 = an+1 + zk χn+1 (61) k 3. Compute the total (21) and elastic (22) deformations at each layer k εn+1 = k

1 ln Cn+1 k 2

(62)

n+1 n − [εεp ]k [εεe ]k = εn+1 k

4. Compute the trial Hencky elastic stresses (23) at each layer k n+1

Tn+1 = H [εεe ]k k

(63)

5. Check the plasticity condition and return to the plasticity surface. If necn+1 essary correct the plastic strains [εεp ]k at each layer 6. Compute the second Piola-Kirchhoff stress vector σ n+1 and the generalk ized stresses σ n+1 = m

NL h0 X σ n+1 wk k NL k=1

σ n+1 = b

NL h0 X σ n+1 zk wk k NL

(64)

k=1

Where wk is the weight of the through-the-thickness integration point. Recall that zk is the current distance of the layer to the mid-surface and not the original distance. However, for small strain plasticity this distinction is not important. This computation of stresses is exact for an elastic problem. 7. Compute the residual force vector from ZZ ZZ Li t dA − (BTmi σ m + BTbi σ b )dA (65) rei = A

A◦

Box 1. Computation of the internal forces vector

254

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3.0

10 .2 r v egio 03 0= n 36 w i n 50 it in h /s ec

h = 0.125 in

8 6

12.56

ky = 44 000 lb/in2 k’y = 0 lb/in2

R=2.9375 Z

2

E = 10.5 x 10 lb/in ρ = 2.5 x 104 lb sec2/in4 ν = 0.33

Y

X Z

Y X

Fig. 3. Cylindrical panel under impulse loading. Geometry and material properties. Deformed meshes for time = 1msec

1.4

1.2

Deflection [in]

1

0.8

0.6

0.4 Experimental BST mesh 3 EBST1 mesh 3 BST mesh 1 EBST1 mesh 1

0.2

0

0

0.2

0.4 0.6 Time [msec.]

0.8

1

Fig. 4. Cylindrical panel under impulse loading. Time evolution of the displacement of two points along the crown line. Upper lines y = 6.28in. Lower lines y = 9.42 in. Comparison of results obtained with BST and EBST1 elements (mesh 1: 6 × 12 elements and mesh 3: 18 × 48 elements) and experimental values

Enhanced Rotation-Free Basic Shell Triangle

255

The numerical values of the vertical displacement at the two reference points obtained with the BST and EBST1 elements after a time of 0.4 ms using the 16 × 32 mesh are compared in Table 2 with a numerical solution obtained by Stolarski et al. [31] using a curved triangular shell element and the 16 × 32 mesh. Experimental results reported in [32] are also given for comparison. It is interesting to note the reasonable agreement of the results for y = 6.28in. and the discrepancy of present and other published numerical solutions with the experimental value for y = 9.42in. Table 2. Cylindrical panel under impulse load. Comparison of vertical displacement values of two central points for t = 0.4 ms Vertical displacement (in.) element/mesh y = 6.28in y = 9.42in BST (6 × 12 el.) -1.310 -0.679 BST (18 × 48 el.) -1.181 -0.587 EBST1 (6 × 12 el.) -1.147 -0.575 EBST1 (18 × 48 el.) -1.171 -0.584 Stolarski et al. [31] -1.183 -0.530 Experimental [32] -1.280 -0.700

The deformed shapes of the transverse section for y = 6.28in. and the longitudinal section for x = 0 obtained with the both elements for the coarse and the ﬁne meshes after 1ms. are compared with the experimental results in Figs. 5 and 6. Excellent agreement is observed for the ﬁne mesh for both elements.

7 Application to Sheet Metal Forming Problems The features of tghe EBST1 element make it ideal for analysis of sheet metal stamping processes. A number of examples of simulations of practical problems of this kind are presented. Numerical results have been obtained with the sheet stamping simulation code STAMPACK where the EBST1 element has been implemented [35]. 7.1 S-rail Sheet Stamping The next problem corresponds to one of the sheet stamping benchmark tests proposed in NUMISHEET’96 [33]. The analysis comprises two parts, namely, simulation of the stamping of a S-rail sheet component and springback computations once the stamping tools are removed. Figure 7 shows the deformed sheet after springback.

256

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3

Z [in]

2

Original Experimental EBST1 mesh 1 BST mesh 1 EBST1 mesh 3 BST mesh 3

1

0

1

2

X [in]

Fig. 5. Cylindrical panel under impulse loading. Final deformation (t = 1msec) of the panel at the cross section y = 6.28in. Comparison with experimental values

Z-direction [in]

3

2

Experimental BST mesh 3 EBST1 mesh 3 BST mesh 1 EBST1 mesh 1

1

0

0

2

4

6

8

10

12

Y-direction [in]

Fig. 6. Cylindrical panel under impulse loading. Final deformation (t = 1msec) of the panel at the crown line (x = 0.00in). Comparison with experimental values

The detailed geometry and material data can be found in the proceedings of the conference [33] or in the web [34]. The mesh used for the sheet has 6000 triangles and 3111 points (Fig. 7). The tools are treated as rigid bodies.

Enhanced Rotation-Free Basic Shell Triangle

G"

257

Z

X

Y

B"

Fig. 7. Stamping of a S-rail. Final deformation of the sheet after springback obtained in the simulation. The triangular mesh of the deformed sheet is also shown

The meshes used for the sheet and the tools are those provided by the benchmark organizers. The material considered here is a mild steel (IF) with Young Modulus E = 2.06GP a and Poisson ratio ν = 0.3. Mises yield criterion was used for plasticity behaviour with non-linear isotropic hardening deﬁned by σy (ep ) = 545(0.13 + ep )0.267 [M P a]. A uniform friction of 0.15 was used for all the tools. A low (10kN) blank holder force was considered in this simulation. Figure 8 compares the punch force during the stamping stage obtained with both BST and EBST1 elements for the simulation and experimental values. Also for reference the average values of the simulations presented in the conference are included. Explicit and implicit simulations are considered as diﬀerent curves. There is a remarkable coincidence between the experimental values and the results obtained with both the BST and EBST1 elements. Figure 9 plots the Z coordinate along line B”–G” after springback. The top surface of the sheet does not remain plane due to some instabilities due to the low blank holder force used. Results obtained with the simulations compare very well with the experimental values. 7.2 Stamping of Industrial Automotive Part Figure 10 shows the geometry of the lateral panel of a car and the mesh of 457760 EBST1 elements used for the computation. Results of the stamping simulation are shown in Fig. 11. Note that the outpus of the simulation have been translated into graphical plots indicating the quality of the stamping process and the risk of failure in the diﬀerent zones of the panel. This helps designers to taking decissions on the adequacy of the stamping process and for introducing changes in the design of the stamping tools (dies, punch, blankholders, etc.) and the process parameters if needed. Figure 12 shows the geometry mesh and results of the stamping of a front fender part of an automotive. The initial mesh had 121960 EBST1 elements.

258

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

40

Punch Force [kN]

30

20

Experimental Explicit (average) Implicit (average) BST EBST1

10

0

0

10

20

30

40

Punch Travel [mm]

Fig. 8. Stamping of a S-rail. Punch force versus punch travel. Average of explicit and implicit results reported at the benchmark conference are also shown

Adaptive mesh reﬁnement was used along the simulation process leading to a ﬁnal mesh of 389870 elements. Finally, Figs. 13 and 14 show the same type of information for the stamping of a car tail gate. The initial and ﬁnal meshes (after adaptive mesh reﬁnement) had 186528 and 489560 EBST1 elements, respectively. The simulation results are displayed in both problems with an “engineering insight” in order to help the design and manufacturing of the stamping tools and the deﬁnition of the stamping process as previously mentioned.

8 Concluding Remarks An enhanced rotation-free shell triangle (termed EBST) is obtained by using a quadratic interpolation of the geometry in terms of the six nodes belonging to the four elements patch associated to each triangle. This allows to computing an assumed constant curvature ﬁeld and an assumed linear membrane strain ﬁeld which improves the in-plane behaviour of the original element. A simple and economic version of the element using a single integration point has been presented. The eﬃciency of the rotation-free shell triangle has been demonstrated in examples of application including the analysis of a cylinder under impulse loading and practical sheet stamping problems.

Enhanced Rotation-Free Basic Shell Triangle

259

Z coordinate[mm]

39

38

37 Experimental Explicit (average) Implicit (average) BST EBST1 36

0

50

100

150

200

250

distance [mm]

Fig. 9. Stamping of a S-rail. Z-coordinate along line B”—G” after springback. Average of explicit and implicit results reported at the benchmark conference are also shown

Fig. 10. Lateral panel of an automotive. Finite element mesh of 457760 triangles used for the simulation

260

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

Fig. 11. Lateral panel of a car. Results of the stamping analysis

The enhanced rotation-free basic shell triangle element with a single integration point (the EBST1 element) is an excellent candidate for solving practical sheet metal stamping problems and other non linear shell problems in engineering involving complex geometry, dynamics, material and geometrical non linearities and frictional contact conditions.

Enhanced Rotation-Free Basic Shell Triangle

261

Fig. 12. Front fender. Results of the stamping analysis using an initial mesh of 121960 EBST1 elements. The ﬁnal adapted mesh had 389870 elements

262

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

Fig. 13. Car tail gate. Geometry and ﬁnal adapted mesh of 489560 EBST1 elements used for the stamping simulation

ACKNOWLEDGEMENTS The support of the company QUANTECH (www.quantech.es) providing the code STAMPACK [35] is gratefully acknowledged. This research was partially supported by project SEDUREC of the Consolider Programme of the Ministerio de Educaci´ on y Ciencia of Spain.

Enhanced Rotation-Free Basic Shell Triangle

263

Fig. 14. Car tail gate. Map of relative thickness distribution and forming zones on the stamped part

References 1. O˜ nate E (1994) A review of some ﬁnite element families for thick and thin plate and shell analysis. Publication CIMNE N. 53, May 2. Flores FG, O˜ nate E, Z´ arate F (1995) New assumed strain triangles for non-linear shell analysis. Computational Mechanics 17:107–114

264

Eugenio O˜ nate, Fernando G. Flores and Laurentiu Neamtu

3. Argyris JH, Papadrakakis M, Apostolopoulou C, Koutsourelakis S (2000) The TRIC element. Theoretical and numerical investigation. Comput Meth Appl Mech Engrg 182:217–245 4. Zienkiewicz OC, Taylor RL (2005) The ﬁnite element method. Solid Mechanics. Vol II, Elsevier 5. Stolarski H, Belytschko T, Lee S-H (1995) A review of shell ﬁnite elements and corotational theories. Computational Mechanics Advances vol. 2 (2), NorthHolland 6. Ramm E, Wall WA (2002) Shells in advanced computational environment. In V World Congress on Computational Mechanics, Eberhardsteiner J, Mang H, Rammerstorfer F (eds), Vienna, Austria, July 7–12. http://wccm.tuwien.ac.at. 7. Bushnell D, Almroth BO (1971) Finite diﬀerence energy method for non linear shell analysis. J Computers and Structures 1:361 8. Timoshenko SP (1971) Theory of Plates and Shells, McGraw Hill, New York 9. Ugural AC (1981) Stresses in Plates and Shells, McGraw Hill, New York 10. Nay RA, Utku S (1972) An alternative to the ﬁnite element method. Variational Methods Eng vol. 1 11. Hampshire JK, Topping BHV, Chan HC (1992) Three node triangular elements with one degree of freedom per node. Engng Comput 9:49–62 12. Phaal R, Calladine CR (1992) A simple class of ﬁnite elements for plate and shell problems. I: Elements for beams and thin plates. Int J Num Meth Engng 35:955–977 13. Phaal R, Calladine CR (1992) A simple class of ﬁnite elements for plate and shell problems. II: An element for thin shells with only translational degrees of freedom. Int J Num Meth Engng 35:979–996 14. O˜ nate E, Cervera M (1993) Derivation of thin plate bending elements with one degree of freedom per node. Engineering Computations 10:553–561 15. Brunet M, Sabourin F (1994) Prediction of necking and wrinkles with a simpliﬁed shell element in sheet forming. Int Conf of Metal Forming Simulation in Industry II:27–48, Kr¨ oplin B (ed) 16. Rio G, Tathi B, Laurent H (1994) A new eﬃcient ﬁnite element model of shell with only three degrees of freedom per node. Applications to industrial deep drawing test. In Recent Developments in Sheet Metal Forming Technology, Barata Marques MJM (ed), 18th IDDRG Biennial Congress, Lisbon 17. Rojek J, O˜ nate E (1998) Sheet springback analysis using a simple shell triangle with translational degrees of freedom only. Int J of Forming Processes 1(3):275– 296 18. Rojek J, O˜ nate E, Postek E (1998) Application of explicit FE codes to simulation of sheet and bulk forming processes. J of Materials Processing Technology 8081:620–627 19. Jovicevic J, O˜ nate E (1999) Analysis of beams and shells using a rotation-free ﬁnite element-ﬁnite volume formulation, Monograph 43, CIMNE, Barcelona 20. O˜ nate E, Z´ arate F (2000) Rotation-free plate and shell triangles. Int J Num Meth Engng 47:557–603 21. Cirak F, Ortiz M (2000) Subdivision surfaces: A new paradigm for thin-shell ﬁnite element analysis. Int J Num Meths in Engng 47:2039-2072 22. Cirak F, Ortiz M (2001) Fully C 1 -conforming subdivision elements for ﬁnite deformations thin-shell analysis. Int J Num Meths in Engng 51:813-833 23. Flores FG, O˜ nate E (2001) A basic thin shell triangle with only translational DOFs for large strain plasticity. Int J Num Meths in Engng 51:57–83

Enhanced Rotation-Free Basic Shell Triangle

265

24. Engel G, Garikipati K, Hughes TJR, Larson MG, Mazzei L, Taylor RL (2002). Continuous/discontinuous ﬁnite element approximation of fourth-order elliptic problems in structural and continuum mechanics with applications to thin beams and plates, and strain gradient elasticity. Comput Methods Appl Mech Engrg 191:3669–3750 25. O˜ nate E, Cendoya P, Miquel J (2002) Non linear explicit dynamic analysis of shells using the BST rotation-free triangle. Engineering Computations 19(6):662–706 26. Flores FG, O˜ nate E (2005) Improvements in the membrane behaviour of the three node rotation-free BST shell triangle using an assumed strain approach. Comput Meth Appl Mech Engng 194(6-8):907–932 27. O˜ nate E, Flores FG (2005) Advances in the formulation of the rotation-free basic shell triangle. Comput Meth Appl Mech Engng 194(21–24):2406–2443 28. Zienkiewicz OC, O˜ nate E (1991) Finite Elements vs. Finite Volumes. Is there really a choice?. Nonlinear Computational Mechanics. State of the Art. Wriggers P, Wagner R (eds), Springer Verlag, Heidelberg 29. O˜ nate E, Cervera M, Zienkiewicz OC (1994) A ﬁnite volume format for structural mechanics. Int J Num Meth Engng 37:181–201 30. Hill R (1948) A Theory of the Yielding and Plastic Flow of Anisotropic Metals. Proc Royal Society London A193:281 31. Stolarski H, Belytschko T, Carpenter N (1984) A simple triangular curved shell element. Eng Comput 1:210–218 32. Balmer HA, Witmer EA (1964) Theoretical experimental correlation of large dynamic and permanent deformation of impulsively loaded simple structures. Air force ﬂight Dynamic Lab Rep FDQ-TDR-64-108, Wright-Patterson AFB, Ohio, USA 33. NUMISHEET’96 Third International Conference and Workshop on Numerical Simulation of 3D Sheet Forming Processes, Lee EH, Kinzel GL, Wagoner RH (eds), Dearbon-Michigan, USA, 1996 34. http://rclsgi.eng.ohio-state.edu/%7Elee-j-k/numisheet96/ 35. STAMPACK. A General Finite Element System for Sheet Stamping and Forming Problems, Quantech ATZ, Barcelona, Spain, 2007. (www.quantech.es)

Computational Methods in Applied Sciences 1. 2. 3. 4. 5. 6.

7.

J. Holnicki-Szulc and C.A.M. Soares (eds.): Advances in Smart Technologies in Structural Engineering. 2004 ISBN 3-540-22331-2 J.A.C. Ambrósio (ed.): Advances in Computational Multibody Systems. 2005 ISBN 1-4020-3392-3 E. Oñate and B. Kröplin (eds.): Textile Composites and Inflatable Structures. 2005 ISBN 1-4020-3316-8 J.C. García Orden, J.M. Goicolea and J. Cuadrado (eds.): Multibody Dynamics. Computational Methods and Applications. 2007 ISBN 1-4020-5683-4 V.M.A. Leitão, C.J.S. Alves and C.A. Duarte (eds.): Advances in Meshfree Techniques. 2007 ISBN 1-4020-6094-6 C.A.M. Soares, J.A.C. Martins, H.C. Rodrigues and J.A.C. Ambrósio (eds.): Computational Mechanics. Solids, Structures and Coupled Problems. 2006 ISBN 978-1-4020-4978-1 E. Oñate and R. Owen (eds.): Computational Plasticity. 2007 ISBN 978-1-4020-6576-7

www.springer.com

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close